Eric Le Bourhis
Glass
Related Titles McGee, T
Glass Manufacturing Engineering 2006 ISBN-13: 978-0-471-50836-6
Affa...

Author:
Eric Le Bourhis

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Eric Le Bourhis

Glass

Related Titles McGee, T

Glass Manufacturing Engineering 2006 ISBN-13: 978-0-471-50836-6

Affatigato, M.

Advances in Glass and Optical Materials II Ceramic Transactions. Volume 197 August 2006 ISBN-13: 978-0-470-08343-7

Doremus, R. H.

Glass Science Second edition 1994 ISBN-13: 978-0-471-89714-1

Eric Le Bourhis

Glass Mechanics and Technology

The Author Professor Eric Le Bourhis Universite´ de Poitiers Laboratoire. de Me´tallurgie Physique, UMR 6630 CNRS, SPMI-Te´le´port 2-Bd. Marie et Pierre Curie, BP 30179 86962 Futuroscope-Chasseneuil Cedex France

All books published by Wiley-VCH are carefully produced. Nevertheless, authors, editors, and publisher do not warrant the information contained in these books, including this book, to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate. Library of Congress Card No.: applied for British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library. Bibliographic information published by the Deutsche Nationalbibliothek The Deutsche Nationalbibliothek lists this publication in the Deutsche Nationalbibliograﬁe; detailed bibliographic data are available in the Internet at . # 2008 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim All rights reserved (including those of translation into other languages). No part of this book may be reproduced in any form – by photoprinting, microﬁlm, or any other means – nor transmitted or translated into a machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not speciﬁcally marked as such, are not to be considered unprotected by law. Typesetting Thomson Digital, India Printing betz-druck GmbH, Darmstadt Binding Litges & Dopf Buchbinderei GmbH, Heppenheim Cover Design WMX-Design, Bruno Winkler, Heidelberg Printed in the Federal Republic of Germany Printed on acid-free paper ISBN: 978-3-527-31549-9

V

Contents Foreword XIII Preface XV Symbols and Deﬁnitions (units in parentheses) Physical Constants XXI Abbreviations XXIII 1

Introduction

2 2.1 2.2 2.3 2.4 2.5

Glass, A Ceramic Material 5 Four Classes of Materials 5 Materials Properties 10 Selecting Materials 12 Performance Indices 15 Shape Factors in Mechanical Design

3 3.1 3.2 3.3 3.4 3.4.1 3.4.2

Glass Prehistory and History 25 Natural Glasses 25 Early Glasses 29 First Optical Glasses 32 Modern Glasses 34 Soda-Lime-Silica Glasses 34 Borosilicate and Aluminosilicate Glasses

4 4.1 4.2 4.3 4.4 4.5 4.6

Applications of Glass 39 Glazing 39 Containers 44 Optical Glass 46 Glass Fibres for Insulation and Reinforcement Abrasive Tools 49 Glass Manufacturers 50

XVII

1

18

37

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

48

VI

Contents

5 5.1 5.2 5.2.1 5.2.2 5.2.3 5.3 5.4 5.5 5.6 5.6.1 5.6.2 5.6.2.1 5.6.2.2 5.6.3 5.6.4 5.6.5 5.6.6 5.7 5.7.1 5.7.2 5.7.3 5.7.4 5.8 5.8.1 5.8.2 5.8.3 5.8.3.1 5.8.3.2 5.8.3.3 5.8.4

Glass Structure 53 Introduction 53 Silica Glass and Related Glasses 54 Glass Network 54 Glass Network Modiﬁcation 57 Short-Range Order 60 Borate Glass and Related Glasses 64 Organic and Chalcogenide Glasses 65 Metallic Glasses 65 Avoiding Crystallization 66 Nucleation and Growth of Crystallized Phases 66 Nucleation of Crystallized Phases 67 Homogeneous Nucleation 68 Heterogeneous Nucleation 70 Crystal Growth 71 TTT Diagram 74 Devitriﬁcation 75 Factors That Favour Glass Formation 76 Vitroceramic Fabrication 76 Introduction 76 Conventional Method (two stages) 77 Modiﬁed Conventional Method (single stage) 77 Laser-Induced Method 77 Glass Surface 78 Surface Reaction 78 Molecular Diffusion 79 Glass Network Interaction with Water 79 Water Reaction 80 Ion Exchange 80 Glass Corrosion 81 Surface Properties 81

6 6.1 6.1.1 6.1.2 6.1.2.1 6.1.2.2 6.1.2.3 6.1.3 6.1.3.1 6.1.3.2 6.1.3.3 6.1.3.4 6.2

Glass Rheology 83 Viscosity 83 Viscosity and Process 83 Viscosity Measurement 86 Rotation Viscometer 87 Falling Sphere Viscometer 88 Fibre Elongation Viscometer 88 Viscosity Variation with Temperature 90 Introduction 90 Fragility 93 VFT Empirical Formula 94 Microscopic Approach 94 Glass Transition and Its Observation 99

VII

6.2.1 6.2.2 6.2.3 6.3 6.4 6.4.1 6.4.2 6.4.3 6.4.4 6.4.5 6.4.5.1 6.4.5.2 6.4.5.3 6.4.5.4 6.5 6.5.1 6.5.2 6.5.3 6.5.4 6.6 6.7 6.7.1 6.7.2 6.7.3 6.7.4

‘Observing’ the Glass Transition 99 Dilatometry 101 Differential Scanning Calorimetry 103 Viscous Response of Glass 104 Viscoelastic Response of Glass 106 Introduction 106 Maxwell and Kelvin Solids 107 Dynamic Mechanical Analysis 109 Modelling Real Solids 111 Functional Formulation 113 Creep 113 Stress Relaxation 114 Elastic–Viscoelastic Correspondence 116 Superposition Principle (simple thermorheological behaviour) Tempering of Glass 119 Introduction 119 Freezing Theory 120 Stress Relaxation 122 Structural Relaxation 123 Transient Stresses 128 Chemical Tempering of Glass 130 Introduction 130 Ion Exchange and Stress Build-Up 131 Stress Relaxation 132 Engineered Stress Proﬁle Glasses 132

7 7.1 7.2 7.3 7.3.1 7.3.2 7.4 7.5 7.6 7.6.1 7.6.2 7.6.3 7.7 7.7.1 7.7.2 7.7.3 7.7.4 7.8 7.8.1

Mechanical Strength of Glass 135 Theoretical Strength 135 Tensile Resistance of Glass 136 Stress Concentration and Grifﬁth Energy Balance 141 Stress Concentration 141 Energy Balance 143 Linear Elasticity Crack Tip Stress Field 144 SIF under Non-uniform Stress 145 Toughness Measurement 146 Compact Tension 146 Notch Beam Test 146 Double Torsion 147 Inﬂuence of Residual Stress on Strength and Fragmentation Inﬂuence of Residual Thermal Stress on Strength 150 Inﬂuence of Residual Chemical Stress on Strength 150 Inﬂuence of Residual Stress on Fragmentation 151 Impact-Induced Fracture 152 Statistical Weibull Analysis 153 Introduction 153

116

148

VIII

Contents

7.8.2 7.8.2.1 7.8.2.2 7.8.3

Functional Formulation 153 Uniform Tensile Stress 155 Non-uniform Tensile Stress 155 Population of Flaws 157

8 8.1 8.1.1 8.1.2 8.1.2.1 8.1.2.2 8.1.3 8.1.3.1 8.1.3.2 8.1.3.3 8.1.3.4 8.1.3.5 8.1.3.6 8.1.3.7 8.2 8.3 8.4 8.5

Contact Resistance of Glass 161 Sharp and Blunt Contact 161 Introduction 161 Spherical Indentation 162 Elastic Loading 162 Hertz Fracture and Indentation Toughness 164 Sharp Indentation 167 Elastic Loading 167 Elastic–Plastic Loading 169 Hardness 170 Radial–Median Cracking 174 Indentation Toughness 177 Lateral Cracking and Chipping 179 Brittleness Index 180 Sharp Contact Resistance 181 Scratch Resistance 185 Abrasion Resistance 186 Cutting and Drilling of Glass 188

9 9.1 9.1.1 9.1.2 9.2 9.2.1 9.2.2 9.2.3 9.3 9.4 9.5 9.6 9.7

Ageing of Glass 191 Fatigue in Glass 191 Static Fatigue 191 Testing Methods 191 Stress Corrosion 192 Introduction (Domain III) 192 Domains O and I: Reaction Controlled Domain II: Transport Controlled 195 Charles and Hillig Theory 195 Lifetime Under Static Fatigue 196 Applications 199 NiS Phase Transformation 199 Crack Healing 201

10 10.1 10.1.1 10.1.2 10.1.3 10.1.4 10.2

Mechanics of Glass Processes Introduction 203 Batching 204 Melting 205 Fining 207 Forming 208 Float Process 208

203

193

IX

10.3 10.4 10.4.1 10.4.2 10.5 10.5.1 10.5.2

Fusion Draw 212 Container Process 213 Pressing 215 Press-and-Blow, Blow-and-Blow Processes Fibre Process 218 Tensile Drawing 219 Centrifugal Drawing 221

11 11.1 11.2 11.3 11.4 11.4.1 11.4.2

Production Control of Residual Stresses 225 Introduction 225 Residual Stresses in Flat Glass 226 Basic of Photoelasticity in Flat Glass 227 Stress Meters 231 Edge Stress Meters 231 Surface Stress Meters 234

12 12.1 12.2 12.2.1 12.2.2 12.2.3 12.3 12.3.1 12.3.2 12.3.3 12.4 12.5

High-tech Products and R&D 235 Market Trend-Driven R&D 235 Flat Display Panels 236 Active Matrix Liquid Crystal Displays 237 Plasma Display Panels 237 Glass Stability 238 Thin-Film Technology 240 Chemical Vapour Deposition 243 Physical Vapour Deposition 244 Sol–Gel Routes 249 Residual Stresses in Thin Films 252 Applications of Coatings and Summary 254

13

Conclusion

216

257

Appendix 1 Light Absorption, Dispersion and Polarization A1.1 Electromagnetic Spectrum 259 A1.2 Light Absorption 259 A1.3 Light Dispersion 261 A1.4 Light Polarization 262 Appendix 2 Atomic Structure and Bond Formation A2.1 Atomic Structure 265 A2.2 Mendeleev Table 267 A2.3 Bond Formation 267 Appendix 3 Thermal Expansion and Elasticity A3.1 The a–E Trend 271 A3.2 Qualitative Approach 271

271

265

259

X

Contents

A3.3 A3.4

Expansion Modelling 272 Differential Expansion Measurement

273

Appendix 4 Falling Sphere Viscometer and Fining of Glass A4.1 Falling Sphere 275 A4.1.1 Asymptotic Regime 275 A4.1.2 Transient Regime 276 A4.2 Fining of Glass 277 Appendix 5

Theoretical Strength of a Solid

Appendix 6

Weibull Analysis

275

279

283

Appendix 7 Photoelastic Set-Up for Lectures 287 A7.1 Set-Up for Photoelastic Projection 287 A7.2 Example of a Beam under Flexion (Transient Stresses) 287 A7.3 Example of Tempered Specimens (Residual Stresses) 288 Appendix 8 Instrumented Nanoindentation Applied to Thin Films 291 A8.1 Instrumented Nanoindentation 291 A8.2 Indentation Strain Field 295 A8.3 Hardness, Yield Stress and Representative Flow Stress 296 A8.4 Coating–Substrate Composite Response 300 A8.5 Time-Dependent Response 302 A8.5.1 Viscoelastic Indentation Curves 303 A8.5.2 Viscous Elastic–Plastic Indentation F(h) Curves 305 A8.6 Elastic–Plastic Ratios 307 Appendix 9 Strain and Stress 311 A9.1 Stress and Strain 311 A9.2 Stress and Strain Tensors 312 A9.3 Uniaxial Tensile Test 314 A9.4 Simple Shear 314 A9.5 Plane Stress 315 A9.6 Hydrostatic Pressure and Stress Deviator 316 A9.7 Generalized Hooke’s Law 317 A9.8 Kelvin and Maxwell Models 318 A9.9 Generalized Maxwell Model 319 Appendix 10 Flow and Plasticity in Glass 321 A10.1 Introduction 321 A10.2 From Newtonian to Non-Newtonian Flow 322 A10.3 From Homogeneous to Heterogeneous Flow 325

XI

Appendix 11 Finite Element Analysis 329 A11.1 FEM of the Pressing of a Parison 329 A11.2 FEM of the Precision Moulding of a Glass Lens 329 A11.3 FEM of Fracture 330 A11.4 FEM of Contact Loading 333 Appendix 12 X-Ray Diffraction Analysis of Thin-Film Residual Stresses 335 A12.1 Thin-Film Stress and Strain 335 A12.2 X-Ray Diffraction Method 337 A12.3 The e–sin2c Method 338 Appendix 13 Diffusion 341 A13.1 Diffusion Laws 341 A13.2 Steady-State Diffusion 345 A13.3 Non-steady-State Diffusion 347 Glossary

351

References Index

361

353

XIII

Foreword It is a pleasure to introduce this book which approaches glass from the scientiﬁc and technological sides. This is an important contribution to the glass literature since few books address both these aspects together. Glass mechanics has appeared as a preliminary for further development of glass functionality and performance. This issue is complex and requires detailed understanding of glass science and industry. This textbook gives a comprehensive approach to glass mechanics taking constant care to keep as close as possible to the applications. The author shares his own experiences both in the academic and industrial ﬁelds resulting in an illustrative and relevant description of glass research and development. This book will be of great interest as training material for people entering the glass industry as well as future engineers and researchers in the ﬁeld. Aubervilliers, France June 2007

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

Rene´ Gy

XV

Preface The project of writing this book started from lectures given to future engineers in materials science. The prime idea was to present both science and technology that participate in industrial R&D. I chose the glass industry as an example having working experiences on both industrial and academic sides. The science–technology approach and concepts developed and illustrated in the book can be utilized in other contexts and for other materials. Fracture and ageing, photoelasticity, rheology, contact resistance, diffusion and production tools issues are shared by many ﬁelds. For teaching purposes, appendices suggest exercises and experimental approaches. It is hoped to offer an overview of the background science and technology used in industry and R&D. The book focuses on mechanics, which has to be considered throughout the industrial process. Preparing this book, I am indebted to many colleagues from industry and academe for their support, discussions and motivations. I would like to thank R. Gy, H. Arribart, J. Prieur, S. Valladeau, E. Bodiot, O. Gaume, N. Brown, J. Zhang, C. Bleuze, J.M. Poujade, P.H. Guering, M.H. Chopinet, E. Barthel, L. Lesage (Saint Gobain group), A. Alliche (ECP Paris), R. Vacher, C. Levelut, D. Cavaille´, J. Pelous (Montpellier University), M.M. Chaudhri (Cambridge University), C.R. Kurkjian (Rutgers University), T. Rouxel, J.C. Sangleboeuf, V. Keryvin (Rennes University), G. Patriarche, L. Largeau (LPN Marcoussis), P. Gadaud (ENSMA Poitiers), D. Mousserion, P.O. Renault, P. Goudeau, J. Bonneville, C. Jaouen, C. Templier, T. Cabioc’h, F. Tranchant, C. Coupeau (Poitiers University), L. Pranevicius and S. Tamulevicius (Kaunas University). I should like to acknowledge support from Wiley VCH, in particular K. Sora and W. Wu¨st. The author also wishes to thank S. Valladeau for his help in carrying out again fractography and photoelasticity experiments, and R. Gy, E. Barthel and F. Mammeri for critical reading and suggestions on parts of the book. Some students worked with me to develop research and applicative studies, and their contributions have been of utmost importance. I would like to thank M. Bustarret, C Teles, M. Beaurain, N. Tournerie, D. Metayer, F. Mammeri, D. Faurie and N. Chemin who shared investigation interest during their training period. This book is dedicated to my wife, sons and parents. Futuroscope-Chasseneuil September 2007 Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

Eric Le Bourhis

XVII

Symbols and Deﬁnitions (units in parentheses) a Contact radius a Distance a Acceleration ao Atomic diffusion jump ac Atomic diffusion interface path a Mark diagonal A Cation ﬁeld intensity A Elastic anisotropy Ap Projected surface Ac Contact projected surface B Brittleness index B, B Magnetic ﬁeld BON Bridging oxygen number c(x, t) Concentration c Radial crack length cl Lateral crack length cP Speciﬁc heat cR Cooling rate C Brewster constant Cg Atomic packing density D Diffusion coefﬁcient E Young’s modulus (2(1 þ n)G) E, E Electric ﬁeld Ei Indenter Young’s modulus Ep Potential energy Es Specimen Young’s modulus f Friction coefﬁcient F Load, force Fc Critical load for fracture Fm Maximum force g Gravitational acceleration g(T ) Growth rate Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

(m) (m) (m s2) (m) (m) (m) (m2) (m2) (m2) (m1/2) (T) (m3) (m) (m) (J kg1 K1) (K s1) (B) (m2 s1) (Pa) (V m) (Pa) (J) (Pa) (N m1 s) (N) (N) (N) (m s2) (m s1)

XVIII

Symbols and Deﬁnitions

Dg Energy barrier for diffusion jump Dg 0 Energy barrier for diffusion at nucleus interface Dg 00 Energy barrier for diffusion at germ interface G Shear modulus G0 Conservation or storage modulus G00 Loss modulus G(t) Relaxation modulus DG Energy barrier for diffusion jump DG0 Energy barrier for diffusion at nucleus interface DG00 Energy barrier for diffusion at particle interface DGv Molar enthalpy of the transformation from liquid to crystal h Penetration h Total penetration he Elastic penetration hl Depth of lateral crack hm Maximum penetration hp Plastic penetration hv Viscous penetration H Hardness or mean pressure Hv Vickers hardness (0.927p) H(t) Heaviside function (¼ 1 for t > 1; ¼ 0 for t 0) I Second moment Io Incidence angle J Diffusion ﬂux J Shear compliance J(t) Compliance k Thermal conductivity k Wave vector K Stress intensity factor (SIF) Kc Fracture toughness L Length m Fragility m Weibull modulus m, M Mass M Torque n Optical index n Volumic concentration n Surface concentration n(T) Nucleation rate p Polarisation vector p Pressure P Property Ps Probability Q Heat r Position or distance

(J at1) (J at1) (J at1) (Pa) (Pa) (Pa) (Pa) (J mol1) (J mol1) (J mol1) (J mol1) (m) (m) (m) (m) (m) (m) (m) (Pa) (Pa) (m4) (rad) (m2 s1) (Pa1) (Pa1) (W m1 K1) (rad m1) (Pa m1/2) (Pa m1/2) (m)

(kg) (N m) (m3) (m2) (m3 s1) (C m) (Pa)

(J) (m)

XIX

r Radius rc Cation radius ro Interatomic distance rO Oxygen radius R Radius RD(r) Radial distribution S Surface, section S Entropy t Time tH Thickness T Temperature Tf Glass ﬁctive temperature Tg Glass transition temperature TL Liquidus temperature Tm Melting temperature TR Relaxation time (h/G) DT Thermal gradient tan(d) Loss factor U Fractured specimen total energy v Velocity vf Free volume (per atom) vl Limit velocity v Minimal volume for atomic jump V Volume Vm Molar volume w Angular velocity wc Critical energy for a particle to form Y Yield stress or yield pressure YR Representative ﬂow stress z Impacter (indenter) penetration Z Atomic number Z Cation valence a Shear angle al Thermal expansion coefﬁcient of the liquid as Thermal expansion coefﬁcient of the solid b Phase shift b Angle between indenter ﬂank and specimen surface g Shear strain d Loss angle e Strain e1, e2, e3 Principal strains z, zcl, zcs, zsl Surface energies h Viscosity

(m) (m) (m) (m) (m) (m2) (J K1) (s) (m) (K) (K) (K) (K) (K) (s) (K) (J) (m s1) (m3) (m s1) (m3) (m3) (m3 mol1) (rad s1) (J) (Pa) (Pa) (m)

(rad) (K1) (K1) (rad) (rad) (rad)

(J m2) (Pa s)

XX

Symbols and Deﬁnitions

hR Viscosity at reference temperature u Wetting angle u Distortion l Wavelength lm Wavelength at maximum light intensity n Poisson’s ratio nE Atomic transition frequency, Einstein frequency ni Indenter Poisson’s ratio ns Specimen Poisson’s ratio j Reduced time r Density s Stress s1, s2, s3 Principal stresses sc Core stress (s(z ¼ 0)) sm Mean stress sM Maximum stress ss, Surface stress (s(z ¼ tH/2)) t Shear stress y Reciprocal dispersion f Shape factor fi Volume fraction f(T) Shift factor F Heat ﬂow c1(t) Shear relaxation function c2(t) Hydrostatic relaxation function V Atomic volume

(Pa s) (rad) (rad) (m) (m) (Hz)

(s) (m3) (Pa) (Pa) (Pa) (Pa) (Pa) (Pa) (Pa)

(J s1)

(m3)

Shorthand Notation @ @x @ Gradient operator r ¼ @y @ @z @/@t, @/@x Partial derivatives For an x only or r only space variation r ¼ d/dx or d/dr Overbar or overdot ¼ d/dt Time derivative Double overdot ¼ d2/dt2 Second time derivative 0 ¼ d/dV Volume derivative [ ] Concentration

(m1) (s1) (s2) (m3) (mol l1 or m3)

XXI

Physical Constants g Gravitational acceleration: 9.8 m s2 N Avogadro number: 6.022 1023 mol1 h Planck’s constant: 6.626 1034 J s R Perfect gas constant: 8.314 J mol1 K1 k Boltzmann’s constant (¼ R/N): 1.381 1023 J K1 e Electron charge: 1.6 1019 C eo Vacuum permittivity (moeoc2 ¼ 1, 4peo ¼ 1/(9 109)) c velocity of light: 3 108 m s1 me electron mass: 9.11 1031 kg mp proton mass: 1.673 1027 kg mn neutron mass: 1.675 1027 kg Vm Perfect gas standard volume: 22.4 l mol1 International System Length: metre (m) Mass: kilogram (kg) Time: second (s) Electrical current: ampere (A) Temperature: kelvin (K) Amount of substance: mole (mol) Luminous intensity: candela (Cd) Preﬁxes Tera (T), 1012 Giga (G), 109 Mega (M), 106 Kilo (k), 103 Milli (m), 103 Micro (m), 106 Nano (n), 109 Pico (p), 1012 Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

XXII

Physical Constants

Femto (f), 1015 Atto (a), 1018 Units Conversion 1 atm ¼ 1.015 bar ¼ 0.1 MPa 1 A˚ ¼ 0.1 nm 1 eV ¼ 1.6 1019 J 1 Hz ¼ 1 s1 1J¼1Nm 0 K ¼ 273.2 8C 1 l ¼ 103 m3 1 N ¼ 1 kg m s2 1 P ¼ 0.1 Pa s 1 Pa ¼ 1 N m2 1 torr ¼ 1.33 mbar ¼ 133 Pa 1 W ¼ 1 J s1 1C¼1As 1 V ¼ 1 W A1 1 V ¼ 1 V A1 1 cal ¼ 4.186 J 1 F¼ Ne C mol1 1 in ¼ 25.4 mm Useful Conversions and Numbers k ¼ 0.086 meV K1; for 25 8C, kT ¼ 25 meV N mp N mn 1 g mol1 Human hair diameter is 100 mm, living blood cell diameter 8 mm Glass hardness is about 5 GPa ¼ 50 000 atm!

XXIII

Abbreviations 1D 2D 3D AFM ALS AMLCD AZS BCC BMG BO CBED CEC CRN CSC CT CVD DRM DT DMA ESC ESP EXAFS FCC FDP FEM FIB GFRP HEC IR IS ISE ITO

One dimension Two dimensions Three dimensions Atomic force microscopy Aluminosilicate Active matrix liquid crystal display Alumina–zirconia–silica refractory Body centred cubic Bulk metallic glasses Bridging oxygen Convergent beam electron diffraction Cold end coating Continuous random network Composed semiconductor Compact tension Chemical vapour deposition Dynamic resonance method Double torsion Dynamic mechanical analysis Elemental semiconductor Engineered stress proﬁle Extended X-ray absorption ﬁne structure Face centred cubic Flat display panel Finite element modelling Focused ion beam Glass ﬁbre-reinforced polymer Hot end coating Infrared Individual section Indentation size effect Indium tin oxide, or tin-doped indium oxide

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

XXIV

Abbreviations

LCD Low-E MEMS MD MNR NBO NBT PDP PER PMMA PVB PVD RD R&D RT SEM SENB SIF SLS TEM TEOS TTT UV VDW VFT XPS XRD

Liquid crystal display Low emissivity Micro-electro-mechanical system Molecular dynamics Magnetic nuclear resonance Non-bridging oxygen Notch beam test Plasma display panel Paramagnetic electronic resonance Poly(methyl methacrylate) Polyvinylbutyral Physical vapour deposition Radial distribution Research and development Room temperature Scanning electron microscopy Single edge notched beam specimen Stress intensity factor soda-lime-silica Transmission electron microscopy Tetraethoxysilane Time–temperature–transformation Ultraviolet Van der Waals Vogel–Fulcher–Tammann X-ray photoelectron spectroscopy X-ray diffraction

1

1 Introduction Glass, existing for millions of years, has fascinated and attracted much interest both scientiﬁcally and technologically. For long, glass was considered a ‘fourth state of matter’ before the realization of its ‘liquid-like’ structure. Glass appears on cooling down a liquid continuously until its viscosity becomes so high that it freezes to a glassy state. This happens at some range of temperatures that depends on thermal history. This lets glass be a mysterious material, since the way it is prepared may change its properties. Nowadays open questions are still raised and we shall address some of these within the present book. These theoretical considerations did not however prevent the development and use of glass over the centuries. Empirical knowledge and know-how have developed through the ages so that, nowadays, glass is a commonly available material. The application of glass science to the improvement of industrial tools, so called research and development (R&D), occurred only in the past century, with a few exceptions, as for instance regarding porcelain researches focused on developing processes in Sax and Worcester (Dr J. Wall’s group by 1750, refer also to Limoges (France) and Worcester (UK) museums). In their ‘Perspective on the history of glass composition’ Kurkjian and Prindle (1998) noted that the age of glass science started only in 1886 with the disclosure of the work of Schott and Enrst (Chapter 4). Science and technology were then becoming more and more interrelated. Glass has been employed in many forms to fabricate glazing and containers for centuries while it is now entering new applications that are appearing in nanotechnology (ﬁbres and displays). Many qualities make glass attractive since it is transparent, chemically inert, environmentally friendly and keeps very strong. In fact, no other materials being mass-produced have shown such qualities over so many centuries. Nowadays glass offers recycling opportunities and allows for tailoring new and dedicated applications. The glass industry has been developing considerably in efﬁciency in terms of production rate and quality over the past few decades. Studying glass history in terms of raw materials and process offers an interesting perspective and understanding of how the glass industry progressively developed. These progresses were achieved because of further knowledge on materials properties and tools. While great achievements were accomplished empirically, R&D offered new opportunities. It is much accepted nowadays that an industry has to Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

2

1 Introduction

progress continuously to face the strong competition that has been developing since globalization (with the emergence of low-labour-cost countries). The evolution in technology varies much according to the area of application. As far as glass is concerned, many different ﬁelds are to be considered, from mass production (glazing, containers) to nanotechnology processing (optical ﬁbres, coatings). The glass industry encompasses several international industrial groups that have strengthened their own R&D units. New products and tools are developed and patented before being launched in production. Research products become of utmost importance for these groups that face always strong technological competition. As the glass industry covers so many different applications, this supposes important technological investment and know-how. Conventional silica-soda-lime glass industry covers large application ﬁelds comprising glazing (for transportation and buildings; Fig. 1.1) and containers, and this still represents the most important glass productions in terms of volumes. At the same time, added-value functions have been developed to sustain industrial competition. Glass R&D has allowed great progresses in the manufacturing of new functional glasses improving continuously performance and quality. Nowadays R&D is aimed at adding functions to glass objects with an interdisciplinary approach involving chemistry, mechanics and optics. New ﬁelds are being opened in electronics and displays and glass technology is expected to play an important role in nanotechnology. Different routes are being employed by manufacturers to add the designed functions, either modifying the glass substrate or using coatings. The former alternative is more expensive since up-stream operations have to be modiﬁed to adjust the tools to the changes in melt composition (high-temperature ﬂow). The development of new coatings looks more attractive and

Fig. 1.1 Modern building with glass walls (near the author’s university).

Introduction

would be preferred since no up-stream operations need to be changed; however, this ﬁeld is newly opened and many issues are still to be solved. In particular, one has to tailor coating strength otherwise the designed function would not resist against abrasion over time. In fact, the overall development and production of glass involve important and interdisciplinary knowledge and know-how. This book presents an overview of background science and technology used in the glass industry and R&D. It focuses on mechanics that is to be considered throughout the industrial process. It is well known that glass is a brittle material and one understands why it is important to improve the strength of glass objects. Not so well accepted is that to achieve such a result and also to improve other performances (optical, dielectrical), one has to consider mechanics at most steps of the production. A literature survey reveals in fact strong interest in glass mechanics since 15 % of articles addressing glass science focus on its mechanical properties. This is the reason for the focus of this book. the most important technological property of glass is its viscosity. It determines the melting conditions, the temperatures for working and annealing and the upper temperature for use (devitriﬁcation rates). Glass quality is directly dependent on the way it is homogenized and this is also related to the viscous ﬂow in the glass melt (Chapter 6). Also, proper quenching of the glass allows for the production of residual stresses that will strengthen the glass and protect it from subcritical crack growth (Chapters 7 and 9). The dimensional adjustment of display front and back plates at the pixel resolution requires control of the thermal history and knowledge of the structural relaxation of glass substrates (Chapter 10). Contact mechanics controls the density of superﬁcial defects generated while transferring products (including elevated temperatures; Chapter 8). The distribution and importance of the superﬁcial defects affect the strength of the manufactured object (Chapter 7). Among the few examples listed above, one understands that glass mechanics is a very broad ﬁeld while being one of the most important issues for the glassmaker. The book is composed of 13 chapters; Chapters 2 to 4 are introductory while Chapters 5 to 12 propose a progressive route into glass mechanics and technology, with a main text that could be ﬁrst read following the proposed chronology. Notes, appendices and further references (books, scientiﬁc papers, videos and web sites) are proposed throughout the text for deeper insight. Appendices recall basic concepts and also illustrate through exercises and applications parts of the book. Also, examples throughout the text allow one to employ the concepts used to describe glass behaviour while their application to glass technology is extensively discussed. Some parts with more mathematics will help in getting more insight into glass behaviour. For a ﬁrst lecture these can be skipped.

3

5

2 Glass, A Ceramic Material1) 2.1 Four Classes of Materials

A commonly used classiﬁcation of the materials separates these into four categories (Askeland, 1989; Ashby and Jones, 1991; Mozdierz et al., 1993): i. the metals, ii. the ceramics, iii. the polymers, and iv. the composites, the last mentioned being obtained from mixing materials from the three main categories. This is illustrated in Fig. 2.1 where the three main categories of materials are shown at the centre while the composites made of two of these are shown at the periphery. This classiﬁcation is based on the type of bonding and the related properties as discussed in more detail below. This classiﬁcation can be examined in view of the Mendeleev table (Fig. 2.2; see also Appendix 2). Most elements in the left-hand side of the table display a metallic behaviour while the other elements are considered as non-metals. Metals may be pure or alloyed with other metals and also non-metals (steel being an Fe–C alloy). They are conductors of electricity and heat. Ceramics are inorganic materials and result from the combination of either (i) metals and non-metals (ionic ceramics, NaCl, MgO, Al2O3, TiN, ZrO2) or (ii) only non-metals (covalent ceramics, SiO2, Si3N4). Combination with oxygen, nitrogen and carbon yields oxides (SiO2, MgO, Al2O3), nitrides (TiN, Si3N4) and carbides (WC) respectively. Ceramics show a refractory behaviour; they are electrically and thermally resistant. Polymers are formed by organic chains (–CH2–) and show thermal and electrical resistances. Composites are formed by two or more materials pertaining to two different classes of materials. For instance, a polymer matrix can be reinforced by ceramic ﬁbres to form a new material with properties combining those of its constituents. The proposed

1)

In this chapter, and also in this book, we consider mostly inorganic glasses.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

6

2 Glass, A Ceramic Material

Fig. 2.1 Materials classes.

classiﬁcation is mostly based on the type of bonding between the constituents of the related materials. It suggests that the structure at the nanoscale determines the properties of the material. This is true for many properties (elasticity, thermal expansion; see Chapter 7 and Appendices 1 and 3) while defects happen to play a major role in others (diffusion, fracture, plasticity; see Chapters 6 and 7, and Appendices 3 and 10). We generally distinguish four types of bonding listed in Table 2.1. Ionic and covalent bonds show the highest binding energy. Such bonds are formed in covalent and ionic ceramics. The lowest binding energy is obtained for van der Waals (VDW) bonds. Theses bonds are formed between polymer chains in thermoplastics. VDW and covalent bonds are found in thermosets that are stronger than thermoplastics. Therefore, the related properties are expected to differ drastically from one group to another (for instance from polymers to ceramics). The main properties of the four categories of materials are listed in Table 2.2. Subjective criteria are suggested

Fig. 2.2 Metals and non-metals in the Mendeleev table.

2.1 Four Classes of Materials Tab. 2.1

Binding energies for the four bonding types (after Askeland, 1989).

Bond

Binding energy (kJ mol1)

Ionic Covalent Metallic Van der Waals

600–1600 500–1300 100–840 50 MPa m1/2) Elevated melting point (Tm 1000 8C) Good thermal and electrical conductivity Rigid E 200 GPa Elevated yield stress Y > 3 GPa High hardness Elevated melting point (Tm 2000 8C) Corrosion resistance Good thermal and electrical resistance Ductile, complex shape production Corrosion resistance Low density

Low yield stress for pure metals Y 1 MPa ! Alloys Hardness: H 3Y ! Alloys Corrosion ! Coatings Elevated density

Ceramics

Polymers

Composites

Stiffness (E > 50 GPa) Elevated yield stress (Y 200 MPa) Toughness (Kic > 20 MPa m1/2) Fatigue resistance Corrosion resistance Tailored and low density

Low toughness (Kic < 2 MPa m1/2) Low thermal shock resistance (DT 200 8C) Difﬁculty in complex shape production Elevated density Low stiffness (E 2 GPa) Low yield stress (Y 2–1000 MPa) Low transition temperature (Tg 100 8C) ! Creep Low toughness (Kic 1 MPa m1/2) Complex shape production difﬁculty Cost Creep (for polymer matrix)

7

8

2 Glass, A Ceramic Material Tab. 2.3 Matter state as a function order distance (ro is the interatomic distance). Perfect gas means that interactions between molecules can be neglected. Perfect crystal is a concept used to describe crystal structure with a repeated unit cell. In fact, all real crystals have defects.

Ordering distance increases from gas to crystal. In a sense, glass looks closer to a liquid than to a crystal. In fact, glass can be considered as a frozen liquid for which viscosity becomes so high that the atomic motions have slowed to the extent that characteristic relaxation time exceeds the observation period (Chapter 6). Many properties of glass can in fact be related to its liquid-like structure. Freezing happens at glass transition that sets a boundary between the glassy state and the liquid state. The ‘ﬁctive’ path from the crystal state to the glass state will be illustrated in Chapter 5 in order to get insight into the complex glass structure. Both transitions, i.e. glass to crystal and liquid to glass transitions (arrowed in Table 2.3), correspond to real instability of the glassy state. Both phenomena are discussed extensively in Chapters 5 and 6 respectively. Oxide glasses, the most common one being silico-soda-lime glass, are used to produce glazing or containers. As discussed in more detail in Chapter 5, such a glass is formed by an Si–O network that is modiﬁed by Na+ and Ca2+ ions. This means that such oxide glasses are formed by covalent Si–O bonds while modifying ions interact with non-bridging oxygen (NBO) atoms through ionic bonds (Chapter 5). This allows for the strong bonding characteristic of the ceramics group. It is to be noted that modiﬁcation with Ca2+ leads to less viscosity change than with Na+ since Ca2+ may link two NBO atoms. Organic glasses belong to the polymer category since they are formed by polymer chains interacting through VDW (thermoplastics) or VDW and covalent bonds (thermosets). Let us consider the energy–distance curve related to a single bond. Interatomic spacing ro is the equilibrium distance between atoms forming a bond and results from the balance between the repulsion predominant at short distances and attraction predominant at longer distances. The two contributions shown in Fig. 2.3 result in a potential energy curve that shows a minimum value reached for the atoms at

2.1 Four Classes of Materials

Fig. 2.3 Potential energy as a function of distance resulting from repulsion predominant at short distance and attraction predominant at long distance.

equilibrium distance ro. This can be functionalized in the form of two terms corresponding to repulsion and attraction (see also Appendix 2): Ep ¼ Erep þ Eattr ¼

a b rm rn

Since repulsion is predominant at short distance we have necessarily m > n. Attraction is responsible for the bond formation while electron repulsion happens when atoms overlap (the Pauli exclusion principle of quantum mechanics). The distance ro allows for determining atom radius (half of the bond distance between identical atoms). This concept is very important in the modelling of material structure and we shall use it in Chapter 5. The hard-sphere model supposes that atoms pack as hard spheres, allowing for establishing relationships between atom radii and crystal parameter and quantifying packing density of glasses (Chapter 5). The minimum energy of the bond is deﬁned as the binding energy and is the energy required to break the bond since it is the energy required to separate the atoms or ions to an inﬁnite distance (Appendix 5). Consequently, materials having a high binding energy like oxide glasses also have a high strength and a high melting temperature. Fig. 2.4 plots

Fig. 2.4 Applied force as a function of distance for two types of bonds (weak and strong) showing the relationship between bonding strength and elastic modulus. Steep slope (dF/dr) results in high modulus (see also Appendix 5).

9

10

2 Glass, A Ceramic Material

the applied force as a function of distance, the equilibrium being obtained for a resulting force equal to zero. The elastic modulus of a material which is the amount that it will stretch when a force is applied to it, is related to the slope of the force– distance curve at equilibrium (r ¼ ro, Fig. 2.4; Appendix 5). We shall see that, in fact, elastic moduli do not depend only on the interatomic bonding strength but also depend on the short-range ordering (possible formation of ring chain, atomic packing density; Chapter 5). The curves are shown for two materials, one with a strong bond and maximum force superior to that of a weak bond. A steep slope at r ¼ ro that correlates with an elevated binding energy and hence an elevated melting point, signiﬁes that a greater force is necessary to stretch the bond. Therefore, the material has an elevated elastic modulus. In a similar but more complex manner, the thermal expansion coefﬁcient can be related to the energy–distance curve (Appendix 3). When the material is heated, the atoms or ions separate because of the additional energy supplied to the material. When the binding energy is large enough, the additional energy causes only small changes in the separation distance between ions or atoms as compared to what happens for a material showing a lower binding energy. Therefore, materials showing a large binding energy also show a small thermal expansion (Appendix 3).

2.2 Materials Properties

The next step in the classiﬁcation of materials consists in fabricating the properties charts that show the classiﬁcation of the materials according to one or several performances (Askeland, 1989; Ashby and Jones, 1991). In these charts the ﬁrst three groups mentioned at the start of Section 2.1 (ceramics, metals and polymers) show different trends as expected from the different bond strengths. However, the different groups show a large range of response with partial overlapping of the properties between groups of materials. Fig. 2.5 shows three important diagrams from the mechanical point of view, where yield stress Y, Young’s modulus E and fracture toughness Kc are reported. These properties will be deﬁned in more detail in the following chapters. Here, we mention that these properties characterize the plastic, elastic and brittle resistances of a material corresponding to three most important modes of deformation (compaction may become an important deformation mode in a silica-rich glass network; see Chapters 5 and 8). The trends mentioned in Table 2.2 are clearly observed in Fig. 2.5. For instance, the ceramics exhibit elevated yield stress and Young’s modulus while their toughness is relatively low. Therefore, ceramics are expected to deform elastically up to brittle failure. Brittle behaviour gives origin to the sudden fracture of glass once critical stress is reached at a defect present in the glass. This will also be discussed in detail later in the book (Chapter 7). Instead, polymers show low stiffness and yield strength. They will deform dramatically elastically and plastically until fracture. Fabricating a composite consists in mixing materials and thereafter in mixing the properties of each component. According to the scale of the phases, nanocomposites

2.2 Materials Properties

Fig. 2.5 Four classes of materials (according to Ashby and Jones, 1991).

and microcomposites are formed. Sol–gel techniques allow the fabrication of inorganic–organic materials with a mixing at the atomic scale (see also Chapter 12). Observing the high strength achieved by glass ﬁbres, engineers incorporated them into polymers and succeeded in obtaining great reinforcement. This is now well developed and used in several ﬁelds (laminated structures, boats, car front ends and truck cabs). We can observe that indeed the composite domain covers parts of the ranges covered by the materials used for their fabrication. Changing the

11

12

2 Glass, A Ceramic Material

Fig. 2.6 Longitudinal El and traversal Et moduli of a ﬁbrereinforced composite as a function of ﬁbre volume fraction ff (all ﬁbres are supposed to be aligned along one direction, namely longitudinal; 70 and 7 GPa moduli are taken for the ﬁbre and matrix respectively).

concentration of the reinforcing component allows for tailoring the composite strength. The way that properties P are mixed is a complex issue. In the simplest case a rule of mixture may be employed. In its simplest form, it is written as a linear law P ¼ f1P1 þ f2P2, where fi are the volume fractions of the components (0 < fi < 1 and f1 ¼ 1 f2) and Pi the respective properties. It is observed that when f1 approaches 0 or 1 then the property P approaches the properties of the components P2 or P1 respectively. Let us consider for instance the elastic resistance of a ﬁbre-reinforced matrix. For unidirectionally distributed ﬁbres in a matrix, the Young’s modulus along ﬁbres is El ¼ f1E1 þ f2E2 while it is 1/Et ¼ f1/E1 þ f2/E2 along the normal direction (so called model of springs in parallel or series respectively weighted by the volume fraction of the respective phases; see Chapter 6). The resulting moduli are shown in Fig. 2.6. Using the mixing rules allows tailoring the composite properties between the component properties, adjusting the volume fractions as well as the orientation of the ﬁbres. It is well known so far that the simple linear rule presented above does not apply for all properties of technological importance. While a rule of mixture applies quite well to density and elasticity, it fails to predict the composite material toughness Kc because adhesion and interface issues are of utmost importance in the response and hence in the performance of a composite.

2.3 Selecting Materials

Generally not only one performance is to be optimized but several. An industrial product is then optimized to yield the best compromise between the required properties. For instance, a windscreen is designed with optical transparency, with strength to protect the driver from wind and weather, and with new functions introduced into the

2.3 Selecting Materials Tab. 2.4

Attractive glass properties for different applications.

Glazing Containers Optical glass Glass wool Fibres for reinforcement

Transparency

Strength

Rheology

Chemical inertness

++ + +++

++ ++ + ++

++ ++ + ++ ++

++ +++ ++ ++

laminate (solar control, antenna, etc.). By the way, to achieve such a product, the manufacturing tools have to work in given ranges of properties, for instance viscosity and diffusion. The development of a new product supposes a compromise to be met between all these parameters. This is referred as co-selection. Table 2.4 lists the main properties of glass according to various applications. Transparency is obviously of utmost importance for glazing and optical glasses. This performance combined with strength, rheology and cost make glass very competitive as compared to polymers. In fact, rheology is a very important issue as regards the process. Glass even though not showing exceptional performances in all ﬁelds presents a combination of desired properties that makes it very attractive. Let us consider its transparency according to its cost (or price that takes into account the cost of raw materials, process, marketing and labour; see also Section 12.1), as shown in Fig. 2.7. In this ﬁgure transparency is plotted as a function of price per volume from the materials data base elaborated by Ashby’s team (CES 4, Granta Design; Ashby, 2001). The optical performance is separated into four categories (opaque, translucent, transparent, optical quality). When considering transparency, the glassmaker is interested into the two last categories. Only dedicated optical devices require optical quality (i.e. extremely low optical loss). From the transparency–price chart we already observe that glass is a very good compromise, since only polymers compete. Glass is generally preferred because of its strength, UV protection (in containers), chemical protection, chemical inertness (allowing for conservation of foods and liquid, a property that may remain at elevated temperatures) and tailored optical properties. Developments of glazing encompass tailoring optical properties with transparency at visible wavelength while being opaque to IR and UV (Lehmann, 2005; see also Chapter 4). A chart showing so many parameters requires several dimensions; instead, Ashby (2001) proposes different methodologies to select the optimized materials or compositions either by a step-by-step selection or by using a weighted combination of the important properties that are of interest (weight-factors method). It is out of the scope of this book to detail all these methods and the interested reader should refer to dedicated books cited in the bibliography. As a preliminary, we shall see in the next section how several properties can be combined in a performance index and hence how to select a material in view of a combination of 3–4 properties using graphical methods. The example of selection according to transparency is an archetype. Let us consider a more realistic selection of a glass according to more quantitative properties. As

13

14

2 Glass, A Ceramic Material

Fig. 2.7 Transparency–cost chart (obtained from CES 4, Granta Design, Ashby, 2001).

discussed in detail in Chapter 6, viscosity is one of the most important properties from the process point of view since it controls the stresses and strains to be applied to form the glass. The selection will then be according to the process requirements that set such a parameter (the viscosity in this case) at a given temperature. Research on glass has revealed that in limited domains empirical relations exist between the compositions of oxide glasses and the properties (Priven, 2004). Notably, glass composition can be continuously varied since no stoichiometric laws prevail, in contrast to crystalline solids. This allows for adjusting and approaching the desired performance. The optimization of the composition for process optimization can then be made using these empirical laws to deﬁne a range of compositions likely to yield a glass with the required properties. The estimated ranges of compositions are obviously as accurate as the empirical correlations used for the procedure. For more accuracy in the prediction, further experiments can be made for a selected domain of compositions. One will never ensure that such a range of compositions is indeed a solution to the problem, but it indicates in what range of compositions the costly experiments are probably worth undertaking. The use of designed industrial experiment plans (Sado and Sado, 1991) allows one to minimize the number of fabricated and tested specimens and to predict at minimum costs the selected domain.

2.4 Performance Indices

2.4 Performance Indices

We have seen that selecting materials requires many parameters to be taken into account (co-selection). In fact, an extensive survey of the technological applications has been made by M.F. Ashby’s team and they proposed different performance indices according to the target applications that are combinations of relevant properties of the materials. Let us for instance consider the thermal shock resistance, also known as thermal endurance, deﬁned as the maximum sudden change in temperature which a glass surface can withstand without breaking. Thermal shock happens, for example, when an object is moved abruptly from or into a furnace. These are complex thermomechanical loading conditions that are of utmost importance for the glass (and other) industry since heat treatments are extensively used to produce glazing either during forming or tempering steps (as detailed in Chapter 6). Stresses generated under a thermal gradient are proportional to thermal strains (Hooke’s law; see also Appendix 9) while thermal strains are proportional to the thermal expansion coefﬁcient of the material and to the temperature variation amplitude (DT; see also Chapter 6). The resulting stresses s are written s ¼ CaEDT

ð2:1Þ

where a is the thermal expansion coefﬁcient, E Young’s modulus and C a coefﬁcient dependent on the Poisson ratio (C ¼ 1 for axial constraint, (1 n)1 for biaxial constraint or normal quenching and (1 2n)1 for triaxial constraint, where n is the Poisson ratio; see also Chapter 6 and Appendices 3 and 9). It should be said that the actual value of the stresses developed by a given thermal shock would depend in fact upon many other factors, such as the thermal conductivity of the glass, the thermal conductivity of the ﬂuid that applies the thermal shock and the thickness of the glass (these three factors change the magnitude of DT ). Such factors are neglected here. Ashby (2001) suggested plotting a versus E in a log–log diagram (Fig. 2.8), since in such a plot aE contours are shown as parallel lines: aE constant implies log a ¼ log E þ constant, which for a log–log plot is represented by a straight line of slope –1. On a same line, the value of aE product is then a constant and is deﬁned as the performance index as regards thermal shock stresses. Observing that aE is expressed in MPa K1, the materials shown on the same line are submitted to identical thermal stress amplitude under the same thermal variation amplitude. For instance, along the line indexed 1 MPa K1, all materials would experience thermal stresses of 100 MPa amplitude when submitted to instantaneous (this hypothesis allows neglecting of thermal conductivity mentioned above) thermal shock of amplitude 100 8C. Fig. 2.8 shows that the different groups of materials locate at separated places even though partial overlapping is observed. Overlapping of composite and ceramics groups is not unexpected. Interestingly most important oxide glasses, that is soda-lime-silica (SLS) and borosilicate glasses match the ceramics group. As regards all the materials, one observes that aE index shows a very large variation ranging between 0.01 and

15

16

2 Glass, A Ceramic Material

Fig. 2.8 Thermal expansion coefﬁcient a as a function of Young’s modulus E (according to Ashby, 2001).

10 MPa K1. This map actually allows for a wide materials selection according to what is required for the application (either high or low thermal stresses). Metals show the highest aE index values, while woods and elastomers show minimum values. Regarding glasses, silica is observed to be below 0.1 MPa K1 while SLS glasses could be submitted to more elevated thermal stresses (about 0.5 MPa K1). In fact, for applications requiring thermal shock resistance, silica-rich and borosilicate glasses have been developed, so-called Nonex (for nonexpanding, invented in 1912 by E.C. Sullivan and W.C. Taylor to reduce lantern globe breakage by 50%) and Pyrex developed by Corning (Kurkjian and Prindle, 1998; see also Chapter 3). On the contrary, when tempering is considered elevated aE indices are required. This is in favour of utilizing compositions of standard silico-soda-lime type that are actually produced as tempered glazing. When considering the risk of breakage, the next step consists in considering another important property of the material in this context, that is, its ultimate stress sf at rupture or, say, the stress at which the material will break. As we shall see in Chapter 7 ceramics (and indeed glass) show statistical fracture. We consider here an average or representative stress at which such articles break. Then under thermal shock, breakage will happen when the thermal stresses reach the ultimate stress. This condition is written sf ¼ CaEDT

ð2:2aÞ

2.4 Performance Indices

or forming members without units: sf =E ¼ CaDT

ð2:2bÞ

where sf/E is the strain at fracture for a brittle material (see Section 7.2). Fig. 2.9 plots sf/E as a function of thermal expansion coefﬁcient a again using logarithmic scales for both axes. This presentation allows one to show resistances at a given thermal shock amplitude DT as straight and parallel lines. Again materials shown on the same line have the same thermal shock resistance. For instance, the materials shown on the 100 8C straight lines resist a thermal shock of amplitude less than or equal to 100 8C. The materials showing larger resistance are those appearing on the left and upper part of the ﬁgure. This ﬁgure shows also that the different groups of materials locate at separate places even though partial overlapping is observed. Again, overlapping of composite and metals groups is not unexpected. Oxide glasses match the ceramics group again. As expected from the a–E chart, materials show a very broad range of resistance. Ceramics cover a 10–1000 8C domain while glasses cover a reduced domain ranging from 50 to 300 8C. Different performance indices (combining relevant properties) allow optimization of materials selection for a given application employing Table 2.5. An important parameter is the cost which can be combined with density.

Fig. 2.9 Chart for thermal shock resistance showing sf/E as a function of thermal expansion coefﬁcient a (according to Ashby, 2001).

17

18

2 Glass, A Ceramic Material Performance indices for mechanical design (after Ashby, 2001). Parameter C is the cost per kg (see also Chapter 12).

Tab. 2.5

Function, objective and constraint

Index

Window, maximum thermal shock resistance Tie, minimum weight, stiffness prescribed Beam, minimum weight, stiffness prescribed Beam, minimum weight, strength prescribed Beam, minimum cost, stiffness prescribed Beam, minimum cost, strength prescribed Column, minimum cost, buckling load prescribed

sf/Ea E/r E1/2/r Y2/3/r E1/2/Cr Y2/3/Cr E1/2/Cr

2.5 Shape Factors in Mechanical Design

We shall see that, besides choosing the right material, it is also important to select the right shape to produce the manufactured object. Consider for instance a paper sheet placed vertically: it shows poor buckling resistance when compressed. Instead, when folded its resistance dramatically increases. Also, plastic chair legs are fold shaped. Fig. 2.10 shows a glass roof supported by long glass beams with rectangular section set in such a way that their larger side is vertical. As discussed in detail a rectangular section allows a much better mechanical performance than a square section. It is important to note that it is the elastic failure and not the brittle failure (Chapter 7) that limits the present structural application. In fact a single tempered beam with its larger side set vertically is able to support 12.5 tons under four-point bending before buckling happens (R. Gy, personal communication).

Fig. 2.10 Glass atrium at the top ﬂoor of the building at 53–55 Av. Georges V (Paris). The glass roof is supported by tempered and laminated glass beams. These have 2 19 mm2 sections, the larger side being set

vertically. The longer beam is approximately 7.1 m long. Architects: J.L. Robert, J.W. Wilmotte, P. Granger. The atrium at the 8th ﬂoor was designed to allow maximum daylight. (Courtesy R. Gy, Saint Gobain Recherche.)

2.5 Shape Factors in Mechanical Design

Both shape and materials selections should be carried out together since shaping depends on the type of material, e.g. ceramics are more difﬁcult to shape than metals. Let us concentrate on mechanics, which is the focus of the book, and more precisely now on the mechanical design that has been extensively reviewed by Ashby (2001). Several performance indices are listed in Table 2.5 according to the application. At this stage, these indices do not yet consider shape. Let us take an example to determine the performance index and determine how shape inﬂuences this performance. This will allow us to introduce the shape factor and hence understand how shape contributes to object strength. Let us consider a beam under ﬂexure (Figs. 2.11 and 2.12). We prescribe a given stiffness with minimum weight. The following expression holds (Fig. 2.12a): F IE ¼k 3 d l

ð2:3Þ

where F is the load, d the displacement of the beam centre, l the distance between supporting points (all ﬁxed by the customer), E Young’s modulus and I the second Ð moment (I ¼ section y2 dA, where y is the distance from axis and dA the related surface at distance y). For a square section of area b2, the second moment is ð I¼

b=2 ð

y dA ¼ 2

section

y2 bdy ¼ b=2

b 3 b=2 b4 y b=2 ¼ 3 12

and Eq. (2.3) is written F k b4 E ¼ d 12 l3

Fig. 2.11 Tempered glass beam under ﬂexure (four-point bending). For the experiment here, the larger side is set horizontally. This set-up was used to determine the delayed elastic response (Gy, 1999; see also Chapter 6. Courtesy R. Gy, Saint Gobain Recherche.)

ð2:4Þ

19

20

2 Glass, A Ceramic Material

Fig. 2.12 (a) Beam under elastic ﬂexure; (b) two beams with identical section area but different shape.

The mass of the beam is simply M ¼ rlb2

ð2:5aÞ

and with Eq. (2.4) is 1=2 F 12 l3 M ¼ rl d k E

ð2:5bÞ

This can be rewritten, separating the geometrical characteristics and the material properties, as M¼

F 12 3 1=2 r l d k E 1=2

ð2:5cÞ

For a given application, mass is then minimized when E 1=2 r

ð2:6Þ

is maximized. This ratio is called the performance index. Note again that shape is not considered until now (or assumed to be the same up to this point).

2.5 Shape Factors in Mechanical Design

As we shall see now, shaping the beam allows one to improve further the performance. Let us still consider a beam under ﬂexure but now consider two different but simple shapes for the beam (Fig. 2.12b) with the same section b2. One of the beams has a square cross-section (already studied) while the second has a rectangular cross-section, its smaller side being set horizontally. In fact, when the beam is set on its larger side then the ﬂexure performance is poorer; this can be easily shown using the method described now or experienced in everyday life. The second moments are I ¼ b4 =12

ð2:7aÞ

and I0 ¼

ð

ðb y2 dA ¼

section

b

b b b b4 y2 dy ¼ y3 b ¼ 2 6 3

ð2:7bÞ

for the square and rectangular section respectively. Equations (2.3) with (2.7b) show that the rectangular shape offers stiffer response. Calling f ¼ I 0 =I

ð2:8Þ

the shape factor (f ¼ 4 in the present case) and using the same procedure as before shows that the performance index transforms into ðfEÞ1=2 r

ð2:9Þ

This shows a square dependence on shape factor (in the present case performance is then twice as high for the elongated beam). Therefore, the shape of the beam is expected to play an important role in mechanical design. The performance can be considerably improved when using an elevated shape factor. As mentioned before, shaping has materials constraints. Then, one has to consider all required performance factors (co-selection). Shape should be considered at different scales: (i) at the macroscopic level (glazing, glass beam shape, arrangement and placing to be optimized for different applications (buildings, vehicles)); and (ii) at the microscopic scale (the arrangement of glass ﬁbres in glass wool, in a composite or in a mat is to be optimized). In fact, there is still R&D effort towards optimizing glass wool recovery. When glass wool is produced, it is packed and stored under different environments. Glass wool recovery on unpacking is essential to allow maximum insulation and hence performance and this recovery will depend on the ﬁnal arrangement of glass ﬁbres. The study of the mechanical response of entangled glass ﬁbres is complex and still the subject of ongoing research (Durville, 2005; Bergonnier et al., 2005).

21

22

2 Glass, A Ceramic Material

Ashby (2001) proposed the use of charts to predict shape inﬂuence and determine the gain that can be achieved. Let us consider again the loaded beam under ﬂexure as an illustrative example. The method is the following. A simple mathematical operation consists in dividing both parts of Eq. (2.9) by f so that ðfEÞ1=2 r

ð2:10Þ

transforms into ðE=fÞ1=2 E 1=2 ¼ r=f r

ð2:11Þ

Then the charts can be used to select ‘shaped materials’ that are placed on the chart as artiﬁcial ones at coordinates E ¼ E/f and r ¼ r/f. A shaped material is positioned relative to the unshaped one on the chart as shown in Fig. 2.13. As expected a shaped material offers a better performance than an unshaped one. In fact, on this chart, the performance index E1/2/Cr that corresponds to a beam with minimum weight and stiffness prescribed is represented by lines of slopes þ2 (as usually the performance is identical on the same line). It is then observed that the shaped material is positioned towards the left and bottom side as compared to the unshaped one. The magnitude of

Fig. 2.13 Young’s modulus–density chart (according to Ashby, 2001).

2.5 Shape Factors in Mechanical Design

the achieved improvement can be predicted plotting the (E, r) position. Interestingly, composites like wood having natural microshapes show the best performance for the designed beam. Shaping engineered materials allows one to approach the domain covered by natural or biomaterials as illustrated in Fig. 2.13. In fact, bio-inspired materials have become an important ﬁeld of research (so-called biomimetic materials) since great gains in performance are expected.

23

25

3 Glass Prehistory and History 3.1 Natural Glasses

Natural glass has existed since the beginnings of time, formed when rocks melt as a result of high-temperature phenomena such as volcanic eruptions, lightning strikes or the impact of meteorites, and then cool and solidify rapidly enough so that a liquid-like structure can be frozen in glassy state (see Fig. 5.15). Rocks can be classiﬁed according to the way they form either from sediments or eruptions (Dejean-Arrecgros, 1978). The compositions of volcanic rocks do not differ signiﬁcantly from sedimentary ones contrary to their respective thermal histories. It is well known that glass formation is a kinetic phenomenon (Chapter 6; Tammann, 1925). Most well-known natural glass is obsidian that is believed to be one of the ﬁrst glasses that appeared on earth at least 40 million years ago. Such an impressive age demonstrates that the vitreous state may be resistant in the long term against devitriﬁcation and water corrosion (Fig. 3.1; more images can be viewed at http:// www.musee.ensmp.fr/gm//lettres.htm, refer also to Sedgwick Museum of Earth Sciences collection, Cambridge U.K.). Glass utilization would have started when stone-age people became aware of the strength and sharpness that could be obtained from obsidian. Stone-age humans (75 000 BC, long before humans learned how to make glass) are believed to have formed (here form means mechanically, not thermomechanically) and used cutting tools and arrowheads made of obsidian. The formation of natural glasses may happen under three main conditions, the ﬁrst two corresponding to a compromise between the glass composition (viscosity regime) and the cooling conditions (as discussed in more detail in Chapter 5): i. Magmatic formation: the silicate (silica-rich) melt being rejected from earth’s mantle at the surface by volcanic activity cools down at rates scaling from 1 8C per minute to 1 8C per month (Chapter 5). ii. Metamorphic formation: these conditions correspond to extremely fast heating and cooling of rocks and melts (1 8C per second) during impact, friction or lightning. Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

26

3 Glass Prehistory and History

Fig. 3.1 Obsidian. (Copyright Ecole des Mines de Paris.)

iii. Sedimentary silica gel may be formed after drying over large periods of time scaling from years to thousands of years. Also natural biological glass forms sponge (Fig. 3.2, refer also to University Museum of Zoology, Cambridge U.K.) and mollusc skeleton and shell (Sundar et al., 2003). These mild synthetic conditions have inspired sol–gel science (see Chapter 12). Figure 3.3 shows the composition ranges of natural glasses together with humanmade glasses according to the relative concentrations of formers, modiﬁers and amphoteric ions (see Chapter 5 for precise deﬁnitions). The classiﬁcation is based on the way the ions participate in the glass network (forming the network or modifying it, amphoteric being intermediate). Such a diagram is very instructive since it shows that the chemical domain occupied by industrial glasses separates dramatically from the one occupied by natural glasses. The relation between network modiﬁers,

Fig. 3.2 Silica glass sponge; scale bar is 5 cm. (Reprinted from Sundar et al., 2003, with permission from Macmillans Publishers Ltd.)

3.1 Natural Glasses

Fig. 3.3 Compositional ranges of manufactured and natural glasses. Network modiﬁers: Li, Na, K, Ba, Ca, Mg, Fe2+, Pb, Zn; network formers: Si, P, B; amphoteric or intermediate ions: Al, Fe3+. (According to Heide et al., 2003.)

network formers and intermediate oxides is indeed much different since industrial glasses have more network modiﬁer than natural ones. The majority of natural glasses are peraluminous (Al2O3 > Na2O þ K2O þ CaO) whereas human-made glasses are peralkaline (Al2O3 < Na2O þ K2O þ CaO) in terms of geosciences. Magmatic glasses (obsidian; Table 3.1) tend to be silica-rich and contain less than 10 % of alkaline. Their dark colour is due to iron oxides. Their purity and elevated viscosity allowed for the natural production of these glasses. Notably on the Moon, eruptive glasses form more easily because of the absence water, which leads to the induced elevated viscosity. Magmatic glasses can be found in Iceland, the Canaries and Wyoming. Premise stones have compositions close to that of obsidian, while Typical glass compositions of natural and manufactured glasses. Natural (magmatic: obsidian; metamorphic: australite, lunar glass) (weight percent, E and S glass fibre for composites).

Tab. 3.1

Glass

SiO2

Obsidian Australite Lunar glass Egypt (1500 BC) Italy (9000 BC) Container glass Glazing Glass wool Nonex Pyrex E glass (ALS) S glass

74.6 70.4 54.5 67.8 77.8 67–70 71–73 65 73 80.5 54 65

B2O3

4.5 16.5 12.9 10.0

Na2O

K2O

4.0 4.7 1.6 2.5 0.1 n1). The light beam follows Descartes’ law with reﬂection at the refractive index interface.

moisture and contact by hermetic coatings which are deposited during the sizing step (Chapter 10). As a matter of fact, ﬁbres offer exceptional stxrength and optical performance that have yield such an impressive development in communications. One drawback of glass when considered for lenses is its density, and load gains are accomplished by controlling better glass distribution (Section 4.2). It should be noted that nowadays spectacles are made of organic glasses. These allow load gains and comfort. Organic glasses are polymers formed by long organic chains (similarly, chalcogenide glasses are constituted of Se chains, their applications being described below). One single spectacle lens is composed of several layers, some of these being

Fig. 4.9 Transmission of ‘infrared’ glasses compared to silica. BIG is a multicomponent ﬂuoride glass based on BaF2, InF3 and GaF3. TeX is a multicomponent chalcogenide glass based on the combination of Te, Se and I2 (according to Lucas, 1999). Observe the huge changes in the IR window.

47

48

4 Applications of Glass

only protective because of the poor scratch resistance of polymers as compared to glass (Chapter 8). More recently chalcogenide glasses have been proposed for application in IR vision (they are also used for DVD-RW taking advantage of their laser-induced glass– ceramic transition). In fact these glasses formed with group VI atoms associated with either group IV or V atoms (Appendix 2) allow for improved transparency in the IR domain (Appendix 1; 8–12 mm wavelengths, Fig. 4.9). This leads to application for night observations, detection of thermal loss in buildings and in situ medical observation (Lucas, 1999). These glasses while showing ‘plastic’ behaviour remain very brittle at room temperature (Guin et al., 2002; see Chapters 7 and 8). Hence, there is an important demand for improving the contact resistance and hence extending their future applications.

4.4 Glass Fibres for Insulation and Reinforcement

The glazing, packaging and optical applications of glass are the most well known since they refer to glass transparency. Glass is also used for thermal and acoustic insulation or to reinforce plastics (Figs 4.10 and 4.11) and concrete (CEM-FIL1) because of their low cost and high strength. In the latter case, compositions incorporating ZrO2 allow to resist concrete chemical attack. Polymers reinforced by glass ﬁbres are fabricated as composites and used in transportation applications (automotive front ends, vehicle furniture, plane cockpits, etc.). As discussed in Chapter 2, composite properties are a mix of those of the constituent parts, sometime in a complex way. In the simplest case a rule of mixture of properties may be employed in a linear form: P ¼ f1P1 + f2P2, where fi are the volume fractions of each component (glass and polymer in the present context). It allows

Fig. 4.10 (a) Glass wool (copyright Saint-Gobain) and (b) ﬁbre-reinforced composite used for the front end of an automobile.

4.5 Abrasive Tools

Fig. 4.11 Glass mats: (a) Saint-Gobain Uniﬁlo1 and (b) Multimat formed by E-glass ﬁbres.

tailoring stiffness (Fig. 2.6) and load gains that are attractive for transportation and in particular for airplanes since, for instance, saving a mass of 1 kg on commercial planes increases the travelled distance by about 1 mile (Gay, 1997). Moreover as discussed later in the book (Chapter 7), ﬁbres can be produced with much higher mechanical strength than any glazing. This makes the ﬁbres very attractive for improving composite strength. Glass wool is produced for buildings and vehicles and forms an air–ﬁbre composite. Notably, the glass composition is tailored accordingly for different applications (Table 4.1; Chapter 5). Wool ﬁbres have been optimized to allow maximum recovery when unpacked and set (Chapter 2). Also, their dissolution in vitro has been of utmost importance since the problems generated by asbestos (see water diffusion and hydrolysis of siloxane bonds, Chapters 5 and 7). Biodegradable glass ﬁbres have been developed accordingly (Chartier, 1997).

4.5 Abrasive Tools

Abrasive applications are not so well known. Glass can be used as a bond between abrasive grits to fabricate cutting tools. Glass composition is then tailored to obtain grit wetting and a strong grit–glass interface (Alliche and Le Bourhis, 2000). Figure 4.12 shows different grinding wheels composed of grits (alumina, silicon carbide) that are bonded together by a glass matrix. A scanning electron micrograph shows different grey contrast for the grits and bonds (Fig. 4.13). Note the elevated porosity of such a wheel. In fact, porosity is required for cooling and evacuating the metal chips generated when tooling a piece (Coes, 1971; Malkin, 1989; Tawakoli, 1993; Alliche and Le Bourhis, 2000). For high-speed grinding operations, wheels are made of a metal core (with high thermal conductivity) and abrasive segments ﬁxed at the wheel circumference.

49

50

4 Applications of Glass

Fig. 4.12 Vitriﬁed bonded abrasive wheels. (Copyright Saint-Gobain.)

Fig. 4.13 Scanning electron micrograph of a vitriﬁed bonded abrasive.

4.6 Glass Manufacturers

Some well-known glass manufacturers are listed below, subdivided into the applications reviewed above.

4.6 Glass Manufacturers

i. Flat glass: Saint Gobain (France), Guardian (USA), Pilkington (UK), PPG (USA), Glaverbel (USA), Asahi (Japan), Schott (Germany). ii. Packaging: Saint Gobain (France), BSN Glasspack (USA), Anchor Glass (USA), Owens Illinois (USA), Rexam, Vitro (Mexico), Gerresheim (Germany, USA), Pochet (France), Rocco Bormioli (Italy), Wheaton (USA). iii. Optical glass: Heraeus (Germany), Schott (Germany), Corning (USA). iv. Glass wool: Saint Gobain (France), Amstrong (USA), Johns Manville (USA), Owens Corning (USA), Rockwool (EC), Uralita (EC). v. Reinforcing ﬁbres: Saint Gobain (France), Johns Manville (USA), PPG (USA), Owens Corning (USA), Nottobo, Porcher. vi. Abrasives: Saint Gobain1) (France), Asahi (Japan), Noritake (Japan), 3M (USA), SAIT (Italy), SIA (Switzerland), Tyrolit (Austria). Note that none of the manufacturers are present in all six main domains. As a matter of fact, each domain requires speciﬁc know-how and tools.

1)

Winter, Unicorn and Norton are now part of Saint Gobain group.

51

53

5 Glass Structure 5.1 Introduction

Glass structure is out of equilibrium. It is obtained when a liquid is cooled down in such a way that on passing the melting temperature or liquidus temperature (TL), ‘freezing’ happens instead of crystallization (Tammann, 1925). The ﬁnal temperature must be so low that molecules or atoms move too slowly to rearrange to the more stable crystalline form. In Chapter 6 we shall discuss extensively the atomic mobility in terms of viscosity. In particular, we shall see that glass structure may depend upon thermal history. For instance, a liquid will yield denser glasses when the cooling rate decreases. This chapter shows the prominent characteristics of glass disordered structure. Alternatively, glass can be built up onto a substrate, either by deposition or chemical reaction from the vapour, the substrate being cold enough that rearrangement cannot take place. In fact, although they are named differently, amorphous silica (a-SiO2) ﬁlms and silica glass bulk are the same materials having the same chemical composition and a random network. Ryu and Tomozawa (2006) suggest that the concept of ﬁctive temperature can be used to describe a-SiO2 ﬁlm structure as well (see also Chapter 6). However, amorphous layers have been achieved with a limited number of substances as compared to the usual route (Doremus, 1994). Many deﬁnitions of glass have been proposed: we shall use the most commonly used one that deﬁnes it as an amorphous solid showing a glass transition (Zarzycki, 1982). The glass is frozen in a structure showing only short-range order that makes its characterization quite difﬁcult as compared to crystalline structure that presents long-range order (periodical structure with the repetition of a unit cell; see also Table 2.3). As discussed below, diffraction experiments on glasses yield results that most closely resemble those of liquids (see also Chapter 2).

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

54

5 Glass Structure

Let us start with silica and related glasses because of their practical importance and the well-documented literature.

5.2 Silica Glass and Related Glasses 5.2.1 Glass Network

Silicon (Si) is in group IV of the Mendeleev table (Appendix 2) and tends to bond to four different oxygen (O) atoms. Note that what is described here applies as well to germania glasses changing Si into Ge. Hence, each oxygen atom is shared by two silicon atoms. In three dimensions (3D), Si and O atoms arrange to form oxygen tetrahedral elements with a Si atom at the centre (Fig. 5.1). This is in terms of chemistry the resulting bonding through four sp3 hybrid orbitals of silicon and two 2p orbitals of oxygen atoms (see also Appendix 2). Then the structure can be thought of as built up by the sharing of corners by pairs of these oxygen tetrahedra. Two tetrahedra meet at only one corner, but all corners of all tetrahedra are actually shared. This is shown in Fig. 5.2 for the crystalline and glass form of SiO2. Interestingly, a very open 3D structure may then be built in many ways, in which the Si–O–Si lines may or may not be straight. One observes rings of atoms of different sizes when a disordered structure is generated (this will be more obvious in 2D). In fact, it is helpful to project the structure on a surface where tetrahedra become triangular elements. One can also consider the projected glass as an imaginary 2D oxide Si2O3 (Jones, 1956). In such a 2D projection of the network we shall shift from a perfectly ordered structure to a disordered one (Fig. 5.3). Figure 5.3a shows again the crystalline projected structure of SiO2 (quartz) while Fig. 5.3b shows the continuous random network (CRN), or a network without periodicity illustrated now in 2D and ﬁrst proposed for silica glass by Zachariasen (1932). It is observed in both structures that oxygen atoms are bonded to two silicon atoms forming Si–O–Si chains. Figure 5.3a reveals a long-range order characteristic of a crystalline solid (repetition in space of a unit cell). In fact, any atom’s position can be predicted in this ordered structure. Figure 5.3b shows instead only a short-range order that is in great contrast with the 2D projection view of Fig. 5.3a. In fact, it reveals no long-range order any more while the structure still respects the stoichiometry

Fig. 5.1 Elemental tetrahedron, Si (group IV) bonds to four O.

5.2 Silica Glass and Related Glasses

Fig. 5.2 SiO2 structure: (a) crystal form; (b) glassy form. An elemental tetrahedron is shown in each case (dashed lines).

since all oxygen atoms are bonded to two silicon atoms forming Si–O–Si bonds. The atomic arrangement cannot be predicted any more in the latter case. One further observes the existence of rings with a different number of bonds. It seems from modelling that smaller rings would appear on cooling glass rapidly or, say, so-called network polymerization would be affected by thermal history (Ito and Taniguchi, 2004). In fact, the glass structure is known to be determined by its past thermal history and this phenomenon will affect the details of the structure and the structural relaxation as discussed extensively in Chapter 6.

55

56

5 Glass Structure

Fig. 5.3 2D projections of structures showing the path from crystalline to glassy structure: (a) crystalline form of SiO2; (b) glassy form of SiO2; (c) glassy form of SiO2 modiﬁed by Na+ ions. Note the presence of one NBO per Na+. The projection of a tetrahedron is shown in each case (dashed lines).

5.2 Silica Glass and Related Glasses

Fig. 5.3 (Continued )

5.2.2 Glass Network Modiﬁcation

In Fig. 5.3c the CNR is shown this time when sodium oxide is added to the structure (or more generally an alkaline or an alkaline earth oxide). Na+ is called a modiﬁer since when added to the glass it modiﬁes the Si–O network. Na+ ions are charged with an elemental positive charge þe and each of them are compensated by the formation of one non-bridging oxygen (NBO) atom that holds a negative charge e. Therefore, in a glass containing modifying ions, NBO atoms appear (as opposed to bridging oxygen (BO) atoms which form the network). Figure 5.3c shows additionally that two Na+ ions are necessary for compensating the charges generated by the rupture of one O–O bond (one Na+ ion compensates one NBO). The two tetrahedra still interact electrostatically. In fact, electrostatic interactions exist between the two NBO atoms and the two Na+ ions. As revealed experimentally however, glass network modiﬁcation induces a viscosity decrease or a greater facility for viscous ﬂow. CRN model accounts quite well for the observed change in properties as the glass composition is modiﬁed. Modiﬁers disrupt the network and are used in fact to lower the viscosity of the glass melt and hence to facilitate its fabrication at lower temperatures (Chapter 6). In fact, silica glass is difﬁcult to process and instead of standard melting procedure (Chapter 10) it is produced following ceramic routes. The melting temperature of silica is as high as 1713 8C corresponding to cristobalite–liquid equilibrium. Instead, adding 25 % of soda to silica lowers the liquidus temperature to only 793 8C (Jones, 1956). Alkali metal ions like Naþ are mobile and allow for electrical conductivity, ion

57

58

5 Glass Structure

migration. In contrast, alkaline earth ions like Ca2+ ions (one alkaline earth ion is compensated electrically by two NBOs) are relatively immobile and can hinder the diffusion of other ions, in particular alkali, and hence improve the chemical resistance of the glass (see also Section 5.8). It is then clear why most important commercial glass, SLS glass, is based on a mixture of silica (network former), sodium and calcium oxides (alkaline and alkaline earth modiﬁers respectively). As expected then, the relative concentration of bridging and non-bridging oxygen atoms has an important inﬂuence on the properties of glasses (Kurkjian and Prindle, 1998; De´riano, 2002). Let us call BON the number of bridging oxygen atoms in a tetrahedral element; we can anticipate the following rules: i. For BON ¼ 4, that is [O]/[Si] ¼ 2 since each BO is shared by two silicon atoms, the network is a three-dimensional one with all four corners bridging. ii. For BON ¼ 3, [O]/[Si] ¼ 2.5, the network is two-dimensional with three corners bridging (note that some tetrahedra may be linked to four others and some therefore to less than three, the said number being the average value over the network). iii. For BON ¼ 2, [O]/[Si] ¼ 3, the network is formed by one-dimensional chains with one corner bridging. iv. For BON < 2, [O]/[Si] > 3, the network is composed of individual SiO4 tetrahedral elements, some of these being bound together. Using Qx terminology with x the number of bridging oxygen atoms on a tetrahedron, we refer to (i) Q4, (ii) Q3, (iii) Q2 and (iv) Q1, Q0 structures respectively. The stiffness of the network decreases gradually by replacing the bridging oxygen atoms by non bridging ones until only individual isolated tetrahedra remain. Consider a modiﬁed oxide glass of general composition (A2O)x(SiO2)1x with A the alkali metal.TheconcentrationofBOandNBOvarieswithxasshowninFig.5.41).Forx ¼ 0,thatis for pure silica, only BO exist (Q4), the relative concentration being then 2, while increasing alkali concentration yields a dramatic decrease of BO and an increase of NBO accordingly. Dietzel (1942) proposed classifying the oxides according to their ability to form or modify the glass network in view of their cation ﬁeld. He deﬁned the cation ﬁeld intensity A as a charge-to-distance squared ratio: A¼

Z ðrc þ ro Þ2

ð5:1Þ

where Z is the cation valence and rc and ro are the cation and oxygen radii respectively (Appendix 2). The Dietzel ﬁeld amplitude varies within a relatively broad range of 1.2 to 0.1 (Table 5.1) and is indicative of the magnitude of the electrostatic attractive force 1)

Introducing x A2O yields 2x NBO. The total number of oxygens is x + 2(1 x). Hence introducing xA2 O leaves xþ2ð1xÞ2x ¼ ð23xÞ NBO. ½NBO=½Si¼2x=ð1xÞ. ½BO= ½Si ¼ ð23xÞ=ð1xÞ.

5.2 Silica Glass and Related Glasses

Fig. 5.4 Relative concentrations of bridging oxygen (BO) and non-bridging oxygen NBO as a function of x in a modiﬁed silica glass of general formula (A2O)x(SiO2)1x.

between the considered element and oxygen (Appendix 2). The ordered sequence of oxides is relatively convincing, since for A > 1 we ﬁnd the oxides that form the glass network while for A < 0.35 the oxides (alkali in particular) are known to modify the network. Between these two extreme behaviours, intermediate oxides may show both behaviours according to the glass composition (Table 5.1). Dietzel’s approach suggests that both smallness and high charge of the cation favour the formation of glassy oxides. Too much importance must not be attached to one criterion or another (for instance single bond strength to heat of dissociation ratio). These are mostly empirical and break down when structures are unusual, as in As2O3 and PbO for instance (Jones, 1956). Also the situation is very complex when weak VDW bonds coexist with strong covalent bonds as in chalcogenide glasses (Section 5.4). Besides decreasing the viscosity, modiﬁers allow for the liquidus (or melting) temperature to decrease to a more viscous domain and hence favour glass formation Tab. 5.1

˚ ). Dietzel field intensity and role of cations in glass (r0 = 1.4 A

Role

Cation

Z

˚) rc (A

A

Network formers

Si B Ge Ti Al Zr Be Mg Zn Ca Pb Li Na K

4 3 4 4 3 4 2 2 2 2 2 1 1 1

0.4 0.25 0.53 0.74 0.53 0.86 0.41 0.86 0.88 1.14 1.33 0.90 1.16 1.52

1.23 1.10 1.07 0.87 0.80 0.78 0.61 0.39 0.38 0.31 0.27 0.19 0.15 0.11

Intermediates

Modiﬁers

59

60

5 Glass Structure

Fig. 5.5 Modiﬁed random network as proposed by Greaves (1985) showing Si-rich zones connected by modiﬁer-rich percolating channels marked in grey.

(Barton and Guillemet, 2005). Alkali metal ions (Li, Na, K, valence 1) are more efﬁcient than alkaline earth ones (Ca) for inducing both effects. Pb, while being classiﬁed as a modiﬁer, allows fabrication of glass associated with only 8 wt% of silica. This supposes Pb atoms are forming the network while bridging two oxygen atoms. This question is still open and under debate. Alumina modiﬁes the silica network (decrease of the viscosity); when introduced with alkali metal, Al may participate in network formation with a related increase of the viscosity. More recently Greaves (1985) introduced a modiﬁed random network where modiﬁers form zones connecting silica-rich volumes as shown for a modiﬁed silica glass in Fig. 5.5. This model offers interesting predictions and suggestions as regards the plastic deformation of silicate glasses. It can be anticipated that such glasses would preferentially ﬂow through modiﬁer-rich zones (see also Chapter 8 and Appendix 10). 5.2.3 Short-Range Order

Short-range order can be investigated using techniques like X-ray and neutron diffusion, some results being discussed in more detail below. X-ray diffraction was among the ﬁrst techniques allowing for detailed insight into glass structure. It remains a tool of utmost importance allowing for the detection of residual crystallites. Mathematical analysis of the glass response allows extraction of the radial atomic distribution of a given atom as detailed below. Neutron diffraction gives the same information as X-ray diffraction but allows for

5.2 Silica Glass and Related Glasses Tab. 5.2

Experimental tools and associated information.

Experimental tool

Information

X-ray or neutron diffraction IR and Raman spectroscopies, MNR EXAFS X-ray photoelectron spectroscopy (XPS) X-ray reﬂectometry

Radial distribution and/or crystal phase Local symmetry, coordination Local symmetry, radial distribution, coordination Surface arrangement (Section 5.8) Surface arrangement (Section 5.8)

penetrating deeper into specimens. Neutron diffraction requires a nuclear reactor. More recently, extended X-ray absorption edge ﬁne structure (EXAFS) has been extensively used to extract coordination numbers and interatomic spacings. The power of this technique is that by selecting the X-ray energy, the structure around a single kind of atom can be explored rather than getting composite information involving all kinds of atoms as for Xray diffraction. Also, infrared (IR) and Raman spectroscopies (Chapter 8), magnetic nuclear resonance (MNR, including ‘magic angle spinning’ improvements), paramagnetic electronic resonance (PER) and Mo¨ssbauer spectroscopy (Zarzycki, 1982; Williams et al., 1997) are employed to get further insights into local symmetries, coordinations and ion environments. The last two techniques listed in Table 5.2 are very important as regards surfaces. In fact, a glass surface is transformed by water and alkali diffusions depending on the environment and the atmosphere. As a result, glass surfaces may show very different structures and properties as compared to the glass bulk. With the nanotechnology breakthrough, the surface structure and its related properties become of utmost importance and have attracted much scientiﬁc and technological interest. Let us consider X-ray or neutron diffraction. The results of such experiments are usefully presented in terms of a radial distribution where we select an atom at random and consider a series of concentric spheres around it (Fig. 5.6). From the experimental spectra, the radial distribution (RD) can be extracted in the form (Fig. 5.7) RDðrÞdr ¼ 4pr 2 rðrÞdr

ð5:2Þ

where r(r) is the density at distance r. RD(r) corresponds to the probability of ﬁnding a neighbouring atom at the distance r from another atom the position of which is

Fig. 5.6 Schematic glass structure centred on a given atom.

61

62

5 Glass Structure

considered arbitrarily as the reference (r ¼ 0). For a crystal (Chapter 2), the radial distribution would exhibit sharp peaks at periodic distances. Instead in a glass one observes: (i) at small distances diffuse maxima with expected deviation in bond angles and bond lengths, the area under the peak being indicative of the coordination and (ii) at long distances (r ! 1) RD(r) converges to the mean distribution, that is, 4pr2ro, where ro is the average density of the considered glass2). This is indeed observed in Fig. 5.7 since glass RD converges towards a parabolic evolution at long distance with less and less characteristic features being observed. At short distance, RD peaks are observed corresponding to the short-range order of the glass. For instance, in silica (Fig. 5.7a) we observe that silicon atoms are bonded to oxygen atoms at a distance of about 0.16 nm while the distance between two silicon atoms (pertaining to two different tetrahedra) is about 0.32 nm, that is, about twice the previous value, indicating that Si–O–Si lines pﬃﬃﬃﬃﬃﬃﬃare ﬃ not very far from collinear. In between, the O–O band is detected at about 8=3 times the Si–O distance, as expected in a tetrahedral arrangement. After about ﬁve interatomic distances, order almost vanishes, conﬁrming the view that no long-range order prevails in a silica glass. The radial distribution of soda-silica glass shows similar information for Si–O and O–O distances being almost unaffected (Fig. 5.7b). A new peak appears corresponding to the Na–O distance (Jones, 1956). This suggests that the Na ions occupy the free space left in the silica open structure. This view is supported by the fact that the density of silica increases when soda is incorporated, while gas permeability decreases (at least by 5 decades in soda-rich glasses; Jones, 1956; see also Appendix 13). Obviously, we do not suggest that Na+ ions simply ﬁll network holes, for at the same time we must consider a change in the number of silicon and oxygen atoms. The short-range order of the glass will control the density or the atomic packing density Cg of the glass that has an important role in glass properties (elastic modulus, Poisson ratio, glass ﬂow). As for a crystalline structure the atomic packing density Cg is deﬁned as the ratio between the minimum theoretical volume occupied by the ions and the corresponding effective volume of the glass. For a glass of composition AaBb, Cg is written Cg ¼

ava þ bvb ava þ bvb ¼ rN aMA þ bMB a MNA þ b MNB =r

ð5:3aÞ

Here r is the glass density, N the Avogadro number, Mi the molar mass and vi the theoretical ion volume: 4 vi ¼ pri3 3 where ri is the ion radius (Appendix 2). 2)

For a gas of non-interacting point particles (structureless) the curve would be a parabola with its vertical axis and its apex at the origin. The probability of ﬁnding a second atom at a given distance from a ﬁrst one is dependent only on the volume available, and therefore varies with the square of the distance. For a perfectly ordered crystal, it

ð5:3bÞ

consists of a number of vertical lines of inﬁnite height, one at each of the possible interatomic distances (depending on the structure type). A hump above the parabola is indicative of a more than random probability of ﬁnding a second atom within a given range of distances from the chosen atom that is a degree of order.

5.2 Borate Glass and Related Glasses

Fig. 5.7 Radial distribution curves of (a) vitreous silica and (b) Na2O–SiO2 extracted from X-ray diffraction data (according to McMillan, 1979).

Silica glass packing density Cg is 0.45 and is lower than that of standard ﬂoat glass (Cg ¼ 0.52; Rouxel, 2006) both being below that of a crystalline structure where the highest atomic packing density is obtained for a face centred cubic (FCC) structure and is 0.74. As discussed below, metallic glasses show the highest atomic packing density greater than 0.7. The Poisson ratio increases accordingly from 0.2 for silica glass to 0.4 for metallic glasses (Appendix 9). Hence, silica and related glasses show excess volumes that have important consequence on the properties (transport, mechanical; see Chapter 6). Metallic glasses as compared to other glasses show the lowest excess volumes.

63

64

5 Glass Structure

5.3 Borate Glass and Related Glasses

Boron (B) is in group III of the Mendeleev table (Appendix 2) and is a network former with strong Dietzel ﬁeld (Table 5.1). It tends to bond to three different oxygen ions adopting a triangular coordination. Tetrahedral coordination is also found. As regards the three coordinated B atoms, it has been suggested that these form boroxyl groups B3O6. These groups are planar and linked to form a three-dimensional network by boron–oxygen–boron bonds (Fig. 5.8). Such a structure is in good agreement with X-ray diffraction results (Doremus, 1994). Such a structure is then much different from that of silica. When adding alkali metals to borates the induced changes are opposite to those generated in silica; this is called in the literature the ‘boron oxide anomaly’. In fact, the viscosity may increase and the thermal expansion decrease when adding alkali metal, contrary to what is generally observed in silicabased glasses. It is believed that such a trend could be related to a change in the coordination of boron atoms. Borosilicate glasses play an important role in glass manufacturing since they are corrosion resistant to water and allow for low thermal expansion. They are composed of Si and B atoms which form the network, Si being four coordinated and B three coordinated. The resulting network is softer than silica with lower viscosity and lower melting temperature. Contrary to what happens when modiﬁers are introduced in silica, the bond potential remains symmetrical in borosilicates inducing low variation in the mean distances with increasing temperature, that is, a low thermal expansion (see also Appendix 3). In borosilicate glasses, alkali metal ions like Na+ ions will either modify the network introducing NBOs or change the boron coordination (from 3 to 4). The latter phenomenon is believed to be responsible for the ‘boron oxide anomaly’ where viscosity may increase with increasing alkali metal concentration as stated for borate glasses.

Fig. 5.8 Boroxyl groups sharing a common oxygen atom.

5.5 Metallic Glasses

Fig. 5.9 Schematic structure of organic or chalcogenide glasses with chains and cross-linking.

5.4 Organic and Chalcogenide Glasses

Organic glasses are used to produce optical lenses and to protect glass articles (cold-end coatings, ﬁbre sizing; see also Chapters 4 and 12). They are formed by organic chains either cross-linked or not (Fig. 5.9). In thermoplastics only weak bonds (VDW) are formed between chains. In thermosets, cross-linking is obtained when covalent bonds form between the organic chains. The simplest polymer known as polyethylene is formed by long chains made of –CH2– moieties. The length of the carbon–carbon chain depends on the way the polymer is fabricated. Moreover, side group functions can be added to the carbon chains. When cooled from a melt, the polymer will generally present a mixture of very small crystalline regions embedded in a glassy matrix. The crystalline regions consist of oriented chains. Only when quenching is rapid enough, the chains cannot rearrange and a glassy phase is obtained. The chains form a glass three-dimensional network with strong (covalent) and/or weak (VDW) bonding between chains with related properties. Strong cross-links result in higher viscosity regime for instance. Interestingly, chalcogenide glasses can be described in analogy to organic glasses, the term polymerization being sometimes employed in the glass context as well. A chalcogenide glass is formed from group VI and IV atoms (GeSe for instance; Chapter 2, Appendix 2). Group VI atoms form long chains (Se chains for instance) interacting through VDW bonds and cross-linking due to the covalent bonding between the group IV atoms (Ge for instance). Note that Ge can bond four different chains (Guin et al., 2002) inducing strong network stiffness.

5.5 Metallic Glasses

Metallic glasses have been fabricated only recently. Duwez’s team pioneered in the 1960s elevated cooling rates (106 K s1) to fabricate binary glass compositions like AuSi glass (Klement et al., 1960). More recently more complex alloys of 4 to 6 different elements have been produced at much lower cooling rates (1 K s1) offering the possibility of producing larger specimens (so called bulk metallic glasses (BMGs); Johnson, 1996; Inoue, 2000). As a matter of fact, the actual structure of the alloys made with so many elements is complex (Fig. 5.10) as reviewed by Wang et al. (2004) and is still debated (Sheng et al., 2006). These glasses did not yield a technological breakthrough in terms of technological applications, even though they present more

65

66

5 Glass Structure

Fig. 5.10 Different atomic conﬁgurations of three types of BMGs (according to Inoue and Takeuchi 2002).

elevated elastic limit and corrosion resistance than crystalline metals. They have played an important role in the past decades in the study and understanding of glass mechanical properties since they can be plastically deformed as bulk (under compression) well below their glass transition (Appendix 10). This has allowed great insight into plasticity and ﬂow in glass (Chapters 6 and 8 and Appendix 8). BMGs were found to have a new type of glassy structure with a high degree of dense randomly packed atomic conﬁgurations with much smaller excess volume and higher packing density (Cg > 0.7) than in oxide glasses. Density measurements show that the density difference between BMG and the fully crystallized state is in the range 0.3– 1.0 % which is much smaller than the reported range of about 2 % for ordinary amorphous alloys (Wang et al., 2004). This indicates that BMGs have higher density randomly packed atomic conﬁgurations. Inoue classiﬁed the BMGs into three types: metal–metal type, metal–metalloid type and Pd–metalloid type alloys. The conﬁgurations are different according to the three types of BMGs shown in Fig. 5.10. Metal–metal alloys present icosahedral local order which after annealing may yield icosahedral quasicrystalline phase. Some authors have questioned the stability of these glasses during a stay at elevated temperatures when observing superplasticity (Nieh et al., 2002; Appendix 10). Metal–metalloid-type glassy alloys present network atomic conﬁgurations consisting of trigonal prisms which are connected with each other through ‘glue’ atoms comprising Zr, Nb, Ta or lanthanide metal. Pd-based BMGs consist of two large clustered units of a trigonal prism capped with three half-octahedra for the Pd–Ni–P and a tetragonal dodecahedron for the Pd–Cu–P region, as shown in Fig. 5.10.

5.6 Avoiding Crystallization 5.6.1 Nucleation and Growth of Crystallized Phases

As mentioned above, glass forms when a liquid is cooled down in such a way that ‘freezing’ happens instead of crystallization. In fact, the cooling rate must be large enough so that no appreciable amount of crystalline material is formed. It cannot be excluded that some glasses have crystalline regions. This issue is much debated today for metallic glasses (Appendix 10). The detection of crystalline phases is dependent on the

5.6 Avoiding Crystallization

Fig. 5.11 Nucleation n and growth g rates as a function of temperature; note the qualitative graph with arbitrary units (differing for n and g: n(T) is in m3 s1, g(T) in m s1).

tool employed (optical observation, electron microscopy, X-ray diffraction). If some crystals grow in the interior of a glass, the optical properties of the glass for instance will be changed. Light scattering will deleteriously affect the long-distance transmission of an optical ﬁbre for instance. Figure 5.11 shows the nucleation and growth rates which both depend on the temperature. Growth (g) starts at the melting or liquidus temperature TL. Nucleation (n) starts at a lower temperature (T2) resulting from the energy barrier wc that we calculate below. There is no barrier for growth, so it occurs at any undercooling. Hence, crystalline phases may appear in the critical zone situated between T2 and T3. Therefore, glass formation depends on the overlapping of growth (g) and nucleation (n) curves and on their respective kinetics as compared to thermal history (Zarzycki, 1982; Ashby and Jones, 1991). As will be illustrated below the viscous regime at these temperatures plays a very important role and the cooling rate amplitude will determine whether crystallites form or not. Modiﬁers allow for the liquidus temperature to decrease to more viscous domains hence favouring glass formation. The curves shown qualitatively in Fig. 5.11 can be described using a simple analytical approach described below. We shall consider a very simple glass constituted by only one type of atoms. Modelling becomes very difﬁcult in a more realistic case (Fokin et al., 2006). The methods allowing for reliable measurements of nucleation rates are also not straightforward (Doremus, 1994). The physics captured here will help obtain an insight into glass formation. 5.6.2 Nucleation of Crystallized Phases

Crystallite nucleation is controlled by thermodynamics. i. When atoms aggregate, a new surface is created between the emerging crystals and the embedding liquid requiring energy, while phase transformation from liquid to crystal provides energy to the process. We shall deﬁne wc as the energy necessary to form a particle that further develops into a crystallite. Below the critical energy wc, atoms aggregate and later separate. We shall develop in more detail below the expression of this energy barrier in simple conﬁgurations obtained for a monatomic melt in either homogeneous or heterogeneous nucleation regime.

67

68

5 Glass Structure

ii. The former phenomenon (i) will take place if particles can reach the nucleus passing through the diffusion barrier Dg0 . Correspondingly, nucleation rate can be expressed as a function of two terms showing energy barrier wc and diffusion barrier Dg0 respectively: w Dg 0 Nwc DG0 c exp ¼ nvE exp exp nðTÞ ¼ nvE exp kT kT RT RT

ð5:4Þ

where n is the concentration of atoms, vE the atomic transition frequency in the liquid (order of magnitude 1013 s1), T the temperature and N the Avogadro number. The ﬁrst term exp(Nwc/RT) regards the thermal activation related to the energy barrier wc for a particle to form as stated above. The second term exp(DG0/RT) is the diffusion contribution. In the case of a unique atom type, the vicinity of the particle always presents structural units to grow the particle. Therefore, no diffusion on long distances is necessary and the diffusion barrier is that appearing for the viscous ﬂow in the melt (DG0 ¼ DG; Chapter 6). We shall consider now two nucleation conﬁgurations to determine wc. The ﬁrst situation is when nucleation happens homogeneously within the liquid while the second situation (the most realistic one) is when nucleation happens at heterogeneities (at impurities or surfaces; Fig. 5.12).

5.6.2.1 Homogeneous Nucleation Considering ﬁrst the case of homogeneous nucleation, the energy of a particle w is the sum of two contributions: i. the liquid to crystal formation wf ii. the interface energy wi.

These two terms can be expressed as wf ¼

V 4pr 3 DGv ¼ DGv Vm 3Vm

ð5:5aÞ

where r is the particle radius (assumed to be spherical), DGv the molar enthalpy of the transformation from liquid to crystal and Vm the molar volume of the crystal, and wi ¼ 4pr 2 zsl

ð5:5bÞ

where zsl is the surface energy (at the interface between the solid s and the liquid l). Figure 5.12 plots w ¼ wf + wi as a function of particle radius r, and shows a maximum value for a particle radius of rc ¼ 2zsl Vm =DGv

ð5:6aÞ

The maximum energy is then determined to be wc ¼

16pz3sl Vm2 3DG2v

ð5:6bÞ

5.6 Avoiding Crystallization

Fig. 5.12 Schematic (a) homogeneous and (b) heterogeneous nucleation representations. (c) w(r) plot showing rc, wc maximum.

This maximum in energy wc sets a limit on size rc. When an aggregate reaches this critical size, it will develop further. Instead, below this critical size the atoms aggregate and further separate. Let us consider now the Stokes–Einstein relation to express the diffusion term. The diffusion coefﬁcient is written kT DG ð5:7Þ ¼ vE a2o exp D¼ 3pao h RT

69

70

5 Glass Structure

where a0 is the distance of the atomic jump (taken as twice the particle radius) and h the viscosity. Then, we get for the nucleation rate DG Nwc D Nwc exp ¼ n 2 exp nðTÞ ¼ nvE exp RT ao RT RT kT Nwc exp ¼n 3pa3o h RT

ð5:8Þ

We observe that there is balance between the contribution of wc decrease (DGv increases with decreasing temperature, it is zero at TL) and viscosity increase when temperature decreases. This corresponds qualitatively to the plot shown in Fig. 5.11 with an observed maximum between T2 and T4. 5.6.2.2 Heterogeneous Nucleation We consider now a more realistic situation where heterogeneous nucleation originates from solid impurities in the glass melt. Heterogeneous nucleation is to be prevented on forming a glass article. Instead, vitroceramics are fabricated introducing metallic impurities in the glass melt to induce heteronucleation as detailed in Section 5.7. In such a case, nucleation may happen much more easily as we will show below. We shall refer to impurities that help crystallization as catalysers. Let us calculate the energy barrier wc. In the case of heterogeneous nucleation three interfaces have to be considered instead of one. The mechanical equilibrium of a particle on the catalyser is given by the Young Dupre´ equation (Fig. 5.12; see also Chapter 12): zcl ¼ zcs þ zsl cosu

ð5:9Þ

The surface of the particle is the sum of its surface in contact with the liquid Ssl and its surface in contact with the catalyser Scs: S ¼ Ssl þ Scs

ð5:10Þ

with Zu Ssl ¼

2pr sin u0 r du0 ¼ 2pr 2 ð1 cosuÞ

ð5:11Þ

0

Scs ¼ pr 2 sin2 u ¼ pr 2 ð1 cos2 uÞ

ð5:12Þ

while its volume is Zu V¼ 0

pðr sin u0 Þ2 rsinu0 du0 ¼ 2=3pr 3 ð1 3=2cosu þ 1=2cos3 uÞ

ð5:13Þ

5.6 Avoiding Crystallization

Again the energy of the particle is the sum of two contributions (volume wf and surface wi): wf ¼ V=Vm DGv ¼ 2=3pr 3 ð1 3=2cosu þ 1=2cos3 uÞDGv =Vm

ð5:14Þ

and wi ¼ zsl Ssl þ zcs Scs zcl Scs ¼ zsl Ssl þ ðzcs zcl ÞScs

ð5:15aÞ

Substituting the mechanical equilibrium equation allows one to write wi ¼ zsl Ssl ðzsl cos uÞScs ¼ zsl pr 2 ½2ð1 cos uÞ ð1 cos2 uÞcos u ¼ zsl pr 2 ð2 3cos u þ cos3 uÞ

ð5:15bÞ

It follows that w ¼ wi þ wf ¼ ð1 3=2cos u þ 1=2cos3 uÞf2=3pr 3 DGv =Vm þ 2zsl pr 2 g ð5:16Þ

Therefore, the maximum of the function is found for the same critical radius as for homogeneous nucleation: rc ¼ 2zsl Vm =DGv

ð5:17Þ

while wc het ¼ ð1 3=2cos u þ 1=2cos3 uÞwc hom =2 ¼ ð1=2 3=4 cos u þ 1=4 cos3 uÞwc hom

ð5:18Þ

The ratio wc het/wc hom is plotted as a function of angle u in Fig. 5.13 and this ﬁgure illustrates why heterogeneous nucleation has to be carefully considered since even for wetting angles as high as 308 the wc het/wc hom ratio is less than 1 %. Therefore, ‘dangerous’ catalysers are such that they allow wetting of the solid (u ! 0) and a related decrease of the energy barrier enhancing heterogeneous nucleation. It should be noted that for a given volume, heterogeneous nucleation leads to much larger particle radius since the radius ratio is rhet =rhom ¼ ½ð1 3=2cos u þ 1=2cos3 uÞ=21=3

ð5:19Þ

5.6.3 Crystal Growth

The nuclei being formed, they will then grow. Growth rate g can be calculated assuming a thermally activated transfer of atoms from the liquid phase to the solid

71

72

5 Glass Structure

Fig. 5.13 Plot of wc het/wc hom as a function of angle u.

phase and from the solid phase to the liquid phase (Fig. 5.14): gðTÞ ¼ fac ðvls vsl Þ

ð5:20Þ

where f is the fraction of surface site (0 < f < 1), ac the solid–liquid interface thickness and vls and vsl the frequencies for respective transfers (Fig. 5.14). We have DG00 ; vls ¼ vE exp RT

DGv þ DG00 vsl ¼ vE exp RT

ð5:21Þ

with vE the atomic transition frequency in the liquid, T the temperature and DG00 and DGv þ DG00 the respective barriers. DGv is the molar enthalpy of liquid–crystal transformation. One can write DG00 DGv 1 exp gðTÞ ¼ fac vE exp RT RT

ð5:22Þ

The interface transport can be described by a diffusion coefﬁcient. In the general case we do not know the energy barrier for diffusion through the interface. Longdistance diffusion is to be considered. As a ﬁrst approximation and since only one type of atom is considered here, we can suppose the diffusion barrier is the same

5.6 Avoiding Crystallization

Fig. 5.14 Liquid–solid interface modelling. Note we consider only one type of atom and hence the same composition for the liquid and the solid. This is rarely the case (l, liquid; s, solid).

as that appearing in viscous ﬂow, DG00 ¼ DG, and take again the Stokes–Einstein relation D¼

kT DG ¼ vE a2o exp 3pao h RT

and express the growth rate supposing that ac ¼ ao (twice the particle radius) as kT DGv 1 exp gðTÞ ¼ f 2 ao 3ph RT

ð5:23Þ

Note that at T ¼ TL, DGv is null so that g ¼ 0, while DGv amplitude increases when temperature decreases. However, viscosity increases as well and progressively balances the DGv contribution. This also describes well qualitatively the growth (g) curve shown in Fig. 5.12 with a maximum being observed between TL and T3. The role of viscosity in inhibiting nucleation, growth and hence crystallization should be emphasized. This result applies to general glass compositions. In fact, glass formation is made possible using compositions allowing for a viscous regime around the liquidus temperature. In Chapter 6 we shall further discuss the importance of this property when glass is to be frozen in. Regarding crystallization, it is well known that

73

74

5 Glass Structure

adding alkali to silica allows a decrease in viscosity. As a matter of fact, at very high content of alkali, say that corresponding to the composition of orthosilicate, glasses are never obtained since the rates of nucleation and crystallization become too high. Also, devitriﬁcation will depend on the viscosity regime (Section 5.6.5). As mentioned at the beginning of this section, once glass is not composed of a single atom type (which indeed is unrealistic) crystallization becomes complex to model (Fokin et al., 2006). In general the crystalline phase presents a different composition from the original glass, so that glass composition in the surrounding of the growing crystalline phases changes with implication for the viscosity regime. Also, a depleted zone may appear for the elements present at higher stoichiometry in the crystalline phases. 5.6.4 T T T Diagram

The simple monatomic models presented above allow an insight into glass formation even though we made rough approximations. The practical need however is to form a realistic glass without detectable crystalline phases. In this regard temperature– time–transformation (TTT) diagrams have to be elaborated theoretically and experimentally for more complex glass compositions (Fig. 5.15). The TTTdiagram shows in a temperature–time plot the crystalline and glass domains. When forming a glass, the cooling route must, in no case, pass through the crystalline domain (Fig. 5.15). Then the critical cooling rate allowing for the production of glass is that tangent to the ‘nose’ (Tn, tn) of the limiting front: dT Tm Tn ¼ dtc tn

ð5:24Þ

The critical cooling rate is 102–103 K s1 for silica glass while pure metals require cooling rates as high as 106 K s1 (Fig. 5.16). Some metallic alloys (BMGs) can now be formed as bulk glasses at moderate rates (Inoue et al., 1996; Lu et al., 2003; Wang et al., 2004). While pure metals can be produced by melt spinning, alloys can be produced by arc melting and drop casting at cooling rates as low as e1 K s1.

Fig. 5.15 Schematic T T T diagram and one thermal history for producing glass (arrow).

5.6 Avoiding Crystallization

Fig. 5.16 Critical cooling rate for different classes of glass as a function of reduced glass transition temperature Trg = Tg/Tm. (Reprinted from Wang et al., 2004, with permission from Elsevier.)

5.6.5 Devitriﬁcation

Once the glass is formed, the discussion turns to its devitriﬁcation upon a heat treatment. In fact, there have been measurements to determine the rate of growth of crystalline phases in an annealed glass. Once the temperature increases crystal growth may happen whenever the relative nucleation and growth curves overlap or whenever impurities serve as nuclei. Growth rate increases steeply to a maximum and then decreases to zero at liquidus temperature. Such a curve is shown for a silicosoda-lime glass in Fig. 5.17 when the growth of crystals of composition Na2O–3 CaO–6SiO2 called devitrite is observed. This phenomenon is to be avoided when a glass article is heat treated unless a glass–ceramic material is to be formed from a parent glass as detailed in the next section. Addition of a few percent of oxides like

Fig. 5.17 Rate of growth of devitrite in a soda-lime-silica glass (according to Jones, 1956).

75

76

5 Glass Structure

MgO or Al2O3 allows for reducing devitriﬁcation risks in ordinary oxide glasses (window glass). Also, care must be taken regarding preferential sites for nucleation like surfaces, dust, bubbles or inhomogeneities. 5.6.6 Factors That Favour Glass Formation

In view of a number of complex issues it is important to summarize factors that favour glass formation: i. Viscosity is the controlling parameter, and a high-viscosity regime is searchedforatliquidustemperatureandaroundtheTTTdiagram nose. This means low transport and hence small rearrangement rates leading to low rates of nucleation and crystallization. ii. Avoid heterogeneous nucleation. iii. Consider systems with a large crystal–liquid interfacial energy. iv. Consider systems with a large concentration change between the liquid and the crystal phases.

5.7 Vitroceramic Fabrication 5.7.1 Introduction

Glass–ceramics are ﬁne-grained polycrystalline materials formed when glasses of suitable compositions are heat treated and thus undergo controlled crystallization. The parent glasses have speciﬁc compositions comprising precursors as detailed below. Indeed, ordinary window glass is too stable and difﬁcult to crystallize, whereas other compositions crystallize in an uncontrolled manner resulting in undesirable microstructures. Usually, a glass–ceramic is not fully crystalline; typically the microstructure is 50–95 vol.% crystalline with the balance volume being the residual glass. One or more crystalline phases may form during the heat treatment and as their composition is normally different from the parent glass, it follows that the composition of the residual glass is also different from that of the parent glass. The mechanical properties of glass–ceramics are superior to those of the parent glass. Vitroceramics are fabricated for ﬁre resistance (cooking tops and containers; refer to Eurokera activity, Saint Gobain group and Corning ware) since the combination of crystalline and vitreous states allows for a lower thermal expansion and a higher strength. For astronomy, Zerodur (Schott) has allowed the fabrication of an 8.2 m telescope based in Chile with thermal expansion as low as 107 8C1. Surprisingly, only recently have such materials been produced. It must be said that while glasses tend to devitrify, the control of such a phenomenon is very difﬁcult and was reported only by 1950. In fact, it requires well-controlled thermal treatments in view of nucleation and growing curves (Fig. 5.18) and the use of nucleation agents.

5.7 Vitroceramic Fabrication

Fig. 5.18 Two-stage heat treatment for a system showing negligible overlap of nucleation and growing curves (according to Rawlings et al., 2006).

5.7.2 Conventional Method (two stages)

The conventional method for producing a glass–ceramic is to devitrify the parent glass by a two-stage heat treatment (Fig. 5.18). The ﬁrst stage is a low-temperature (TN) heat treatment that gives a high nucleation rate thus forming a high density of nuclei throughout the interior of the glass (Rawlings et al., 2006). A high density of nuclei is important since it leads to a desirable microstructure consisting of a large number of small crystals. The second stage is a higher temperature (TG) heat treatment to produce growth of the nuclei. The achievement of such a microstructure is helped by nucleation agents that can be metallic (Au, Cu, Ag, Pt, Pd) or non-metallic (TiO2, P2O5 and ﬂuorides). These aggregate and subsequently induce controlled ceramic nucleation. Designed crystals embedded into the glass matrix are then formed. 5.7.3 Modiﬁed Conventional Method (single stage)

The reason for the two-stage heat treatment of the glass is a consequence of the limited overlap between nucleation and growth rate curves. If, on the contrary, there is extensive overlap of the rate curves then nucleation and growth can take place during a single-stage heat treatment at temperature TNG (Fig. 5.19). The rate curves and particularly the nucleation curve are sensitive to composition, and hence optimizing the glass composition (choice of nucleating agents) is in some cases possible to obtain the necessary overlap. 5.7.4 Laser-Induced Method

For some years now, glass to ceramic transformation could be conﬁned using a focused laser beam. This allows for patterning a glass object in three dimensions

77

78

5 Glass Structure

Fig. 5.19 Single-stage heat treatment for a system showing overlap of nucleation and growing curves (according to Rawlings et al., 2006).

(Lehmann, 2005). The nature of the local transformation (cavity, crystallite, composition change) is however still under debate.

5.8 Glass Surface

The ﬁrst approach to study a glass surface is to start from the bulk structure and move towards the surface. The presence of the surface allows for the interaction of glass with the atmosphere. Surface structure is changed by the physical and chemical interactions. Koike and Tomozawa (2006) report that surface structural relaxation takes place more rapidly than bulk structural relaxation in particular in the presence of water diffusion (see also Chapter 6). Gas molecules penetrate the glass network through its excess volume and may react with the glass. We know that the bulk glass structure is not unique but depends on modiﬁer concentration and network formers. We shall consider here mainly silica and suppose it is modiﬁed by alkali (Naþ) knowing that variations are expected for more complex compositions. 5.8.1 Surface Reaction

When silica cools down its surface reacts with water molecules to form silanol bonds (Fig. 5.20). The reaction can be written as SiOSi þ H2 O ! SiOH þ HOSi

ð5:25Þ

The reaction energy is elevated and around 80 kJ mol1. The water reaction leads to a high density of silanol groups that can reach 4.6 sites per nm2 (Bather and Gray, 1976). According to the proximity to other silanol groups, hydrogen bonding will be possible. Also, the silanol groups may react with water without dissociation of the water molecules. This reaction is referred to as water physisorption. The glass surface may

5.8 Glass Surface

Fig. 5.20 Representation of the hydration of a silica surface.

hence be covered by several monolayers of water depending on the water partial pressure in the atmosphere. Not only water but also organic pollutants may adsorb. It should be noted that although an annealing treatment at 100 8C allows the desorption of water molecules, a treatment at a much higher temperature is necessary to form again siloxane groups (reversing reaction 5.25). 5.8.2 Molecular Diffusion

Molecules diffuse through the glass network. This phenomenon follows diffusion laws (Appendix 13). The smaller the molecule size the more important the diffusion. Diffusion of rare gases (He, Ne, Ar) and molecules (H2, O2, H2O) has been documented3) for different compositions of glasses (Doremus, 1994) and allows for tailoring glass permeability. Importantly, some of these molecules once in the glass may react and change glass properties and behaviour (viscosity, electrical conductivity). The role of the water reaction is discussed in more detail below. 5.8.3 Glass Network Interaction with Water

In fact, water interaction is not conﬁned to the surface (Section 5.8.1) because of water diffusion through the glass excess volume (Appendix 13). Moreover, when we consider a glass with modiﬁers, non-bridging oxygen (NBO) atoms appear so that they open the network while mobile ions (alkaline ions) will diffuse. The deleterious role of alkali can be limited by introducing alumina and/or B2O3 in the glass melt. The elevated resistance of natural glasses over millions of years is to be attributed to their aluminosilicate-rich compositions while borosilicate glasses are used for 3)

Brown and Kobayashi (1998) entitled one of their papers ‘Is your glass full of water?’ Water concentration in commercial silicate glasses is in the range 0.01–0.1 wt%.

79

80

5 Glass Structure

pharmaceutical packaging (Chapters 3 and 4). In sodium-rich glass, Na+/H3O+ interdiffusion promotes water interaction within the network and can be followed eventually by corrosion of the network depending on the alkalinity of the solution (pH) at the glass surface4). 5.8.3.1 Water Reaction Water is present in the glass excess volume. Let us consider ﬁrst silica. Water reacts with the silicon–oxygen bonds as already discussed for the surface as follows: SiOSi þ H2 O ! SiOH þ HOSi

ð5:26Þ

This reaction is of utmost importance in glass mechanics since it is enhanced at crack tips and is responsible for the fatigue of glass (Chapter 9). The reaction is enhanced as water concentration is increased. 5.8.3.2 Ion Exchange Let us consider an alkali-modiﬁed silica glass. Because of mobile modiﬁers, the glass will undergo ion exchange, alkali being leached. Let us consider for instance sodium. Water diffusion (in fact H3O+) into the glass network is as follows: SiO Naþ þ H3 Oþ ! SiOH þ H2 O þ Naþ

ð5:27Þ

The superﬁcial glass loses sodium ions (glass leaching) while it incorporates water (it may also affect other mobile modiﬁers). This happens for external glazing or when in contact with water. The formation of a silica gel at a glass surface can be described by Fick’s law (Appendix 13), the typical thickness of the gel layer being about 0.1 mm.

Fig. 5.21 In vitro degradation of a glass ﬁbre. (Courtesy ´ Henri Hermine Dika, Pr Bertrand Rihn, Universite ´, Nancy 1, France.) Poincare

4)

pH ¼ log½H3 Oþ ¼ log Ke log½OH ; ¼ pKe log½OH ; pKe ¼ 14 where the square brackets indicate the

5.8 Glass Surface Surface energy (glass–water vapour) and wetting angle according to the type of surface (after Chartier, 1997).

Tab. 5.3

Native glass surface ‘Clean’ glass surface Polluted glass surface

Surface energy, z (mJ m2)

Water contact angle (8)

400–1000 70 20–40

– 0 20–60

Such a layer can be detected by X-ray reﬂectometry (Table 5.1) because glass subsurface presents different properties as compared to the bulk. Also the hydrated glass surface exhibits lower resistance to contact loading (Chapter 8, Appendix 10) and this is beneﬁcial when abrading the glass edges. 5.8.3.3 Glass Corrosion Na+ diffusion towards a glass surface increases the alkalinity (pH) of the aqueous solution in contact with the glass. When pH reaches 9 then siloxane bonds may react with hydroxide ions as follows: SiOSi þ OH ! SiOH þ O Si

ð5:28Þ

Such a pH value is achieved when the glass remains in the same humid and conﬁned environment as for stored glass panels and glass wool. As matter of fact, it may happen that glass products are damaged by corrosion. This is limited when storing glass panels using acidic paper in between. This phenomenon is well known to glass manufacturers and can be tailored using Na2O, K2O, CaOrich glasses to enhance it or using Al2O3, B2O3, ZrO2, TiO2rich glasses to limit it (these oxides act as barriers). The development of bioglass (biodegradable ﬁbres in particular) is a further illustration of tailored glass chemical resistance. These have been motivated by the asbestos scare (Fig 5.21). Nowadays, environmentally safe ﬁbres can be produced so that their half-life is less than 40 days in lungs. For the conﬁnement of complex and dangerous wastes from the biosphere, glasses resisting water corrosion are needed (see also Chapter 3). Aluminoborosilicates are being developed to achieve glass loss of less 0.1 % over 100 centuries. 5.8.4 Surface Properties

It should be noted that all reactions described in Section 5.8 change dramatically surface properties, in particular the surface energy (Table 5.3). The complex glass surface can ﬁnally be schematized as: glass bulk/hydrated glass/water/pollution. Functionalizing the surface of glass supposes it is ﬁrst cleaned up; it can also be treated (Chapter 12).

81

83

6 Glass Rheology 6.1 Viscosity 6.1.1 Viscosity and Process

One of the most important properties from a glass process point of view is the viscosity, which changes dramatically as the temperature changes. Viscosity determines the melting conditions, the temperature regimes for forming, annealing and tempering, and the maximum temperature to avoid devitriﬁcation. Moreover, glass quality is dependent on the way it is homogenized and this is also related to the viscosity regimes. Viscosity measures the resistance of a viscous liquid to shear deformation. The higher the viscosity, the higher the resistance to ﬂow. Consider a liquid between two planes (surface S) and apply a tangential force F to the upper plane (Fig. 6.1). For a solid (inﬁnite viscosity) no ﬂow will occur. On the contrary, a viscous liquid will ﬂow. A velocity gradient will appear in the liquid. If we assume that there is no relative displacement between the plate and the liquid, then velocity varies from zero at the bottom plate to the velocity of the upper plane at distance a (Fig. 6.1). Velocity gradient is then determined as 5v ¼ (v 0)/a and increases when the force F or shear stress (t ¼ F/S) applied to the upper plate increases. The relationship between the velocity gradient and the shear stress is written t ¼ F=S ¼ hrn

ð6:1aÞ

where h is the viscosity in Pa s. An industrial process can be considered according to its velocity gradient (Table 6.1) and one can observe huge differences between these. Equation (6.1a) means that the viscosity regime (temperature, as discussed below) has to be carefully controlled when forming the glass according to the different processes. Also, it is of utmost importance to prepare the glass under uniform temperature. This operation is referred as ﬁning (Chapter 10). Viscosity controls the quality and the homogenization of the glass. During this step, the elimination of bubbles also depends on the viscosity (Chapter 10, Appendix 4). Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

84

6 Glass Rheology

Fig. 6.1 Shear ﬂow in a viscous liquid. Tab. 6.1

Processes and associated ranges of velocity gradient.

Process

Velocity gradient 5v (s1)

Moulding Extrusion Wire drawing

0.1–10 102–103 104–106

The related stresses to be applied by the tools will depend strongly on viscosity regime. From a mechanical point of view (Appendix 9) it is of interest to rewrite Eq. (6.1a) in terms of shear strain. Such an equation shows the time dependence of shear stress t as a function shear strain g.1) t ¼ hrv ¼ hg

ð6:1bÞ

This behaviour is completely different from that of an elastic solid that shows no time dependence (Appendix 9). In fact in the elastic regime shear stress is proportional to shear strain, t ¼ Gg, where G is the shear modulus. Therefore, while an elastic solid shows a response to stress independent of time, a viscous liquid shows a response that depends not only on stress amplitude but also on time. Hence, the control of the tools for a process involving viscous liquids requires the control of viscosity regime, stress amplitude and loading time. Glassmakers have set several important temperatures that deﬁne ranges of viscosity that are important from a process point of view. These temperatures are listed in Table 6.2. In fact, viscosity depends strongly on the temperature as shown in Fig. 6.2 and process temperatures are set relative to the deﬁned reference temperatures. This will be discussed in detail in Section 6.1.3. Composition also may change the viscosity 1)

An ideal Newtonian flow is assumed here with a viscosity independent of strain rate. The plot of () is linear. This hypothesis is true at elevated temperature and under low stresses. Instead, non-Newtonian flow (viscosity depending on strain rate) is reported at intermediate temperature closer to Tg and for high strain rates (Simmons et al., 1988) yielding more difficulty in the control of tools. A drastic decrease of viscosity is observed with increasing strain rate. So called rheofluidification may be advantageous

from a process point of view if one considers the required stress. For a non-Newtonian flow, the stress-strain relationship is ¼ ðÞ with a viscosity depending on shear strain rate . It can be approximated by ¼ m, where m is the strain-rate sensitivity exponent (m < 1), similar to that used to describe metal plasticity and it is pointed out that non-Newtonian regime allows for prevention of ‘necking’ (Jones, 1956). The apparent viscosity is = ¼ m1 (Appendix 10).

6.1 Viscosity Tab. 6.2 Reference temperatures and viscosity regime8). Practical melting temperature is not the melting temperature associated with the crystal–liquid phase transition (Chapter 5) but the working temperature.

Reference temperature

Viscosity (Pa s)

Practical melting temperature Working point Littleton softening point Annealing point Glass transition Strain point

1–10 103 106.6 1012 1012–1012.5 1013.5

Fig. 6.2 Viscosity variations with temperature and composition (SLS, soda-lime-silica glass; ALS, aluminosilicate glass; according to Zarzycki, 1982).

drastically. Modiﬁers (Chapter 5) are introduced into the melt to reduce the working temperatures and hence increase industrial yields saving costs in processing. In fact, the same viscosity regime (horizontal line in Fig. 6.2) is obtained for increasing temperatures as glass is changed from lead glass, soda-lime-silica (SLS) glass, borosilicate glass and ﬁnally pure silica. Modiﬁers lead to the formation of nonbridging oxygens and allow viscous ﬂow to occur at much lower temperatures in SLS glasses than in silica (Chapter 5). The ALS glass curve crosses the other with a higher transition temperature than SLS (see also Section 6.7). 2)

For comparison we list the viscosity (in mPa s) of common materials: hydrogen, 0.0086; gas, 0.01–0.02; water, 1; kerosene, 10; oil, 100; honey, yogurt, 103–106; glue, paint, resin, 102–107; asphalt, 105–108.

85

86

6 Glass Rheology

To optimize production tools and processing, it is of utmost importance to fabricate a glass with homogeneous temperature and composition or in other words homogeneous viscosity. In fact, the temperature of the glass delivered from the melting furnace and its composition have to be regulated with extreme care. From the control or R&D perspectives, it is necessary to determine carefully and precisely the viscosity as a function of both temperature and composition. This is not straightforward since viscosity varies in a wide range and instruments have been developed accordingly. Interestingly, such measurements revealed that in limited domains empirical relations exist between the compositions and the properties of glass (Priven, 2004). The optimization of the composition for processing can then be made using these empirical laws to deﬁne a range of compositions likely to yield a glass with the required properties (see also Chapter 2). Nonetheless, one also has to take into account the complex shape of the produced article as well as its complex thermomechanical loading. This can be achieved again for R&D purposes using numerical modelling to consider the properties of the material and its loading at each point of the specimen (Appendix 11). 6.1.2 Viscosity Measurement

Different instruments have been designed according to viscosity ranges (Table 6.3), and the overall viscosity curve is obtained using complementary techniques. We shall describe some of these – rotating cylinder and ﬁbre elongation viscometers – allowing for low (10–103 Pa s) and high (106–1013 Pa s) viscosity measurement respectively. At intermediate temperatures, crystallization may interfere with the measurements and caution should be taken with the resulting data. Viscosity experiments can be divided in several ways: whether they are strain-rate controlled (resultant stress being measured, e.g. concentric cylinders) or stress controlled (resultant strain rate being measured, e.g. ﬁbre elongation), whether they involve pure shear (e.g. concentric cylinders) or a combination of shear and volume stress (beam bending, ﬁbre elongation). Usually the viscometer is calibrated with a liquid of known viscosity; absolute measurements can be made with care. Tab. 6.3

Measurement methods for viscosity.

Range

Method

Viscosity value, h (Pa s)

Melting

Falling sphere/bubble rise Rotational methods (concentric cylinders, cone-and-plate) Parallel plate

Tg) can be ﬁtted empirically by the Vogel–Fulcher–Tammann (VFT; see Section 6.1.3.3) formula that captures relatively well the non-Arrhenius temperature dependence over the meltforming region. The reason for observing either strong or fragile behaviour has been widely debated. It is believed that fragile liquids lack intermediate-range order; some theoretical backgrounds are developed in Sections 6.1.3.2 and 6.1.3.4. We may still use an Arrhenius temperature dependence when considering limited domains of temperatures and we adopted this procedure in Chapter 5. Instead, when variations over a large range of temperatures are to be predicted for fragile glass, nonArrhenius temperature dependence is to be taken into account in order to get suitable predictions of glass behaviour. At temperatures below Tg (Fig. 6.6) the viscosity curve is still unknown and debated. In fact the question mark is shown on Fig. 6.6 to indicate the domain where viscosity is uncertain. Above 1015 Pa s viscosity values should be considered with great care. As plotted in Fig. 6.6, the curve suggests that the rate of increase of viscosity with decreasing temperature becomes greatly reduced. There is a qualitative explanation for such an expected behaviour since the glass below Tg is frozen in a liquid-like structure the conﬁguration of which corresponds roughly to that in equilibrium near the glass transition temperature (see also ﬁctive temperature in Section 6.5.3). Hence glass structure is not at equilibrium. Further consideration of the related viscosity at these temperatures is necessary from the experimental point of view. Indeed, the apparent viscosity commonly measured using penetration viscosimetry is non-Newtonian at these low temperatures and therefore strain rate dependent (Appendix 10). Moreover, the measured deformation is not purely viscous because of delayed elasticity, as stated above and detailed in Section 6.4.4. Hence, it is not possible to measure the equilibrium viscosity at these temperatures. This fact may account for the huge discrepancy in viscosity values published in the literature since apparent viscosity depends on stress and strain rate amplitude, or on experimental conditions. The ﬁnding is that the apparent viscosity decreases under these conditions.2)

2)

There exists a very broad range of values in the literature. For instance, Frischat (1987) reports a 1020 Pa s value while Macosco (1994) reports 1040 Pa s. These values would correspond to relaxation time (refer to precise definition below) from 109 s (30 years) to 1029 s. These discrepancies yielded sometimes controversy in the observed geometry of stained glasses in cathedrals. In fact, it has been observed that cathedral windows are wavy and thicker at the bottom. Would glass have flowed when standing in place for some hundreds of years? There have been speculations on this subject. In fact, when measuring viscosity at low temperature elevated stresses are to be applied to the specimens. Under such conditions the apparent viscosity

is expected to decrease with the amplitude of stress and strain rate (Appendix 10). Discrepancies are then expected between authors as the Newtonian viscosity is not determined. On the other hand, it would be problematic extrapolating high-temperature data (in particular in the case of a fragile melt). It is not possible to predict glass flow under moderate stress. On the other hand, undeformed glass vases (>2000 years old) have been discovered, while natural glasses maintain their structure. In fact, medieval windows could have been blown and subsequently flattened manually and non-uniformly (Chapter 3); then architects would have put the thicker part at the bottom (see also Chapter 12).

6.1 Viscosity

6.1.3.2 Fragility Transition temperature is of great importance as well as the properties changes in the melt-forming region. Observation of a viscosity curve on a log h 1/T diagram indicates that indeed the behaviour depends dramatically on the type of glass, with greater curvature being observed for fragile glasses. A strong glass has then a larger viscosity than a fragile glass on approaching Tg. It is quite helpful to employ a unique temperature scale for all glasses using the transition temperature to temperature ratio as the x-axis (Fig. 6.7). On such a graph all glass responses meet at a common point corresponding to the glass transition at a viscosity of 1012–1012.5 Pa s and Tg/T ratio equal to 1. In such a graph, the glass behaviour is nothing but unique and really composition dependent. The question is why we observe such different behaviours (Doremus, 1994, 2003; Angels, 1995; Kieffer, 2002; Novikov and Sokolov, 2004; Tanaka, 2005). In fact, while the nature of the transformation by which a supercooled liquid ‘freezes’ to a glass has been the subject of intense investigations and substantial progress has been made in understanding this phenomenon over the past two decades, yet many key questions remain. In particular, the factors that control the temperature-dependent relaxation and viscous properties of the liquid phase as the glass transition is approached, that is, whether the glass-forming liquid is ‘fragile’ or ‘strong’, remain unclear (Angels, 1995).3) The fragility of liquids characterizes the deviation from Arrhenius behaviour or the curvature from a straight evolution (expected from Eyring theory; see Section 6.1.3.4; Fig. 6.2 or Fig. 6.7 replotted with respect to transition temperature). Silica shows strong or almost Arrhenius behaviour since a linear variation is observed for all temperatures (Fig. 6.7). In contrast metal ﬂuoride glasses show important deviations from such an Arrhenius behaviour. Fragility can be numerically deﬁned as the apparent activation energy of shear viscosity h at the glass transition temperature Tg, normalized to Tg (Angels, 1995): m¼

qlogh qðTg =TÞT¼Tg

ð6:12Þ

Hence, m characterizes the steepness of the slope of the log h dependence on Tg/T near Tg. A stronger deviation (larger m) from Arrhenius behaviour corresponds to a more fragile system. As mentioned above, Fig. 6.7 shows that fragility depends on the material. Silica demonstrates Arrhenius behaviour over the logarithm of viscosity range from 1 to 13, whereas fragile glasses demonstrate an almost continuously changing slope, or one that can be approximated by two straight lines (one at elevated temperature and another at the transition). Strong behaviour is controlled by continuous Si–O–Si bonding as in silica while the break-up of this bonding controls

3)

The belief that a glass is a supercooled liquid in which atomic motions have slowed to the extent that characteristic relaxation time exceeds the observation period (thousand years for stained medieval windows) is debated and the possibility that glass

corresponds to a different physical state from the liquid is considered. This suggests that glass would require an independent set of parameters and this is not done yet in engineering or scientific calculations (Kieffer, 2002).

93

94

6 Glass Rheology

network modiﬁed glasses. Hence, alkali silicates are less resistant to thermal degradation and could ﬂow within alkali-rich regions (Chapter 5). Empirical formulas have been proposed to correct for the deviation from non-Arrhenius temperature dependence (Section 6.1.3.3). The most well known is the VFTempirical law, which is extensively employed in research and industry. 6.1.3.3 VFT Empirical Formula A supercooled fragile liquid shows a viscosity that can be approximated by the VFT (Vogel–Fulcher–Tammann) formula hðTÞ ¼ ho exp

B T To

ð6:13Þ

where B and ho are temperature-independent coefﬁcients. This law can be considered as a correction of the Arrhenius law adding a To term. In fact, taking To ¼ 0 K or assuming T To transforms the VFT formula into an Arrhenius temperature dependence. The VFTapproximation is still easy to use and allows for close prediction of the actual viscosity. It is an empirical law that allows one to capture the curvature of the experimental ln(h) 1/T curves. As will be discussed in detail below, different approaches have been proposed to model the actual behaviour represented by the VFT empirical law; these are complex and still matters of debate. In accordance with the VFT equation above, the viscosity of a glass will be inﬁnite at To or below Tg (no mobility). This is unlikely to be correct (Section 6.1.3.1, Appendix 10). For a silicosoda-lime glass for instance, the VFT parameters are determined to be B ¼ 4320 K, To ¼ 542 K and ln ho ¼ 2.77 (Guillemet and Gy, 1996). 6.1.3.4 Microscopic Approach Eyring theory for molecular mobility supposes that the movement of each molecule (or structural unity) is thermally activated (Fig. 6.8). Given a barrier energy Dg, the jump frequency is written Dg DG ¼ nE exp nE exp kT RT

ð6:14Þ

where nE is the atomic transition frequency in the liquid (order of magnitude 1013 s1; Einstein frequency). The applied force or shear stress t modiﬁes the barriers as shown in Fig. 6.8c (Douglas, 1958), ﬂow being biased so that the probability of a forward jump (supported by the shear stress) is higher than for the backward jump (against stress). The jump frequency along the direction of ﬂow nþ and in the opposite direction n is written Dg tV=2 nþ ¼ nE exp kT

ð6:15Þ

6.1 Viscosity

Fig. 6.8 Representation of an individual atomic jump: the basic step for macroscopic diffusion and ﬂow.

Dg þ tV=2 n ¼ nE exp kT

ð6:16Þ

where V is the atomic volume. The effective jump frequency is written Dg tV=2 tV=2 exp exp n ¼ nþ n ¼ nE exp kT kT kT Dg tV sinh ¼ 2nE exp kT 2kT

ð6:17Þ

95

96

6 Glass Rheology

When all the atoms in a specimen make one jump ao (assuming ao ¼ 2r, where r is the atom radius) in the direction of shear, macroscopic shear strain g ¼ 1. Shear strain rate is then written Dg tV sinh g ¼ 2nE exp kT 2kT

ð6:18Þ

and for a low applied stress, the strain rate is written (since sinh(x) ! x for x ! 0) g¼

tV Dg nE exp kT kT

ð6:19Þ

We note that Newtonian ﬂow (t g) is obtained under these conditions and that the viscosity is written kT Dg h¼ exp VnE kT Dg DG h ¼ ho exp ¼ ho exp kT RT

ð6:20Þ ð6:21Þ

with ho ¼ kT/VnE. Temperature dependence of ho is often neglected, in the present framework it is determined to be linearly dependent on T, and hence ho varies usually far less than an exponential term (see also Appendix 13). On cooling the liquid, ﬂow becomes impossible because of unavailable free volume for atomic jump. The main theories accounting for this phenomenon are the free-volume model (Cohen and Turnbull, 1959; Turnbull and Cohen, 1961) and the conﬁgurational entropy model (Adams and Gibbs, 1965). Free-volume models follow the idea that on cooling the supercooled liquid, free volume progressively reduces,4) and hence mobility becomes impossible. The mobility of an atom (or more generally a structural unit) is supposed to be possible only when a free volume which can contain the atom exists next to it. We shall consider in the following the average free volume per atom. Let us call v the minimum volume of a cavity that can contain the atom or the mobile structural unit. Diffusion of the atom will depend on the free volume size vf per atom. Hence either ðiÞ nf < n

ð6:22Þ

and there is no diffusion of the atom, or ðiiÞ nf > n

and there is diffusion of the atom. 4)

Density fluctuation can be revealed using SAXS techniques (Levelut et al., 2002) and is observed to depend on temperature and thermal history.

ð6:23Þ

6.1 Viscosity

The probability of ﬁnding an atom with a free volume next to it of size between v and v þ dv is given by (Cohen and Turnbull, 1959) a v dv ð6:24Þ exp a vf vf where a is a geometrical factor between 12 and 1. The probability that the atom is on a potential jump site is then Z1 v

a v v exp a dv ¼ exp a vf vf vf

ð6:25Þ

To obtain the shear strain rate one has to consider that only potential sites for jump contribute and hence v tV sinh g ¼ 2nE exp a 2kT vf

ð6:26Þ

Again, for low applied stresses, we still obtain Newtonian ﬂow (t g): g¼

tV v nE exp a kT vf

ð6:27Þ

while viscosity no longer shows Arrhenius behaviour but instead is written in a WLF form (Williams et al., 1955; Ferry, 1970): v h ¼ ho exp a vf

ð6:28Þ

Cohen and Turnbull 1959 further suggested that the free volume can be obtained from thermal expansion coefﬁcients of the amorphous and liquid phases (above the glass transition temperature). Calling the difference in coefﬁcients of thermal expansion Da ¼ al as between the liquid and glass (see also Section 6.2) they wrote vf ¼ 0 for T < Tg

ð6:29aÞ

vf ¼ vm aðT To Þ for T > Tg

ð6:29bÞ

Also, pressure dependence can also be incorporated. We obtain v v 1 av =vm Da ¼ ho exp a ¼ ho exp ð6:30Þ hðTÞ ¼ ho exp a T To vf vm Da T To

This expression is similar to the VFT empirical expression found for viscosity. As the temperature is lowered, the (T To) term causes curvature below Arrhenius

97

98

6 Glass Rheology

behaviour (so-called fragility). However, if To ¼ Tg then the curvature is too large and To ¼ Tg DT must be used with DT 20–50 8C. Note this model predicts too large a viscosity curvature near Tg and ignores conﬁgurational arrangements. Macedo and Litovitz 1965 argued that the free volume model neglects the activation energy required for making a diffusive jump. Thus they developed a hybrid equation that combines the free volume term with the Eyring term (see also Appendix 10): v Dg hðTÞ ¼ ho exp a þ vf kT

ð6:31Þ

Then the Arrhenius temperature dependence of the viscosity can occur if either of the following facts are true: (i) the material is a low-expanding one such as fused silica; (ii) free volume is proportional to temperature. In the liquid where a

v Dg kT vf

the viscosity reduces to a WLF-type equation further simpliﬁed into the VFT formula assuming Eq. (6.28b). The Macedo and Litovitz 1965 approach ﬁxed one of the problems of the free volume model in that it exhibits Arrhenius viscosity for ﬂow under constant free volume conditions (isostructural). Also, some of the free volume model limitations have been addressed by the conﬁgurational entropy model where it is postulated that rearrangement of the structure happens when a region containing at least two structural conﬁgurational states is available. It is logical to consider the motion as a cooperative process involving a simultaneous rearrangement of a large number of atoms or units. The Adam–Gibbs 1965 model is based on the idea that motion occurs by internal cooperative rearrangement of independent regions of n atoms (Avramov, 2005). When the temperature decreases, the motion of one atom disturbs an increasingly larger number n of its neighbours, or one can say the coherence length of an atom or a molecular motion increases. The Adam and Gibbs 1965 model assumed that the barrier for rearrangement is proportional to n, and determined the temperature dependence of n in terms of the conﬁgurational entropy Sc. Finally, viscosity is written hðTÞ ¼ ho exp

C TSc

ð6:32Þ

where C and ho are temperature-independent coefﬁcients and the conﬁgurational entropy Sc is written Sc ¼ DCp

T To T

ð6:33Þ

where DCp is the variation of molar speciﬁc heat between the liquid and the glass, To being the temperature at which conﬁgurational entropy becomes null which plays

6.2 Glass Transition and Its Observation

the same role here as that corresponding to the vanishing of free volume. These equations combine into hðTÞ ¼ ho exp

C=DCp C ¼ ho exp TS T To

ð6:34Þ

showing the same form as the VFT empirical equation.

6.2 Glass Transition and Its Observation 6.2.1 ‘Observing’ the Glass Transition

As mentioned above, the occurrence of glass depends on the cooling history followed by the viscous liquid. Figure 6.9 shows the volume of a specimen as a function of temperature on cooling (we shall see that heating and cooling curves differ because of structural relaxation; Section 6.5.4). In Figure 6.9, l, g and c correspond to the liquid, glass and crystal respectively. Let us start from the liquid at elevated temperatures (high-temperature end of the diagram). On decreasing the temperature, the liquid contracts ﬁrst. Whenever the cooling rate is too low, then nucleation and growth of crystallites happen as discussed in Chapter 5. Crystals form at the melting or liquidus temperature (TL ¼Tm) and a discontinuity in the volume V of the specimen is observed. The cooling rate may be high enough so that the melting temperature is passed without volume discontinuity, the liquid being then supercooled. Next, the supercooled liquid freezes into glass at the transition temperature with less volume

Fig. 6.9 Volume–temperature cooling curves. Note the discontinuity at melting or liquidus temperature (TL = Tm) when crystals form while liquid to glass path is continuous with lower contraction being observed once the glass transition is passed.

99

100

6 Glass Rheology Tab. 6.4

Transition temperature ranges.

Glass

Transition temperature (K)

Silica Soda-lime-silica Metallic Chalcogenide

1500–1600 800–850 550–700 300–600

contraction observed. This is called transition instead of transformation since the path is continuous. It is signiﬁcant that the viscosity does not show an abrupt change at the glass transition temperature (Section 6.1). This suggests that the viscosity determines the rate at which a property (here the volume) relaxes to some equilibrium value. The presence of the glass transition results from the slowing down of viscous relaxation in the liquid. At a viscosity of 1012 Pa s the relaxation time is in the range of minutes to a few hours, corresponding to usual times of experiments. Changes at glass transition allow for transition temperature determination as detailed in Fig. 6.9. Glass structure and hence its density and volume will depend on the cooling rate. When the cooling rate increases freezing happens at a higher temperature. In fact, less time is allowed for atomic rearrangement and a ‘higher temperature’ conﬁguration is frozen in. Let us consider two glasses (g1, g2) cooled at different rates. On cooling down more slowly, further atom arrangements are made possible and hence a denser structure is obtained. Therefore, the glass volume and transition temperature of glass g2 are lower than those of glass g1. The glass transition temperature is then not unique but instead an interval should be considered. Table 6.4 lists representative values for common glasses. Glass transition temperature can be determined experimentally using dilatometry or calorimetry as detailed in Sections 6.2.2 and 6.2.3. Now consider a supercooled liquid that can be cooled inﬁnitely slowly. The volume curve followed would be that of the liquid with enough time for a denser structure to organize. The resulting glass (we suppose no crystals appear) would show denser structure (less entropy).5) Hence, glasses formed under realistic conditions are expected to be unstable and driven towards a denser and stabilized conﬁguration whenever they are held at temperatures where atomic rearrangements become nonnegligible. This structural relaxation is discussed in Section 6.5.4. Another important feature is that glass will show a lower density than the crystal (see also Chapter 5). As a matter of fact, glass contains excess volume ve , a part of which called free volume vf ¼ ve vo appears to play an important role in glass mechanics (see Section 6.1.3.4; Turnbull and Cohen, 1961).

4)

Glass entropy value at 0 K is still an open question. Residual entropy of glassy states plays against the third law of thermodynamics that suggests it is zero. As temperature decreases more and more time is required for the liquid to be at equilibrium.

The question arises as to what would be the structure of the equilibrium perfectly ordered liquid at zero entropy. If crystalline, it would then suggest that there is a continuous change from the amorphous to the crystalline state.

6.2 Glass Transition and Its Observation

6.2.2 Dilatometry

A dilatometer allows for the continuous measurement of the length of a given specimen which increases continuously with temperature at a constant heating rate (Fig. 6.10; see also Appendix 3). It is generally in the range 1–50 8C min1. It has to be controlled carefully since the glass transition depends on the thermal history (see Sections 6.2.1 and 6.5.2). The same remark applies to calorimetry (Section 6.2.3). The expansion of the specimen is monitored by a stylus (or a measuring device) that contacts the specimen under a small force. Note that only the difference between the expansion of the specimen and the cylindrical support is determined (Appendix 3). Therefore, correction of the data has to be made to add the expansion of the instrument itself. Examples of corrected expansion curves are shown in Fig. 6.11. The curve shows a straight line for silica over the whole temperature range while the other two glasses show ﬁrst a linear domain (elastic), a transition around 550 and 600 8C to the liquid domain (viscous) with a change in the observed slope and then a maximum of the curve (around 620 and 680 8C). The ﬁrst transition corresponds to

Fig. 6.10 Dilatometer: (a) general view and (b) sample–stylus contact.

101

102

6 Glass Rheology

Fig. 6.11 Thermal expansion heating curves for silica, silico-soda-lime and tin-rich silico-soda-lime glasses.

the glass transition while the second one corresponds to the dilatometric softening point (obtained for a viscosity of h ¼ 1010 Pa s). Glass transition temperature can be determined at the intersecting point of the tangents of the solid and liquid domains. It is about 560 and 620 8C for the SLS and tin-rich glasses shown in Fig. 6.11. In the linear domain the slope of the curve allows one to determine the thermal expansion of the solid glass, that is, the relative expansion per temperature unit: as ¼

1 dL L dT

ð6:35Þ

where L is the specimen length and T the temperature. Glass thermal expansion is determined from Fig. 6.11 to be about 9 106 8C1 (8.9 106 and 8.3 106 8C1 for the SLS glass and the tin-rich glass respectively; Le Bourhis, 1998b). The increase in slope after transition indicates that the thermal expansion of the liquid al is larger than that of the glass. From the curves shown in Fig. 6.11, the liquid thermal expansion is estimated to be about three to four times that of the solid. However, care has to be taken with the values obtained from dilatometry for T > Tg, since expansion is measured by a contacting stylus which progressively penetrates into the viscous liquid and thermal expansion is underestimated. Further penetration of the stylus explains the end and maximum of the curve. In fact, when viscosity falls to about 1010–1011 Pa s, the glass becomes so soft that it no longer behaves as a rigid specimen. It sags if lying horizontally and suspended at only a small number of points, and it may deform under the action of the small force necessary to keep the measuring device (stylus) in contact with the specimen. In practice, whatever the arrangement adopted, the apparent maximum is found at nearly the same temperature, that is, the softening temperature. An important characteristic of modiﬁed glasses is that they show larger thermal expansion than silica. When a specimen is annealed the average distance between atoms changes according to the asymmetry of the potential energy curve or bond. When modiﬁers are introduced non-bridging oxygen (NBO) atoms are formed

6.2 Glass Transition and Its Observation

(Chapter 5) leading to bond asymmetry and hence more thermal expansion (Appendix 3). In contrast, borosilicates offer the possibility to form the glass at lower temperatures as in a modiﬁed glass while B atoms participate to the formation of the glass network. As a matter of fact no NBO atoms are formed and thermal expansion is reduced. As discussed in Chapter 2, these glasses offer good resistance to thermal shock. 6.2.3 Differential Scanning Calorimetry

A differential scanning calorimeter allows the continuous measurement of the heat ﬂow rate F between a given specimen (S) and a reference (R) as a function of temperature (Figs. 6.12 and 6.13). The reference is often the empty crucible, the same as that used for containing the specimen. The difference in heat ﬂow rate F allows for the determination of the speciﬁc heat of the specimen. Let us consider a period of time from t1 to t2 during which the specimen temperature rises from T1 to T2. Heat Q is written Zt2 Q¼

FðtÞdt ¼ mcp ðT2 T1 Þ

ð6:36Þ

t1

where m is the mass of the specimen and cp its speciﬁc heat. When glass transition is passed there is a change in speciﬁc heat that is detected by the instrument as schematically represented in Fig. 6.14 (see also Fig. 6.32). Glass transition temperature can be determined at the inﬂection point. DSC softwares offer three different determinations of the transition as shown schematically in Fig. 6.14. Tgip is determined at the point of inﬂection, Tgon at the onset of the transition and Tgend at the end of

Fig. 6.12 Differential scanning calorimeter set-up.

103

104

6 Glass Rheology

Fig. 6.13 Differential scanning calorimeter principle (R, ¨hne et al., 1996). reference; S, for specimen; according to Ho

Fig. 6.14 Heat ﬂow rate at glass transition as a function of temperature.

the transition. Notably, experimental curves often show a hump at Tgend because of relaxation phenomena; this is illustrated in Fig. 6.32 and discussed in detail in Section 6.5.4 (Ho¨hne et al., 1996; Heilmaier and Eckert, 2005). This may lead to erroneous transition temperature determination on heating curves. Below and above the glass transition, it is possible to determine the speciﬁc heat of a specimen of known weight employing Eq. (6.36) and analysing the heat ﬂow in the respective domains. When temperature is further increased, crystallization may appear (exothermic ﬂow) that further melts at melting temperature (endothermic ﬂow).

6.3 Viscous Response of Glass

An important consequence of the viscous behaviour is that glass shows timedependent properties at temperatures approaching the glass transition temperature.

6.3 Viscous Response of Glass

In fact, these phenomena appear when the characteristic time of the observations scales with the relaxation time of the glass, TR ¼ h/G, where h is the viscosity and G the shear modulus. This relaxation time will be introduced in more detail in Section 6.4.2. The time dependence appears in the shear stress–shear strain equation introduced above: t ¼ hg

ð6:37Þ

It should be noted again that, in contrast, an elastic material shows a response independent of time: t ¼ Gg

ð6:38Þ

From these equations a phenomenological correspondence has been proposed to pass from an elastic solution to a viscous one in which the elastic constants in the elastic equations are replaced with a time-dependent operator. Following Goodier 1936, the analogy between the steady viscous motion and the elastic deformation enables one to take over from the elastic theory solutions for viscous ﬂow. One has to suppose two isotropic and homogeneous bodies of the same shape, one purely viscous the other one purely elastic and incompressible. The two are loaded in the same way. ‘If certain displacements are prescribed as given function in the elastic body, then the corresponding velocities in the viscous body are prescribed as the same functions when the coefﬁcient of viscosity h is substituted for G as long as the deformation makes no signiﬁcant change in the boundaries’ (Goodier, 1936). Applying this simple rule allows the tensile representation of a viscous solid to be determined passing from s ¼ Ee ¼ 2(1 þ n)Ge to s ¼ 2ð1 þ 0:5Þhe ¼ 3he, viscous ﬂow being volume conservative (so-called prefactors 1 and 3 for shear and tensile loading respectively). Elongational viscosity is then obtained to be three times higher than shear viscosity introduced in Section 6.1.2.3. Let us now consider the forming of glass by gravity (Fig. 6.15). This is used for production of laminated windshields for instance. The elastic solution is given by

Fig. 6.15 Diagram of the deformation of a plate under gravity.

105

106

6 Glass Rheology

Timoshenko (1951): d¼k

rga4 rga4 ¼k 2 EtH 2ð1 nÞGt2H

ð6:39Þ

where d is the elastic displacement of the sheet centre, a and tH the dimension and the thickness of the sheet, r and M its density and its mass, E the Young’s modulus, g the gravitational acceleration and k a shape factor (3/4p for a circular plate). The solution of Eq. (6.39) is valid for d < tH. Changing the elastic solution using a time operator allows determination of the viscous solution: Z rga4 dt ð6:40Þ d¼k 2 h 3tH Here, we neglect the elastic part of the deformation and still suppose d < tH. This limit is quite unrealistic for commonly produced shapes and the nonlinear solution is to be considered. Adding the elastic and viscous solutions (Eqs (6.39) and (6.40)) results in a Maxwell modelling of the plate behaviour as detailed in Section 6.4. Equation (6.40) cannot be integrated simply unless the temperature (the viscosity) is supposed to be constant, which is rarely the case when an industrial process is considered. From this simple approach it is clear that complex shapes are achieved when the thermal route can be carefully controlled. In practice, two sheets of glass are twinned and subsequently treated together to form laminated windshields. When the sheet thickness and colour are identical the thermomechanical route is the same, assuming no thermal gradient is present through the sheets when heating and cooling rates are low enough. This allows one to obtain parallelism of the formed sheets and hence optimized optical properties. In practice, glass sheets are different (either in terms of thickness or colour) and the processing line is operated so that the top sheet bows onto the bottom sheet (without contact damage; see Chapter 8).

6.4 Viscoelastic Response of Glass 6.4.1 Introduction

Between the elastic and viscous extremities stands the viscoelastic behaviour that is expected around the glass transition. The purely viscous response of a melt is often termed ‘liquid’ behaviour whereas purely elastic response is termed ‘glassy’ behaviour. The intermediate transition is not sharp but shows a viscoelastic regime. Therefore, at the transition both the elastic and the viscous behaviour are to be combined. At short times the behaviour will predominantly be elastic while viscous behaviour appears at times long enough to attain steady-state ﬂow. Then viscoelastic behaviour is expected at intermediate times. The simplest approach is to combine in series or parallel these behaviours as detailed below. We will introduce an important

6.4 Viscoelastic Response of Glass

parameter, the relaxation time (that combines both properties), which allows prediction of whether for a given period of time the material behaves like an elastic, a viscous or a viscoelastic material. 6.4.2 Maxwell and Kelvin Solids

Further understanding of viscoelasticity requires in a ﬁrst step the consideration of simple models. We shall consider an elastic solid to be represented by a spring (t ¼ Gg) while a viscous solid will be represented by a dash pot (t ¼ hg; Fig. 6.16). Hence, as said above the viscous description of a solid can be found by replacing the elastic constants in the elastic solution and taking into account the time dependence. Associating the two solids (elastic and viscous) allows an insight into the viscoelastic behaviour (intermediate between purely elastic or purely viscous). The simplest association of these two elements is in parallel (Kelvin’s solid) and in series (Maxwell’s solid). Let us consider the respective combinations (Fig. 6.17). For a Kelvin solid we combine t ¼ t1 þ t2; t1 ¼ Gg and t2 ¼ hg and obtain t ¼ Gg þ hg

ð6:41Þ

For a Maxwell solid we have g ¼ g1 þ g2; t ¼ Gg1 and t ¼ hg2 . Then taking a time derivation of the ﬁrst and second equation and combining g ¼ g1 þ g2 ; t ¼ Gg1 and t ¼ hg2 we get t=h þ t=G ¼ g

ð6:42Þ

These solids allow creep and relaxation to be modelled with a characteristic relaxation time TR. Consider for instance a Maxwell solid submitted to a constant deformation g(t) ¼ go so that g ¼ 0. Shear stress relaxation with time is found solving t=h þ t=G ¼ g ¼ 0

ð6:43Þ

Taking TR ¼ h=G

Fig. 6.16 Spring and dash pot.

ð6:44Þ

107

108

6 Glass Rheology

Fig. 6.17 (a) Kelvin and (b) Maxwell solids and related creep and stress relaxation.

we ﬁnd tðtÞ ¼ to expðt=TR Þ

ð6:45Þ

which is plotted in Fig. 6.17b. We can observe that to apply a constant deformation to a Maxwell solid, a vanishing stress has to be applied. A very important parameter has appeared: the relaxation time TR. For t TR the solid behaves elastically, while for t TR viscous ﬂow is prominent. Similarly considering a Kelvin solid under constant applied stress to we have t ¼ to ¼ Gg þ hg

ð6:46Þ

The solution to this equation is gðtÞ ¼ to =G½1 expðt=TR Þ

ð6:47Þ

Hence, it is found that a Kelvin solid ﬂows under constant stress once time is of the order of TR (Fig. 6.17a). Some authors refer to Kelvin TR as retardation time. As discussed below glass delayed elasticity and ﬂow can be captured with a Burger solid that combines in series a Kelvin and a Maxwell solid. A Kelvin solid yields retardation while a Maxwell one yields relaxation. Relaxation time informs on the time scales at which a viscoelastic solid will behave elastically or relax. Let us consider glass transition: the viscosity is 1012–1012.5 Pa s while shear modulus of most glasses scale with 1010–1011 Pa so that relaxation time is of the order of 100 s. This means that at the glass transition temperature stress relaxation happens after a couple of minutes.

6.4 Viscoelastic Response of Glass

6.4.3 Dynamic Mechanical Analysis

Dynamic mechanical analysis (DMA) consists in applying a periodical stress ﬁeld to a material. We can anticipate from Section 6.4.2 that the behaviour of a viscoelastic material will depend strongly on the frequency v of the applied stress. Consider a shear stress applied periodically to a viscoelastic solid. We take a sinusoidal function having in mind that any periodic function is a Fourier series of sinusoidal functions. Shear stress is written t ¼ to cosvt

ð6:48Þ

A generalized relation between stress and strain is obtained using complex notation (t ¼ tocos vt þ itosin vt ¼ toexp ivt) in the form t ¼ G g

ð6:49Þ

G being a complex number of the form G ¼ G0 þ iG00. The real part or storage modulus describes the capacity of the material to store energy elastically upon deformation. The imaginary part is called loss modulus since it provides a measure of the energy dissipated by the material. Both moduli show a dependence on frequency. The phase shift d between stress and strain is given by tan d ¼ G00=G0

ð6:50Þ

where d is the loss angle and tan d the loss factor related to the dissipated mechanical energy DW by DW/We ¼ 2ptan d (where We is the stored elastic energy). Q1 ¼ DW/ We ¼ 2ptan d is also called the damping coefﬁcient. The elastic, viscous and viscoelastic behaviours are shown schematically in Fig. 6.18. In the elastic regime, stress and strain are in phase (no time dependence). In the viscous regime stress and strain are phase shifted by 908. Viscoelastic behaviour corresponds to an intermediate phase shift. Let us illustrate this behaviour for the case of a Maxwell solid. The modulus expression for G can be found taking again Eq. (6.42) with the complex notation (with t ¼ ivt ): t =h þ t =G ¼ t =h þ ivt =G ¼ t ð1=h þ iv=GÞ ¼ g ¼ ivg

ð6:51Þ

We extract t ¼ iv=ð1=h þ iv=GÞg

ð6:52Þ

and obtain G ¼

iv 1=h þ iv=G

ð6:53Þ

109

110

6 Glass Rheology

Fig. 6.18 Elastic, viscous and viscoelastic dynamic response.

Storage and loss moduli are G0 ¼

v2 TR2 G 1 þ v2 TR2

ð6:54aÞ

vTR G 1 þ v2 TR2

ð6:54bÞ

G00 ¼

These expressions yield for vTR ! 1; G0 ! G; G00 ! 0; d ! 0

ð6:55aÞ

that is, a purely elastic regime for large frequencies, while for vTR ! 0; G0 ! 0; G00 ! 0; d ! p=2

ð6:55bÞ

that corresponds to a purely viscous behaviour. At intermediate frequencies the material shows a viscoelastic behaviour with an intermediate loss angle (0 < d < p/2). These trends can be generalized. In fact when forced at a high frequency, a glass or a ﬂuid reacts rigidly. Deformations are small and all energy introduced into the system can be regained upon releasing strain. The storage modulus is large and the loss modulus small (Fig. 6.19). At intermediate frequencies, deformations become large enough for structural elements in the liquid to be permanently removed from their original position. Such displacements dissipate energy. At a particular frequency, a resonance occurs where the loss modulus peaks while storage modulus goes through an inﬂection (Fig. 6.19; for a Maxwell solid it is expected for w ¼ 1/TR). Towards low frequencies, the loss modulus decreases again. The ﬂuid ﬂows effortlessly, resulting in large irreversible deformations, indicating that the storage modulus becomes smaller.

6.4 Viscoelastic Response of Glass

Fig. 6.19 Loss and storage moduli as a function of frequency for 2SiO2–Na2O glass (master curve; see also Section 6.4.5.4). (Reprinted from Mills, 1974 with permission from Elsevier.)

Alternatively, glass behaviour can be investigated as a function of temperature for a given frequency (Fig. 6.20). The graph obtained for a chalcogenide glass shows that the dynamic response (at a given frequency, Fig. 6.20b) varies considerably with temperature. The Young’s modulus E curve shows a dramatic decrease of storage modulus while damping (proportional to loss factor) increases dramatically near the glass transition (Tg ¼ 280 8C). In fact, at low temperatures glass shows an elastic behaviour (rigid with no loss) that progressively changes into viscoelastic behaviour. 6.4.4 Modelling Real Solids

The modelling of glass behaviour requires the association of several Maxwell elements and/or Kelvin elements. The simplest model allowing capture of instantaneous and delayed elasticity as well as viscous ﬂow is the Burger association of a Maxwell (G1, h1) element and a Kelvin (G2, h2) element in series. Under an applied constant stress, strain is written (Fig 6.21):6) 1 1 t t ð6:56Þ gðtÞ ¼ to þ 1 exp 2 þ 1 G1 G2 TR TR where TR1 ¼ h1/G1 and TR2 ¼ h2/G2. The solution is plotted in Fig. 6.21.

6)

t = tK = tM, g = gK + gM; to/h1 = M ! gM = to/h1t + to/G1; to = G2gK + h2 K ! gK = to/G2[1 exp(t/TR2)].

111

112

6 Glass Rheology

Fig. 6.20 (a) Dynamic resonance method (DRM) head (a parallelepiped beam is observed at the centre of the head). (Courtesy P. Gadaud, ENSMA Poitiers.) (b) Young’s modulus and damping coefﬁcient Q1 = 2ptan d as a function of a temperature for a GeAsSe chalcogenide glass obtained with a DRM device. (From Le Bourhis et al , 2001a with permission from Elsevier.)

Fig. 6.21 Burger solid and its response to a constant applied stress. On loading under to an instantaneous elastic strain gi, a delayed elastic strain gd and a viscous strain gd appear. On unloading only elastic strain gi and delayed elastic strain gd recover.

6.4 Viscoelastic Response of Glass

Equation (6.56) produces an instantaneous elastic strain (ﬁrst term, gi ¼ to/G1), a delayed elastic strain (second term, gd ðtÞ ¼ ðto =G2 Þ½1 expðt=TR2 Þ) and a viscous strain (third term, gv ðtÞ ¼ to t=TR1 ). The ﬁrst two terms recover on unloading, whereas viscous ﬂow is irreversible. Often used in the literature, anelasticity refers to the instantaneous plus delayed recoverable deformation while viscous ﬂow, in contrast, is not recoverable. Generalized Maxwell and Kelvin models are combinations of several Maxwell elements in parallel or Kelvin elements in series respectively. They were introduced to describe discrete relaxation times. The generalized Maxwell model is written n X tðtÞ ¼ g0 GðtÞ ¼ g0 Gk expðt=TkR Þ ð6:57Þ k¼1

with the relaxation times of the different elements being TkR ¼ hk =Gk . This distribution of relaxation time may be due to a real spatial distribution of regions having different viscosities (because of temperature and composition heterogeneities). More fundamentally, such a distribution can be associated with the fact that the heights of the potential barriers impeding atomic or molecular motions are not equal. We generally only consider the average value while in fact there might be a broad and continuous distribution of barrier heights and hence relaxation times. 6.4.5 Functional Formulation 6.4.5.1 Creep Let us consider the stress being applied instantaneously and take a Heaviside function tðtÞ ¼ to Hðt t j Þ

ð6:58Þ

with H ¼ 0 for t t j < 0

ð6:59aÞ

H ¼ 1 for t t j 0

ð6:59bÞ

Deformation is taken as a function of history (it is history dependent): gðtÞ ¼ Jðt t j Þto

ð6:60Þ

where J is the compliance characteristic of the material. For a Kelvin solid J(t) ¼ go/ so[1 exp(t/TR)]. Now we consider stress is applied with n successive steps: tðtÞ ¼

n X Dt j Hðt t j Þ j¼1

ð6:61Þ

113

114

6 Glass Rheology

Assuming linear viscoelasticity, strain becomes n X Dt j Jðt t j Þ

gðtÞ ¼

ð6:62Þ

j¼1

Equation (6.62) can be generalized to a continuously varying stress as Zt gðtÞ ¼ 0

dtðt0 Þ Jðt t0 Þdt0 dt0

ð6:63Þ

For the case of successive steps and continuously varying stress between steps then one has to add Eqs (6.62) and (6.63). With a single creep measurement, one can theoretically calculate the entire creep compliance. Thereafter, any response can be calculated using this compliance and changing the stress history t(t). There are experimental difﬁculties in imposing a true step stress function and in measuring J(t) at long times. In practice, glass is assumed to have simple thermorheological behaviour. The mechanisms are considered to be independent of temperature, and only the kinetics is changed with the temperature. The creep function at a temperature can be determined from experiments at other different temperatures, the overall evolution with time arbitrarily plotted for a reference temperature (Section 6.4.5.4). 6.4.5.2 Stress Relaxation Using the same approach as for creep we consider strain to be gðtÞ ¼ go Hðt t j Þ

ð6:64Þ

Stress relaxation is written tðtÞ ¼ Gðt t j Þgo

ð6:65Þ

where G is the relaxation modulus of the material. For a Maxwell solid G(t) ¼ so/ goexp(t/TR). For a continuously varying strain we have Zt tðtÞ ¼ 0

dgðt0 Þ Gðt t0 Þdt0 dt0

ð6:66Þ

These relations can be generalised for a three-dimensional loading (Appendix 9). The deviator sij and hydrostatic s stress tensor being determined using the following similar equations: Zt si j ¼ 0

dei j Gðt t0 Þdt0 dt0

ð6:67Þ

6.4 Viscoelastic Response of Glass Tab. 6.5

k

T (s) R 1k

w1k

Shear relaxation times of the Prony series according to Rekhson (1986);

Pn

k¼1

w1k ¼ 1:

1

2

3

4

5

6

19 0.0438

291.9 0.0611

1843 0.0899

11 800 0.2516

49 490 0.2974

171 700 0.2561

Zt sðtÞ ¼ 0

de Kðt t0 Þdt0 dt0

ð6:68Þ

where eij is the deviator strain tensor and e the hydrostatic strain tensor. G(t) and K(t) are the shear and hydrostatic relaxation moduli: GðtÞ ¼ 2Gc1 ðtÞ

ð6:69Þ

KðtÞ ¼ 3Ke ð3Ke 3Kg Þc2 ðtÞ

ð6:70Þ

where ci are the relaxation functions, G and Kg the shear and bulk instantaneous elastic constants and Ke the bulk equilibrium elastic modulus that accounts for both instantaneous and delayed volumetric elasticity. Kurkjian 1963 and Rekhson 1986 proposed the use of generalized Maxwell models in the form of Prony series (Table 6.5) for the shear relaxation function c1(t):7) c1 ðtÞ ¼

n X R w1k expðt=T1k Þ

ð6:71Þ

k¼1

Moreover the hydrostatic relaxation function relaxes much more slowly and is often supposed to be (Guillemet and Gy, 1996). c2 ðtÞ ¼ c1 ðt=10Þ

ð6:72Þ

The Prony series proposed by Rekhson 1986 for the shear relaxation is composed of six different elements with shear relaxation times which are to be considered by their relative contribution (Table 6.5).

7)

This function can be written for a continuous spectrum of relaxation time asRc1(t)= R1 1 0 F(TR)exp(t/TR)dTR with 0 F(TR)dTR=1. Taking p = 1/TR and N(p) = 1/p2F(1/p) allows one to show c1(t) to be the

Laplace transform of N(p): c1(t)= R1 0 N(p)exp(pt)dp. This formalism can be employed to rationalize elastic-viscoelastic correspondence discussed in Section 6.4.5.3.

115

116

6 Glass Rheology

6.4.5.3 Elastic–Viscoelastic Correspondence Let us consider the stress relationship obtained from the functional formulation for a viscoelastic material. We obtain Zt tðtÞ ¼ 0

dg Gðt t0 Þdt0 dt0

ð6:73Þ

Let us compare this relation to that of an elastic solid t ¼ Gg. The elastic–viscoelastic correspondence says that the viscoelastic solution can be generated from the incompressible (n ¼ 0.5) elastic one using a Boltzmann hereditary integral (hereditary for past dependent) with respect to past time from t0 ¼ 0 to the present time t0 ¼ t. This is illustrated as Zt G! 0

d Gðt t0 Þdt0 dt0

ð6:74Þ

This procedure is very useful for complex loading conditions (contact loading for instance; see Appendix 8). As a matter of fact, the solutions to these integral equations are completely dependent on the choice of material relaxation modulus G(t). 6.4.5.4 Superposition Principle (simple thermorheological behaviour) We shall assume that glass shows a simple thermorheological behaviour or, in other words, the mechanisms are independent of the temperature and only the kinetic is changed. Once the behaviour is known at a temperature (so-called reference temperature), it can be determined at any temperature using shift factors f(T) for the relaxation time (Ferry, 1970), or at different times, relaxation curves are derived from another by a change in time scale (Figs. 6.22 and 6.23). Kurkjian 1963 studied extensively glass stress relaxation at different temperatures. Glass rods were ﬁrst stabilized at a given temperature and twisted. The overall results were observed to adjust on a single master curve (Fig. 6.23). This can occur only if all relaxation times characterizing the material have the same temperature dependence and the weighting factors are constant. This implies that all the processes involved in the relaxation have the same activation energy and that the same processes are active at all temperatures. Indeed if a new process appears, the weighting factors must change, altering the shape of the curve. Fortunately, real glasses do exhibit thermorheological simplicity to a high level of approximation. Like Lee et al. 1965 we shall introduce the thermorheological simplicity of glass by using the reduced time deﬁned by Zt j¼

dj

ð6:75aÞ

0

with dj ¼ fðTÞdt0

ð6:75bÞ

6.4 Viscoelastic Response of Glass

Fig. 6.22 Normalized stress as a function of logarithm of time, at seven experimental temperatures (according to Kurkjian, 1963).

Fig. 6.23 Master curve at 473 8C produced from the data obtained at various experimental temperatures (Fig. 6.22; according to Kurkjian, 1963).

117

118

6 Glass Rheology

In general temperature varies and the integral cannot be simpliﬁed. When the temperature is constant, reduced time is proportional to time and is written j ¼ f(T)t. We assume that at any temperature T, the stress relaxation function is cT(t) ¼ cR(j), where cR is the stress relaxation at reference temperature (f(TR) ¼ 1). The shifting procedure can be illustrated in a graph showing the c dependence with log(t). Consider only two different temperatures (reference and studied temperature): cT ðlogtÞ ¼ cR ðlogjÞ ¼ cR ðlog½fðTÞtÞ ¼ cR ðlogt þ log½fðTÞÞ

ð6:76Þ

Then, the simple thermorheological behaviour says that the stress relaxation function at any temperature is obtained in the log scale by shifting the curve by log[f(T)]. A reverse operation consists of determining the behaviour of the glass and shifting the creep functions (so called equivalence between time and temperature) to obtain the master curve evolution with time at a reference temperature (Section 6.4.3; Figure 6.24). Shift factor can be obtained from viscosity data: fðTÞ ¼

hR h

ð6:77Þ

where hR is the viscosity at the reference temperature. Under a continuously varying temperature, reduced time incorporates the varying scale factor (see also Section 6.5). Assuming a Prony series, the reference temperature is to be ﬁxed by the following equation: TR ¼

n hR X R w1k T1k ¼ G k¼1

Then, the relaxation functions can be obtained at any temperature using the shift factor presented above. For instance, for a soda-lime-silica glass, the Prony series is shown in Table 6.5 and is to be taken for a reference temperature of 508 8C with hR ¼ 1.86 1015 Pa s (Guillemet and Gy, 1996).

Fig. 6.24 Shear relaxation function as a function of time for two different temperatures.

6.5 Tempering of Glass

6.5 Tempering of Glass 6.5.1 Introduction

The thermal history of glass has to be carefully controlled in order to design the level of residual stresses. When the material passes through the viscous–elastic domain submitted to a thermal gradient, compressive residual stresses appear at the surface (tensile in the core). Fast cooling rate will allow tempering of the glass while slow cooling rate and annealing of the glass will allow stabilization of the structure and reduction of residual stresses. A tempering set-up comprises either a ventilator or a compressor injecting air through nozzles that reaches the glass surface (Figs. 6.25 and 6.26). A parabolic stress proﬁle showing compressive and tensile zones is represented and is typical of thermal tempering. Figure 6.27 shows a tempered backlight showing signatures of the process (nozzle air marks) since glass photoelasticity allows for thermal residual stress heterogeneities to be observed (see also Chapter 11).

Fig. 6.25 (a) Schematic representation of tempering with nozzles injecting cooling air (grey arrows) and (b) residual stress proﬁle in a thermally tempered glass sheet.

119

120

6 Glass Rheology

Fig. 6.26 Bending and tempering unit. (Courtesy Tamglass Ltd, http://www.tamglass.com/.)

6.5.2 Freezing Theory

Glass tempering prediction is a complex problem since i. thermal transfer involves unknowns, ii. thermal and structure histories are complex, and iii. triaxial stress build up is to be determined.

Fig. 6.27 Nozzle photoelastic signatures (due to tempering) are observed here on a backlight (they correspond to residual stress heterogeneities and are better observed at dawn; see also Chapter 11).

6.5 Tempering of Glass

In a ﬁrst approach, Adams and Williamson 1920 proposed a thermoelastic model to determine the stresses in a glass sheet cooled at a constant rate cR. The outer layers of the glass sheet will become rigid ﬁrst, then as the inside cools, it tries to shrink, but is restrained by the rigid outer layers. Then, a simple representation of the tempering is to separate the sheet into three parts (the two surfaces and the core) and allow viscous ﬂow in the core until it freezes (Fig. 6.28). A thermal gradient appears throughout the sheet. On passing the glass transition with cooling down to room temperature, the difference in displacements between the surface and the core cannot be accommodated any longer and residual stresses build in. If the glass is cooled at a constant rate, the temperature proﬁle is parabolic and temperature variation through the sheet (between the surface and the centre) is written DT ¼ t2H cR cP =8k

ð6:78Þ

where tH, cR, cP and k are the thickness of the sheet, the cooling rate, the speciﬁc heat and thermal conductivity of the glass respectively. The biaxial stresses are sðzÞ ¼

Ea ½T TðzÞ 1n

Fig. 6.28 Schematic representation of residual stress generation in a thermally tempered glass sheet. Viscous ﬂow is possible over Tg. Thermal gradient builds in. On passing the glass transition and obtaining uniform temperature, stress builds in.

ð6:79Þ

121

122

6 Glass Rheology

where T is the mean temperature, T(z) the temperature at position z, E the Young’s modulus, n the Poisson ratio (E/(1 n) is often called the biaxial modulus) and a the thermal expansion coefﬁcient of the glass. When the temperature distribution is parabolic, maximum tensile stress appears at the centre of the glass sheet: sc ¼ as E=3ð1 nÞDT ¼ At2H cR

ð6:80Þ

This very simple relation shows that a thicker sheet yields larger thermal gradient and hence larger residual stresses. The effect of using larger cooling rate is also straightforward leading to more tempering. It can be anticipated that tempering of thin glasses is difﬁcult since it requires technology for large cooling rates. One must also consider that such tempering may mark the glass as strong air ﬂows have to be injected through the nozzles which may deform the glass surface and damage the optical quality. The three-part model can to be extended to a continuous model allowing for a parabolic proﬁle of stresses to be obtained (Aben and Guillemet, 1993; Figure 6.25). Equibiaxial stress ﬁeld is written " # 1 z 2 ð6:81Þ sx ¼ sy ¼ 3sc 2 3 tH where sc is the tensile residual stress at the sheet centre (at z ¼ 0, core stress). At the surface, residual stress is ss ¼ 2sc. Stress is null for z/tH ¼ 0.3 or at a distance of 1/ 5tH from the surface. 6.5.3 Stress Relaxation

The ﬁrst approach described above supposes that stresses are frozen at Tg while stress relaxation happens at characteristic times that depend on the temperature because of the viscous–elastic behaviour of glass. Supposing glass has a simple thermorheological behaviour (Section 6.4.5.4), we consider reduced time and have Zt j¼

dj

ð6:82Þ

hR 0 dt h

ð6:83Þ

0

with dj ¼

Stresses build in and partially relax because of the viscoelasticity of glass. Stresses are written assuming an equibiaxial stress ﬁeld (subscript B, this is to be reconsidered close to an edge or a hole, see Chapter 11): Zt sðz; tÞ ¼ 0

GBR ðj j0 Þ

q ½eðt0 Þ as Tðz; t0 Þdt0 qt0

ð6:84Þ

6.5 Tempering of Glass

where GBR is the relaxation modulus for biaxial stress which is deduced from the shear and hydrostatic relaxation moduli, e(t0 ) is the strain at time t0 which is the same for all values of z (the deviation of the induced thermal strains from the uniform actual value generates the stresses in the different layers of glass) and is deﬁned by the equation of mechanical equilibrium, as is the thermal expansion coefﬁcient for glass and T(z, t0 ) is the temperature at position z and time t0 . The viscoelastic approach was revealed to yield a non-negligible discrepancy between modelling and experiments (Gardon, 1978; Narayanaswamy, 1978), because the rapid cooling of glass causes also its structure to deviate considerably from the stabilized (equilibrium) state. Hence realistic models have to consider the glass structural relaxation in order to be more predictive (Section 6.5.4). As a matter of fact, R&D numerical tools incorporate stress and structure relaxations. 6.5.4 Structural Relaxation

Not only stress relaxation has to be considered when modelling glass tempering but also the structural relaxation, since the glass structure is known to be out of equilibrium. This issue was addressed ﬁrst by Acloque (1951). At a given temperature glass will tend to approach the liquid conﬁguration. This indeed happens without applying any stress to the material. When a supercooled liquid freezes it departs from the liquid curve (see for instance Section 6.2.1). Then, the liquid freezes in a less dense conﬁguration than the supercooled liquid would present at the same temperature. When time is allowed for the glass to rearrange it will progressively tend to the denser liquid conﬁguration and hence glass structure is expected to change with time. At room temperature the time scale is beyond the human time scale and hence structural relaxation of glass is not detected. The situation is different when the glass is set at a higher temperature. Some examples are shown in Fig. 6.29 where two pieces of glass were set at the same temperature while previously being stabilized at two different temperatures (Moynihan, 1996). The glass that was stabilized at a temperature higher than that imposed relaxes more rapidly than the one that was stabilized at a lower temperature. The ﬁrst glass presents a more open structure as it was stabilized at a higher temperature and shows a greater average volume, and hence a reduced resistance to conﬁgurational changes. In contrast, the glass stabilized at a lower temperature shows a denser structure and hence more resistance to structural changes. When tempering the glass, this phenomenon has to be taken into account as well. In the transformation range, the glass no longer has enough time to reach its equilibrium state at each temperature because of its high viscosity. Glass structure will depend on tempering conditions (cooling rates; Gardon, 1978; Narayanaswamy, 1978; Scherer, 1982, 1996; Guillemet, 1990; Aben and Guillemet, 1993). Markowsky and Soules 1984 proposed a way to predict the structure of glass as a function of its thermal history using the concept of ﬁctive temperature ﬁrst introduced by Tool 1946. Contrary to a liquid whose structure is known from its actual temperature, glass structure can be obtained knowing both the temperature T

123

124

6 Glass Rheology

Fig. 6.29 Structural relaxation of two pieces of glass stabilized at two different temperatures (according to Moynihan, 1996).

and the ﬁctive temperature Tf, that is, its instantaneous temperature and its prior history. When glass approaches transition, equilibrium state cannot be reached because of the elevated viscosity. By deﬁnition, the ﬁctive temperature Tf of a glass corresponds to the temperature of the liquid which is in the same structural state as the glass under study. In a stabilized glass, Tf ¼ T while in a non-stabilized glass Tf 6¼ T. In practice, the ﬁctive temperature corresponding to the state A of a glass is represented in Fig. 6.30 by point B and can be obtained by taking the line parallel to the expansion curve of the solid and determining its intercept with the expansion

Fig. 6.30 Volume–temperature cooling curves showing ﬁctive temperature geometrical determination (l and g, liquid and glass domains; A, the point at which ﬁctive determination is made; B, the intercept of the expansion curve of the liquid and the line parallel to glass expansion curve passing through A). The temperature at B is by deﬁnition the ﬁctive temperature at point A.

6.5 Tempering of Glass

curve of the liquid. A glassy state can be viewed as a liquid-like state which has been frozen in. The liquid-like structure is then known from the ﬁctive temperature of the liquid-like structure. When a supercooled liquid is cooled more rapidly, the glass freezes at a higher temperature, the liquid-like structure corresponds to a higher temperature and hence the ﬁctive temperature is higher. Let us consider again Fig. 6.29. The glass that was stabilized at a higher temperature shows a higher ﬁctive temperature, and when forced at a lower temperature it relaxes to a liquid-like structure presenting a lower ﬁctive temperature. Then, the second glass ﬁctive temperature will instead increase progressively. Fictive temperature evolution depends on thermal history and this is the reason for the difference between the two glass behaviours. The glass presenting a higher ﬁctive temperature that has a more open structure relaxes more rapidly. Markowsky and Soules 1984 proposed an algorithm to determine the ﬁctive temperature evolution. Structural evolution being a nonlinear phenomenon, an iterative computational scheme was proposed. Both stress and structural relaxation phenomena are to be taken into account in the modelling of glass tempering, structural relaxation accounting for approximately 25 % of the total residual temper stresses (Narayanaswamy, 1978; Rekhson, 1986). Shear stress relaxation happens at characteristic time scaling with TR while structure is accepted to relax about ten times slower (KTR 9TR; Guillemet, 1990; Gy et al., 1994; Guillemet and Gy, 1996). A Prony series is then adopted again with characteristic relaxation times shifted by approximately one order of magnitude. Alternatively, a simpler KWW function often ﬁts well the relaxation of glasses (Debast and Gilard, 1963; Scherer, 1996). Let us consider an increment in time dt; from a given step numbered n 1 to the following step numbered n, we have dj ¼

hR dt h

ð6:85Þ

j being referred to as the reduced time (Aben and Guillemet, 1993) and subscript R indicates the reference temperature. Here, the viscosity function has to capture structural relaxations (ﬁctive temperature). This is obtained from the Adam and Gibbs theory of cooperative relaxations (Section 6.1.3.4) and is written hðT; Tf Þ ¼ ho exp

B T½1 ðTo =Tf Þ

ð6:86Þ

When glass is at an elevated temperature its structure is at equilibrium and is that of the melt so that Tf ¼ T and we get a VFT expression for the viscosity. Close to glass transition, glass freezes progressively, Tf departs from T and viscosity is affected. After each increment of time the ﬁctive temperature (structure) can be calculated following the Markowsky and Soules (1986) algorithm that suggests the use of ‘partial ﬁctive temperatures’ Tfk and a Prony series: Tfk;n ¼ T n ðT n Tfk;n1 Þexpðdj=Ktk Þ

ð6:87aÞ

125

126

6 Glass Rheology

Tf ¼

6 X wk Tfk

ð6:87bÞ

k¼1

Tf ðz; 0Þ ¼ Ti

ð6:87cÞ

where Ti is the initial temperature. Figure 6.31 shows the ﬁctive temperature (structure) evolution following this algorithm on cooling and then re-heating a glass at the same rate and then on cooling the same glass at a higher cooling rate. It can be seen that the two curves obtained with the same rate (on cooling and heating) coincide only well below Tg and well above it. In fact, hysteresis results from structural relaxation and can be detected experimentally using DSC as shown in Fig. 6.32 and care has to be taken in analysing experimental results (Ho¨hne et al., 1996). In Section 6.2.1, we actually focus on one single route (cooling path). The actual behaviour can be commented on in view of the discussion regarding Fig. 6.29. In fact, on heating the glass the starting point is a liquid-like structure at a lower ﬁctive temperature than the supercooled liquid following the cooling curve. This means that the starting point for the heating curve corresponds to a denser structure and rearrangement will be slower. Then the heating curve will always be below the cooling curve (for the same cooling and heating rate). Note also that on cooling a glass more rapidly, a larger ﬁctive temperature is obtained, or a less dense glass (Fig. 6.31; silica shows an anomaly with a reverse trend).

Fig. 6.31 Structure (ﬁctive temperature, Tf ) as a function of temperature on cooling and heating a glass piece. For comparison fast cooling route is shown and yields a glass with a higher ﬁctive temperature (less dense glass).

6.5 Tempering of Glass

Fig. 6.32 DSC heating curves of annealed and quenched ¨hne et al., 1996). Note relaxation glasses (according to Ho peaks, the higher being observed for annealed glass resulting from the non-equilibrium nature of glass. DSC analysis should be considered with care since it would appear that the conventional glass transition temperatures of quenched glass is lower than that of annealed glass while it is the contrary in fact.

The calculation of residual stresses requires consideration of the thermal expansion mismatch between the liquid and the glass when the actual structural state is to be determined as described above. Assuming equibiaxial stress ﬁeld (subscript B), stress is given by a formula incorporating structural relaxation through the ﬁctive temperature parameter: Zt sðz; tÞ ¼ 0

GBR ðj j0 Þ

q ½eðt0 Þ as Tðz; t0 Þ ðal as ÞTf ðz; t0 Þdt0 qt0

ð6:88Þ

where GBR is the relaxation modulus for biaxial stress, e(t0 ) is the strain at time t0 which is the same for all values of z and is deﬁned by the equation of mechanical equilibrium, as and al are the thermal expansion coefﬁcients for glass and liquid respectively and T(z, t0 ) is the temperature at position z and time t0 (we ignore edges here). Figure 6.33 shows the amplitude of core tensile residual stresses that build in under different experimental conditions. It shows a very good agreement between the calculated and experimental values allowing for great precision in the predictions. Figure 6.33 shows that, in fact, to generate residual stresses the initial temperature of the glazing needs to be over the transition temperature. This is not unexpected, since cold glass is elastic and therefore cannot be tempered. The potential for temper is fully developed only for quenching from temperatures well above the transition

127

128

6 Glass Rheology

Fig. 6.33 Dependence of residual mid-plane tensile stress (sc ¼ s(0, 1)) on the initial temperature Ti of a glass and on the heat transfer h (W m2 K1); thickness 6.1 mm, natural convection corresponds approximately to the lowest curve (according to Narayanaswamy, 1978). They actually used the viscosity function h(T, Tf ) ¼ ho exp {B[(x/T) + (1 x)/Tf ]} with x 0.5 instead of Eq. (6.86).

temperature. Also higher heat transfer (air ﬂow) induces higher plateau-level temper residual stresses and increases the temperature at which the plateau is reached. When quenching the glass, it is important not to mark it by nozzles air impact. In R&D, it is important to consider also the complex geometry and thermal history of the glazing (holes, edges) and containers. This requires numerical methods and adjustment to observed results. These complex geometries can be considered using ﬁnite element analysis (FEA; Appendix 11). It is beyond the scope of this book to describe these methods in detail. It has been realized that before designing a new tool to produce for instance backlights, different series of numerical experiments will allow one to approach the optimized tool. This tool once fabricated shows great potentiality to produce a glazing prototype close to the demanded one. This of course allows for economical gains since many experimental tests are saved.

6.6 Transient Stresses

The simple gradient model shown in Fig. 6.28 can also be used to model thermal shock (see Chapter 2). When the glass sheet is annealed at T < Tg the material

6.6 Transient Stresses

remains elastic (i.e. no viscous ﬂow happens). On cooling, transient compressive and tensile stresses build up and vanish when uniform temperature is reached. Stress is written s ¼ as E=ð1 nÞDT

ð6:89Þ

where DT is the temperature variation through the sheet (between its surface and its centre), as the thermal expansion coefﬁcient of the glass, E the Young modulus and n the Poisson ratio. These transient tensile stresses at the surface are dangerous for the glazing since fracture may originate from a superﬁcial ﬂaw when it is under tension (see Chapter 7). As a matter of fact, thermal shock with DT < 0 (on cooling down) is the most dangerous, as illustrated in Fig. 6.34, since tensile stresses develop at the surface where ﬂaws are known to exist (see Chapter 8). Much greater temperature differences can be withstood in sudden heating than in sudden cooling because only when cooling is the surface placed under tension. Also, thermal endurance can be greatly increased by a toughening process which places the surface under compression. Transient stresses are proportional to Young’s modulus and thermal expansion coefﬁcient. In Chapter 2, we discussed extensively the way to select materials in view of relevant parameters that are the thermal expansion, the elastic modulus and the ultimate stress at fracture. We showed the potential of silica-rich glasses and borosilicates for applications requiring a high resistance to thermal shocks.

Fig. 6.34 Schematic representation of the transient stress generation in a glass sheet under thermal shock (DT < 0, T < Tg) showing transient tensile stress at the surface and transient compressive stress in the centre. When temperature is uniform, transient stresses vanish.

129

130

6 Glass Rheology

Transient stresses should be very carefully considered also during the tempering process. Their partial relaxation leads to permanent stresses as discussed above. Under fast cooling there is a risk of the glass breaking under transient stresses. As discussed in Chapters 8 and 10, manufacturers control carefully production lines in order to avoid any abrasion of the glass surface (from the rollers, while packing) and this is surveyed up to the tempering operations. These procedures permit a gain in production yield as transient stress-induced breakages are avoided. The determination of transient stresses when the transition temperature is reached is more complex than when T < Tg. As reviewed above, for such temperatures stress and structural relaxation of the glass have to be taken into account.

6.7 Chemical Tempering of Glass 6.7.1 Introduction

Chemical tempering is applied for dedicated applications like aeroplane and highspeed train windshields, requiring high safety levels, and for thin glazing for which conventional thermal tempering would mark the surface or would not allow for sufﬁcient strengthening. Although production yields are much less important, chemical tempering has to be used to achieve very high level of stresses required in the range of 500–600 MPa. The treated depth of glass (diffusion length) is reduced to hundreds of micrometres. The glass to be treated is immersed in a salt bath containing cations the radii of which are larger than those to be exchanged in the glass (Fig. 6.35). Ion exchange induces compression at the glazing surface. Generally, the

Fig. 6.35 Chemical tempering principle.

6.7 Chemical Tempering of Glass

cations are alkali metal ions since they diffuse in glass much more rapidly than any other ions (Appendix 13). For instance, a glass containing sodium is strengthened by immersion into a potassium salt bath (generally KNO3). To enhance diffusion elevated temperatures (400–500 8C) are used for the treatment. Unfortunately, these temperatures, while being below the transition temperature of the glass, are high enough for stress relaxation to take place and this phenomenon balances diffusion effects in common glasses. Therefore, aluminosilicate (ALS) glasses were developed to replace soda-lime-silica (SLS) glasses because alkali metal diffusion is more rapid in ALS glasses while viscous relaxation at treatment temperature is slower. Both effects allow for achieving higher stress levels. Incidentally, as the viscosity of ALS glasses is larger than that of SLS ones at the same temperature (Fig. 6.2), ALS glass fabrication is more difﬁcult and expensive than that of SLS glass. 6.7.2 Ion Exchange and Stress Build-Up

The concentration of introduced ions can be calculated using Fick’s diffusion law. As detailed in Appendix 13 since surface concentration cs remains approximately constant, concentration c(z, t) at depth is written 0 z cðz; tÞ ¼ cs 1 erf pﬃﬃﬃﬃﬃ 2 Dt

ð6:90Þ

where z0 ¼ tH/2 z is the distance to the surface, cs the concentration at the surface, D the coefﬁcient of interdiffusion between the two kinds of atoms and t the immersion time. We shall assume in a ﬁrst step that no stress relaxation takes place at the bath temperature. The biaxial stresses are sðzÞ ¼

EB ½hci cðz; tÞ 1n

ð6:91Þ

where hci is the mean concentration of the exchanged ions, c(z, t) the concentration at position z and time t, E the Young modulus, n the Poisson ratio, B the ion exchangeinduced dilation coefﬁcient and t the total exchange time. B is analogous to the thermal expansion coefﬁcient in that the concentration c replaces the temperature. Thus B is the linear strain produced per unit exchange of ions (Tyagi and Varshneya, 1998): B¼

1 dV 3V dc

ð6:92Þ

A typical residual stress proﬁle is shown in Fig. 6.36. As compared to thermally tempered glazing only a thin layer is under compressive stresses (Fig. 6.25). Chemical tempering allows for treating more complex glass shapes than thermal tempering. However, care has to be taken so that the treatment penetrates the surface over ﬂaw extension (100 mm; see also Section 7.7.2).

131

132

6 Glass Rheology

Fig. 6.36 Residual stress proﬁle in a chemically tempered glass sheet.

6.7.3 Stress Relaxation

As mentioned above, stress relaxation may take place at treatment temperatures. This phenomenon is now considered. One has to make further assumptions: (i) diffusion does not modify the viscosity of the superﬁcial layers and (ii) relaxation happens at the treatment temperature and we neglect relaxation while cooling rapidly the specimens. Assumption (i) is quite realistic while assumption (ii) allows for using time instead of reduced time (we neglect structural relaxation). Then, stress relaxation is written (Shen and Green, 2004) Zt sðz; tÞ ¼ 0

GBR ðt t0 ÞB

q½hci cðz; t0 Þ 0 dt qt0

ð6:93Þ

where GBR is the biaxial relaxation function. 6.7.4 Engineered Stress Proﬁle Glasses

Recently, a new approach for chemical strengthening has been proposed by Green et al. 1999. The key feature is to carefully design the residual stress proﬁle in such a way that the maximum compression is moved away from the external surface while stress gradient is carefully controlled in the surface region (Fig. 6.37). These glasses have been termed engineered stress proﬁle (ESP) glasses. Normally, ion-exchanged glasses are processed to maximize the magnitude of the surface compression and the extent over which it acts (within economic constraints). In ESP glasses, it is not the overall depth of the surface compression that is important but rather the form of the stress proﬁle in the near-surface region. In fact, cracks are ‘trapped’ within the surface region (Fig. 6.38). These glasses show multiple cracking as a warning of the ﬁnal failure. The processing may not necessitate deep compressive layers. This is economically attractive as it may lead to

6.7 Chemical Tempering of Glass

Fig. 6.37 Stress proﬁle in ESP glazing obtained after a two-step ion exchange. (From Abrams et al., 2003, with permission from Elsevier.) For comparison a single ion exchange proﬁle is shown; note even for single ion exchange there is surface stress relaxation. This is avoided at low temperature with smaller treated depth (Guillemet and Gy, 1996).

Fig. 6.38 Multiple surface cracks in a two-step ion-exchanged glass tested under four-point bending. Loading axis is perpendicular to crack direction (HF acid etching was used to widen cracks for better visibility; the white bar is 1 mm long). (From Abrams et al., 2003, with permission from Elsevier.)

133

134

6 Glass Rheology

Fig. 6.39 Weibull distribution of ESP glass compared to untreated glass. (From Abrams et al., 2003, with permission from Elsevier.)

reduced processing times and, thereby, give rise to energy savings. The treatment is in two steps. In the ﬁrst step, molten KNO3 is used as a salt bath (at a temperature of 450 8C) to treat the aluminosilicate glasses. Here again soda-lime-silicate glass is difﬁcult to ion exchange, as exchange depths are limited by slow diffusion rates and stress relaxation. Therefore ALS glasses are preferred. A second exchange uses a mixed KNO3/NaNO3 salt bath at some lower temperature (400 8C). The effect of the second exchange is to make the stress gradient steeper near the surface and control the position of maximum compression. Another important issue for these glasses is the low strength variability while improving the average strength, as illustrated in Fig. 6.39. Strength variability will be discussed in more detail in the next chapter. While annealed silicate glasses were tested in the Weibull modulus range of 5–10, ESP Weibull modulus may exceed 60. Both strength and variability are important issues as regards glass application. To the author’s knowledge, these ESP glazings have not met commercial success.

135

7 Mechanical Strength of Glass Glass failure at temperatures below the glass transition is brittle and statistical. Fracture happens at much lower stresses when the specimen is loaded under tension than when loaded under compression (see also Appendix 10) and is of utmost importance for glass applications.

7.1 Theoretical Strength

Orowan 1949 ﬁrst proposed a rupture criterion in terms of elastic strength, surface energy (two new surfaces being generated upon fracture) and atomic structure. Fracture was expected to happen under tensile stress sth determined as (Appendix 5) rﬃﬃﬃﬃﬃﬃ Ez sth ¼ ro

ð7:1Þ

where E is Young’s modulus and z the surface energy (z is usually identiﬁed with the free surface energy of the cleavage surface, although this is still under debate; Mattoni et al., 2005). Equation (7.1) shows that stress at fracture increases together with surface energy and Young’s modulus. Taking for a soda-lime-silica glass E ¼ 70 GPa, z ¼ 0.6 J m2 (Table 7.1) and ro ¼ 0.15 nm (Si–O distance; see Section 5.2) one ﬁnds a theoretical strength sth as high as 16 GPa. Unfortunately, this value is well above experimental and usual values (50 MPa for ﬂat glass). Such a huge discrepancy was attributed to the presence of ﬂaws at the glass surface as discussed in detail below (see also Appendix 5). In fact, it was observed that strength was much dependent on the glass object. For instance, glass ﬁbres show a much higher strength than ﬂat glass. It became more and more obvious that ﬂaws (or defects) were responsible for the deteriorated strength of glass as compared to the estimated strength.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

136

7 Mechanical Strength of Glass Toughness, Young’s modulus and surface energy2) values for different glasses (Aben and Guillemet, 1993; Barton and Guillemet, 2005). Tab. 7.1

Glass

Kc (MPa m1/2)

E (GPa)

0.74–0.81 0.72–0.82 0.75–0.82 0.85–0.96 0.62–0.73

73 70–74 64–89 83–91 58–65

Silica Soda-lime-silica Borosilicate Aluminosilicate Lead–silicate

z (J m2) 0.65 0.4–1 0.63 0.63 0.44

7.2 Tensile Resistance of Glass

The simplest way to test a glass in tension is in principle to pull a rod or ﬁbre, although one must note that in practice there are several difﬁculties in gripping the specimens. Three- and four-point bending is often used as well as biaxial ﬂexure and brasilian or diametral compression tests (Zhou et al., 2006). The latter allows generation of a tensile zone into the specimen (Le Bourhis, 1996). Except for ﬁne and long ﬁbres (Appendix 6) where gripping problems can be solved, one should make the central and tested zone smaller in diameter on using uniaxial tensile tests so that failure happens from the ﬁbres and not at the grips. Glass is a so-called brittle material at temperature well below Tg and deforms elastically until fracture (Fig. 7.1). In the elastic domain (domain 1) the uniaxial tensile loading curve s(e) of a glass specimen is then linear.1)

Fig. 7.1 (a) Tensile stressed specimen; (b) s–e tensile curve. Domain 1, slope is Young’s modulus E. Domain 2 corresponds to fracture. sf and ef ¼ sf/E are the stress and strain at rupture respectively. 1)

2)

Deviation from Hooke’s law is observed under elevated strains (10%). Glass becomes either stiffer (silica, germania) or less stiff (SLS; Hillig, 1962; Krause et al., 1979). Such elevated strains can be commonly obtained in coated ﬁbres (Shiue et al., 1996). Native surface (see Chapter 5). Considering that Gc ¼ Kc2/E is the energy release on fracture,

one ﬁnds with E ¼ 70GPa and K ¼ 0.7 MPa m1/ , Gc ¼ 7 J m2, that is, one order of magnitude larger than the actual value. This discrepancy is attributed to the rearrangement (relaxation) of the surface after breakage. Another reason might be the dissipation of energy in the plastic zone conﬁned at the crack tip (see Section 7.4). 2

7.2 Tensile Resistance of Glass

Stress s is written s ¼ Ee

where e is the elastic strain and E the elastic modulus (Young’s modulus). A larger value of E means a stiffer material, that is, a larger resistance to elastic deformations. While the material deforms along the loading axis, also a side deformation is induced the amplitude of which depends on the Poisson ratio (Appendix 9). Elastic modulus depends on glass composition and reﬂects both the interatomic bonding strength and connectivity of the network (packing density). The moduli of glasses are observed to increase together with the glass transition temperature (Fig. 7.2a). Metallic glasses

Fig. 7.2 (a) Young’s modulus E (at 293 K except for amorphous ice at 77 K) as a function of transition temperature (according to Rouxel, 2006); (b) Young’s modulus E of silicate glass as a function of modiﬁer concentration (according to Scholze, 1991).

137

138

7 Mechanical Strength of Glass

while showing transition temperatures below those of oxide glasses show much higher Young’s modulus because of their higher packing density (Cg 0.7 as compared to 0.5 for common glasses; Chapter 5). When modiﬁers are introduced into the oxide glasses network, these atoms locate in the excess volumes while they weaken the network inducing NBO. These two phenomena play opposite roles. The resulting trends in silicate glass are shown in Fig. 7.2b demonstrating that the latter phenomenon is predominant since moduli of silicate glasses are observed below that of silica whatever the introduced alkali. The softening of the glass is more pronounced for a modiﬁer having less Dietzel ﬁeld intensity or for a modiﬁer that is expected to show weaker interaction with oxygen (see Chapter 5) as seen in Fig. 7.2b. In contrast to a modiﬁer, B2O3 oxide participates in the glass network and allows for maintaining and or even increasing Young’s modulus (Livshits et al., 1982). The elastic domain is terminated by catastrophic failure, the area under the linear curve corresponding to the elastic energy. Metallic glasses allow large elastic energy storage since they present elevated strengths. Failure is a dramatic event that has to be prevented. As discussed in Chapters 6, thermal and chemical tempering have been developed to strengthen glass articles. This issue is discussed in Section 7.7. In practice, thestress ﬁeld is much more complexthan in thespecimen studiedhere underuniform and uniaxial tensile stress. Fracture will happen in tensile stressed zones. Hence, it is of utmost importance to understand fracture in order to improve strength and predict the domain where glass articles can be used safely. As we discuss now, fracture depends on intrinsic properties but more importantly on extrinsic ones (process-induced and damage-induced ﬂaws) that make the problem very complex. Having all these parameters in mind, ﬁnite element analysis (FEA) can be carriedoutto predict the behaviour of glazing under realistic and complex loading conditions (Appendix 11). Failure originates from a defect in the glass generally at the surface of the specimen. We reject here bubbles as an origin since these can be avoided nowadays in industrial processes thanks to ﬁning or control operations (Chapters 10 and 11). As stated above, when we assume there is no defect in the glass and fracture originates from individual bonds, then tensile strength values are predicted to be much higher than those observed (Section 7.1 and Appendix 5). In fact, fracture starts at a critical defect or ﬂaw and further propagates. The ﬂaw at the origin of fracture can be easily detected in a ﬂat glass among the broken pieces because it is surrounded by a smooth mirror zone (Fig. 7.3) the extension of which allows empirical determination of the level of stress at failure (Aben and Guillemet, 1993; Carre´, 1996). This phenomenon has been of much help in detecting the origin of spontaneous fracture and to develop a treatment against NiS inclusions instability (Chapter 9; Barry et al., 1998). Stress at pﬃﬃ rupture is determined from sr ¼ M= r , with M the mirror constant and r the mirror radius. M is about 2 MPa m1/2 for a silico-soda-lime glass. This equation is of considerable practical importance since it allows estimation of fracture stress without having to measure it directly. This is very useful in complex shaped glass articles. In Fig. 7.3 the superﬁcial origin can be easily located at the glass edge surface (on the top surface shown in the photograph). The crack expands ﬁrst at a low speed creating ﬂat or mirror-like surfaces. At higher speeds, rougher, less reﬂective surfaces are formed, a ‘mist’ area being observed around the mirror zone. Finally very rough and irregular

7.2 Tensile Resistance of Glass

Fig. 7.3 Origin of fracture observed at the centre of the mirror zone (white bar is 1 mm long).

faceted surfaces form the so-called ‘hackle’ area. Further expansion of the crack yields crack branching that is a multiplication of the number of cracks. Surface origin of fracture is further conﬁrmed by etching the glass surface (Pavelchek and Doremus, 1974). It was also realized for a long time that a ﬁre-ﬁnished surface presented a higher strength than a polished one although this effect was not permanent, because of further surface damage after a period of time. Experiments carried out with hydroﬂuoric acid (HF) reveal that strength does not increase much when etch depth is less than 1–2 mm (Doremus, 1994). As the etch process is continued, some samples show great strength presumably because they are etched free of original ﬂaws and fracture starts from shallow ones. The way superﬁcial ﬂaws are generated in a ﬂat glass under a contact is extensively discussed in Chapter 8. Flaw generation may happen in the production line and in use. The nature of the ﬂaws in glass ﬁbres is more controversial. It is observed that ﬁbre strength approaches the ultimate strength and hence ﬂaws are to be searched for at the microstructural scale. They might be microscopic bubbles which are difﬁcult to eliminate. Fining period (Chapter 10) would be too short as compared to the long period of time required to eliminate the smallest bubbles that are the slowest in rising to the melt surface (Appendix 4). Melting or ﬁning operations are continued until visible bubbles are detected but invisible bubbles might still remain. Moreover, the glassy state presents a liquid-like structure, with a characteristic ﬁctive temperature (Chapter 6) close to the glass transition temperature, or a structure frozen at the glass transition. The glass presents, as detailed in Chapters 5 and 6, an open structure giving rise to microscopic ﬂaws. Moreover, glass ﬁbre is quenched at much larger cooling rates than a ﬂat glass because of a higher surface to volume ratio. Fibre ﬁctive temperature is hence higher than that of a ﬂat glass and presents a more open structure. Let us consider a specimen containing a ﬂaw of size 2a loaded under a uniform tensile stress s (Fig. 7.4). It will fail when stress concentration (stress intensity factor, SIF) pﬃﬃﬃ K ¼ sY a

ð7:2Þ

139

140

7 Mechanical Strength of Glass

Fig. 7.4 Schematic representation of a specimen under tensile loading containing a ﬂaw with extension 2a. Tab. 7.2

Y for most used crack geometry.

Y pﬃﬃﬃﬃﬃﬃﬃ ðpÞ pﬃﬃﬃﬃﬃﬃﬃ 1.12 ðpÞ pﬃﬃﬃﬃﬃﬃﬃ 2/ ðpÞ

Crack geometry Straight crack in inﬁnite specimen Edge crack in semi-inﬁnite specimen Penny crack in inﬁnite specimen

reaches a critical value called fracture toughness Kc that is related to Young’s modulus pﬃﬃﬃﬃﬃﬃﬃﬃ and surface energy by Kc ¼ 2Ez.3) Y is a geometrical factor depending on the ﬂaw pﬃﬃﬃﬃ geometry that can be found in Sih (1972) and Schzalke (1981). We take usually Y ¼ p valid for a straight crack in an inﬁnite specimen (Table 7.2). Equation 7.2 is written at failure as pﬃﬃﬃ Kc ¼ sf Y a ð7:3aÞ or Kc sf ¼ pﬃﬃﬃ Y a

ð7:3bÞ

The criterion of Eq. (7.3a) corresponds to an energy balance between the energy required to form two surface energy 2za and that elastically released Ya2 s2 =2E as detailed below. Equation (7.3b) shows that fracture stress amplitude increases with the toughness and decreases with the ﬂaw size. We assume that there are no residual stresses (glass being fully annealed). Otherwise, these contribute negative stress intensity factor when compressive 3)

This relation can be rewritten in terms of critical pﬃﬃﬃﬃﬃﬃﬃﬃﬃ mechanical energy release rate Gc: Kc ¼ Gc E (Lawn, 1993). Gc is the energy required to create two new fracture surfaces and for ideally brittle materials is 2z, where z is the surface energy per unit area. Plane stress conditions (for a thin

plate; see also Appendix 9). Under plane strain conditions (for a thick plate) rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Gc E Kc ¼ 1 v2

7.3 Stress Concentration and Griffith Energy Balance

Fig. 7.5 Schematic representation of the three modes of fracture, namely modes I, II and III.

(Kr < 0; see Section 7.7). Furthermore, we considered mode I corresponding to the opening of the ﬂaw that is most commonly observed as compared to modes II and III corresponding respectively to sliding and ‘tearing’ (Fig. 7.5). From here onward, we only consider mode I and note the fracture toughness Kc. Table 7.1 reports the toughness value at room temperature for different oxide glasses. These values are within a small range 0.7–0.8 MPa m1/2 (see also Chapter 2 for comparison with other materials). In contrast, metallic glasses show high toughness 50 MPa m1/2 and can be deformed at low temperature ( b) is

141

142

7 Mechanical Strength of Glass

Fig. 7.6 Strength sf as a function of critical ﬂaw dimension a (Kc ¼ 0.7 MPa m1/2, Y ¼ Hp). Damaging the glass surface yields reduced performances (see also Chapter 8).

present in a beam submitted to uniform tensile stress s. The ﬂaw concentrates stresses at the points of minimum curvature, and the maximum stress s0 is given by s0 ¼ sð1 þ 2a=bÞ

ð7:4Þ

If one considers a shape factor a/b of about 4.5, Eq. (7.4) tells us that stress concentration reaches s0 /s ¼ 10. Hence, the stress s0 at the minimum curvature is one order of magnitude larger than the uniform applied stress s. This simple calculation shows that stress concentration may reach very high values when the ﬂaw

Fig. 7.7 Elliptical ﬂaw of semi-axes a and b in a beam under uniform tensile stress s.

7.3 Stress Concentration and Griffith Energy Balance

tip becomes sharper. Fracture will then extend at the ﬂaw tip and further propagate until specimen fracture. 7.3.2 Energy Balance

Further understanding of fracture is accomplished considering the total energy of the fractured specimen U. U is the sum of the mechanical Um and surface Us energies: U ¼ Um þ Us

ð7:5Þ

When fracture propagates a distance da the energy change is dU ¼ dUm þ dUs ¼ Gda þ dUs

ð7:6Þ

where G is the mechanical energy release and dUs the variation in energy induced by creation of new surfaces. Equilibrium is written dU=da ¼ 0 ¼ Gc þ dUs =da

ð7:7Þ

where Gc is the critical mechanical energy release. Considering, as Inglis (1913) did, an inﬁnitely narrow elliptical ﬂaw (b ! 0), we have per unit width along the crack front (in fact two fronts) Um ¼ G¼

pa2 s2 E

dUm dðpa2 s2 =EÞ ¼ 2da 2da

ð7:8Þ ð7:9Þ

while Us ¼ 4az

ð7:10Þ

Total energy is U¼

pa2 s2 þ 4az E

ð7:11Þ

Both terms (Um and Us) are plotted in Fig. 7.8. Us varies linearly and dominates for small crack size values. In contrast, for large crack sizes, Um dominates and the total energy passes through a maximum (dU/da ¼ 0) that allows determination of equilibrium for rﬃﬃﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2Ez EGc sf ¼ ¼ ð7:12Þ pa pa Over this value catastrophic failure happens.

143

144

7 Mechanical Strength of Glass

Fig. 7.8 Energy of an inﬁnitely narrow elliptical ﬂaw under uniform tensile stress s. Crack equilibrium corresponds to U maximum (z ¼ 1 J m2, E ¼ 70 GPa, s ¼ 2 MPa).

7.4 Linear Elasticity Crack Tip Stress Field

Considering mode I, the stress ﬁeld at the crack tip proximity is determined to be (Irwin, 1958; Paris and Sih, 1965; Fig. 7.9) 0

sx

1

0

cosðu=2Þ½1 sinðu=2Þsinð3u=2Þ

1

K B C B s C pﬃﬃﬃﬃﬃﬃﬃﬃ @ yA¼ @ cosðu=2Þ½1 þ sinðu=2Þsinð3u=2Þ A 2pr txy sinðu=2Þcosðu=2Þcosð3u=2Þ

Fig. 7.9 (a) x, y axis and stress components; (b) schematic representation of stress concentration at crack tip (dashed line) and inﬂuence of a plastic zone (continuous line).

ð7:13Þ

7.5 SIF under Non-uniform Stress

This reduces to si j ¼ Kð2prÞ1=2 fi j ðuÞ

ð7:14Þ

showing stress concentration at the proximity of the crack tip with dependence of the form r1/2. It should be noted that a mathematical singularity is obtained at r ¼ 0 because the tip extremity curvature radius was taken as 0. We have not considered that stress concentration may induce a conﬁned plastic deformation that shifts the singularity (Fig. 7.9b). Using the Dugdale (1960) model one may estimate the size l of the plastic zone at the crack tip to be p Kc 2 l¼ 8 Y

ð7:15Þ

where Y is the yield stress. For a soda-lime-silica glass (Kc ¼ 0.7 MPa m1/2, Y H/ 3 2 GPa; Appendix 8) one ﬁnds a plastic zone at the tip extremity of size l 50 nm. This very small value is to be compared to that obtained for a metal: l 1 mm. This result emphasizes the actual brittle behaviour of glass since, contrary to a metal, only a few bonds at the crack tip support the elevated stress concentration. The presence of a plastic zone at the crack tip has been until recently quite speculative given the relevant length scale. Using atomic force microscopy (AFM), Creuzet et al. (1993) could measure the deformation of a glass specimen at the emergence of a crack (or the topography of the surface at crack emergence). They showed that the experimental results in the vicinity of crack emergence were not in agreement with linear elasticity. More recently Ce´larie´ et al. (2003) suggested that ‘Glass breaks like metal, but at a nanometer scale’, although further experimental evidences are demanded (Guin and Wiederhorn, 2004). Furthermore, Mattoni et al. (2005) emphasize that for very a short crack it is difﬁcult to discriminate between bond breaking and incipient plasticity yielding departure from classic Grifﬁth theory.

7.5 SIF under Non-uniform Stress

To this point we supposed the specimen was uniformly loaded. Instead let us consider a straight crack (0 < x < a) in an inﬁnite specimen under a varying stress s(x) normal to the crack surface. SIF is given by pﬃﬃﬃ ða 2 a sðxÞ K ¼ pﬃﬃﬃﬃ dx p ða2 x 2 Þ1=2 0

ð7:16aÞ

145

146

7 Mechanical Strength of Glass 1=2

The term 1=ða2 x 2 Þ can be considered as a weight factor on stress s(x) and is called the Green’s function. It maximizes at the crack tip vicinity. For a uniformly loaded specimen one ﬁnds again (taking for the integration x/a ¼ sin d) pﬃﬃﬃ ða pﬃﬃﬃﬃpﬃﬃﬃ 2 a dx K ¼ pﬃﬃﬃﬃ s ¼s p a 1=2 2 2 p ða x Þ

ð7:16bÞ

0

For an edge crack in a semi-inﬁnite specimen, the integration is to be corrected with Y ¼ Hp replaced by 1.12Hp (Table 7.2): K¼

pﬃﬃﬃ ða 2Y a sðxÞ dx p ða2 x 2 Þ1=2

ð7:16cÞ

0

7.6 Toughness Measurement

Toughness measurements require that specimens are prepared with care introducing a sharp crack of known size a. As detailed below, glass is characterized by a distribution of ﬂaws that yields statistical fracture, the introduced crack being the critical one from where fracture initiates. Different loading modes are used and give their name to the related methods. When increasing the applied load F, stress concentration increases and yields crack growth. Stress concentration reaches toughness value at rupture. Stress concentration K as a function of applied load is given for the three main loading geometries, a being the crack length, and b, L and e being geometrical factors (Fig. 7.10). 7.6.1 Compact Tension

Under compact tension (CT) stress concentration is K¼

pﬃﬃﬃ a2 a3 a4 F a a 1:017 þ638:6 29:6 185:5 þ 655:7 be b b b b

ð7:17aÞ

7.6.2 Notch Beam Test

For the notch beam test (NBT or SENB) stress concentration is pﬃﬃﬃ a2 a3 a4 3FL a a 1:96 2:75 þ 13:66 K¼ 23:98 þ25:22 b b b b 2b2 e

ð7:17bÞ

7.6 Toughness Measurement

Fig. 7.10 Specimens for toughness measurement and loading conditions.

7.6.3 Double Torsion

Under double torsion (DT) stress concentration shows no dependence on introduced ﬂaw size a and is 3ð1 þ nÞ 1=2 K ¼ Fb Le4

ð7:17cÞ

All expressions show a linear variation of the stress intensity factor K with the applied force F. Interestingly on loading the specimens, the crack propagation can be measured in a domain where K < Kc, that is, before catastrophic failure. This domain

147

148

7 Mechanical Strength of Glass

is referred to as the subcritical domain. Subcritical crack growth has important implications on the ageing of glass, that is, its behaviour with time. This issue is addressed extensively in Chapter 9. It should also be noted that an indentation method may be employed to determine toughness when small quantities of material are available. This issue is discussed in more detail in Chapter 8.

7.7 Inﬂuence of Residual Stress on Strength and Fragmentation

As mentioned above, compressive residual stresses contribute negative SIF (Kr < 0). Stress concentration superimposes; hence we have pﬃﬃﬃ K ¼ sY a þ Kr

ð7:18aÞ

Also, fracture happens when the stress intensity factor K reaches the critical value Kc: pﬃﬃﬃ Kc ¼ sf Y a þ Kr

ð7:18bÞ

pﬃﬃﬃ Equation (7.18b) is sometimes rewritten in the form T ¼ sf Y a ¼ Kc Kr with T the apparent toughness including the residual stresses as a part of the crack resistance of the material. For compressive residual stresses (Kr < 0) there is a beneﬁcial effect on T. Equation (7.18b) can be written (for compressive stresses we take the absolute value) sf ¼

Kc Kr Kc þ jKr j pﬃﬃﬃ ¼ pﬃﬃﬃ Y a Y a

ð7:19Þ

Hence, for compressive residual stresses, fracture happens under greater applied stresses than for the residual stress-free state. In fact, tempering is used commonly to strengthen the glass surface. As discussed in Chapter 6, compressive stresses build at the surface and are equilibrated by tensile stresses in the core of the glass. Therefore, breakage happens either (i) when tensile applied stresses allow for Eq. (7.19) to reach the critical value sf at a critical ﬂaw present most probably at the surface (see also Section 7.8 and Chapter 8) or (ii) when an impact-generated ﬂaw reaches the tensile zone (Fig. 7.11). The latter situation corresponds to complex loading and complex

! Fig. 7.11 High-speed photographic sequence showing the catastrophic failure of a thermally tempered soda-lime-silica glass block caused by the impact of a 2 mm diameter tungsten carbide sphere at a velocity of 150 m s1. The fringes are isochromatics, the arrow points to the black fringe, which marks the region of zero stress

(see Chapter 11). The catastrophic failure begins in frame 4. Note the change in shape of the stress pattern as well as the bifurcation of the cracks in frames 6 to 12. Surface compressive stresses are 200 MPa, inter-frame time is 1 ms. (Reprinted from Chaudhri and Liangyi, 1986, with permission from Macmillan Publishers Ltd.)

7.7 Influence of Residual Stress on Strength and Fragmentation

149

150

7 Mechanical Strength of Glass

fracture path as revealed by high-speed photography (Fig. 7.11). This is discussed in Section 7.7.4. Let us consider ﬁrst situation (i) with a critical ﬂaw present at glass surface either in a thermally or chemically tempered glazing, or under slowly and rapidly varying residual stresses respectively (Figs. 6.25 and 6.36). We suppose the glazing is stressed uniformly and illustrate then the beneﬁcial role played by strengthening since applied stress at rupture increases accordingly. 7.7.1 Inﬂuence of Residual Thermal Stress on Strength

Thermal residual stress varies slowly with depth. We suppose it can be considered constant over crack length. We suppose cracks are present at the glass surface and take pﬃﬃﬃ the residual stress equal to the surface compressive stress; hence Kr ¼ ss Y a (ss < 0). We may consider crack length is negligible as compared to glass thickness a tH so pﬃﬃﬃﬃ that Y ¼ 1:12 p (valid for an edge crack in a semi-inﬁnite solid). Stress at rupture is Kc Kc sf ¼ pﬃﬃﬃ ss ¼ pﬃﬃﬃ þ jss j Y a Y a

ð7:20Þ

Therefore, strengthening at the glass surface is directly related to the amplitude of the residual surface stresses. This means that thermally tempered glazing strength is shifted by the thermal residual surface stress amplitude.

7.7.2 Inﬂuence of Residual Chemical Stress on Strength

Chemical residual stresses vary much more rapidly with depth than thermal residual stresses. Let us suppose the compressive stress varies linearly and is null at a depth h (so-called exchanged depth; Chapter 6). Then, residual stress variation with depth z0 (¼ tH/2 z) is written sr ¼ (1 z0 /h)ss. We have (Section 7.5) pﬃﬃﬃ ða pﬃﬃﬃ ða 2Y a sr ðz0 Þ 2Y a ss ½1 ðz0 =hÞ 0 0 Kr ¼ dz ¼ dz p p ða2 z02 Þ1=2 ða2 z02 Þ1=2 0 0 pﬃﬃﬃ 2a ¼ Y ass 1 ph

ð7:21Þ

Finally stress at rupture is Kc 2a Kc 2a ¼ pﬃﬃﬃ þ jss j 1 sf ¼ pﬃﬃﬃ ss 1 ph ph Y a Y a

ð7:22Þ

7.7 Influence of Residual Stress on Strength and Fragmentation

Again, we ﬁnd that stress at rupture increases with the residual stress amplitude. In the case of chemical tempering, not only the stress level is to be considered in evaluating the beneﬁcial role of residual stresses, but also the treated layer thickness through the a/h ratio that plays an important role. This results from the fact that the superﬁcial ﬂaw size is not negligible as compared to the exchange depths reached under commercially available conditions. In fact, let us consider a high exchanged depth for which a/h ! 0. Then stress at rupture can be approximated by pﬃﬃﬃ sf ðKc =Y aÞ þ jss j and we obtain a result similar to that obtained for thermal tempering. 7.7.3 Inﬂuence of Residual Stress on Fragmentation

On breakage, release of tempering-induced elastic energy happens. When crack speed approaches half the Raleigh wave speed, it is possible for the crack to split into multiple branches (Fig. 7.11). Crack multiplication allows for dissipating more energy since more surfaces are generated. This phenomenon happens for a critical value of SIF about four times Kc (around 3 MPa m1/2 for a silico-soda-lime glass). Akeyoshi et al. (1967) showed that the density of the fragments generated on breakage is to be related to the level of residual stresses (degree of temper) (Fig. 7.12). It has been argued that the elastic energy stored in the tensile zone is the parameter controlling the glass breaking (Bouyne and Gaume, 2001).

Fig. 7.12 Fragment densities (in a 5 5 cm2 area) as a function of residual tensile stress (according to Akeyoshi et al., 1967).

151

152

7 Mechanical Strength of Glass

The number of fragments increases with residual stress level and the thickness of the glass sheet, that is, the amplitude of elastic energy stored during the tempering process. Akeyoshi et al. (1967) carried out extensive experimental tests to determine the fragment densities in broken samples of different thickness and tempering degree. They produced a map showing the fragment density as a function of tensile core residual stress amplitude for commercially available ﬂat glass thicknesses. This map is still in use and allows for determination and control of residual stresses in ﬂat glass. A glass article is taken from the batch and fractured. The fragment density is then determined and residual stress amplitude extracted from the Akeysohi et al. chart. This control is demanded to ﬁt the R43 international standard for tempered automotive glazing. Not only must tempering produce strength, but also on breakage the residual stresses are to be designed so that harmless fragments are generated. The R43 standard ﬁxes the number of glass fragments in all 5 5 cm2 areas to be over 40 and below 400. Such a control of the residual stresses is destructive and nondestructive methods are preferred (Chapter 11). Notably, the Akeyoshi et al. (1967) approach for thermally tempered glasses can be generalized to chemically tempered glasses (Bouyne and Gaume, 2001). The consequence of the above results is that toughened glass cannot be cut or otherwise modiﬁed in shape as this would disturb the system of prestresses, and with fracture beginning at any point in the glass, the whole sheet would shatter immediately into small (although harmless) fragments. Hence, glass tempering is carried out ofﬂine after cutting, drilling and edge grinding operations.

7.7.4 Impact-Induced Fracture

There has been little experimental work dedicated to the way an impact crack generates and further enters the tensile region causing fracture. Figure 7.11 is hence of much interest as it shows a high-speed photographic sequence in crosssection of a thermally tempered soda-lime-silica glass impacted by a hard sphere thrown at 150 m s1 towards its surface. The dark fringe corresponds to zero stress (these are photoelastic images; see also Chapter 11). As the sphere impacts the block, stress ﬁeld changes as revealed by the photoelastic survey of the zone (frames 1–3). Interestingly between frames 4 and 5 the cracks enter the region of tensile stress and this leads to the initiation of catastrophic failure of the sample. The cracked area is observed as a dark and growing surface as time increases. The velocity of the cracks depends on the direction they propagate. The velocity of the cracks moving towards the surface of the impact is much smaller (200–300 m s1) than the velocity of the cracks spreading along the loading axis. In frames 7–12 cracks further spread and bifurcate, the images showing chaotic features. In fact, ﬁnite element analysis (FEM) happens to be of great help in getting insight into impact failure (Appendix 11) while we further discuss crack initiation under contact loading in Chapter 8.

7.8 Statistical Weibull Analysis

7.8 Statistical Weibull Analysis 7.8.1 Introduction

The strength of a glass and more generally of a brittle material depends on its toughness Kc that is generally known and the critical ﬂaw size a that depends on the industrial process and use, the ultimate stress being extracted from the following relationship (Section 7.2): pﬃﬃﬃ Kc ¼ sf Y a

ð7:23Þ

Therefore, the determination of the glass mechanical performance requires the knowledge of ﬂaw population which has to be determined statistically. Weibull (1951, 1952) statistics has been commonly used to characterize the statistical variation of the fracture strength of brittle materials such as ceramics, glasses and solid catalysts. It is based on the ‘weakest link theory’ which means that the most serious ﬂaw in the material will control the strength, like a chain breaking if its weakest link fails (Fig. 7.13). The most serious ﬂaw is not necessarily the largest one because its severity also relies on its location and orientation. In fact, strength is controlled by the ﬂaw subjected to the highest SIF. 7.8.2 Functional Formulation

We must consider that ﬂaws are distributed into the specimens. We shall suppose that the probability that two independent events occur is the product of the respective probabilities (Kittl and Diaz, 1988). Let us consider a volume V of the specimen and decompose it into two smaller volumes V1 and V2: V ¼ V1 þ V2

Fig. 7.13 Loaded chain of n links. The chain fails from its weakest link.

ð7:24Þ

153

154

7 Mechanical Strength of Glass

Ps(V, s) is the probability that a given volume V resists the stress s. We have Ps ðV; sÞ ¼ Ps ðV1 þ V2 ; sÞ ¼ Ps ðV1 ; sÞPs ðV2 ; sÞ

ð7:25Þ

Using this relationship for a volume of V + DV allows one to write Ps ðV þ DV; sÞ ¼ Ps ðV; sÞPs ðDV; sÞ

ð7:26Þ

while we have also Ps ðV þ DV; sÞ ¼ Ps ðV; sÞ þ Ps0 ðV; sÞDV

ð7:27Þ

Thereafter we have Ps0 ðV; sÞ ¼ ½Ps ðV þ DV; sÞ Ps ðV; sÞ=DV

ð7:28Þ

Using Eq. (7.26), Eq. (7.28) becomes Ps0 ðV; sÞ ¼ ½Ps ðV; sÞPs ðDV; sÞ Ps ðV; sÞ=DV

ð7:29Þ

Ps0 ðV; sÞ=Ps ðV; sÞ ¼ ½Ps ðDV; sÞ 1=DV

ð7:30Þ

Then

which for DV ! 0 becomes Ps0 ðV; sÞ=Ps ðV; sÞ ¼ Ps0 ð0; sÞ ¼ FðsÞ=Vo

ð7:31Þ

where F(s) is the risk function for stress s and Vo a unit volume. Equation (7.31) is integrated as follows: ð lnPs ðV; sÞ ¼ V

FðsÞ dV Vo

ð7:32Þ

so that 0

1 FðsÞ Ps ðV; sÞ ¼ [email protected] dV A Vo ð

ð7:33Þ

V

Weibull suggested the following risk function: m 8 > < s su s0 FðsÞ ¼ > : 0

s su 0 s su

ð7:34Þ

7.8 Statistical Weibull Analysis

where su is the stress for which the probability for rupture is null, and is taken as su ¼ 0 for a brittle material, and m is the Weibull modulus. Therefore we have FðsÞ ¼

s s0

m ð7:35Þ

We have to consider two situations to integrate Eq. (7.33): stress is either uniform (Section 7.8.2.1) or not uniform (Section 7.8.2.2). 7.8.2.1 Uniform Tensile Stress Under uniform tensile stress (for instance in a uniaxially tensile stressed ﬁbre) Eq. (7.33) becomes V s m Ps ðV; sÞ ¼ exp Vo so

ð7:36Þ

This is the most commonly used form of Weibull resistance probability. Parameter m is called the Weibull modulus and is indicative of strength scatter; so is indicative of strength level and corresponds to fracture stress with a failure probability of 63.2%. It is closely related Ð 1 to the mean strength sm of the distribution by sm ¼ soG(1 þ 1/m), with GðxÞ ¼ 0 et tx1 dt (see also Appendix 8). For a Weibull modulus in the range of 10 typical for ceramics, G(1 + 1/m) is about 0.9 to 1. 7.8.2.2 Non-uniform Tensile Stress When stress varies in the volume of the material, Eq. (7.33) becomes 0

1 2 3 ð m FðsÞ 1 s Ps ðV; sÞ ¼ [email protected] dV A ¼ exp4 dV 5 Vo Vo s o ð V

ð7:37Þ

V

Integration of Eq. (7.37) requires knowledge of the stress ﬁeld. Let us consider for instance a beam under ﬂexure (Chapter 2; Fig. 7.14). Stress changes from compressive at the top surface to tensile at the bottom surface. The neutral line is where stress amplitude vanishes (Appendix 7). Accordingly, the stress

Fig. 7.14 Beam under ﬂexure.

155

156

7 Mechanical Strength of Glass

ﬁeld is written 0

z l=2 x B tH =2 l=2 B sðx; zÞ ¼ sM B @ z l=2 þ x tH =2 l=2

for x 2 ½0; l=2 ð7:38Þ for x 2 ½l=2; 0

where sM is the maximum stress (at the beam surface). Integration on volume V (in fact considering only the so-called tensile zones) yields4) "

m # V 1 sM Ps ðV; s Þ ¼ exp Vo 2ðm þ 1Þ2 so 0

ð7:39Þ

Equations (7.36) and (7.39) were obtained using the same risk function. However, one notes that for the same given applied stress (tensile stress s equal to maximum ﬂexure stress sM) the probability that the specimen resists is higher under ﬂexure. This is further discussed below and results from an intrinsic size effect, the maximum tensile stresses being applied to only a small part of the bent specimen. 3)

Crack opening happens in tensile zones. Since stress is tensile for z 2 ½tH =2; 0 integration is over half of the beam volume. The beam volume V is V ¼ lwtH . We have 2 3 ð m 1 s dV 5 Ps ðV; sÞ ¼ exp4 Vo s o V

ð V

ððð

m

s so

dV ¼ V

s so

m

ð0

0 w=2 0

ð V

s so

m

dV ¼ 2

ð

V

s so

m

dV ¼ 2w

s so

sM 1 1 so tH =2 l=2

¼ 2w

m

m dxdydz

m dxdydz:

m

sM 1 1 so tH =2 l=2

sM so

s so

l=2w=2 0

l=2 ð w=2 ð tHð=2

þ

w=2 ð tHð=2

dxdydz ¼

m

ðl=2 xÞmþ1 mþ1

l=2 mþ1 tH =2 z w mþ1 0 0

ðl=2Þmþ1 ðtH =2Þmþ1 ðm þ 1Þ2

ðl=2ÞðtH =2Þ 2

ðm þ 1Þ

¼

V 2

2ðm þ 1Þ

m V 1 sM : then Ps ðV; sÞ ¼ exp 2 Vo 2ðm þ 1Þ so

sM so

m

7.8 Statistical Weibull Analysis Tab. 7.3

Weibull modulus for different classes of materials.

Material

Weibull modulus

Glass container, ﬂat glass Glass ﬁbre Ceramics Metals

3–7 10–30 10 40

7.8.3 Population of Flaws

Glass specimens present a ﬂaw size distribution. The determination of ﬂaw population passes through an experimental study of a representative series of samples that are to be tested. Weibull statistics is subsequently used to ﬁt the resistance probability Ps(V) as a function of stress (Appendix 6). Weibull statistics is also applied extensively for studying brittle fracture even at the nanoscale (Pugno and Ruoff, 2006) as well as the interfacial rupture (Piellard, 2005). The scatter of ﬂaw size distribution and of the fracture strength is indicated by the so-called Weibull modulus m (Table 7.3). From an engineering point of view, a high Weibull modulus can be as important as a high strength. A higher m value leads to a steeper ﬂaw size distribution and thus to a lower dispersion of the fracture strength (Fig. 7.15). Interestingly a glass edge can be carefully abraded to obtain m as high as 10 (Barton and Guillemet, 2005). The highest Weibull moduli for glasses are obtained from ﬁbres that can be produced almost ﬂawfree, m approaching 30 and tensile strength being close to the intrinsic one. Modern

Fig. 7.15 Weibull probability Ps(Vo) to resist stress s (so ¼ 1 GPa). Three different Weibull moduli have been considered (m ¼ 10, 25 and 100).

157

158

7 Mechanical Strength of Glass

Fig. 7.16 Weibull probability to resist stress s (so ¼ 1 GPa, m ¼ 25). Three volumes have been considered (V/Vo ¼ 1, 10 and 100).

fused silica optical communications ﬁbres show m in the range 30–100! Some authors argued that the variation observed for m > 30 could result only from section variation of the studied ﬁbre. The ‘intrinsic’ strength of silica ﬁbre would then be about 12 GPa, close to the theoretical strength determined in Section 7.1. Let us consider uniformly stressed specimens; we have V s m Ps ðV; sÞ ¼ exp Vo so

ð7:40Þ

When larger specimens are considered (size effect from laboratory to practical application) the probability that the sample resists stress s is Ps ðV; sÞ ¼ Ps ðVo ; sÞn with V ¼ nVo

ð7:41Þ

Figure 7.16 plots the probability Ps(V, s) for increasing sizes (namely V/Vo ¼ 1, 10 and 100) where mean strength is observed to decrease accordingly. Size effect is indeed inherent to brittle fracture. The load applied to lead the specimen to fracture decreases as the volume of the tested specimen increases because of the greater probability of containing dangerous ﬂaws. A corollary to this is that higher average strength values are always observed in bending than in tensile tests, because the maximum stresses are applied to only a small part of the bent specimen (Sections 7.8.2.1 and 7.8.2.2). Here, we suppose that residual stresses are null. If not, the situation is then even more in favour of bending resistance since superﬁcial residual stresses are compressive. Whenever critical ﬂaws can be supposed to locate at the surface as for ﬂat glass

7.8 Statistical Weibull Analysis

(because of contact damage; see Chapter 8) the difference becomes less. When a ﬁbre is considered, longitudinal and transversal size effects are expected. This statistical behaviour has very important technological consequences: i. Diameter size effect could provide a way of improving strength by obtaining ﬁner ﬁlaments. Composites formed from ﬁbre embedded in a polymer matrix are of interest in view of the outstanding ﬁbre strength as compared to ﬂat glass. ii. If signiﬁcant enough, size effect could be used to perform accelerated testing increasing size. iii. Wide difference may arise from small-scale laboratory specimens to larger structures. So far, quantitative extrapolation methods following the Weibull law are still questioned in the literature (Zinck et al., 1999).

159

161

8 Contact Resistance of Glass 8.1 Sharp and Blunt Contact 8.1.1 Introduction

As detailed in Chapter 7, glass strength depends mostly on ﬂaws (defects) from which cracks develop. The existence of ﬂaws is the reason why glass specimens show a mechanical strength much below the theoretical one. These ﬂaws may be either in the glass bulk like small bubbles remaining after ﬁning operations and crystalline phases (refer to Chapter 10) or at the surface like microcracks generated by the contact between the glass and tools and later in use (Fig. 8.1). These may be generated during the process itself or from handling and service conditions. We address in the present chapter the generation mechanisms of such contact-induced ﬂaws. During the production process the glass follows a complex thermomechanical route involving contact with tools at different temperatures (with the possibility of a thermal gradient between glass and tool), while in use the contact is generally isothermal (both the contactor and glass being at room temperature). As discussed in detail below, over a given threshold the contact is no longer reversible (excursion out of the elastic domain). Non-reversible deformation and cracks can be observed. All these phenomena lead to the introduction of ﬂaws at the glass surface and glass strength is dramatically affected (Gy, 1997). We shall not address chemical reaction with the surface. It is well known that just touching lightly the surface of a pristine silica rod dramatically lowers its strength. For instance, halogen lamp operating notes often recommend no contact between the ﬁngers and the lamp. Microanalysis of fracture origin shows alkali and alkaline earth contaminants. Figure 8.1 shows the dramatic scratches at the internal surface of a used plate. We review the mechanics of such phenomena. Glassmakers have been aware of these phenomena for a long time and coating technology was developed accordingly to protect glass surfaces from erosion and damage either for mechanical or aesthetics purposes (ﬁbre sizing, container hot end treatments; Chapters 10 and 12). More fundamentally, tailoring contact resistance has attracted much scientiﬁc and technological interest and Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

162

8 Contact Resistance of Glass

Fig. 8.1 Scratches on a used glass plate as observed by optical microscopy.

fracture mechanics described here was applied with success to many other types of materials showing brittle fracture (Le Bourhis et al. 2001b; Cook, 2006). In the literature, two schematic contact conditions are generally considered. Blunt contact conditions consider that the material under a sphere deforms elastically up to brittle fracture. In contrast, under a sharp contact glass deforms elastically, plastically and ﬁnally fractures. The term ‘plastic’ is to be considered with caution for glass that is amorphous and ‘plastic’ means irreversible in this context. Glass may deform ‘plastically’ or inelastically below the glass transition temperature when small volumes are highly stressed. Under a sharp contact, pressure scales typically with hardness H that is commonly of the order of some gigapascals, while the deformed zone is elastically constrained by the surrounding volume of the material as discussed below. Experimental tools have been developed using a spherical indenter to produce blunt contact while sharp contact is produced by conical or pyramidal tips as reviewed below. Also, scratch testing allows production of a lateral movement during the contact and hence a frictional force. These testing modes allow to approach real contact conditions. 8.1.2 Spherical Indentation 8.1.2.1 Elastic Loading Figure 8.2 shows a diagram of the elastic loading of a glass surface by a spherical indenter. In such an experiment, a sphere of radius R is loaded under a force F, the contact radius being a. The specimen surface around the contact area also deforms elastically as shown schematically in Fig. 8.2. Load (F)–penetration (h) relationship is known as the Hertz (1881) contact solution: 4 F ¼ R1=2 E h3=2 3 where R is the radius of the tip and E the composite modulus, given by 1 1 n2i 1 n2s ¼ þ E Ei Es

ð8:1Þ

ð8:2Þ

8.1 Sharp and Blunt Contact

Fig. 8.2 Diagram of the elastic loading of a spherical indenter on a glass surface.

where E and n are elastic modulus and Poisson ratio with subscripts i and s referring to the indenter and the specimen respectively. For a diamond tip usually employed in the laboratory, Ei ¼ 1141 GPa, ni ¼ 0.07. For materials much softer than diamond we have 1=E ¼ ð1 n2s Þ=Es , and the indenter can be supposed perfectly rigid. In the general case, the glass and indenter properties are to be considered. When the two materials in contact are identical, a glass against another glass for instance, we have 1=E ¼ 2ð1 n2s Þ=Es , and both the specimen and the indenter deform. Figure 8.3 shows the calculated reversible loading curves of a glass under two spherical diamond indenters with different radii. The smaller the radius, the larger the penetration. The contact radius a is given by a ¼ R

1=3 3 F 4 E R2

Fig. 8.3 Calculated load–penetration curve of a spherical diamond indenter into a standard silico-soda-lime glass surface (E ¼ 72 GPa, R ¼ 1 or 0.1 mm).

ð8:3Þ

163

164

8 Contact Resistance of Glass

Fig. 8.4 Mean pressure as a function of penetration of a spherical diamond indenter into a standard silico-soda-lime glass surface (E ¼ 72 GPa, R ¼ 1 or 0.1 mm).

while the mean pressure p is p ¼ F=Ac ¼ F=pa2

ð8:4Þ

which is zero for F ¼ 0 and progressively increases as load increases (Fig. 8.4). Under usual loading conditions, the mean pressure is found to be well below the yield stress of the glass (Y H/3 2 GPa for an SLS glass; Appendix 8) so that only elastic loading is considered up to fracture. Notably, we can observe that when the sphere radius decreases the mean pressure for a given penetration of the indenter increases (Fig. 8.4). The maximum tensile stress in the specimen occurs at the contact circle: 1 sm ¼ ð1 2nÞ p 2

ð8:5Þ

while the maximum shear stress is located along the loading axis at depth 0.5a below the surface: tm ¼ 0:48 p

ð8:6Þ

8.1.2.2 Hertz Fracture and Indentation Toughness Under a spherical indenter, the mean pressure progressively increases when the applied load increases. Eventually, cone cracks may extend into the material as shown schematically in Fig. 8.5 and revealed experimentally in Figs. 8.6 and 8.7. Outside the contact area, pre-existing ﬂaws are subjected to tensile stress, which at some point (depending on the ﬂaw size) run around the contact forming a surface ring crack that grows downward following the principal stress conical trajectories, while on unloading the cracks close. The fracture usually remains visible because of the imperfect

8.1 Sharp and Blunt Contact

Fig. 8.5 Fracture under a blunt indenter: (a) cone fracture sequence on loading (þ) and unloading (); (b) cone fracture geometry (according to Lawn, 1993).

closure at the crack (Fig. 8.6). Notably, the residual stress ﬁeld changes the crack geometry as revealed in Fig. 8.6b. Also, the load required for generation of cracks of similar size is superior in tempered specimens. In thermally tempered glazing, the skirt of the cone crack is almost parallel to the indented surface, while it is inclined to the surface in an annealed (stress-free) specimen. The crack evolution is depicted schematically in Fig. 8.5 (Lawn, 1993, 1998) with the plus sign indicating loading and the minus sign unloading. Next, let us consider a specimen with small residual stresses. The mechanics of cone crack initiation started with Auerbach (1891). He showed empirically that the critical load to initiate a cone fracture in ﬂat specimens was proportional to the radius of the indenting sphere Fc R. For decades (Tillett, 1956; Lawn, 1993), Auerbach’s law was debated since fracture theory suggests that cracks

165

166

8 Contact Resistance of Glass

Fig. 8.6 Side views of the cone cracks under load in annealed and thermally tempered sodalime glass formed under a 2.5 mm radius steel indenter. Note that the skirt of the cone crack in the annealed glass makes a signiﬁcantly larger angle with the indented surface than that in the

tempered glass (Reprinted from Chaudhri and Phillips, 1990, with permission from Taylor & Francis Ltd. http://www.informaworld.com). (a) load 793 N, cone base 2.4 mm; (b) load 2060 N, cone base 2.85 mm.

initiate at the points where maximum tensile stress in the Hertzian ﬁeld equals the strength of the material. Using Eqs. (8.4) and (8.5) results in an Fc R2 relationship. The paradox was solved taking into account the statistical nature of fracture and showing the so-called Auerbach’s range in a domain where Fc shows an insensitivity to ﬂaw size. Then, the toughness of a glass can be determined using the critical load for crack generation (Auerbach’s law) or the extension of the cracks (Franck and Lawn model) as reviewed by Geandier et al. (2003). The toughness and the critical load are related in Auerbach’s range by (Lawn, 1993; Warren, 1995; Fischer-Cripps, 2004a) Kc ¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ E Fc CR

ð8:7Þ

where Fc is the critical load for cone crack generation, C a constant that has to be calculated for a given material and indenter (Warren, 1995), R the indenter radius and E the composite modulus deﬁned above. For glass contacting glass, C ¼ 3131; it is 2790 for alumina contacting alumina (Warren, 1995).

Fig. 8.7 Top view of ring cracks generated by a sphere (0.2 mm diameter) on the atmospheric side of a ﬂoat glass.

8.1 Sharp and Blunt Contact

In the Frank and Lawn (1967) model, only the cone crack is considered; the initial small circular shaped crack perpendicular to the surface is neglected, due to its small size compared to the cone length. It is assumed that the crack is propagating along the direction of the smallest principal stress (s3) perpendicularly to the maximum principal stress (Hertz stress ﬁeld s1; we suppose no residual stresses) and that the crack presence and propagation do not modify the initial stress ﬁeld. The critical stress intensity factor is then obtained by integration along the crack length c (Fig. 8.5; Section 7.5): rﬃﬃﬃﬃ ðc c s1 ðxÞ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dx Kc ¼ 2 p c2 x2

ð8:8Þ

0

where s1(x) is the Hertzian stress value along the crack (the opening stress normal to crack direction). Interestingly, Chaudhri and Kurkjian 1986 showed that cone cracks also form on dynamic loading with lower cone angles. The cone formed is 468, that is, smaller than that of 62.88 formed under static loading (Chaudhri and Kurkjian, 1986). Moreover, the angle amplitude depends on the Poisson ratio of the studied glass and the residual stresses as discussed above. A typical Hertz fracture obtained after a blunt impact is shown in Fig. 8.8 on a laminated (annealed) windscreen. Even small cracks develop under humid environments as discussed in more detail in Chapter 9 and should be repaired before they damage dramatically the glazing. 8.1.3 Sharp Indentation 8.1.3.1 Elastic Loading Figure 8.9 shows a diagram of the elastic loading of a glass surface by a conical indenter. The approach can be extended to pyramidal tips (Vickers, cube corner, Berkovich 1951) and more generally self-similar tips taking Ac ¼ pa2 ¼ ah2 and neglecting the inﬂuence of the indenter edges. A cone loaded under force F penetrates the specimen down to the penetration depth h, the contact radius being

Fig. 8.8 Hertz fracture on a laminated windscreen.

167

168

8 Contact Resistance of Glass

Fig. 8.9 Diagram of the elastic loading of a conical indenter on a glass surface.

a. Again as for a spherical tip, the specimen deforms elastically around the contact area as shown in Fig. 8.9 (see also Appendix 8). Load (F)–penetration (h) relationship is known as the Sneddon (1965) contact solution and shows a square dependence on penetration (so-called self-similarity or geometrical similarity of the contact): F¼

2 Er h 2 ptanb

ð8:9Þ

where b is the angle between the indenter ﬂank and the specimen surface and Er is the reduced modulus deﬁned as 1 1 n2s ¼ Er Es

ð8:10Þ

where subscript s indicates the specimen. The contact radius a is given by a¼

2h ptanb

ð8:11Þ

while the mean pressure p is p ¼ Er tanb=2

ð8:12Þ

which interestingly is independent of the penetration (geometrical similarity). Mean pressure shows dependence on ﬂank angle. For a sharper tip (larger b), a larger pressure is generated. Using standard silico-soda-lime glass characteristics (Er ¼ 76 GPa) and a ﬂank angle b ¼ 198 (a cone angle with the same area function as that of a Berkovich or Vickers tip) one ﬁnds a pressure p 13 GPa well above the glass yield strength (Y ¼ H/3 2 GPa; Appendix 8). In fact, glass is ‘plastically’ deformed as revealed by the indenter mark left on its surface (Fig. 8.10). The mark shows the symmetry of the indenter used (here four-fold symmetry since a Vickers pyramid tip was used). The image shows also fracture events that are discussed in more detail below. Most tips are not perfectly sharp but show tip rounding at their extremity. Under low loads the tip rounding yields

8.1 Sharp and Blunt Contact

Fig. 8.10 Indented surface showing the permanent deformation and the radial cracks (scanning electron microscopy observation of standard glass indented under 5 N); c and a correspond to crack and mark lengths respectively.

a Hertz dependence between force and penetration with no plastic deformation being generated, while the response tends to Sneddon’s law for elevated penetrations. 8.1.3.2 Elastic–Plastic Loading As discussed above, a sharp contact yields elastic and irreversible deformations. Different approaches have been proposed to model the elastic–plastic response (Loubet et al., 1986; Sakai 1999). Basically purely elastic and purely plastic components are connected in series (Chapter 6; Oyen and Cook, 2003). The total displacement of the indenter is the sum of the elastic he and plastic hp displacements (a viscous hv component may be added; Oyen and Cook, 2003; Mammeri et al., 2004; Appendix 8): h ¼ he þ hp

ð8:13Þ

Because of the geometric similarity of the sharp indenter, all constitutive equations show the square of the respective penetrations: F ¼ AEr he2

ð8:14Þ

F ¼ BHhp2

ð8:15Þ

where A and B (24.5 for a Vickers or Berkovich tip) are constant1 for a bulk, Er the reduced modulus and H the hardness. It should be noted that we assume here that the

1)

Parameter A may include mechanical properties (H/E ratio). Penetration can be written h ¼ hs þ hc, where hs is the elastic deformation of the surface (Appendix 8)

where H/E ratio appears (Loubet et al., 1986; Hainsworth et al., 1987; Malzbender et al., 2000).

169

170

8 Contact Resistance of Glass

sharp tip is a perfect pyramid or cone while tip rounding has to be considered as already discussed above. The reﬁnement of the present approach can be obtained using numerical tools like ﬁnite element analysis (FEA; Appendix 11). Combining Eqs. (8.13) to (8.15) yields h¼

rﬃﬃﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ F F 1 1 þ ¼ F pﬃﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ AEr BH AEr BH

ð8:16aÞ

Hence we obtain a square dependence of the force F on the total penetration: F¼

2 1 1 pﬃﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ h2 ¼ Kh2 AEr BH

ð8:16bÞ

where K is an elastic–plastic prefactor. This result suggests that elastic–plastic response under a conical remains self-similar. 8.1.3.3 Hardness Hardness measures the plastic resistance of a surface to contact loading, that is, its resistance to permanent deformation. Most experiments are carried out using a Vickers diamond pyramid. When a Vickers diamond (four-sided) pyramid is loaded over the plastic threshold, one can determine, after the test, the mean pressure or hardness H deﬁned by the ratio between the applied load and the projected surface Ap of the permanent deformation left by the indenter. This area can be determined from the mark diagonals (Ap ¼ 2a2; Fig. 8.10) observed under elevated loads by means of optical microscopy. Hardness is H ¼ F=Ap

ð8:17Þ

A large mean pressure (large hardness) means that the specimen shows an elevated resistance to plastic deformation under contact loading. Historically, the hardness ratio was deﬁned using the actual surface of the indent and not its projected surface so that a geometric factor relates the hardness number (Vickers, Knoop, Brinell, etc.) and the mean pressure. For instance, for a Vickers tip the Vickers hardness Hv is 0.927H (92.7% of the mean pressure). According to the load range, macro-, micro- and nanoindentation domains have been deﬁned. These domains should be borne in mind since indentation size effect (ISE, that is, a decrease of hardness with load in most cases) is reported for many materials including glasses, so that hardness values are to be compared within the same domain. It should be noted that these domains also refer to different ways to determine the surface of the indent. In the macro- and microindentation domains the indent surface is generally determined after unloading by optical microscopy. We shall refer to this area as Ap (projected area deﬁned above). Going to the nanoindentation domain (Appendix 8), observation of the indent becomes tedious and hardness is determined under load and is deﬁned as the ratio of the force to the projected contact area Ac that is extracted from the

8.1 Sharp and Blunt Contact Microhardness of different glasses (Aben and Guillemet, 1993; Barton and Guillemet, 2005).

Tab. 8.1

Microhardness, H (GPa)

Glass Silica Aluminosilicate Borosilicate Soda-lime-silica Lead-silicate Aluminophosphate

7.0–7.5 5.4–5.9 5.8–6.6 5.4–6.6 4.5 3.2

loading–unloading curves (Appendix 8): H ¼ F=Ac

ð8:18Þ

Microhardness values are reported for different glasses in Table 8.1 and do not show strong difference according to the composition of the glass even though they are known to deform quite differently whether they are considered normal or anomalous glasses. The nature of the permanent deformation is still controversial however. It depends on the type of glass, on the temperature and also on the strain rate. At room temperature, so-called anomalous glasses like fused silica show a volume densiﬁcation while normal glasses show shear ﬂow (Mackenzie, 1963; Peter, 1964; Neely and Mackenzy, 1968; Arora et al., 1979). In amorphous semiconductors (a-Ge) phase transition to crystalline phases is even observed (Patriarche et al., 2004). Normal glasses contain alkali and alkaline earth modiﬁers leading to non-bridging oxygen (NBO) atoms allowing for heterogeneous shear bands to form. Some authors suggested following Greaves’ (1985) modiﬁed random network that shear would happen preferentially at the frontiers between modiﬁer-rich and silica-rich volumes (Chapter 5). Heterogeneous ﬂow yields non-Newtonian viscoplasticity. The same formalism is used by the plasticity community and this explains why the term ‘plasticity’ is used for a glass even though the dislocation concept has to be reconsidered in a non-periodical structure (G’Sell, 2001). Douglas (1958) argued that ‘when the load is ﬁrst applied’ to the glass specimen ‘the pressure under the point of the diamond will be very high and the viscosity will be reduced’ (this is nonNewtonian ﬂow), and ‘ﬂow will take place until the diamond has penetrated sufﬁciently so that the force is no longer great enough to cause sufﬁcient reduction in viscosity for ﬂow to continue’. Also, water incorporation at glass surfaces (Chapter 5) is suspected to play a role in glass response (Han and Tomozawa, 1990). In contrast, anomalous glasses which contain very few modifying ions (silica being the archetype), present a much cross-linked network preventing heterogeneous ﬂow. Thereafter, indentation induces compaction (or densiﬁcation) of the glass. It occurs by bending and twisting but not breaking the silicon–oxygen bonds in the glass network. In fact, when the glass is heated up sufﬁciently the mark recovers (Neely and Mackenzy, 1968; Yoshida et al., 2001).

171

172

8 Contact Resistance of Glass

Fig. 8.11 Hardness H of silicate glass as a function of modiﬁer concentration (according to Kennedy et al., 1980).

Kennedy et al. (1980) reported changes in the hardness of silica as modiﬁers are progressively introduced. As observed for Young’s modulus E changes with alkali (Chapter 7), softening of the silica glass is more pronounced for a modiﬁer having a lower Dietzel ﬁeld intensity, that is, for a modiﬁer that is expected to form weaker interaction with oxygen (Chapter 5; Fig. 8.11). While heterogeneous shear ﬂow is volume-conservative, compaction, as the word suggests, leads to decrease in volume. This is the reason why the residual stresses caused by indentation into an anomalous glass are smaller than those in a normal glass. This has been clearly demonstrated by Arora et al. 1979 using photoelasticity (Chapter 10) to reveal differences in stresses around indent sites for normal and anomalous glasses. More recently, Perriot (2005) carried out cross-sectional Raman investigation on indented silica and revealed compaction gradient in silica (Fig. 8.12). Also, Yoshida et al. (2005) showed that compaction contribution to indentation deformation in normal glass could be greater than generally accepted. In fact, the separation of anomalous and normal glasses according to the presence of modiﬁers is still questioned. Rouxel et al. (2006) showed recently that SLS glasses show substantial compaction (obviously less than silica) that recovers upon annealing. Furthermore there seems to be a close relationship between densiﬁcation and Poisson’s ratio. The mechanical behaviour of a glass becomes more and more time dependent as the temperature is increased and as the viscous behaviour becomes predominant over densiﬁcation process (Westbrook, 1960; Wiederhorn and Hockey, 1980; Le Bourhis and Metayer, 2000; Le Bourhis and Rouxel, 2003). Under large strain rates, the supercooled liquid shows non-Newtonian behaviour with an apparent viscosity decreasing with the strain rate amplitude (Simmons et al., 1988; Appendix 10). Although this behaviour makes the process operations more difﬁcult, it can yield

8.1 Sharp and Blunt Contact

Fig. 8.12 Cross-sectional compaction map in silica under a Vickers indentation (Perriot, 2005).

advantages since the operations can be carried out under lower stresses (for the same ﬂow, rheoﬂuidiﬁcation) once high strain rates can be achieved. Hardness depends strongly on the temperature as shown in Fig. 8.13 for a sodalime-silica glass. As the temperature approaches Tg, viscous ﬂow (volume conservative) comes into play. Strangely, very few data existed before the 1990s while this behaviour is very important from the process point of view. These studies are in fact not easy to carry out and discrepancies appear between authors (Westbrook, 1960; Watanabe et al., 2001; Le Bourhis and Rouxel, 2003; Shang and Rouxel, 2005). These have been attributed to the differences in loading time, hold period and surface roughness employed by different authors. Also, modelling of the behaviour has to consider both viscosity and elasticity (Chapter 6, Appendix 8). Viscous deformation is

Fig. 8.13 Mean hardness as a function of temperature for soda-lime-silica glass: &, Watanabe et al. (2001); , Smith and Zheng (2000); , Le Bourhis and Metayer (2000);, Westbrook (1960). (Reprinted from Le Bourhis and Rouxel, 2003, with permission from Elsevier.)

173

174

8 Contact Resistance of Glass

Fig. 8.14 Hardness (log scale) as a function of reciprocal temperature for soda-lime-silica glass: &, Watanabe et al. (2001); ~, Smith and Zheng (2000); ^, Le Bourhis and Metayer (2000); ^, Kurkjian et al. (1995). (Reprinted from Le Bourhis and Rouxel, 2003, with permission from Elsevier.)

time-dependent and depends on history. Also, well below the glass transition, a decrease of the hardness is observed on increasing the temperature. At such low temperature ( m (this is also the case for most ceramics) and hence m < 1 corresponding to a large spread of lifetime values. In contrast, glass ﬁbres show much higher Weibull modulus so that n 2 < m and m > 2 allowing for a better prediction of fatigue strength. Equation (9.11) can be written in the form t ¼ sn f ½Ps ðV; sÞ

ð9:14Þ

9.6 NiS Phase Transformation

where f is a function of Ps(V,s). Interestingly, this result shows again a strong dependence on applied stress s as 1/sn.

9.5 Applications

Delayed fracture has to be determined and known in order to predict glazing performance. This is a complex task since it involves environment-dependent parameters, while glass fracture prediction supposes ﬂaw population statistics to be known. As mentioned above, for glass articles showing low Weibull modulus, a large spread of lifetime would be obtained. Proof testing is a way to eliminate weak members. The elements are subjected to a short-term stress cycle similar to that employed in service while in excess of that required. The articles with the largest ﬂaws fail and are eliminated from the distribution which is biased towards the highstrength region. As a matter of fact, the articles can be used under service conditions with a higher degree of conﬁdence. Alternatively, there exist ways to prevent stress corrosion. One of these is to temper the glass. Then, the cracks that are generally present at the surface (Chapter 8) are submitted to compressive stresses provided that the glazing has been designed in such a way that the service tensile stress does not exceed the residual compression (Chapters 6 and 7). Another way is to take advantage of the development of hydrophobic thin ﬁlms which might also yield new solutions to fatigue issues (Chapter 12). Such ﬁlms can be used to protect the glass from moisture. As detailed in Chapter 12, one problem of such coatings is their physical and mechanical stability with time (poor resistance against UV and contact loadings; see Chapter 8).

9.6 NiS Phase Transformation

Ageing of glass may also be observed because of the physical transformation of internal defects like metastable nickel sulphide (NiS) inclusions. These undergo a slow transformation at room temperature from a denser to a lower density phase. These inclusions can be of different compositions, namely NiS, Ni1xS or Ni7S6, with sizes in the range 1–10 mm (Barry et al., 1998). S comes from the raw materials and combustion, while Ni might appear because of the abrasion of the tools used for batching (Chapter 10). In fact, it remains impossible to eliminate these NiS inclusions. Their content is estimated at about 1 particle for 10 tons of glass. The transformation takes place around 335–380 8C and is written a-NiSðhigh temperatureÞ ! b-NiSðlow temperatureÞ

ð9:15Þ

199

200

9 Ageing of Glass

with a relative increase in volume of the inclusion given by e ¼ DV=V 2 4%

ð9:16Þ

Transformation strain can be accommodated over Tg by viscous ﬂow. On the contrary, below Tg transformation strain remains in the glass article. It may drive the slow growth of the cracks up to the point where they become unstable in the residual tensile stress ﬁeld in the core of the tempered glass yielding spontaneous fracture (Swain, 1981; Aben and Guillemet, 1993). In fact, the inspection of fragmented windows reveals that NiS particles are present at the origin of the fracture (at the centre of the mirror zone; Chapter 7) and located at the glass centre. This does not mean they are not uniformly distributed in the glass but, rather, fracture happens only when the particles are in the tensile zone. Phase-transformed NiS inclusion can be observed in a polarizing microscope using photoelasticity to reveal the induced stress ﬁeld (Aben and Guillemet, 1993; for details on photoelasticity see Chapter 11). The radial displacement at a distance r is a function of the increase in volume e: ur ¼

e R 3 3 r

ð9:17Þ

where R is the particle size. Radial displacement increases considerably with particle size (as R3). The maximum stress resulting from phase transformation (when NiS volume change is not accommodated at elevated temperatures) scales with s eG

ð9:18Þ

where G is the shear elastic modulus. At 800 8C (in the glass melt) only the a phase exists. When the cooling rate is low, there is time enough for all NiS particles to transform into the b form. The change in volume can be accommodated when the glass is still viscoelastic. The result is that all NiS inclusions are in the b form and the glazing is stabilized. This is the case for a ﬂoat glass at the lehr exit (Chapter 10). On the contrary, when the glazing is tempered the ﬂoat glass is to be re-annealed at about 650 8C while NiS inclusions transform from the b into the a form again. On tempering the glass, the change back to the b phase cannot take place at elevated temperatures because of the very fast cooling rates being employed but continues at room temperature (Chapter 6). It is accelerated by solar radiation absorption that increases the temperature of the glazing. This transformation follows kinetics over a long time frame; the volume mismatch induces stresses into the glass so that fracture may actually happen a long time after production (some months or years). Obviously there are several parameters that yield a more rapid fracture (Barry et al., 1998): i. the size of the inclusion, ii. the presence of a ﬂaw at its proximity, iii. the intensity of the tensile stress, and iv. the tempering degree of the glazing.

9.7 Crack Healing

Glassmakers report fracture induced by 40–100 mm particles for glazing tempered at compressive surface stresses of 100–120 MPa. Thereafter, it has been of utmost importance to ﬁnd a treatment to transform the NiS particles into their b stable phase, in particular in tempered glazing. Therefore, a thermal treatment (heat soak test, HST) of these glazings has been added to accelerate the transformation of NiS inclusions. This modiﬁcation of the manufacturing process of tempered glass (‘heat soaking’) can prevent the phase transformation from taking place during service and thus efﬁciently guarantees the product against such spontaneous failures (Barry et al., 1998; Gy, 2003). The temperatures during such a treatment are assumed to be low enough as compared to the transition temperature so that we may neglect changes in glass thermal strengthening. In fact, heat soaking treatment is carried out at about 300 8C. At this temperature, NiS transformation is completed after 2 h (Barry et al., 1998) and thus any products containing particles of size larger than the critical dimension break, thus eliminating the risk of breakage during use (Aben and Guillemet, 1993). Moreover, since a properly tempered glass has a compressive residual stress everywhere in the surfaces, tempered glazings designed in this way are protected against ageing since static fatigue is avoided as detailed above. Nonetheless, this heat soak test involves industrial added costs since (i) it requires heattreating furnaces, (ii) it increases the operation times and (iii) it may affect the tempering whenever deviation of maximum treatment temperature happens in the HST processing.

9.7 Crack Healing

All the ageing phenomena mentioned above are room temperature events. Obviously, thermal treatments may considerably change the behaviour of glass since viscous ﬂow may progressively appear. In fact, crack healing is reported with related ‘closing’ of the cracks. Thereafter, the mechanical performance may be improved (Fig. 9.7). Nonetheless after the heat treatment is completed, ageing is observed again in the annealed glass as its stress at rupture decreases with the lifetime as detailed in Section 9.3 (see also Chapter 7).

201

203

10 Mechanics of Glass Processes 10.1 Introduction

Industrial processes are numerous and depend on the application (glazing, containers, ﬁbres, etc.). It is beyond the scope of this book to review all of them. Instead, we shall illustrate by some examples how glass mechanics is to be considered throughout the industrial process. We have selected widespread industrial tools regarding ﬂoat glass, containers and ﬁbres. This chapter can also be nicely illustrated by a video produced by France Te´le´vision (FR3) entitled ‘C’est pas sorcier se met au verre’. All processes require a furnace with a high capacity, a long production line for upstream operations (batching, melting, ﬁning, forming and annealing), while downstream operations (reheating, forming, moulding, coating, tempering, laminating) can be performed on-site or off-site (Fig. 10.1). All these operations require a deep understanding and application of mechanics. At elevated temperatures, viscosity controls the homogeneity of the glass melt, the ﬂatness of the glass while the thermomechanical properties determine the strength of the refractories used to fabricate the tools. At lower temperatures the tribological resistance of glass products will control surface quality and strength of the manufactured objects (ﬂat glass, containers). Industrial production numbers show that tools have achieved great efﬁciencies since the industrial furnaces for ﬂoat line and bottle line produce an average of 500 and 300 tons of glass per day respectively. A unique ﬂoat line produces per day glazing surfaces required for one building as high as Montparnasse tower (Flessel, 2003). The production frequency of bottles is about 10 per second in a conventional production line. Further evolutions are carried out to meet increased capacity, ﬂexibility, availability and glass quality. In fact, maintenance, cleanliness and fabrication practices have been considerably modiﬁed. Four primary operations for glass manufacturing are i. batching, ii. melting, iii. ﬁning and iv. forming. Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

204

10 Mechanics of Glass Processes

Fig. 10.1 Fibreglass production unit at Ladenbourg. (Copyright Saint-Gobain.)

Batching, melting and ﬁning operations are common to all glass manufacturing processes with some variations according to the furnace type. The forming and postprocess depend on the end product. 10.1.1 Batching

Batching encompasses raw material selection based on chemistry, purity, uniformity and particle size. The batch comprises sand for silica, while modiﬁers are introduced as carbonates instead of oxides to reduce energy costs (Table 10.1). The batch selection is adapted to the end product, for instance ﬁbre production requires more selection and ﬁner raw material particle size than container production. Also raw material humidity is controlled using IR analyser on modern production lines; also, impurity concentrations (Fe, Ni) are checked. Recycling of the glass has become an important parameter at this step and allows energy gains since a lower energy is required to melt the raw materials mixed with the recycled glass. Flat glass manufacturers recycle up to 30 % of their own cullet while domestic recycling of the containers has become widespread (60 to 90 % of the domestic packaging is recycled in Europe for instance). Recycled containers are separated according to their Tab. 10.1

Raw material composition for standard soda-lime-silica glass production.

Raw material

Sand

Sodium carbonate

Calcium carbonate

Metal oxides

Concentration (%)

54

24

16

2

10.1 Introduction

colour to optimize the achieved product. Also, recycling may introduce ceramic contaminants that undergo reactions with the glass melt and are present as inclusions in the ﬁnished product. Metal and organic contaminants create instability during glass processing (through reduction/oxidation reactions) and degrade the quality of the glass. Delivery, mixing and sizing processes are highly abrasive, and equipments contain metals and ceramic-coated wear surfaces. Therefore, contamination risks exist from the tools and, actually, nickel sulphide particles are believed to form from nickel contained in such tools and from sulphur impurities introduced by combustion and are responsible for the delayed fracture of tempered glazing (Chapter 9). 10.1.2 Melting

Melting consists of complex chemical and physical phenomena. A large energy above the thermodynamic value 2.7 MJ kg1 is required to fabricate soda-lime-silica glass. Out of 1.2 kg of raw materials, 1 kg forms the glass while 0.2 kg forms the gas, mainly CO2. These large volumes of gas help in the ﬁning of the glass as discussed in the next section. Sand and sodium carbonate grains react as follows: SiO2 þ Na2 CO3 ! Na2 SiO3 þ CO2

While calcium carbonate transform as CaCO3 ! CaO þ CO2

Glass furnaces are used for melting the raw material particles and for transforming these into glass. The low melting constituents (alkali oxides) melt and dissolve the higher melting constituents such as quartz and alumina. Different furnaces are used for producing containers, ﬁbreglass, ﬂat glass and speciality glass. They can be divided into those heated electrically and those heated primarily by combustion. Often electrical heating is used in combination with fuel ﬁring (so-called electric boost) to improve heating uniformity and melt efﬁciency and to reduce gas consumption and emissions that is a matter of prime importance in the context of global climate changes. Recycling glass allows emissions to be reduced, which were at a maximum in 1980 before decreasing up to the present (Flessel, 2003). Other polluting emissions (NOx, SOx) are generated and are reduced improving combustion (using oxygen instead of air) and fuel quality. Furnaces are all made of refractories that allow for long lifetimes (of 10 years for ﬂoat and container furnaces) before requiring rebuild costs. The cost of rebuilding a ﬂoat or container furnace is in the region of s1 million. Electrical heating is used extensively and exclusively in smaller speciality and ﬁbreglass melting units because of its lower initial cost and low emissions as compared to combustion furnaces even though energy costs remain high. This

205

206

10 Mechanics of Glass Processes

drawback is compensated by ﬂexibility in particular when small production volumes are required for speciality products. Glass conductivity plays an important role in this process: while being electrically insulating at room temperature, the glass melt can be heated by the Joules effect (see also Appendix 13). Most furnaces are combustion heated which can be further divided according to the method used to recover exhaust waste heat and the way fuel is burnt (with air or oxygen). Oxygen fuel technology offers several advantages even though requiring pure oxygen. Regenerators can be avoided, eliminating furnace superstructures. Heat recovery is of utmost importance since only 10 % is used for the melt while 70 % is lost through exhaust. Exhaust waste heat recovery is performed using regenerators that alternately store and recover heat, the shift being about every 20 minutes.

Fig. 10.2 (a) Glass furnace interior. (Copyright Saint Gobain.) (b) Glass furnace schematic. Burning and air ﬂow alternate, regenerators being either active or passive accordingly.

10.1 Introduction

In ﬂoat furnaces, several regenerators (their number depending on the furnace capacity) are placed on each side of the furnace while in container furnaces, two regenerators are placed both on the back side (the gas ﬂow forming a U loop). Regenerators consist of enormous thermal capacity refractories that alternately either store energy or recover warm air to the active burners. In a ﬂoat furnace, burners are located on opposite sidewalls (Fig. 10.2). Firing alternates from side to side, the regenerators being alternately passive (stocking) or active (restitution). Such a procedure allows for production of glass with only twice the thermodynamic number (5.4 MJ kg1; Flessel, 2003). Alumina-zirconia-silica (AZS) refractories are used to contain the glass melt and to resist corrosion. The furnace roof is made of silica which presents low thermal expansion, which is important since the roof experiences elevated temperature (1600 8C), the melt being annealed from its top. Also when dislodged pieces fall into the melt, they are more easily dissolved. Downstream, dislodged pieces cannot be dissolved any longer and then dedicated materials are selected: pure alumina is used for the exit of ﬂoat glass furnaces and feeders used for delivery of automatic blowing machines. Large thermal gradients exist in the melt because raw materials are introduced progressively. Convection ﬂow (velocity of the order of millimetres per second) is induced and favours thermal exchange and glass homogeneity. Of much interest for the glassmaker, two principal convection ﬂows are generated in the ﬂoat furnace, one in the melting zone and another in the ﬁning zone. This allows preservation of the ﬁning zone from the batch. In container furnaces, separation is obtained by a barrier placed at the bottom of the furnace. In contrast, radiative transfer is the dominant exchange mode between the roof and the glass melt surface. 10.1.3 Fining

Glass ﬁning produces a molten glass that is uniform in terms of composition and temperature, and bubble free. In fact, the temperature of the glass delivered from the melting furnace, and its composition, has to be regulated with extreme care. This requirement inﬂuences the next operation, that is, glass forming, and as seen in Chapter 6, the latter operation is dependent on viscosity, that is, on the way the glass has been prepared. Consider for instance that a glass gob is to fall under its own weight in order to become correctly placed in a mould. If the viscosity is too high it will not do so in time for the next operation (say the introduction of compressed air to blow the glass out to the shape of the mould) but if it is too low the glass will fall too far and the ﬁnished article may be too thick at its base. Fortunately, large volumes of gas are rejected from the raw materials before transformation in a glass melt and this helps homogenize the melt considerably. Before glass delivery, bubbles have to be eliminated. Bubbles contain trapped air (oxygen, nitrogen) and decomposition products of the raw materials, mainly carbon dioxide. Large bubbles rise to the top of the melt and participate in melt homogenization. In contrast, small bubbles would not eliminate because of increasing required time as their size diminishes (Appendix 4). There are then two alternatives: either gas dissolves into the melt or bubbles are increased in size so that they rise more rapidly to the surface. These

207

208

10 Mechanics of Glass Processes

operations are accelerated by ﬁning agents that are introduced in small quantities in the batch and hence in the glass melt. Fining agents like arsenic and antimony increase dissolution rates. The mechanism by which these agents enhance dissolution of gas from bubbles is still debated; a change in oxidation state of the melt or increasing the rate of oxygen diffusion is suggested. Sodium or calcium sulphate ﬁx on small bubbles that are favourable nucleation sites for ﬁning agents and release gas, increasing the related bubble size and this hence facilitates their elimination (Appendix 4): 2Na2 SO4 ! 2Na2 O þ O2 þ 2SO2

The ﬁning zone is generally gas ﬁred; an electric boost can also provide increased efﬁciency in getting uniform temperature. 10.1.4 Forming

As stated above, the forming operations have been developed for different applications. Flat glass, container and ﬁbre tools present different viscosity, stress and strain rate regimes. The tools have been developed accordingly. Some of these are described in the continuation of this chapter.

10.2 Float Process

Let us consider the fabrication of ﬂat glass which is produced nowadays by the ﬂoat process. This process was introduced by Pilkington Brothers Ltd in the 1950s (see Chapter 3). Firstly, the raw materials (sand, soda, lime) are continuously introduced into the furnace, melted at 1500 8C, homogenized by convection and ﬁned to eliminate bubbles (Fig. 10.3). The furnace contains typically 2000 tons of glass and produces every day 500 tons of glass. The viscous liquid travels onto the ﬂoat at a temperature of 1100 8C under a nitrogen atmosphere in order to prevent corrosion of the tin bath. Under these conditions the equilibrium thickness of the glass sheet is about 6 mm so that the sheet has to be expanded or contracted by top rolls (or rollers working from the top of glass) to produce thinner or thicker glass sheets respectively. The equilibrium equation is written (Fig. 10.4; Langmuir, 1933) gt2H rg rg 1 ¼ zga þ zgb zba 2 rb

where g is the gravitational acceleration, tH the sheet thickness, rg and rb the density of glass and bath, z the surface energy and subscripts g, b and a indicate glass, bath and atmosphere respectively. Taking rg ¼ 2500 kg m3, rb ¼ 6500 kg m3, zba ¼ zgb ¼ 0.5 J m2 and zga ¼ 0.35 J m2, one ﬁnds tH¼6.8 mm.

10.2 Float Process

Fig. 10.3 (a) Float line at Chennai. (Copyright Saint-Gobain.) (b) Schematic representation of a ﬂoat line (CVD and spray unit locations are indicated and optional). (c) Float glass line end showing transiting glass on rollers. (Copyright Saint-Gobain.)

209

210

10 Mechanics of Glass Processes

Fig. 10.4 Float ribbon mechanical equilibrium on a tin bath.

Several pairs of top rolls are used; they are made of steel and are water cooled. Their rotation axis is horizontal and shifted out of the ﬂoat axis to draw the glass ribbon. The range of commercial thickness is between 2 and 19 mm. Glass with lower thickness ( 1. Potential energy is the sum of attraction and repulsion contributions: Ep ¼ Erep þ Eattr ¼

a 1 qq0 m r 4peo r

Potential energy is plotted in Fig. A2.4; ro is the distance corresponding to the energy minimum (force is then zero). This corresponds to the equilibrium distance

A2.3 Bond Formation

Fig. A2.4 Potential energy as a function of distance resulting from electron repulsion predominant at short distance and ion attraction predominant at long distance.

and is called the bond distance. Bond distance allows for ion size to be determined. In the present case ro ¼ rNaþ þ rCl . Ionic crystals are formed by ions that all interact electrostatically with r1 being a decreasing function. A simple calculation of the attractive energy can be made for a one-dimensional chain of N ions of opposite charge (q ¼ q0 ; Kittel, 1983; Fig. A2.5): lnð1 þ xÞ ¼

x2 x3 x4 x þ 2 3 4

NEattr ¼ 2N

qq0 1 1 1 1 þ 4peo r 2r 3r 4r

1 qq0 1 1 1 1 qq0 ¼ 2N 1 þ ¼ 2N ln2 4peo r 2 3 4 4peo r Eattr ¼ 2

1 1 2ln2 1 b ln2 ¼ ¼ 4peo r 4peo r r

where 2 ln 2 (¼ 1.38) is the Madelung constant for a one-dimensional chain. For a three-dimensional solid, the calculation is more difﬁcult and yields a Madelung constant of 1.74 for NaCl.

Fig. A2.5 One-dimensional and periodical ion chain.

269

270

Appendix 2: Atomic Structure and Bond Formation

The variation of Ep can be generalized to any bonds and solids in the following form: Ep ¼ Erep þ Eattr ¼

a b rm rn

with m > n since repulsion is dominant over attraction at low r. The Lennard-Jones potential is written for m ¼ 12 and n ¼ 6.

271

Appendix 3 Thermal Expansion and Elasticity A3.1 The a–E Trend

Materials’ thermal expansion coefﬁcient a and stiffness (elastic modulus E ) are related. In fact a ceramic (stiff material) will expand less than a polymer. This general trend is observed in the a–E chart (Fig. 2.8) where all classes of materials are considered. This trend is mathematically formulated as a¼

gG rcv 3E

where the Gru¨neisen ‘constant’ gG is not a constant but varies within one order of magnitude (0.4 < gG < 4), r is the density and cv the speciﬁc heat cv cp. A simple approach to thermal expansion is proposed by Zarzycki 1982 and Kittel 1983. We shall review brieﬂy here their approaches.

A3.2 Qualitative Approach

Figure A3.1 shows schematically the potential energy of bonded atoms. The continuous line is for a more rigid material since it shows a deeper potential. Parameter ro corresponds to the equilibrium distance at T ¼ 0 K. This temperature cannot be produced, so for clarity we take this temperature as a reference point. At T > 0 K, atoms oscillate around their equilibrium position. It is important to note that the potential is not symmetric. For small oscillations, one generally neglects this phenomenon and takes a parabolic function in the form Ep ¼ (1/2)k(r ro)2 also called the harmonic potential. Force is then F ¼ k(r ro). Under such an assumption, no thermal expansion is found (Fig. A3.2). Now considering the fact that the potential is not symmetric, the average distance between atoms shifts towards the right-hand side of Fig. A3.1, or the materials are expected to expand when they are heated. Here, we do not consider any phase Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

272

Appendix 3: Thermal Expansion and Elasticity

Fig. A3.1 Potential energy as a function of distance for weak (dashed line) and strong (continuous line) bonds.

changes which either yield contraction or expansion. Materials showing a deeper potential (stiffer materials) show less potential asymmetry (for the same additional thermal energy kT ). Hence, these materials present a lower thermal expansion coefﬁcient than materials having a shallow potential (soft materials). Considering now silicate glasses, when modiﬁers are introduced in the silicate glass, NBOs are formed and yield Si–O potential asymmetry and hence lead to large thermal expansion. In contrast, in borosilicate glasses, B atoms participate in glass network formation and no NBOs are formed maintaining the potential symmetry and hence less thermal expansion is observed for these glasses.

A3.3 Expansion Modelling

In a ﬁrst approximation we may add one asymmetric term to the harmonic potential that we have deﬁned above: Ep ¼ ð1=2Þkðr ro Þ2 þ gðr ro Þ3 ¼ cx 2 þ gx 3

with c ¼ ½k, x ¼ r ro, g < 0 and we assume gx3 kT. When g ¼ 0, we get again a harmonic or parabolic potential.

Fig. A3.2 Potential energy as a function of distance curve showing the harmonic approximation.

A.3.4 Differential Expansion Measurement

Following Kittel 1983, we consider a Boltzmann distribution and the average distance shift at temperature T is R1 xexpðEp =kTÞ hxi ¼ R1 1 1 expðEp =kTÞ

With the following approximation: Ep cx 2 þ gx 3 cx 2 gx 3 ¼ exp ¼ exp 1 exp kT kT kT kT

a series of calculations yields hxi ¼

3g kT 4c2

This simple approach then yields a constant thermal expansion coefﬁcient proportional to g (asymmetric term): a¼

3g k 4c2 r0

We ﬁnd that stronger binding (larger value of c, stiffer materials) yields indeed lower thermal expansion while larger asymmetry (larger value of g) yields larger thermal expansion.

A3.4 Differential Expansion Measurement

A dilatometer is used to determine the thermal expansion coefﬁcient of a specimen submitted to a thermal ramp (constant heating rate). Not only does the specimen expand but also the dilatometer (Fig. A3.3). Hence, differential expansion is

Fig. A3.3 Schematic representation of thermal expansion of both sample and dilatometer.

273

274

Appendix 3: Thermal Expansion and Elasticity

measured and correction is necessary to include the dilatometer expansion in the experimental data. Consider for instance an alumina specimen in an alumina cylindrical support: the apparent expansion would be zero because all expand the same relative length. A diagram can be constructed showing the measured and actual (and superior) expansion (Fig. A3.3).

275

Appendix 4 Falling Sphere Viscometer and Fining of Glass A4.1 Falling Sphere A4.1.1 Asymptotic Regime

Let us consider a sphere of radius r, volume V and mass M ¼ rsV (rs being the sphere density) falling in a viscous ﬂuid of density r (Fig. A4.1). It is subjected to three different forces: (i) gravitational force, (ii) Archimedes reaction and (iii) viscous friction. Newton’s principle is written Mg þ A þ f ¼ Ma

where g is the gravitational acceleration and a is the acceleration of the ball. We have Mg ¼ rs Vg A ¼ rVg f ¼ kv

where v is the velocity and k is taken as the Stokes coefﬁcient: k ¼ 6phr

The ball reaches a constant velocity after a transient period (v ¼ vl, a ¼ 0) that is given by Mg þ A þ f ¼ 0 ðrs rÞVg ¼ kvl

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

276

Appendix 4: Falling Sphere Viscometer and Fining of Glass

Fig. A4.1 Falling sphere in a viscous liquid.

We ﬁnally ﬁnd vl ¼

ðrs rÞVg 2gr 2 ðrs rÞ ¼ k 9h

A4.1.2 Transient Regime

When a falling sphere viscometer is used, one supposes that the asymptotic regime is reached or the transient regime (from velocity v = 0 to vl) is achieved. This regime is obtained solving Mg þ A þ f ¼ Ma

This equation is rewritten as rs V

dv þ kv ¼ Vgðrs rÞ dt

with initially

vðt ¼ 0Þ ¼ 0

The solution is vðtÞ ¼ vl ½1 expðt=TÞ

with T ¼ rs V=k

The solution is qualitatively plotted (Fig. A4.2) for two different values of k (or h). Notably when viscosity increases T and vl decrease. Hence, the asymptotic regime is

A4.2 Fining of Glass

Fig. A4.2 Velocity evolution with time of a falling sphere in a viscous liquid (k1 < k2).

reached more rapidly and after a shorter falling distance. Therefore such conditions are more favourable for the method to be employed. A4.2 1. Fining of Glass Fining of Glass Let us consider the limit velocity solution and consider a bubble formed in a glass melt. The asymptotic solution becomes vl ¼

2gr 2 r 9h

It is of utmost importance to eliminate bubbles in the glass (Fig. A4.3). Considering a period of time t, the distance d that a bubble travels is d ¼ vl t ¼

2gr 2 r t 9h

Fig. A4.3 Handmade and old-fashioned container showing a large amount of bubbles with different sizes.

277

278

Appendix 4: Falling Sphere Viscometer and Fining of Glass

showing a dependence on the square of the bubble size and an inverse dependence on the viscosity: d/

r2 t h

At 1330 8C in a standard melt, it takes 1 minute for a 1 mm diameter bubble to move a distance of 1 mm, while this time becomes 5 h and 20 days for 100 mm and 10 mm diameter bubbles respectively. There are two main ways to accelerate the elimination of bubbles (Chapter 10): (i) decreasing the viscosity, which is done by imposing a higher temperature at the surface; and (ii) increasing the bubbles size, which is done using ﬁning agents.

279

Appendix 5 Theoretical Strength of a Solid Let us consider like Orowan (1949) the potential energy of bonded atoms as shown schematically in Fig. A5.1. Parameter ro corresponds to the equilibrium distance (rigorously, only at T ¼ 0 K; see Appendix 3). Let us apply a force to separate the atoms: F ¼ dEp =dr ðpositive sign since it is the applied forceÞ

Figure A5.1 transforms into Fig. A5.2 when the applied force is plotted as a function of the distance, equilibrium distance ro being obtained for F ¼ 0. The force curve maximizes at Fm. Let us consider a specimen loaded under applied force F with unit section surface made of n atoms (Fig. A5.3). The applied stress is s ¼ nF

Note that we only consider the interactions between atoms in front of each other. This is the ﬁrst assumption. Theoretical strength is written sth ¼ nFm

We have in the elastic domain (for r ro) s ¼ Ee ¼ E

r ro ro

While in this domain we have also s¼n

dF ðr ro Þ dr r¼ro

The work W necessary to cause the fracture of the specimen corresponds to the area shown in Fig. A5.2 and is Z1 W¼

nFðr 0 Þdr 0 ¼ 2z

ro

where z is the surface energy (two surfaces are created on fracture). Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

280

Appendix 5: Theoretical Strength of a Solid

Fig. A5.1 Potential energy as a function of distance.

Next, we shall approximate the F(r) curve by a sinusoidal function to facilitate the calculations as suggested by Gilman (1949). This second approximation leads to the underestimation of the work W; the calculation shows that the theoretical strength is much greater than the observed one (see Section 7.1). In fact the model suggested here leads to the multiple fracture of the specimen since the situation for a given plane is to be considered for all planes. Thereafter, the specimen would be sliced into monatomic planes after such a test. rr o FðrÞ ¼ Fm sin 2p l

Fig. A5.2 Applied force as a function of distance.

Fig. A5.3 Tensile test on a unit surface (n atoms).

Appendix 5: Theoretical Strength of a Solid

Then in the elastic domain (for r ro) we have rr o FðrÞ ¼ Fm 2p l

so that r r o o ¼ sth 2p E ¼ nFm 2p l l

while ro þl=2 Z

nFðr 0 Þdr 0 ¼ nFm

W ¼ 2z >

l l ¼ sth p p

ro

Then multiplying the latter two equations allows one to obtain s2th ro ¼ Ez

that is rewritten rﬃﬃﬃﬃﬃﬃ Ez sth ¼ ro

281

283

Appendix 6 Weibull Analysis The investigation of the strength of brittle solids requires numerous experiments since fracture is statistical. This results from the ﬂaw size distribution of the material. For a ﬁrst experimental approach, one can consider a population of N ¼ 50 ﬁbre specimens of the same length sectioned in ﬂexure (Fig. A6.1). Care is taken in order not to damage the tested length (contact damage, ﬁnger moisture). We suggest the ﬁbre segments be manipulated only by their extremities. Theprocedure consists in testingundertensile stressopticalﬁbresupto fracture.The loading curve F Dl is checked as to its linearity up to fracture. The N stress values at fracture are then ranked in ascending order. Deﬁning x as the number of unfractured specimens at stress s, the probability estimator is taken as Ps ðVÞ ¼ ðx 0:5Þ=N

ðA6:1Þ

where V is the volume of the considered ﬁbres. We use here this simplest expression for the estimator. The precise form of the estimator is still the subject of ongoing research. Several expression for Ps(V) have been proposed in the literature (Bergman, 1984; Wu et al., 2004, 2006): Ps(V) ¼ x/N (simplest one but not generally used because it is not quite statistically correct), Ps(V) ¼ x/(N þ 1), Ps(V) ¼ (x 0.3)/(N þ 0.4), Ps(V) ¼ (x 0.25)/(N þ 0.25), Ps(V) ¼ (x 0.375)/(N þ 0.25) and more generally Ps(V) ¼ (x a)/(N þ b). The step-by-step procedure is then shown in Table A6.1. Figure A6.2 shows Ps(V) as a function of stress for a studied population. The next step consists in obtaining a Weibull diagram plotting ln{ln[1/Ps(V)]} as a function of ln(s). We use here the simplest method, i.e. the linear regression (LR) method. For the weighted linear regression, maximum likelihood and moments methods see Wu et al. 2006. For a single defect population (bimodal populations are not uncommon and lead to strong deviations from a linear plot) the Weibull diagram shows a linear evolution which allows determination of the Weibull modulus, that is, the slope of the linear ﬁt and so from the y-axis intercept

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

284

Appendix 6: Weibull Analysis Tab. A6.1

Glass fibre strength and step procedure to determine Weibull parameters.

s

ln(s)

x

Ps(V ) ¼ (x 0.5)/N

ln{ln[1/Ps(V )]}

Ps(V ), Weibull

2.10 2.11 2.11 2.26 2.26 2.30 2.30 2.30 2.30 2.31 2.32 2.32 2.32 2.32 2.34 2.34 2.34 2.36 2.37 2.38 2.42 2.42 2.42 2.44 2.46 2.46 2.47 2.47 2.47 2.47 2.47 2.50 2.50 2.50 2.52 2.52 2.54 2.54 2.55 2.55 2.58 2.58 2.58 2.58 2.58 2.62 2.62 2.63 2.65

0.74 0.75 0.75 0.82 0.82 0.83 0.83 0.83 0.83 0.84 0.84 0.84 0.84 0.84 0.85 0.85 0.85 0.86 0.86 0.87 0.88 0.88 0.88 0.89 0.90 0.90 0.90 0.90 0.90 0.90 0.90 0.92 0.92 0.92 0.92 0.92 0.93 0.93 0.94 0.94 0.95 0.95 0.95 0.95 0.95 0.96 0.96 0.97 0.97

49 48 48 46 46 44 44 44 44 40 39 39 39 39 35 35 35 32 31 30 29 29 29 26 25 25 23 23 23 23 23 18 18 18 15 15 13 13 11 11 9 9 9 9 9 4 4 2 1

0.99 0.97 0.97 0.93 0.93 0.89 0.89 0.89 0.89 0.81 0.79 0.79 0.79 0.79 0.70 0.70 0.70 0.64 0.62 0.60 0.58 0.58 0.58 0.52 0.50 0.50 0.46 0.46 0.46 0.46 0.46 0.36 0.36 0.36 0.30 0.30 0.26 0.26 0.21 0.21 0.17 0.17 0.17 0.17 0.17 0.07 0.07 0.03 0.01

4.58 3.47 3.47 2.60 2.60 2.13 2.13 2.13 2.13 1.53 1.42 1.42 1.42 1.42 1.05 1.05 1.05 0.82 0.75 0.68 0.61 0.61 0.61 0.43 0.37 0.37 0.25 0.25 0.25 0.25 0.25 0.03 0.03 0.03 0.20 0.20 0.31 0.31 0.43 0.43 0.56 0.56 0.56 0.56 0.56 0.97 0.97 1.25 1.52

0.98 0.97 0.97 0.89 0.89 0.84 0.84 0.84 0.84 0.83 0.81 0.81 0.81 0.81 0.78 0.78 0.78 0.74 0.72 0.70 0.60 0.60 0.60 0.54 0.48 0.48 0.45 0.45 0.45 0.45 0.45 0.36 0.36 0.36 0.29 0.29 0.24 0.24 0.21 0.21 0.13 0.13 0.13 0.13 0.13 0.07 0.07 0.05 0.03

Appendix 6: Weibull Analysis

Fig. A6.1 Rolled glass ﬁbre.

Fig. A6.2 Ps(V) as a function of stress s and Weibull modelled curve with the parameters extracted from least squares ﬁt of ln{ln[1/Ps(V)]} versus ln(s) as illustrated in Fig. A6.3.

Fig. A6.3 Procedure to determine Weibull parameters from a least squares ﬁt of ln{ln[1/Ps(V)]} versus ln(s).

285

286

Appendix 6: Weibull Analysis

since

1 ¼ m lnðsÞ m lnðso Þ ln ln Ps ðVÞ

ðA6:2Þ

This is illustrated in Table A6.1 and Fig. A6.3. The Weibull adjustment is then shown on the Ps(s) plot (Fig. A6.3). Two defect populations may sometimes be observed, due to damage induced while making the experiments. In such a case, the analysis can be made separately for the two populations.

287

Appendix 7 Photoelastic Set-Up for Lectures A7.1 Set-Up for Photoelastic Projection

The proposed set-up comprises a projector used for the projection of slides (Fig. A7.1). This is available in most classrooms and allows the demonstration of transient (Fig. A7.2) and residual stresses (Fig. A7.3). A polarizer or analyser can be obtained as 1 1 m2 panel (HN32 from Sarelec, 91560 Crosne, France, the panels being sold with one edge parallel to the polarization axis). It has to be cut into two squares with area covering the projector plate. For protection these square polarizers can be placed and sealed between two square and annealed glass sheets. One of the panels serves as the polarizer and is set on the projector. The other one serves as the analyser and is rotated by 908 from the polarizer. The glass specimens are then set in between. The image can be projected for a classroom focusing on the glass specimen, and examples are discussed below. Before setting a specimen one checks that polarizer and analyser are shifted by 908 when darkness appears on the screen.

A7.2 Example of a Beam under Flexion (Transient Stresses)

A 3.5 20 400 mm3 glass beam is cut from an annealed glass sheet and the edges abraded. It is to be set under ﬂexion taking the beam by its extremities. The beam is then placed at 458 from the polarization axis. Again analyser and polarizer are rotated preliminarily by 908 to get darkness on the screen, the contrast being maximum under such conditions while vanishing is observed when aligning the beam along polarization axis (isoclinics along principal stress). The photoelastic contrast increases as applied stresses increases. One observes in Fig. A7.2 under white contrast both edges, one being under compressive stress, the other being under tensile stress (top and bottom respectively) while the beam centre shows minimum

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

288

Appendix 7: Photoelastic Set-Up for Lectures

Fig. A7.1 Set-up for photoelasticity experiments in a classroom (A, analyser; P, polarizer; G, glass specimen; S, screen).

intensity at the neutral line. Note that one does not distinguish here tensile and compressive stresses. This can be done adding a wavelength sheet to the set-up. When ﬂexure is released, photoelastic contrast vanishes, showing that these applied stresses are transient.

A7.3 Example of Tempered Specimens (Residual Stresses)

Two glass specimens 3.5 100 100 and 6 100 100 mm3 were thermally tempered under the same conditions. The two shown in Fig. A7.3 correspond to these two specimens and were obtained under the same conditions with the analyser axis perpendicular to the polarizer axis. Again darkness is to be observed before starting the observation of glass specimens. The degree of temper is expected to be more important for the thicker glass since a larger thermal gradient is generated (Chapter 6). One indeed observes more contrast in the photoelastic image for the thicker specimen. This is particularly obvious at the four corners of the specimens where coloured contrasts are even obtained for the thicker specimens. Notably, not only

Fig. A7.2 Photoelasticity image of a beam under ﬂexion (P, polarizer; A, analyser).

A7.3 Example of Tempered Specimens (Residual Stresses)

Fig. A7.3 Photoelasticity images of two specimens, 3.5 100 100 and 6 100 100 mm3, thermally tempered and observed under the same conditions. The thicker one shows more contrast (P, polarizer; A, analyser).

does the stress intensity play a role in the photoelastic contrast here, but also the glass thickness tH since phase shift b ¼ (2p/l)d is proportional to glass thickness and principal stresses difference s1 s2 (Chapter 11). One further observes the signature left by the nozzles as seen at dawn on car backlights (Chapters 3 and 6). These contrasts appear without applying any forces on the specimens showing that stresses are residual.

289

291

Appendix 8 Instrumented Nanoindentation Applied to Thin Films A8.1 Instrumented Nanoindentation

Instrumented indentation allows for monitoring the penetration of a tip into a specimen as a function of load. This technique has become very popular in thin-ﬁlm technology (Fischer-Cripps, 2004a). In fact, when low loads are used, the observation of indents becomes tedious, requiring dedicated instruments like atomic force and/ or transmission electron microscopes, and is time consuming (Le Bourhis and Patriarche, 2003). Therefore, it has become of importance to extract the mechanical properties from the loading–unloading curves (Fig. A8.1). The test consists of loading up to a maximum value Fm (a hold period may be programmed) and unloading to zero. A typical curve is shown in Fig. A8.1. The loading and unloading curves separate when irreversible deformation is generated in the specimen (only the elastic deformation recovers on unloading). Most indentation machines are load controlled. The tip is ﬁxed to a coil merged into a magnetic ﬁeld. Controlling the intensity of the current through the coil allows the force to be controlled. Because of the Joule effect one has to consider carefully the inherent thermal drift of the machine. Displacement is determined using a capacitive sensor (Fig. A8.2). The tips are categorized into sharp and blunt (see also Chapter 8). Sharp tips are generally three-faced Berkovich tips allowing for a better deﬁnition of the contact area Ac than four-sided Vickers tips. However, the aspect ratio is the same for both tips (Ac ¼ 24.5hc2, where hc is the contact depth). Spherical ‘blunt’ tips are used to determine the overall stress–strain s(e) curves (Le Bourhis and Patriarche, 2003; Section A8.2). The proﬁle of a deformed surface under load is shown in Fig. A8.3. The cone loaded by force Fm penetrates the specimen down to hm. The specimen and cone are in contact to depth hc, that is, up to point B. The specimen is observed to deform elastically around the contact area as discussed also in Chapter 8. Assuming unloading is purely elastic, the surrounding surface recovers to its original position shown as A in Fig. A8.3. The mean pressure under load can be extracted from the load–penetration curves (Fig. A8.1) employing the well-known Oliver and Pharr and Field and Swain Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

292

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.1 Typical loading–unloading curve. These curves separate because the specimen has deformed ‘plastically’ on loading while unloading is mainly elastic.

methods, named after their respective authors (Oliver and Pharr, 1992; Field and Swain, 1993). These methods have several limitations. Firstly, one major assumption of both methods is that only elastic recovery happens while unloading; this might not be strictly the case as revealed for very slight indents and when ﬁlms show viscoelastic response (Le Bourhis and Patriarche, 2003). Secondly, the methodology was derived from the solution to elastic contact problems, while prior to unloading the contact conditions involve plastic deformation. Thirdly, the material around the contact may exhibit substantial pile-up or sink-in, the projected contact area being then either underestimated or overestimated, yielding errors in the hardness values (Oliver and Pharr, 1992; Field and Swain, 1993). Considering a sharp contact, the unloading curve can be ﬁtted by (Oliver and Pharr, 1992) F ¼ kðh hr Þm ; 1 < m < 2

Fig. A8.2 Instrumented indentation principle. Loading is electromagnetic while the displacement sensor is capacitive.

ðA8:1Þ

A8.1 Instrumented Nanoindentation

Fig. A8.3 (a) Schematic indentation proﬁle; (b) Experimental indentation proﬁle (Reprinted from Lim and Chaudhri, 2004, with permission from Taylor & Francis Ltd http://www.informa world.com). Original surface is shown as A; contact between specimen and indenter is up to B. Elastic deformation of the surface is observed all around the indenter.

where F is the load applied to the indenter, h its penetration and hr the residual depth (after complete unloading). Contact stiffness (S ¼ dF/dh) at maximum load is then determined as S ¼ kmðhm hr Þm1

ðA8:2Þ

where hm is the maximum penetration of the indenter. The contact depth hc (Fig. A8.3) is then given by hc ¼ hm eFm =S

ðA8:3Þ

293

294

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

where hm, Fm and S are the penetration, force and stiffness at maximum load and e is obtained from the following equations (Woirgard and Dargenton, 1997; Fig. A8.4). We adopt the modiﬁed Sneddon (1965) solution in the following, although it is still debated in the literature (Lim and Chaudhri, 2004, 2006): e ¼ mð1 gÞ

ðA8:4Þ

1 G½ð1=2Þn þ 1=2 g ¼ pﬃﬃﬃﬃ p G½ð1=2Þn þ 1

ðA8:5Þ

where G is the gamma function, GðxÞ ¼

Ð1 0

et tx1 dt, and

n ¼ 1=ðm 1Þ

ðA8:6Þ

where m is the exponent of the unloading curve deﬁned above. Then, from the contact depth knowledge, contact area is determined by Ac ¼ 24:5hc2

ðA8:7Þ

and hardness is calculated as H ¼ Fm =Ac

ðA8:8Þ

It should be noted that hardness values obtained from instrumented nanoindentation and microindentation may differ signiﬁcantly and this phenomenon is invoked as the indentation size effect (ISE).

Fig. A8.4 e(m) curve.

A8.2 Indentation Strain Field

Another advantage of instrumented nanoindentation is that the elastic properties of materials can be determined. The composite modulus (specimen–tip) E is extracted from rﬃﬃﬃﬃﬃ @F Ac ¼ 2bE S¼ ðA8:9Þ @h p where S is the stiffness at maximum penetration, Ac the contact depth and b is a correcting factor depending on the tip geometry (b ¼ 1.034 for a Berkovich tip). The composite modulus (specimen–tip) E is 1 1 n2D 1 n2S ¼ þ E ED ES

ðA8:10Þ

where E and n are Young’s modulus and Poisson’s ratio, and subscripts D and S indicate diamond and specimen respectively (ED ¼ 1141 GPa, nD ¼ 0.07). The reduced modulus is often referred to as 1 1 n2S ¼ Er ES

ðA8:11Þ

Note that when viscoelastic materials are considered, it is important to control carefully the loading–unloading procedure (Fischer-Cripps, 2004a; Mammeri et al., 2004, 2005). In fact, for such kinds of materials indentation response is time dependent with a characteristic relaxation time TR ¼ h/G, where h and G are the viscosity and shear modulus of the material (Chapter 6; see also Section A8.5.1). Interestingly, some instrumented machines allow for adding a force modulation to the applied force at a given frequency and hence dynamic mechanical analysis can be performed (Chapter 6; Fischer-Cripps, 2004a).

A8.2 Indentation Strain Field

When indenting a sample a plastic zone is generated and surrounded by the undeformed solid. Hence, a plastic strain gradient remains in the specimens after unloading. The representative indentation strain eR is deﬁned as (Tabor, 1951; Johnson, 1985) eR ¼ 0:2d=D for a spherical indenter

ðA8:12aÞ

eR ¼ 0:2tanb for a conical indenter

ðA8:12bÞ

and

where d and D are the residual indent diameter (or contact area diameter) and the sphere diameter respectively, while b is the angle between the original surface and the conical indenter ﬂank. eR increases continuously as load is increased under a spherical tip (Eq. A8.12a). This point has motivated the use of a spherical tip to

295

296

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

determine the overall s(e) stress–strain curve (Field and Swain, 1993). Under a conical indenter the representative strain remains unchanged (assuming a perfect sharpness of the tip), a property that is often referred to as self-similarity or autosimilarity. The self-similarity of the strain ﬁeld under a conical indenter is attributed to the geometric similarity of the tip (Ac / hc2 , where hc is the contact depth). Selfsimilarity is also assumed for non-axisymmetric tips like Berkovich and Vickers tips. Parameter b is then the angle between the original surface and the ﬂank of a conical indenter with equivalent aspect ratio. For instance, for the Vickers and Berkovich tips which are most commonly used, the contact area is Ac ¼ 24:5 hc2 so that b is to be taken as 198. A question has risen as to the signiﬁcance of eR in view of strain gradient (Chaudhri, 1998). Furthermore, Eqs (A8.12) were established originally for metals and applied regardless of the type of material. Indentation residual strain can be determined experimentally in brittle materials (AlAs/GaAs superlattice) using a focussed ion beam (FIB) milled cross-section through the centre of a Vickers indentation. The sub-layers in the superlattice allow then mapping of the deformation, the interfaces between the AlAs (or GaAs) sub-layers being used as markers (Largeau et al., 2005). The distance e between two GaAs layers at different points of the sample was compared to the period eo of the superlattice (Fig. A8.5) and the ez strain component along the loading axis can be calculated using equation ez ¼ (e eo)/eo. Figure A8.5 shows the ez contours, and as reported for metals very high strains and strain gradients are generated just beneath the indent site. The highest ez value is determined to be about 28 % in good agreement with Chaudhri (1998) who estimated the strain e to be as large as 20 % under a Vickers indenter in heavily work-hardened mild steel. These strain values are considerably higher than the representative strain value eR that is commonly accepted for a Vickers geometry (about 7.2 % (Eq. (A8.12b) with b ¼ 198 for a Vickers tip). The representative strain eR is hence to be considered as an averaged strain. Nonetheless, it is still unclear which deformed volume should be considered when averaging the strain (Chaudhri, 1998; Largeau et al., 2002).

A8.3 Hardness, Yield Stress and Representative Flow Stress

Hardness measures the resistance of a surface to contact loading (Tabor, 1951, 1996; Fischer-Cripps, 2004a). Traditionally, a spherical or a Vickers diamond (four-sided) pyramid is loaded on the investigated surface. The hardness (or mean pressure) p is deﬁned by the ratio between the applied load and the projected surface of the permanent deformation left by the indenter: p ¼ Fm =Ap

ðA8:13Þ

We denote it p in this appendix (H in the main text) in order to compare microhardness p and nanohardness H as extracted from nanoindentation curves. As discussed in detail, p and H may differ. Macro-, micro- and nanoindentation

A8.3 Hardness, Yield Stress and Representative Flow Stress

Fig. A8.5 (a) FIB-TEM cross-sectional view of an indented brittle semiconductor (AlAs/GaAs superlattice); (b) ez strain contours as obtained from (a). Strain values are given in percent. The dark area drawn on the graph represents the material punched into the sample (residual indentation).

domains have been deﬁned and hardness values are to be compared in the respective domain since an ISE is reported for many types of materials (Gao et al., 1999; Sangwal et al., 2000; Elmustafa and Stone, 2003). In the macro- and microindentation domains the surface is generally determined after unloading by optical microscopy. We shall refer to this area as Ap (projected area deﬁned above). Going to the nanoindentation domain, observation of the indent becomes tedious

297

298

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

and requires scanning electron microscopy (SEM), atomic force microscopy (AFM) or eventually transmission electron microscopy (TEM) resolutions. Hence, hardness is determined under load and is deﬁned as the ratio of the force to the projected contact area Ac (Section A8.1): H ¼ Fm =Ac

ðA8:14Þ

It should be noted also that hardness values p and H may differ signiﬁcantly. Let us consider for instance the elastic domain (before plastic onset). The indent recovers entirely so that Ap ¼ 0 and p is not deﬁned. In contrast, H can be determined advantageously by mean of an instrumented indentation machine. Also, plastic relaxation of the indents may yield differences between Ap and Ac and this phenomenon has been invoked sometimes to interpret the ISE. It should be noted that for elastic–perfectly plastic materials, the mean pressure under a conical indenter p is generally assumed to be three times the yield stress Y (Tabor, 1951; Johnson, 1985): p ¼ 3Y

ðA8:15aÞ

For the particular case of a Vickers tip, Eq. (A8.15a) is rewritten Hv ¼ 2:8Y

ðA8:15bÞ

These relationships can be extended to strain-hardening materials with good approximation if Y is replaced by the representative ﬂow stress YR measured in simple compression at the representative strain eR (Johnson, 1985): p ¼ 3YR ¼ 3YðeR Þ

ðA8:15cÞ

Strain hardening is often taken as YR ¼ Ke1=n (Hollomon, 1945). In the R literature, it must be said that there has been some confusion between the different Eqs (A8.15) which have been used regardless of their domain of validity. However, the aperture of the tips commonly used is generally large so that the representative strain is below 8 %, which for low strain-hardening materials leads to Y YR. Nonetheless, sharp cube-corner tips are now being employed to lower the plastic onset and, hence, to deform the specimens under smaller loads. For such a tip, Eqs. (A8.15) should be used more carefully. In terms of resolved yield stress Eqs (A8.15) and (A8.15c) are rewritten p ¼ 6tc and p ¼ 6tR (where tR is the representative resolved yield stress and using the Tresca factor). In fact, according to the class of materials, the relationship between and H and Y (or H and t) is to be reconsidered with care since ratio H/Y varies (Gilman, 1973; Johnson, 1985). Hence we shall introduce a constraint factor C into Eqs (A8.15) which is expected to vary according to the type of material: p ¼ CYR

ðA8:15dÞ

A8.3 Hardness, Yield Stress and Representative Flow Stress

A general relationship is written (Marsh, 1964; Johnson, 1985) p 2 1 EeR ¼ 1 þ ln YR 3 0:6 YR

ðA8:15eÞ

Indentation with a conical tip allows determination of the representative ﬂow stress YR at the representative indentation strain eR. Following Johnson’s model, Harvey et al. (1993) and Kramer et al. (1999) suggested that the representative ﬂow stress YR of a material could be determined measuring the plastic zone radius c as a function of the maximum load F applied to the indenter using Eq. (A8.16a) (Le Bourhis and Patriarche, 2003): YR ¼

3 F 2p c 2

ðA8:16aÞ

This relation is established balancing the radial forces at the elastic–plastic boundary (Kramer et al., 1999; Fig. A8.6): F ¼ pc2 sr ðcÞ

ðA8:16bÞ

where the radial stress sr at the elastic–plastic boundary is given by (Johnson, 1985) 2 sr ðcÞ ¼ YR 3

ðA8:16cÞ

The proper use of Eq. (A8.16a) supposes that small indenting loads are applied to the specimens in order to avoid fracture and remain in the plastic regime. This is possible using the nanoindentation technique. Equation (A8.16a) indicates that the plastic zone size varies linearly with the square root of the applied load. Figure A8.7b plots the central plastic zone size c as well as the rosette arm length (LA and SA, Fig. pﬃﬃﬃﬃﬃﬃﬃﬃ A8.7a) as a function of the square root of the maximum load, Fmax , measured in an indented brittle material (single-crystal (1 1 1) GaAs). All the sizes can be measured precisely on TEM plan views (Fig. A8.7a). Very interestingly it can be observed that all sizes (central zone radius c as well as the SA and LA sizes) are observed to increase pﬃﬃﬃﬃﬃﬃﬃﬃ linearly with Fmax as expected from Eq. (A8.16a) (greater discrepancy is obtained for the LA sizes however).

Fig. A8.6 Indentation stress balance.

299

300

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.7 (a) TEM plan view image of an indent site made under 5 mN at room temperature in a brittle semiconductor ((1 1 1)A face of GaAs, g ¼ [220] diffraction condition). The central plastic zone (c), long arms (LA), short arms (SA) and microtwins (M) are shown. (b) Central plastic zone radius c and lengths of the rosette arms (LA and SA) as p a ﬃﬃﬃﬃﬃ function of the square root of ﬃ the maximum applied load ( Fm ) ((1 1 1)A and (111)B indented surfaces of GaAs crystal; Le Bourhis et al., 2004).

It should be noted that AFM can also be employed to determine the plastic zone size measuring the topography of the indent proximity (Harvey et al., 1993; Kramer et al., 1999). In that case, the plastic zone size is estimated from the upset region or pile-up. Except for very small indents where plastic recovery is observed, the upset zone radius determined by AFM shows also a square root dependence on load (Lilleodden et al., 1995). Interestingly, microindentation at elevated temperature also yields a square root dependence on load of the rosette arm length in a wide variety of materials as reviewed by Chaudhri (2004). pﬃﬃﬃﬃﬃﬃﬃﬃ Using the linear variation of the central plastic zone with Fmax plotted in Fig. A8.7, the ﬂow stress is estimated to be about 3.4 GPa yielding an H/YR ratio about 2.5 close to the value expected from the expanding cavity model (H/YR 3; Johnson, 1985).

A8.4 Coating–Substrate Composite Response

Using low load and increasing progressively the load, the instrumented nanoindentation technique allows for investigation of the elastic–plastic response of coatings as well as their adhesion to the substrate (Fig. A8.8). Indeed, the probe size can be adjusted to the ﬁlm thickness using appropriate loads. For dedicated study, in particular when surface roughness is important, cross-sectional nanoindentation can be carried out on smoothly prepared cross-sections and a mechanical proﬁle is extracted (Marot et al., 2002).

A8.4 Coating–Substrate Composite Response

Fig. A8.8 Two different ways to characterize the indentation response of thin ﬁlms either testing a prepared cross-section under constant load (CSN) or testing the ﬁlm surface under decreasing loads (PN).

Mencik et al. 1997 reviewed models to predict the indentation modulus of homogeneous thin ﬁlms on a homogeneous substrate as a function of the penetration. All of them consider the substrate and ﬁlm properties and suppose the ﬁlms are homogeneous: 1 1 hc 1 hc þ f 1f ¼ sf Er Er Er e e

ðA8:17Þ

where superscripts s and f indicate the substrate and ﬁlm respectively. Er is the measured substrate–ﬁlm composite property. Assuming a given function f (for hc ! 0, f ! 0 and for hc ! 1, f ! 1), allows determination of the unknowns (Erf ) once Ers is characterized and Er measured as a function of contact penetration hc (Mencik et al., 1997). A similar procedure can be applied to determine the hardness of the ﬁlms. In fact, the combined contributions of the coating and the substrate are measured. Notably, at equal indentation depth, the inﬂuence of the substrate on the measured hardness is less than on the indentation modulus. Indeed, the plastic strain ﬁeld is much less extended spatially than the elastic strain ﬁeld (Fig. A8.9). From Fig. A8.9, one further observes that the 10 % rule of thumb (in other words, ﬁlm response is determined with relative penetration depth less than 0.1) has to be used very carefully. Beegan and Laugier (2005) reviewed models to predict the indentation hardness of homogeneous thin ﬁlms on a homogeneous substrate as a function of penetration. As for moduli, all of them consider the substrate and ﬁlm properties and suppose the ﬁlms are homogeneous (Bhattacharya and Nix, 1988; Puchi-Cabrera, 2002): hc H ¼ Hs þ ðHf Hs Þf e

0

ðA8:18Þ

301

302

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.9 Hardness and modulus evolution with relative penetration for the same ﬁlm deposited on two different substrates. More rapid convergence at small depth is observed for hardness. The ﬁlm is a hybrid TEOS–PMMA ﬁlm deposited onto glass or PMMA substrates (Mammeri, 2003).

where subscripts s and f indicate the substrate and ﬁlm respectively. H is the measured substrate–ﬁlm composite property. Assuming a given function f0 (for 0 0 hc ! 0, f ! 1 and for hc ! 1, f ! 0), allows determination of the unknowns (Hf) once Hs is characterized and H measured as a function of contact penetration hc. Recently Veprek et al. (2005) emphasized that to measure correctly the hardness of hard coatings on softer substrates, the maximum indentation depth must not exceed 10 % of the thickness of the coating because, above this value, plastic deformation occurs in the softer substrate. Recent FEM simulations of indentation into superhard coatings with hardness 40 GPa revealed that because of the higher strength of these materials, the maximum indentation depth should not exceed about 5 % of the coating thickness in order to avoid plastic deformation in the substrate. Therefore, in order to avoid possible artefacts, Veprek et al. (2005) recommend to use relatively high loads of 30–150 mN, with indentation depths >0.3 mm not exceeding about 5 % of the thickness of the coatings. Their conclusion is that to meet these requirements, coatings 6 mm thick are needed. This requirement is not straightforwardly met (Tavares et al., 2005). Instead, as discussed above the survey of the mechanical response as a function of penetration allows extraction of the ﬁlm contribution.

A8.5 Time-Dependent Response

As mentioned in Section A8.1, when viscoelastic materials are considered, the loading–unloading procedure has to be considered carefully since the mechanical response is time dependent (see also Chapter 6). Time dependence of the indentation

A8.5 Time-Dependent Response

response has been the subject of earlier work (Radok, 1957; Lee and Radok, 1960; Ting, 1966; Johnson, 1985). Because of the growing interest in polymeric and hybrid sol–gel coatings new interest has focused on this subject (Shimizu et al., 1999; Oyen and Cook, 2003; Fischer-Cripps, 2004b; Mammeri et al., 2004; Atanacio et al., 2005; Sakai et al., 2005). Moreover instrumented indentation allows for the monitoring of the overall F(h) curves and allows creep to be studied when a load plateau is programmed. It is important to separate again sharp and blunt indenter geometries. In fact, under a blunt indenter, a general assumption is that plasticity can be neglected. In that case the viscoelastic solution can be obtained from the elastic– viscoelastic correspondence using the hereditary Boltzmann integral. For a sharp indenter, it has to be considered whether plasticity can or cannot be neglected. In the ﬁrst case, the approach is the same as for a blunt contact. If plasticity is to be considered then the solution is complex since elastic, plastic and viscous behaviours are to be considered together. Under indentation, of course, the deformation and stress ﬁelds are complex with a combination of multiaxial compression and shear. We review here phenomenological approaches allowing for F(h) loading curves to be predicted and for creep to be analysed. A8.5.1 Viscoelastic Indentation Curves

The solution for an elastic contact was given by Hertz (1981) and Sneddon (1965) (Chapter 8) for a blunt and sharp indenter respectively. The solutions can be written in the general form (Chapter 8; we suppose the indenter is much more rigid than the specimen) F¼A

E hn 1 n2

ðA8:19aÞ

where A is a geometrical factor and n an exponent equal to 1.5 and 2 for a spherical and a cone indenter respectively. Equation (A8.19a) is rewritten for an incompressible solid (n ¼ 0.5) as F¼A

2G n h ¼ 4AGhn 1n

ðA8:19bÞ

Using the elastic–viscoelastic correspondence with hereditary Boltzmann integral allows for the general solution to be found as (Shimizu et al., 1999; Sakai, 2002; Fisher-Cripps, 2004b; Cheng and Cheng, 2005; Oyen, 2005) ðt dhðt0 Þn 0 FðtÞ ¼ 4A Gðt t0 Þ dt dt0

ðA8:20Þ

0

ðt 1 dFðt0 Þ 0 h ðtÞ ¼ Jðt t0 Þ dt 4A dt0 n

0

ðA8:21Þ

303

304

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.10 Viscoelastic solids (Voigt, Voigt and spring in series, Burger) used to model the indentation creep of viscoelastic solids.

The solution of this integral is completely dependent on the choice of the material relaxation modulus G(t) and compliance J(t). Fischer-Cripps (2004b) proposed empirical solutions for creep analysis during a load plateau (at Fm) based on Maxwell and Voigt elements. The solutions for a conical indenter (Fig. A8.10) are Maxwell element : h2 ðtÞ ¼

p 1 1 Fm cot a þ t 2 Er h

Voigt and spring elements in series : h2 ðtÞ ¼

ðA8:22Þ

p 1 1 Fm cot a þ 1 etEr2 =h 2 Er1 Er2 ðA8:23Þ

1 p 1 1 tEr2 =h2 Burger viscoelastic solid : h ðtÞ ¼ Fm cot a þ t þ 1e 2 Er1 Er2 h1 ðA8:24Þ 2

where a is the semi-angle of the cone, Eri the respective reduced moduli and hi the respective viscosities. These solutions can also be obtained for a spherical contact (Fisher-Cripps, 2004b). The models are applied to a HEMA–TEOS sol–gel ﬁlm under indentation creep (Fig. A8.11). The Maxwell element shows the expected linear dependence of the square of the penetration. This does not ﬁt the experimental data well. In fact, it is necessary to consider a more complex scheme of the solid in order to obtain a representative behaviour. A satisfactory ﬁt is obtained using either a combination in series of Voigt and spring elements or a Burger solid.

A8.5 Time-Dependent Response

Fig. A8.11 Indentation creep curve of HEMA–TEOS thin ﬁlm (Chemin, 2007).

A8.5.2 Viscous Elastic–Plastic Indentation F(h) Curves

Sharp indentation curves of time-dependent materials can be modelled using the Oyen and Cook (2003) viscous elastic–plastic (VEP) model which extends the Sakai (1999) representation of elastic–plastic (EP) materials (Chapter 8). The total displacement of the indenter is taken as the sum of the elastic he, plastic hp and viscous hv displacements: h ¼ he þ hp þ hv

ðA8:25Þ

Because of the geometric similarity of a sharp conical (or Berkovich) indenter, all constitutive equations show the square of the penetration and are assumed to be F ¼ AEr he2

ðA8:26aÞ

F ¼ BHhp2

ðA8:26bÞ

F ¼ Chðdhv =dtÞ2

ðA8:26cÞ

where A (4.4), B (24.6 for a Berkovich indenter) and C are geometrical factors, and Er , H and h the reduced modulus, the true hardness and the quadratic viscosity respectively. Taking the derivation of the displacement equation and combining with constitutive equations yields

h¼

pﬃﬃﬃ dh 1 1 dF 1 1 dF F ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ þ dt 2 AEr F dt 2 BH F dt Ch

ðA8:27Þ

305

306

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.12 Loading–unloading curves of a PMMA–TEOS specimen obtained under periodic load–reload sequence. The model curve is obtained for Er ¼ 7.6 GPa, H ¼ 3.9 GPa, Ch ¼ 1.0 1015 Pa s2. (Reprinted from Mammeri et al., 2004, with permission from Elsevier.)

Once the loading (or unloading) rate is set constant or zero (hold period), Eq (A8.27) can be solved easily yielding h(t). This is illustrated for PMMA–TEOS sol–gel coatings in Figs. A8.12 and A8.13 that show the h(t) solutions under two different loading procedures (Mammeri et al. 2004). One of these shows a holding

Fig. A8.13 Loading–unloading curves of a PMMA–TEOS specimen obtained under loading–hold–rapid unloading sequence. The model curve is obtained for Er ¼ 7.2 GPa, H ¼ 3.9 GPa, Ch ¼ 0.9 1015 Pa s2. (Reprinted from Mammeri et al., 2004, with permission from Elsevier.)

A8.6 Elastic–Plastic Ratios

Fig. A8.14 Normalized loading–unloading curves obtained under two different loads but same loading and unloading times. Specimen is PMMA. Note the superposition of the curves.

period during which time-dependent penetration is observed. Without this holding period, the unloading curve shows unusual curvature: a ‘nose’ can be observed under low unloading rates and results from viscous ﬂow. The presence of such a nose may be detrimental to extract the mechanical properties from the related unloading curves. It is observed that the time-dependent part of the deformation (viscous deformation hv) allows prediction of creep under a holding period (Fig. A8.13). It should be noted that viscous ﬂow happens during the whole indentation procedure. When the unloading time is not negligible as compared to the relaxation time of the material, viscous ﬂow cannot be neglected during unloading. The relaxation time t of the VEP solid may be extracted from the ﬁtting parameter (Oyen and Cook, 2003; Mammeri et al., 2004): t¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ch AE r

ðA8:28Þ

An interesting prediction of the VEP model is that the response is controlled by the total rise time and not by the actual loading rate, which is illustrated for PMMA in Fig. A8.14. The curves were obtained under two different loads but keeping the same loading and unloading time (about 30 s). It is observed using normalized load F/Fmax and normalized depth h/hmax that the curves obtained under two different maximum loads (namely 0.25 and 5 mN) but with the same loading and unloading time superimpose quite well.

A8.6 Elastic–Plastic Ratios

We introduced in Chapter 9 the brittleness index as the hardness–toughness ratio to characterize the competition between the plastic and brittle deformations of glass.

307

308

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Here again, a similar approach can be used instructively in order to balance the elastic and plastic deformations. Hence, we introduce hardness–elastic modulus ratios in order to quantify the competition between elastic and plastic responses. An instrumented indentation machine allows for extraction of hardness H and elastic modulus E; different ratios have been considered, the simplest one being H/E. The higher the ratio the higher the resistance to plastic deformation and hence the higher the elastic compliance of the ﬁlm. Some authors also use ratio H/E that can be related theoretically to residual depth–maximum depth ratio (Chen and Bull, 2006) and experimentally veriﬁed (Fouquet et al., 2004; Chen and Bull, 2006). Taking again the unloading curve function (Section A8.1) we have F ¼ kðh hr Þm

ðA8:29Þ

Contact stiffness at maximum load is S ¼ kmðhm hr Þm1 ¼ mFm =ðhm hr Þ Hence hm hr ¼ mFm =S

ðA8:30Þ

1 hr =hm ¼ mFm =ðShm Þ

ðA8:31Þ

or

Moreover hm ¼ (p/2)hc (Sneddon, 1965), Fm ¼ HAc and S ¼ @[email protected] ¼ 2bE then

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ac =p,

pﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃ hr HAc H Ac H m 24:5 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ p ﬃﬃﬃ ﬃ p pﬃﬃﬃﬃ 1 ¼m ¼m ¼ hm bE phc E b p 2bE Ac =pðp=2Þhc

or 1

hr H hm E

ðA8:32Þ

As regards indentation, Joslin and Oliver (1990) introduced the ratio H/E 2 that can be extracted without requiring any tip area calibration of the nanoindenter

Tab. A8.1

Elastic–plastic ratios and units.

Elastic–plastic ratio

Unit

H/E H/E H/E 2 H3/E 2

– – Pa1 Pa

A8.6 Elastic–Plastic Ratios

since we have a simple relationship between this ratio and force-to-stiffness ratio F/S2: H F 2b ¼ E 2 S2 p

ðA8:33Þ

Another important ratio is H3/E2 that has units of pressure and is representative of the ﬁlm resistance to plastic deformation (Johnson, 1985). This ratio is widely employed in the development of hard coatings for tribological applications (Musil, 2000). Various elastic–plastic ratios and units are summarized in Table A8.1.

309

311

Appendix 9 Strain and Stress A9.1 Stress and Strain

There are two kinds of forces: surface forces or body forces. Surface forces are distributed over the surface of the specimen (for instance contact between objects), while body forces are distributed within the volume (for instance gravitational, electric, magnetic forces). The mean stress sm resulting from a force F acting over a surface or section S is sm ¼

F S

where F is expressed in N, S in m2 and sm in Pa. Positive values are used for tensile stresses and negative for compressive stresses. In general, the force is inclined to the surface and decomposes into its normal N and tangential T components (Fig. A9.1). The related normal and shear stress components are s¼

N S

t¼

T S

Strain refers to the relative displacement resulting from the applied stresses. Consider a solid under normal stress s. It deforms from size lo to l (Fig. A9.2). Strain is deﬁned as the relative deformation and is written e¼

l lo lo

The logarithmic form is also used: e ¼ ln

l lo

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

312

Appendix 9: Strain and Stress

Fig. A9.1 Surface force, normal and shear stresses.

and reduces for small strains to (see also Appendix 12) e ¼ ln

l lo þ l lo l lo l lo ¼ ln ¼ ln 1 þ lo lo lo lo

Side deformation also occurs and lateral strain is ne where n is Poisson’s ratio (n 0.5). n ¼ 0.5 corresponds to volume conservative deformation. As detailed in the main part of this book, Poisson’s ratio depends on glass type and increases as glass structure packing density increases. It is 0.2 for oxide glasses (Cg 0.5) and 0.4 for metallic glasses (Cg > 0.7). Consider now a solid under shear stress t (Fig. A9.2). Distortion appears and shear strain g is written g ¼ tanu u

A9.2 Stress and Strain Tensors

Considering a general loading of a specimen requires the stress and strain tensors to be considered (Fig. A9.3). Stress tensor [s] is 0

s11 ½s ¼ @ s21 s31

s12 s22 s32

1 s13 s23 A s33

Fig. A9.2 Solid under (a) stress and (b) shear stress; elastic deformation and distortion are exaggerated for clarity.

A9.2 Stress and Strain Tensors

Fig. A9.3 Identiﬁcation of components of stress tensor.

Or using stress s and shear stress t notations 0

s11 ½s ¼ @ t21 t31

t12 s22 t32

1 t13 t23 A s33

Let us deﬁne u, v, w as the displacement vector of any point x, y, z of the solid (Fig. A9.4). Normal strains are written e11 ¼

qu ; qx

e22 ¼

qv ; qy

e33 ¼

qw qz

while shear strains are written g12 ¼ 2e12 ¼

qv qu þ ; qx qy

g23 ¼ 2e23 ¼

qw qv þ ; qy qz

Strain tensor [e] is 0

e11 ½e ¼ @ e21 e31

e12 e22 e32

1 e13 e23 A e33

Or using strain e and shear strain g notations 0 1 e11 g12 =2 g13 =2 ½e ¼ @ g21 =2 e22 g23 =2 A e33 g31 =2 g32 =2

Fig. A9.4 Displacement vector.

g31 ¼ 2e31 ¼

qu qw þ qz qx

313

314

Appendix 9: Strain and Stress

Fig. A9.5 Specimen under uniaxial stress.

A9.3 Uniaxial Tensile Test

Under uniaxial tensile testing (Fig. A9.5), the stress tensor is 0

1 s 0 0 @ 0 0 0A 0 0 0

The strain tensor is in the elastic domain 0

s=E @ 0 0

0 ns=E 0

1 0 0 A ns=E

where E is Young’s modulus and n Poisson’s ratio.

A9.4 Simple Shear

Under simple shear stress (Fig. A9.6), the stress tensor is 0

1 0 t 0 @t 0 0A 0 0 0

Fig. A9.6 Specimen under simple shear.

A9.5 Plane Stress

The strain tensor becomes in the elastic domain 0

1 0 t=2G 0 @ t=2G 0 0A 0 0 0

where G is the shear modulus (E ¼ 2G(1 þ n)). For a viscous ﬂow the strain tensor derivative is 1 0 0 t=2h 0 g=2 0 @ g=2 0 0 0 A ¼ @ t=2h 0 0 0 0 0 0

1 0 0A 0

A9.5 Plane Stress

Under plane stress or two-dimensional state of stress, the stress tensor becomes 0

s11 @ t21 0

t12 s22 0

1 0 sx 0 0 A ¼ @ txy 0 0

txy sy 0

1 0 0A 0

Principal stresses are obtained after diagonalization of the stress tensor. Eigenvalues l are obtained solving [s] [x] ¼ l[x] or ([s] l[1])[x] ¼ [0]. l are the roots of the equation detð½s l½1Þ ¼ 0 ¼ ðsx lÞðsy lÞ t2xy ¼ l2 lðsx þ sy Þ þ sx sy t2xy

We get then

l ¼

¼

sx þ sy

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðsx þ sy Þ2 4ðsx sy t2xy Þ

2 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sx þ sy ðsx sy Þ2 þ 4t2xy 2

Principal stress tensor is written 0

s1 @ 0 0

0 s2 0

1 0 0A 0

sx þ sy ¼ 2

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s s 2 x y þt2xy 2

315

316

Appendix 9: Strain and Stress

with s1 ¼

sx þ sy þ 2

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r s x s y 2 2 þtxy 2

s2 ¼

sx þ sy 2

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r s x s y 2 2 þtxy 2

Under equibiaxial stresses, the stress tensor becomes 0

1 s 0 0 @ 0 s 0A 0 0 0

Opposite principal stresses is also referred as pure shear 0

1 s 0 0 @ 0 s 0 A 0 0 0

A9.6 Hydrostatic Pressure and Stress Deviator

The stress tensor can be separated into a deviator (trace is null) and a hydrostatic tensor: 0 1 s11 s12 s13 B C @ s21 s22 s23 A s31 s32 s33 0 1 1 s12 s11 Trð½sÞ s13 B C 3 B C 1 B C ¼B C s23 s21 s22 Trð½sÞ B C 3 @ A 1 s31 s32 s33 Trð½sÞ 3 01 1 Trð½sÞ 0 0 B3 C B C 1 B C þB C 0 Trð½sÞ 0 B C 3 @ A 1 0 0 Trð½sÞ 3 0 1 0 1 s11 s12 s13 s11 s12 s13 1 B C B C ¼ @ s21 s22 s23 A þ Trð½sÞ½I ¼ @ s21 s22 s23 A þ s½I 3 s31 s32 s33 s31 s32 s33

A9.7 Generalized Hooke’s Law

with Trð½sÞ ¼ s11 þ s22 þ s33

The hydrostatic pressure is s ¼ Trð½sÞ=3 ¼ ðs11 þ s22 þ s33 Þ=3

For simple shear stress, the stress tensor reduces to its deviator (hydrostatic tensor is zero).

A9.7 Generalized Hooke’s Law

Under complex loading and in the elastic domain the stress–strain relationship is referred to as the generalized Hooke’s law: si j ¼ Ci jkl ekl

where Cijkl are the stiffness tensor components. This equation can be inverted into ei j ¼ Ji jkl skl

where Jijkl are the compliance tensor components. For cubic materials, there are only three independent components in the Cijkl matrix. Hooke’s law is then written 0s 1 11

0C

11

B s22 C B C12 B C B Bs C BC B 33 C B 12 B C¼B B s12 C B 0 B C B @ s13 A @ 0 s23 0

C12 C11 C12 0 0 0

C12 C12 C11 0 0 0

0 0 0 C44 0 0

0 0 0 0 C44 0

0 10 e11 1 B C 0 C CB e22 C B C 0 CB e33 C C CB C 0 CB 2e12 C CB C 0 [email protected] 2e13 A 2e23 C44

For an isotropic material, the stiffness tensor can be further simpliﬁed and Hooke’s law is written 0

s11 @ s21 s31

s12 s22 s32

1 0 1 0 s13 s23 A ¼ lTrð½eÞ@ 0 1 0 0 s33

1 0 0 e11 0 A þ [email protected] e21 1 e31

e12 e22 e32

1 e13 e23 A e33

with Tr([e]) ¼ e11 þ e22 þ e33, C11 ¼ l þ2m, C12 ¼ l and C44 ¼ m. C44 ¼ ½(C11 C12), A ¼ C44/½(C11 C12) ¼ 1; see also Appendix 12.

Then

317

318

Appendix 9: Strain and Stress

Parameters l and m are Lame coefﬁcients related to Poisson’s ratio n and Young’s modulus E: n¼

l C12 ¼ 2ðl þ mÞ C11 þ C12

E¼

mð3l þ 2mÞ ðC11 C12 ÞðC11 þ 2C12 Þ ¼ lþm C11 þ C12

The strain tensor is written 0

e11 @ e21 e31

e12 e22 e32

1 0 s11 e13 1 þ n @ s21 e23 A ¼ E e33 s31

s12 s22 s32

1 0 1 1 0 0 s13 n s23 A Trð½sÞ @ 0 1 0 A E s33 0 0 1

A9.8 Kelvin and Maxwell Models

Viscoelasticity is obtained combining elastic and viscous components, the Kelvin and Maxwell models being the most simple (Chapter 6). The stress tensor for a Kelvin solid is 0

s11 B @ s21

s12 s22

1 0 1 s13 1 0 0 C B C s23 A ¼ lðTrð½eÞ þ ul Trð½eÞÞ@ 0 1 0 A

s31

s32

s33

20

e11 6B þ [email protected] e21 e31

e12 e22 e32

0 0 1 1 0

e11 e13 dB C e23 A þ um @ e21 dt e33 e31

The strain tensor for a Maxwell solid is 0 e11 dB @ e21 dt e31

e12

e13

1

C e22 e23 A e32 e33 2 0 s11 s12 1 þ n6d B ¼ 4 @ s21 s22 E dt s31 s32

1 0 s13 s11 1 C B s23 A þ @ s21 t1 s33 s31 0 1 1 0 0 Trð½sÞ n B C Trð½sÞ þ @0 1 0A t2 E 0 0 1

s12 s22 s32

13 s13 C7 s23 A5 s33

e12 e22 e32

13 e13 C7 e23 A5 e33

A9.9 Generalized Maxwell Model

where ul, um, t1 and t2 are coefﬁcients that depend on the viscosity of the material.

A9.9 Generalized Maxwell Model

The stress and strain tensors are separated into their deviators (sij, eij) and volume (s[I], e[I] hydrostatic) tensors (Section A9.5). The stress deviator is written ðt si j ðtÞ ¼ 0

dei j Gðt t0 Þdt0 dt00

while hydrostatic tensor is written ðt sðtÞ ¼ 0

de Kðt t0 Þdt0 dt0

with si j ðtÞ ¼ si j ðtÞ þ sdi j

ei j ðtÞ ¼ si j ðtÞ þ edi j

di j ¼ 1 when i ¼ j; di j ¼ 0 when i 6¼ j

GðtÞ ¼ 2Gc1 ðtÞ

KðtÞ ¼ 3Ke ð3Ke 3Kg Þc2 ðtÞ

where G and Kg are the shear and bulk instantaneous elastic constants and Ke the bulk equilibrium elastic modulus. Using a generalized Maxwell model, relaxation functions is written c1 ðtÞ ¼

n X R w1k expðt=T1k Þ k¼1

and c2 ðtÞ ¼

n X R w2k expðt=T2k Þ k¼1

319

320

Appendix 9: Strain and Stress

Average shear relaxation time is given by TR ¼

n hR X R ¼ w1k T1k G k¼1

Hydrostatic relaxation time is often assumed to be ten times the shear relaxation time (Guillemet and Gy, 1996): c2 ðtÞ ¼ c1 ðt=10Þ

When stress is not pure shear or pure hydrostatic pressure, one can always consider any stress state be the sum of both former components. Under uniaxial loading, relaxation times should be multiplied by (Gy et al., 1994; Guillemet and Gy, 1996) 3 1:2 2ð1 þ nÞ

while for equibiaxial stresses (existing in ﬂat glass) the factor is 3ð1 nÞ 1:9 2ð1 þ nÞ

321

Appendix 10 Flow and Plasticity in Glass A10.1 Introduction

Mechanical properties were presented in two separated parts in the main text: i. Chapter 6 presented elevated temperature behaviour characterized by viscous ﬂow. ii. Chapters 7 and 8 presented low-temperature behaviour characterized by brittleness and plasticity. This presentation tends to separate the phenomena. Plasticity and viscous ﬂow might have similarities and Spaepen (1977) proposed a uniﬁed perspective, strain rate and temperature controlling the mechanical response (Spaepen, 1977; Steif et al., 1982). Figure A10.1 shows the shear stress–temperature map for a glass as proposed originally by Frost and Ashby (1982) for crystalline materials. At elevated temperatures and low strain rates, homogeneous ﬂow controls the glass behaviour. Going to lower temperatures and larger strain rates changes homogeneous ﬂow into heterogeneous ﬂow. As regards homogeneous ﬂow a transition from Newtonian to nonNewtonian ﬂow appears once strain rate increases. This is further analysed below. Spaepen (1977) proposed a general strain–stress relationship as v tV Dg exp 2nE sinh g˙ ¼ D f exp a 2kT kT vf

The ﬁrst term on the right-hand side refers either to the homogeneity (Df ¼ 1, deformed volume fraction being 100%) or to the heterogeneity (Df ! 0) of the deformation. The second term follows free-volume theory and takes into account the glass fragility, that is, the viscosity–temperature deviation from the Arrhenius law (Chapter 6). This term is a constant at a given temperature (constant free volume) unless elevated stresses allow for increasing free volume within the material. This in fact may happen in a reduced volume of the deformed specimen, that is, within slip bands (or less viscous bands). This phenomenon can be taken into account by taking Df ! 0 and reduced viscosity in related bands Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

322

Appendix 10: Flow and Plasticity in Glass

Fig. A10.1 Deformation map. (Reprinted from Spaepen, 1977, with permission from Elsevier.)

(heterogeneous ﬂow). The third term reveals that ﬂow is biased along the stress direction. For low stresses it reduces to tV tV sinh 2kT 2kT yielding Newtonian ﬂow (strain rate being proportional to shear stress). The fourth term is the Eyring term (Macedo and Litovitz (1965) hybrid solution; see also Section 6.1.3.4).

A10.2 From Newtonian to Non-Newtonian Flow

Simmons et al. (1988) showed evidences of a transition from Newtonian to nonNewtonian ﬂow when strain rate was increased or temperature lowered. The data plotted in Fig. A10.2 correspond to silico-soda-lime glass. As strain rate increase, apparent viscosity decreases. The empirical relationship proposed for the apparent viscosity by those authors was ho h¼ 1 þ je˙

A10.2 From Newtonian to Non-Newtonian Flow

Fig. A10.2 Normalized viscosity versus normalized strain rate. (Reprinted from Simmons et al., 1988, with permission from Elsevier.)

where ho is the Newtonian shear viscosity and j an adjustable parameter. Hence SLS glass shows a reduced apparent viscosity under elevated strain rate. Similar behaviour was reported more recently for metallic glasses in the supercooled domain (Kawamura et al., 1998; Lu et al., 2003). Moreover, homogeneous non-Newtonian ﬂow was observed to yield superplasticity, which has important industrial applications. At room temperature (below glass transition) non-Newtonian ﬂow has attracted much attention in the past two decades thanks to instrumented indentation tools that allow for strain rate controlled experiments (Appendix 8). Hardness H is related to yield stress Y,1) the dependence of which on strain rate may be written in the form (Han and Tomozawa, 1990; Keulen, 1993) Y ¼ H=3 ¼ bem

where b is a constant. Indentation strain rate e is for a sharp indenter (Han and Tomozawa, 1990; Le Bourhis and Patriarche, 2003) e¼ 1)

h h

We may neglect strain hardening in glass (Appendix 8; YR ¼ Y). Notably deformation of glass is shown to be elastic–perfectly plastic (Bruck et al., 1994; Xing et al., 1998; Inoue, 2000). In crystalline solids, the motion

and mutual interaction of dislocations gives rise to work hardening, that is, increasing ﬂow stress with strain that yields stable plastic ﬂow. Instead, in glasses there are no dislocations and plastic deformation is unstable.

323

324

Appendix 10: Flow and Plasticity in Glass

Fig. A10.3 (a) Strain rate exponent. T means Han and Tomozawa (1990), K means Keulen, 1993). (Reprinted from Grau et al., 1998, with permission from Blackwell Publishing.) (b) Viscosity as a function of strain rate. (Reprinted from Han and Tomozawa, 1990, with permission from Blackwell Publishing.)

When m ¼ 1 ﬂow is Newtonian, while non-Newtonian ﬂow is obtained for m 6¼ 1. A great deviation from Newtonian ﬂow for soda-lime-silica glass has been observed with m in the range 0.05–0.3 reported in Fig. A10.3 (Han and Tomozawa, 1990; Grau et al., 1998), that is, m is determined to be much below 1. This yields reduced viscous

A10.3 From Homogeneous to Heterogeneous Flow

resistance as observed in Fig. A10.3 and suggested by Douglas (1958). Apparent viscosity can be extracted from indentation data dividing stress and strain rate (Chapter 6). Hence viscosity is written h ¼ cem1

where c is a constant. For m ¼ 1, viscosity is independent of strain rate. The reported experimental viscosity values are shown in Fig. A10.3 as a function of strain rate showing instead a dramatic drop of the apparent viscosity as the strain rate increases. The reported changes in apparent viscosity explain in part the large discrepancy reported for glass viscosity at room temperature in the literature as extensively discussed in Chapter 6. Also, Han and Tomozawa (1990) insist on the inﬂuence of glass surface hydration. In fact, water is known to enter a glass surface and change its superﬁcial property (Chapter 5, Appendix 13). Both molecular diffusion and chemical reaction with the glass network happen. Of much importance also is the intrinsic structure of the glass at such a temperature that is not at equilibrium and dependent on the thermal history (Chapter 6).

A10.3 From Homogeneous to Heterogeneous Flow

At temperatures below the glass transition, non-Newtonian ﬂow is generally also associated with heterogeneous ﬂow. Figures A10.4 and A10.5 show such slip bands in indented and uniaxially compressed glass specimens. The nature of these slip bands has been the subject of controversy and still attracts much scientiﬁc interest. Hagan (1979) showed that conﬁned plasticity at an indent tip in silico-soda-lime glass yielded slip lines that could be observed on sectioning the sample through the indent site. It has been suggested that such slip bands could correspond to Na-rich zones allowing for enhanced ﬂow in soda-lime-silica glass. As discussed in Chapter 9, Na ion diffusion is known to be enhanced under elevated stresses as revealed by Nghiem (1998) at crack tip vicinity. Interestingly, in metallic glasses, ﬂow can be induced in large volumes and the resulting slip lines obtained under uniaxial compression look similar to those observed at the sides of crystalline samples deformed under compression (Pampillo and Chen, 1974; Fig. A10.5). More recently, Schuh et al. (2004) using instrumented indentation showed that metallic glass loading response was dependent on strain rate with emphasized discontinuities in the curves observed under low strain rate. In fact, serrated ﬂow has been reported extensively for many metallic glasses.2) Such serrations are observed in

2)

Metallic glasses have attracted much attention since they can be deformed as bulk over a wide range of temperature including temperatures below Tg (Hufnagel, 1996) and have become available as bulk, the most well known being

Vitreloy developed by Johnson’s team at Caltech (Johnson, 2006). This allowed for great progress in the understanding of plasticity and ﬂow of glass.

325

Fig. A10.4 Heterogeneous ﬂow in indented metallic glass. (Reprinted from Ramamurty et al., 2005, with permission from Elsevier.) (b) The shear band morphology underneath the indenter shown in a higher magniﬁcation image obtained from within the deformed region of (a).

Fig. A10.5 Heterogeneous ﬂow in uniaxially compressed metallic glasses. (Reprinted from Pampillo and Chen, 1974, with permission from Elsevier.)

A10.3 From Homogeneous to Heterogeneous Flow

Fig. A10.6 Serration on loading curves of metallic glasses. (Reprinted from Schuh et al., 2004, with permission from Elsevier.)

Fig. A10.6 as small jumps on the curve. The correlation between serration and slip lines is however still debated. All these observations led several authors to consider the dislocation concept in amorphous solids (G’Sell, 2001). Notably, phenomenologically plasticity and heterogeneous non-Newtonian ﬂow are similar and both characterized by localized ﬂow. Spaepen (1977) suggested that increased free volume (lower viscosity) in localized slip bands (Df ! 0) was responsible for this behaviour in glass. Figure A10.7 shows how under elevated stress an atom forces its path even though initially the free volume at its surrounding is too small for a jump (see also Chapter 6). Supposing such a phenomenon can happen implies that the free volume increases under elevated stresses. This is suspected to happen within slip bands where free volume increase leads to viscosity decrease. Experiments could be conducted on metallic glass bulk under compression showing localized bands along the maximum shear stress direction (458, in fact the angle is slightly less than 458 in compression (428)

Fig. A10.7 Free volume creation.

327

328

Appendix 10: Flow and Plasticity in Glass

Fig. A10.8 Transition from homogeneous Newtonian to non-Newtonian heterogeneous and non-Newtonian homogeneous ﬂow. (Reprinted from Schuh et al., 2004, with permission from Elsevier.)

and slightly above in tension (50–578); Fig. A10.5). It is of interest to mention that Pampillo and Chen (1974) showed preferential etching of these slip bands. More recently, slip bands were revealed under lighter contrast in TEM micrographs (Kim et al., 2002; Chang et al., 2006). Based on serration events, Schuh et al. (2004) showed a new transition from heterogeneous non-Newtonian to homogeneous non-Newtonian ﬂow in metallic glasses using indentation tools under different temperatures (Fig. A10.8). Those authors showed such transitions at very elevated loading strain rates for which only light serrations were observed similar to those observed for very small strain rates. Hence, they suggested that the inhomogeneous deformation domain was surrounded by homogeneous deformation domains; one at small strain rates, the other at large strain rates with frontiers depending on temperature. The question whether at high strain rates ﬂow is homogeneous or inhomogeneous with ﬁner slip bands and serration is still under debate (Jiang and Atzmon, 2003).

329

Appendix 11 Finite Element Analysis Finite element analysis (FEA) or ﬁnite element modelling (FEM) decomposes a solid into a mesh made of discrete elements. For each element, the relevant parameters are supposed to be known (physical, chemical, mechanical properties) or locally determined (stress, temperature). Then after each increment of time the overall behaviour of the object can be determined. A step-by-step procedure is used to determine the behaviour of a glass object with time. Notably, when the shape varies the mesh has to be redeﬁned continuously. This technique has become widely used since it allows complex loading and geometries to be considered that make it very attractive for industry and R&D.

A11.1 FEM of the Pressing of a Parison

We consider ﬁrst the pressing of a parison (Chapter 10; press-blow and press-press techniques). The parison is under a stress gradient and a temperature gradient. Also at elevated temperatures the inﬂuence of gravity on glass ﬂow comes into play. Figure A11.1 shows the mesh that is to be deﬁned again after each penetration increment. Pressure ﬁeld shows a gradient with maxima of intensity at the penetrator proximity. Such a pressure ﬁeld in the glass can be calculated under realistic conditions considering the outside pressure from the mould. The numerical tool can be iterated to adjust viscosity regime, mould geometry and hence achieve optimized glass distribution over the articles. This issue is very important in order to reduce container weight.

A11.2 FEM of the Precision Moulding of a Glass Lens

The second process example considers high-precision lens moulding (Fig. A11.2). Here, great precision in the dimensional calculation is required. The glass blank is moulded between two parallel moulds (upper and lower ones) under pressure. Both Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

330

Appendix 11: Finite Element Analysis

Fig. A11.1 FEM modelling of the pressing of a glass parison; mesh and pressure ﬁeld (Laevsky, 2003).

moulds are curved to achieve the ﬁnal lenses shape. The blank ﬂows progressively while stress and stress gradients increase. Stress gradient is more intense at mould folding where strain gradient is expected as well. One should consider friction between the tools and the lens, which FEM manages. Also, FEM allows adjustment of mould geometric characteristics and tool loading carrying out numerical iterations. In order to improve the prediction precision, Jain et al. (2005) recommend determining the viscosity regime under similar compressive conditions and using these inputs so that the FEM will achieve even more precise predictions of the moulding operation.

A11.3 FEM of Fracture

Moving to the mechanical response at fracture, numerical simulations are of great interest since fracture mechanics requires statistics to be considered. Modelling

A11.3 FEM of Fracture

Fig. A11.2 FEM modelling of the compression moulding of a BK7 glass lens at a forming temperature of 671 8C and with a transition temperature of 557 8C. Predicted stresses are shown. (a) Initial glass blank and mould set-up; (b) compression of the glass blank; (c) ﬁnal lens shape. (Reprinted from Jain et al., 2005, with permission from Blackwell Publishing.)

saves expensive and time-consuming experiments. Also, glazing may involve complex assemblies of several sheets of glass having different strengthening treatments and related interfaces. FEM yields helpful and valuable information in this domain. The study of the resistance of a laminated glass presented in Fig. A11.3 is difﬁcult because of interfaces and sliding. Both glass sheets and polyvinylbutyral (PVB) bond have to be taken into account. Moreover, an impact is a dynamic loading and thanks to FEM great insight into glazing crack propagation is obtained (Du Bois et al., 2003). The dynamic impact of a ball (diameter 300 mm, mass 70 kg and initial velocity 10 m s1) on a laminated safety glass (length 1500 mm, thickness 5 mm) is shown in Fig. A11.3, the

331

332

Appendix 11: Finite Element Analysis

Fig. A11.3 Temporal evolution of an impact on a laminated safety glass. (Reprinted from Du Bois et al., 2003, with permission from Elsevier.)

resistance with time being observed. Du Bois et al. 2003 show very a realistic fracture pattern of the laminated glass, and indicate that the fracture pattern is sensitive to mesh reﬁnement and regularity. The authors assume a failure strain at 0.1 % for the glass and no failure for the PVB interlayer. At 10 ms, the ﬁrst elements fail and cracks start to propagate in different directions (bright areas are failed elements where only the PVB interlayer carries the load). Between 30 and 40 ms, some larger glass fragments are formed, which are still joined by the membrane. This can be observed until the end of the impact at 80 ms. These studies are also helpful in understanding

A11.4 FEM of Contact Loading

how fracture propagates. Experimentally, high-speed photography is required (Chapters 7 and 8). Instead, FEM can be carried out at the appropriate time scale.

A11.4 FEM of Contact Loading

As detailed extensively in Chapter 8, glass response to contact loading is complex, in particular once plasticity and fracture are operating. Stress and strain ﬁelds are

Fig. A11.4 FEM mesh used in the threedimensional analysis of the Vickers indentation experiment by Zeng et al. (1995). (a) General view. (b) Detail of the mesh at the contact region (8524 eight-noded elements, 9914 nodes). (c) Loading–unloading curves of

Vickers indentation on soda-lime glass obtained from the FEM as compared to experimental data reported by Cook and Pharr (1990). H ¼ 5.9 GPa, Y ¼ 2.8 GPa, E ¼ 74.3 GPa. (Reprinted from Zeng et al., 1995, with permission from Elsevier.)

333

334

Appendix 11: Finite Element Analysis

complex (see also Appendix 8). Again FEM is shown to be valuable and allows one to get great insight into glass response. As shown in Fig. A11.4, contact mechanics FEM is shown to account well for plasticity. Zeng et al. (1995) used a mesh with higher resolution at the indenter proximity, where plasticity is important and where stress and strain ﬁelds change rapidly. Using elastic and plastic behaviour inputs, they were able to predict quite well the experimental curves obtained for glass by Cook and Pharr (1990). The next step is to take into account fracture and have a predictable model for contact fracture.

335

Appendix 12 X-Ray Diffraction Analysis of Thin-Film Residual Stresses A12.1 Thin-Film Stress and Strain

Let us consider a ﬁlm under simple equibiaxial stresses. The stress tensor is (Appendix 9) 0

1 s 0 0 @ 0 s 0A 0 0 0

and the strain tensor is 0

ek @0 0

0 ek 0

1 0 0 A e?

ejj and e? being the in-plane and out-of-plane strains respectively. Most deposited FCC metallic thin ﬁlms show two particular orientations or textures: either (0 0 1) or (1 1 1). Crystallites show a or preferential direction along the growth direction (surface normal). In such cases, stress–strain relationships are written s ¼ Mhkl ejj

and hhkl ¼ e ? =ejj

Mhkl is deﬁned as the biaxial modulus and hhkl the ratio of out-of-plane to inplane strains depending on crystallographic direction [hkl]. Mhkl and hhkl are listed for the two respective ﬁlms texture in Table A12.1 We deﬁne now anisotropy ratio A of cubic crystals as A¼

2C44 C11 C12

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

336

Appendix 12: X-Ray Diffraction Analysis of Thin-Film Residual Stresses Tab. A12.1 Biaxial modulus Mhkl and the ratio of out-of-plane to in-plane strains hhkl for the two most common textures of thin FCC films

(0 0 1)

(1 1 1)

ðMC11 C12 ÞðC11 þ 2C12 Þ C11

Mhkl hhkl

2

6C44 ðC11 þ 2C12 Þ C11 þ 2C12 þ 4C44

C12 C11

2

C11 þ 2C12 2C44 C11 þ 2C12 þ 4C44

Most metals (Table A12.2) show elastic anisotropy. Note that a thin ﬁlm is polycrystalline, that is, formed of monocrystalline grains, the size and orientation of which depend on deposition conditions. They will exhibit elastic macroscopic anisotropy only when texture is present, that is, when crystallites show a preferential orientation (001 or 111 for instance). Tungsten is an archetype since the crystallites are elastically isotropic. Hence tungsten ﬁlms show microscopic and macroscopic elastic isotropy. For A ¼ 1 the elastic properties are completely deﬁned by two elastic constants E and n and we have M ¼ E=ð1 nÞ

h ¼ 2n=ð1 nÞ

Note that for n ¼ 0.33, we have h ¼ 1, that is, out-of-plane strain is exactly opposite of the in-plane strain.

Tab. A12.2 Biaxial modulus Mhkl and the ratio of out-of-plane to in-plane strains hhkl for various elements

Element

C11 (GPa)

C12 (GPa)

C44 (GPa)

A

M001 (GPa)

h001

M111 (GPa)

h111

Al V Nb Ta Cr Mo W Fe Ni Pd Pt Cu Ag Au

108 228 246 267 350 460 501 238 246 227 346 168 124 186

61 119 134 161 57 176 198 133 147 176 250 121 93 157

28 42 28 82 101 110 151 110 124 71 76 75 46 42

1.2 0.8 0.5 1.6 0.7 0.8 1 2.1 2.5 2.8 1.6 3.2 3 2.9

100 222 234 233 388 501 542 222 217 130 234 114 76 78

1.1 1 1.1 1.2 0.3 0.8 0.8 1.1 1.2 1.5 1.4 1.4 1.5 1.7

114 187 140 317 324 428 542 352 389 287 337 261 173 188

1 1.2 1.5 0.9 0.6 0.9 0.8 0.6 0.6 1 1.2 0.7 0.9 1.2

A12.2 X-Ray Diffraction Method

Fig. A12.1 X-ray diffraction principle and experimental set-up (four-circle goniometer) with, from right to left, the X-ray source, the sample holder and the detector.

A12.2 X-Ray Diffraction Method

X-ray diffraction (XRD) allows for the precise measurement of diffraction peak positions from which we obtain the inter-planar spacing d according to Bragg’s law: 2d sin u ¼ kl

where l is the wavelength of the radiation and u the incident angle. Calling do the strain-free spacing one can derive the corresponding strain using (Fig. A12.1) e ¼ ðd do Þ=do

or in its rational form (this form is much helpful in the XRD frame; see Appendix 9) e ¼ lnðd=do Þ

Once in-plane djj and out-of-plane d? lattice parameters can be measured, one can determine the stress- and strain-free parameter using the biaxial modulus M, and the

337

338

Appendix 12: X-Ray Diffraction Analysis of Thin-Film Residual Stresses

ratio of out-of-plane to in-plane strains h since we have s¼M

dk do do

and do ¼

d ? þ hdk 1þh

Stress-free parameter do informs on the structure of ﬁlms, in particular the presence of impurities or vacancies that yield a different value of the stress-free parameter as compared to that of the bulk reference. Residual stress amplitude s is of utmost importance for ﬁlm mechanical stability as detailed in Chapter 12. A12.3 1. The e–sin2c Method

The X-ray diffraction method can be generalized in the so-called e–sin2c method (Clemens and Bain, 1992; Hauk, 1997; Faurie et al., 2004; Thomas et al., 2004). It encompasses the strain e measurement as a function of angle c deﬁned as the angle between surface normal and diffracting plane normal. A series of lattice spacing measurements is carried out for different orientations with respect to the surface normal (Fig. A12.2). For an equibiaxial stress state we have ec ¼ ek sin2 c þ e ? cos2 c

Fig. A12.2 X-ray diffraction method.

A12.3 The e–sin2c Method 339

Fig. A12.3 Strain e versus sin2c for a polycrystalline tungsten ﬁlm. Circles: as-deposited; diamonds, squares and triangles: increasing loading states (the specimens being tensile stressed). As stress state changes, the slope of the line, that is, stress varies. (Reprinted from Faurie et al., 2004, with permission from Elsevier.)

that shows only c angle dependence (shown in Fig. A12.2, independent of angle f) and which can be rewritten ec ¼

1þh h ssin2 c s M M

This latter equation shows that plotting ec–sin2c one should obtain a straight line the slope of which yields the stresses in the ﬁlm (Faurie et al., 2004; Fig. A12.3). For a particular direction co strain is zero as observed in Fig. A12.3. The zero strain relationship is written sin2 co ¼ h=ð1 þ hÞ

that for an isotropic material like tungsten is sin2 co ¼ 2n=ð1 þ nÞ

allowing for Poisson ratio to be determined.

341

Appendix 13 Diffusion Diffusion plays an important role in glass science and technology since it governs electrical conductivity, corrosion resistance, container permeability, ion exchange used for inducing index gradient or residual stresses, and ﬁning of glass. The diffusion of gas out of a bubble can control its rate of contraction and is then of utmost importance in bubble removal from glass melt. The rate of shrinkage can be determined from diffusion equations. Diffusion controls the atomic movement and hence the melt homogenization.

A13.1 Diffusion Laws

Diffusion is a time-dependent process. Without external force (electrical ﬁeld, temperature gradient, stress) the diffusion ﬂux Jx along the x direction is proportional to concentration gradient along this direction (we suppose concentration is only a function of x and t): Jx ¼ D

qc qx

The constant of proportionality D is called the diffusion coefﬁcient which is expressed in m2 s1, c is the concentration in m3 and hence Jx is expressed in m2 s1. The negative sign in this expression indicates that the direction of diffusion is opposite to the concentration gradient. This means that diffusion happens from a high- to a lowconcentration region. This relationship between concentration gradient and ﬂux is called Fick’s ﬁrst law and is formally identical to the Fourier law that relates thermal ﬂux to temperature gradient. Consider now matter conservation in an inﬁnitesimal volume of size dx (Fig. A13.1). We derive qc qJx q qc dxdt ¼ ðJx ðxÞ Jx ðx þ dxÞÞdt ¼ D dxdt dxdt ¼ qt qx qx qx Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

342

Appendix 13: Diffusion

Fig. A13.1 Elemental volume subjected to diffusion along x-axis.

qc q qc ¼ D qt qx qx

When D is independent of concentration, Fick’s second law is derived: qc q2 c ¼D 2 qt q x

This equation is to be solved to extract concentration as a function of time and position. The solution to extract c(x, t) is complex and we shall review in Section A13.3 two important solutions, namely for constant surface concentration and for instantaneous plan source. Diffusion coefﬁcient D increases with temperature and follows generally an Arrhenius-type law: DH D ¼ Do exp RT

where DH is the energy barrier and Do the pre-exponential factor. Let us consider ﬁrst the case of neutral molecule diffusion (rare gas) where the molecules do not interact with the glass network (Fig. A13.2). The molecules diffuse through the network excess volume. Values of D and DH are given in Table A13.1 and show that higher diffusion of atomic species is obtained for smaller species. The pre-exponential factor is often taken as a constant in a given range of temperatures. Studies over a wide range of temperatures in particular in silica showed that this factor changes with temperature almost linearly as expected from Fig. A13.2 that plots D/T as a function of reciprocal temperature (Doremus, 1994). Diffusion of water, hydrogen and oxygen is complicated by reactions of these gases with the silica lattice. Indeed corrosion of glass is known to result from the reaction of water with silica (with formation of –OH groups; Chapters 5 and 9). Therefore, molecular diffusion of such species is to be measured and considered carefully. A term has to be added to the diffusion equation: qc q2 c qr ¼D 2 qt q x qt

A13.1 Diffusion Laws

Fig. A13.2 Diffusion of neon in fused silica (open points from Frank et al. (1961); dark points from Perkins and Begeal (1971)).

where r is the concentration of reacted or immobilized species. As shown again in Table A13.1, molecular diffusion of a species is observed to depend on its size. When the diffusing species appear also in the glass network, one expects network diffusion to happen in addition to molecular diffusion and viscosity should be closely linked to diffusion when network diffusion is predominant. For instance viscous activation energy for silica is about 580 kJ mol1 and compares favourably with that measured for Si diffusion in silica (about 700 kJ mol1; Table A13.2). Moreover,

Tab. A13.1

Molecular diffusion coefficients in silica.

Species

Diameter (nm)

He Ne

0.2 0.24

Ar

0.32

H2

0.25

O2 H2O

0.32 0.33

D (cm2 s1) at 25 8C 8

2.4 10 5 1012

2.2 1011

D (cm2 s1) at 1000 8C 5

DH (kJ mol1)

5.5 10 2.5 106

1.1 2.1

1.4 109

0.6

7.3 106

2.0

6.6 109 2 107

6.0 4.0

Authors Swets et al. (1961) Frank et al. (1961); Perkins and Begeal (1971) Perkins and Begeal (1971); Nakayama and Shackelford (1990) Lee (1963); Perkins and Begeal (1971) Norton (1961) Shelby (1961); Doremus (1969)

343

344

Appendix 13: Diffusion Tab. A13.2

Diffusion coefficients.

Naþ in silica O2 in silica Si4þ in silica

Do (m2 s1)

DH (kJ mol1)

Range of temperature (8C)

Authors

2.6 104 328 104

90–125 453 579

200–1000 1200–1400 1100–1400

Frischat (1968) Mickelsen (1984) Brebec et al. (1980)

applying Stokes’ law (k ¼ 6phr) and calling r the radius of the ion, one gets the Stokes–Einstein law: D¼

kT 6prh

This allows determination of a ln(D) versus 1/T plot shown as a continuous line in Fig. A13.3. It applies well for O and Si that form the glass network. Below the transition temperature diffusion mechanisms are still debated. The variation of D is shown for alkali metal ions (Naþ) in Fig. A13.4 and shows a good ﬁt with a constant pre-exponential Do. Interestingly when the concentration of ions increases the diffusion rate increases as well. This is attributed to more lattice network discontinuities that facilitate ion transport. Alkali diffusion is important to consider since electrical conduction of most commercial glasses results from sodium ions. While in many applications glass serves as an electrical insulator, ionic transport

Fig. A13.3 Diffusion coefﬁcient D for oxygen in SLS glass as a function of temperature (according to Yinnon and Cooper, (1980)). We observe two regimes with Q ¼ 57.8 and 208 kJ mol1 below and above Tg respectively. Curvature is observed above Tg as suggested by the Stokes–Einstein law. Note the change in behaviour at Tg.

A13.2 Steady-State Diffusion

Fig. A13.4 Diffusion coefﬁcient D for Naþ in silica as a function of temperature. The line is a guide for the eye. (After Frischat, 1968).

and hence conduction plays an important role in the manufacture of glass. Ionic conduction can be approximately estimated from Einstein’s law s¼

Z2 F 2 Dc RT

where Z is the ionic charge, F the Faraday ¼Ne, N: Avogadro number, D the diffusion coefﬁcient, c the concentration, R the gas constant and T the temperature. A still debated issue is the so-called mixed alkali effect that is one of the classical anomalies of glass science and has important technological consequences. Curiously when a glass contains two alkalis, for instance Naþ and Kþ, diffusion is faster for the one in larger concentration. When chemically tempering a glass, this effect can be used to increase diffusion.

A13.2 Steady-State Diffusion

If diffusion ﬂux does not change with time, a steady-state condition exists. One common example is the diffusion of atoms of a gas through a vessel or tube for which the concentrations (or pressures) of diffusing species on both surfaces (external and internal) are held constant. This is represented in Fig. A13.5. Then J¼D

ci ce tH

345

346

Appendix 13: Diffusion

Fig. A13.5 Steady-state diffusion.

This simple relationship is applied to determine the diffusion coefﬁcient (so-called membrane technique) or the lost volume of gas when a tube is used to transport gaseous reactive species. Consider a tube (Fig. A13.6) of length L, radius r and thickness tH (r). The lost volume of gas is V ¼ VmJ 2prL ¼ VmD(ci ce) 2prL/ tH, where Vm is the molar volume (22.4 l mol1 in standard conditions). Also, air diffusion is to be prevented in electrical lamp envelopes and television tubes. In practice the concentration gradient is unknown in the glass so one has to use Henry’s law that relates internal and external pressures and concentrations: c ¼ SP

where S is the solubility. Alternatively permeability K ¼ DS is employed. Combining the above equations yields J ¼ DS

Pi Pe Pi Pe ¼K tH tH

When a vacuum is maintained inside the bulb or tube we have K ¼

tH J Pe

Fig. A13.6 Steady-state diffusion in liners.

A13.3 Non-steady-State Diffusion

Fig. A13.7 Permeability K variation for different gases in silica (according to Shelby, 1996).

One observes that permeability increases when the atom or molecule size decreases (Fig. A13.7). Since permeability K is proportional to D one observe an Arrhenius evolution of K in the studied domains.

A13.3 Non-steady-State Diffusion

Most practical diffusion situations are non-steady-state ones. The diffusion ﬂux and concentration gradient at some point in a solid vary with time, with a net accumulation or depletion of the diffusing species. This is illustrated in Fig. A13.8. Solutions to Fick’s second law can be extracted using boundary conditions. One practically important solution is for a semi-inﬁnite solid in which surface concentration cs is held constant. These conditions are met for chemical tempering when the

Fig. A13.8 Non-steady-state diffusion under constant surface concentration.

347

348

Appendix 13: Diffusion

Fig. A13.9 Erf(z) function.

glass is immersed in a molten salt solution (Chapter 6) as well as for glass surface hydration (Chapter 5; diffusion depth being much less than the thickness, the two opposite surfaces can be considered separately). We shall assume that before diffusion, solute atoms are uniformly distributed with concentration co. The solution is written cðx; tÞ co x ¼ 1 erf pﬃﬃﬃﬃﬃ cs co 2 Dt

pﬃﬃﬃﬃ R z The erf(z) function is plotted in Fig. A13.9 (erfðzÞ ¼ ð2= pÞ 0 expðy2 Þdy). When initial concentration is zero or negligible (co c or cs) the equation reduces to x cðx; tÞ ¼ cs 1 erf pﬃﬃﬃﬃﬃ 2 Dt

Note that for the same Dt value the diffusion proﬁle is the same. Hence, the same diffusion proﬁle can be obtained more rapidly using a higher temperature and maintaining the same Dt product (decreasing time accordingly). Another important solution is for an instantaneous plan source of diffusing species. This is used to determine diffusion coefﬁcient, using radioactive tracers and plotting log c as a function of x2. This also corresponds to the application of thin coatings with the diffusion element at a plane surface of the studied material (in practice it can be sandwiched, concentration being then taken as half the total value).

A13.3 Non-steady-State Diffusion

Fig. A13.10 Non-steady-state diffusion for an instantaneous plan source.

Diffusion solution is written Q x2 cðx; tÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ exp 4Dt pDt

where Q is the amount of substance per unit area at time zero. It is half a Gaussian curve and is shown in Fig. A13.10 (at x = 0, qc=qxjx¼0 ¼ 0).

349

351

Glossary Annealing: Thermal treatment to remove stress from glassware Batch: Raw materials, properly proportioned and mixed for delivery to the furnace Batch charger: Metallic device for mechanically conducting batch to furnace Batch house: Place where batch materials are received, weighed and mixed before being delivered Blister: Bubble or inclusion in glass Bloom: Surface ﬁlm resulting from attack by moisture or other vapour Blow mould: Metal mould for blowing glass to its ﬁnal shape Blower: Person who forms the glass by blowing Blowpipe: Pipe that the glassmaker uses for gathering glass and blowing Borosilicate glass: Glass containing boron oxide Chain marks: Marks left on the bottom of glass articles by the chain belt Check: Surface crack at glass article surface Chemical durability: Chemical resistance of glass to moisture Chip: Abraded and removed glass piece Cold end: Operations on cold glass (polymer coating, cutting, scoring) Continuous tank: Glass furnace allowing continuous delivery Cord: Glass inhomogeneity Cullet: Waste and recycled broken glass used at furnace input Devitriﬁcation: Crystallization in glass Etch: Glass surface chemical attack for marking and decorating Fining: Operation consisting in homogenizing and eliminating bubbles from glass melt Float glass: Flat glass used in house, building and vehicle windows Forming: Shaping hot glass Gather: Hot glass collected at blowpipe extremity Glass blowing: Shaping glass by air pressure Gob: Hot glass delivered by the feeder Hackle marks: Marks on fracture path Hot end: Operations on hot glass (melting, forming, annealing)

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

352

Glossary

Lehr: Long tunnel oven for annealing glass Melting temperature: Temperature used by commercial furnace for melting raw materials. This is well above the melting temperature deﬁning liquid-crystal phase change often called liquidus temperature Mould: metallic mould used to shape glass Mould mark: mark at mould joint Oven glass: Borosilicate glass Pressed glass: Glassware formed by pressure between a mould and plunger Quartz: Most common form of silica Residual stresses: Permanent stresses reinforcing glass Recycling: Using glass (cullet) as raw material to produce new glass Sagging: Glass deformation under gravity Silica glass: Pure SiO2 glass Silico-soda-lime glass: Glass containing silica associated with soda and lime Soda: Sodium oxide Na2O Stria: Cord Tank: Melting unit Temper: Strengthen glass (build in stress) Tempered glass: Strengthened glass Thermal shock resistance: Resistance to temperature variation Weathering: Attack of glass surface by atmosphere

353

References Aben, H. and Guillemet, C. (1993) Photoelasticity of Glass, Springer-Verlag, Berlin. Abrams, M.B., Green, D.J., Glass, S.J. (2003) J. Non-Cryst. Solids, 321, 10. Acloque, P. (1951) Verres Refract, 5, 247. Adams, G. and Gibbs, J.H. (1965) J. Chem. Phys, 43, 139. Adams, L.H. and Williamson, E.D. (1920) J. Franklin Inst, 190, 597. Akeyoshi, K., Kanai, E., Yamamoto, K., Shima, S. (1967) Rep. Res. Lab. Asahi Glass., 17, 23. Alliche, A. and Le Bourhis, E. (2000) Mater. Sci. Eng. A, 278, 255. Angell, C.A. (1995) Science, 267, 1924. Anstis, G.R., Chantikul, P., Lawn, B.R., Marshall, D.B. (1981) J. Am. Ceram. Soc., 64, 533. Arbad, M., Shelestak, L.J., Harris, C.S. (2005) Am. Ceram. Soc. Bull, 84, 34. Argon, A.S. (1979) Acta Metall., 27, 47. Arora, A., Marshall, D.B., Lawn, B.R., Swain, M.V. (1979) J. Non-Cryst. Solids, 31, 415. Ashby, M.F. (2001) Materials Selection in Mechanical Design, ButterworthHeinemann, Oxford, UK. Ashby, M. and Johnson, K. (2003) Mater. Today., 12, 24. Ashby, M.F. and Jones, D.R.H. (1991) Mate´riaux 1 & 2, Dunod, France. Askeland, D.R. (1989) The Science and Engineering of Materials, PWS-Kent Publishing, Boston, MA. Atanacio, A.J., Latella, B.A., Barbe´, C.J., Swain, M.V. (2005) Surf. Coat. Technol., 192, 254. Auerbach, F. (1891) Ann. Phys. Chem., 43, 61.

Avramov, I. (2005) J. Non-Cryst. Solids, 351, 3165. Barry, F., Chaunac, M., Chiale, D., Cordier, A., Criaud, A., De La Rochefoucauld, C., Deschanet, P., De´sert, C., De Zorzi, M., Faivre Delord, C., Grell, P., Holle, R., Lafarge, M., Levet, J., Macocco, B., Marozeau, D., Thibault, P. (1998) Verre., 12, 12. Bartoe, R.D. and McDanel, V. (2003) Industrie Ce´ram. & Verrie`re, 986, pp. 58. Barton, J. and Guillemet, C. (2005) Le verre, science et technologie, EDP Sciences, Les Ulis, France. Bather, J.M. and Gray, R.A.A.C. (1976) J. Chromatog, 122, 159. Beegan, D. and Laugier, M.T. (2005) Surf. Coat. Technol., 199, 32. Bergman, B. (1984) J. Mater. Sci. Lett., 3, 689. Bergonnier, S., Hild, F., Rieunier, J.B., Roux, S. (2005) J. Mater. Sci., 40, 5949. Berkovich, E.S. (1951) Ind. Diamond Rev., 11, 129. Bertin, M., Faroux, J.P., Renault, J. (1984) Electromagne´tisme 4, Dunod, Paris. Bertoldi, M. and Sglavo, V.M. (2004) J. NonCryst. Solids, 344, 51. Bhattacharya, A.K. and Nix, W.D. (1988) Int. J. Solids Struct., 24, 1287. Boccaccini, A.R. (1997) J. Mater. Sci. Proc. Tech., 65, 302. Bouyne, E. and Gaume, O. (2001) Proc. Int. Cong. Glass, 2, 106. Brebec, G., Seguin, R., Sella, C., Bevenot, J., Martin, J.C. (1980) Acta Metall, 28, 327. Briard, R. (2004) Renforcement du verre par un revetement hybride en formulation aqueuse, Thesis, Rennes.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

354

References Brinker, C.J. and Scherrer, G.W. (1990) Sol-Gel Science: The Physics and Chemistry of Sol-Gel Processing, Academic Press, San Diego, CA. Brown, J.T., Kobayashi, H., (1998) Am. Ceram. Soc. Bull., 77, 81. Bruck, H.A., Christman, T., Rosakis, A.J., Johnson, W.L. (1994) Scripta Mater, 30, 429. Buehl, W.M. and Ryszyticoskyj, W.P. (1991) SID91 Digest., 667. Buijs, M. (1994) J. Am. Ceram. Soc, 77, 1676. Cable, M. and Smedley, J.W. (1989) Glass Sci. Technol, 30, 39. Caillot, E., Barlier, P., Moffatt-Fairbanks, D.M., Tennent, D.L. (1997) Verre., 3, 3. Carre´, H. (1996) Etude du comportement a` la rupture d’un mate´riau fragile pre´contraint: le verre trempe´, Thesis, Paris. Ce´larie´, F., Prades, S., Bonamy, D., Ferrero, L., Bouchaud, E., Guillot, C., Marlie`re, C. (2003) Phys. Rev. Lett., 90, 0755504. Chandrasekar, S. and Chaudhri, M.M. (1993) Phil. Mag. A, 67, 1187. Chang, H.J., Kim, D.H., Kim, T.M., Kim, T.J., Chattopadhyay, K. (2006) Scripta Mater, 55, 509. Charles, R.J., Hillig, W.B. (1962) The Kinetics of Glass Failure by Stress Corrosion, Union Scientiﬁque Continentale du Verre, Belgium. Chartier, P. (1997) Verre, 3, 5. Chaudhri, M.M. (1998) Acta Mater, 46, 3047. Chaudhri, M.M. (2004) in FRN Nabarro Collection, chapter 70. Chaudhri, M.M. and Kurkjian, C.R. (1986) J. Am. Ceram. Soc., 69, 404. Chaudhri, M.M. and Liangyi, C. (1986) Nature, 320, 48. Chaudhri, M.M. and Phillips, M.A. (1990) Phil. Mag. A, 62, 1. Chemin, N. (2007) Relation entre la structure et les proprie´te´s me´caniques de ﬁlms minces hybrides sol-gel, Thesis, Paris VI. Chen, J. and Bull, S.J. (2006) J. Mater. Res., 21, 2617. Cheng, Y.T. and Cheng, C.M. (2005) J. Mater. Res., 20, 1046. Clemens, B.M. and Bain, J.A. (1992) Mater. Res. Soc. Bull, 17, 46. Coes, L. (1971) Abrasives, Springer Verlag, New York.

Cohen, M.H. and Turnbull, D. (1959) J. Chem. Phys, 31, 1164. Cook, R.F. (2006) J. Mater. Sci., 41, 841. Cook, R.F. and Pharr, G.M. (1990) J. Am. Ceram. Soc., 73, 787. Creuzet, F., Guilloteau, E., Arribart, H. (1993) Fundamentals of Glass Science and Technology, Proc. Second Conf. ESG, 163. Dally, J.W. and Riley, W.F. (1965) Experimental Stress Analysis, McGraw-Hill, New York. DeBast, J. and Gilard, P. (1963) Phys. Chem. Glasses, 4, 117. Dejean-Arrecgros, J. (1978) Petit guide panoramique des roches, Delachaux & Niestle´, Paris. De´riano, S. (2002) Conception chimique de verres silicate´s a` hautes performances me´caniques, Thesis, Rennes. De´riano, S., Jarry, A., Rouxel, T., Sangleboeuf, J.-C., Hampshire, S. (2004) J. Non-Cryst. Solids, 344, 44. Dietzel, A. (1942) Z. Electrochem, 48, 3. Doremus, R.H. (1969) Reactivity of Solids eds J.W.Mitchell, R.C. Devries, R.W. Roberts, P. Cannon, Wiley, New York. pp. 667. Doremus, R.H. (1994) Glass Science, 2nd edn, John Wiley, New York. Doremus, R.H. (2003) Am. Ceram. Soc. Bull, 82, 1. Douglas, R.W. (1958) J. Soc. Glass Technol, 42, 145T. Du Bois, P.A., Kolling, S., Fassnacht, W. (2003) Comput. Mater. Sci, 28, 675. Dubois Petroff, M.P. (2001) Recettes d’Architecture-la cuisine, Massin, Paris. Dugdale, D.S. (1960) J. Mech. Phys. Solids, 8, 100. Durville, D. (2005) J. Mater. Sci., 40, 5941. Elmustafa, A.A. and Stone, D.S. (2003) J. Mech. Phys. Solids., 51, 357. Entwistle, K.M., (1993) J. Mater. Sci., 28, 2007. Ernout, A. et al. (eds) (1947) Pline l’Ancien, Histoire naturelle. Faraday, M. (1830) Phil. Trans. R. Soc, 49. Faraday, M. (1857) Phil. Mag, 14, 401. Faurie, D., Renault, P.O., Le Bourhis, E., Villain, P., Goudeau, P., Badawi, F. (2004) Thin Solid Films, 469/470, 201.

References Ferry, J.D. (1970) Viscoelastic Properties of Polymers, John Wiley, New York. Feynmann, R.P., Leighton, R.B., Sands, M. (1979) Physique, Volume 1, Interedition. Field, J.S. and Swain, M.V. (1993) J. Mater. Res., 8, 297. Fischer-Cripps, A.C. (2004a) Nanoindentation, Springer. Fischer-Cripps, A.C. (2004b) Mater. Sci. Eng. A, 385, 74. Flessel, J.M. (2003) Bull. Soc. Fran. Phys., 140, 28. Fokin, V.M., Zanotto, E.D., Yuritzyn, N.S., Schmelzer, J.W.P. (2006) J. Non-Cryst. Solids, 352, 2681. Fouquet, V., Le Bourhis, E., Pichon, L., Drouet, M., Straboni, A. (2004) Scripta Mater, 51, 899. Franc¸ois-Baillet and Marchi, 2006 Franc¸oisBaillet, B. and Marchi, A. (2006) Est Magazine, 3, 6. Frank, F.C., Lawn, B.R. (1967) Proc. R. Soc. A, 229, 291. Frank, R.C., Swets, D.E., Lee, R.W. (1961) J. Chem. Phys, 35, 1451. Freiman, S.W. (1985) Strength of Inorganic Glass (ed C.R.Kurkjian), Plenum, New York, 197. Friedman, G.S., Cushman, K., Doremus, R.H. (1982) J. Mater. Sci., 17, 994. Frischat, G.H. (1968) J. Am. Ceram. Soc, 51, 528. Frischat, G.H. (1987) in Glas-Struktur und Eigenschaften, (ed. Lohmeyer et al.), Werkstoff Glas I. Ehningen: ex-pert, p. 47. Frischat, G.H. (2002) C.R. Chimie, 5, 759. Frischat, G.H., Heide, G., Muller, B., Weeks, R.A. (2001) Phys. Chem. Glasses, 42, 179. Frost, H.J. and Ashby, M.F. (1982) Deformation-Mechanism Maps, Pergamon, New York, (electronic version available at http://thayer.dartmouth.edu/defmech/). Gadaud, P. and Pautrot, S. (2003) J. NonCryst. Solids, 316, 146. Gao, H., Huang, Y., Nix, W.D., Hutchinson, J.W. (1999) J. Mech. Phys. Solids., 47, 1239. Garcia-Valle`s, M., Gimeno-Torrente, D., Martinez-Manent, S., Fernandez-Turiel, J.L. (2003) Am. Miner, 88, 1996. Gardon, R. (1978) J. Am. Ceram. Soc, 61, 143. Gay, D. (1997) Mate´riaux composites, Hermes, France.

Geandier, G., Denis, S., Mocellin, A. (2003) J. Non-Cryst. Solids, 318, 284. Gilman, J.J. (1949) Rep. Prog. Phys, 12, 48. Gilman, J.J., (1973) The Science of Hardness Testing and Its Research Applications, in ed. J.H.Westbrook, H.Conrad, American Society for Metals, Metal Park, OH, chapter 4. Goodier, J.N. (1936) Phil. Mag, 22, 678. Grau, P., Berg, G., Meinhard, H., Mosch, S. (1998) J. Am. Ceram. Soc, 81, 1557. Greaves, G.N. (1985) J. Non-Cryst. Solids, 71, 203. Green, D.J., Tandon, R., Sglavo, V.M. (1999) Science, 283, 1295. Grifﬁth, A. (1920) Phil. Trans. R. Soc., A221, 163. Grifﬁth, A. (1924) Int. Congr. Appl. Mech., 61, 55. G’Sell, C. (2001) Mater. Sci. Eng. A, 309/310, 539. Guillemet, C. (1990) J. Non-Cryst. Solids, 123, 415. Guillemet, C. and Gy, R. (1996) Rev. Metall, 701. Guin, J.P. and Wiederhorn, S.M. (2004) Phys. Rev. Lett., 92, 215502. Guin, J.P., Rouxel, T., Sangleboeuf, J.C., Melscoe¨y, I., Lucas, J. (2002) J. Am. Ceram. Soc, 85, 1545. Gy, R. (1997) Verre, 3, 21. Gy, R. (1999) Proceedings of Glass Processing Days, Tempere, Finland. Gy, R. (2003) J. Non-Cryst. Solids., 316, 1. Gy, R., Duffre`ne, L., Labrot, M. (1994) J. Non-Cryst. Solids, 175, 103. Hagan, J.T. (1979) J. Mater. Sci., 14, 462. Hainsworth, S.V., Chandler, H.W., Page, T.F. (1987) J. Mater. Res., 11, 2283. Han, W.T. and Tomozawa, M. (1990) J. Am. Ceram. Soc., 73, 3626. Hand, R., Ellis, B., Whittle, B., Wang, F. (2003) J. Non-Cryst. Solids., 315, 276. Harvey, S., Huang, H., Venkataraman, S., Gerberich, W.W. (1993) J. Mater. Res., 8, 1291. Hauk, V. (1997) Structural and Residual Stress Analysis by Non Destructive Methods: Evaluation, Application, Assessment, Elsevier, Amsterdam. Heide, K., Kletti, H., Vo¨lksch, G. (2003) Glass Sci. Technol, 76, 118. Heilmaier, M. and Eckert, J. (2005) Adv. Eng. Mater, 7, 833.

355

356

References Heller, A. (1995) Acc. Chem. Res., 28, 503. Hertz, H.H. (1881) J Reine Angew. Math, 92, 156. Translated and reprinted in English in Hertz’s Miscellaneous Papers, Macmillan, London, 1896. Hillig, W.B. (1962) Modern Aspects of the Vitreous State, vol. II (ed J.D.Mackenzie), Butterworths, London, pp. 152. Ho¨hne, G., Hemminger, W., Flammershein, H.J. (1996) DSC: An Introduction to Practitioners, Springer-Verlag, Berlin. Hollomon, J.H. (1945) AIME Trans., 162, 268. Hufnagel, T.C. (ed) (2006) Scripta Mater, 54, pp. 317. Inglis, C. (1913) Trans. Inst. Naval. Archit., 55. Inoue, A. (2000) Acta Mater, 48, 279. Inoue, A. and Takeuchi, A. (2002) Mater. Trans. JIM, 43, 1892. Inoue, A., Kawamura, Y., Shibata, T., Sasamori, K. (1996) Mater. Trans, 37, 1337. Irwin, G.R. (1958) Fracture, Handbuch der Physik, Springer-Verlag, Berlin. Ishikawa, H. and Shinkai, N. (1982) J. Am. Ceram. Soc., 65, C124. Ito, S. and Taniguchi, T. (2004) J. Non-Cryst. Solids, 349, 173. Jain, A., Firestone, G.C., Yi, A.Y. (2005) J. Am. Ceram. Soc, 88, 2409. James, F.A.J.L. (1991) Phys. Educ, 26, 296. Jiang, W.H. and Atzmon, M. (2003) J. Mater. Res, 18, 755. Johnson, K.L. (1985) Contact Mechanics, University Press, Cambridge. Johnson, W.L. (1996) Mater. Sci. Forum, 225/227, 35. Jones, G.O. (1956) Glass, Methuen’s Monographs on Physical Subjects, Methuen, London. Joslin, D.L. and Oliver, W.C. (1990) J. Mater. Res., 5, 123. Kawamura, Y., Nakamura, T., Inoue, A. (1998) Scripta Mater, 39, 301. Kennedy, C.R., Bradt, R.C., Rindone, G.E. (1980) Phys. Chem. Glasses, 21, 99. Keulen, N.M. (1993) J. Am. Ceram. Soc, 76, 904. Kieffer, J. (2002) Am. Ceram. Soc. Bull, 81, 1. Kim, J.J., Choi, Y., Suresh, S., Argon, A.S. (2002) Science, 25, 654. Kittel, C. (1983) Physique de l’e´tat solide, Dunod, France.

Kittl, P. and Diaz, G. (1988) Int. J. Struc. Mech. Mater. Sci., 24, 99. Klement, W., Willens, R.H., Duwez, P. (1960) Nature, 187, 869. Koike, A. and Tomozawa, M. (2006) J. Non-Cryst. Solids, 352, 3787. Kramer, D., Huang, H., Kriese, M., Robach, J., Nelson, J., Wright, A., Bahr, D., Gerberich, W.W. (1999) Acta Mater, 47, 333. Krause, J.T., Testardi, L.R., Thurston, R.N. (1979) Phys. Chem. Glasses., 20, 135. Kurkjian, C.R. (1963) Phys. Chem. Glasses, 4, 128. Kurkjian, C.R. and Prindle, W.R. (1998) J. Am. Ceram. Soc, 81, 795. Kurkjian, C.R., Kammlot, G.W., Chaudhri, M.M. (1995) J. Am. Ceram. Soc., 78, 737. Laevsky, K.Y. (2003) Pressing of glass in bottle and jar manufacturing: numerical analysis and computation, PhD thesis, Eindhoven University of Technology. Landau, L. and Levich, B. (1942) Acta Physiochim., 17, 42. Langmuir, I. (1933) J. Chem. Phys., 1, 756. Largeau, L., Patriarche, G., Le Bourhis, E. (2002) J. Mater. Sci. Lett, 21, 401. Lawn, B. (1993) Fracture of Brittle Solids, Cambridge Solid State Science Series, Cambridge. Lawn, B. (1998) J. Am. Ceram. Soc., 81, 1977. Lawn, B.R. and Evans, A.G. (1977) J. Mater. Sci., 12, 2195. Lawn, B.R. and Marschall, D.B. (1979) J. Am. Ceram. Soc., 62, 347. Le Bourhis, E. (1996) Vitriﬁed bonded abrasives: post-annealing inﬂuence on residual stresses and wheel strength, Saint-Gobain internal report. Le Bourhis, E. (1998a) Endommagement du verre par contact, Saint-Gobain internal report. Le Bourhis, E. (1998b) Verre, 4, 5. Le Bourhis, E. and Le Guiner, F. (1986) Report, Laboratoire de recherche des Muse´es de France, Paris. Le Bourhis, E. and Metayer, D. (2000) J. Non-Cryst. Solids, 272, 34. Le Bourhis, E. and Patriarche, G. (2003) Prog. Cryst. Growth Charac. Mater, 47, 1. Le Bourhis, E. and Rouxel, T. (2003) J. NonCryst. Solids, 316, 153.

References Le Bourhis, E., Gadaud, P., Guin, J.-P., Tournerie, N., Zhang, X.H., Lucas, J., Rouxel, T. (2001a) Scripta Mater, 45, 317. Le Bourhis, E., Largeau, L., Patriarche, G., Rivie`re, J.P. (2001b ) J. Mater. Sci. Lett, 20, 1361. Le Bourhis, E., Patriarche, G., Largeau, L., Rivie`re, J.P. (2004) J. Mater. Res, 9, 131. Le Houe´rou, V., Sangleboeuf, J.C., De´riano, S., Rouxel, T., Duisit, G. (2003) J. NonCryst. Solids, 316, 54. Lee, E.H. and Radok, J.R.M. (1960) Trans. ASME Ser. E, J. Appl. Mech., 27, 438. Lee, E.H., Rogers, T.G., Woo, T.C. (1965) J. Am. Ceram. Soc, 48, 480. Lee, R.W. (1963) J. Chem. Phys, 38, 448. Lehmann, J.C. (2005) Bull. Soc. Fran. Phys., 150, 4. English version: Europhysicsnews 2006, 37, 23. Levelut, C., Faivre, A., Le Parc, R., Champagnon, B., Hazemann, J.-L., David, L., Rochas, C., Simon, J.P. (2002) J. Non-Cryst. Solids, 307/310, 426. Lilleodden, E.T., Bonin W, W., Nelson, J., Wyrobek, J.T., Gerberich, W.W.(1995) J. Mater. Res.,10,2162. Lim, Y.Y. and Chaudhri, M.M. (2004) Phil. Mag., 84, 2877. Lim, Y.Y. and Chaudhri, M.M. (2006) Mech. Mater., 38, 1213. Livshits, V.Y., Tennison, D.G., Gukasyan, S.B. (1982) Sov. J. Glass Phys. Chem., 8, 463. Lornage, T. (2004) Optimisation des bouteilles par mode´lisation, Lecture, Re´union annuelle GDR Verre. Loubet, J.L., Georges, J.M., Meille, J. (1986) Microindentation Techniques in Materials Science and Engineering (eds P.J.Blau and B.R.Lawn), ASTM International, Philadelphia, PA, pp. 72. Lu, J., Ravichandran, G., Johnson, W.L. (2003) Acta Mater, 51, 3429. Lucas, J. (1999) Curr. Opin. Solid State Mater Sci. 4, 181. McCurty, C. (2000) Proceedings of Coating on Glass Workshop, Livermore, CA, p. 5. Macedo, P.B. and Litovitz, T.A. (1965) J. Chem. Phys, 42, 245. Mackenzie, J.D. (1963) J. Am. Ceram. Soc., 46, 461. McKown, C. (2000) Proceedings of Coating on Glass Workshop, Livermore, CA, p. 8.

McMillan, P.W. (1979) Phys. Educ, 14, 441. Macosco, C.W. (1994) Rheology: Principles, Measurements and Applications, VCH, New York. Malkin, S. (1989) Grinding Technology, Theory and Applications of Machining with Abrasive, Ellis Horwood, Chichester, UK. Malzbender, J., de With, G., den Toonder, J. (2000) J. Mater. Res., 15, 1209. Mammeri, F. (2003) Relation entre la structure et les proprie´te´s me´caniques de ﬁlms minces hybrides organiquesinorganiques pre´pare´s par voie sol-gel, Thesis, Paris VI. Mammeri, F., Le Bourhis, E., Rozes, L., Sanchez, C., Huignard, A., Lefevre, D. (2004) J. Non-Cryst. Solids, 345/346, 610. Mammeri, F., Le Bourhis, E., Rozes, L., Sanchez, C. (2005) J. Mater. Chem., 15, 3787. Mamor, M., Dufour-Gergam, E., Finkman, L., Tremblay, G., Meyer, F., Bouziane, K. (1995) Appl. Surf. Sci., 91, 342. Markovsky, A. and Soules, T.F. (1984) J. Am. Ceram. Soc, 67, C56. Marot, L., Le Bourhis, E., Straboni, A. (2002) Mater. Lett., 56, 76. Marschall, D.B., Lawn, B.R., Evans, A.G. (1982) J. Am. Ceram. Soc., 65, 561. Marsh, D.M. (1964) Proc. R. Soc, A279, 420. Mattoni, A., Colombo, L., Cleri, F. (2005) Phys. Rev. Lett., 95, 115501. Mencik, J., Munz, D., Quandt, E., Weppelmann, E.R., Swain, M.V. (1997) J. Mater. Res., 12, 2475. Meyerhofer, D. (1978) J. Appl. Phys., 49, 3993. Mickelsen, J.C. (1984) Appl. Phys. Lett, 45, 1187. Mills, J.J. (1974) J. Non-Cryst. Solids, 14, 255. Morris, D.J., Myers, S.B., Cook, R.F. (2004) J. Mater. Sci., 39, 2399. Moseler, D., Heide, G., Frischat, G.H. (2002) Glass Sci. Technol., 75, 174. Moynihan, C.T. (1996) Structural relaxation and the glass transition, Structure, Dynamics and Properties of Silicate Melts (eds J.F. Stebbins, P.F. McMillan, D.B. Dingwell), Mineral Society of America. Mozdierz, N., Le Bourhis, E., Peyrot, A., Rivie`re, J.P. (1993) Ce´ramiques, polyme`res et mate´riaux composites, Encyclope´die CLARTE, 1, 3390.

357

358

References Murphy, D.L. (2005) Am. Ceram. Soc. Bull, 84, 41. Musil, J. (2000) Surf. Coat. Technol., 125, 515. Nakayama, G.S. and Schackelford, J.F. (1990) J. Non-Cryst. Solids, 126, 249. Narayanaswamy, O.S. (1978) J. Am. Ceram. Soc, 61, 146. Neely, J.E. and Mackenzy, J.D. (1968) J. Mater. Sci., 3, 603. Nghieˆm, B. (1998) Thesis, Universite´ Paris-VI. Ngoˆ, H. and Ngoˆ, C. (1988) Physique statistique, Masson, Paris. Nieh, T.G., Schuh, C., Wadsworth, J., Li, Y. (2002) Intermetallics, 10, 1177. Norton, F.J. (1961) Nature, 191, 701. Novikov, V.N. and Sokolov, A.P. (2004) Nature, 431, 961. Oliver, W.C. and Pharr, G.M. (1992) J. Mater. Res., 7, 1564. Orowan, E. (1949) Rep. Prog. Phys., 12, 185. Oyen, M.L. (2005) J. Mater. Res., 20, 2094. Oyen, M.L. and Cook, R.F. (2003) J. Mater. Res., 18, 139. Palucka, T. (2006) Mater. Res. Soc. Bull, 31, 697. Pampillo, C.A. and Chen, H.S. (1974) Mater. Sci. Eng., 13, 181. Pantano, C.G., Bojan, V., Verita, M., GeottiBianchini, F., Hreglich, S. (1993) 2nd Conf. European Soc. Glass Sci. Techn., Venice. Paris, P.C. and Sih, G.C. (1965) ASTM Spec. Tech. Publ., 381, 30. Patriarche, G., Le Bourhis, E., Khayyat, M.M., Chaudhri, M.M. (2004) J. Appl. Phys., 96, 1464. Pavelchek, E.K. and Doremus, D.H. (1974) J. Mater. Sci., 9, 1803. Pe´rez, J.P., Carles, R., Fleckinger, R. (1997) Electromagne´tisme, Masson, Paris. Perkins, W.G. and Begeal, D.R. (1971) J. Chem. Phys, 54, 1683. Perriot, A. (2005) Nanoindentation de couches minces deposes sur substrat de verre de silice, Thesis, Paris VI. Peter, K.W. (1964) Glasstech. Ber., 37, 333. Piellard, M., 2005 Etude de la liaison Platine-Alumine, Thesis, Poitiers. Pilkington, A. (1969) Proc. R. Soc. Lond. A, 314, 1. Priven, A.I. (2004) Glass Technol, 45, 244.

Puchi-Cabrera, E.S. (2002) Surf. Coat. Technol, 160, 177. Pugno, N.M. and Ruoff, R.S. (2006) J. Appl. Phys., 99, 024301. Radok, J.R.M. (1957) Q. Appl. Math, 15, 198. Ramamurty, U., Jana, S., Kawamura, Y., Chattopadhyay, K. (2005) Acta Mater, 53, 705. Rawlings, R.D., Wu, J.P., Boccaccini, A.R. (2006) J. Mater. Sci, 41, 733. Redner, A.S. (1998) Measurement of Residual Strain in Glass Products, Short course lecture notes, Strainoptics Technologies. Rehren, T. (2006) GEO, 334, 118. Rekhson, S.M. (1986) (eds D.R.Uhlmann and N.J.Kreidl), Glass Science and Technology, Academic, Orlando, FL, vol. 3, chap. 1. Reuss, R.H., Hopper, D.G., Park, J.G. (2006) Mater. Res. Soc. Bull., 31, 447. Ridealgh, J.A. (2006) Mater. Res. Soc. Symp. Proc., 890, Y01-10.1. Rizkalla, A.S., Jones, D.W., Miller, R.P. (1996) Brit. Ceram. Trans., 95, 151. Rouxel, T. (2006) C. R. Mecanique, in press. Rouxel, T. and Sangleboeuf, J.C. (2000) J. Non-Cryst. Solids, 271, 224. Rouxel, T., Yoshida, S., Shang, H., Sangleboeuf, J.C. (2006) Mater. Res. Soc. Proc., 904, BB02-03.1. Ryu, S.R. and Tomozawa, M. (2006) J. Non-Cryst. Solids, 352, 3929. Sado, G. and Sado, M.C. (1991) Les plans d’expe´riences, AFNOR Technique, France. Sakaı¨, M. (1999) J. Mater. Res, 14, 3630. Sakaı¨, M. (2002) Phil. Mag. A, 82, 1841. Sakaı¨, M., Sasaki, M., Matsuda, A. (2005) Acta Mater, 53, 4455. Sangwal, K.J. (2000) Opto Adv. Mater., 2, 105. Scherer, G.W. (1982) J. Am. Ceram. Soc, 65, 352. Scherer, G.W. (1996) Relaxation in Glass and Composites, Wiley Interscience, New York. Scholze, H. (1991) Glass: Nature, Structure, and Properties, Springer-Verlag, New York. Schottner, G. (2001) Chem. Mater., 13, 3422. Schuh, C.A., Lund, A.C., Nieh, T.G. (2004) Acta Mater, 52, 5879. Schzalke, K. (1981) Test Technique in Fracture, Pergamon Press. Sehgal, J., Nakao, Y., Takahashi, H., Ito, S. (1995) J. Mater. Sci. Lett., 14, 167.

References Sehgal, J. Nakao, Y. Takahashi, H. Ito, S. Patent EP 07570020A1. Sglavo, V.M. and Green, D.J. (2001) J. Eur. Ceram. Soc., 21, 561. Shang, H. and Rouxel, T. (2005) J. Am. Ceram. Soc., 88, 2625. Shelby, J.E. (1961) J. Am. Ceram. Soc, 54, 125. Shelby, J.E. (1996) Handbook of Gas Diffusion in Solids and Melts, ASM International, Materials Park, OH. Shen, J. and Green, D.J. (2004) J. Non-Cryst. Solids, 344, 79. Sheng, H.W., Luo, W.K., Alamgir, F.M., Bai, J.M., Ma, E. (2006) Nature, 439, 419. Shimizu, S., Yanagimoto, T., Sakai, M. (1999) J. Mater. Res., 14, 4075. Shiue, Y.S., Matthewson, M.J., Kurkjian, C.R., Biswas, D.R. (1996) SPIE, 2611, 117. Sih, G. (1972) Mechanics of Fracture, Wolters Noordhoff. Simmons, J.H., Ochoa, R., Simmons, K.D., Mills, J.J. (1988) J. Non-Cryst. Solids, 105, 313. Smith, J.F. and Zheng, S. (2000) Surf. Eng., 16, 143. Sneddon, I.N. (1965) Int. J. Eng. Sci., 3, 47. Spaepen, F. (1977) Acta Metall., 25, 407. Steif, P.S., Spaepen, F., Hutchinson, J.W. (1982) Acta Metall, 30, 447. Stella, A. and Verita, M. (1993) 2nd Conf. European Soc. Glass Sci. Techn., Venice. Stoney, G.G. (1909) Proc. R. Soc. Lond., A82, 172. Sundar, V.C., Yablon, A.D., Grazul, J.L., Ilan, M., Aizenberg, J. (2003) Nature, 424, 899. Suscavage, M.J. and Pantano, C.G. (1983) Glastech. Ber., 56K, 498. Swain, M.V. (1981) J. Mater. Sci., 16, 151. Swets, D.E., Lee, R.W., Frank, R.C. (1961) J. Chem. Phys, 34, 17. Tabor, D. (1951) The Hardness of Metals, Oxford at Clarendon Press, London. Tabor, D. (1996) Phil. Mag A., 4, 1207. Tammann, G. (1925) The States of Aggregation, Van Nostrand, New York. Tanaka, H. (2005) J. Non-Cryst. Solids, 351, 3371, 3385, 3396. Tandon, R. and Cook, R.F. (1992) J. Am. Ceram. Soc., 75, 2877. Tandon, R. and Cook, R.F. (1993) J. Am. Ceram. Soc., 76, 885.

Tavares, C.J., Vidrago, C., Rebouta, L., Rivie`re, J.P., Le Bourhis, E., Denanot, M.F. (2005) Surf. Coat. Technol, 200, 288. Tawakoli, T. (1993) High Efﬁciency Deep Grinding, VDI-Verlag, Germany. Thomas, O., Labat, S., Bigault, T., Gergaud, P., Bocquet, F. (2004) J. Meta. Nanocryst. Mater, 19, 129. Thonggoom, R. and Funkenbusch, P.D. (2005) J. Mater. Sci., 40, 4279. Thornston, J.A. and Hoffman, D.W. (1989) Thin Solid Films., 171, 5. Tillett, J.P.A. (1956) Proc. Phys. Soc. B, 69, 47. Timoshenko, M. (1951) The´orie des plaques et des coques, Librairie Polytechnique, France. Ting, T.C.T. (1966) J. Appl. Mech, 33, 845. Tomozawa, M. (1998) Phys. Chem. Glasses., 39, 65. Tool, A.Q. (1946) J. Am. Ceram. Soc, 29, 240. Turnbull, D. and Cohen, M.H. (1961) J. Chem. Phys, 34, 120. Tyagi, V. and Varshneya, A.K. (1998) J. NonCryst. Solids, 238, 186. Van Mol, A.M.B., Alcott, G.R., Allendorf, M.D. (2005) Am. Ceram. Soc. Bull., 84, 37. Veprek, S., Veprek-Heijman, M.G.J., Karvankova, P., Prochazka, J. (2005) Thin Solid Films., 476, 1. Wang, T.J. (1997) Glass Technol, 38, 104. Wang, W.H., Dong, C., Shek, C.H. (2004) Mater. Sci. Eng. R, 44, 45. Warren, P.D. (1995) J. Eur. Ceram. Soc., 15, 201. Watanabe, T., Puratsubaki, K., Benino, Y., Saitoh, H., Komatsu, T. (2001) J. Mater. Sci., 36, 2427. Weibull, W.A. (1951) J. Appl. Phys., 18, 293. Weibull, W.A. (1952) Appl. Mech. Rev., 5, 11. Westbrook, J.H. (1960) Phys. Chem. Glasses, 1, 32. Wiederhorn, S.M. (1967) J. Am. Ceram. Soc., 50, 407. Wiederhorn, S.M. and Bolz, L.H. (1970) J. Am. Ceram. Soc., 53, 543. Wiederhorn, S.M. and Hockey, B.J. (1980) J. Non-Cryst. Solids, 38/39, 433. Williams, K.F.E., Johnson, C.E., Greegrass, J., Tilley, B.P., Gelder, D., Johnson, J.A. (1997) J. Non-Cryst. Solids, 211, 164. Williams, M.L., Landel, R.F., Ferry, J.D. (1955) J. Am. Chem. Soc, 77, 3701. Woirgard, J. and Dargenton, J.C. (1997) J. Mater. Res., 12, 2455.

359

360

References Wu, D., Lu, G., Jiang, H., Li, Y. (2004) J. Am. Ceram. Soc., 87, 1799. Wu, D., Zhou, J., Li, Y. (2006) J. Mater. Sci, 41, 5630. Xing, L.Q., Bertrand, C., Dallas, J.P., Cornet, M. (1998) Mater. Sci. Eng. A, 241, 216. Yinnon, H. and Cooper, A.R. (1980) Phys. Chem. Glasses, 21, 204. Yoshida, S., Isono, S., Matsuoka, J., Soga, N. (2001) J. Am. Ceram. Soc., 84, 2141. Yoshida, S., Sangleboeuf, J.C., Rouxel, T. (2005) J. Mater. Res., 20, 3404. Zachariasen, W.H. (1932) J. Am. Chem. Soc, 54, 3841. Zandonella, C. (2005) Courrier Int, 755, 60. Zarzycki, J. (1982) Les verres et l’e´tat vitreux, Masson, Paris. [Glasses and the Vitreous State, Cambridge University Press, Cambridge, 1991.] Zeng, K., Giannakopoulos, A.E., Rowcliffe, D.J. (1995) Acta Metall. Mater, 43, 1945. Zhou, J., Wang, Y., Xia, Y. (2006) J. Mater. Sci., 41, 5778. Zinck, P., Pays, M.F., Rezakhnlou, R., Gerard, J.F. (1999) Phil. Mag. A., 79, 2103. Zou, X. and Toratani, H. (2001) J. Non-Cryst. Solids, 290, 180.

Web Sites http://thayer.dartmouth.edu/~defmech/ http://www.musee.ensmp.fr/gm// lettres.html http://www.saint-gobain.com/fr/html/ groupe/verre_plat.asp http://www.saint-gobain-glass.com/fr/ b1107.htm http://www.saint-gobain-glass.com/saint-just/ http://www.saint-gobain.com/fr/html/ investisseurs/pdf/LeGuide2i.pdf http://www.sharplesstress.com/ http://www.strainoptic.com/ http://www.tamglass.com/ http://www.webelements.com/webelements/

Video ‘C’est pas sorcier se met au verre’, France Te´le´vision (FR3).

361

Index a abrasion –performance 186–188 –principles 186–188 Adams and Williamson 121 ageing 191ff Akeyoshi chart 151 alkali –diffusion 78–81, 130, 131, 195, 196, 341–345 –mixed 345 –modiﬁer 57–60 –rich regions 60 alumino-silicate glass 37, 85, 88, 131, 134 –applications 130, 131, 235ff –composition 27 annealing 83ff, 203ff annealing point 85 applications of glass –abrasive tools 49 –containers 44–46 –ﬁbres for –insulation 48f –reinforcement 48f –glazing 39–44 –optical glass 46 atmosphere 29, 36, 61, 78f, 208, 210, 212 atomic bond see bonds Auerbach’s law 165f

blowing 30, 35, 207, 216f blowpipe 30 blunt contact 162 Botzmann hereditary integral 116 bonds –covalent 6–8 –data 5–10 –energy 6–10, 267–270 –formation 267–270 –ionic 5–8 –metallic 7 –Van der Waals 6f borosilicate glass –applications 44–46 –composition 37 –structure 64 Brewster 229 bridging oxygen 53ff, 135ff, 161ff brittle fracture see fracture brittleness –deﬁnition 180f –index 180f –measurement 180f bubble –detection 225 –diffusion 341–345 –elimination 83–86, 207f, 277f –size 277f buckling 18 Burger solid 111–113, 303f

b

c

batch 204f beam –fracture 155f –ﬂexure 19–22 –photoelasticity 287f –shape 18–23

calorimetry 103f ceramics –advantages/drawbacks 7 –brittle fracture 135ff –contact resistance 161ff –group 7f, 15–17

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

362

Index chalcogenide glass –applications 47f –contact resistance 174–177 –structure 65 Charles and Hillig theory 195 chart –thermal expansion/Young modulus 15–18 –toughness 10–12 –transparency 15–18 –strain at rupture/thermal expansion 15–18 –yield strength 10–12 –Young modulus 10–12 –Young modulus/density 18–23 –Young modulus/transition temperature 136–139 chemical –inertness 13, 39, 44f –reactions 78f –tempering 44, 130f, 138, 148, 151f, 181, 345ff –vapour deposition (CVD) 39ff, 235ff, 257 –process 243f chip 167–169 class of materials 5–10 coating 240–245, 248–151, 300–303, 306, 309 compaction 171f, 174 composites –advantages/drawbacks 7 –group 6 compositions of glasses 25–29 computer simulation see ﬁnite element analysis conductivity 206, 341 cold end coating 218 cone crack 164–167 contact mechanics 161ff, 291ff container –applications 44–50 –coating 203ff –history 34f –process 203ff continuous random network (CRN) 54 corrosion 53ff, 191ff cost 5ff, 235ff covalent bond 6, 8, 59, 65 crack 135ff, 161ff, 191ff –branching 139 –healing 201 –propagation 147, 193, 196

crash 329ff creep 107f, 113f, 118, 303–307 crown 33f crystallisation 53, 66, 70–76 cullet 204, 225 cutting –machine 189 –principles 188–190 CVD see chemical vapour deposition

d delayed –elastic strain 113 –fracture 191ff density 7, 9, 10, 12, 17, 61–66, 77, 184, 185 deposition 212, 218, 220, 237, 239–241, 243f, 252, 254 devitriﬁcation 75f Dietzel’s ﬁeld 59 diffusion –coefﬁcient 341–345 –laws 341–345 –of alkali 80f, 195f, 341–345 –of gas 341–345 –non-steady state 347–349 –steady state 345–347 dilatometry 101–103, 271 dip coating 250 display panels –stability 238f –structure 236f distance of order 7f drawing 218f drilling 188–190 dynamic mechanical analysis 109–111

e early glasses 29–32 elasticity 83ff, 135ff, 311ff elastic modulus 115, 129, 137, 163, 174, 271, 308, 319 elastic–viscoelastic correspondence 116, 303 electromagnetic –absorption 259–261 –dispersion 261–263 –polarization 262, 263 –spectrum 259 –wave 227–230 engineered stress proﬁle 132 etching 139 Evan’s law 194f, 197–199 excess volume 63, 66, 78–80, 100

Index

f

glass

fatigue 191ff ﬁbre 5, 11–13, 21, 39f, 46–49, 51, 161, 184, 188, 190, 203–205, 208, 218–224 ﬁbre process 218ff Fick’s law 80, 131, 341f, 347 ﬁctive temperature 123–127 ﬁlms 240–243, 245, 247, 250–255 ﬁning 83, 90f, 203–205, 207ff, 275ff, 341 ﬁnite element analysis –of contact loading 333ff –of crash 330ff –of the pressing of a parison 329ff –of the pression moulding of a glass lens 329ff ﬁnite element modelling see ﬁnite element analysis ﬂat (ﬂoat) glass 1ff, 30, 33ff, 51, 83ff, 203ff, 226ff, 232ff, 250, 254 ﬂaw 135, 138ff, 175, 183 ﬂaw size distribution 157, 283 ﬂint 39ff ﬂoat 35, 39, 41, 203ff ﬂow 83, 89, 94, 98, 103–106, 108, 110, 113, 121f, 171–174, 183, 185 force-penetration curve 162ff, 183, 291, 293–295, 301–305, 307, 329 former 58f, 64, 68, 78 forming 83, 91–93, 105, 203–205, 207f, 214–220 fracture –of bulk 141 –under contact 161ff fragile glass 83ff fragmentation of glass 148, 151 –chart 152 –mechanisms 151f –norm 151f free volume 96, 321, 327 freezing 90, 100, 120 furnace 208, 211 fusion draw 37, 212, 213

–anomalous 172 –assembly 235f –blowing 30, 32, 35, 216f –former 58f, 64, 68 –industry 1–3, 210, 258 –leaching 80, 237f –manufacturers 50f –modiﬁer 53 –network 53 –normal 171f –properties/application 12–14 –process 203 ff –structure 53, 55, 60f –surface 78, 80f –transition 85, 90, 92f, 97, 99, 100ff, 106, 108, 111, 121, 125, 127 –data 99f –deﬁnition 90, 99 –measurement 86–88, 101, 103 –wool 13, 21, 39, 48f, 51, 81 glass-ceramics see vitroceramics glass ﬁber reinforced composites 10–12 glassy state 1, 8, 25, 55f, 90f, 125 glazing –applications –in building 39–44 –in vehicles 41, 43f –coating 240–245, 248–255 –control 225, 232ff –history 27, 35, 37 –mechanical design 18f, 21 –process 203, 205, 210ff –strength 138, 150, 152 –tempering 130f, 133, gob 29 gob feeder 214f Grifﬁth 141, 145 growth of crystals 71–74

g gas 78, 205–208, 219, 341f, 345f

h Hackle zone 139 hardness 170, 172ff –data 173f –deﬁnition 170 –measurement 170, 323 heat soak test 201 history of glass 25–33 hot end coating 218 hydrated glass 81

363

364

Index

i impact fracture 152, 334 indentation –cracks 164–167, 169, 174ff, 189 –curves 303, 305, 333f –plasticity 171 –representative strain 171–173, 296, 298f –stress 162, 167f, 296–300 –toughness 164, 166, 177–179 industrial tools 1, 203, 258 infrared rays 40, 235, 259 ion exchange 80, 130–134, 341 ionic bond 8, 267f

k Kelvin solid 107f, 318

l lateral crack 179 Lehr 210, 212 lenses moulding 203, 329f lifetime 196–199, 201 light see electromagnetic wave liquid state 8, 99–101 liquidus temperature 53, 57, 59, 67, 73, 75f, 99 loss modulus 109f

molecular diffusion 79, 341ff mould –ﬁnishing 216, 218 –mark 216f –parison 216–218

n nanoindentation 291ff natural glass 25–29 network –former 58f –modiﬁer 57–60 –polymerization 55 Newtonian ﬂow 84, 96f, 321–324 nickel sulphide inclusion 199, 205 non-bridging oxygen 57–59, 171 non-Newtonian ﬂow 84, 321–328 nucleation –agents 76f –of crack 174, 178, 189 –of crystals 67, 75 –heterogeneous 70f –homogeneous 68–70

o obsidian 25–27 optical glass 13, 32–34, 46–48, 51 organic glasses 65 Owens process 35

p m Market 235f, 257 materials –properties 10–12 –selection 12–14 matter state 8 Maxwell solid 107f, 304, 318 mechanical design 18–23 median crack 174–177 melting of glass 33f, 205–207 Mendeleev table 5, 6, 54, 64, 266f metallic –bond 6–10 –glasses 63, 65f, 323, 325–328 metals 46 –advantage/drawbacks 7 –group 6–8 mirror zone 138f mist zone 138 mixed-alkali effect 345 modes of fracture 141 modiﬁer 57f, 60 moisture 191, 193f, 199

packing density 62f, 66, 185 performance indices 15–18 permeability 341, 346f photoelasticity –images 288f –principles 227–230 physical vapour deposition (PVD) 43, 240, 241, 244–247, 250, 252, 254f, 258 –process 244–247 –diode sputtering 245 –magnetron sputtering 247f physisorption 78 plane stress 228, 315 plastic deformation 169f, 323 –compaction 171–174, 185 –shear ﬂow 171f, 174 plastics 48 polishing 33, 36, 210, 213 polymers –advantages/drawbacks 7 –group 5f polyvinylbutyral (PVB) 39, 241, 331 precursors 76, 246, 249–251

Index pressing 213, 215–217 process 1ff, 3ff, 203ff proof testing 199 propagation of crack 147, 167, 177, 185, 189, 193, 196, 331 Pyrex 27, 37 PVD see physical vapour deposition

q quality control 225

r radial –distribution 60–63 –median crack 174–177 radioactive wastes 29 recycling 1, 204f reduced time 116, 118 reference temperature 116, 118 refractive index 33f, 46f, 221, 228, 260f refractory 35, 212f regenerators 34, 206f relaxation 6ff, 291ff, 311ff research and development (R&D) 1–3 residual stresses 44, 6–12, 287ff, 335ff –build in 121f, 127 –measurement 231f, 234, 254, 337f –curvature method 253 –photoelastic method 226 –X-ray method 335–339 –proﬁle 119, 131 ring of atoms 54 rule of mixture 12

s sagging 211, 216, 218 scoring 188–190, 210 scratch 185f selection of materials 12–14 self-cleaning 240f, 249 serration 325, 327f shape factor 18–23 sharp contact 169, 175 shear stress 83, 84, 90, 94, 105, 107, 109, 125, 311–314, 317 silica 54–63 silica-soda-lime glass –applications 39ff –composition 25ff –history 25ff –structure 54–63

size effect 157–159 sizing 219f, 240, 254 softening 85f, 90, 102 sol-gel 240–243, 249–252, 254, 255 –process 249–251 spin coating 250 spontaneous fracture 200 static fatigue 191–193, 196f, 201 statistical –analysis 153–159 –fracture 135, 146, 153 strength –deﬁnition 135 –measurement 287–289 –theoretical 135f storage modulus 109–111 strain 5ff, 83ff, 135ff, 161ff, 191ff, 311ff –at fracture 15–17, 136–141 –point 85 –rate 321–325, 328 –tensor 312f strength 135ff, 161, 166, 168, 180 stress 5ff, 83ff, 135ff, 161ff, 191ff, 311ff –concentration 141f –corrosion 192–195 –deviator 316f –ﬁeld –at crack tip 144f –in a beam under ﬂexure 155f –intensity factor 139f, 147f, 167, 181, 192–194 –under non-uniform stress 145, 146 –under uniform stress 138f –meters 231–234 –edge 231–233 –surface 234 –principal 315f –relaxation 107f, 114, 116, 118, 122f, 125, 131–134 –strain curve 136 –tensor 312f structural relaxation 90, 99f, 123–127, 130, 132 sub-critical crack growth 193, 196 super-cooled liquid 90, 92f, 96, 99f, 123, 125f surface 53ff, 161ff, 191ff, 291ff –energy 39–42, 81, 135f, 140, 193, 250 –data 81, 136–141 –mechanics 161f, 165, 291ff –structure 78

365

366

Index

t

v

tektites 28 tempered glass 119, 121, 132, 152, 166, 182f tempering 83, 119, 120–123, 125, 130f, 148, 151f, 181, 203, 211f tensile –drawing 219–221 –stresses 136, 138f –test 136 theoretical strength 135, 158, 279ff thermal –endurance see thermal shock resistance –expansion 6, 10, 15–17, 89, 97, 101–103, 122f, 127, 129, 131, 271ff –shock resistance 15–18 –chart 17 –deﬁnition 15 –tempering 44, 83, 119–128, 130–134, 138, 148, 151f, 181, 200f, 203, 211f thermorheological simplicity 116 thin ﬁlms –function 240–251 –process 240–251 –residual stress 252–254 toughness 7, 10, 12, 136, 140f, 146–148, 153, 164, 166, 177–181, 183f, 192f –chart 10–12 –data 136–141 –deﬁnition 140 –measurement 146–148 –compact tension 146 –double torsion 147–148, 177–179 –indentation 164–167 –notch beam test 146 transient stresses 128–130, 225, 287f transition –homogeneous to heterogeneous ﬂow 328 –Newtonian to non-Newtonian ﬂow 322f –temperature see glass transition transparency 12ff, 39–41, 44–46, 48 TTT diagram 74

van der Waals bond 6, 65 viscoelasticity 107, 114, 122, 292, 295, 302–304 viscometry 86–89, 275ff –falling sphere viscometer 88 –ﬁber elongation viscometer 88f –rotation viscometer 87 viscosity 83ff, 171–173, 203, 207f, 211, 215, 221, 276, 278, 295, 305, 319, 321–325, 327, 329f –data 83–86 –deﬁnition 83 –measurement 86–89 –Newtonian 84, 92 –non-Newtonian 321–325, 327f viscous ﬂow 85, 89, 91, 105, 108, 111, 113, 121, 129, 173, 183, 307, 321 vitroceramics 76 Vogel-Fulcher-Tamman formula 94

w water –corrosion 81 –diffusion 61, 78–80, 95f, 342 –repellence 240–242 weathering 29 weibull –modulus –data 157f –deﬁnition 155 –determination 283–285 –statistics 153, 157, 198, 283ff wetting 49, 241 –angle 242 working point 85, 90

x X-ray diffraction 60f, 63, 335ff

y yield stress 7, 10, 145 Young modulus 10, 12, 15f, 19, 22, 106, 111f, 122, 129, 131, 135–138, 140, 314, 318 –chart 10, 13 –data 136–141 –deﬁnition 137

z Zachariasen model 54

Glass

Related Titles McGee, T

Glass Manufacturing Engineering 2006 ISBN-13: 978-0-471-50836-6

Affatigato, M.

Advances in Glass and Optical Materials II Ceramic Transactions. Volume 197 August 2006 ISBN-13: 978-0-470-08343-7

Doremus, R. H.

Glass Science Second edition 1994 ISBN-13: 978-0-471-89714-1

Eric Le Bourhis

Glass Mechanics and Technology

The Author Professor Eric Le Bourhis Universite´ de Poitiers Laboratoire. de Me´tallurgie Physique, UMR 6630 CNRS, SPMI-Te´le´port 2-Bd. Marie et Pierre Curie, BP 30179 86962 Futuroscope-Chasseneuil Cedex France

All books published by Wiley-VCH are carefully produced. Nevertheless, authors, editors, and publisher do not warrant the information contained in these books, including this book, to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate. Library of Congress Card No.: applied for British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library. Bibliographic information published by the Deutsche Nationalbibliothek The Deutsche Nationalbibliothek lists this publication in the Deutsche Nationalbibliograﬁe; detailed bibliographic data are available in the Internet at . # 2008 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim All rights reserved (including those of translation into other languages). No part of this book may be reproduced in any form – by photoprinting, microﬁlm, or any other means – nor transmitted or translated into a machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not speciﬁcally marked as such, are not to be considered unprotected by law. Typesetting Thomson Digital, India Printing betz-druck GmbH, Darmstadt Binding Litges & Dopf Buchbinderei GmbH, Heppenheim Cover Design WMX-Design, Bruno Winkler, Heidelberg Printed in the Federal Republic of Germany Printed on acid-free paper ISBN: 978-3-527-31549-9

V

Contents Foreword XIII Preface XV Symbols and Deﬁnitions (units in parentheses) Physical Constants XXI Abbreviations XXIII 1

Introduction

2 2.1 2.2 2.3 2.4 2.5

Glass, A Ceramic Material 5 Four Classes of Materials 5 Materials Properties 10 Selecting Materials 12 Performance Indices 15 Shape Factors in Mechanical Design

3 3.1 3.2 3.3 3.4 3.4.1 3.4.2

Glass Prehistory and History 25 Natural Glasses 25 Early Glasses 29 First Optical Glasses 32 Modern Glasses 34 Soda-Lime-Silica Glasses 34 Borosilicate and Aluminosilicate Glasses

4 4.1 4.2 4.3 4.4 4.5 4.6

Applications of Glass 39 Glazing 39 Containers 44 Optical Glass 46 Glass Fibres for Insulation and Reinforcement Abrasive Tools 49 Glass Manufacturers 50

XVII

1

18

37

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

48

VI

Contents

5 5.1 5.2 5.2.1 5.2.2 5.2.3 5.3 5.4 5.5 5.6 5.6.1 5.6.2 5.6.2.1 5.6.2.2 5.6.3 5.6.4 5.6.5 5.6.6 5.7 5.7.1 5.7.2 5.7.3 5.7.4 5.8 5.8.1 5.8.2 5.8.3 5.8.3.1 5.8.3.2 5.8.3.3 5.8.4

Glass Structure 53 Introduction 53 Silica Glass and Related Glasses 54 Glass Network 54 Glass Network Modiﬁcation 57 Short-Range Order 60 Borate Glass and Related Glasses 64 Organic and Chalcogenide Glasses 65 Metallic Glasses 65 Avoiding Crystallization 66 Nucleation and Growth of Crystallized Phases 66 Nucleation of Crystallized Phases 67 Homogeneous Nucleation 68 Heterogeneous Nucleation 70 Crystal Growth 71 TTT Diagram 74 Devitriﬁcation 75 Factors That Favour Glass Formation 76 Vitroceramic Fabrication 76 Introduction 76 Conventional Method (two stages) 77 Modiﬁed Conventional Method (single stage) 77 Laser-Induced Method 77 Glass Surface 78 Surface Reaction 78 Molecular Diffusion 79 Glass Network Interaction with Water 79 Water Reaction 80 Ion Exchange 80 Glass Corrosion 81 Surface Properties 81

6 6.1 6.1.1 6.1.2 6.1.2.1 6.1.2.2 6.1.2.3 6.1.3 6.1.3.1 6.1.3.2 6.1.3.3 6.1.3.4 6.2

Glass Rheology 83 Viscosity 83 Viscosity and Process 83 Viscosity Measurement 86 Rotation Viscometer 87 Falling Sphere Viscometer 88 Fibre Elongation Viscometer 88 Viscosity Variation with Temperature 90 Introduction 90 Fragility 93 VFT Empirical Formula 94 Microscopic Approach 94 Glass Transition and Its Observation 99

VII

6.2.1 6.2.2 6.2.3 6.3 6.4 6.4.1 6.4.2 6.4.3 6.4.4 6.4.5 6.4.5.1 6.4.5.2 6.4.5.3 6.4.5.4 6.5 6.5.1 6.5.2 6.5.3 6.5.4 6.6 6.7 6.7.1 6.7.2 6.7.3 6.7.4

‘Observing’ the Glass Transition 99 Dilatometry 101 Differential Scanning Calorimetry 103 Viscous Response of Glass 104 Viscoelastic Response of Glass 106 Introduction 106 Maxwell and Kelvin Solids 107 Dynamic Mechanical Analysis 109 Modelling Real Solids 111 Functional Formulation 113 Creep 113 Stress Relaxation 114 Elastic–Viscoelastic Correspondence 116 Superposition Principle (simple thermorheological behaviour) Tempering of Glass 119 Introduction 119 Freezing Theory 120 Stress Relaxation 122 Structural Relaxation 123 Transient Stresses 128 Chemical Tempering of Glass 130 Introduction 130 Ion Exchange and Stress Build-Up 131 Stress Relaxation 132 Engineered Stress Proﬁle Glasses 132

7 7.1 7.2 7.3 7.3.1 7.3.2 7.4 7.5 7.6 7.6.1 7.6.2 7.6.3 7.7 7.7.1 7.7.2 7.7.3 7.7.4 7.8 7.8.1

Mechanical Strength of Glass 135 Theoretical Strength 135 Tensile Resistance of Glass 136 Stress Concentration and Grifﬁth Energy Balance 141 Stress Concentration 141 Energy Balance 143 Linear Elasticity Crack Tip Stress Field 144 SIF under Non-uniform Stress 145 Toughness Measurement 146 Compact Tension 146 Notch Beam Test 146 Double Torsion 147 Inﬂuence of Residual Stress on Strength and Fragmentation Inﬂuence of Residual Thermal Stress on Strength 150 Inﬂuence of Residual Chemical Stress on Strength 150 Inﬂuence of Residual Stress on Fragmentation 151 Impact-Induced Fracture 152 Statistical Weibull Analysis 153 Introduction 153

116

148

VIII

Contents

7.8.2 7.8.2.1 7.8.2.2 7.8.3

Functional Formulation 153 Uniform Tensile Stress 155 Non-uniform Tensile Stress 155 Population of Flaws 157

8 8.1 8.1.1 8.1.2 8.1.2.1 8.1.2.2 8.1.3 8.1.3.1 8.1.3.2 8.1.3.3 8.1.3.4 8.1.3.5 8.1.3.6 8.1.3.7 8.2 8.3 8.4 8.5

Contact Resistance of Glass 161 Sharp and Blunt Contact 161 Introduction 161 Spherical Indentation 162 Elastic Loading 162 Hertz Fracture and Indentation Toughness 164 Sharp Indentation 167 Elastic Loading 167 Elastic–Plastic Loading 169 Hardness 170 Radial–Median Cracking 174 Indentation Toughness 177 Lateral Cracking and Chipping 179 Brittleness Index 180 Sharp Contact Resistance 181 Scratch Resistance 185 Abrasion Resistance 186 Cutting and Drilling of Glass 188

9 9.1 9.1.1 9.1.2 9.2 9.2.1 9.2.2 9.2.3 9.3 9.4 9.5 9.6 9.7

Ageing of Glass 191 Fatigue in Glass 191 Static Fatigue 191 Testing Methods 191 Stress Corrosion 192 Introduction (Domain III) 192 Domains O and I: Reaction Controlled Domain II: Transport Controlled 195 Charles and Hillig Theory 195 Lifetime Under Static Fatigue 196 Applications 199 NiS Phase Transformation 199 Crack Healing 201

10 10.1 10.1.1 10.1.2 10.1.3 10.1.4 10.2

Mechanics of Glass Processes Introduction 203 Batching 204 Melting 205 Fining 207 Forming 208 Float Process 208

203

193

IX

10.3 10.4 10.4.1 10.4.2 10.5 10.5.1 10.5.2

Fusion Draw 212 Container Process 213 Pressing 215 Press-and-Blow, Blow-and-Blow Processes Fibre Process 218 Tensile Drawing 219 Centrifugal Drawing 221

11 11.1 11.2 11.3 11.4 11.4.1 11.4.2

Production Control of Residual Stresses 225 Introduction 225 Residual Stresses in Flat Glass 226 Basic of Photoelasticity in Flat Glass 227 Stress Meters 231 Edge Stress Meters 231 Surface Stress Meters 234

12 12.1 12.2 12.2.1 12.2.2 12.2.3 12.3 12.3.1 12.3.2 12.3.3 12.4 12.5

High-tech Products and R&D 235 Market Trend-Driven R&D 235 Flat Display Panels 236 Active Matrix Liquid Crystal Displays 237 Plasma Display Panels 237 Glass Stability 238 Thin-Film Technology 240 Chemical Vapour Deposition 243 Physical Vapour Deposition 244 Sol–Gel Routes 249 Residual Stresses in Thin Films 252 Applications of Coatings and Summary 254

13

Conclusion

216

257

Appendix 1 Light Absorption, Dispersion and Polarization A1.1 Electromagnetic Spectrum 259 A1.2 Light Absorption 259 A1.3 Light Dispersion 261 A1.4 Light Polarization 262 Appendix 2 Atomic Structure and Bond Formation A2.1 Atomic Structure 265 A2.2 Mendeleev Table 267 A2.3 Bond Formation 267 Appendix 3 Thermal Expansion and Elasticity A3.1 The a–E Trend 271 A3.2 Qualitative Approach 271

271

265

259

X

Contents

A3.3 A3.4

Expansion Modelling 272 Differential Expansion Measurement

273

Appendix 4 Falling Sphere Viscometer and Fining of Glass A4.1 Falling Sphere 275 A4.1.1 Asymptotic Regime 275 A4.1.2 Transient Regime 276 A4.2 Fining of Glass 277 Appendix 5

Theoretical Strength of a Solid

Appendix 6

Weibull Analysis

275

279

283

Appendix 7 Photoelastic Set-Up for Lectures 287 A7.1 Set-Up for Photoelastic Projection 287 A7.2 Example of a Beam under Flexion (Transient Stresses) 287 A7.3 Example of Tempered Specimens (Residual Stresses) 288 Appendix 8 Instrumented Nanoindentation Applied to Thin Films 291 A8.1 Instrumented Nanoindentation 291 A8.2 Indentation Strain Field 295 A8.3 Hardness, Yield Stress and Representative Flow Stress 296 A8.4 Coating–Substrate Composite Response 300 A8.5 Time-Dependent Response 302 A8.5.1 Viscoelastic Indentation Curves 303 A8.5.2 Viscous Elastic–Plastic Indentation F(h) Curves 305 A8.6 Elastic–Plastic Ratios 307 Appendix 9 Strain and Stress 311 A9.1 Stress and Strain 311 A9.2 Stress and Strain Tensors 312 A9.3 Uniaxial Tensile Test 314 A9.4 Simple Shear 314 A9.5 Plane Stress 315 A9.6 Hydrostatic Pressure and Stress Deviator 316 A9.7 Generalized Hooke’s Law 317 A9.8 Kelvin and Maxwell Models 318 A9.9 Generalized Maxwell Model 319 Appendix 10 Flow and Plasticity in Glass 321 A10.1 Introduction 321 A10.2 From Newtonian to Non-Newtonian Flow 322 A10.3 From Homogeneous to Heterogeneous Flow 325

XI

Appendix 11 Finite Element Analysis 329 A11.1 FEM of the Pressing of a Parison 329 A11.2 FEM of the Precision Moulding of a Glass Lens 329 A11.3 FEM of Fracture 330 A11.4 FEM of Contact Loading 333 Appendix 12 X-Ray Diffraction Analysis of Thin-Film Residual Stresses 335 A12.1 Thin-Film Stress and Strain 335 A12.2 X-Ray Diffraction Method 337 A12.3 The e–sin2c Method 338 Appendix 13 Diffusion 341 A13.1 Diffusion Laws 341 A13.2 Steady-State Diffusion 345 A13.3 Non-steady-State Diffusion 347 Glossary

351

References Index

361

353

XIII

Foreword It is a pleasure to introduce this book which approaches glass from the scientiﬁc and technological sides. This is an important contribution to the glass literature since few books address both these aspects together. Glass mechanics has appeared as a preliminary for further development of glass functionality and performance. This issue is complex and requires detailed understanding of glass science and industry. This textbook gives a comprehensive approach to glass mechanics taking constant care to keep as close as possible to the applications. The author shares his own experiences both in the academic and industrial ﬁelds resulting in an illustrative and relevant description of glass research and development. This book will be of great interest as training material for people entering the glass industry as well as future engineers and researchers in the ﬁeld. Aubervilliers, France June 2007

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

Rene´ Gy

XV

Preface The project of writing this book started from lectures given to future engineers in materials science. The prime idea was to present both science and technology that participate in industrial R&D. I chose the glass industry as an example having working experiences on both industrial and academic sides. The science–technology approach and concepts developed and illustrated in the book can be utilized in other contexts and for other materials. Fracture and ageing, photoelasticity, rheology, contact resistance, diffusion and production tools issues are shared by many ﬁelds. For teaching purposes, appendices suggest exercises and experimental approaches. It is hoped to offer an overview of the background science and technology used in industry and R&D. The book focuses on mechanics, which has to be considered throughout the industrial process. Preparing this book, I am indebted to many colleagues from industry and academe for their support, discussions and motivations. I would like to thank R. Gy, H. Arribart, J. Prieur, S. Valladeau, E. Bodiot, O. Gaume, N. Brown, J. Zhang, C. Bleuze, J.M. Poujade, P.H. Guering, M.H. Chopinet, E. Barthel, L. Lesage (Saint Gobain group), A. Alliche (ECP Paris), R. Vacher, C. Levelut, D. Cavaille´, J. Pelous (Montpellier University), M.M. Chaudhri (Cambridge University), C.R. Kurkjian (Rutgers University), T. Rouxel, J.C. Sangleboeuf, V. Keryvin (Rennes University), G. Patriarche, L. Largeau (LPN Marcoussis), P. Gadaud (ENSMA Poitiers), D. Mousserion, P.O. Renault, P. Goudeau, J. Bonneville, C. Jaouen, C. Templier, T. Cabioc’h, F. Tranchant, C. Coupeau (Poitiers University), L. Pranevicius and S. Tamulevicius (Kaunas University). I should like to acknowledge support from Wiley VCH, in particular K. Sora and W. Wu¨st. The author also wishes to thank S. Valladeau for his help in carrying out again fractography and photoelasticity experiments, and R. Gy, E. Barthel and F. Mammeri for critical reading and suggestions on parts of the book. Some students worked with me to develop research and applicative studies, and their contributions have been of utmost importance. I would like to thank M. Bustarret, C Teles, M. Beaurain, N. Tournerie, D. Metayer, F. Mammeri, D. Faurie and N. Chemin who shared investigation interest during their training period. This book is dedicated to my wife, sons and parents. Futuroscope-Chasseneuil September 2007 Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

Eric Le Bourhis

XVII

Symbols and Deﬁnitions (units in parentheses) a Contact radius a Distance a Acceleration ao Atomic diffusion jump ac Atomic diffusion interface path a Mark diagonal A Cation ﬁeld intensity A Elastic anisotropy Ap Projected surface Ac Contact projected surface B Brittleness index B, B Magnetic ﬁeld BON Bridging oxygen number c(x, t) Concentration c Radial crack length cl Lateral crack length cP Speciﬁc heat cR Cooling rate C Brewster constant Cg Atomic packing density D Diffusion coefﬁcient E Young’s modulus (2(1 þ n)G) E, E Electric ﬁeld Ei Indenter Young’s modulus Ep Potential energy Es Specimen Young’s modulus f Friction coefﬁcient F Load, force Fc Critical load for fracture Fm Maximum force g Gravitational acceleration g(T ) Growth rate Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

(m) (m) (m s2) (m) (m) (m) (m2) (m2) (m2) (m1/2) (T) (m3) (m) (m) (J kg1 K1) (K s1) (B) (m2 s1) (Pa) (V m) (Pa) (J) (Pa) (N m1 s) (N) (N) (N) (m s2) (m s1)

XVIII

Symbols and Deﬁnitions

Dg Energy barrier for diffusion jump Dg 0 Energy barrier for diffusion at nucleus interface Dg 00 Energy barrier for diffusion at germ interface G Shear modulus G0 Conservation or storage modulus G00 Loss modulus G(t) Relaxation modulus DG Energy barrier for diffusion jump DG0 Energy barrier for diffusion at nucleus interface DG00 Energy barrier for diffusion at particle interface DGv Molar enthalpy of the transformation from liquid to crystal h Penetration h Total penetration he Elastic penetration hl Depth of lateral crack hm Maximum penetration hp Plastic penetration hv Viscous penetration H Hardness or mean pressure Hv Vickers hardness (0.927p) H(t) Heaviside function (¼ 1 for t > 1; ¼ 0 for t 0) I Second moment Io Incidence angle J Diffusion ﬂux J Shear compliance J(t) Compliance k Thermal conductivity k Wave vector K Stress intensity factor (SIF) Kc Fracture toughness L Length m Fragility m Weibull modulus m, M Mass M Torque n Optical index n Volumic concentration n Surface concentration n(T) Nucleation rate p Polarisation vector p Pressure P Property Ps Probability Q Heat r Position or distance

(J at1) (J at1) (J at1) (Pa) (Pa) (Pa) (Pa) (J mol1) (J mol1) (J mol1) (J mol1) (m) (m) (m) (m) (m) (m) (m) (Pa) (Pa) (m4) (rad) (m2 s1) (Pa1) (Pa1) (W m1 K1) (rad m1) (Pa m1/2) (Pa m1/2) (m)

(kg) (N m) (m3) (m2) (m3 s1) (C m) (Pa)

(J) (m)

XIX

r Radius rc Cation radius ro Interatomic distance rO Oxygen radius R Radius RD(r) Radial distribution S Surface, section S Entropy t Time tH Thickness T Temperature Tf Glass ﬁctive temperature Tg Glass transition temperature TL Liquidus temperature Tm Melting temperature TR Relaxation time (h/G) DT Thermal gradient tan(d) Loss factor U Fractured specimen total energy v Velocity vf Free volume (per atom) vl Limit velocity v Minimal volume for atomic jump V Volume Vm Molar volume w Angular velocity wc Critical energy for a particle to form Y Yield stress or yield pressure YR Representative ﬂow stress z Impacter (indenter) penetration Z Atomic number Z Cation valence a Shear angle al Thermal expansion coefﬁcient of the liquid as Thermal expansion coefﬁcient of the solid b Phase shift b Angle between indenter ﬂank and specimen surface g Shear strain d Loss angle e Strain e1, e2, e3 Principal strains z, zcl, zcs, zsl Surface energies h Viscosity

(m) (m) (m) (m) (m) (m2) (J K1) (s) (m) (K) (K) (K) (K) (K) (s) (K) (J) (m s1) (m3) (m s1) (m3) (m3) (m3 mol1) (rad s1) (J) (Pa) (Pa) (m)

(rad) (K1) (K1) (rad) (rad) (rad)

(J m2) (Pa s)

XX

Symbols and Deﬁnitions

hR Viscosity at reference temperature u Wetting angle u Distortion l Wavelength lm Wavelength at maximum light intensity n Poisson’s ratio nE Atomic transition frequency, Einstein frequency ni Indenter Poisson’s ratio ns Specimen Poisson’s ratio j Reduced time r Density s Stress s1, s2, s3 Principal stresses sc Core stress (s(z ¼ 0)) sm Mean stress sM Maximum stress ss, Surface stress (s(z ¼ tH/2)) t Shear stress y Reciprocal dispersion f Shape factor fi Volume fraction f(T) Shift factor F Heat ﬂow c1(t) Shear relaxation function c2(t) Hydrostatic relaxation function V Atomic volume

(Pa s) (rad) (rad) (m) (m) (Hz)

(s) (m3) (Pa) (Pa) (Pa) (Pa) (Pa) (Pa) (Pa)

(J s1)

(m3)

Shorthand Notation @ @x @ Gradient operator r ¼ @y @ @z @/@t, @/@x Partial derivatives For an x only or r only space variation r ¼ d/dx or d/dr Overbar or overdot ¼ d/dt Time derivative Double overdot ¼ d2/dt2 Second time derivative 0 ¼ d/dV Volume derivative [ ] Concentration

(m1) (s1) (s2) (m3) (mol l1 or m3)

XXI

Physical Constants g Gravitational acceleration: 9.8 m s2 N Avogadro number: 6.022 1023 mol1 h Planck’s constant: 6.626 1034 J s R Perfect gas constant: 8.314 J mol1 K1 k Boltzmann’s constant (¼ R/N): 1.381 1023 J K1 e Electron charge: 1.6 1019 C eo Vacuum permittivity (moeoc2 ¼ 1, 4peo ¼ 1/(9 109)) c velocity of light: 3 108 m s1 me electron mass: 9.11 1031 kg mp proton mass: 1.673 1027 kg mn neutron mass: 1.675 1027 kg Vm Perfect gas standard volume: 22.4 l mol1 International System Length: metre (m) Mass: kilogram (kg) Time: second (s) Electrical current: ampere (A) Temperature: kelvin (K) Amount of substance: mole (mol) Luminous intensity: candela (Cd) Preﬁxes Tera (T), 1012 Giga (G), 109 Mega (M), 106 Kilo (k), 103 Milli (m), 103 Micro (m), 106 Nano (n), 109 Pico (p), 1012 Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

XXII

Physical Constants

Femto (f), 1015 Atto (a), 1018 Units Conversion 1 atm ¼ 1.015 bar ¼ 0.1 MPa 1 A˚ ¼ 0.1 nm 1 eV ¼ 1.6 1019 J 1 Hz ¼ 1 s1 1J¼1Nm 0 K ¼ 273.2 8C 1 l ¼ 103 m3 1 N ¼ 1 kg m s2 1 P ¼ 0.1 Pa s 1 Pa ¼ 1 N m2 1 torr ¼ 1.33 mbar ¼ 133 Pa 1 W ¼ 1 J s1 1C¼1As 1 V ¼ 1 W A1 1 V ¼ 1 V A1 1 cal ¼ 4.186 J 1 F¼ Ne C mol1 1 in ¼ 25.4 mm Useful Conversions and Numbers k ¼ 0.086 meV K1; for 25 8C, kT ¼ 25 meV N mp N mn 1 g mol1 Human hair diameter is 100 mm, living blood cell diameter 8 mm Glass hardness is about 5 GPa ¼ 50 000 atm!

XXIII

Abbreviations 1D 2D 3D AFM ALS AMLCD AZS BCC BMG BO CBED CEC CRN CSC CT CVD DRM DT DMA ESC ESP EXAFS FCC FDP FEM FIB GFRP HEC IR IS ISE ITO

One dimension Two dimensions Three dimensions Atomic force microscopy Aluminosilicate Active matrix liquid crystal display Alumina–zirconia–silica refractory Body centred cubic Bulk metallic glasses Bridging oxygen Convergent beam electron diffraction Cold end coating Continuous random network Composed semiconductor Compact tension Chemical vapour deposition Dynamic resonance method Double torsion Dynamic mechanical analysis Elemental semiconductor Engineered stress proﬁle Extended X-ray absorption ﬁne structure Face centred cubic Flat display panel Finite element modelling Focused ion beam Glass ﬁbre-reinforced polymer Hot end coating Infrared Individual section Indentation size effect Indium tin oxide, or tin-doped indium oxide

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

XXIV

Abbreviations

LCD Low-E MEMS MD MNR NBO NBT PDP PER PMMA PVB PVD RD R&D RT SEM SENB SIF SLS TEM TEOS TTT UV VDW VFT XPS XRD

Liquid crystal display Low emissivity Micro-electro-mechanical system Molecular dynamics Magnetic nuclear resonance Non-bridging oxygen Notch beam test Plasma display panel Paramagnetic electronic resonance Poly(methyl methacrylate) Polyvinylbutyral Physical vapour deposition Radial distribution Research and development Room temperature Scanning electron microscopy Single edge notched beam specimen Stress intensity factor soda-lime-silica Transmission electron microscopy Tetraethoxysilane Time–temperature–transformation Ultraviolet Van der Waals Vogel–Fulcher–Tammann X-ray photoelectron spectroscopy X-ray diffraction

1

1 Introduction Glass, existing for millions of years, has fascinated and attracted much interest both scientiﬁcally and technologically. For long, glass was considered a ‘fourth state of matter’ before the realization of its ‘liquid-like’ structure. Glass appears on cooling down a liquid continuously until its viscosity becomes so high that it freezes to a glassy state. This happens at some range of temperatures that depends on thermal history. This lets glass be a mysterious material, since the way it is prepared may change its properties. Nowadays open questions are still raised and we shall address some of these within the present book. These theoretical considerations did not however prevent the development and use of glass over the centuries. Empirical knowledge and know-how have developed through the ages so that, nowadays, glass is a commonly available material. The application of glass science to the improvement of industrial tools, so called research and development (R&D), occurred only in the past century, with a few exceptions, as for instance regarding porcelain researches focused on developing processes in Sax and Worcester (Dr J. Wall’s group by 1750, refer also to Limoges (France) and Worcester (UK) museums). In their ‘Perspective on the history of glass composition’ Kurkjian and Prindle (1998) noted that the age of glass science started only in 1886 with the disclosure of the work of Schott and Enrst (Chapter 4). Science and technology were then becoming more and more interrelated. Glass has been employed in many forms to fabricate glazing and containers for centuries while it is now entering new applications that are appearing in nanotechnology (ﬁbres and displays). Many qualities make glass attractive since it is transparent, chemically inert, environmentally friendly and keeps very strong. In fact, no other materials being mass-produced have shown such qualities over so many centuries. Nowadays glass offers recycling opportunities and allows for tailoring new and dedicated applications. The glass industry has been developing considerably in efﬁciency in terms of production rate and quality over the past few decades. Studying glass history in terms of raw materials and process offers an interesting perspective and understanding of how the glass industry progressively developed. These progresses were achieved because of further knowledge on materials properties and tools. While great achievements were accomplished empirically, R&D offered new opportunities. It is much accepted nowadays that an industry has to Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

2

1 Introduction

progress continuously to face the strong competition that has been developing since globalization (with the emergence of low-labour-cost countries). The evolution in technology varies much according to the area of application. As far as glass is concerned, many different ﬁelds are to be considered, from mass production (glazing, containers) to nanotechnology processing (optical ﬁbres, coatings). The glass industry encompasses several international industrial groups that have strengthened their own R&D units. New products and tools are developed and patented before being launched in production. Research products become of utmost importance for these groups that face always strong technological competition. As the glass industry covers so many different applications, this supposes important technological investment and know-how. Conventional silica-soda-lime glass industry covers large application ﬁelds comprising glazing (for transportation and buildings; Fig. 1.1) and containers, and this still represents the most important glass productions in terms of volumes. At the same time, added-value functions have been developed to sustain industrial competition. Glass R&D has allowed great progresses in the manufacturing of new functional glasses improving continuously performance and quality. Nowadays R&D is aimed at adding functions to glass objects with an interdisciplinary approach involving chemistry, mechanics and optics. New ﬁelds are being opened in electronics and displays and glass technology is expected to play an important role in nanotechnology. Different routes are being employed by manufacturers to add the designed functions, either modifying the glass substrate or using coatings. The former alternative is more expensive since up-stream operations have to be modiﬁed to adjust the tools to the changes in melt composition (high-temperature ﬂow). The development of new coatings looks more attractive and

Fig. 1.1 Modern building with glass walls (near the author’s university).

Introduction

would be preferred since no up-stream operations need to be changed; however, this ﬁeld is newly opened and many issues are still to be solved. In particular, one has to tailor coating strength otherwise the designed function would not resist against abrasion over time. In fact, the overall development and production of glass involve important and interdisciplinary knowledge and know-how. This book presents an overview of background science and technology used in the glass industry and R&D. It focuses on mechanics that is to be considered throughout the industrial process. It is well known that glass is a brittle material and one understands why it is important to improve the strength of glass objects. Not so well accepted is that to achieve such a result and also to improve other performances (optical, dielectrical), one has to consider mechanics at most steps of the production. A literature survey reveals in fact strong interest in glass mechanics since 15 % of articles addressing glass science focus on its mechanical properties. This is the reason for the focus of this book. the most important technological property of glass is its viscosity. It determines the melting conditions, the temperatures for working and annealing and the upper temperature for use (devitriﬁcation rates). Glass quality is directly dependent on the way it is homogenized and this is also related to the viscous ﬂow in the glass melt (Chapter 6). Also, proper quenching of the glass allows for the production of residual stresses that will strengthen the glass and protect it from subcritical crack growth (Chapters 7 and 9). The dimensional adjustment of display front and back plates at the pixel resolution requires control of the thermal history and knowledge of the structural relaxation of glass substrates (Chapter 10). Contact mechanics controls the density of superﬁcial defects generated while transferring products (including elevated temperatures; Chapter 8). The distribution and importance of the superﬁcial defects affect the strength of the manufactured object (Chapter 7). Among the few examples listed above, one understands that glass mechanics is a very broad ﬁeld while being one of the most important issues for the glassmaker. The book is composed of 13 chapters; Chapters 2 to 4 are introductory while Chapters 5 to 12 propose a progressive route into glass mechanics and technology, with a main text that could be ﬁrst read following the proposed chronology. Notes, appendices and further references (books, scientiﬁc papers, videos and web sites) are proposed throughout the text for deeper insight. Appendices recall basic concepts and also illustrate through exercises and applications parts of the book. Also, examples throughout the text allow one to employ the concepts used to describe glass behaviour while their application to glass technology is extensively discussed. Some parts with more mathematics will help in getting more insight into glass behaviour. For a ﬁrst lecture these can be skipped.

3

5

2 Glass, A Ceramic Material1) 2.1 Four Classes of Materials

A commonly used classiﬁcation of the materials separates these into four categories (Askeland, 1989; Ashby and Jones, 1991; Mozdierz et al., 1993): i. the metals, ii. the ceramics, iii. the polymers, and iv. the composites, the last mentioned being obtained from mixing materials from the three main categories. This is illustrated in Fig. 2.1 where the three main categories of materials are shown at the centre while the composites made of two of these are shown at the periphery. This classiﬁcation is based on the type of bonding and the related properties as discussed in more detail below. This classiﬁcation can be examined in view of the Mendeleev table (Fig. 2.2; see also Appendix 2). Most elements in the left-hand side of the table display a metallic behaviour while the other elements are considered as non-metals. Metals may be pure or alloyed with other metals and also non-metals (steel being an Fe–C alloy). They are conductors of electricity and heat. Ceramics are inorganic materials and result from the combination of either (i) metals and non-metals (ionic ceramics, NaCl, MgO, Al2O3, TiN, ZrO2) or (ii) only non-metals (covalent ceramics, SiO2, Si3N4). Combination with oxygen, nitrogen and carbon yields oxides (SiO2, MgO, Al2O3), nitrides (TiN, Si3N4) and carbides (WC) respectively. Ceramics show a refractory behaviour; they are electrically and thermally resistant. Polymers are formed by organic chains (–CH2–) and show thermal and electrical resistances. Composites are formed by two or more materials pertaining to two different classes of materials. For instance, a polymer matrix can be reinforced by ceramic ﬁbres to form a new material with properties combining those of its constituents. The proposed

1)

In this chapter, and also in this book, we consider mostly inorganic glasses.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

6

2 Glass, A Ceramic Material

Fig. 2.1 Materials classes.

classiﬁcation is mostly based on the type of bonding between the constituents of the related materials. It suggests that the structure at the nanoscale determines the properties of the material. This is true for many properties (elasticity, thermal expansion; see Chapter 7 and Appendices 1 and 3) while defects happen to play a major role in others (diffusion, fracture, plasticity; see Chapters 6 and 7, and Appendices 3 and 10). We generally distinguish four types of bonding listed in Table 2.1. Ionic and covalent bonds show the highest binding energy. Such bonds are formed in covalent and ionic ceramics. The lowest binding energy is obtained for van der Waals (VDW) bonds. Theses bonds are formed between polymer chains in thermoplastics. VDW and covalent bonds are found in thermosets that are stronger than thermoplastics. Therefore, the related properties are expected to differ drastically from one group to another (for instance from polymers to ceramics). The main properties of the four categories of materials are listed in Table 2.2. Subjective criteria are suggested

Fig. 2.2 Metals and non-metals in the Mendeleev table.

2.1 Four Classes of Materials Tab. 2.1

Binding energies for the four bonding types (after Askeland, 1989).

Bond

Binding energy (kJ mol1)

Ionic Covalent Metallic Van der Waals

600–1600 500–1300 100–840 50 MPa m1/2) Elevated melting point (Tm 1000 8C) Good thermal and electrical conductivity Rigid E 200 GPa Elevated yield stress Y > 3 GPa High hardness Elevated melting point (Tm 2000 8C) Corrosion resistance Good thermal and electrical resistance Ductile, complex shape production Corrosion resistance Low density

Low yield stress for pure metals Y 1 MPa ! Alloys Hardness: H 3Y ! Alloys Corrosion ! Coatings Elevated density

Ceramics

Polymers

Composites

Stiffness (E > 50 GPa) Elevated yield stress (Y 200 MPa) Toughness (Kic > 20 MPa m1/2) Fatigue resistance Corrosion resistance Tailored and low density

Low toughness (Kic < 2 MPa m1/2) Low thermal shock resistance (DT 200 8C) Difﬁculty in complex shape production Elevated density Low stiffness (E 2 GPa) Low yield stress (Y 2–1000 MPa) Low transition temperature (Tg 100 8C) ! Creep Low toughness (Kic 1 MPa m1/2) Complex shape production difﬁculty Cost Creep (for polymer matrix)

7

8

2 Glass, A Ceramic Material Tab. 2.3 Matter state as a function order distance (ro is the interatomic distance). Perfect gas means that interactions between molecules can be neglected. Perfect crystal is a concept used to describe crystal structure with a repeated unit cell. In fact, all real crystals have defects.

Ordering distance increases from gas to crystal. In a sense, glass looks closer to a liquid than to a crystal. In fact, glass can be considered as a frozen liquid for which viscosity becomes so high that the atomic motions have slowed to the extent that characteristic relaxation time exceeds the observation period (Chapter 6). Many properties of glass can in fact be related to its liquid-like structure. Freezing happens at glass transition that sets a boundary between the glassy state and the liquid state. The ‘ﬁctive’ path from the crystal state to the glass state will be illustrated in Chapter 5 in order to get insight into the complex glass structure. Both transitions, i.e. glass to crystal and liquid to glass transitions (arrowed in Table 2.3), correspond to real instability of the glassy state. Both phenomena are discussed extensively in Chapters 5 and 6 respectively. Oxide glasses, the most common one being silico-soda-lime glass, are used to produce glazing or containers. As discussed in more detail in Chapter 5, such a glass is formed by an Si–O network that is modiﬁed by Na+ and Ca2+ ions. This means that such oxide glasses are formed by covalent Si–O bonds while modifying ions interact with non-bridging oxygen (NBO) atoms through ionic bonds (Chapter 5). This allows for the strong bonding characteristic of the ceramics group. It is to be noted that modiﬁcation with Ca2+ leads to less viscosity change than with Na+ since Ca2+ may link two NBO atoms. Organic glasses belong to the polymer category since they are formed by polymer chains interacting through VDW (thermoplastics) or VDW and covalent bonds (thermosets). Let us consider the energy–distance curve related to a single bond. Interatomic spacing ro is the equilibrium distance between atoms forming a bond and results from the balance between the repulsion predominant at short distances and attraction predominant at longer distances. The two contributions shown in Fig. 2.3 result in a potential energy curve that shows a minimum value reached for the atoms at

2.1 Four Classes of Materials

Fig. 2.3 Potential energy as a function of distance resulting from repulsion predominant at short distance and attraction predominant at long distance.

equilibrium distance ro. This can be functionalized in the form of two terms corresponding to repulsion and attraction (see also Appendix 2): Ep ¼ Erep þ Eattr ¼

a b rm rn

Since repulsion is predominant at short distance we have necessarily m > n. Attraction is responsible for the bond formation while electron repulsion happens when atoms overlap (the Pauli exclusion principle of quantum mechanics). The distance ro allows for determining atom radius (half of the bond distance between identical atoms). This concept is very important in the modelling of material structure and we shall use it in Chapter 5. The hard-sphere model supposes that atoms pack as hard spheres, allowing for establishing relationships between atom radii and crystal parameter and quantifying packing density of glasses (Chapter 5). The minimum energy of the bond is deﬁned as the binding energy and is the energy required to break the bond since it is the energy required to separate the atoms or ions to an inﬁnite distance (Appendix 5). Consequently, materials having a high binding energy like oxide glasses also have a high strength and a high melting temperature. Fig. 2.4 plots

Fig. 2.4 Applied force as a function of distance for two types of bonds (weak and strong) showing the relationship between bonding strength and elastic modulus. Steep slope (dF/dr) results in high modulus (see also Appendix 5).

9

10

2 Glass, A Ceramic Material

the applied force as a function of distance, the equilibrium being obtained for a resulting force equal to zero. The elastic modulus of a material which is the amount that it will stretch when a force is applied to it, is related to the slope of the force– distance curve at equilibrium (r ¼ ro, Fig. 2.4; Appendix 5). We shall see that, in fact, elastic moduli do not depend only on the interatomic bonding strength but also depend on the short-range ordering (possible formation of ring chain, atomic packing density; Chapter 5). The curves are shown for two materials, one with a strong bond and maximum force superior to that of a weak bond. A steep slope at r ¼ ro that correlates with an elevated binding energy and hence an elevated melting point, signiﬁes that a greater force is necessary to stretch the bond. Therefore, the material has an elevated elastic modulus. In a similar but more complex manner, the thermal expansion coefﬁcient can be related to the energy–distance curve (Appendix 3). When the material is heated, the atoms or ions separate because of the additional energy supplied to the material. When the binding energy is large enough, the additional energy causes only small changes in the separation distance between ions or atoms as compared to what happens for a material showing a lower binding energy. Therefore, materials showing a large binding energy also show a small thermal expansion (Appendix 3).

2.2 Materials Properties

The next step in the classiﬁcation of materials consists in fabricating the properties charts that show the classiﬁcation of the materials according to one or several performances (Askeland, 1989; Ashby and Jones, 1991). In these charts the ﬁrst three groups mentioned at the start of Section 2.1 (ceramics, metals and polymers) show different trends as expected from the different bond strengths. However, the different groups show a large range of response with partial overlapping of the properties between groups of materials. Fig. 2.5 shows three important diagrams from the mechanical point of view, where yield stress Y, Young’s modulus E and fracture toughness Kc are reported. These properties will be deﬁned in more detail in the following chapters. Here, we mention that these properties characterize the plastic, elastic and brittle resistances of a material corresponding to three most important modes of deformation (compaction may become an important deformation mode in a silica-rich glass network; see Chapters 5 and 8). The trends mentioned in Table 2.2 are clearly observed in Fig. 2.5. For instance, the ceramics exhibit elevated yield stress and Young’s modulus while their toughness is relatively low. Therefore, ceramics are expected to deform elastically up to brittle failure. Brittle behaviour gives origin to the sudden fracture of glass once critical stress is reached at a defect present in the glass. This will also be discussed in detail later in the book (Chapter 7). Instead, polymers show low stiffness and yield strength. They will deform dramatically elastically and plastically until fracture. Fabricating a composite consists in mixing materials and thereafter in mixing the properties of each component. According to the scale of the phases, nanocomposites

2.2 Materials Properties

Fig. 2.5 Four classes of materials (according to Ashby and Jones, 1991).

and microcomposites are formed. Sol–gel techniques allow the fabrication of inorganic–organic materials with a mixing at the atomic scale (see also Chapter 12). Observing the high strength achieved by glass ﬁbres, engineers incorporated them into polymers and succeeded in obtaining great reinforcement. This is now well developed and used in several ﬁelds (laminated structures, boats, car front ends and truck cabs). We can observe that indeed the composite domain covers parts of the ranges covered by the materials used for their fabrication. Changing the

11

12

2 Glass, A Ceramic Material

Fig. 2.6 Longitudinal El and traversal Et moduli of a ﬁbrereinforced composite as a function of ﬁbre volume fraction ff (all ﬁbres are supposed to be aligned along one direction, namely longitudinal; 70 and 7 GPa moduli are taken for the ﬁbre and matrix respectively).

concentration of the reinforcing component allows for tailoring the composite strength. The way that properties P are mixed is a complex issue. In the simplest case a rule of mixture may be employed. In its simplest form, it is written as a linear law P ¼ f1P1 þ f2P2, where fi are the volume fractions of the components (0 < fi < 1 and f1 ¼ 1 f2) and Pi the respective properties. It is observed that when f1 approaches 0 or 1 then the property P approaches the properties of the components P2 or P1 respectively. Let us consider for instance the elastic resistance of a ﬁbre-reinforced matrix. For unidirectionally distributed ﬁbres in a matrix, the Young’s modulus along ﬁbres is El ¼ f1E1 þ f2E2 while it is 1/Et ¼ f1/E1 þ f2/E2 along the normal direction (so called model of springs in parallel or series respectively weighted by the volume fraction of the respective phases; see Chapter 6). The resulting moduli are shown in Fig. 2.6. Using the mixing rules allows tailoring the composite properties between the component properties, adjusting the volume fractions as well as the orientation of the ﬁbres. It is well known so far that the simple linear rule presented above does not apply for all properties of technological importance. While a rule of mixture applies quite well to density and elasticity, it fails to predict the composite material toughness Kc because adhesion and interface issues are of utmost importance in the response and hence in the performance of a composite.

2.3 Selecting Materials

Generally not only one performance is to be optimized but several. An industrial product is then optimized to yield the best compromise between the required properties. For instance, a windscreen is designed with optical transparency, with strength to protect the driver from wind and weather, and with new functions introduced into the

2.3 Selecting Materials Tab. 2.4

Attractive glass properties for different applications.

Glazing Containers Optical glass Glass wool Fibres for reinforcement

Transparency

Strength

Rheology

Chemical inertness

++ + +++

++ ++ + ++

++ ++ + ++ ++

++ +++ ++ ++

laminate (solar control, antenna, etc.). By the way, to achieve such a product, the manufacturing tools have to work in given ranges of properties, for instance viscosity and diffusion. The development of a new product supposes a compromise to be met between all these parameters. This is referred as co-selection. Table 2.4 lists the main properties of glass according to various applications. Transparency is obviously of utmost importance for glazing and optical glasses. This performance combined with strength, rheology and cost make glass very competitive as compared to polymers. In fact, rheology is a very important issue as regards the process. Glass even though not showing exceptional performances in all ﬁelds presents a combination of desired properties that makes it very attractive. Let us consider its transparency according to its cost (or price that takes into account the cost of raw materials, process, marketing and labour; see also Section 12.1), as shown in Fig. 2.7. In this ﬁgure transparency is plotted as a function of price per volume from the materials data base elaborated by Ashby’s team (CES 4, Granta Design; Ashby, 2001). The optical performance is separated into four categories (opaque, translucent, transparent, optical quality). When considering transparency, the glassmaker is interested into the two last categories. Only dedicated optical devices require optical quality (i.e. extremely low optical loss). From the transparency–price chart we already observe that glass is a very good compromise, since only polymers compete. Glass is generally preferred because of its strength, UV protection (in containers), chemical protection, chemical inertness (allowing for conservation of foods and liquid, a property that may remain at elevated temperatures) and tailored optical properties. Developments of glazing encompass tailoring optical properties with transparency at visible wavelength while being opaque to IR and UV (Lehmann, 2005; see also Chapter 4). A chart showing so many parameters requires several dimensions; instead, Ashby (2001) proposes different methodologies to select the optimized materials or compositions either by a step-by-step selection or by using a weighted combination of the important properties that are of interest (weight-factors method). It is out of the scope of this book to detail all these methods and the interested reader should refer to dedicated books cited in the bibliography. As a preliminary, we shall see in the next section how several properties can be combined in a performance index and hence how to select a material in view of a combination of 3–4 properties using graphical methods. The example of selection according to transparency is an archetype. Let us consider a more realistic selection of a glass according to more quantitative properties. As

13

14

2 Glass, A Ceramic Material

Fig. 2.7 Transparency–cost chart (obtained from CES 4, Granta Design, Ashby, 2001).

discussed in detail in Chapter 6, viscosity is one of the most important properties from the process point of view since it controls the stresses and strains to be applied to form the glass. The selection will then be according to the process requirements that set such a parameter (the viscosity in this case) at a given temperature. Research on glass has revealed that in limited domains empirical relations exist between the compositions of oxide glasses and the properties (Priven, 2004). Notably, glass composition can be continuously varied since no stoichiometric laws prevail, in contrast to crystalline solids. This allows for adjusting and approaching the desired performance. The optimization of the composition for process optimization can then be made using these empirical laws to deﬁne a range of compositions likely to yield a glass with the required properties. The estimated ranges of compositions are obviously as accurate as the empirical correlations used for the procedure. For more accuracy in the prediction, further experiments can be made for a selected domain of compositions. One will never ensure that such a range of compositions is indeed a solution to the problem, but it indicates in what range of compositions the costly experiments are probably worth undertaking. The use of designed industrial experiment plans (Sado and Sado, 1991) allows one to minimize the number of fabricated and tested specimens and to predict at minimum costs the selected domain.

2.4 Performance Indices

2.4 Performance Indices

We have seen that selecting materials requires many parameters to be taken into account (co-selection). In fact, an extensive survey of the technological applications has been made by M.F. Ashby’s team and they proposed different performance indices according to the target applications that are combinations of relevant properties of the materials. Let us for instance consider the thermal shock resistance, also known as thermal endurance, deﬁned as the maximum sudden change in temperature which a glass surface can withstand without breaking. Thermal shock happens, for example, when an object is moved abruptly from or into a furnace. These are complex thermomechanical loading conditions that are of utmost importance for the glass (and other) industry since heat treatments are extensively used to produce glazing either during forming or tempering steps (as detailed in Chapter 6). Stresses generated under a thermal gradient are proportional to thermal strains (Hooke’s law; see also Appendix 9) while thermal strains are proportional to the thermal expansion coefﬁcient of the material and to the temperature variation amplitude (DT; see also Chapter 6). The resulting stresses s are written s ¼ CaEDT

ð2:1Þ

where a is the thermal expansion coefﬁcient, E Young’s modulus and C a coefﬁcient dependent on the Poisson ratio (C ¼ 1 for axial constraint, (1 n)1 for biaxial constraint or normal quenching and (1 2n)1 for triaxial constraint, where n is the Poisson ratio; see also Chapter 6 and Appendices 3 and 9). It should be said that the actual value of the stresses developed by a given thermal shock would depend in fact upon many other factors, such as the thermal conductivity of the glass, the thermal conductivity of the ﬂuid that applies the thermal shock and the thickness of the glass (these three factors change the magnitude of DT ). Such factors are neglected here. Ashby (2001) suggested plotting a versus E in a log–log diagram (Fig. 2.8), since in such a plot aE contours are shown as parallel lines: aE constant implies log a ¼ log E þ constant, which for a log–log plot is represented by a straight line of slope –1. On a same line, the value of aE product is then a constant and is deﬁned as the performance index as regards thermal shock stresses. Observing that aE is expressed in MPa K1, the materials shown on the same line are submitted to identical thermal stress amplitude under the same thermal variation amplitude. For instance, along the line indexed 1 MPa K1, all materials would experience thermal stresses of 100 MPa amplitude when submitted to instantaneous (this hypothesis allows neglecting of thermal conductivity mentioned above) thermal shock of amplitude 100 8C. Fig. 2.8 shows that the different groups of materials locate at separated places even though partial overlapping is observed. Overlapping of composite and ceramics groups is not unexpected. Interestingly most important oxide glasses, that is soda-lime-silica (SLS) and borosilicate glasses match the ceramics group. As regards all the materials, one observes that aE index shows a very large variation ranging between 0.01 and

15

16

2 Glass, A Ceramic Material

Fig. 2.8 Thermal expansion coefﬁcient a as a function of Young’s modulus E (according to Ashby, 2001).

10 MPa K1. This map actually allows for a wide materials selection according to what is required for the application (either high or low thermal stresses). Metals show the highest aE index values, while woods and elastomers show minimum values. Regarding glasses, silica is observed to be below 0.1 MPa K1 while SLS glasses could be submitted to more elevated thermal stresses (about 0.5 MPa K1). In fact, for applications requiring thermal shock resistance, silica-rich and borosilicate glasses have been developed, so-called Nonex (for nonexpanding, invented in 1912 by E.C. Sullivan and W.C. Taylor to reduce lantern globe breakage by 50%) and Pyrex developed by Corning (Kurkjian and Prindle, 1998; see also Chapter 3). On the contrary, when tempering is considered elevated aE indices are required. This is in favour of utilizing compositions of standard silico-soda-lime type that are actually produced as tempered glazing. When considering the risk of breakage, the next step consists in considering another important property of the material in this context, that is, its ultimate stress sf at rupture or, say, the stress at which the material will break. As we shall see in Chapter 7 ceramics (and indeed glass) show statistical fracture. We consider here an average or representative stress at which such articles break. Then under thermal shock, breakage will happen when the thermal stresses reach the ultimate stress. This condition is written sf ¼ CaEDT

ð2:2aÞ

2.4 Performance Indices

or forming members without units: sf =E ¼ CaDT

ð2:2bÞ

where sf/E is the strain at fracture for a brittle material (see Section 7.2). Fig. 2.9 plots sf/E as a function of thermal expansion coefﬁcient a again using logarithmic scales for both axes. This presentation allows one to show resistances at a given thermal shock amplitude DT as straight and parallel lines. Again materials shown on the same line have the same thermal shock resistance. For instance, the materials shown on the 100 8C straight lines resist a thermal shock of amplitude less than or equal to 100 8C. The materials showing larger resistance are those appearing on the left and upper part of the ﬁgure. This ﬁgure shows also that the different groups of materials locate at separate places even though partial overlapping is observed. Again, overlapping of composite and metals groups is not unexpected. Oxide glasses match the ceramics group again. As expected from the a–E chart, materials show a very broad range of resistance. Ceramics cover a 10–1000 8C domain while glasses cover a reduced domain ranging from 50 to 300 8C. Different performance indices (combining relevant properties) allow optimization of materials selection for a given application employing Table 2.5. An important parameter is the cost which can be combined with density.

Fig. 2.9 Chart for thermal shock resistance showing sf/E as a function of thermal expansion coefﬁcient a (according to Ashby, 2001).

17

18

2 Glass, A Ceramic Material Performance indices for mechanical design (after Ashby, 2001). Parameter C is the cost per kg (see also Chapter 12).

Tab. 2.5

Function, objective and constraint

Index

Window, maximum thermal shock resistance Tie, minimum weight, stiffness prescribed Beam, minimum weight, stiffness prescribed Beam, minimum weight, strength prescribed Beam, minimum cost, stiffness prescribed Beam, minimum cost, strength prescribed Column, minimum cost, buckling load prescribed

sf/Ea E/r E1/2/r Y2/3/r E1/2/Cr Y2/3/Cr E1/2/Cr

2.5 Shape Factors in Mechanical Design

We shall see that, besides choosing the right material, it is also important to select the right shape to produce the manufactured object. Consider for instance a paper sheet placed vertically: it shows poor buckling resistance when compressed. Instead, when folded its resistance dramatically increases. Also, plastic chair legs are fold shaped. Fig. 2.10 shows a glass roof supported by long glass beams with rectangular section set in such a way that their larger side is vertical. As discussed in detail a rectangular section allows a much better mechanical performance than a square section. It is important to note that it is the elastic failure and not the brittle failure (Chapter 7) that limits the present structural application. In fact a single tempered beam with its larger side set vertically is able to support 12.5 tons under four-point bending before buckling happens (R. Gy, personal communication).

Fig. 2.10 Glass atrium at the top ﬂoor of the building at 53–55 Av. Georges V (Paris). The glass roof is supported by tempered and laminated glass beams. These have 2 19 mm2 sections, the larger side being set

vertically. The longer beam is approximately 7.1 m long. Architects: J.L. Robert, J.W. Wilmotte, P. Granger. The atrium at the 8th ﬂoor was designed to allow maximum daylight. (Courtesy R. Gy, Saint Gobain Recherche.)

2.5 Shape Factors in Mechanical Design

Both shape and materials selections should be carried out together since shaping depends on the type of material, e.g. ceramics are more difﬁcult to shape than metals. Let us concentrate on mechanics, which is the focus of the book, and more precisely now on the mechanical design that has been extensively reviewed by Ashby (2001). Several performance indices are listed in Table 2.5 according to the application. At this stage, these indices do not yet consider shape. Let us take an example to determine the performance index and determine how shape inﬂuences this performance. This will allow us to introduce the shape factor and hence understand how shape contributes to object strength. Let us consider a beam under ﬂexure (Figs. 2.11 and 2.12). We prescribe a given stiffness with minimum weight. The following expression holds (Fig. 2.12a): F IE ¼k 3 d l

ð2:3Þ

where F is the load, d the displacement of the beam centre, l the distance between supporting points (all ﬁxed by the customer), E Young’s modulus and I the second Ð moment (I ¼ section y2 dA, where y is the distance from axis and dA the related surface at distance y). For a square section of area b2, the second moment is ð I¼

b=2 ð

y dA ¼ 2

section

y2 bdy ¼ b=2

b 3 b=2 b4 y b=2 ¼ 3 12

and Eq. (2.3) is written F k b4 E ¼ d 12 l3

Fig. 2.11 Tempered glass beam under ﬂexure (four-point bending). For the experiment here, the larger side is set horizontally. This set-up was used to determine the delayed elastic response (Gy, 1999; see also Chapter 6. Courtesy R. Gy, Saint Gobain Recherche.)

ð2:4Þ

19

20

2 Glass, A Ceramic Material

Fig. 2.12 (a) Beam under elastic ﬂexure; (b) two beams with identical section area but different shape.

The mass of the beam is simply M ¼ rlb2

ð2:5aÞ

and with Eq. (2.4) is 1=2 F 12 l3 M ¼ rl d k E

ð2:5bÞ

This can be rewritten, separating the geometrical characteristics and the material properties, as M¼

F 12 3 1=2 r l d k E 1=2

ð2:5cÞ

For a given application, mass is then minimized when E 1=2 r

ð2:6Þ

is maximized. This ratio is called the performance index. Note again that shape is not considered until now (or assumed to be the same up to this point).

2.5 Shape Factors in Mechanical Design

As we shall see now, shaping the beam allows one to improve further the performance. Let us still consider a beam under ﬂexure but now consider two different but simple shapes for the beam (Fig. 2.12b) with the same section b2. One of the beams has a square cross-section (already studied) while the second has a rectangular cross-section, its smaller side being set horizontally. In fact, when the beam is set on its larger side then the ﬂexure performance is poorer; this can be easily shown using the method described now or experienced in everyday life. The second moments are I ¼ b4 =12

ð2:7aÞ

and I0 ¼

ð

ðb y2 dA ¼

section

b

b b b b4 y2 dy ¼ y3 b ¼ 2 6 3

ð2:7bÞ

for the square and rectangular section respectively. Equations (2.3) with (2.7b) show that the rectangular shape offers stiffer response. Calling f ¼ I 0 =I

ð2:8Þ

the shape factor (f ¼ 4 in the present case) and using the same procedure as before shows that the performance index transforms into ðfEÞ1=2 r

ð2:9Þ

This shows a square dependence on shape factor (in the present case performance is then twice as high for the elongated beam). Therefore, the shape of the beam is expected to play an important role in mechanical design. The performance can be considerably improved when using an elevated shape factor. As mentioned before, shaping has materials constraints. Then, one has to consider all required performance factors (co-selection). Shape should be considered at different scales: (i) at the macroscopic level (glazing, glass beam shape, arrangement and placing to be optimized for different applications (buildings, vehicles)); and (ii) at the microscopic scale (the arrangement of glass ﬁbres in glass wool, in a composite or in a mat is to be optimized). In fact, there is still R&D effort towards optimizing glass wool recovery. When glass wool is produced, it is packed and stored under different environments. Glass wool recovery on unpacking is essential to allow maximum insulation and hence performance and this recovery will depend on the ﬁnal arrangement of glass ﬁbres. The study of the mechanical response of entangled glass ﬁbres is complex and still the subject of ongoing research (Durville, 2005; Bergonnier et al., 2005).

21

22

2 Glass, A Ceramic Material

Ashby (2001) proposed the use of charts to predict shape inﬂuence and determine the gain that can be achieved. Let us consider again the loaded beam under ﬂexure as an illustrative example. The method is the following. A simple mathematical operation consists in dividing both parts of Eq. (2.9) by f so that ðfEÞ1=2 r

ð2:10Þ

transforms into ðE=fÞ1=2 E 1=2 ¼ r=f r

ð2:11Þ

Then the charts can be used to select ‘shaped materials’ that are placed on the chart as artiﬁcial ones at coordinates E ¼ E/f and r ¼ r/f. A shaped material is positioned relative to the unshaped one on the chart as shown in Fig. 2.13. As expected a shaped material offers a better performance than an unshaped one. In fact, on this chart, the performance index E1/2/Cr that corresponds to a beam with minimum weight and stiffness prescribed is represented by lines of slopes þ2 (as usually the performance is identical on the same line). It is then observed that the shaped material is positioned towards the left and bottom side as compared to the unshaped one. The magnitude of

Fig. 2.13 Young’s modulus–density chart (according to Ashby, 2001).

2.5 Shape Factors in Mechanical Design

the achieved improvement can be predicted plotting the (E, r) position. Interestingly, composites like wood having natural microshapes show the best performance for the designed beam. Shaping engineered materials allows one to approach the domain covered by natural or biomaterials as illustrated in Fig. 2.13. In fact, bio-inspired materials have become an important ﬁeld of research (so-called biomimetic materials) since great gains in performance are expected.

23

25

3 Glass Prehistory and History 3.1 Natural Glasses

Natural glass has existed since the beginnings of time, formed when rocks melt as a result of high-temperature phenomena such as volcanic eruptions, lightning strikes or the impact of meteorites, and then cool and solidify rapidly enough so that a liquid-like structure can be frozen in glassy state (see Fig. 5.15). Rocks can be classiﬁed according to the way they form either from sediments or eruptions (Dejean-Arrecgros, 1978). The compositions of volcanic rocks do not differ signiﬁcantly from sedimentary ones contrary to their respective thermal histories. It is well known that glass formation is a kinetic phenomenon (Chapter 6; Tammann, 1925). Most well-known natural glass is obsidian that is believed to be one of the ﬁrst glasses that appeared on earth at least 40 million years ago. Such an impressive age demonstrates that the vitreous state may be resistant in the long term against devitriﬁcation and water corrosion (Fig. 3.1; more images can be viewed at http:// www.musee.ensmp.fr/gm//lettres.htm, refer also to Sedgwick Museum of Earth Sciences collection, Cambridge U.K.). Glass utilization would have started when stone-age people became aware of the strength and sharpness that could be obtained from obsidian. Stone-age humans (75 000 BC, long before humans learned how to make glass) are believed to have formed (here form means mechanically, not thermomechanically) and used cutting tools and arrowheads made of obsidian. The formation of natural glasses may happen under three main conditions, the ﬁrst two corresponding to a compromise between the glass composition (viscosity regime) and the cooling conditions (as discussed in more detail in Chapter 5): i. Magmatic formation: the silicate (silica-rich) melt being rejected from earth’s mantle at the surface by volcanic activity cools down at rates scaling from 1 8C per minute to 1 8C per month (Chapter 5). ii. Metamorphic formation: these conditions correspond to extremely fast heating and cooling of rocks and melts (1 8C per second) during impact, friction or lightning. Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

26

3 Glass Prehistory and History

Fig. 3.1 Obsidian. (Copyright Ecole des Mines de Paris.)

iii. Sedimentary silica gel may be formed after drying over large periods of time scaling from years to thousands of years. Also natural biological glass forms sponge (Fig. 3.2, refer also to University Museum of Zoology, Cambridge U.K.) and mollusc skeleton and shell (Sundar et al., 2003). These mild synthetic conditions have inspired sol–gel science (see Chapter 12). Figure 3.3 shows the composition ranges of natural glasses together with humanmade glasses according to the relative concentrations of formers, modiﬁers and amphoteric ions (see Chapter 5 for precise deﬁnitions). The classiﬁcation is based on the way the ions participate in the glass network (forming the network or modifying it, amphoteric being intermediate). Such a diagram is very instructive since it shows that the chemical domain occupied by industrial glasses separates dramatically from the one occupied by natural glasses. The relation between network modiﬁers,

Fig. 3.2 Silica glass sponge; scale bar is 5 cm. (Reprinted from Sundar et al., 2003, with permission from Macmillans Publishers Ltd.)

3.1 Natural Glasses

Fig. 3.3 Compositional ranges of manufactured and natural glasses. Network modiﬁers: Li, Na, K, Ba, Ca, Mg, Fe2+, Pb, Zn; network formers: Si, P, B; amphoteric or intermediate ions: Al, Fe3+. (According to Heide et al., 2003.)

network formers and intermediate oxides is indeed much different since industrial glasses have more network modiﬁer than natural ones. The majority of natural glasses are peraluminous (Al2O3 > Na2O þ K2O þ CaO) whereas human-made glasses are peralkaline (Al2O3 < Na2O þ K2O þ CaO) in terms of geosciences. Magmatic glasses (obsidian; Table 3.1) tend to be silica-rich and contain less than 10 % of alkaline. Their dark colour is due to iron oxides. Their purity and elevated viscosity allowed for the natural production of these glasses. Notably on the Moon, eruptive glasses form more easily because of the absence water, which leads to the induced elevated viscosity. Magmatic glasses can be found in Iceland, the Canaries and Wyoming. Premise stones have compositions close to that of obsidian, while Typical glass compositions of natural and manufactured glasses. Natural (magmatic: obsidian; metamorphic: australite, lunar glass) (weight percent, E and S glass fibre for composites).

Tab. 3.1

Glass

SiO2

Obsidian Australite Lunar glass Egypt (1500 BC) Italy (9000 BC) Container glass Glazing Glass wool Nonex Pyrex E glass (ALS) S glass

74.6 70.4 54.5 67.8 77.8 67–70 71–73 65 73 80.5 54 65

B2O3

4.5 16.5 12.9 10.0

Na2O

K2O

4.0 4.7 1.6 2.5 0.1 n1). The light beam follows Descartes’ law with reﬂection at the refractive index interface.

moisture and contact by hermetic coatings which are deposited during the sizing step (Chapter 10). As a matter of fact, ﬁbres offer exceptional stxrength and optical performance that have yield such an impressive development in communications. One drawback of glass when considered for lenses is its density, and load gains are accomplished by controlling better glass distribution (Section 4.2). It should be noted that nowadays spectacles are made of organic glasses. These allow load gains and comfort. Organic glasses are polymers formed by long organic chains (similarly, chalcogenide glasses are constituted of Se chains, their applications being described below). One single spectacle lens is composed of several layers, some of these being

Fig. 4.9 Transmission of ‘infrared’ glasses compared to silica. BIG is a multicomponent ﬂuoride glass based on BaF2, InF3 and GaF3. TeX is a multicomponent chalcogenide glass based on the combination of Te, Se and I2 (according to Lucas, 1999). Observe the huge changes in the IR window.

47

48

4 Applications of Glass

only protective because of the poor scratch resistance of polymers as compared to glass (Chapter 8). More recently chalcogenide glasses have been proposed for application in IR vision (they are also used for DVD-RW taking advantage of their laser-induced glass– ceramic transition). In fact these glasses formed with group VI atoms associated with either group IV or V atoms (Appendix 2) allow for improved transparency in the IR domain (Appendix 1; 8–12 mm wavelengths, Fig. 4.9). This leads to application for night observations, detection of thermal loss in buildings and in situ medical observation (Lucas, 1999). These glasses while showing ‘plastic’ behaviour remain very brittle at room temperature (Guin et al., 2002; see Chapters 7 and 8). Hence, there is an important demand for improving the contact resistance and hence extending their future applications.

4.4 Glass Fibres for Insulation and Reinforcement

The glazing, packaging and optical applications of glass are the most well known since they refer to glass transparency. Glass is also used for thermal and acoustic insulation or to reinforce plastics (Figs 4.10 and 4.11) and concrete (CEM-FIL1) because of their low cost and high strength. In the latter case, compositions incorporating ZrO2 allow to resist concrete chemical attack. Polymers reinforced by glass ﬁbres are fabricated as composites and used in transportation applications (automotive front ends, vehicle furniture, plane cockpits, etc.). As discussed in Chapter 2, composite properties are a mix of those of the constituent parts, sometime in a complex way. In the simplest case a rule of mixture of properties may be employed in a linear form: P ¼ f1P1 + f2P2, where fi are the volume fractions of each component (glass and polymer in the present context). It allows

Fig. 4.10 (a) Glass wool (copyright Saint-Gobain) and (b) ﬁbre-reinforced composite used for the front end of an automobile.

4.5 Abrasive Tools

Fig. 4.11 Glass mats: (a) Saint-Gobain Uniﬁlo1 and (b) Multimat formed by E-glass ﬁbres.

tailoring stiffness (Fig. 2.6) and load gains that are attractive for transportation and in particular for airplanes since, for instance, saving a mass of 1 kg on commercial planes increases the travelled distance by about 1 mile (Gay, 1997). Moreover as discussed later in the book (Chapter 7), ﬁbres can be produced with much higher mechanical strength than any glazing. This makes the ﬁbres very attractive for improving composite strength. Glass wool is produced for buildings and vehicles and forms an air–ﬁbre composite. Notably, the glass composition is tailored accordingly for different applications (Table 4.1; Chapter 5). Wool ﬁbres have been optimized to allow maximum recovery when unpacked and set (Chapter 2). Also, their dissolution in vitro has been of utmost importance since the problems generated by asbestos (see water diffusion and hydrolysis of siloxane bonds, Chapters 5 and 7). Biodegradable glass ﬁbres have been developed accordingly (Chartier, 1997).

4.5 Abrasive Tools

Abrasive applications are not so well known. Glass can be used as a bond between abrasive grits to fabricate cutting tools. Glass composition is then tailored to obtain grit wetting and a strong grit–glass interface (Alliche and Le Bourhis, 2000). Figure 4.12 shows different grinding wheels composed of grits (alumina, silicon carbide) that are bonded together by a glass matrix. A scanning electron micrograph shows different grey contrast for the grits and bonds (Fig. 4.13). Note the elevated porosity of such a wheel. In fact, porosity is required for cooling and evacuating the metal chips generated when tooling a piece (Coes, 1971; Malkin, 1989; Tawakoli, 1993; Alliche and Le Bourhis, 2000). For high-speed grinding operations, wheels are made of a metal core (with high thermal conductivity) and abrasive segments ﬁxed at the wheel circumference.

49

50

4 Applications of Glass

Fig. 4.12 Vitriﬁed bonded abrasive wheels. (Copyright Saint-Gobain.)

Fig. 4.13 Scanning electron micrograph of a vitriﬁed bonded abrasive.

4.6 Glass Manufacturers

Some well-known glass manufacturers are listed below, subdivided into the applications reviewed above.

4.6 Glass Manufacturers

i. Flat glass: Saint Gobain (France), Guardian (USA), Pilkington (UK), PPG (USA), Glaverbel (USA), Asahi (Japan), Schott (Germany). ii. Packaging: Saint Gobain (France), BSN Glasspack (USA), Anchor Glass (USA), Owens Illinois (USA), Rexam, Vitro (Mexico), Gerresheim (Germany, USA), Pochet (France), Rocco Bormioli (Italy), Wheaton (USA). iii. Optical glass: Heraeus (Germany), Schott (Germany), Corning (USA). iv. Glass wool: Saint Gobain (France), Amstrong (USA), Johns Manville (USA), Owens Corning (USA), Rockwool (EC), Uralita (EC). v. Reinforcing ﬁbres: Saint Gobain (France), Johns Manville (USA), PPG (USA), Owens Corning (USA), Nottobo, Porcher. vi. Abrasives: Saint Gobain1) (France), Asahi (Japan), Noritake (Japan), 3M (USA), SAIT (Italy), SIA (Switzerland), Tyrolit (Austria). Note that none of the manufacturers are present in all six main domains. As a matter of fact, each domain requires speciﬁc know-how and tools.

1)

Winter, Unicorn and Norton are now part of Saint Gobain group.

51

53

5 Glass Structure 5.1 Introduction

Glass structure is out of equilibrium. It is obtained when a liquid is cooled down in such a way that on passing the melting temperature or liquidus temperature (TL), ‘freezing’ happens instead of crystallization (Tammann, 1925). The ﬁnal temperature must be so low that molecules or atoms move too slowly to rearrange to the more stable crystalline form. In Chapter 6 we shall discuss extensively the atomic mobility in terms of viscosity. In particular, we shall see that glass structure may depend upon thermal history. For instance, a liquid will yield denser glasses when the cooling rate decreases. This chapter shows the prominent characteristics of glass disordered structure. Alternatively, glass can be built up onto a substrate, either by deposition or chemical reaction from the vapour, the substrate being cold enough that rearrangement cannot take place. In fact, although they are named differently, amorphous silica (a-SiO2) ﬁlms and silica glass bulk are the same materials having the same chemical composition and a random network. Ryu and Tomozawa (2006) suggest that the concept of ﬁctive temperature can be used to describe a-SiO2 ﬁlm structure as well (see also Chapter 6). However, amorphous layers have been achieved with a limited number of substances as compared to the usual route (Doremus, 1994). Many deﬁnitions of glass have been proposed: we shall use the most commonly used one that deﬁnes it as an amorphous solid showing a glass transition (Zarzycki, 1982). The glass is frozen in a structure showing only short-range order that makes its characterization quite difﬁcult as compared to crystalline structure that presents long-range order (periodical structure with the repetition of a unit cell; see also Table 2.3). As discussed below, diffraction experiments on glasses yield results that most closely resemble those of liquids (see also Chapter 2).

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

54

5 Glass Structure

Let us start with silica and related glasses because of their practical importance and the well-documented literature.

5.2 Silica Glass and Related Glasses 5.2.1 Glass Network

Silicon (Si) is in group IV of the Mendeleev table (Appendix 2) and tends to bond to four different oxygen (O) atoms. Note that what is described here applies as well to germania glasses changing Si into Ge. Hence, each oxygen atom is shared by two silicon atoms. In three dimensions (3D), Si and O atoms arrange to form oxygen tetrahedral elements with a Si atom at the centre (Fig. 5.1). This is in terms of chemistry the resulting bonding through four sp3 hybrid orbitals of silicon and two 2p orbitals of oxygen atoms (see also Appendix 2). Then the structure can be thought of as built up by the sharing of corners by pairs of these oxygen tetrahedra. Two tetrahedra meet at only one corner, but all corners of all tetrahedra are actually shared. This is shown in Fig. 5.2 for the crystalline and glass form of SiO2. Interestingly, a very open 3D structure may then be built in many ways, in which the Si–O–Si lines may or may not be straight. One observes rings of atoms of different sizes when a disordered structure is generated (this will be more obvious in 2D). In fact, it is helpful to project the structure on a surface where tetrahedra become triangular elements. One can also consider the projected glass as an imaginary 2D oxide Si2O3 (Jones, 1956). In such a 2D projection of the network we shall shift from a perfectly ordered structure to a disordered one (Fig. 5.3). Figure 5.3a shows again the crystalline projected structure of SiO2 (quartz) while Fig. 5.3b shows the continuous random network (CRN), or a network without periodicity illustrated now in 2D and ﬁrst proposed for silica glass by Zachariasen (1932). It is observed in both structures that oxygen atoms are bonded to two silicon atoms forming Si–O–Si chains. Figure 5.3a reveals a long-range order characteristic of a crystalline solid (repetition in space of a unit cell). In fact, any atom’s position can be predicted in this ordered structure. Figure 5.3b shows instead only a short-range order that is in great contrast with the 2D projection view of Fig. 5.3a. In fact, it reveals no long-range order any more while the structure still respects the stoichiometry

Fig. 5.1 Elemental tetrahedron, Si (group IV) bonds to four O.

5.2 Silica Glass and Related Glasses

Fig. 5.2 SiO2 structure: (a) crystal form; (b) glassy form. An elemental tetrahedron is shown in each case (dashed lines).

since all oxygen atoms are bonded to two silicon atoms forming Si–O–Si bonds. The atomic arrangement cannot be predicted any more in the latter case. One further observes the existence of rings with a different number of bonds. It seems from modelling that smaller rings would appear on cooling glass rapidly or, say, so-called network polymerization would be affected by thermal history (Ito and Taniguchi, 2004). In fact, the glass structure is known to be determined by its past thermal history and this phenomenon will affect the details of the structure and the structural relaxation as discussed extensively in Chapter 6.

55

56

5 Glass Structure

Fig. 5.3 2D projections of structures showing the path from crystalline to glassy structure: (a) crystalline form of SiO2; (b) glassy form of SiO2; (c) glassy form of SiO2 modiﬁed by Na+ ions. Note the presence of one NBO per Na+. The projection of a tetrahedron is shown in each case (dashed lines).

5.2 Silica Glass and Related Glasses

Fig. 5.3 (Continued )

5.2.2 Glass Network Modiﬁcation

In Fig. 5.3c the CNR is shown this time when sodium oxide is added to the structure (or more generally an alkaline or an alkaline earth oxide). Na+ is called a modiﬁer since when added to the glass it modiﬁes the Si–O network. Na+ ions are charged with an elemental positive charge þe and each of them are compensated by the formation of one non-bridging oxygen (NBO) atom that holds a negative charge e. Therefore, in a glass containing modifying ions, NBO atoms appear (as opposed to bridging oxygen (BO) atoms which form the network). Figure 5.3c shows additionally that two Na+ ions are necessary for compensating the charges generated by the rupture of one O–O bond (one Na+ ion compensates one NBO). The two tetrahedra still interact electrostatically. In fact, electrostatic interactions exist between the two NBO atoms and the two Na+ ions. As revealed experimentally however, glass network modiﬁcation induces a viscosity decrease or a greater facility for viscous ﬂow. CRN model accounts quite well for the observed change in properties as the glass composition is modiﬁed. Modiﬁers disrupt the network and are used in fact to lower the viscosity of the glass melt and hence to facilitate its fabrication at lower temperatures (Chapter 6). In fact, silica glass is difﬁcult to process and instead of standard melting procedure (Chapter 10) it is produced following ceramic routes. The melting temperature of silica is as high as 1713 8C corresponding to cristobalite–liquid equilibrium. Instead, adding 25 % of soda to silica lowers the liquidus temperature to only 793 8C (Jones, 1956). Alkali metal ions like Naþ are mobile and allow for electrical conductivity, ion

57

58

5 Glass Structure

migration. In contrast, alkaline earth ions like Ca2+ ions (one alkaline earth ion is compensated electrically by two NBOs) are relatively immobile and can hinder the diffusion of other ions, in particular alkali, and hence improve the chemical resistance of the glass (see also Section 5.8). It is then clear why most important commercial glass, SLS glass, is based on a mixture of silica (network former), sodium and calcium oxides (alkaline and alkaline earth modiﬁers respectively). As expected then, the relative concentration of bridging and non-bridging oxygen atoms has an important inﬂuence on the properties of glasses (Kurkjian and Prindle, 1998; De´riano, 2002). Let us call BON the number of bridging oxygen atoms in a tetrahedral element; we can anticipate the following rules: i. For BON ¼ 4, that is [O]/[Si] ¼ 2 since each BO is shared by two silicon atoms, the network is a three-dimensional one with all four corners bridging. ii. For BON ¼ 3, [O]/[Si] ¼ 2.5, the network is two-dimensional with three corners bridging (note that some tetrahedra may be linked to four others and some therefore to less than three, the said number being the average value over the network). iii. For BON ¼ 2, [O]/[Si] ¼ 3, the network is formed by one-dimensional chains with one corner bridging. iv. For BON < 2, [O]/[Si] > 3, the network is composed of individual SiO4 tetrahedral elements, some of these being bound together. Using Qx terminology with x the number of bridging oxygen atoms on a tetrahedron, we refer to (i) Q4, (ii) Q3, (iii) Q2 and (iv) Q1, Q0 structures respectively. The stiffness of the network decreases gradually by replacing the bridging oxygen atoms by non bridging ones until only individual isolated tetrahedra remain. Consider a modiﬁed oxide glass of general composition (A2O)x(SiO2)1x with A the alkali metal.TheconcentrationofBOandNBOvarieswithxasshowninFig.5.41).Forx ¼ 0,thatis for pure silica, only BO exist (Q4), the relative concentration being then 2, while increasing alkali concentration yields a dramatic decrease of BO and an increase of NBO accordingly. Dietzel (1942) proposed classifying the oxides according to their ability to form or modify the glass network in view of their cation ﬁeld. He deﬁned the cation ﬁeld intensity A as a charge-to-distance squared ratio: A¼

Z ðrc þ ro Þ2

ð5:1Þ

where Z is the cation valence and rc and ro are the cation and oxygen radii respectively (Appendix 2). The Dietzel ﬁeld amplitude varies within a relatively broad range of 1.2 to 0.1 (Table 5.1) and is indicative of the magnitude of the electrostatic attractive force 1)

Introducing x A2O yields 2x NBO. The total number of oxygens is x + 2(1 x). Hence introducing xA2 O leaves xþ2ð1xÞ2x ¼ ð23xÞ NBO. ½NBO=½Si¼2x=ð1xÞ. ½BO= ½Si ¼ ð23xÞ=ð1xÞ.

5.2 Silica Glass and Related Glasses

Fig. 5.4 Relative concentrations of bridging oxygen (BO) and non-bridging oxygen NBO as a function of x in a modiﬁed silica glass of general formula (A2O)x(SiO2)1x.

between the considered element and oxygen (Appendix 2). The ordered sequence of oxides is relatively convincing, since for A > 1 we ﬁnd the oxides that form the glass network while for A < 0.35 the oxides (alkali in particular) are known to modify the network. Between these two extreme behaviours, intermediate oxides may show both behaviours according to the glass composition (Table 5.1). Dietzel’s approach suggests that both smallness and high charge of the cation favour the formation of glassy oxides. Too much importance must not be attached to one criterion or another (for instance single bond strength to heat of dissociation ratio). These are mostly empirical and break down when structures are unusual, as in As2O3 and PbO for instance (Jones, 1956). Also the situation is very complex when weak VDW bonds coexist with strong covalent bonds as in chalcogenide glasses (Section 5.4). Besides decreasing the viscosity, modiﬁers allow for the liquidus (or melting) temperature to decrease to a more viscous domain and hence favour glass formation Tab. 5.1

˚ ). Dietzel field intensity and role of cations in glass (r0 = 1.4 A

Role

Cation

Z

˚) rc (A

A

Network formers

Si B Ge Ti Al Zr Be Mg Zn Ca Pb Li Na K

4 3 4 4 3 4 2 2 2 2 2 1 1 1

0.4 0.25 0.53 0.74 0.53 0.86 0.41 0.86 0.88 1.14 1.33 0.90 1.16 1.52

1.23 1.10 1.07 0.87 0.80 0.78 0.61 0.39 0.38 0.31 0.27 0.19 0.15 0.11

Intermediates

Modiﬁers

59

60

5 Glass Structure

Fig. 5.5 Modiﬁed random network as proposed by Greaves (1985) showing Si-rich zones connected by modiﬁer-rich percolating channels marked in grey.

(Barton and Guillemet, 2005). Alkali metal ions (Li, Na, K, valence 1) are more efﬁcient than alkaline earth ones (Ca) for inducing both effects. Pb, while being classiﬁed as a modiﬁer, allows fabrication of glass associated with only 8 wt% of silica. This supposes Pb atoms are forming the network while bridging two oxygen atoms. This question is still open and under debate. Alumina modiﬁes the silica network (decrease of the viscosity); when introduced with alkali metal, Al may participate in network formation with a related increase of the viscosity. More recently Greaves (1985) introduced a modiﬁed random network where modiﬁers form zones connecting silica-rich volumes as shown for a modiﬁed silica glass in Fig. 5.5. This model offers interesting predictions and suggestions as regards the plastic deformation of silicate glasses. It can be anticipated that such glasses would preferentially ﬂow through modiﬁer-rich zones (see also Chapter 8 and Appendix 10). 5.2.3 Short-Range Order

Short-range order can be investigated using techniques like X-ray and neutron diffusion, some results being discussed in more detail below. X-ray diffraction was among the ﬁrst techniques allowing for detailed insight into glass structure. It remains a tool of utmost importance allowing for the detection of residual crystallites. Mathematical analysis of the glass response allows extraction of the radial atomic distribution of a given atom as detailed below. Neutron diffraction gives the same information as X-ray diffraction but allows for

5.2 Silica Glass and Related Glasses Tab. 5.2

Experimental tools and associated information.

Experimental tool

Information

X-ray or neutron diffraction IR and Raman spectroscopies, MNR EXAFS X-ray photoelectron spectroscopy (XPS) X-ray reﬂectometry

Radial distribution and/or crystal phase Local symmetry, coordination Local symmetry, radial distribution, coordination Surface arrangement (Section 5.8) Surface arrangement (Section 5.8)

penetrating deeper into specimens. Neutron diffraction requires a nuclear reactor. More recently, extended X-ray absorption edge ﬁne structure (EXAFS) has been extensively used to extract coordination numbers and interatomic spacings. The power of this technique is that by selecting the X-ray energy, the structure around a single kind of atom can be explored rather than getting composite information involving all kinds of atoms as for Xray diffraction. Also, infrared (IR) and Raman spectroscopies (Chapter 8), magnetic nuclear resonance (MNR, including ‘magic angle spinning’ improvements), paramagnetic electronic resonance (PER) and Mo¨ssbauer spectroscopy (Zarzycki, 1982; Williams et al., 1997) are employed to get further insights into local symmetries, coordinations and ion environments. The last two techniques listed in Table 5.2 are very important as regards surfaces. In fact, a glass surface is transformed by water and alkali diffusions depending on the environment and the atmosphere. As a result, glass surfaces may show very different structures and properties as compared to the glass bulk. With the nanotechnology breakthrough, the surface structure and its related properties become of utmost importance and have attracted much scientiﬁc and technological interest. Let us consider X-ray or neutron diffraction. The results of such experiments are usefully presented in terms of a radial distribution where we select an atom at random and consider a series of concentric spheres around it (Fig. 5.6). From the experimental spectra, the radial distribution (RD) can be extracted in the form (Fig. 5.7) RDðrÞdr ¼ 4pr 2 rðrÞdr

ð5:2Þ

where r(r) is the density at distance r. RD(r) corresponds to the probability of ﬁnding a neighbouring atom at the distance r from another atom the position of which is

Fig. 5.6 Schematic glass structure centred on a given atom.

61

62

5 Glass Structure

considered arbitrarily as the reference (r ¼ 0). For a crystal (Chapter 2), the radial distribution would exhibit sharp peaks at periodic distances. Instead in a glass one observes: (i) at small distances diffuse maxima with expected deviation in bond angles and bond lengths, the area under the peak being indicative of the coordination and (ii) at long distances (r ! 1) RD(r) converges to the mean distribution, that is, 4pr2ro, where ro is the average density of the considered glass2). This is indeed observed in Fig. 5.7 since glass RD converges towards a parabolic evolution at long distance with less and less characteristic features being observed. At short distance, RD peaks are observed corresponding to the short-range order of the glass. For instance, in silica (Fig. 5.7a) we observe that silicon atoms are bonded to oxygen atoms at a distance of about 0.16 nm while the distance between two silicon atoms (pertaining to two different tetrahedra) is about 0.32 nm, that is, about twice the previous value, indicating that Si–O–Si lines pﬃﬃﬃﬃﬃﬃﬃare ﬃ not very far from collinear. In between, the O–O band is detected at about 8=3 times the Si–O distance, as expected in a tetrahedral arrangement. After about ﬁve interatomic distances, order almost vanishes, conﬁrming the view that no long-range order prevails in a silica glass. The radial distribution of soda-silica glass shows similar information for Si–O and O–O distances being almost unaffected (Fig. 5.7b). A new peak appears corresponding to the Na–O distance (Jones, 1956). This suggests that the Na ions occupy the free space left in the silica open structure. This view is supported by the fact that the density of silica increases when soda is incorporated, while gas permeability decreases (at least by 5 decades in soda-rich glasses; Jones, 1956; see also Appendix 13). Obviously, we do not suggest that Na+ ions simply ﬁll network holes, for at the same time we must consider a change in the number of silicon and oxygen atoms. The short-range order of the glass will control the density or the atomic packing density Cg of the glass that has an important role in glass properties (elastic modulus, Poisson ratio, glass ﬂow). As for a crystalline structure the atomic packing density Cg is deﬁned as the ratio between the minimum theoretical volume occupied by the ions and the corresponding effective volume of the glass. For a glass of composition AaBb, Cg is written Cg ¼

ava þ bvb ava þ bvb ¼ rN aMA þ bMB a MNA þ b MNB =r

ð5:3aÞ

Here r is the glass density, N the Avogadro number, Mi the molar mass and vi the theoretical ion volume: 4 vi ¼ pri3 3 where ri is the ion radius (Appendix 2). 2)

For a gas of non-interacting point particles (structureless) the curve would be a parabola with its vertical axis and its apex at the origin. The probability of ﬁnding a second atom at a given distance from a ﬁrst one is dependent only on the volume available, and therefore varies with the square of the distance. For a perfectly ordered crystal, it

ð5:3bÞ

consists of a number of vertical lines of inﬁnite height, one at each of the possible interatomic distances (depending on the structure type). A hump above the parabola is indicative of a more than random probability of ﬁnding a second atom within a given range of distances from the chosen atom that is a degree of order.

5.2 Borate Glass and Related Glasses

Fig. 5.7 Radial distribution curves of (a) vitreous silica and (b) Na2O–SiO2 extracted from X-ray diffraction data (according to McMillan, 1979).

Silica glass packing density Cg is 0.45 and is lower than that of standard ﬂoat glass (Cg ¼ 0.52; Rouxel, 2006) both being below that of a crystalline structure where the highest atomic packing density is obtained for a face centred cubic (FCC) structure and is 0.74. As discussed below, metallic glasses show the highest atomic packing density greater than 0.7. The Poisson ratio increases accordingly from 0.2 for silica glass to 0.4 for metallic glasses (Appendix 9). Hence, silica and related glasses show excess volumes that have important consequence on the properties (transport, mechanical; see Chapter 6). Metallic glasses as compared to other glasses show the lowest excess volumes.

63

64

5 Glass Structure

5.3 Borate Glass and Related Glasses

Boron (B) is in group III of the Mendeleev table (Appendix 2) and is a network former with strong Dietzel ﬁeld (Table 5.1). It tends to bond to three different oxygen ions adopting a triangular coordination. Tetrahedral coordination is also found. As regards the three coordinated B atoms, it has been suggested that these form boroxyl groups B3O6. These groups are planar and linked to form a three-dimensional network by boron–oxygen–boron bonds (Fig. 5.8). Such a structure is in good agreement with X-ray diffraction results (Doremus, 1994). Such a structure is then much different from that of silica. When adding alkali metals to borates the induced changes are opposite to those generated in silica; this is called in the literature the ‘boron oxide anomaly’. In fact, the viscosity may increase and the thermal expansion decrease when adding alkali metal, contrary to what is generally observed in silicabased glasses. It is believed that such a trend could be related to a change in the coordination of boron atoms. Borosilicate glasses play an important role in glass manufacturing since they are corrosion resistant to water and allow for low thermal expansion. They are composed of Si and B atoms which form the network, Si being four coordinated and B three coordinated. The resulting network is softer than silica with lower viscosity and lower melting temperature. Contrary to what happens when modiﬁers are introduced in silica, the bond potential remains symmetrical in borosilicates inducing low variation in the mean distances with increasing temperature, that is, a low thermal expansion (see also Appendix 3). In borosilicate glasses, alkali metal ions like Na+ ions will either modify the network introducing NBOs or change the boron coordination (from 3 to 4). The latter phenomenon is believed to be responsible for the ‘boron oxide anomaly’ where viscosity may increase with increasing alkali metal concentration as stated for borate glasses.

Fig. 5.8 Boroxyl groups sharing a common oxygen atom.

5.5 Metallic Glasses

Fig. 5.9 Schematic structure of organic or chalcogenide glasses with chains and cross-linking.

5.4 Organic and Chalcogenide Glasses

Organic glasses are used to produce optical lenses and to protect glass articles (cold-end coatings, ﬁbre sizing; see also Chapters 4 and 12). They are formed by organic chains either cross-linked or not (Fig. 5.9). In thermoplastics only weak bonds (VDW) are formed between chains. In thermosets, cross-linking is obtained when covalent bonds form between the organic chains. The simplest polymer known as polyethylene is formed by long chains made of –CH2– moieties. The length of the carbon–carbon chain depends on the way the polymer is fabricated. Moreover, side group functions can be added to the carbon chains. When cooled from a melt, the polymer will generally present a mixture of very small crystalline regions embedded in a glassy matrix. The crystalline regions consist of oriented chains. Only when quenching is rapid enough, the chains cannot rearrange and a glassy phase is obtained. The chains form a glass three-dimensional network with strong (covalent) and/or weak (VDW) bonding between chains with related properties. Strong cross-links result in higher viscosity regime for instance. Interestingly, chalcogenide glasses can be described in analogy to organic glasses, the term polymerization being sometimes employed in the glass context as well. A chalcogenide glass is formed from group VI and IV atoms (GeSe for instance; Chapter 2, Appendix 2). Group VI atoms form long chains (Se chains for instance) interacting through VDW bonds and cross-linking due to the covalent bonding between the group IV atoms (Ge for instance). Note that Ge can bond four different chains (Guin et al., 2002) inducing strong network stiffness.

5.5 Metallic Glasses

Metallic glasses have been fabricated only recently. Duwez’s team pioneered in the 1960s elevated cooling rates (106 K s1) to fabricate binary glass compositions like AuSi glass (Klement et al., 1960). More recently more complex alloys of 4 to 6 different elements have been produced at much lower cooling rates (1 K s1) offering the possibility of producing larger specimens (so called bulk metallic glasses (BMGs); Johnson, 1996; Inoue, 2000). As a matter of fact, the actual structure of the alloys made with so many elements is complex (Fig. 5.10) as reviewed by Wang et al. (2004) and is still debated (Sheng et al., 2006). These glasses did not yield a technological breakthrough in terms of technological applications, even though they present more

65

66

5 Glass Structure

Fig. 5.10 Different atomic conﬁgurations of three types of BMGs (according to Inoue and Takeuchi 2002).

elevated elastic limit and corrosion resistance than crystalline metals. They have played an important role in the past decades in the study and understanding of glass mechanical properties since they can be plastically deformed as bulk (under compression) well below their glass transition (Appendix 10). This has allowed great insight into plasticity and ﬂow in glass (Chapters 6 and 8 and Appendix 8). BMGs were found to have a new type of glassy structure with a high degree of dense randomly packed atomic conﬁgurations with much smaller excess volume and higher packing density (Cg > 0.7) than in oxide glasses. Density measurements show that the density difference between BMG and the fully crystallized state is in the range 0.3– 1.0 % which is much smaller than the reported range of about 2 % for ordinary amorphous alloys (Wang et al., 2004). This indicates that BMGs have higher density randomly packed atomic conﬁgurations. Inoue classiﬁed the BMGs into three types: metal–metal type, metal–metalloid type and Pd–metalloid type alloys. The conﬁgurations are different according to the three types of BMGs shown in Fig. 5.10. Metal–metal alloys present icosahedral local order which after annealing may yield icosahedral quasicrystalline phase. Some authors have questioned the stability of these glasses during a stay at elevated temperatures when observing superplasticity (Nieh et al., 2002; Appendix 10). Metal–metalloid-type glassy alloys present network atomic conﬁgurations consisting of trigonal prisms which are connected with each other through ‘glue’ atoms comprising Zr, Nb, Ta or lanthanide metal. Pd-based BMGs consist of two large clustered units of a trigonal prism capped with three half-octahedra for the Pd–Ni–P and a tetragonal dodecahedron for the Pd–Cu–P region, as shown in Fig. 5.10.

5.6 Avoiding Crystallization 5.6.1 Nucleation and Growth of Crystallized Phases

As mentioned above, glass forms when a liquid is cooled down in such a way that ‘freezing’ happens instead of crystallization. In fact, the cooling rate must be large enough so that no appreciable amount of crystalline material is formed. It cannot be excluded that some glasses have crystalline regions. This issue is much debated today for metallic glasses (Appendix 10). The detection of crystalline phases is dependent on the

5.6 Avoiding Crystallization

Fig. 5.11 Nucleation n and growth g rates as a function of temperature; note the qualitative graph with arbitrary units (differing for n and g: n(T) is in m3 s1, g(T) in m s1).

tool employed (optical observation, electron microscopy, X-ray diffraction). If some crystals grow in the interior of a glass, the optical properties of the glass for instance will be changed. Light scattering will deleteriously affect the long-distance transmission of an optical ﬁbre for instance. Figure 5.11 shows the nucleation and growth rates which both depend on the temperature. Growth (g) starts at the melting or liquidus temperature TL. Nucleation (n) starts at a lower temperature (T2) resulting from the energy barrier wc that we calculate below. There is no barrier for growth, so it occurs at any undercooling. Hence, crystalline phases may appear in the critical zone situated between T2 and T3. Therefore, glass formation depends on the overlapping of growth (g) and nucleation (n) curves and on their respective kinetics as compared to thermal history (Zarzycki, 1982; Ashby and Jones, 1991). As will be illustrated below the viscous regime at these temperatures plays a very important role and the cooling rate amplitude will determine whether crystallites form or not. Modiﬁers allow for the liquidus temperature to decrease to more viscous domains hence favouring glass formation. The curves shown qualitatively in Fig. 5.11 can be described using a simple analytical approach described below. We shall consider a very simple glass constituted by only one type of atoms. Modelling becomes very difﬁcult in a more realistic case (Fokin et al., 2006). The methods allowing for reliable measurements of nucleation rates are also not straightforward (Doremus, 1994). The physics captured here will help obtain an insight into glass formation. 5.6.2 Nucleation of Crystallized Phases

Crystallite nucleation is controlled by thermodynamics. i. When atoms aggregate, a new surface is created between the emerging crystals and the embedding liquid requiring energy, while phase transformation from liquid to crystal provides energy to the process. We shall deﬁne wc as the energy necessary to form a particle that further develops into a crystallite. Below the critical energy wc, atoms aggregate and later separate. We shall develop in more detail below the expression of this energy barrier in simple conﬁgurations obtained for a monatomic melt in either homogeneous or heterogeneous nucleation regime.

67

68

5 Glass Structure

ii. The former phenomenon (i) will take place if particles can reach the nucleus passing through the diffusion barrier Dg0 . Correspondingly, nucleation rate can be expressed as a function of two terms showing energy barrier wc and diffusion barrier Dg0 respectively: w Dg 0 Nwc DG0 c exp ¼ nvE exp exp nðTÞ ¼ nvE exp kT kT RT RT

ð5:4Þ

where n is the concentration of atoms, vE the atomic transition frequency in the liquid (order of magnitude 1013 s1), T the temperature and N the Avogadro number. The ﬁrst term exp(Nwc/RT) regards the thermal activation related to the energy barrier wc for a particle to form as stated above. The second term exp(DG0/RT) is the diffusion contribution. In the case of a unique atom type, the vicinity of the particle always presents structural units to grow the particle. Therefore, no diffusion on long distances is necessary and the diffusion barrier is that appearing for the viscous ﬂow in the melt (DG0 ¼ DG; Chapter 6). We shall consider now two nucleation conﬁgurations to determine wc. The ﬁrst situation is when nucleation happens homogeneously within the liquid while the second situation (the most realistic one) is when nucleation happens at heterogeneities (at impurities or surfaces; Fig. 5.12).

5.6.2.1 Homogeneous Nucleation Considering ﬁrst the case of homogeneous nucleation, the energy of a particle w is the sum of two contributions: i. the liquid to crystal formation wf ii. the interface energy wi.

These two terms can be expressed as wf ¼

V 4pr 3 DGv ¼ DGv Vm 3Vm

ð5:5aÞ

where r is the particle radius (assumed to be spherical), DGv the molar enthalpy of the transformation from liquid to crystal and Vm the molar volume of the crystal, and wi ¼ 4pr 2 zsl

ð5:5bÞ

where zsl is the surface energy (at the interface between the solid s and the liquid l). Figure 5.12 plots w ¼ wf + wi as a function of particle radius r, and shows a maximum value for a particle radius of rc ¼ 2zsl Vm =DGv

ð5:6aÞ

The maximum energy is then determined to be wc ¼

16pz3sl Vm2 3DG2v

ð5:6bÞ

5.6 Avoiding Crystallization

Fig. 5.12 Schematic (a) homogeneous and (b) heterogeneous nucleation representations. (c) w(r) plot showing rc, wc maximum.

This maximum in energy wc sets a limit on size rc. When an aggregate reaches this critical size, it will develop further. Instead, below this critical size the atoms aggregate and further separate. Let us consider now the Stokes–Einstein relation to express the diffusion term. The diffusion coefﬁcient is written kT DG ð5:7Þ ¼ vE a2o exp D¼ 3pao h RT

69

70

5 Glass Structure

where a0 is the distance of the atomic jump (taken as twice the particle radius) and h the viscosity. Then, we get for the nucleation rate DG Nwc D Nwc exp ¼ n 2 exp nðTÞ ¼ nvE exp RT ao RT RT kT Nwc exp ¼n 3pa3o h RT

ð5:8Þ

We observe that there is balance between the contribution of wc decrease (DGv increases with decreasing temperature, it is zero at TL) and viscosity increase when temperature decreases. This corresponds qualitatively to the plot shown in Fig. 5.11 with an observed maximum between T2 and T4. 5.6.2.2 Heterogeneous Nucleation We consider now a more realistic situation where heterogeneous nucleation originates from solid impurities in the glass melt. Heterogeneous nucleation is to be prevented on forming a glass article. Instead, vitroceramics are fabricated introducing metallic impurities in the glass melt to induce heteronucleation as detailed in Section 5.7. In such a case, nucleation may happen much more easily as we will show below. We shall refer to impurities that help crystallization as catalysers. Let us calculate the energy barrier wc. In the case of heterogeneous nucleation three interfaces have to be considered instead of one. The mechanical equilibrium of a particle on the catalyser is given by the Young Dupre´ equation (Fig. 5.12; see also Chapter 12): zcl ¼ zcs þ zsl cosu

ð5:9Þ

The surface of the particle is the sum of its surface in contact with the liquid Ssl and its surface in contact with the catalyser Scs: S ¼ Ssl þ Scs

ð5:10Þ

with Zu Ssl ¼

2pr sin u0 r du0 ¼ 2pr 2 ð1 cosuÞ

ð5:11Þ

0

Scs ¼ pr 2 sin2 u ¼ pr 2 ð1 cos2 uÞ

ð5:12Þ

while its volume is Zu V¼ 0

pðr sin u0 Þ2 rsinu0 du0 ¼ 2=3pr 3 ð1 3=2cosu þ 1=2cos3 uÞ

ð5:13Þ

5.6 Avoiding Crystallization

Again the energy of the particle is the sum of two contributions (volume wf and surface wi): wf ¼ V=Vm DGv ¼ 2=3pr 3 ð1 3=2cosu þ 1=2cos3 uÞDGv =Vm

ð5:14Þ

and wi ¼ zsl Ssl þ zcs Scs zcl Scs ¼ zsl Ssl þ ðzcs zcl ÞScs

ð5:15aÞ

Substituting the mechanical equilibrium equation allows one to write wi ¼ zsl Ssl ðzsl cos uÞScs ¼ zsl pr 2 ½2ð1 cos uÞ ð1 cos2 uÞcos u ¼ zsl pr 2 ð2 3cos u þ cos3 uÞ

ð5:15bÞ

It follows that w ¼ wi þ wf ¼ ð1 3=2cos u þ 1=2cos3 uÞf2=3pr 3 DGv =Vm þ 2zsl pr 2 g ð5:16Þ

Therefore, the maximum of the function is found for the same critical radius as for homogeneous nucleation: rc ¼ 2zsl Vm =DGv

ð5:17Þ

while wc het ¼ ð1 3=2cos u þ 1=2cos3 uÞwc hom =2 ¼ ð1=2 3=4 cos u þ 1=4 cos3 uÞwc hom

ð5:18Þ

The ratio wc het/wc hom is plotted as a function of angle u in Fig. 5.13 and this ﬁgure illustrates why heterogeneous nucleation has to be carefully considered since even for wetting angles as high as 308 the wc het/wc hom ratio is less than 1 %. Therefore, ‘dangerous’ catalysers are such that they allow wetting of the solid (u ! 0) and a related decrease of the energy barrier enhancing heterogeneous nucleation. It should be noted that for a given volume, heterogeneous nucleation leads to much larger particle radius since the radius ratio is rhet =rhom ¼ ½ð1 3=2cos u þ 1=2cos3 uÞ=21=3

ð5:19Þ

5.6.3 Crystal Growth

The nuclei being formed, they will then grow. Growth rate g can be calculated assuming a thermally activated transfer of atoms from the liquid phase to the solid

71

72

5 Glass Structure

Fig. 5.13 Plot of wc het/wc hom as a function of angle u.

phase and from the solid phase to the liquid phase (Fig. 5.14): gðTÞ ¼ fac ðvls vsl Þ

ð5:20Þ

where f is the fraction of surface site (0 < f < 1), ac the solid–liquid interface thickness and vls and vsl the frequencies for respective transfers (Fig. 5.14). We have DG00 ; vls ¼ vE exp RT

DGv þ DG00 vsl ¼ vE exp RT

ð5:21Þ

with vE the atomic transition frequency in the liquid, T the temperature and DG00 and DGv þ DG00 the respective barriers. DGv is the molar enthalpy of liquid–crystal transformation. One can write DG00 DGv 1 exp gðTÞ ¼ fac vE exp RT RT

ð5:22Þ

The interface transport can be described by a diffusion coefﬁcient. In the general case we do not know the energy barrier for diffusion through the interface. Longdistance diffusion is to be considered. As a ﬁrst approximation and since only one type of atom is considered here, we can suppose the diffusion barrier is the same

5.6 Avoiding Crystallization

Fig. 5.14 Liquid–solid interface modelling. Note we consider only one type of atom and hence the same composition for the liquid and the solid. This is rarely the case (l, liquid; s, solid).

as that appearing in viscous ﬂow, DG00 ¼ DG, and take again the Stokes–Einstein relation D¼

kT DG ¼ vE a2o exp 3pao h RT

and express the growth rate supposing that ac ¼ ao (twice the particle radius) as kT DGv 1 exp gðTÞ ¼ f 2 ao 3ph RT

ð5:23Þ

Note that at T ¼ TL, DGv is null so that g ¼ 0, while DGv amplitude increases when temperature decreases. However, viscosity increases as well and progressively balances the DGv contribution. This also describes well qualitatively the growth (g) curve shown in Fig. 5.12 with a maximum being observed between TL and T3. The role of viscosity in inhibiting nucleation, growth and hence crystallization should be emphasized. This result applies to general glass compositions. In fact, glass formation is made possible using compositions allowing for a viscous regime around the liquidus temperature. In Chapter 6 we shall further discuss the importance of this property when glass is to be frozen in. Regarding crystallization, it is well known that

73

74

5 Glass Structure

adding alkali to silica allows a decrease in viscosity. As a matter of fact, at very high content of alkali, say that corresponding to the composition of orthosilicate, glasses are never obtained since the rates of nucleation and crystallization become too high. Also, devitriﬁcation will depend on the viscosity regime (Section 5.6.5). As mentioned at the beginning of this section, once glass is not composed of a single atom type (which indeed is unrealistic) crystallization becomes complex to model (Fokin et al., 2006). In general the crystalline phase presents a different composition from the original glass, so that glass composition in the surrounding of the growing crystalline phases changes with implication for the viscosity regime. Also, a depleted zone may appear for the elements present at higher stoichiometry in the crystalline phases. 5.6.4 T T T Diagram

The simple monatomic models presented above allow an insight into glass formation even though we made rough approximations. The practical need however is to form a realistic glass without detectable crystalline phases. In this regard temperature– time–transformation (TTT) diagrams have to be elaborated theoretically and experimentally for more complex glass compositions (Fig. 5.15). The TTTdiagram shows in a temperature–time plot the crystalline and glass domains. When forming a glass, the cooling route must, in no case, pass through the crystalline domain (Fig. 5.15). Then the critical cooling rate allowing for the production of glass is that tangent to the ‘nose’ (Tn, tn) of the limiting front: dT Tm Tn ¼ dtc tn

ð5:24Þ

The critical cooling rate is 102–103 K s1 for silica glass while pure metals require cooling rates as high as 106 K s1 (Fig. 5.16). Some metallic alloys (BMGs) can now be formed as bulk glasses at moderate rates (Inoue et al., 1996; Lu et al., 2003; Wang et al., 2004). While pure metals can be produced by melt spinning, alloys can be produced by arc melting and drop casting at cooling rates as low as e1 K s1.

Fig. 5.15 Schematic T T T diagram and one thermal history for producing glass (arrow).

5.6 Avoiding Crystallization

Fig. 5.16 Critical cooling rate for different classes of glass as a function of reduced glass transition temperature Trg = Tg/Tm. (Reprinted from Wang et al., 2004, with permission from Elsevier.)

5.6.5 Devitriﬁcation

Once the glass is formed, the discussion turns to its devitriﬁcation upon a heat treatment. In fact, there have been measurements to determine the rate of growth of crystalline phases in an annealed glass. Once the temperature increases crystal growth may happen whenever the relative nucleation and growth curves overlap or whenever impurities serve as nuclei. Growth rate increases steeply to a maximum and then decreases to zero at liquidus temperature. Such a curve is shown for a silicosoda-lime glass in Fig. 5.17 when the growth of crystals of composition Na2O–3 CaO–6SiO2 called devitrite is observed. This phenomenon is to be avoided when a glass article is heat treated unless a glass–ceramic material is to be formed from a parent glass as detailed in the next section. Addition of a few percent of oxides like

Fig. 5.17 Rate of growth of devitrite in a soda-lime-silica glass (according to Jones, 1956).

75

76

5 Glass Structure

MgO or Al2O3 allows for reducing devitriﬁcation risks in ordinary oxide glasses (window glass). Also, care must be taken regarding preferential sites for nucleation like surfaces, dust, bubbles or inhomogeneities. 5.6.6 Factors That Favour Glass Formation

In view of a number of complex issues it is important to summarize factors that favour glass formation: i. Viscosity is the controlling parameter, and a high-viscosity regime is searchedforatliquidustemperatureandaroundtheTTTdiagram nose. This means low transport and hence small rearrangement rates leading to low rates of nucleation and crystallization. ii. Avoid heterogeneous nucleation. iii. Consider systems with a large crystal–liquid interfacial energy. iv. Consider systems with a large concentration change between the liquid and the crystal phases.

5.7 Vitroceramic Fabrication 5.7.1 Introduction

Glass–ceramics are ﬁne-grained polycrystalline materials formed when glasses of suitable compositions are heat treated and thus undergo controlled crystallization. The parent glasses have speciﬁc compositions comprising precursors as detailed below. Indeed, ordinary window glass is too stable and difﬁcult to crystallize, whereas other compositions crystallize in an uncontrolled manner resulting in undesirable microstructures. Usually, a glass–ceramic is not fully crystalline; typically the microstructure is 50–95 vol.% crystalline with the balance volume being the residual glass. One or more crystalline phases may form during the heat treatment and as their composition is normally different from the parent glass, it follows that the composition of the residual glass is also different from that of the parent glass. The mechanical properties of glass–ceramics are superior to those of the parent glass. Vitroceramics are fabricated for ﬁre resistance (cooking tops and containers; refer to Eurokera activity, Saint Gobain group and Corning ware) since the combination of crystalline and vitreous states allows for a lower thermal expansion and a higher strength. For astronomy, Zerodur (Schott) has allowed the fabrication of an 8.2 m telescope based in Chile with thermal expansion as low as 107 8C1. Surprisingly, only recently have such materials been produced. It must be said that while glasses tend to devitrify, the control of such a phenomenon is very difﬁcult and was reported only by 1950. In fact, it requires well-controlled thermal treatments in view of nucleation and growing curves (Fig. 5.18) and the use of nucleation agents.

5.7 Vitroceramic Fabrication

Fig. 5.18 Two-stage heat treatment for a system showing negligible overlap of nucleation and growing curves (according to Rawlings et al., 2006).

5.7.2 Conventional Method (two stages)

The conventional method for producing a glass–ceramic is to devitrify the parent glass by a two-stage heat treatment (Fig. 5.18). The ﬁrst stage is a low-temperature (TN) heat treatment that gives a high nucleation rate thus forming a high density of nuclei throughout the interior of the glass (Rawlings et al., 2006). A high density of nuclei is important since it leads to a desirable microstructure consisting of a large number of small crystals. The second stage is a higher temperature (TG) heat treatment to produce growth of the nuclei. The achievement of such a microstructure is helped by nucleation agents that can be metallic (Au, Cu, Ag, Pt, Pd) or non-metallic (TiO2, P2O5 and ﬂuorides). These aggregate and subsequently induce controlled ceramic nucleation. Designed crystals embedded into the glass matrix are then formed. 5.7.3 Modiﬁed Conventional Method (single stage)

The reason for the two-stage heat treatment of the glass is a consequence of the limited overlap between nucleation and growth rate curves. If, on the contrary, there is extensive overlap of the rate curves then nucleation and growth can take place during a single-stage heat treatment at temperature TNG (Fig. 5.19). The rate curves and particularly the nucleation curve are sensitive to composition, and hence optimizing the glass composition (choice of nucleating agents) is in some cases possible to obtain the necessary overlap. 5.7.4 Laser-Induced Method

For some years now, glass to ceramic transformation could be conﬁned using a focused laser beam. This allows for patterning a glass object in three dimensions

77

78

5 Glass Structure

Fig. 5.19 Single-stage heat treatment for a system showing overlap of nucleation and growing curves (according to Rawlings et al., 2006).

(Lehmann, 2005). The nature of the local transformation (cavity, crystallite, composition change) is however still under debate.

5.8 Glass Surface

The ﬁrst approach to study a glass surface is to start from the bulk structure and move towards the surface. The presence of the surface allows for the interaction of glass with the atmosphere. Surface structure is changed by the physical and chemical interactions. Koike and Tomozawa (2006) report that surface structural relaxation takes place more rapidly than bulk structural relaxation in particular in the presence of water diffusion (see also Chapter 6). Gas molecules penetrate the glass network through its excess volume and may react with the glass. We know that the bulk glass structure is not unique but depends on modiﬁer concentration and network formers. We shall consider here mainly silica and suppose it is modiﬁed by alkali (Naþ) knowing that variations are expected for more complex compositions. 5.8.1 Surface Reaction

When silica cools down its surface reacts with water molecules to form silanol bonds (Fig. 5.20). The reaction can be written as SiOSi þ H2 O ! SiOH þ HOSi

ð5:25Þ

The reaction energy is elevated and around 80 kJ mol1. The water reaction leads to a high density of silanol groups that can reach 4.6 sites per nm2 (Bather and Gray, 1976). According to the proximity to other silanol groups, hydrogen bonding will be possible. Also, the silanol groups may react with water without dissociation of the water molecules. This reaction is referred to as water physisorption. The glass surface may

5.8 Glass Surface

Fig. 5.20 Representation of the hydration of a silica surface.

hence be covered by several monolayers of water depending on the water partial pressure in the atmosphere. Not only water but also organic pollutants may adsorb. It should be noted that although an annealing treatment at 100 8C allows the desorption of water molecules, a treatment at a much higher temperature is necessary to form again siloxane groups (reversing reaction 5.25). 5.8.2 Molecular Diffusion

Molecules diffuse through the glass network. This phenomenon follows diffusion laws (Appendix 13). The smaller the molecule size the more important the diffusion. Diffusion of rare gases (He, Ne, Ar) and molecules (H2, O2, H2O) has been documented3) for different compositions of glasses (Doremus, 1994) and allows for tailoring glass permeability. Importantly, some of these molecules once in the glass may react and change glass properties and behaviour (viscosity, electrical conductivity). The role of the water reaction is discussed in more detail below. 5.8.3 Glass Network Interaction with Water

In fact, water interaction is not conﬁned to the surface (Section 5.8.1) because of water diffusion through the glass excess volume (Appendix 13). Moreover, when we consider a glass with modiﬁers, non-bridging oxygen (NBO) atoms appear so that they open the network while mobile ions (alkaline ions) will diffuse. The deleterious role of alkali can be limited by introducing alumina and/or B2O3 in the glass melt. The elevated resistance of natural glasses over millions of years is to be attributed to their aluminosilicate-rich compositions while borosilicate glasses are used for 3)

Brown and Kobayashi (1998) entitled one of their papers ‘Is your glass full of water?’ Water concentration in commercial silicate glasses is in the range 0.01–0.1 wt%.

79

80

5 Glass Structure

pharmaceutical packaging (Chapters 3 and 4). In sodium-rich glass, Na+/H3O+ interdiffusion promotes water interaction within the network and can be followed eventually by corrosion of the network depending on the alkalinity of the solution (pH) at the glass surface4). 5.8.3.1 Water Reaction Water is present in the glass excess volume. Let us consider ﬁrst silica. Water reacts with the silicon–oxygen bonds as already discussed for the surface as follows: SiOSi þ H2 O ! SiOH þ HOSi

ð5:26Þ

This reaction is of utmost importance in glass mechanics since it is enhanced at crack tips and is responsible for the fatigue of glass (Chapter 9). The reaction is enhanced as water concentration is increased. 5.8.3.2 Ion Exchange Let us consider an alkali-modiﬁed silica glass. Because of mobile modiﬁers, the glass will undergo ion exchange, alkali being leached. Let us consider for instance sodium. Water diffusion (in fact H3O+) into the glass network is as follows: SiO Naþ þ H3 Oþ ! SiOH þ H2 O þ Naþ

ð5:27Þ

The superﬁcial glass loses sodium ions (glass leaching) while it incorporates water (it may also affect other mobile modiﬁers). This happens for external glazing or when in contact with water. The formation of a silica gel at a glass surface can be described by Fick’s law (Appendix 13), the typical thickness of the gel layer being about 0.1 mm.

Fig. 5.21 In vitro degradation of a glass ﬁbre. (Courtesy ´ Henri Hermine Dika, Pr Bertrand Rihn, Universite ´, Nancy 1, France.) Poincare

4)

pH ¼ log½H3 Oþ ¼ log Ke log½OH ; ¼ pKe log½OH ; pKe ¼ 14 where the square brackets indicate the

5.8 Glass Surface Surface energy (glass–water vapour) and wetting angle according to the type of surface (after Chartier, 1997).

Tab. 5.3

Native glass surface ‘Clean’ glass surface Polluted glass surface

Surface energy, z (mJ m2)

Water contact angle (8)

400–1000 70 20–40

– 0 20–60

Such a layer can be detected by X-ray reﬂectometry (Table 5.1) because glass subsurface presents different properties as compared to the bulk. Also the hydrated glass surface exhibits lower resistance to contact loading (Chapter 8, Appendix 10) and this is beneﬁcial when abrading the glass edges. 5.8.3.3 Glass Corrosion Na+ diffusion towards a glass surface increases the alkalinity (pH) of the aqueous solution in contact with the glass. When pH reaches 9 then siloxane bonds may react with hydroxide ions as follows: SiOSi þ OH ! SiOH þ O Si

ð5:28Þ

Such a pH value is achieved when the glass remains in the same humid and conﬁned environment as for stored glass panels and glass wool. As matter of fact, it may happen that glass products are damaged by corrosion. This is limited when storing glass panels using acidic paper in between. This phenomenon is well known to glass manufacturers and can be tailored using Na2O, K2O, CaOrich glasses to enhance it or using Al2O3, B2O3, ZrO2, TiO2rich glasses to limit it (these oxides act as barriers). The development of bioglass (biodegradable ﬁbres in particular) is a further illustration of tailored glass chemical resistance. These have been motivated by the asbestos scare (Fig 5.21). Nowadays, environmentally safe ﬁbres can be produced so that their half-life is less than 40 days in lungs. For the conﬁnement of complex and dangerous wastes from the biosphere, glasses resisting water corrosion are needed (see also Chapter 3). Aluminoborosilicates are being developed to achieve glass loss of less 0.1 % over 100 centuries. 5.8.4 Surface Properties

It should be noted that all reactions described in Section 5.8 change dramatically surface properties, in particular the surface energy (Table 5.3). The complex glass surface can ﬁnally be schematized as: glass bulk/hydrated glass/water/pollution. Functionalizing the surface of glass supposes it is ﬁrst cleaned up; it can also be treated (Chapter 12).

81

83

6 Glass Rheology 6.1 Viscosity 6.1.1 Viscosity and Process

One of the most important properties from a glass process point of view is the viscosity, which changes dramatically as the temperature changes. Viscosity determines the melting conditions, the temperature regimes for forming, annealing and tempering, and the maximum temperature to avoid devitriﬁcation. Moreover, glass quality is dependent on the way it is homogenized and this is also related to the viscosity regimes. Viscosity measures the resistance of a viscous liquid to shear deformation. The higher the viscosity, the higher the resistance to ﬂow. Consider a liquid between two planes (surface S) and apply a tangential force F to the upper plane (Fig. 6.1). For a solid (inﬁnite viscosity) no ﬂow will occur. On the contrary, a viscous liquid will ﬂow. A velocity gradient will appear in the liquid. If we assume that there is no relative displacement between the plate and the liquid, then velocity varies from zero at the bottom plate to the velocity of the upper plane at distance a (Fig. 6.1). Velocity gradient is then determined as 5v ¼ (v 0)/a and increases when the force F or shear stress (t ¼ F/S) applied to the upper plate increases. The relationship between the velocity gradient and the shear stress is written t ¼ F=S ¼ hrn

ð6:1aÞ

where h is the viscosity in Pa s. An industrial process can be considered according to its velocity gradient (Table 6.1) and one can observe huge differences between these. Equation (6.1a) means that the viscosity regime (temperature, as discussed below) has to be carefully controlled when forming the glass according to the different processes. Also, it is of utmost importance to prepare the glass under uniform temperature. This operation is referred as ﬁning (Chapter 10). Viscosity controls the quality and the homogenization of the glass. During this step, the elimination of bubbles also depends on the viscosity (Chapter 10, Appendix 4). Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

84

6 Glass Rheology

Fig. 6.1 Shear ﬂow in a viscous liquid. Tab. 6.1

Processes and associated ranges of velocity gradient.

Process

Velocity gradient 5v (s1)

Moulding Extrusion Wire drawing

0.1–10 102–103 104–106

The related stresses to be applied by the tools will depend strongly on viscosity regime. From a mechanical point of view (Appendix 9) it is of interest to rewrite Eq. (6.1a) in terms of shear strain. Such an equation shows the time dependence of shear stress t as a function shear strain g.1) t ¼ hrv ¼ hg

ð6:1bÞ

This behaviour is completely different from that of an elastic solid that shows no time dependence (Appendix 9). In fact in the elastic regime shear stress is proportional to shear strain, t ¼ Gg, where G is the shear modulus. Therefore, while an elastic solid shows a response to stress independent of time, a viscous liquid shows a response that depends not only on stress amplitude but also on time. Hence, the control of the tools for a process involving viscous liquids requires the control of viscosity regime, stress amplitude and loading time. Glassmakers have set several important temperatures that deﬁne ranges of viscosity that are important from a process point of view. These temperatures are listed in Table 6.2. In fact, viscosity depends strongly on the temperature as shown in Fig. 6.2 and process temperatures are set relative to the deﬁned reference temperatures. This will be discussed in detail in Section 6.1.3. Composition also may change the viscosity 1)

An ideal Newtonian flow is assumed here with a viscosity independent of strain rate. The plot of () is linear. This hypothesis is true at elevated temperature and under low stresses. Instead, non-Newtonian flow (viscosity depending on strain rate) is reported at intermediate temperature closer to Tg and for high strain rates (Simmons et al., 1988) yielding more difficulty in the control of tools. A drastic decrease of viscosity is observed with increasing strain rate. So called rheofluidification may be advantageous

from a process point of view if one considers the required stress. For a non-Newtonian flow, the stress-strain relationship is ¼ ðÞ with a viscosity depending on shear strain rate . It can be approximated by ¼ m, where m is the strain-rate sensitivity exponent (m < 1), similar to that used to describe metal plasticity and it is pointed out that non-Newtonian regime allows for prevention of ‘necking’ (Jones, 1956). The apparent viscosity is = ¼ m1 (Appendix 10).

6.1 Viscosity Tab. 6.2 Reference temperatures and viscosity regime8). Practical melting temperature is not the melting temperature associated with the crystal–liquid phase transition (Chapter 5) but the working temperature.

Reference temperature

Viscosity (Pa s)

Practical melting temperature Working point Littleton softening point Annealing point Glass transition Strain point

1–10 103 106.6 1012 1012–1012.5 1013.5

Fig. 6.2 Viscosity variations with temperature and composition (SLS, soda-lime-silica glass; ALS, aluminosilicate glass; according to Zarzycki, 1982).

drastically. Modiﬁers (Chapter 5) are introduced into the melt to reduce the working temperatures and hence increase industrial yields saving costs in processing. In fact, the same viscosity regime (horizontal line in Fig. 6.2) is obtained for increasing temperatures as glass is changed from lead glass, soda-lime-silica (SLS) glass, borosilicate glass and ﬁnally pure silica. Modiﬁers lead to the formation of nonbridging oxygens and allow viscous ﬂow to occur at much lower temperatures in SLS glasses than in silica (Chapter 5). The ALS glass curve crosses the other with a higher transition temperature than SLS (see also Section 6.7). 2)

For comparison we list the viscosity (in mPa s) of common materials: hydrogen, 0.0086; gas, 0.01–0.02; water, 1; kerosene, 10; oil, 100; honey, yogurt, 103–106; glue, paint, resin, 102–107; asphalt, 105–108.

85

86

6 Glass Rheology

To optimize production tools and processing, it is of utmost importance to fabricate a glass with homogeneous temperature and composition or in other words homogeneous viscosity. In fact, the temperature of the glass delivered from the melting furnace and its composition have to be regulated with extreme care. From the control or R&D perspectives, it is necessary to determine carefully and precisely the viscosity as a function of both temperature and composition. This is not straightforward since viscosity varies in a wide range and instruments have been developed accordingly. Interestingly, such measurements revealed that in limited domains empirical relations exist between the compositions and the properties of glass (Priven, 2004). The optimization of the composition for processing can then be made using these empirical laws to deﬁne a range of compositions likely to yield a glass with the required properties (see also Chapter 2). Nonetheless, one also has to take into account the complex shape of the produced article as well as its complex thermomechanical loading. This can be achieved again for R&D purposes using numerical modelling to consider the properties of the material and its loading at each point of the specimen (Appendix 11). 6.1.2 Viscosity Measurement

Different instruments have been designed according to viscosity ranges (Table 6.3), and the overall viscosity curve is obtained using complementary techniques. We shall describe some of these – rotating cylinder and ﬁbre elongation viscometers – allowing for low (10–103 Pa s) and high (106–1013 Pa s) viscosity measurement respectively. At intermediate temperatures, crystallization may interfere with the measurements and caution should be taken with the resulting data. Viscosity experiments can be divided in several ways: whether they are strain-rate controlled (resultant stress being measured, e.g. concentric cylinders) or stress controlled (resultant strain rate being measured, e.g. ﬁbre elongation), whether they involve pure shear (e.g. concentric cylinders) or a combination of shear and volume stress (beam bending, ﬁbre elongation). Usually the viscometer is calibrated with a liquid of known viscosity; absolute measurements can be made with care. Tab. 6.3

Measurement methods for viscosity.

Range

Method

Viscosity value, h (Pa s)

Melting

Falling sphere/bubble rise Rotational methods (concentric cylinders, cone-and-plate) Parallel plate

Tg) can be ﬁtted empirically by the Vogel–Fulcher–Tammann (VFT; see Section 6.1.3.3) formula that captures relatively well the non-Arrhenius temperature dependence over the meltforming region. The reason for observing either strong or fragile behaviour has been widely debated. It is believed that fragile liquids lack intermediate-range order; some theoretical backgrounds are developed in Sections 6.1.3.2 and 6.1.3.4. We may still use an Arrhenius temperature dependence when considering limited domains of temperatures and we adopted this procedure in Chapter 5. Instead, when variations over a large range of temperatures are to be predicted for fragile glass, nonArrhenius temperature dependence is to be taken into account in order to get suitable predictions of glass behaviour. At temperatures below Tg (Fig. 6.6) the viscosity curve is still unknown and debated. In fact the question mark is shown on Fig. 6.6 to indicate the domain where viscosity is uncertain. Above 1015 Pa s viscosity values should be considered with great care. As plotted in Fig. 6.6, the curve suggests that the rate of increase of viscosity with decreasing temperature becomes greatly reduced. There is a qualitative explanation for such an expected behaviour since the glass below Tg is frozen in a liquid-like structure the conﬁguration of which corresponds roughly to that in equilibrium near the glass transition temperature (see also ﬁctive temperature in Section 6.5.3). Hence glass structure is not at equilibrium. Further consideration of the related viscosity at these temperatures is necessary from the experimental point of view. Indeed, the apparent viscosity commonly measured using penetration viscosimetry is non-Newtonian at these low temperatures and therefore strain rate dependent (Appendix 10). Moreover, the measured deformation is not purely viscous because of delayed elasticity, as stated above and detailed in Section 6.4.4. Hence, it is not possible to measure the equilibrium viscosity at these temperatures. This fact may account for the huge discrepancy in viscosity values published in the literature since apparent viscosity depends on stress and strain rate amplitude, or on experimental conditions. The ﬁnding is that the apparent viscosity decreases under these conditions.2)

2)

There exists a very broad range of values in the literature. For instance, Frischat (1987) reports a 1020 Pa s value while Macosco (1994) reports 1040 Pa s. These values would correspond to relaxation time (refer to precise definition below) from 109 s (30 years) to 1029 s. These discrepancies yielded sometimes controversy in the observed geometry of stained glasses in cathedrals. In fact, it has been observed that cathedral windows are wavy and thicker at the bottom. Would glass have flowed when standing in place for some hundreds of years? There have been speculations on this subject. In fact, when measuring viscosity at low temperature elevated stresses are to be applied to the specimens. Under such conditions the apparent viscosity

is expected to decrease with the amplitude of stress and strain rate (Appendix 10). Discrepancies are then expected between authors as the Newtonian viscosity is not determined. On the other hand, it would be problematic extrapolating high-temperature data (in particular in the case of a fragile melt). It is not possible to predict glass flow under moderate stress. On the other hand, undeformed glass vases (>2000 years old) have been discovered, while natural glasses maintain their structure. In fact, medieval windows could have been blown and subsequently flattened manually and non-uniformly (Chapter 3); then architects would have put the thicker part at the bottom (see also Chapter 12).

6.1 Viscosity

6.1.3.2 Fragility Transition temperature is of great importance as well as the properties changes in the melt-forming region. Observation of a viscosity curve on a log h 1/T diagram indicates that indeed the behaviour depends dramatically on the type of glass, with greater curvature being observed for fragile glasses. A strong glass has then a larger viscosity than a fragile glass on approaching Tg. It is quite helpful to employ a unique temperature scale for all glasses using the transition temperature to temperature ratio as the x-axis (Fig. 6.7). On such a graph all glass responses meet at a common point corresponding to the glass transition at a viscosity of 1012–1012.5 Pa s and Tg/T ratio equal to 1. In such a graph, the glass behaviour is nothing but unique and really composition dependent. The question is why we observe such different behaviours (Doremus, 1994, 2003; Angels, 1995; Kieffer, 2002; Novikov and Sokolov, 2004; Tanaka, 2005). In fact, while the nature of the transformation by which a supercooled liquid ‘freezes’ to a glass has been the subject of intense investigations and substantial progress has been made in understanding this phenomenon over the past two decades, yet many key questions remain. In particular, the factors that control the temperature-dependent relaxation and viscous properties of the liquid phase as the glass transition is approached, that is, whether the glass-forming liquid is ‘fragile’ or ‘strong’, remain unclear (Angels, 1995).3) The fragility of liquids characterizes the deviation from Arrhenius behaviour or the curvature from a straight evolution (expected from Eyring theory; see Section 6.1.3.4; Fig. 6.2 or Fig. 6.7 replotted with respect to transition temperature). Silica shows strong or almost Arrhenius behaviour since a linear variation is observed for all temperatures (Fig. 6.7). In contrast metal ﬂuoride glasses show important deviations from such an Arrhenius behaviour. Fragility can be numerically deﬁned as the apparent activation energy of shear viscosity h at the glass transition temperature Tg, normalized to Tg (Angels, 1995): m¼

qlogh qðTg =TÞT¼Tg

ð6:12Þ

Hence, m characterizes the steepness of the slope of the log h dependence on Tg/T near Tg. A stronger deviation (larger m) from Arrhenius behaviour corresponds to a more fragile system. As mentioned above, Fig. 6.7 shows that fragility depends on the material. Silica demonstrates Arrhenius behaviour over the logarithm of viscosity range from 1 to 13, whereas fragile glasses demonstrate an almost continuously changing slope, or one that can be approximated by two straight lines (one at elevated temperature and another at the transition). Strong behaviour is controlled by continuous Si–O–Si bonding as in silica while the break-up of this bonding controls

3)

The belief that a glass is a supercooled liquid in which atomic motions have slowed to the extent that characteristic relaxation time exceeds the observation period (thousand years for stained medieval windows) is debated and the possibility that glass

corresponds to a different physical state from the liquid is considered. This suggests that glass would require an independent set of parameters and this is not done yet in engineering or scientific calculations (Kieffer, 2002).

93

94

6 Glass Rheology

network modiﬁed glasses. Hence, alkali silicates are less resistant to thermal degradation and could ﬂow within alkali-rich regions (Chapter 5). Empirical formulas have been proposed to correct for the deviation from non-Arrhenius temperature dependence (Section 6.1.3.3). The most well known is the VFTempirical law, which is extensively employed in research and industry. 6.1.3.3 VFT Empirical Formula A supercooled fragile liquid shows a viscosity that can be approximated by the VFT (Vogel–Fulcher–Tammann) formula hðTÞ ¼ ho exp

B T To

ð6:13Þ

where B and ho are temperature-independent coefﬁcients. This law can be considered as a correction of the Arrhenius law adding a To term. In fact, taking To ¼ 0 K or assuming T To transforms the VFT formula into an Arrhenius temperature dependence. The VFTapproximation is still easy to use and allows for close prediction of the actual viscosity. It is an empirical law that allows one to capture the curvature of the experimental ln(h) 1/T curves. As will be discussed in detail below, different approaches have been proposed to model the actual behaviour represented by the VFT empirical law; these are complex and still matters of debate. In accordance with the VFT equation above, the viscosity of a glass will be inﬁnite at To or below Tg (no mobility). This is unlikely to be correct (Section 6.1.3.1, Appendix 10). For a silicosoda-lime glass for instance, the VFT parameters are determined to be B ¼ 4320 K, To ¼ 542 K and ln ho ¼ 2.77 (Guillemet and Gy, 1996). 6.1.3.4 Microscopic Approach Eyring theory for molecular mobility supposes that the movement of each molecule (or structural unity) is thermally activated (Fig. 6.8). Given a barrier energy Dg, the jump frequency is written Dg DG ¼ nE exp nE exp kT RT

ð6:14Þ

where nE is the atomic transition frequency in the liquid (order of magnitude 1013 s1; Einstein frequency). The applied force or shear stress t modiﬁes the barriers as shown in Fig. 6.8c (Douglas, 1958), ﬂow being biased so that the probability of a forward jump (supported by the shear stress) is higher than for the backward jump (against stress). The jump frequency along the direction of ﬂow nþ and in the opposite direction n is written Dg tV=2 nþ ¼ nE exp kT

ð6:15Þ

6.1 Viscosity

Fig. 6.8 Representation of an individual atomic jump: the basic step for macroscopic diffusion and ﬂow.

Dg þ tV=2 n ¼ nE exp kT

ð6:16Þ

where V is the atomic volume. The effective jump frequency is written Dg tV=2 tV=2 exp exp n ¼ nþ n ¼ nE exp kT kT kT Dg tV sinh ¼ 2nE exp kT 2kT

ð6:17Þ

95

96

6 Glass Rheology

When all the atoms in a specimen make one jump ao (assuming ao ¼ 2r, where r is the atom radius) in the direction of shear, macroscopic shear strain g ¼ 1. Shear strain rate is then written Dg tV sinh g ¼ 2nE exp kT 2kT

ð6:18Þ

and for a low applied stress, the strain rate is written (since sinh(x) ! x for x ! 0) g¼

tV Dg nE exp kT kT

ð6:19Þ

We note that Newtonian ﬂow (t g) is obtained under these conditions and that the viscosity is written kT Dg h¼ exp VnE kT Dg DG h ¼ ho exp ¼ ho exp kT RT

ð6:20Þ ð6:21Þ

with ho ¼ kT/VnE. Temperature dependence of ho is often neglected, in the present framework it is determined to be linearly dependent on T, and hence ho varies usually far less than an exponential term (see also Appendix 13). On cooling the liquid, ﬂow becomes impossible because of unavailable free volume for atomic jump. The main theories accounting for this phenomenon are the free-volume model (Cohen and Turnbull, 1959; Turnbull and Cohen, 1961) and the conﬁgurational entropy model (Adams and Gibbs, 1965). Free-volume models follow the idea that on cooling the supercooled liquid, free volume progressively reduces,4) and hence mobility becomes impossible. The mobility of an atom (or more generally a structural unit) is supposed to be possible only when a free volume which can contain the atom exists next to it. We shall consider in the following the average free volume per atom. Let us call v the minimum volume of a cavity that can contain the atom or the mobile structural unit. Diffusion of the atom will depend on the free volume size vf per atom. Hence either ðiÞ nf < n

ð6:22Þ

and there is no diffusion of the atom, or ðiiÞ nf > n

and there is diffusion of the atom. 4)

Density fluctuation can be revealed using SAXS techniques (Levelut et al., 2002) and is observed to depend on temperature and thermal history.

ð6:23Þ

6.1 Viscosity

The probability of ﬁnding an atom with a free volume next to it of size between v and v þ dv is given by (Cohen and Turnbull, 1959) a v dv ð6:24Þ exp a vf vf where a is a geometrical factor between 12 and 1. The probability that the atom is on a potential jump site is then Z1 v

a v v exp a dv ¼ exp a vf vf vf

ð6:25Þ

To obtain the shear strain rate one has to consider that only potential sites for jump contribute and hence v tV sinh g ¼ 2nE exp a 2kT vf

ð6:26Þ

Again, for low applied stresses, we still obtain Newtonian ﬂow (t g): g¼

tV v nE exp a kT vf

ð6:27Þ

while viscosity no longer shows Arrhenius behaviour but instead is written in a WLF form (Williams et al., 1955; Ferry, 1970): v h ¼ ho exp a vf

ð6:28Þ

Cohen and Turnbull 1959 further suggested that the free volume can be obtained from thermal expansion coefﬁcients of the amorphous and liquid phases (above the glass transition temperature). Calling the difference in coefﬁcients of thermal expansion Da ¼ al as between the liquid and glass (see also Section 6.2) they wrote vf ¼ 0 for T < Tg

ð6:29aÞ

vf ¼ vm aðT To Þ for T > Tg

ð6:29bÞ

Also, pressure dependence can also be incorporated. We obtain v v 1 av =vm Da ¼ ho exp a ¼ ho exp ð6:30Þ hðTÞ ¼ ho exp a T To vf vm Da T To

This expression is similar to the VFT empirical expression found for viscosity. As the temperature is lowered, the (T To) term causes curvature below Arrhenius

97

98

6 Glass Rheology

behaviour (so-called fragility). However, if To ¼ Tg then the curvature is too large and To ¼ Tg DT must be used with DT 20–50 8C. Note this model predicts too large a viscosity curvature near Tg and ignores conﬁgurational arrangements. Macedo and Litovitz 1965 argued that the free volume model neglects the activation energy required for making a diffusive jump. Thus they developed a hybrid equation that combines the free volume term with the Eyring term (see also Appendix 10): v Dg hðTÞ ¼ ho exp a þ vf kT

ð6:31Þ

Then the Arrhenius temperature dependence of the viscosity can occur if either of the following facts are true: (i) the material is a low-expanding one such as fused silica; (ii) free volume is proportional to temperature. In the liquid where a

v Dg kT vf

the viscosity reduces to a WLF-type equation further simpliﬁed into the VFT formula assuming Eq. (6.28b). The Macedo and Litovitz 1965 approach ﬁxed one of the problems of the free volume model in that it exhibits Arrhenius viscosity for ﬂow under constant free volume conditions (isostructural). Also, some of the free volume model limitations have been addressed by the conﬁgurational entropy model where it is postulated that rearrangement of the structure happens when a region containing at least two structural conﬁgurational states is available. It is logical to consider the motion as a cooperative process involving a simultaneous rearrangement of a large number of atoms or units. The Adam–Gibbs 1965 model is based on the idea that motion occurs by internal cooperative rearrangement of independent regions of n atoms (Avramov, 2005). When the temperature decreases, the motion of one atom disturbs an increasingly larger number n of its neighbours, or one can say the coherence length of an atom or a molecular motion increases. The Adam and Gibbs 1965 model assumed that the barrier for rearrangement is proportional to n, and determined the temperature dependence of n in terms of the conﬁgurational entropy Sc. Finally, viscosity is written hðTÞ ¼ ho exp

C TSc

ð6:32Þ

where C and ho are temperature-independent coefﬁcients and the conﬁgurational entropy Sc is written Sc ¼ DCp

T To T

ð6:33Þ

where DCp is the variation of molar speciﬁc heat between the liquid and the glass, To being the temperature at which conﬁgurational entropy becomes null which plays

6.2 Glass Transition and Its Observation

the same role here as that corresponding to the vanishing of free volume. These equations combine into hðTÞ ¼ ho exp

C=DCp C ¼ ho exp TS T To

ð6:34Þ

showing the same form as the VFT empirical equation.

6.2 Glass Transition and Its Observation 6.2.1 ‘Observing’ the Glass Transition

As mentioned above, the occurrence of glass depends on the cooling history followed by the viscous liquid. Figure 6.9 shows the volume of a specimen as a function of temperature on cooling (we shall see that heating and cooling curves differ because of structural relaxation; Section 6.5.4). In Figure 6.9, l, g and c correspond to the liquid, glass and crystal respectively. Let us start from the liquid at elevated temperatures (high-temperature end of the diagram). On decreasing the temperature, the liquid contracts ﬁrst. Whenever the cooling rate is too low, then nucleation and growth of crystallites happen as discussed in Chapter 5. Crystals form at the melting or liquidus temperature (TL ¼Tm) and a discontinuity in the volume V of the specimen is observed. The cooling rate may be high enough so that the melting temperature is passed without volume discontinuity, the liquid being then supercooled. Next, the supercooled liquid freezes into glass at the transition temperature with less volume

Fig. 6.9 Volume–temperature cooling curves. Note the discontinuity at melting or liquidus temperature (TL = Tm) when crystals form while liquid to glass path is continuous with lower contraction being observed once the glass transition is passed.

99

100

6 Glass Rheology Tab. 6.4

Transition temperature ranges.

Glass

Transition temperature (K)

Silica Soda-lime-silica Metallic Chalcogenide

1500–1600 800–850 550–700 300–600

contraction observed. This is called transition instead of transformation since the path is continuous. It is signiﬁcant that the viscosity does not show an abrupt change at the glass transition temperature (Section 6.1). This suggests that the viscosity determines the rate at which a property (here the volume) relaxes to some equilibrium value. The presence of the glass transition results from the slowing down of viscous relaxation in the liquid. At a viscosity of 1012 Pa s the relaxation time is in the range of minutes to a few hours, corresponding to usual times of experiments. Changes at glass transition allow for transition temperature determination as detailed in Fig. 6.9. Glass structure and hence its density and volume will depend on the cooling rate. When the cooling rate increases freezing happens at a higher temperature. In fact, less time is allowed for atomic rearrangement and a ‘higher temperature’ conﬁguration is frozen in. Let us consider two glasses (g1, g2) cooled at different rates. On cooling down more slowly, further atom arrangements are made possible and hence a denser structure is obtained. Therefore, the glass volume and transition temperature of glass g2 are lower than those of glass g1. The glass transition temperature is then not unique but instead an interval should be considered. Table 6.4 lists representative values for common glasses. Glass transition temperature can be determined experimentally using dilatometry or calorimetry as detailed in Sections 6.2.2 and 6.2.3. Now consider a supercooled liquid that can be cooled inﬁnitely slowly. The volume curve followed would be that of the liquid with enough time for a denser structure to organize. The resulting glass (we suppose no crystals appear) would show denser structure (less entropy).5) Hence, glasses formed under realistic conditions are expected to be unstable and driven towards a denser and stabilized conﬁguration whenever they are held at temperatures where atomic rearrangements become nonnegligible. This structural relaxation is discussed in Section 6.5.4. Another important feature is that glass will show a lower density than the crystal (see also Chapter 5). As a matter of fact, glass contains excess volume ve , a part of which called free volume vf ¼ ve vo appears to play an important role in glass mechanics (see Section 6.1.3.4; Turnbull and Cohen, 1961).

4)

Glass entropy value at 0 K is still an open question. Residual entropy of glassy states plays against the third law of thermodynamics that suggests it is zero. As temperature decreases more and more time is required for the liquid to be at equilibrium.

The question arises as to what would be the structure of the equilibrium perfectly ordered liquid at zero entropy. If crystalline, it would then suggest that there is a continuous change from the amorphous to the crystalline state.

6.2 Glass Transition and Its Observation

6.2.2 Dilatometry

A dilatometer allows for the continuous measurement of the length of a given specimen which increases continuously with temperature at a constant heating rate (Fig. 6.10; see also Appendix 3). It is generally in the range 1–50 8C min1. It has to be controlled carefully since the glass transition depends on the thermal history (see Sections 6.2.1 and 6.5.2). The same remark applies to calorimetry (Section 6.2.3). The expansion of the specimen is monitored by a stylus (or a measuring device) that contacts the specimen under a small force. Note that only the difference between the expansion of the specimen and the cylindrical support is determined (Appendix 3). Therefore, correction of the data has to be made to add the expansion of the instrument itself. Examples of corrected expansion curves are shown in Fig. 6.11. The curve shows a straight line for silica over the whole temperature range while the other two glasses show ﬁrst a linear domain (elastic), a transition around 550 and 600 8C to the liquid domain (viscous) with a change in the observed slope and then a maximum of the curve (around 620 and 680 8C). The ﬁrst transition corresponds to

Fig. 6.10 Dilatometer: (a) general view and (b) sample–stylus contact.

101

102

6 Glass Rheology

Fig. 6.11 Thermal expansion heating curves for silica, silico-soda-lime and tin-rich silico-soda-lime glasses.

the glass transition while the second one corresponds to the dilatometric softening point (obtained for a viscosity of h ¼ 1010 Pa s). Glass transition temperature can be determined at the intersecting point of the tangents of the solid and liquid domains. It is about 560 and 620 8C for the SLS and tin-rich glasses shown in Fig. 6.11. In the linear domain the slope of the curve allows one to determine the thermal expansion of the solid glass, that is, the relative expansion per temperature unit: as ¼

1 dL L dT

ð6:35Þ

where L is the specimen length and T the temperature. Glass thermal expansion is determined from Fig. 6.11 to be about 9 106 8C1 (8.9 106 and 8.3 106 8C1 for the SLS glass and the tin-rich glass respectively; Le Bourhis, 1998b). The increase in slope after transition indicates that the thermal expansion of the liquid al is larger than that of the glass. From the curves shown in Fig. 6.11, the liquid thermal expansion is estimated to be about three to four times that of the solid. However, care has to be taken with the values obtained from dilatometry for T > Tg, since expansion is measured by a contacting stylus which progressively penetrates into the viscous liquid and thermal expansion is underestimated. Further penetration of the stylus explains the end and maximum of the curve. In fact, when viscosity falls to about 1010–1011 Pa s, the glass becomes so soft that it no longer behaves as a rigid specimen. It sags if lying horizontally and suspended at only a small number of points, and it may deform under the action of the small force necessary to keep the measuring device (stylus) in contact with the specimen. In practice, whatever the arrangement adopted, the apparent maximum is found at nearly the same temperature, that is, the softening temperature. An important characteristic of modiﬁed glasses is that they show larger thermal expansion than silica. When a specimen is annealed the average distance between atoms changes according to the asymmetry of the potential energy curve or bond. When modiﬁers are introduced non-bridging oxygen (NBO) atoms are formed

6.2 Glass Transition and Its Observation

(Chapter 5) leading to bond asymmetry and hence more thermal expansion (Appendix 3). In contrast, borosilicates offer the possibility to form the glass at lower temperatures as in a modiﬁed glass while B atoms participate to the formation of the glass network. As a matter of fact no NBO atoms are formed and thermal expansion is reduced. As discussed in Chapter 2, these glasses offer good resistance to thermal shock. 6.2.3 Differential Scanning Calorimetry

A differential scanning calorimeter allows the continuous measurement of the heat ﬂow rate F between a given specimen (S) and a reference (R) as a function of temperature (Figs. 6.12 and 6.13). The reference is often the empty crucible, the same as that used for containing the specimen. The difference in heat ﬂow rate F allows for the determination of the speciﬁc heat of the specimen. Let us consider a period of time from t1 to t2 during which the specimen temperature rises from T1 to T2. Heat Q is written Zt2 Q¼

FðtÞdt ¼ mcp ðT2 T1 Þ

ð6:36Þ

t1

where m is the mass of the specimen and cp its speciﬁc heat. When glass transition is passed there is a change in speciﬁc heat that is detected by the instrument as schematically represented in Fig. 6.14 (see also Fig. 6.32). Glass transition temperature can be determined at the inﬂection point. DSC softwares offer three different determinations of the transition as shown schematically in Fig. 6.14. Tgip is determined at the point of inﬂection, Tgon at the onset of the transition and Tgend at the end of

Fig. 6.12 Differential scanning calorimeter set-up.

103

104

6 Glass Rheology

Fig. 6.13 Differential scanning calorimeter principle (R, ¨hne et al., 1996). reference; S, for specimen; according to Ho

Fig. 6.14 Heat ﬂow rate at glass transition as a function of temperature.

the transition. Notably, experimental curves often show a hump at Tgend because of relaxation phenomena; this is illustrated in Fig. 6.32 and discussed in detail in Section 6.5.4 (Ho¨hne et al., 1996; Heilmaier and Eckert, 2005). This may lead to erroneous transition temperature determination on heating curves. Below and above the glass transition, it is possible to determine the speciﬁc heat of a specimen of known weight employing Eq. (6.36) and analysing the heat ﬂow in the respective domains. When temperature is further increased, crystallization may appear (exothermic ﬂow) that further melts at melting temperature (endothermic ﬂow).

6.3 Viscous Response of Glass

An important consequence of the viscous behaviour is that glass shows timedependent properties at temperatures approaching the glass transition temperature.

6.3 Viscous Response of Glass

In fact, these phenomena appear when the characteristic time of the observations scales with the relaxation time of the glass, TR ¼ h/G, where h is the viscosity and G the shear modulus. This relaxation time will be introduced in more detail in Section 6.4.2. The time dependence appears in the shear stress–shear strain equation introduced above: t ¼ hg

ð6:37Þ

It should be noted again that, in contrast, an elastic material shows a response independent of time: t ¼ Gg

ð6:38Þ

From these equations a phenomenological correspondence has been proposed to pass from an elastic solution to a viscous one in which the elastic constants in the elastic equations are replaced with a time-dependent operator. Following Goodier 1936, the analogy between the steady viscous motion and the elastic deformation enables one to take over from the elastic theory solutions for viscous ﬂow. One has to suppose two isotropic and homogeneous bodies of the same shape, one purely viscous the other one purely elastic and incompressible. The two are loaded in the same way. ‘If certain displacements are prescribed as given function in the elastic body, then the corresponding velocities in the viscous body are prescribed as the same functions when the coefﬁcient of viscosity h is substituted for G as long as the deformation makes no signiﬁcant change in the boundaries’ (Goodier, 1936). Applying this simple rule allows the tensile representation of a viscous solid to be determined passing from s ¼ Ee ¼ 2(1 þ n)Ge to s ¼ 2ð1 þ 0:5Þhe ¼ 3he, viscous ﬂow being volume conservative (so-called prefactors 1 and 3 for shear and tensile loading respectively). Elongational viscosity is then obtained to be three times higher than shear viscosity introduced in Section 6.1.2.3. Let us now consider the forming of glass by gravity (Fig. 6.15). This is used for production of laminated windshields for instance. The elastic solution is given by

Fig. 6.15 Diagram of the deformation of a plate under gravity.

105

106

6 Glass Rheology

Timoshenko (1951): d¼k

rga4 rga4 ¼k 2 EtH 2ð1 nÞGt2H

ð6:39Þ

where d is the elastic displacement of the sheet centre, a and tH the dimension and the thickness of the sheet, r and M its density and its mass, E the Young’s modulus, g the gravitational acceleration and k a shape factor (3/4p for a circular plate). The solution of Eq. (6.39) is valid for d < tH. Changing the elastic solution using a time operator allows determination of the viscous solution: Z rga4 dt ð6:40Þ d¼k 2 h 3tH Here, we neglect the elastic part of the deformation and still suppose d < tH. This limit is quite unrealistic for commonly produced shapes and the nonlinear solution is to be considered. Adding the elastic and viscous solutions (Eqs (6.39) and (6.40)) results in a Maxwell modelling of the plate behaviour as detailed in Section 6.4. Equation (6.40) cannot be integrated simply unless the temperature (the viscosity) is supposed to be constant, which is rarely the case when an industrial process is considered. From this simple approach it is clear that complex shapes are achieved when the thermal route can be carefully controlled. In practice, two sheets of glass are twinned and subsequently treated together to form laminated windshields. When the sheet thickness and colour are identical the thermomechanical route is the same, assuming no thermal gradient is present through the sheets when heating and cooling rates are low enough. This allows one to obtain parallelism of the formed sheets and hence optimized optical properties. In practice, glass sheets are different (either in terms of thickness or colour) and the processing line is operated so that the top sheet bows onto the bottom sheet (without contact damage; see Chapter 8).

6.4 Viscoelastic Response of Glass 6.4.1 Introduction

Between the elastic and viscous extremities stands the viscoelastic behaviour that is expected around the glass transition. The purely viscous response of a melt is often termed ‘liquid’ behaviour whereas purely elastic response is termed ‘glassy’ behaviour. The intermediate transition is not sharp but shows a viscoelastic regime. Therefore, at the transition both the elastic and the viscous behaviour are to be combined. At short times the behaviour will predominantly be elastic while viscous behaviour appears at times long enough to attain steady-state ﬂow. Then viscoelastic behaviour is expected at intermediate times. The simplest approach is to combine in series or parallel these behaviours as detailed below. We will introduce an important

6.4 Viscoelastic Response of Glass

parameter, the relaxation time (that combines both properties), which allows prediction of whether for a given period of time the material behaves like an elastic, a viscous or a viscoelastic material. 6.4.2 Maxwell and Kelvin Solids

Further understanding of viscoelasticity requires in a ﬁrst step the consideration of simple models. We shall consider an elastic solid to be represented by a spring (t ¼ Gg) while a viscous solid will be represented by a dash pot (t ¼ hg; Fig. 6.16). Hence, as said above the viscous description of a solid can be found by replacing the elastic constants in the elastic solution and taking into account the time dependence. Associating the two solids (elastic and viscous) allows an insight into the viscoelastic behaviour (intermediate between purely elastic or purely viscous). The simplest association of these two elements is in parallel (Kelvin’s solid) and in series (Maxwell’s solid). Let us consider the respective combinations (Fig. 6.17). For a Kelvin solid we combine t ¼ t1 þ t2; t1 ¼ Gg and t2 ¼ hg and obtain t ¼ Gg þ hg

ð6:41Þ

For a Maxwell solid we have g ¼ g1 þ g2; t ¼ Gg1 and t ¼ hg2 . Then taking a time derivation of the ﬁrst and second equation and combining g ¼ g1 þ g2 ; t ¼ Gg1 and t ¼ hg2 we get t=h þ t=G ¼ g

ð6:42Þ

These solids allow creep and relaxation to be modelled with a characteristic relaxation time TR. Consider for instance a Maxwell solid submitted to a constant deformation g(t) ¼ go so that g ¼ 0. Shear stress relaxation with time is found solving t=h þ t=G ¼ g ¼ 0

ð6:43Þ

Taking TR ¼ h=G

Fig. 6.16 Spring and dash pot.

ð6:44Þ

107

108

6 Glass Rheology

Fig. 6.17 (a) Kelvin and (b) Maxwell solids and related creep and stress relaxation.

we ﬁnd tðtÞ ¼ to expðt=TR Þ

ð6:45Þ

which is plotted in Fig. 6.17b. We can observe that to apply a constant deformation to a Maxwell solid, a vanishing stress has to be applied. A very important parameter has appeared: the relaxation time TR. For t TR the solid behaves elastically, while for t TR viscous ﬂow is prominent. Similarly considering a Kelvin solid under constant applied stress to we have t ¼ to ¼ Gg þ hg

ð6:46Þ

The solution to this equation is gðtÞ ¼ to =G½1 expðt=TR Þ

ð6:47Þ

Hence, it is found that a Kelvin solid ﬂows under constant stress once time is of the order of TR (Fig. 6.17a). Some authors refer to Kelvin TR as retardation time. As discussed below glass delayed elasticity and ﬂow can be captured with a Burger solid that combines in series a Kelvin and a Maxwell solid. A Kelvin solid yields retardation while a Maxwell one yields relaxation. Relaxation time informs on the time scales at which a viscoelastic solid will behave elastically or relax. Let us consider glass transition: the viscosity is 1012–1012.5 Pa s while shear modulus of most glasses scale with 1010–1011 Pa so that relaxation time is of the order of 100 s. This means that at the glass transition temperature stress relaxation happens after a couple of minutes.

6.4 Viscoelastic Response of Glass

6.4.3 Dynamic Mechanical Analysis

Dynamic mechanical analysis (DMA) consists in applying a periodical stress ﬁeld to a material. We can anticipate from Section 6.4.2 that the behaviour of a viscoelastic material will depend strongly on the frequency v of the applied stress. Consider a shear stress applied periodically to a viscoelastic solid. We take a sinusoidal function having in mind that any periodic function is a Fourier series of sinusoidal functions. Shear stress is written t ¼ to cosvt

ð6:48Þ

A generalized relation between stress and strain is obtained using complex notation (t ¼ tocos vt þ itosin vt ¼ toexp ivt) in the form t ¼ G g

ð6:49Þ

G being a complex number of the form G ¼ G0 þ iG00. The real part or storage modulus describes the capacity of the material to store energy elastically upon deformation. The imaginary part is called loss modulus since it provides a measure of the energy dissipated by the material. Both moduli show a dependence on frequency. The phase shift d between stress and strain is given by tan d ¼ G00=G0

ð6:50Þ

where d is the loss angle and tan d the loss factor related to the dissipated mechanical energy DW by DW/We ¼ 2ptan d (where We is the stored elastic energy). Q1 ¼ DW/ We ¼ 2ptan d is also called the damping coefﬁcient. The elastic, viscous and viscoelastic behaviours are shown schematically in Fig. 6.18. In the elastic regime, stress and strain are in phase (no time dependence). In the viscous regime stress and strain are phase shifted by 908. Viscoelastic behaviour corresponds to an intermediate phase shift. Let us illustrate this behaviour for the case of a Maxwell solid. The modulus expression for G can be found taking again Eq. (6.42) with the complex notation (with t ¼ ivt ): t =h þ t =G ¼ t =h þ ivt =G ¼ t ð1=h þ iv=GÞ ¼ g ¼ ivg

ð6:51Þ

We extract t ¼ iv=ð1=h þ iv=GÞg

ð6:52Þ

and obtain G ¼

iv 1=h þ iv=G

ð6:53Þ

109

110

6 Glass Rheology

Fig. 6.18 Elastic, viscous and viscoelastic dynamic response.

Storage and loss moduli are G0 ¼

v2 TR2 G 1 þ v2 TR2

ð6:54aÞ

vTR G 1 þ v2 TR2

ð6:54bÞ

G00 ¼

These expressions yield for vTR ! 1; G0 ! G; G00 ! 0; d ! 0

ð6:55aÞ

that is, a purely elastic regime for large frequencies, while for vTR ! 0; G0 ! 0; G00 ! 0; d ! p=2

ð6:55bÞ

that corresponds to a purely viscous behaviour. At intermediate frequencies the material shows a viscoelastic behaviour with an intermediate loss angle (0 < d < p/2). These trends can be generalized. In fact when forced at a high frequency, a glass or a ﬂuid reacts rigidly. Deformations are small and all energy introduced into the system can be regained upon releasing strain. The storage modulus is large and the loss modulus small (Fig. 6.19). At intermediate frequencies, deformations become large enough for structural elements in the liquid to be permanently removed from their original position. Such displacements dissipate energy. At a particular frequency, a resonance occurs where the loss modulus peaks while storage modulus goes through an inﬂection (Fig. 6.19; for a Maxwell solid it is expected for w ¼ 1/TR). Towards low frequencies, the loss modulus decreases again. The ﬂuid ﬂows effortlessly, resulting in large irreversible deformations, indicating that the storage modulus becomes smaller.

6.4 Viscoelastic Response of Glass

Fig. 6.19 Loss and storage moduli as a function of frequency for 2SiO2–Na2O glass (master curve; see also Section 6.4.5.4). (Reprinted from Mills, 1974 with permission from Elsevier.)

Alternatively, glass behaviour can be investigated as a function of temperature for a given frequency (Fig. 6.20). The graph obtained for a chalcogenide glass shows that the dynamic response (at a given frequency, Fig. 6.20b) varies considerably with temperature. The Young’s modulus E curve shows a dramatic decrease of storage modulus while damping (proportional to loss factor) increases dramatically near the glass transition (Tg ¼ 280 8C). In fact, at low temperatures glass shows an elastic behaviour (rigid with no loss) that progressively changes into viscoelastic behaviour. 6.4.4 Modelling Real Solids

The modelling of glass behaviour requires the association of several Maxwell elements and/or Kelvin elements. The simplest model allowing capture of instantaneous and delayed elasticity as well as viscous ﬂow is the Burger association of a Maxwell (G1, h1) element and a Kelvin (G2, h2) element in series. Under an applied constant stress, strain is written (Fig 6.21):6) 1 1 t t ð6:56Þ gðtÞ ¼ to þ 1 exp 2 þ 1 G1 G2 TR TR where TR1 ¼ h1/G1 and TR2 ¼ h2/G2. The solution is plotted in Fig. 6.21.

6)

t = tK = tM, g = gK + gM; to/h1 = M ! gM = to/h1t + to/G1; to = G2gK + h2 K ! gK = to/G2[1 exp(t/TR2)].

111

112

6 Glass Rheology

Fig. 6.20 (a) Dynamic resonance method (DRM) head (a parallelepiped beam is observed at the centre of the head). (Courtesy P. Gadaud, ENSMA Poitiers.) (b) Young’s modulus and damping coefﬁcient Q1 = 2ptan d as a function of a temperature for a GeAsSe chalcogenide glass obtained with a DRM device. (From Le Bourhis et al , 2001a with permission from Elsevier.)

Fig. 6.21 Burger solid and its response to a constant applied stress. On loading under to an instantaneous elastic strain gi, a delayed elastic strain gd and a viscous strain gd appear. On unloading only elastic strain gi and delayed elastic strain gd recover.

6.4 Viscoelastic Response of Glass

Equation (6.56) produces an instantaneous elastic strain (ﬁrst term, gi ¼ to/G1), a delayed elastic strain (second term, gd ðtÞ ¼ ðto =G2 Þ½1 expðt=TR2 Þ) and a viscous strain (third term, gv ðtÞ ¼ to t=TR1 ). The ﬁrst two terms recover on unloading, whereas viscous ﬂow is irreversible. Often used in the literature, anelasticity refers to the instantaneous plus delayed recoverable deformation while viscous ﬂow, in contrast, is not recoverable. Generalized Maxwell and Kelvin models are combinations of several Maxwell elements in parallel or Kelvin elements in series respectively. They were introduced to describe discrete relaxation times. The generalized Maxwell model is written n X tðtÞ ¼ g0 GðtÞ ¼ g0 Gk expðt=TkR Þ ð6:57Þ k¼1

with the relaxation times of the different elements being TkR ¼ hk =Gk . This distribution of relaxation time may be due to a real spatial distribution of regions having different viscosities (because of temperature and composition heterogeneities). More fundamentally, such a distribution can be associated with the fact that the heights of the potential barriers impeding atomic or molecular motions are not equal. We generally only consider the average value while in fact there might be a broad and continuous distribution of barrier heights and hence relaxation times. 6.4.5 Functional Formulation 6.4.5.1 Creep Let us consider the stress being applied instantaneously and take a Heaviside function tðtÞ ¼ to Hðt t j Þ

ð6:58Þ

with H ¼ 0 for t t j < 0

ð6:59aÞ

H ¼ 1 for t t j 0

ð6:59bÞ

Deformation is taken as a function of history (it is history dependent): gðtÞ ¼ Jðt t j Þto

ð6:60Þ

where J is the compliance characteristic of the material. For a Kelvin solid J(t) ¼ go/ so[1 exp(t/TR)]. Now we consider stress is applied with n successive steps: tðtÞ ¼

n X Dt j Hðt t j Þ j¼1

ð6:61Þ

113

114

6 Glass Rheology

Assuming linear viscoelasticity, strain becomes n X Dt j Jðt t j Þ

gðtÞ ¼

ð6:62Þ

j¼1

Equation (6.62) can be generalized to a continuously varying stress as Zt gðtÞ ¼ 0

dtðt0 Þ Jðt t0 Þdt0 dt0

ð6:63Þ

For the case of successive steps and continuously varying stress between steps then one has to add Eqs (6.62) and (6.63). With a single creep measurement, one can theoretically calculate the entire creep compliance. Thereafter, any response can be calculated using this compliance and changing the stress history t(t). There are experimental difﬁculties in imposing a true step stress function and in measuring J(t) at long times. In practice, glass is assumed to have simple thermorheological behaviour. The mechanisms are considered to be independent of temperature, and only the kinetics is changed with the temperature. The creep function at a temperature can be determined from experiments at other different temperatures, the overall evolution with time arbitrarily plotted for a reference temperature (Section 6.4.5.4). 6.4.5.2 Stress Relaxation Using the same approach as for creep we consider strain to be gðtÞ ¼ go Hðt t j Þ

ð6:64Þ

Stress relaxation is written tðtÞ ¼ Gðt t j Þgo

ð6:65Þ

where G is the relaxation modulus of the material. For a Maxwell solid G(t) ¼ so/ goexp(t/TR). For a continuously varying strain we have Zt tðtÞ ¼ 0

dgðt0 Þ Gðt t0 Þdt0 dt0

ð6:66Þ

These relations can be generalised for a three-dimensional loading (Appendix 9). The deviator sij and hydrostatic s stress tensor being determined using the following similar equations: Zt si j ¼ 0

dei j Gðt t0 Þdt0 dt0

ð6:67Þ

6.4 Viscoelastic Response of Glass Tab. 6.5

k

T (s) R 1k

w1k

Shear relaxation times of the Prony series according to Rekhson (1986);

Pn

k¼1

w1k ¼ 1:

1

2

3

4

5

6

19 0.0438

291.9 0.0611

1843 0.0899

11 800 0.2516

49 490 0.2974

171 700 0.2561

Zt sðtÞ ¼ 0

de Kðt t0 Þdt0 dt0

ð6:68Þ

where eij is the deviator strain tensor and e the hydrostatic strain tensor. G(t) and K(t) are the shear and hydrostatic relaxation moduli: GðtÞ ¼ 2Gc1 ðtÞ

ð6:69Þ

KðtÞ ¼ 3Ke ð3Ke 3Kg Þc2 ðtÞ

ð6:70Þ

where ci are the relaxation functions, G and Kg the shear and bulk instantaneous elastic constants and Ke the bulk equilibrium elastic modulus that accounts for both instantaneous and delayed volumetric elasticity. Kurkjian 1963 and Rekhson 1986 proposed the use of generalized Maxwell models in the form of Prony series (Table 6.5) for the shear relaxation function c1(t):7) c1 ðtÞ ¼

n X R w1k expðt=T1k Þ

ð6:71Þ

k¼1

Moreover the hydrostatic relaxation function relaxes much more slowly and is often supposed to be (Guillemet and Gy, 1996). c2 ðtÞ ¼ c1 ðt=10Þ

ð6:72Þ

The Prony series proposed by Rekhson 1986 for the shear relaxation is composed of six different elements with shear relaxation times which are to be considered by their relative contribution (Table 6.5).

7)

This function can be written for a continuous spectrum of relaxation time asRc1(t)= R1 1 0 F(TR)exp(t/TR)dTR with 0 F(TR)dTR=1. Taking p = 1/TR and N(p) = 1/p2F(1/p) allows one to show c1(t) to be the

Laplace transform of N(p): c1(t)= R1 0 N(p)exp(pt)dp. This formalism can be employed to rationalize elastic-viscoelastic correspondence discussed in Section 6.4.5.3.

115

116

6 Glass Rheology

6.4.5.3 Elastic–Viscoelastic Correspondence Let us consider the stress relationship obtained from the functional formulation for a viscoelastic material. We obtain Zt tðtÞ ¼ 0

dg Gðt t0 Þdt0 dt0

ð6:73Þ

Let us compare this relation to that of an elastic solid t ¼ Gg. The elastic–viscoelastic correspondence says that the viscoelastic solution can be generated from the incompressible (n ¼ 0.5) elastic one using a Boltzmann hereditary integral (hereditary for past dependent) with respect to past time from t0 ¼ 0 to the present time t0 ¼ t. This is illustrated as Zt G! 0

d Gðt t0 Þdt0 dt0

ð6:74Þ

This procedure is very useful for complex loading conditions (contact loading for instance; see Appendix 8). As a matter of fact, the solutions to these integral equations are completely dependent on the choice of material relaxation modulus G(t). 6.4.5.4 Superposition Principle (simple thermorheological behaviour) We shall assume that glass shows a simple thermorheological behaviour or, in other words, the mechanisms are independent of the temperature and only the kinetic is changed. Once the behaviour is known at a temperature (so-called reference temperature), it can be determined at any temperature using shift factors f(T) for the relaxation time (Ferry, 1970), or at different times, relaxation curves are derived from another by a change in time scale (Figs. 6.22 and 6.23). Kurkjian 1963 studied extensively glass stress relaxation at different temperatures. Glass rods were ﬁrst stabilized at a given temperature and twisted. The overall results were observed to adjust on a single master curve (Fig. 6.23). This can occur only if all relaxation times characterizing the material have the same temperature dependence and the weighting factors are constant. This implies that all the processes involved in the relaxation have the same activation energy and that the same processes are active at all temperatures. Indeed if a new process appears, the weighting factors must change, altering the shape of the curve. Fortunately, real glasses do exhibit thermorheological simplicity to a high level of approximation. Like Lee et al. 1965 we shall introduce the thermorheological simplicity of glass by using the reduced time deﬁned by Zt j¼

dj

ð6:75aÞ

0

with dj ¼ fðTÞdt0

ð6:75bÞ

6.4 Viscoelastic Response of Glass

Fig. 6.22 Normalized stress as a function of logarithm of time, at seven experimental temperatures (according to Kurkjian, 1963).

Fig. 6.23 Master curve at 473 8C produced from the data obtained at various experimental temperatures (Fig. 6.22; according to Kurkjian, 1963).

117

118

6 Glass Rheology

In general temperature varies and the integral cannot be simpliﬁed. When the temperature is constant, reduced time is proportional to time and is written j ¼ f(T)t. We assume that at any temperature T, the stress relaxation function is cT(t) ¼ cR(j), where cR is the stress relaxation at reference temperature (f(TR) ¼ 1). The shifting procedure can be illustrated in a graph showing the c dependence with log(t). Consider only two different temperatures (reference and studied temperature): cT ðlogtÞ ¼ cR ðlogjÞ ¼ cR ðlog½fðTÞtÞ ¼ cR ðlogt þ log½fðTÞÞ

ð6:76Þ

Then, the simple thermorheological behaviour says that the stress relaxation function at any temperature is obtained in the log scale by shifting the curve by log[f(T)]. A reverse operation consists of determining the behaviour of the glass and shifting the creep functions (so called equivalence between time and temperature) to obtain the master curve evolution with time at a reference temperature (Section 6.4.3; Figure 6.24). Shift factor can be obtained from viscosity data: fðTÞ ¼

hR h

ð6:77Þ

where hR is the viscosity at the reference temperature. Under a continuously varying temperature, reduced time incorporates the varying scale factor (see also Section 6.5). Assuming a Prony series, the reference temperature is to be ﬁxed by the following equation: TR ¼

n hR X R w1k T1k ¼ G k¼1

Then, the relaxation functions can be obtained at any temperature using the shift factor presented above. For instance, for a soda-lime-silica glass, the Prony series is shown in Table 6.5 and is to be taken for a reference temperature of 508 8C with hR ¼ 1.86 1015 Pa s (Guillemet and Gy, 1996).

Fig. 6.24 Shear relaxation function as a function of time for two different temperatures.

6.5 Tempering of Glass

6.5 Tempering of Glass 6.5.1 Introduction

The thermal history of glass has to be carefully controlled in order to design the level of residual stresses. When the material passes through the viscous–elastic domain submitted to a thermal gradient, compressive residual stresses appear at the surface (tensile in the core). Fast cooling rate will allow tempering of the glass while slow cooling rate and annealing of the glass will allow stabilization of the structure and reduction of residual stresses. A tempering set-up comprises either a ventilator or a compressor injecting air through nozzles that reaches the glass surface (Figs. 6.25 and 6.26). A parabolic stress proﬁle showing compressive and tensile zones is represented and is typical of thermal tempering. Figure 6.27 shows a tempered backlight showing signatures of the process (nozzle air marks) since glass photoelasticity allows for thermal residual stress heterogeneities to be observed (see also Chapter 11).

Fig. 6.25 (a) Schematic representation of tempering with nozzles injecting cooling air (grey arrows) and (b) residual stress proﬁle in a thermally tempered glass sheet.

119

120

6 Glass Rheology

Fig. 6.26 Bending and tempering unit. (Courtesy Tamglass Ltd, http://www.tamglass.com/.)

6.5.2 Freezing Theory

Glass tempering prediction is a complex problem since i. thermal transfer involves unknowns, ii. thermal and structure histories are complex, and iii. triaxial stress build up is to be determined.

Fig. 6.27 Nozzle photoelastic signatures (due to tempering) are observed here on a backlight (they correspond to residual stress heterogeneities and are better observed at dawn; see also Chapter 11).

6.5 Tempering of Glass

In a ﬁrst approach, Adams and Williamson 1920 proposed a thermoelastic model to determine the stresses in a glass sheet cooled at a constant rate cR. The outer layers of the glass sheet will become rigid ﬁrst, then as the inside cools, it tries to shrink, but is restrained by the rigid outer layers. Then, a simple representation of the tempering is to separate the sheet into three parts (the two surfaces and the core) and allow viscous ﬂow in the core until it freezes (Fig. 6.28). A thermal gradient appears throughout the sheet. On passing the glass transition with cooling down to room temperature, the difference in displacements between the surface and the core cannot be accommodated any longer and residual stresses build in. If the glass is cooled at a constant rate, the temperature proﬁle is parabolic and temperature variation through the sheet (between the surface and the centre) is written DT ¼ t2H cR cP =8k

ð6:78Þ

where tH, cR, cP and k are the thickness of the sheet, the cooling rate, the speciﬁc heat and thermal conductivity of the glass respectively. The biaxial stresses are sðzÞ ¼

Ea ½T TðzÞ 1n

Fig. 6.28 Schematic representation of residual stress generation in a thermally tempered glass sheet. Viscous ﬂow is possible over Tg. Thermal gradient builds in. On passing the glass transition and obtaining uniform temperature, stress builds in.

ð6:79Þ

121

122

6 Glass Rheology

where T is the mean temperature, T(z) the temperature at position z, E the Young’s modulus, n the Poisson ratio (E/(1 n) is often called the biaxial modulus) and a the thermal expansion coefﬁcient of the glass. When the temperature distribution is parabolic, maximum tensile stress appears at the centre of the glass sheet: sc ¼ as E=3ð1 nÞDT ¼ At2H cR

ð6:80Þ

This very simple relation shows that a thicker sheet yields larger thermal gradient and hence larger residual stresses. The effect of using larger cooling rate is also straightforward leading to more tempering. It can be anticipated that tempering of thin glasses is difﬁcult since it requires technology for large cooling rates. One must also consider that such tempering may mark the glass as strong air ﬂows have to be injected through the nozzles which may deform the glass surface and damage the optical quality. The three-part model can to be extended to a continuous model allowing for a parabolic proﬁle of stresses to be obtained (Aben and Guillemet, 1993; Figure 6.25). Equibiaxial stress ﬁeld is written " # 1 z 2 ð6:81Þ sx ¼ sy ¼ 3sc 2 3 tH where sc is the tensile residual stress at the sheet centre (at z ¼ 0, core stress). At the surface, residual stress is ss ¼ 2sc. Stress is null for z/tH ¼ 0.3 or at a distance of 1/ 5tH from the surface. 6.5.3 Stress Relaxation

The ﬁrst approach described above supposes that stresses are frozen at Tg while stress relaxation happens at characteristic times that depend on the temperature because of the viscous–elastic behaviour of glass. Supposing glass has a simple thermorheological behaviour (Section 6.4.5.4), we consider reduced time and have Zt j¼

dj

ð6:82Þ

hR 0 dt h

ð6:83Þ

0

with dj ¼

Stresses build in and partially relax because of the viscoelasticity of glass. Stresses are written assuming an equibiaxial stress ﬁeld (subscript B, this is to be reconsidered close to an edge or a hole, see Chapter 11): Zt sðz; tÞ ¼ 0

GBR ðj j0 Þ

q ½eðt0 Þ as Tðz; t0 Þdt0 qt0

ð6:84Þ

6.5 Tempering of Glass

where GBR is the relaxation modulus for biaxial stress which is deduced from the shear and hydrostatic relaxation moduli, e(t0 ) is the strain at time t0 which is the same for all values of z (the deviation of the induced thermal strains from the uniform actual value generates the stresses in the different layers of glass) and is deﬁned by the equation of mechanical equilibrium, as is the thermal expansion coefﬁcient for glass and T(z, t0 ) is the temperature at position z and time t0 . The viscoelastic approach was revealed to yield a non-negligible discrepancy between modelling and experiments (Gardon, 1978; Narayanaswamy, 1978), because the rapid cooling of glass causes also its structure to deviate considerably from the stabilized (equilibrium) state. Hence realistic models have to consider the glass structural relaxation in order to be more predictive (Section 6.5.4). As a matter of fact, R&D numerical tools incorporate stress and structure relaxations. 6.5.4 Structural Relaxation

Not only stress relaxation has to be considered when modelling glass tempering but also the structural relaxation, since the glass structure is known to be out of equilibrium. This issue was addressed ﬁrst by Acloque (1951). At a given temperature glass will tend to approach the liquid conﬁguration. This indeed happens without applying any stress to the material. When a supercooled liquid freezes it departs from the liquid curve (see for instance Section 6.2.1). Then, the liquid freezes in a less dense conﬁguration than the supercooled liquid would present at the same temperature. When time is allowed for the glass to rearrange it will progressively tend to the denser liquid conﬁguration and hence glass structure is expected to change with time. At room temperature the time scale is beyond the human time scale and hence structural relaxation of glass is not detected. The situation is different when the glass is set at a higher temperature. Some examples are shown in Fig. 6.29 where two pieces of glass were set at the same temperature while previously being stabilized at two different temperatures (Moynihan, 1996). The glass that was stabilized at a temperature higher than that imposed relaxes more rapidly than the one that was stabilized at a lower temperature. The ﬁrst glass presents a more open structure as it was stabilized at a higher temperature and shows a greater average volume, and hence a reduced resistance to conﬁgurational changes. In contrast, the glass stabilized at a lower temperature shows a denser structure and hence more resistance to structural changes. When tempering the glass, this phenomenon has to be taken into account as well. In the transformation range, the glass no longer has enough time to reach its equilibrium state at each temperature because of its high viscosity. Glass structure will depend on tempering conditions (cooling rates; Gardon, 1978; Narayanaswamy, 1978; Scherer, 1982, 1996; Guillemet, 1990; Aben and Guillemet, 1993). Markowsky and Soules 1984 proposed a way to predict the structure of glass as a function of its thermal history using the concept of ﬁctive temperature ﬁrst introduced by Tool 1946. Contrary to a liquid whose structure is known from its actual temperature, glass structure can be obtained knowing both the temperature T

123

124

6 Glass Rheology

Fig. 6.29 Structural relaxation of two pieces of glass stabilized at two different temperatures (according to Moynihan, 1996).

and the ﬁctive temperature Tf, that is, its instantaneous temperature and its prior history. When glass approaches transition, equilibrium state cannot be reached because of the elevated viscosity. By deﬁnition, the ﬁctive temperature Tf of a glass corresponds to the temperature of the liquid which is in the same structural state as the glass under study. In a stabilized glass, Tf ¼ T while in a non-stabilized glass Tf 6¼ T. In practice, the ﬁctive temperature corresponding to the state A of a glass is represented in Fig. 6.30 by point B and can be obtained by taking the line parallel to the expansion curve of the solid and determining its intercept with the expansion

Fig. 6.30 Volume–temperature cooling curves showing ﬁctive temperature geometrical determination (l and g, liquid and glass domains; A, the point at which ﬁctive determination is made; B, the intercept of the expansion curve of the liquid and the line parallel to glass expansion curve passing through A). The temperature at B is by deﬁnition the ﬁctive temperature at point A.

6.5 Tempering of Glass

curve of the liquid. A glassy state can be viewed as a liquid-like state which has been frozen in. The liquid-like structure is then known from the ﬁctive temperature of the liquid-like structure. When a supercooled liquid is cooled more rapidly, the glass freezes at a higher temperature, the liquid-like structure corresponds to a higher temperature and hence the ﬁctive temperature is higher. Let us consider again Fig. 6.29. The glass that was stabilized at a higher temperature shows a higher ﬁctive temperature, and when forced at a lower temperature it relaxes to a liquid-like structure presenting a lower ﬁctive temperature. Then, the second glass ﬁctive temperature will instead increase progressively. Fictive temperature evolution depends on thermal history and this is the reason for the difference between the two glass behaviours. The glass presenting a higher ﬁctive temperature that has a more open structure relaxes more rapidly. Markowsky and Soules 1984 proposed an algorithm to determine the ﬁctive temperature evolution. Structural evolution being a nonlinear phenomenon, an iterative computational scheme was proposed. Both stress and structural relaxation phenomena are to be taken into account in the modelling of glass tempering, structural relaxation accounting for approximately 25 % of the total residual temper stresses (Narayanaswamy, 1978; Rekhson, 1986). Shear stress relaxation happens at characteristic time scaling with TR while structure is accepted to relax about ten times slower (KTR 9TR; Guillemet, 1990; Gy et al., 1994; Guillemet and Gy, 1996). A Prony series is then adopted again with characteristic relaxation times shifted by approximately one order of magnitude. Alternatively, a simpler KWW function often ﬁts well the relaxation of glasses (Debast and Gilard, 1963; Scherer, 1996). Let us consider an increment in time dt; from a given step numbered n 1 to the following step numbered n, we have dj ¼

hR dt h

ð6:85Þ

j being referred to as the reduced time (Aben and Guillemet, 1993) and subscript R indicates the reference temperature. Here, the viscosity function has to capture structural relaxations (ﬁctive temperature). This is obtained from the Adam and Gibbs theory of cooperative relaxations (Section 6.1.3.4) and is written hðT; Tf Þ ¼ ho exp

B T½1 ðTo =Tf Þ

ð6:86Þ

When glass is at an elevated temperature its structure is at equilibrium and is that of the melt so that Tf ¼ T and we get a VFT expression for the viscosity. Close to glass transition, glass freezes progressively, Tf departs from T and viscosity is affected. After each increment of time the ﬁctive temperature (structure) can be calculated following the Markowsky and Soules (1986) algorithm that suggests the use of ‘partial ﬁctive temperatures’ Tfk and a Prony series: Tfk;n ¼ T n ðT n Tfk;n1 Þexpðdj=Ktk Þ

ð6:87aÞ

125

126

6 Glass Rheology

Tf ¼

6 X wk Tfk

ð6:87bÞ

k¼1

Tf ðz; 0Þ ¼ Ti

ð6:87cÞ

where Ti is the initial temperature. Figure 6.31 shows the ﬁctive temperature (structure) evolution following this algorithm on cooling and then re-heating a glass at the same rate and then on cooling the same glass at a higher cooling rate. It can be seen that the two curves obtained with the same rate (on cooling and heating) coincide only well below Tg and well above it. In fact, hysteresis results from structural relaxation and can be detected experimentally using DSC as shown in Fig. 6.32 and care has to be taken in analysing experimental results (Ho¨hne et al., 1996). In Section 6.2.1, we actually focus on one single route (cooling path). The actual behaviour can be commented on in view of the discussion regarding Fig. 6.29. In fact, on heating the glass the starting point is a liquid-like structure at a lower ﬁctive temperature than the supercooled liquid following the cooling curve. This means that the starting point for the heating curve corresponds to a denser structure and rearrangement will be slower. Then the heating curve will always be below the cooling curve (for the same cooling and heating rate). Note also that on cooling a glass more rapidly, a larger ﬁctive temperature is obtained, or a less dense glass (Fig. 6.31; silica shows an anomaly with a reverse trend).

Fig. 6.31 Structure (ﬁctive temperature, Tf ) as a function of temperature on cooling and heating a glass piece. For comparison fast cooling route is shown and yields a glass with a higher ﬁctive temperature (less dense glass).

6.5 Tempering of Glass

Fig. 6.32 DSC heating curves of annealed and quenched ¨hne et al., 1996). Note relaxation glasses (according to Ho peaks, the higher being observed for annealed glass resulting from the non-equilibrium nature of glass. DSC analysis should be considered with care since it would appear that the conventional glass transition temperatures of quenched glass is lower than that of annealed glass while it is the contrary in fact.

The calculation of residual stresses requires consideration of the thermal expansion mismatch between the liquid and the glass when the actual structural state is to be determined as described above. Assuming equibiaxial stress ﬁeld (subscript B), stress is given by a formula incorporating structural relaxation through the ﬁctive temperature parameter: Zt sðz; tÞ ¼ 0

GBR ðj j0 Þ

q ½eðt0 Þ as Tðz; t0 Þ ðal as ÞTf ðz; t0 Þdt0 qt0

ð6:88Þ

where GBR is the relaxation modulus for biaxial stress, e(t0 ) is the strain at time t0 which is the same for all values of z and is deﬁned by the equation of mechanical equilibrium, as and al are the thermal expansion coefﬁcients for glass and liquid respectively and T(z, t0 ) is the temperature at position z and time t0 (we ignore edges here). Figure 6.33 shows the amplitude of core tensile residual stresses that build in under different experimental conditions. It shows a very good agreement between the calculated and experimental values allowing for great precision in the predictions. Figure 6.33 shows that, in fact, to generate residual stresses the initial temperature of the glazing needs to be over the transition temperature. This is not unexpected, since cold glass is elastic and therefore cannot be tempered. The potential for temper is fully developed only for quenching from temperatures well above the transition

127

128

6 Glass Rheology

Fig. 6.33 Dependence of residual mid-plane tensile stress (sc ¼ s(0, 1)) on the initial temperature Ti of a glass and on the heat transfer h (W m2 K1); thickness 6.1 mm, natural convection corresponds approximately to the lowest curve (according to Narayanaswamy, 1978). They actually used the viscosity function h(T, Tf ) ¼ ho exp {B[(x/T) + (1 x)/Tf ]} with x 0.5 instead of Eq. (6.86).

temperature. Also higher heat transfer (air ﬂow) induces higher plateau-level temper residual stresses and increases the temperature at which the plateau is reached. When quenching the glass, it is important not to mark it by nozzles air impact. In R&D, it is important to consider also the complex geometry and thermal history of the glazing (holes, edges) and containers. This requires numerical methods and adjustment to observed results. These complex geometries can be considered using ﬁnite element analysis (FEA; Appendix 11). It is beyond the scope of this book to describe these methods in detail. It has been realized that before designing a new tool to produce for instance backlights, different series of numerical experiments will allow one to approach the optimized tool. This tool once fabricated shows great potentiality to produce a glazing prototype close to the demanded one. This of course allows for economical gains since many experimental tests are saved.

6.6 Transient Stresses

The simple gradient model shown in Fig. 6.28 can also be used to model thermal shock (see Chapter 2). When the glass sheet is annealed at T < Tg the material

6.6 Transient Stresses

remains elastic (i.e. no viscous ﬂow happens). On cooling, transient compressive and tensile stresses build up and vanish when uniform temperature is reached. Stress is written s ¼ as E=ð1 nÞDT

ð6:89Þ

where DT is the temperature variation through the sheet (between its surface and its centre), as the thermal expansion coefﬁcient of the glass, E the Young modulus and n the Poisson ratio. These transient tensile stresses at the surface are dangerous for the glazing since fracture may originate from a superﬁcial ﬂaw when it is under tension (see Chapter 7). As a matter of fact, thermal shock with DT < 0 (on cooling down) is the most dangerous, as illustrated in Fig. 6.34, since tensile stresses develop at the surface where ﬂaws are known to exist (see Chapter 8). Much greater temperature differences can be withstood in sudden heating than in sudden cooling because only when cooling is the surface placed under tension. Also, thermal endurance can be greatly increased by a toughening process which places the surface under compression. Transient stresses are proportional to Young’s modulus and thermal expansion coefﬁcient. In Chapter 2, we discussed extensively the way to select materials in view of relevant parameters that are the thermal expansion, the elastic modulus and the ultimate stress at fracture. We showed the potential of silica-rich glasses and borosilicates for applications requiring a high resistance to thermal shocks.

Fig. 6.34 Schematic representation of the transient stress generation in a glass sheet under thermal shock (DT < 0, T < Tg) showing transient tensile stress at the surface and transient compressive stress in the centre. When temperature is uniform, transient stresses vanish.

129

130

6 Glass Rheology

Transient stresses should be very carefully considered also during the tempering process. Their partial relaxation leads to permanent stresses as discussed above. Under fast cooling there is a risk of the glass breaking under transient stresses. As discussed in Chapters 8 and 10, manufacturers control carefully production lines in order to avoid any abrasion of the glass surface (from the rollers, while packing) and this is surveyed up to the tempering operations. These procedures permit a gain in production yield as transient stress-induced breakages are avoided. The determination of transient stresses when the transition temperature is reached is more complex than when T < Tg. As reviewed above, for such temperatures stress and structural relaxation of the glass have to be taken into account.

6.7 Chemical Tempering of Glass 6.7.1 Introduction

Chemical tempering is applied for dedicated applications like aeroplane and highspeed train windshields, requiring high safety levels, and for thin glazing for which conventional thermal tempering would mark the surface or would not allow for sufﬁcient strengthening. Although production yields are much less important, chemical tempering has to be used to achieve very high level of stresses required in the range of 500–600 MPa. The treated depth of glass (diffusion length) is reduced to hundreds of micrometres. The glass to be treated is immersed in a salt bath containing cations the radii of which are larger than those to be exchanged in the glass (Fig. 6.35). Ion exchange induces compression at the glazing surface. Generally, the

Fig. 6.35 Chemical tempering principle.

6.7 Chemical Tempering of Glass

cations are alkali metal ions since they diffuse in glass much more rapidly than any other ions (Appendix 13). For instance, a glass containing sodium is strengthened by immersion into a potassium salt bath (generally KNO3). To enhance diffusion elevated temperatures (400–500 8C) are used for the treatment. Unfortunately, these temperatures, while being below the transition temperature of the glass, are high enough for stress relaxation to take place and this phenomenon balances diffusion effects in common glasses. Therefore, aluminosilicate (ALS) glasses were developed to replace soda-lime-silica (SLS) glasses because alkali metal diffusion is more rapid in ALS glasses while viscous relaxation at treatment temperature is slower. Both effects allow for achieving higher stress levels. Incidentally, as the viscosity of ALS glasses is larger than that of SLS ones at the same temperature (Fig. 6.2), ALS glass fabrication is more difﬁcult and expensive than that of SLS glass. 6.7.2 Ion Exchange and Stress Build-Up

The concentration of introduced ions can be calculated using Fick’s diffusion law. As detailed in Appendix 13 since surface concentration cs remains approximately constant, concentration c(z, t) at depth is written 0 z cðz; tÞ ¼ cs 1 erf pﬃﬃﬃﬃﬃ 2 Dt

ð6:90Þ

where z0 ¼ tH/2 z is the distance to the surface, cs the concentration at the surface, D the coefﬁcient of interdiffusion between the two kinds of atoms and t the immersion time. We shall assume in a ﬁrst step that no stress relaxation takes place at the bath temperature. The biaxial stresses are sðzÞ ¼

EB ½hci cðz; tÞ 1n

ð6:91Þ

where hci is the mean concentration of the exchanged ions, c(z, t) the concentration at position z and time t, E the Young modulus, n the Poisson ratio, B the ion exchangeinduced dilation coefﬁcient and t the total exchange time. B is analogous to the thermal expansion coefﬁcient in that the concentration c replaces the temperature. Thus B is the linear strain produced per unit exchange of ions (Tyagi and Varshneya, 1998): B¼

1 dV 3V dc

ð6:92Þ

A typical residual stress proﬁle is shown in Fig. 6.36. As compared to thermally tempered glazing only a thin layer is under compressive stresses (Fig. 6.25). Chemical tempering allows for treating more complex glass shapes than thermal tempering. However, care has to be taken so that the treatment penetrates the surface over ﬂaw extension (100 mm; see also Section 7.7.2).

131

132

6 Glass Rheology

Fig. 6.36 Residual stress proﬁle in a chemically tempered glass sheet.

6.7.3 Stress Relaxation

As mentioned above, stress relaxation may take place at treatment temperatures. This phenomenon is now considered. One has to make further assumptions: (i) diffusion does not modify the viscosity of the superﬁcial layers and (ii) relaxation happens at the treatment temperature and we neglect relaxation while cooling rapidly the specimens. Assumption (i) is quite realistic while assumption (ii) allows for using time instead of reduced time (we neglect structural relaxation). Then, stress relaxation is written (Shen and Green, 2004) Zt sðz; tÞ ¼ 0

GBR ðt t0 ÞB

q½hci cðz; t0 Þ 0 dt qt0

ð6:93Þ

where GBR is the biaxial relaxation function. 6.7.4 Engineered Stress Proﬁle Glasses

Recently, a new approach for chemical strengthening has been proposed by Green et al. 1999. The key feature is to carefully design the residual stress proﬁle in such a way that the maximum compression is moved away from the external surface while stress gradient is carefully controlled in the surface region (Fig. 6.37). These glasses have been termed engineered stress proﬁle (ESP) glasses. Normally, ion-exchanged glasses are processed to maximize the magnitude of the surface compression and the extent over which it acts (within economic constraints). In ESP glasses, it is not the overall depth of the surface compression that is important but rather the form of the stress proﬁle in the near-surface region. In fact, cracks are ‘trapped’ within the surface region (Fig. 6.38). These glasses show multiple cracking as a warning of the ﬁnal failure. The processing may not necessitate deep compressive layers. This is economically attractive as it may lead to

6.7 Chemical Tempering of Glass

Fig. 6.37 Stress proﬁle in ESP glazing obtained after a two-step ion exchange. (From Abrams et al., 2003, with permission from Elsevier.) For comparison a single ion exchange proﬁle is shown; note even for single ion exchange there is surface stress relaxation. This is avoided at low temperature with smaller treated depth (Guillemet and Gy, 1996).

Fig. 6.38 Multiple surface cracks in a two-step ion-exchanged glass tested under four-point bending. Loading axis is perpendicular to crack direction (HF acid etching was used to widen cracks for better visibility; the white bar is 1 mm long). (From Abrams et al., 2003, with permission from Elsevier.)

133

134

6 Glass Rheology

Fig. 6.39 Weibull distribution of ESP glass compared to untreated glass. (From Abrams et al., 2003, with permission from Elsevier.)

reduced processing times and, thereby, give rise to energy savings. The treatment is in two steps. In the ﬁrst step, molten KNO3 is used as a salt bath (at a temperature of 450 8C) to treat the aluminosilicate glasses. Here again soda-lime-silicate glass is difﬁcult to ion exchange, as exchange depths are limited by slow diffusion rates and stress relaxation. Therefore ALS glasses are preferred. A second exchange uses a mixed KNO3/NaNO3 salt bath at some lower temperature (400 8C). The effect of the second exchange is to make the stress gradient steeper near the surface and control the position of maximum compression. Another important issue for these glasses is the low strength variability while improving the average strength, as illustrated in Fig. 6.39. Strength variability will be discussed in more detail in the next chapter. While annealed silicate glasses were tested in the Weibull modulus range of 5–10, ESP Weibull modulus may exceed 60. Both strength and variability are important issues as regards glass application. To the author’s knowledge, these ESP glazings have not met commercial success.

135

7 Mechanical Strength of Glass Glass failure at temperatures below the glass transition is brittle and statistical. Fracture happens at much lower stresses when the specimen is loaded under tension than when loaded under compression (see also Appendix 10) and is of utmost importance for glass applications.

7.1 Theoretical Strength

Orowan 1949 ﬁrst proposed a rupture criterion in terms of elastic strength, surface energy (two new surfaces being generated upon fracture) and atomic structure. Fracture was expected to happen under tensile stress sth determined as (Appendix 5) rﬃﬃﬃﬃﬃﬃ Ez sth ¼ ro

ð7:1Þ

where E is Young’s modulus and z the surface energy (z is usually identiﬁed with the free surface energy of the cleavage surface, although this is still under debate; Mattoni et al., 2005). Equation (7.1) shows that stress at fracture increases together with surface energy and Young’s modulus. Taking for a soda-lime-silica glass E ¼ 70 GPa, z ¼ 0.6 J m2 (Table 7.1) and ro ¼ 0.15 nm (Si–O distance; see Section 5.2) one ﬁnds a theoretical strength sth as high as 16 GPa. Unfortunately, this value is well above experimental and usual values (50 MPa for ﬂat glass). Such a huge discrepancy was attributed to the presence of ﬂaws at the glass surface as discussed in detail below (see also Appendix 5). In fact, it was observed that strength was much dependent on the glass object. For instance, glass ﬁbres show a much higher strength than ﬂat glass. It became more and more obvious that ﬂaws (or defects) were responsible for the deteriorated strength of glass as compared to the estimated strength.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

136

7 Mechanical Strength of Glass Toughness, Young’s modulus and surface energy2) values for different glasses (Aben and Guillemet, 1993; Barton and Guillemet, 2005). Tab. 7.1

Glass

Kc (MPa m1/2)

E (GPa)

0.74–0.81 0.72–0.82 0.75–0.82 0.85–0.96 0.62–0.73

73 70–74 64–89 83–91 58–65

Silica Soda-lime-silica Borosilicate Aluminosilicate Lead–silicate

z (J m2) 0.65 0.4–1 0.63 0.63 0.44

7.2 Tensile Resistance of Glass

The simplest way to test a glass in tension is in principle to pull a rod or ﬁbre, although one must note that in practice there are several difﬁculties in gripping the specimens. Three- and four-point bending is often used as well as biaxial ﬂexure and brasilian or diametral compression tests (Zhou et al., 2006). The latter allows generation of a tensile zone into the specimen (Le Bourhis, 1996). Except for ﬁne and long ﬁbres (Appendix 6) where gripping problems can be solved, one should make the central and tested zone smaller in diameter on using uniaxial tensile tests so that failure happens from the ﬁbres and not at the grips. Glass is a so-called brittle material at temperature well below Tg and deforms elastically until fracture (Fig. 7.1). In the elastic domain (domain 1) the uniaxial tensile loading curve s(e) of a glass specimen is then linear.1)

Fig. 7.1 (a) Tensile stressed specimen; (b) s–e tensile curve. Domain 1, slope is Young’s modulus E. Domain 2 corresponds to fracture. sf and ef ¼ sf/E are the stress and strain at rupture respectively. 1)

2)

Deviation from Hooke’s law is observed under elevated strains (10%). Glass becomes either stiffer (silica, germania) or less stiff (SLS; Hillig, 1962; Krause et al., 1979). Such elevated strains can be commonly obtained in coated ﬁbres (Shiue et al., 1996). Native surface (see Chapter 5). Considering that Gc ¼ Kc2/E is the energy release on fracture,

one ﬁnds with E ¼ 70GPa and K ¼ 0.7 MPa m1/ , Gc ¼ 7 J m2, that is, one order of magnitude larger than the actual value. This discrepancy is attributed to the rearrangement (relaxation) of the surface after breakage. Another reason might be the dissipation of energy in the plastic zone conﬁned at the crack tip (see Section 7.4). 2

7.2 Tensile Resistance of Glass

Stress s is written s ¼ Ee

where e is the elastic strain and E the elastic modulus (Young’s modulus). A larger value of E means a stiffer material, that is, a larger resistance to elastic deformations. While the material deforms along the loading axis, also a side deformation is induced the amplitude of which depends on the Poisson ratio (Appendix 9). Elastic modulus depends on glass composition and reﬂects both the interatomic bonding strength and connectivity of the network (packing density). The moduli of glasses are observed to increase together with the glass transition temperature (Fig. 7.2a). Metallic glasses

Fig. 7.2 (a) Young’s modulus E (at 293 K except for amorphous ice at 77 K) as a function of transition temperature (according to Rouxel, 2006); (b) Young’s modulus E of silicate glass as a function of modiﬁer concentration (according to Scholze, 1991).

137

138

7 Mechanical Strength of Glass

while showing transition temperatures below those of oxide glasses show much higher Young’s modulus because of their higher packing density (Cg 0.7 as compared to 0.5 for common glasses; Chapter 5). When modiﬁers are introduced into the oxide glasses network, these atoms locate in the excess volumes while they weaken the network inducing NBO. These two phenomena play opposite roles. The resulting trends in silicate glass are shown in Fig. 7.2b demonstrating that the latter phenomenon is predominant since moduli of silicate glasses are observed below that of silica whatever the introduced alkali. The softening of the glass is more pronounced for a modiﬁer having less Dietzel ﬁeld intensity or for a modiﬁer that is expected to show weaker interaction with oxygen (see Chapter 5) as seen in Fig. 7.2b. In contrast to a modiﬁer, B2O3 oxide participates in the glass network and allows for maintaining and or even increasing Young’s modulus (Livshits et al., 1982). The elastic domain is terminated by catastrophic failure, the area under the linear curve corresponding to the elastic energy. Metallic glasses allow large elastic energy storage since they present elevated strengths. Failure is a dramatic event that has to be prevented. As discussed in Chapters 6, thermal and chemical tempering have been developed to strengthen glass articles. This issue is discussed in Section 7.7. In practice, thestress ﬁeld is much more complexthan in thespecimen studiedhere underuniform and uniaxial tensile stress. Fracture will happen in tensile stressed zones. Hence, it is of utmost importance to understand fracture in order to improve strength and predict the domain where glass articles can be used safely. As we discuss now, fracture depends on intrinsic properties but more importantly on extrinsic ones (process-induced and damage-induced ﬂaws) that make the problem very complex. Having all these parameters in mind, ﬁnite element analysis (FEA) can be carriedoutto predict the behaviour of glazing under realistic and complex loading conditions (Appendix 11). Failure originates from a defect in the glass generally at the surface of the specimen. We reject here bubbles as an origin since these can be avoided nowadays in industrial processes thanks to ﬁning or control operations (Chapters 10 and 11). As stated above, when we assume there is no defect in the glass and fracture originates from individual bonds, then tensile strength values are predicted to be much higher than those observed (Section 7.1 and Appendix 5). In fact, fracture starts at a critical defect or ﬂaw and further propagates. The ﬂaw at the origin of fracture can be easily detected in a ﬂat glass among the broken pieces because it is surrounded by a smooth mirror zone (Fig. 7.3) the extension of which allows empirical determination of the level of stress at failure (Aben and Guillemet, 1993; Carre´, 1996). This phenomenon has been of much help in detecting the origin of spontaneous fracture and to develop a treatment against NiS inclusions instability (Chapter 9; Barry et al., 1998). Stress at pﬃﬃ rupture is determined from sr ¼ M= r , with M the mirror constant and r the mirror radius. M is about 2 MPa m1/2 for a silico-soda-lime glass. This equation is of considerable practical importance since it allows estimation of fracture stress without having to measure it directly. This is very useful in complex shaped glass articles. In Fig. 7.3 the superﬁcial origin can be easily located at the glass edge surface (on the top surface shown in the photograph). The crack expands ﬁrst at a low speed creating ﬂat or mirror-like surfaces. At higher speeds, rougher, less reﬂective surfaces are formed, a ‘mist’ area being observed around the mirror zone. Finally very rough and irregular

7.2 Tensile Resistance of Glass

Fig. 7.3 Origin of fracture observed at the centre of the mirror zone (white bar is 1 mm long).

faceted surfaces form the so-called ‘hackle’ area. Further expansion of the crack yields crack branching that is a multiplication of the number of cracks. Surface origin of fracture is further conﬁrmed by etching the glass surface (Pavelchek and Doremus, 1974). It was also realized for a long time that a ﬁre-ﬁnished surface presented a higher strength than a polished one although this effect was not permanent, because of further surface damage after a period of time. Experiments carried out with hydroﬂuoric acid (HF) reveal that strength does not increase much when etch depth is less than 1–2 mm (Doremus, 1994). As the etch process is continued, some samples show great strength presumably because they are etched free of original ﬂaws and fracture starts from shallow ones. The way superﬁcial ﬂaws are generated in a ﬂat glass under a contact is extensively discussed in Chapter 8. Flaw generation may happen in the production line and in use. The nature of the ﬂaws in glass ﬁbres is more controversial. It is observed that ﬁbre strength approaches the ultimate strength and hence ﬂaws are to be searched for at the microstructural scale. They might be microscopic bubbles which are difﬁcult to eliminate. Fining period (Chapter 10) would be too short as compared to the long period of time required to eliminate the smallest bubbles that are the slowest in rising to the melt surface (Appendix 4). Melting or ﬁning operations are continued until visible bubbles are detected but invisible bubbles might still remain. Moreover, the glassy state presents a liquid-like structure, with a characteristic ﬁctive temperature (Chapter 6) close to the glass transition temperature, or a structure frozen at the glass transition. The glass presents, as detailed in Chapters 5 and 6, an open structure giving rise to microscopic ﬂaws. Moreover, glass ﬁbre is quenched at much larger cooling rates than a ﬂat glass because of a higher surface to volume ratio. Fibre ﬁctive temperature is hence higher than that of a ﬂat glass and presents a more open structure. Let us consider a specimen containing a ﬂaw of size 2a loaded under a uniform tensile stress s (Fig. 7.4). It will fail when stress concentration (stress intensity factor, SIF) pﬃﬃﬃ K ¼ sY a

ð7:2Þ

139

140

7 Mechanical Strength of Glass

Fig. 7.4 Schematic representation of a specimen under tensile loading containing a ﬂaw with extension 2a. Tab. 7.2

Y for most used crack geometry.

Y pﬃﬃﬃﬃﬃﬃﬃ ðpÞ pﬃﬃﬃﬃﬃﬃﬃ 1.12 ðpÞ pﬃﬃﬃﬃﬃﬃﬃ 2/ ðpÞ

Crack geometry Straight crack in inﬁnite specimen Edge crack in semi-inﬁnite specimen Penny crack in inﬁnite specimen

reaches a critical value called fracture toughness Kc that is related to Young’s modulus pﬃﬃﬃﬃﬃﬃﬃﬃ and surface energy by Kc ¼ 2Ez.3) Y is a geometrical factor depending on the ﬂaw pﬃﬃﬃﬃ geometry that can be found in Sih (1972) and Schzalke (1981). We take usually Y ¼ p valid for a straight crack in an inﬁnite specimen (Table 7.2). Equation 7.2 is written at failure as pﬃﬃﬃ Kc ¼ sf Y a ð7:3aÞ or Kc sf ¼ pﬃﬃﬃ Y a

ð7:3bÞ

The criterion of Eq. (7.3a) corresponds to an energy balance between the energy required to form two surface energy 2za and that elastically released Ya2 s2 =2E as detailed below. Equation (7.3b) shows that fracture stress amplitude increases with the toughness and decreases with the ﬂaw size. We assume that there are no residual stresses (glass being fully annealed). Otherwise, these contribute negative stress intensity factor when compressive 3)

This relation can be rewritten in terms of critical pﬃﬃﬃﬃﬃﬃﬃﬃﬃ mechanical energy release rate Gc: Kc ¼ Gc E (Lawn, 1993). Gc is the energy required to create two new fracture surfaces and for ideally brittle materials is 2z, where z is the surface energy per unit area. Plane stress conditions (for a thin

plate; see also Appendix 9). Under plane strain conditions (for a thick plate) rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Gc E Kc ¼ 1 v2

7.3 Stress Concentration and Griffith Energy Balance

Fig. 7.5 Schematic representation of the three modes of fracture, namely modes I, II and III.

(Kr < 0; see Section 7.7). Furthermore, we considered mode I corresponding to the opening of the ﬂaw that is most commonly observed as compared to modes II and III corresponding respectively to sliding and ‘tearing’ (Fig. 7.5). From here onward, we only consider mode I and note the fracture toughness Kc. Table 7.1 reports the toughness value at room temperature for different oxide glasses. These values are within a small range 0.7–0.8 MPa m1/2 (see also Chapter 2 for comparison with other materials). In contrast, metallic glasses show high toughness 50 MPa m1/2 and can be deformed at low temperature ( b) is

141

142

7 Mechanical Strength of Glass

Fig. 7.6 Strength sf as a function of critical ﬂaw dimension a (Kc ¼ 0.7 MPa m1/2, Y ¼ Hp). Damaging the glass surface yields reduced performances (see also Chapter 8).

present in a beam submitted to uniform tensile stress s. The ﬂaw concentrates stresses at the points of minimum curvature, and the maximum stress s0 is given by s0 ¼ sð1 þ 2a=bÞ

ð7:4Þ

If one considers a shape factor a/b of about 4.5, Eq. (7.4) tells us that stress concentration reaches s0 /s ¼ 10. Hence, the stress s0 at the minimum curvature is one order of magnitude larger than the uniform applied stress s. This simple calculation shows that stress concentration may reach very high values when the ﬂaw

Fig. 7.7 Elliptical ﬂaw of semi-axes a and b in a beam under uniform tensile stress s.

7.3 Stress Concentration and Griffith Energy Balance

tip becomes sharper. Fracture will then extend at the ﬂaw tip and further propagate until specimen fracture. 7.3.2 Energy Balance

Further understanding of fracture is accomplished considering the total energy of the fractured specimen U. U is the sum of the mechanical Um and surface Us energies: U ¼ Um þ Us

ð7:5Þ

When fracture propagates a distance da the energy change is dU ¼ dUm þ dUs ¼ Gda þ dUs

ð7:6Þ

where G is the mechanical energy release and dUs the variation in energy induced by creation of new surfaces. Equilibrium is written dU=da ¼ 0 ¼ Gc þ dUs =da

ð7:7Þ

where Gc is the critical mechanical energy release. Considering, as Inglis (1913) did, an inﬁnitely narrow elliptical ﬂaw (b ! 0), we have per unit width along the crack front (in fact two fronts) Um ¼ G¼

pa2 s2 E

dUm dðpa2 s2 =EÞ ¼ 2da 2da

ð7:8Þ ð7:9Þ

while Us ¼ 4az

ð7:10Þ

Total energy is U¼

pa2 s2 þ 4az E

ð7:11Þ

Both terms (Um and Us) are plotted in Fig. 7.8. Us varies linearly and dominates for small crack size values. In contrast, for large crack sizes, Um dominates and the total energy passes through a maximum (dU/da ¼ 0) that allows determination of equilibrium for rﬃﬃﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2Ez EGc sf ¼ ¼ ð7:12Þ pa pa Over this value catastrophic failure happens.

143

144

7 Mechanical Strength of Glass

Fig. 7.8 Energy of an inﬁnitely narrow elliptical ﬂaw under uniform tensile stress s. Crack equilibrium corresponds to U maximum (z ¼ 1 J m2, E ¼ 70 GPa, s ¼ 2 MPa).

7.4 Linear Elasticity Crack Tip Stress Field

Considering mode I, the stress ﬁeld at the crack tip proximity is determined to be (Irwin, 1958; Paris and Sih, 1965; Fig. 7.9) 0

sx

1

0

cosðu=2Þ½1 sinðu=2Þsinð3u=2Þ

1

K B C B s C pﬃﬃﬃﬃﬃﬃﬃﬃ @ yA¼ @ cosðu=2Þ½1 þ sinðu=2Þsinð3u=2Þ A 2pr txy sinðu=2Þcosðu=2Þcosð3u=2Þ

Fig. 7.9 (a) x, y axis and stress components; (b) schematic representation of stress concentration at crack tip (dashed line) and inﬂuence of a plastic zone (continuous line).

ð7:13Þ

7.5 SIF under Non-uniform Stress

This reduces to si j ¼ Kð2prÞ1=2 fi j ðuÞ

ð7:14Þ

showing stress concentration at the proximity of the crack tip with dependence of the form r1/2. It should be noted that a mathematical singularity is obtained at r ¼ 0 because the tip extremity curvature radius was taken as 0. We have not considered that stress concentration may induce a conﬁned plastic deformation that shifts the singularity (Fig. 7.9b). Using the Dugdale (1960) model one may estimate the size l of the plastic zone at the crack tip to be p Kc 2 l¼ 8 Y

ð7:15Þ

where Y is the yield stress. For a soda-lime-silica glass (Kc ¼ 0.7 MPa m1/2, Y H/ 3 2 GPa; Appendix 8) one ﬁnds a plastic zone at the tip extremity of size l 50 nm. This very small value is to be compared to that obtained for a metal: l 1 mm. This result emphasizes the actual brittle behaviour of glass since, contrary to a metal, only a few bonds at the crack tip support the elevated stress concentration. The presence of a plastic zone at the crack tip has been until recently quite speculative given the relevant length scale. Using atomic force microscopy (AFM), Creuzet et al. (1993) could measure the deformation of a glass specimen at the emergence of a crack (or the topography of the surface at crack emergence). They showed that the experimental results in the vicinity of crack emergence were not in agreement with linear elasticity. More recently Ce´larie´ et al. (2003) suggested that ‘Glass breaks like metal, but at a nanometer scale’, although further experimental evidences are demanded (Guin and Wiederhorn, 2004). Furthermore, Mattoni et al. (2005) emphasize that for very a short crack it is difﬁcult to discriminate between bond breaking and incipient plasticity yielding departure from classic Grifﬁth theory.

7.5 SIF under Non-uniform Stress

To this point we supposed the specimen was uniformly loaded. Instead let us consider a straight crack (0 < x < a) in an inﬁnite specimen under a varying stress s(x) normal to the crack surface. SIF is given by pﬃﬃﬃ ða 2 a sðxÞ K ¼ pﬃﬃﬃﬃ dx p ða2 x 2 Þ1=2 0

ð7:16aÞ

145

146

7 Mechanical Strength of Glass 1=2

The term 1=ða2 x 2 Þ can be considered as a weight factor on stress s(x) and is called the Green’s function. It maximizes at the crack tip vicinity. For a uniformly loaded specimen one ﬁnds again (taking for the integration x/a ¼ sin d) pﬃﬃﬃ ða pﬃﬃﬃﬃpﬃﬃﬃ 2 a dx K ¼ pﬃﬃﬃﬃ s ¼s p a 1=2 2 2 p ða x Þ

ð7:16bÞ

0

For an edge crack in a semi-inﬁnite specimen, the integration is to be corrected with Y ¼ Hp replaced by 1.12Hp (Table 7.2): K¼

pﬃﬃﬃ ða 2Y a sðxÞ dx p ða2 x 2 Þ1=2

ð7:16cÞ

0

7.6 Toughness Measurement

Toughness measurements require that specimens are prepared with care introducing a sharp crack of known size a. As detailed below, glass is characterized by a distribution of ﬂaws that yields statistical fracture, the introduced crack being the critical one from where fracture initiates. Different loading modes are used and give their name to the related methods. When increasing the applied load F, stress concentration increases and yields crack growth. Stress concentration reaches toughness value at rupture. Stress concentration K as a function of applied load is given for the three main loading geometries, a being the crack length, and b, L and e being geometrical factors (Fig. 7.10). 7.6.1 Compact Tension

Under compact tension (CT) stress concentration is K¼

pﬃﬃﬃ a2 a3 a4 F a a 1:017 þ638:6 29:6 185:5 þ 655:7 be b b b b

ð7:17aÞ

7.6.2 Notch Beam Test

For the notch beam test (NBT or SENB) stress concentration is pﬃﬃﬃ a2 a3 a4 3FL a a 1:96 2:75 þ 13:66 K¼ 23:98 þ25:22 b b b b 2b2 e

ð7:17bÞ

7.6 Toughness Measurement

Fig. 7.10 Specimens for toughness measurement and loading conditions.

7.6.3 Double Torsion

Under double torsion (DT) stress concentration shows no dependence on introduced ﬂaw size a and is 3ð1 þ nÞ 1=2 K ¼ Fb Le4

ð7:17cÞ

All expressions show a linear variation of the stress intensity factor K with the applied force F. Interestingly on loading the specimens, the crack propagation can be measured in a domain where K < Kc, that is, before catastrophic failure. This domain

147

148

7 Mechanical Strength of Glass

is referred to as the subcritical domain. Subcritical crack growth has important implications on the ageing of glass, that is, its behaviour with time. This issue is addressed extensively in Chapter 9. It should also be noted that an indentation method may be employed to determine toughness when small quantities of material are available. This issue is discussed in more detail in Chapter 8.

7.7 Inﬂuence of Residual Stress on Strength and Fragmentation

As mentioned above, compressive residual stresses contribute negative SIF (Kr < 0). Stress concentration superimposes; hence we have pﬃﬃﬃ K ¼ sY a þ Kr

ð7:18aÞ

Also, fracture happens when the stress intensity factor K reaches the critical value Kc: pﬃﬃﬃ Kc ¼ sf Y a þ Kr

ð7:18bÞ

pﬃﬃﬃ Equation (7.18b) is sometimes rewritten in the form T ¼ sf Y a ¼ Kc Kr with T the apparent toughness including the residual stresses as a part of the crack resistance of the material. For compressive residual stresses (Kr < 0) there is a beneﬁcial effect on T. Equation (7.18b) can be written (for compressive stresses we take the absolute value) sf ¼

Kc Kr Kc þ jKr j pﬃﬃﬃ ¼ pﬃﬃﬃ Y a Y a

ð7:19Þ

Hence, for compressive residual stresses, fracture happens under greater applied stresses than for the residual stress-free state. In fact, tempering is used commonly to strengthen the glass surface. As discussed in Chapter 6, compressive stresses build at the surface and are equilibrated by tensile stresses in the core of the glass. Therefore, breakage happens either (i) when tensile applied stresses allow for Eq. (7.19) to reach the critical value sf at a critical ﬂaw present most probably at the surface (see also Section 7.8 and Chapter 8) or (ii) when an impact-generated ﬂaw reaches the tensile zone (Fig. 7.11). The latter situation corresponds to complex loading and complex

! Fig. 7.11 High-speed photographic sequence showing the catastrophic failure of a thermally tempered soda-lime-silica glass block caused by the impact of a 2 mm diameter tungsten carbide sphere at a velocity of 150 m s1. The fringes are isochromatics, the arrow points to the black fringe, which marks the region of zero stress

(see Chapter 11). The catastrophic failure begins in frame 4. Note the change in shape of the stress pattern as well as the bifurcation of the cracks in frames 6 to 12. Surface compressive stresses are 200 MPa, inter-frame time is 1 ms. (Reprinted from Chaudhri and Liangyi, 1986, with permission from Macmillan Publishers Ltd.)

7.7 Influence of Residual Stress on Strength and Fragmentation

149

150

7 Mechanical Strength of Glass

fracture path as revealed by high-speed photography (Fig. 7.11). This is discussed in Section 7.7.4. Let us consider ﬁrst situation (i) with a critical ﬂaw present at glass surface either in a thermally or chemically tempered glazing, or under slowly and rapidly varying residual stresses respectively (Figs. 6.25 and 6.36). We suppose the glazing is stressed uniformly and illustrate then the beneﬁcial role played by strengthening since applied stress at rupture increases accordingly. 7.7.1 Inﬂuence of Residual Thermal Stress on Strength

Thermal residual stress varies slowly with depth. We suppose it can be considered constant over crack length. We suppose cracks are present at the glass surface and take pﬃﬃﬃ the residual stress equal to the surface compressive stress; hence Kr ¼ ss Y a (ss < 0). We may consider crack length is negligible as compared to glass thickness a tH so pﬃﬃﬃﬃ that Y ¼ 1:12 p (valid for an edge crack in a semi-inﬁnite solid). Stress at rupture is Kc Kc sf ¼ pﬃﬃﬃ ss ¼ pﬃﬃﬃ þ jss j Y a Y a

ð7:20Þ

Therefore, strengthening at the glass surface is directly related to the amplitude of the residual surface stresses. This means that thermally tempered glazing strength is shifted by the thermal residual surface stress amplitude.

7.7.2 Inﬂuence of Residual Chemical Stress on Strength

Chemical residual stresses vary much more rapidly with depth than thermal residual stresses. Let us suppose the compressive stress varies linearly and is null at a depth h (so-called exchanged depth; Chapter 6). Then, residual stress variation with depth z0 (¼ tH/2 z) is written sr ¼ (1 z0 /h)ss. We have (Section 7.5) pﬃﬃﬃ ða pﬃﬃﬃ ða 2Y a sr ðz0 Þ 2Y a ss ½1 ðz0 =hÞ 0 0 Kr ¼ dz ¼ dz p p ða2 z02 Þ1=2 ða2 z02 Þ1=2 0 0 pﬃﬃﬃ 2a ¼ Y ass 1 ph

ð7:21Þ

Finally stress at rupture is Kc 2a Kc 2a ¼ pﬃﬃﬃ þ jss j 1 sf ¼ pﬃﬃﬃ ss 1 ph ph Y a Y a

ð7:22Þ

7.7 Influence of Residual Stress on Strength and Fragmentation

Again, we ﬁnd that stress at rupture increases with the residual stress amplitude. In the case of chemical tempering, not only the stress level is to be considered in evaluating the beneﬁcial role of residual stresses, but also the treated layer thickness through the a/h ratio that plays an important role. This results from the fact that the superﬁcial ﬂaw size is not negligible as compared to the exchange depths reached under commercially available conditions. In fact, let us consider a high exchanged depth for which a/h ! 0. Then stress at rupture can be approximated by pﬃﬃﬃ sf ðKc =Y aÞ þ jss j and we obtain a result similar to that obtained for thermal tempering. 7.7.3 Inﬂuence of Residual Stress on Fragmentation

On breakage, release of tempering-induced elastic energy happens. When crack speed approaches half the Raleigh wave speed, it is possible for the crack to split into multiple branches (Fig. 7.11). Crack multiplication allows for dissipating more energy since more surfaces are generated. This phenomenon happens for a critical value of SIF about four times Kc (around 3 MPa m1/2 for a silico-soda-lime glass). Akeyoshi et al. (1967) showed that the density of the fragments generated on breakage is to be related to the level of residual stresses (degree of temper) (Fig. 7.12). It has been argued that the elastic energy stored in the tensile zone is the parameter controlling the glass breaking (Bouyne and Gaume, 2001).

Fig. 7.12 Fragment densities (in a 5 5 cm2 area) as a function of residual tensile stress (according to Akeyoshi et al., 1967).

151

152

7 Mechanical Strength of Glass

The number of fragments increases with residual stress level and the thickness of the glass sheet, that is, the amplitude of elastic energy stored during the tempering process. Akeyoshi et al. (1967) carried out extensive experimental tests to determine the fragment densities in broken samples of different thickness and tempering degree. They produced a map showing the fragment density as a function of tensile core residual stress amplitude for commercially available ﬂat glass thicknesses. This map is still in use and allows for determination and control of residual stresses in ﬂat glass. A glass article is taken from the batch and fractured. The fragment density is then determined and residual stress amplitude extracted from the Akeysohi et al. chart. This control is demanded to ﬁt the R43 international standard for tempered automotive glazing. Not only must tempering produce strength, but also on breakage the residual stresses are to be designed so that harmless fragments are generated. The R43 standard ﬁxes the number of glass fragments in all 5 5 cm2 areas to be over 40 and below 400. Such a control of the residual stresses is destructive and nondestructive methods are preferred (Chapter 11). Notably, the Akeyoshi et al. (1967) approach for thermally tempered glasses can be generalized to chemically tempered glasses (Bouyne and Gaume, 2001). The consequence of the above results is that toughened glass cannot be cut or otherwise modiﬁed in shape as this would disturb the system of prestresses, and with fracture beginning at any point in the glass, the whole sheet would shatter immediately into small (although harmless) fragments. Hence, glass tempering is carried out ofﬂine after cutting, drilling and edge grinding operations.

7.7.4 Impact-Induced Fracture

There has been little experimental work dedicated to the way an impact crack generates and further enters the tensile region causing fracture. Figure 7.11 is hence of much interest as it shows a high-speed photographic sequence in crosssection of a thermally tempered soda-lime-silica glass impacted by a hard sphere thrown at 150 m s1 towards its surface. The dark fringe corresponds to zero stress (these are photoelastic images; see also Chapter 11). As the sphere impacts the block, stress ﬁeld changes as revealed by the photoelastic survey of the zone (frames 1–3). Interestingly between frames 4 and 5 the cracks enter the region of tensile stress and this leads to the initiation of catastrophic failure of the sample. The cracked area is observed as a dark and growing surface as time increases. The velocity of the cracks depends on the direction they propagate. The velocity of the cracks moving towards the surface of the impact is much smaller (200–300 m s1) than the velocity of the cracks spreading along the loading axis. In frames 7–12 cracks further spread and bifurcate, the images showing chaotic features. In fact, ﬁnite element analysis (FEM) happens to be of great help in getting insight into impact failure (Appendix 11) while we further discuss crack initiation under contact loading in Chapter 8.

7.8 Statistical Weibull Analysis

7.8 Statistical Weibull Analysis 7.8.1 Introduction

The strength of a glass and more generally of a brittle material depends on its toughness Kc that is generally known and the critical ﬂaw size a that depends on the industrial process and use, the ultimate stress being extracted from the following relationship (Section 7.2): pﬃﬃﬃ Kc ¼ sf Y a

ð7:23Þ

Therefore, the determination of the glass mechanical performance requires the knowledge of ﬂaw population which has to be determined statistically. Weibull (1951, 1952) statistics has been commonly used to characterize the statistical variation of the fracture strength of brittle materials such as ceramics, glasses and solid catalysts. It is based on the ‘weakest link theory’ which means that the most serious ﬂaw in the material will control the strength, like a chain breaking if its weakest link fails (Fig. 7.13). The most serious ﬂaw is not necessarily the largest one because its severity also relies on its location and orientation. In fact, strength is controlled by the ﬂaw subjected to the highest SIF. 7.8.2 Functional Formulation

We must consider that ﬂaws are distributed into the specimens. We shall suppose that the probability that two independent events occur is the product of the respective probabilities (Kittl and Diaz, 1988). Let us consider a volume V of the specimen and decompose it into two smaller volumes V1 and V2: V ¼ V1 þ V2

Fig. 7.13 Loaded chain of n links. The chain fails from its weakest link.

ð7:24Þ

153

154

7 Mechanical Strength of Glass

Ps(V, s) is the probability that a given volume V resists the stress s. We have Ps ðV; sÞ ¼ Ps ðV1 þ V2 ; sÞ ¼ Ps ðV1 ; sÞPs ðV2 ; sÞ

ð7:25Þ

Using this relationship for a volume of V + DV allows one to write Ps ðV þ DV; sÞ ¼ Ps ðV; sÞPs ðDV; sÞ

ð7:26Þ

while we have also Ps ðV þ DV; sÞ ¼ Ps ðV; sÞ þ Ps0 ðV; sÞDV

ð7:27Þ

Thereafter we have Ps0 ðV; sÞ ¼ ½Ps ðV þ DV; sÞ Ps ðV; sÞ=DV

ð7:28Þ

Using Eq. (7.26), Eq. (7.28) becomes Ps0 ðV; sÞ ¼ ½Ps ðV; sÞPs ðDV; sÞ Ps ðV; sÞ=DV

ð7:29Þ

Ps0 ðV; sÞ=Ps ðV; sÞ ¼ ½Ps ðDV; sÞ 1=DV

ð7:30Þ

Then

which for DV ! 0 becomes Ps0 ðV; sÞ=Ps ðV; sÞ ¼ Ps0 ð0; sÞ ¼ FðsÞ=Vo

ð7:31Þ

where F(s) is the risk function for stress s and Vo a unit volume. Equation (7.31) is integrated as follows: ð lnPs ðV; sÞ ¼ V

FðsÞ dV Vo

ð7:32Þ

so that 0

1 FðsÞ Ps ðV; sÞ ¼ [email protected] dV A Vo ð

ð7:33Þ

V

Weibull suggested the following risk function: m 8 > < s su s0 FðsÞ ¼ > : 0

s su 0 s su

ð7:34Þ

7.8 Statistical Weibull Analysis

where su is the stress for which the probability for rupture is null, and is taken as su ¼ 0 for a brittle material, and m is the Weibull modulus. Therefore we have FðsÞ ¼

s s0

m ð7:35Þ

We have to consider two situations to integrate Eq. (7.33): stress is either uniform (Section 7.8.2.1) or not uniform (Section 7.8.2.2). 7.8.2.1 Uniform Tensile Stress Under uniform tensile stress (for instance in a uniaxially tensile stressed ﬁbre) Eq. (7.33) becomes V s m Ps ðV; sÞ ¼ exp Vo so

ð7:36Þ

This is the most commonly used form of Weibull resistance probability. Parameter m is called the Weibull modulus and is indicative of strength scatter; so is indicative of strength level and corresponds to fracture stress with a failure probability of 63.2%. It is closely related Ð 1 to the mean strength sm of the distribution by sm ¼ soG(1 þ 1/m), with GðxÞ ¼ 0 et tx1 dt (see also Appendix 8). For a Weibull modulus in the range of 10 typical for ceramics, G(1 + 1/m) is about 0.9 to 1. 7.8.2.2 Non-uniform Tensile Stress When stress varies in the volume of the material, Eq. (7.33) becomes 0

1 2 3 ð m FðsÞ 1 s Ps ðV; sÞ ¼ [email protected] dV A ¼ exp4 dV 5 Vo Vo s o ð V

ð7:37Þ

V

Integration of Eq. (7.37) requires knowledge of the stress ﬁeld. Let us consider for instance a beam under ﬂexure (Chapter 2; Fig. 7.14). Stress changes from compressive at the top surface to tensile at the bottom surface. The neutral line is where stress amplitude vanishes (Appendix 7). Accordingly, the stress

Fig. 7.14 Beam under ﬂexure.

155

156

7 Mechanical Strength of Glass

ﬁeld is written 0

z l=2 x B tH =2 l=2 B sðx; zÞ ¼ sM B @ z l=2 þ x tH =2 l=2

for x 2 ½0; l=2 ð7:38Þ for x 2 ½l=2; 0

where sM is the maximum stress (at the beam surface). Integration on volume V (in fact considering only the so-called tensile zones) yields4) "

m # V 1 sM Ps ðV; s Þ ¼ exp Vo 2ðm þ 1Þ2 so 0

ð7:39Þ

Equations (7.36) and (7.39) were obtained using the same risk function. However, one notes that for the same given applied stress (tensile stress s equal to maximum ﬂexure stress sM) the probability that the specimen resists is higher under ﬂexure. This is further discussed below and results from an intrinsic size effect, the maximum tensile stresses being applied to only a small part of the bent specimen. 3)

Crack opening happens in tensile zones. Since stress is tensile for z 2 ½tH =2; 0 integration is over half of the beam volume. The beam volume V is V ¼ lwtH . We have 2 3 ð m 1 s dV 5 Ps ðV; sÞ ¼ exp4 Vo s o V

ð V

ððð

m

s so

dV ¼ V

s so

m

ð0

0 w=2 0

ð V

s so

m

dV ¼ 2

ð

V

s so

m

dV ¼ 2w

s so

sM 1 1 so tH =2 l=2

¼ 2w

m

m dxdydz

m dxdydz:

m

sM 1 1 so tH =2 l=2

sM so

s so

l=2w=2 0

l=2 ð w=2 ð tHð=2

þ

w=2 ð tHð=2

dxdydz ¼

m

ðl=2 xÞmþ1 mþ1

l=2 mþ1 tH =2 z w mþ1 0 0

ðl=2Þmþ1 ðtH =2Þmþ1 ðm þ 1Þ2

ðl=2ÞðtH =2Þ 2

ðm þ 1Þ

¼

V 2

2ðm þ 1Þ

m V 1 sM : then Ps ðV; sÞ ¼ exp 2 Vo 2ðm þ 1Þ so

sM so

m

7.8 Statistical Weibull Analysis Tab. 7.3

Weibull modulus for different classes of materials.

Material

Weibull modulus

Glass container, ﬂat glass Glass ﬁbre Ceramics Metals

3–7 10–30 10 40

7.8.3 Population of Flaws

Glass specimens present a ﬂaw size distribution. The determination of ﬂaw population passes through an experimental study of a representative series of samples that are to be tested. Weibull statistics is subsequently used to ﬁt the resistance probability Ps(V) as a function of stress (Appendix 6). Weibull statistics is also applied extensively for studying brittle fracture even at the nanoscale (Pugno and Ruoff, 2006) as well as the interfacial rupture (Piellard, 2005). The scatter of ﬂaw size distribution and of the fracture strength is indicated by the so-called Weibull modulus m (Table 7.3). From an engineering point of view, a high Weibull modulus can be as important as a high strength. A higher m value leads to a steeper ﬂaw size distribution and thus to a lower dispersion of the fracture strength (Fig. 7.15). Interestingly a glass edge can be carefully abraded to obtain m as high as 10 (Barton and Guillemet, 2005). The highest Weibull moduli for glasses are obtained from ﬁbres that can be produced almost ﬂawfree, m approaching 30 and tensile strength being close to the intrinsic one. Modern

Fig. 7.15 Weibull probability Ps(Vo) to resist stress s (so ¼ 1 GPa). Three different Weibull moduli have been considered (m ¼ 10, 25 and 100).

157

158

7 Mechanical Strength of Glass

Fig. 7.16 Weibull probability to resist stress s (so ¼ 1 GPa, m ¼ 25). Three volumes have been considered (V/Vo ¼ 1, 10 and 100).

fused silica optical communications ﬁbres show m in the range 30–100! Some authors argued that the variation observed for m > 30 could result only from section variation of the studied ﬁbre. The ‘intrinsic’ strength of silica ﬁbre would then be about 12 GPa, close to the theoretical strength determined in Section 7.1. Let us consider uniformly stressed specimens; we have V s m Ps ðV; sÞ ¼ exp Vo so

ð7:40Þ

When larger specimens are considered (size effect from laboratory to practical application) the probability that the sample resists stress s is Ps ðV; sÞ ¼ Ps ðVo ; sÞn with V ¼ nVo

ð7:41Þ

Figure 7.16 plots the probability Ps(V, s) for increasing sizes (namely V/Vo ¼ 1, 10 and 100) where mean strength is observed to decrease accordingly. Size effect is indeed inherent to brittle fracture. The load applied to lead the specimen to fracture decreases as the volume of the tested specimen increases because of the greater probability of containing dangerous ﬂaws. A corollary to this is that higher average strength values are always observed in bending than in tensile tests, because the maximum stresses are applied to only a small part of the bent specimen (Sections 7.8.2.1 and 7.8.2.2). Here, we suppose that residual stresses are null. If not, the situation is then even more in favour of bending resistance since superﬁcial residual stresses are compressive. Whenever critical ﬂaws can be supposed to locate at the surface as for ﬂat glass

7.8 Statistical Weibull Analysis

(because of contact damage; see Chapter 8) the difference becomes less. When a ﬁbre is considered, longitudinal and transversal size effects are expected. This statistical behaviour has very important technological consequences: i. Diameter size effect could provide a way of improving strength by obtaining ﬁner ﬁlaments. Composites formed from ﬁbre embedded in a polymer matrix are of interest in view of the outstanding ﬁbre strength as compared to ﬂat glass. ii. If signiﬁcant enough, size effect could be used to perform accelerated testing increasing size. iii. Wide difference may arise from small-scale laboratory specimens to larger structures. So far, quantitative extrapolation methods following the Weibull law are still questioned in the literature (Zinck et al., 1999).

159

161

8 Contact Resistance of Glass 8.1 Sharp and Blunt Contact 8.1.1 Introduction

As detailed in Chapter 7, glass strength depends mostly on ﬂaws (defects) from which cracks develop. The existence of ﬂaws is the reason why glass specimens show a mechanical strength much below the theoretical one. These ﬂaws may be either in the glass bulk like small bubbles remaining after ﬁning operations and crystalline phases (refer to Chapter 10) or at the surface like microcracks generated by the contact between the glass and tools and later in use (Fig. 8.1). These may be generated during the process itself or from handling and service conditions. We address in the present chapter the generation mechanisms of such contact-induced ﬂaws. During the production process the glass follows a complex thermomechanical route involving contact with tools at different temperatures (with the possibility of a thermal gradient between glass and tool), while in use the contact is generally isothermal (both the contactor and glass being at room temperature). As discussed in detail below, over a given threshold the contact is no longer reversible (excursion out of the elastic domain). Non-reversible deformation and cracks can be observed. All these phenomena lead to the introduction of ﬂaws at the glass surface and glass strength is dramatically affected (Gy, 1997). We shall not address chemical reaction with the surface. It is well known that just touching lightly the surface of a pristine silica rod dramatically lowers its strength. For instance, halogen lamp operating notes often recommend no contact between the ﬁngers and the lamp. Microanalysis of fracture origin shows alkali and alkaline earth contaminants. Figure 8.1 shows the dramatic scratches at the internal surface of a used plate. We review the mechanics of such phenomena. Glassmakers have been aware of these phenomena for a long time and coating technology was developed accordingly to protect glass surfaces from erosion and damage either for mechanical or aesthetics purposes (ﬁbre sizing, container hot end treatments; Chapters 10 and 12). More fundamentally, tailoring contact resistance has attracted much scientiﬁc and technological interest and Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

162

8 Contact Resistance of Glass

Fig. 8.1 Scratches on a used glass plate as observed by optical microscopy.

fracture mechanics described here was applied with success to many other types of materials showing brittle fracture (Le Bourhis et al. 2001b; Cook, 2006). In the literature, two schematic contact conditions are generally considered. Blunt contact conditions consider that the material under a sphere deforms elastically up to brittle fracture. In contrast, under a sharp contact glass deforms elastically, plastically and ﬁnally fractures. The term ‘plastic’ is to be considered with caution for glass that is amorphous and ‘plastic’ means irreversible in this context. Glass may deform ‘plastically’ or inelastically below the glass transition temperature when small volumes are highly stressed. Under a sharp contact, pressure scales typically with hardness H that is commonly of the order of some gigapascals, while the deformed zone is elastically constrained by the surrounding volume of the material as discussed below. Experimental tools have been developed using a spherical indenter to produce blunt contact while sharp contact is produced by conical or pyramidal tips as reviewed below. Also, scratch testing allows production of a lateral movement during the contact and hence a frictional force. These testing modes allow to approach real contact conditions. 8.1.2 Spherical Indentation 8.1.2.1 Elastic Loading Figure 8.2 shows a diagram of the elastic loading of a glass surface by a spherical indenter. In such an experiment, a sphere of radius R is loaded under a force F, the contact radius being a. The specimen surface around the contact area also deforms elastically as shown schematically in Fig. 8.2. Load (F)–penetration (h) relationship is known as the Hertz (1881) contact solution: 4 F ¼ R1=2 E h3=2 3 where R is the radius of the tip and E the composite modulus, given by 1 1 n2i 1 n2s ¼ þ E Ei Es

ð8:1Þ

ð8:2Þ

8.1 Sharp and Blunt Contact

Fig. 8.2 Diagram of the elastic loading of a spherical indenter on a glass surface.

where E and n are elastic modulus and Poisson ratio with subscripts i and s referring to the indenter and the specimen respectively. For a diamond tip usually employed in the laboratory, Ei ¼ 1141 GPa, ni ¼ 0.07. For materials much softer than diamond we have 1=E ¼ ð1 n2s Þ=Es , and the indenter can be supposed perfectly rigid. In the general case, the glass and indenter properties are to be considered. When the two materials in contact are identical, a glass against another glass for instance, we have 1=E ¼ 2ð1 n2s Þ=Es , and both the specimen and the indenter deform. Figure 8.3 shows the calculated reversible loading curves of a glass under two spherical diamond indenters with different radii. The smaller the radius, the larger the penetration. The contact radius a is given by a ¼ R

1=3 3 F 4 E R2

Fig. 8.3 Calculated load–penetration curve of a spherical diamond indenter into a standard silico-soda-lime glass surface (E ¼ 72 GPa, R ¼ 1 or 0.1 mm).

ð8:3Þ

163

164

8 Contact Resistance of Glass

Fig. 8.4 Mean pressure as a function of penetration of a spherical diamond indenter into a standard silico-soda-lime glass surface (E ¼ 72 GPa, R ¼ 1 or 0.1 mm).

while the mean pressure p is p ¼ F=Ac ¼ F=pa2

ð8:4Þ

which is zero for F ¼ 0 and progressively increases as load increases (Fig. 8.4). Under usual loading conditions, the mean pressure is found to be well below the yield stress of the glass (Y H/3 2 GPa for an SLS glass; Appendix 8) so that only elastic loading is considered up to fracture. Notably, we can observe that when the sphere radius decreases the mean pressure for a given penetration of the indenter increases (Fig. 8.4). The maximum tensile stress in the specimen occurs at the contact circle: 1 sm ¼ ð1 2nÞ p 2

ð8:5Þ

while the maximum shear stress is located along the loading axis at depth 0.5a below the surface: tm ¼ 0:48 p

ð8:6Þ

8.1.2.2 Hertz Fracture and Indentation Toughness Under a spherical indenter, the mean pressure progressively increases when the applied load increases. Eventually, cone cracks may extend into the material as shown schematically in Fig. 8.5 and revealed experimentally in Figs. 8.6 and 8.7. Outside the contact area, pre-existing ﬂaws are subjected to tensile stress, which at some point (depending on the ﬂaw size) run around the contact forming a surface ring crack that grows downward following the principal stress conical trajectories, while on unloading the cracks close. The fracture usually remains visible because of the imperfect

8.1 Sharp and Blunt Contact

Fig. 8.5 Fracture under a blunt indenter: (a) cone fracture sequence on loading (þ) and unloading (); (b) cone fracture geometry (according to Lawn, 1993).

closure at the crack (Fig. 8.6). Notably, the residual stress ﬁeld changes the crack geometry as revealed in Fig. 8.6b. Also, the load required for generation of cracks of similar size is superior in tempered specimens. In thermally tempered glazing, the skirt of the cone crack is almost parallel to the indented surface, while it is inclined to the surface in an annealed (stress-free) specimen. The crack evolution is depicted schematically in Fig. 8.5 (Lawn, 1993, 1998) with the plus sign indicating loading and the minus sign unloading. Next, let us consider a specimen with small residual stresses. The mechanics of cone crack initiation started with Auerbach (1891). He showed empirically that the critical load to initiate a cone fracture in ﬂat specimens was proportional to the radius of the indenting sphere Fc R. For decades (Tillett, 1956; Lawn, 1993), Auerbach’s law was debated since fracture theory suggests that cracks

165

166

8 Contact Resistance of Glass

Fig. 8.6 Side views of the cone cracks under load in annealed and thermally tempered sodalime glass formed under a 2.5 mm radius steel indenter. Note that the skirt of the cone crack in the annealed glass makes a signiﬁcantly larger angle with the indented surface than that in the

tempered glass (Reprinted from Chaudhri and Phillips, 1990, with permission from Taylor & Francis Ltd. http://www.informaworld.com). (a) load 793 N, cone base 2.4 mm; (b) load 2060 N, cone base 2.85 mm.

initiate at the points where maximum tensile stress in the Hertzian ﬁeld equals the strength of the material. Using Eqs. (8.4) and (8.5) results in an Fc R2 relationship. The paradox was solved taking into account the statistical nature of fracture and showing the so-called Auerbach’s range in a domain where Fc shows an insensitivity to ﬂaw size. Then, the toughness of a glass can be determined using the critical load for crack generation (Auerbach’s law) or the extension of the cracks (Franck and Lawn model) as reviewed by Geandier et al. (2003). The toughness and the critical load are related in Auerbach’s range by (Lawn, 1993; Warren, 1995; Fischer-Cripps, 2004a) Kc ¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ E Fc CR

ð8:7Þ

where Fc is the critical load for cone crack generation, C a constant that has to be calculated for a given material and indenter (Warren, 1995), R the indenter radius and E the composite modulus deﬁned above. For glass contacting glass, C ¼ 3131; it is 2790 for alumina contacting alumina (Warren, 1995).

Fig. 8.7 Top view of ring cracks generated by a sphere (0.2 mm diameter) on the atmospheric side of a ﬂoat glass.

8.1 Sharp and Blunt Contact

In the Frank and Lawn (1967) model, only the cone crack is considered; the initial small circular shaped crack perpendicular to the surface is neglected, due to its small size compared to the cone length. It is assumed that the crack is propagating along the direction of the smallest principal stress (s3) perpendicularly to the maximum principal stress (Hertz stress ﬁeld s1; we suppose no residual stresses) and that the crack presence and propagation do not modify the initial stress ﬁeld. The critical stress intensity factor is then obtained by integration along the crack length c (Fig. 8.5; Section 7.5): rﬃﬃﬃﬃ ðc c s1 ðxÞ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dx Kc ¼ 2 p c2 x2

ð8:8Þ

0

where s1(x) is the Hertzian stress value along the crack (the opening stress normal to crack direction). Interestingly, Chaudhri and Kurkjian 1986 showed that cone cracks also form on dynamic loading with lower cone angles. The cone formed is 468, that is, smaller than that of 62.88 formed under static loading (Chaudhri and Kurkjian, 1986). Moreover, the angle amplitude depends on the Poisson ratio of the studied glass and the residual stresses as discussed above. A typical Hertz fracture obtained after a blunt impact is shown in Fig. 8.8 on a laminated (annealed) windscreen. Even small cracks develop under humid environments as discussed in more detail in Chapter 9 and should be repaired before they damage dramatically the glazing. 8.1.3 Sharp Indentation 8.1.3.1 Elastic Loading Figure 8.9 shows a diagram of the elastic loading of a glass surface by a conical indenter. The approach can be extended to pyramidal tips (Vickers, cube corner, Berkovich 1951) and more generally self-similar tips taking Ac ¼ pa2 ¼ ah2 and neglecting the inﬂuence of the indenter edges. A cone loaded under force F penetrates the specimen down to the penetration depth h, the contact radius being

Fig. 8.8 Hertz fracture on a laminated windscreen.

167

168

8 Contact Resistance of Glass

Fig. 8.9 Diagram of the elastic loading of a conical indenter on a glass surface.

a. Again as for a spherical tip, the specimen deforms elastically around the contact area as shown in Fig. 8.9 (see also Appendix 8). Load (F)–penetration (h) relationship is known as the Sneddon (1965) contact solution and shows a square dependence on penetration (so-called self-similarity or geometrical similarity of the contact): F¼

2 Er h 2 ptanb

ð8:9Þ

where b is the angle between the indenter ﬂank and the specimen surface and Er is the reduced modulus deﬁned as 1 1 n2s ¼ Er Es

ð8:10Þ

where subscript s indicates the specimen. The contact radius a is given by a¼

2h ptanb

ð8:11Þ

while the mean pressure p is p ¼ Er tanb=2

ð8:12Þ

which interestingly is independent of the penetration (geometrical similarity). Mean pressure shows dependence on ﬂank angle. For a sharper tip (larger b), a larger pressure is generated. Using standard silico-soda-lime glass characteristics (Er ¼ 76 GPa) and a ﬂank angle b ¼ 198 (a cone angle with the same area function as that of a Berkovich or Vickers tip) one ﬁnds a pressure p 13 GPa well above the glass yield strength (Y ¼ H/3 2 GPa; Appendix 8). In fact, glass is ‘plastically’ deformed as revealed by the indenter mark left on its surface (Fig. 8.10). The mark shows the symmetry of the indenter used (here four-fold symmetry since a Vickers pyramid tip was used). The image shows also fracture events that are discussed in more detail below. Most tips are not perfectly sharp but show tip rounding at their extremity. Under low loads the tip rounding yields

8.1 Sharp and Blunt Contact

Fig. 8.10 Indented surface showing the permanent deformation and the radial cracks (scanning electron microscopy observation of standard glass indented under 5 N); c and a correspond to crack and mark lengths respectively.

a Hertz dependence between force and penetration with no plastic deformation being generated, while the response tends to Sneddon’s law for elevated penetrations. 8.1.3.2 Elastic–Plastic Loading As discussed above, a sharp contact yields elastic and irreversible deformations. Different approaches have been proposed to model the elastic–plastic response (Loubet et al., 1986; Sakai 1999). Basically purely elastic and purely plastic components are connected in series (Chapter 6; Oyen and Cook, 2003). The total displacement of the indenter is the sum of the elastic he and plastic hp displacements (a viscous hv component may be added; Oyen and Cook, 2003; Mammeri et al., 2004; Appendix 8): h ¼ he þ hp

ð8:13Þ

Because of the geometric similarity of the sharp indenter, all constitutive equations show the square of the respective penetrations: F ¼ AEr he2

ð8:14Þ

F ¼ BHhp2

ð8:15Þ

where A and B (24.5 for a Vickers or Berkovich tip) are constant1 for a bulk, Er the reduced modulus and H the hardness. It should be noted that we assume here that the

1)

Parameter A may include mechanical properties (H/E ratio). Penetration can be written h ¼ hs þ hc, where hs is the elastic deformation of the surface (Appendix 8)

where H/E ratio appears (Loubet et al., 1986; Hainsworth et al., 1987; Malzbender et al., 2000).

169

170

8 Contact Resistance of Glass

sharp tip is a perfect pyramid or cone while tip rounding has to be considered as already discussed above. The reﬁnement of the present approach can be obtained using numerical tools like ﬁnite element analysis (FEA; Appendix 11). Combining Eqs. (8.13) to (8.15) yields h¼

rﬃﬃﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ F F 1 1 þ ¼ F pﬃﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ AEr BH AEr BH

ð8:16aÞ

Hence we obtain a square dependence of the force F on the total penetration: F¼

2 1 1 pﬃﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ h2 ¼ Kh2 AEr BH

ð8:16bÞ

where K is an elastic–plastic prefactor. This result suggests that elastic–plastic response under a conical remains self-similar. 8.1.3.3 Hardness Hardness measures the plastic resistance of a surface to contact loading, that is, its resistance to permanent deformation. Most experiments are carried out using a Vickers diamond pyramid. When a Vickers diamond (four-sided) pyramid is loaded over the plastic threshold, one can determine, after the test, the mean pressure or hardness H deﬁned by the ratio between the applied load and the projected surface Ap of the permanent deformation left by the indenter. This area can be determined from the mark diagonals (Ap ¼ 2a2; Fig. 8.10) observed under elevated loads by means of optical microscopy. Hardness is H ¼ F=Ap

ð8:17Þ

A large mean pressure (large hardness) means that the specimen shows an elevated resistance to plastic deformation under contact loading. Historically, the hardness ratio was deﬁned using the actual surface of the indent and not its projected surface so that a geometric factor relates the hardness number (Vickers, Knoop, Brinell, etc.) and the mean pressure. For instance, for a Vickers tip the Vickers hardness Hv is 0.927H (92.7% of the mean pressure). According to the load range, macro-, micro- and nanoindentation domains have been deﬁned. These domains should be borne in mind since indentation size effect (ISE, that is, a decrease of hardness with load in most cases) is reported for many materials including glasses, so that hardness values are to be compared within the same domain. It should be noted that these domains also refer to different ways to determine the surface of the indent. In the macro- and microindentation domains the indent surface is generally determined after unloading by optical microscopy. We shall refer to this area as Ap (projected area deﬁned above). Going to the nanoindentation domain (Appendix 8), observation of the indent becomes tedious and hardness is determined under load and is deﬁned as the ratio of the force to the projected contact area Ac that is extracted from the

8.1 Sharp and Blunt Contact Microhardness of different glasses (Aben and Guillemet, 1993; Barton and Guillemet, 2005).

Tab. 8.1

Microhardness, H (GPa)

Glass Silica Aluminosilicate Borosilicate Soda-lime-silica Lead-silicate Aluminophosphate

7.0–7.5 5.4–5.9 5.8–6.6 5.4–6.6 4.5 3.2

loading–unloading curves (Appendix 8): H ¼ F=Ac

ð8:18Þ

Microhardness values are reported for different glasses in Table 8.1 and do not show strong difference according to the composition of the glass even though they are known to deform quite differently whether they are considered normal or anomalous glasses. The nature of the permanent deformation is still controversial however. It depends on the type of glass, on the temperature and also on the strain rate. At room temperature, so-called anomalous glasses like fused silica show a volume densiﬁcation while normal glasses show shear ﬂow (Mackenzie, 1963; Peter, 1964; Neely and Mackenzy, 1968; Arora et al., 1979). In amorphous semiconductors (a-Ge) phase transition to crystalline phases is even observed (Patriarche et al., 2004). Normal glasses contain alkali and alkaline earth modiﬁers leading to non-bridging oxygen (NBO) atoms allowing for heterogeneous shear bands to form. Some authors suggested following Greaves’ (1985) modiﬁed random network that shear would happen preferentially at the frontiers between modiﬁer-rich and silica-rich volumes (Chapter 5). Heterogeneous ﬂow yields non-Newtonian viscoplasticity. The same formalism is used by the plasticity community and this explains why the term ‘plasticity’ is used for a glass even though the dislocation concept has to be reconsidered in a non-periodical structure (G’Sell, 2001). Douglas (1958) argued that ‘when the load is ﬁrst applied’ to the glass specimen ‘the pressure under the point of the diamond will be very high and the viscosity will be reduced’ (this is nonNewtonian ﬂow), and ‘ﬂow will take place until the diamond has penetrated sufﬁciently so that the force is no longer great enough to cause sufﬁcient reduction in viscosity for ﬂow to continue’. Also, water incorporation at glass surfaces (Chapter 5) is suspected to play a role in glass response (Han and Tomozawa, 1990). In contrast, anomalous glasses which contain very few modifying ions (silica being the archetype), present a much cross-linked network preventing heterogeneous ﬂow. Thereafter, indentation induces compaction (or densiﬁcation) of the glass. It occurs by bending and twisting but not breaking the silicon–oxygen bonds in the glass network. In fact, when the glass is heated up sufﬁciently the mark recovers (Neely and Mackenzy, 1968; Yoshida et al., 2001).

171

172

8 Contact Resistance of Glass

Fig. 8.11 Hardness H of silicate glass as a function of modiﬁer concentration (according to Kennedy et al., 1980).

Kennedy et al. (1980) reported changes in the hardness of silica as modiﬁers are progressively introduced. As observed for Young’s modulus E changes with alkali (Chapter 7), softening of the silica glass is more pronounced for a modiﬁer having a lower Dietzel ﬁeld intensity, that is, for a modiﬁer that is expected to form weaker interaction with oxygen (Chapter 5; Fig. 8.11). While heterogeneous shear ﬂow is volume-conservative, compaction, as the word suggests, leads to decrease in volume. This is the reason why the residual stresses caused by indentation into an anomalous glass are smaller than those in a normal glass. This has been clearly demonstrated by Arora et al. 1979 using photoelasticity (Chapter 10) to reveal differences in stresses around indent sites for normal and anomalous glasses. More recently, Perriot (2005) carried out cross-sectional Raman investigation on indented silica and revealed compaction gradient in silica (Fig. 8.12). Also, Yoshida et al. (2005) showed that compaction contribution to indentation deformation in normal glass could be greater than generally accepted. In fact, the separation of anomalous and normal glasses according to the presence of modiﬁers is still questioned. Rouxel et al. (2006) showed recently that SLS glasses show substantial compaction (obviously less than silica) that recovers upon annealing. Furthermore there seems to be a close relationship between densiﬁcation and Poisson’s ratio. The mechanical behaviour of a glass becomes more and more time dependent as the temperature is increased and as the viscous behaviour becomes predominant over densiﬁcation process (Westbrook, 1960; Wiederhorn and Hockey, 1980; Le Bourhis and Metayer, 2000; Le Bourhis and Rouxel, 2003). Under large strain rates, the supercooled liquid shows non-Newtonian behaviour with an apparent viscosity decreasing with the strain rate amplitude (Simmons et al., 1988; Appendix 10). Although this behaviour makes the process operations more difﬁcult, it can yield

8.1 Sharp and Blunt Contact

Fig. 8.12 Cross-sectional compaction map in silica under a Vickers indentation (Perriot, 2005).

advantages since the operations can be carried out under lower stresses (for the same ﬂow, rheoﬂuidiﬁcation) once high strain rates can be achieved. Hardness depends strongly on the temperature as shown in Fig. 8.13 for a sodalime-silica glass. As the temperature approaches Tg, viscous ﬂow (volume conservative) comes into play. Strangely, very few data existed before the 1990s while this behaviour is very important from the process point of view. These studies are in fact not easy to carry out and discrepancies appear between authors (Westbrook, 1960; Watanabe et al., 2001; Le Bourhis and Rouxel, 2003; Shang and Rouxel, 2005). These have been attributed to the differences in loading time, hold period and surface roughness employed by different authors. Also, modelling of the behaviour has to consider both viscosity and elasticity (Chapter 6, Appendix 8). Viscous deformation is

Fig. 8.13 Mean hardness as a function of temperature for soda-lime-silica glass: &, Watanabe et al. (2001); , Smith and Zheng (2000); , Le Bourhis and Metayer (2000);, Westbrook (1960). (Reprinted from Le Bourhis and Rouxel, 2003, with permission from Elsevier.)

173

174

8 Contact Resistance of Glass

Fig. 8.14 Hardness (log scale) as a function of reciprocal temperature for soda-lime-silica glass: &, Watanabe et al. (2001); ~, Smith and Zheng (2000); ^, Le Bourhis and Metayer (2000); ^, Kurkjian et al. (1995). (Reprinted from Le Bourhis and Rouxel, 2003, with permission from Elsevier.)

time-dependent and depends on history. Also, well below the glass transition, a decrease of the hardness is observed on increasing the temperature. At such low temperature ( m (this is also the case for most ceramics) and hence m < 1 corresponding to a large spread of lifetime values. In contrast, glass ﬁbres show much higher Weibull modulus so that n 2 < m and m > 2 allowing for a better prediction of fatigue strength. Equation (9.11) can be written in the form t ¼ sn f ½Ps ðV; sÞ

ð9:14Þ

9.6 NiS Phase Transformation

where f is a function of Ps(V,s). Interestingly, this result shows again a strong dependence on applied stress s as 1/sn.

9.5 Applications

Delayed fracture has to be determined and known in order to predict glazing performance. This is a complex task since it involves environment-dependent parameters, while glass fracture prediction supposes ﬂaw population statistics to be known. As mentioned above, for glass articles showing low Weibull modulus, a large spread of lifetime would be obtained. Proof testing is a way to eliminate weak members. The elements are subjected to a short-term stress cycle similar to that employed in service while in excess of that required. The articles with the largest ﬂaws fail and are eliminated from the distribution which is biased towards the highstrength region. As a matter of fact, the articles can be used under service conditions with a higher degree of conﬁdence. Alternatively, there exist ways to prevent stress corrosion. One of these is to temper the glass. Then, the cracks that are generally present at the surface (Chapter 8) are submitted to compressive stresses provided that the glazing has been designed in such a way that the service tensile stress does not exceed the residual compression (Chapters 6 and 7). Another way is to take advantage of the development of hydrophobic thin ﬁlms which might also yield new solutions to fatigue issues (Chapter 12). Such ﬁlms can be used to protect the glass from moisture. As detailed in Chapter 12, one problem of such coatings is their physical and mechanical stability with time (poor resistance against UV and contact loadings; see Chapter 8).

9.6 NiS Phase Transformation

Ageing of glass may also be observed because of the physical transformation of internal defects like metastable nickel sulphide (NiS) inclusions. These undergo a slow transformation at room temperature from a denser to a lower density phase. These inclusions can be of different compositions, namely NiS, Ni1xS or Ni7S6, with sizes in the range 1–10 mm (Barry et al., 1998). S comes from the raw materials and combustion, while Ni might appear because of the abrasion of the tools used for batching (Chapter 10). In fact, it remains impossible to eliminate these NiS inclusions. Their content is estimated at about 1 particle for 10 tons of glass. The transformation takes place around 335–380 8C and is written a-NiSðhigh temperatureÞ ! b-NiSðlow temperatureÞ

ð9:15Þ

199

200

9 Ageing of Glass

with a relative increase in volume of the inclusion given by e ¼ DV=V 2 4%

ð9:16Þ

Transformation strain can be accommodated over Tg by viscous ﬂow. On the contrary, below Tg transformation strain remains in the glass article. It may drive the slow growth of the cracks up to the point where they become unstable in the residual tensile stress ﬁeld in the core of the tempered glass yielding spontaneous fracture (Swain, 1981; Aben and Guillemet, 1993). In fact, the inspection of fragmented windows reveals that NiS particles are present at the origin of the fracture (at the centre of the mirror zone; Chapter 7) and located at the glass centre. This does not mean they are not uniformly distributed in the glass but, rather, fracture happens only when the particles are in the tensile zone. Phase-transformed NiS inclusion can be observed in a polarizing microscope using photoelasticity to reveal the induced stress ﬁeld (Aben and Guillemet, 1993; for details on photoelasticity see Chapter 11). The radial displacement at a distance r is a function of the increase in volume e: ur ¼

e R 3 3 r

ð9:17Þ

where R is the particle size. Radial displacement increases considerably with particle size (as R3). The maximum stress resulting from phase transformation (when NiS volume change is not accommodated at elevated temperatures) scales with s eG

ð9:18Þ

where G is the shear elastic modulus. At 800 8C (in the glass melt) only the a phase exists. When the cooling rate is low, there is time enough for all NiS particles to transform into the b form. The change in volume can be accommodated when the glass is still viscoelastic. The result is that all NiS inclusions are in the b form and the glazing is stabilized. This is the case for a ﬂoat glass at the lehr exit (Chapter 10). On the contrary, when the glazing is tempered the ﬂoat glass is to be re-annealed at about 650 8C while NiS inclusions transform from the b into the a form again. On tempering the glass, the change back to the b phase cannot take place at elevated temperatures because of the very fast cooling rates being employed but continues at room temperature (Chapter 6). It is accelerated by solar radiation absorption that increases the temperature of the glazing. This transformation follows kinetics over a long time frame; the volume mismatch induces stresses into the glass so that fracture may actually happen a long time after production (some months or years). Obviously there are several parameters that yield a more rapid fracture (Barry et al., 1998): i. the size of the inclusion, ii. the presence of a ﬂaw at its proximity, iii. the intensity of the tensile stress, and iv. the tempering degree of the glazing.

9.7 Crack Healing

Glassmakers report fracture induced by 40–100 mm particles for glazing tempered at compressive surface stresses of 100–120 MPa. Thereafter, it has been of utmost importance to ﬁnd a treatment to transform the NiS particles into their b stable phase, in particular in tempered glazing. Therefore, a thermal treatment (heat soak test, HST) of these glazings has been added to accelerate the transformation of NiS inclusions. This modiﬁcation of the manufacturing process of tempered glass (‘heat soaking’) can prevent the phase transformation from taking place during service and thus efﬁciently guarantees the product against such spontaneous failures (Barry et al., 1998; Gy, 2003). The temperatures during such a treatment are assumed to be low enough as compared to the transition temperature so that we may neglect changes in glass thermal strengthening. In fact, heat soaking treatment is carried out at about 300 8C. At this temperature, NiS transformation is completed after 2 h (Barry et al., 1998) and thus any products containing particles of size larger than the critical dimension break, thus eliminating the risk of breakage during use (Aben and Guillemet, 1993). Moreover, since a properly tempered glass has a compressive residual stress everywhere in the surfaces, tempered glazings designed in this way are protected against ageing since static fatigue is avoided as detailed above. Nonetheless, this heat soak test involves industrial added costs since (i) it requires heattreating furnaces, (ii) it increases the operation times and (iii) it may affect the tempering whenever deviation of maximum treatment temperature happens in the HST processing.

9.7 Crack Healing

All the ageing phenomena mentioned above are room temperature events. Obviously, thermal treatments may considerably change the behaviour of glass since viscous ﬂow may progressively appear. In fact, crack healing is reported with related ‘closing’ of the cracks. Thereafter, the mechanical performance may be improved (Fig. 9.7). Nonetheless after the heat treatment is completed, ageing is observed again in the annealed glass as its stress at rupture decreases with the lifetime as detailed in Section 9.3 (see also Chapter 7).

201

203

10 Mechanics of Glass Processes 10.1 Introduction

Industrial processes are numerous and depend on the application (glazing, containers, ﬁbres, etc.). It is beyond the scope of this book to review all of them. Instead, we shall illustrate by some examples how glass mechanics is to be considered throughout the industrial process. We have selected widespread industrial tools regarding ﬂoat glass, containers and ﬁbres. This chapter can also be nicely illustrated by a video produced by France Te´le´vision (FR3) entitled ‘C’est pas sorcier se met au verre’. All processes require a furnace with a high capacity, a long production line for upstream operations (batching, melting, ﬁning, forming and annealing), while downstream operations (reheating, forming, moulding, coating, tempering, laminating) can be performed on-site or off-site (Fig. 10.1). All these operations require a deep understanding and application of mechanics. At elevated temperatures, viscosity controls the homogeneity of the glass melt, the ﬂatness of the glass while the thermomechanical properties determine the strength of the refractories used to fabricate the tools. At lower temperatures the tribological resistance of glass products will control surface quality and strength of the manufactured objects (ﬂat glass, containers). Industrial production numbers show that tools have achieved great efﬁciencies since the industrial furnaces for ﬂoat line and bottle line produce an average of 500 and 300 tons of glass per day respectively. A unique ﬂoat line produces per day glazing surfaces required for one building as high as Montparnasse tower (Flessel, 2003). The production frequency of bottles is about 10 per second in a conventional production line. Further evolutions are carried out to meet increased capacity, ﬂexibility, availability and glass quality. In fact, maintenance, cleanliness and fabrication practices have been considerably modiﬁed. Four primary operations for glass manufacturing are i. batching, ii. melting, iii. ﬁning and iv. forming. Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

204

10 Mechanics of Glass Processes

Fig. 10.1 Fibreglass production unit at Ladenbourg. (Copyright Saint-Gobain.)

Batching, melting and ﬁning operations are common to all glass manufacturing processes with some variations according to the furnace type. The forming and postprocess depend on the end product. 10.1.1 Batching

Batching encompasses raw material selection based on chemistry, purity, uniformity and particle size. The batch comprises sand for silica, while modiﬁers are introduced as carbonates instead of oxides to reduce energy costs (Table 10.1). The batch selection is adapted to the end product, for instance ﬁbre production requires more selection and ﬁner raw material particle size than container production. Also raw material humidity is controlled using IR analyser on modern production lines; also, impurity concentrations (Fe, Ni) are checked. Recycling of the glass has become an important parameter at this step and allows energy gains since a lower energy is required to melt the raw materials mixed with the recycled glass. Flat glass manufacturers recycle up to 30 % of their own cullet while domestic recycling of the containers has become widespread (60 to 90 % of the domestic packaging is recycled in Europe for instance). Recycled containers are separated according to their Tab. 10.1

Raw material composition for standard soda-lime-silica glass production.

Raw material

Sand

Sodium carbonate

Calcium carbonate

Metal oxides

Concentration (%)

54

24

16

2

10.1 Introduction

colour to optimize the achieved product. Also, recycling may introduce ceramic contaminants that undergo reactions with the glass melt and are present as inclusions in the ﬁnished product. Metal and organic contaminants create instability during glass processing (through reduction/oxidation reactions) and degrade the quality of the glass. Delivery, mixing and sizing processes are highly abrasive, and equipments contain metals and ceramic-coated wear surfaces. Therefore, contamination risks exist from the tools and, actually, nickel sulphide particles are believed to form from nickel contained in such tools and from sulphur impurities introduced by combustion and are responsible for the delayed fracture of tempered glazing (Chapter 9). 10.1.2 Melting

Melting consists of complex chemical and physical phenomena. A large energy above the thermodynamic value 2.7 MJ kg1 is required to fabricate soda-lime-silica glass. Out of 1.2 kg of raw materials, 1 kg forms the glass while 0.2 kg forms the gas, mainly CO2. These large volumes of gas help in the ﬁning of the glass as discussed in the next section. Sand and sodium carbonate grains react as follows: SiO2 þ Na2 CO3 ! Na2 SiO3 þ CO2

While calcium carbonate transform as CaCO3 ! CaO þ CO2

Glass furnaces are used for melting the raw material particles and for transforming these into glass. The low melting constituents (alkali oxides) melt and dissolve the higher melting constituents such as quartz and alumina. Different furnaces are used for producing containers, ﬁbreglass, ﬂat glass and speciality glass. They can be divided into those heated electrically and those heated primarily by combustion. Often electrical heating is used in combination with fuel ﬁring (so-called electric boost) to improve heating uniformity and melt efﬁciency and to reduce gas consumption and emissions that is a matter of prime importance in the context of global climate changes. Recycling glass allows emissions to be reduced, which were at a maximum in 1980 before decreasing up to the present (Flessel, 2003). Other polluting emissions (NOx, SOx) are generated and are reduced improving combustion (using oxygen instead of air) and fuel quality. Furnaces are all made of refractories that allow for long lifetimes (of 10 years for ﬂoat and container furnaces) before requiring rebuild costs. The cost of rebuilding a ﬂoat or container furnace is in the region of s1 million. Electrical heating is used extensively and exclusively in smaller speciality and ﬁbreglass melting units because of its lower initial cost and low emissions as compared to combustion furnaces even though energy costs remain high. This

205

206

10 Mechanics of Glass Processes

drawback is compensated by ﬂexibility in particular when small production volumes are required for speciality products. Glass conductivity plays an important role in this process: while being electrically insulating at room temperature, the glass melt can be heated by the Joules effect (see also Appendix 13). Most furnaces are combustion heated which can be further divided according to the method used to recover exhaust waste heat and the way fuel is burnt (with air or oxygen). Oxygen fuel technology offers several advantages even though requiring pure oxygen. Regenerators can be avoided, eliminating furnace superstructures. Heat recovery is of utmost importance since only 10 % is used for the melt while 70 % is lost through exhaust. Exhaust waste heat recovery is performed using regenerators that alternately store and recover heat, the shift being about every 20 minutes.

Fig. 10.2 (a) Glass furnace interior. (Copyright Saint Gobain.) (b) Glass furnace schematic. Burning and air ﬂow alternate, regenerators being either active or passive accordingly.

10.1 Introduction

In ﬂoat furnaces, several regenerators (their number depending on the furnace capacity) are placed on each side of the furnace while in container furnaces, two regenerators are placed both on the back side (the gas ﬂow forming a U loop). Regenerators consist of enormous thermal capacity refractories that alternately either store energy or recover warm air to the active burners. In a ﬂoat furnace, burners are located on opposite sidewalls (Fig. 10.2). Firing alternates from side to side, the regenerators being alternately passive (stocking) or active (restitution). Such a procedure allows for production of glass with only twice the thermodynamic number (5.4 MJ kg1; Flessel, 2003). Alumina-zirconia-silica (AZS) refractories are used to contain the glass melt and to resist corrosion. The furnace roof is made of silica which presents low thermal expansion, which is important since the roof experiences elevated temperature (1600 8C), the melt being annealed from its top. Also when dislodged pieces fall into the melt, they are more easily dissolved. Downstream, dislodged pieces cannot be dissolved any longer and then dedicated materials are selected: pure alumina is used for the exit of ﬂoat glass furnaces and feeders used for delivery of automatic blowing machines. Large thermal gradients exist in the melt because raw materials are introduced progressively. Convection ﬂow (velocity of the order of millimetres per second) is induced and favours thermal exchange and glass homogeneity. Of much interest for the glassmaker, two principal convection ﬂows are generated in the ﬂoat furnace, one in the melting zone and another in the ﬁning zone. This allows preservation of the ﬁning zone from the batch. In container furnaces, separation is obtained by a barrier placed at the bottom of the furnace. In contrast, radiative transfer is the dominant exchange mode between the roof and the glass melt surface. 10.1.3 Fining

Glass ﬁning produces a molten glass that is uniform in terms of composition and temperature, and bubble free. In fact, the temperature of the glass delivered from the melting furnace, and its composition, has to be regulated with extreme care. This requirement inﬂuences the next operation, that is, glass forming, and as seen in Chapter 6, the latter operation is dependent on viscosity, that is, on the way the glass has been prepared. Consider for instance that a glass gob is to fall under its own weight in order to become correctly placed in a mould. If the viscosity is too high it will not do so in time for the next operation (say the introduction of compressed air to blow the glass out to the shape of the mould) but if it is too low the glass will fall too far and the ﬁnished article may be too thick at its base. Fortunately, large volumes of gas are rejected from the raw materials before transformation in a glass melt and this helps homogenize the melt considerably. Before glass delivery, bubbles have to be eliminated. Bubbles contain trapped air (oxygen, nitrogen) and decomposition products of the raw materials, mainly carbon dioxide. Large bubbles rise to the top of the melt and participate in melt homogenization. In contrast, small bubbles would not eliminate because of increasing required time as their size diminishes (Appendix 4). There are then two alternatives: either gas dissolves into the melt or bubbles are increased in size so that they rise more rapidly to the surface. These

207

208

10 Mechanics of Glass Processes

operations are accelerated by ﬁning agents that are introduced in small quantities in the batch and hence in the glass melt. Fining agents like arsenic and antimony increase dissolution rates. The mechanism by which these agents enhance dissolution of gas from bubbles is still debated; a change in oxidation state of the melt or increasing the rate of oxygen diffusion is suggested. Sodium or calcium sulphate ﬁx on small bubbles that are favourable nucleation sites for ﬁning agents and release gas, increasing the related bubble size and this hence facilitates their elimination (Appendix 4): 2Na2 SO4 ! 2Na2 O þ O2 þ 2SO2

The ﬁning zone is generally gas ﬁred; an electric boost can also provide increased efﬁciency in getting uniform temperature. 10.1.4 Forming

As stated above, the forming operations have been developed for different applications. Flat glass, container and ﬁbre tools present different viscosity, stress and strain rate regimes. The tools have been developed accordingly. Some of these are described in the continuation of this chapter.

10.2 Float Process

Let us consider the fabrication of ﬂat glass which is produced nowadays by the ﬂoat process. This process was introduced by Pilkington Brothers Ltd in the 1950s (see Chapter 3). Firstly, the raw materials (sand, soda, lime) are continuously introduced into the furnace, melted at 1500 8C, homogenized by convection and ﬁned to eliminate bubbles (Fig. 10.3). The furnace contains typically 2000 tons of glass and produces every day 500 tons of glass. The viscous liquid travels onto the ﬂoat at a temperature of 1100 8C under a nitrogen atmosphere in order to prevent corrosion of the tin bath. Under these conditions the equilibrium thickness of the glass sheet is about 6 mm so that the sheet has to be expanded or contracted by top rolls (or rollers working from the top of glass) to produce thinner or thicker glass sheets respectively. The equilibrium equation is written (Fig. 10.4; Langmuir, 1933) gt2H rg rg 1 ¼ zga þ zgb zba 2 rb

where g is the gravitational acceleration, tH the sheet thickness, rg and rb the density of glass and bath, z the surface energy and subscripts g, b and a indicate glass, bath and atmosphere respectively. Taking rg ¼ 2500 kg m3, rb ¼ 6500 kg m3, zba ¼ zgb ¼ 0.5 J m2 and zga ¼ 0.35 J m2, one ﬁnds tH¼6.8 mm.

10.2 Float Process

Fig. 10.3 (a) Float line at Chennai. (Copyright Saint-Gobain.) (b) Schematic representation of a ﬂoat line (CVD and spray unit locations are indicated and optional). (c) Float glass line end showing transiting glass on rollers. (Copyright Saint-Gobain.)

209

210

10 Mechanics of Glass Processes

Fig. 10.4 Float ribbon mechanical equilibrium on a tin bath.

Several pairs of top rolls are used; they are made of steel and are water cooled. Their rotation axis is horizontal and shifted out of the ﬂoat axis to draw the glass ribbon. The range of commercial thickness is between 2 and 19 mm. Glass with lower thickness ( 1. Potential energy is the sum of attraction and repulsion contributions: Ep ¼ Erep þ Eattr ¼

a 1 qq0 m r 4peo r

Potential energy is plotted in Fig. A2.4; ro is the distance corresponding to the energy minimum (force is then zero). This corresponds to the equilibrium distance

A2.3 Bond Formation

Fig. A2.4 Potential energy as a function of distance resulting from electron repulsion predominant at short distance and ion attraction predominant at long distance.

and is called the bond distance. Bond distance allows for ion size to be determined. In the present case ro ¼ rNaþ þ rCl . Ionic crystals are formed by ions that all interact electrostatically with r1 being a decreasing function. A simple calculation of the attractive energy can be made for a one-dimensional chain of N ions of opposite charge (q ¼ q0 ; Kittel, 1983; Fig. A2.5): lnð1 þ xÞ ¼

x2 x3 x4 x þ 2 3 4

NEattr ¼ 2N

qq0 1 1 1 1 þ 4peo r 2r 3r 4r

1 qq0 1 1 1 1 qq0 ¼ 2N 1 þ ¼ 2N ln2 4peo r 2 3 4 4peo r Eattr ¼ 2

1 1 2ln2 1 b ln2 ¼ ¼ 4peo r 4peo r r

where 2 ln 2 (¼ 1.38) is the Madelung constant for a one-dimensional chain. For a three-dimensional solid, the calculation is more difﬁcult and yields a Madelung constant of 1.74 for NaCl.

Fig. A2.5 One-dimensional and periodical ion chain.

269

270

Appendix 2: Atomic Structure and Bond Formation

The variation of Ep can be generalized to any bonds and solids in the following form: Ep ¼ Erep þ Eattr ¼

a b rm rn

with m > n since repulsion is dominant over attraction at low r. The Lennard-Jones potential is written for m ¼ 12 and n ¼ 6.

271

Appendix 3 Thermal Expansion and Elasticity A3.1 The a–E Trend

Materials’ thermal expansion coefﬁcient a and stiffness (elastic modulus E ) are related. In fact a ceramic (stiff material) will expand less than a polymer. This general trend is observed in the a–E chart (Fig. 2.8) where all classes of materials are considered. This trend is mathematically formulated as a¼

gG rcv 3E

where the Gru¨neisen ‘constant’ gG is not a constant but varies within one order of magnitude (0.4 < gG < 4), r is the density and cv the speciﬁc heat cv cp. A simple approach to thermal expansion is proposed by Zarzycki 1982 and Kittel 1983. We shall review brieﬂy here their approaches.

A3.2 Qualitative Approach

Figure A3.1 shows schematically the potential energy of bonded atoms. The continuous line is for a more rigid material since it shows a deeper potential. Parameter ro corresponds to the equilibrium distance at T ¼ 0 K. This temperature cannot be produced, so for clarity we take this temperature as a reference point. At T > 0 K, atoms oscillate around their equilibrium position. It is important to note that the potential is not symmetric. For small oscillations, one generally neglects this phenomenon and takes a parabolic function in the form Ep ¼ (1/2)k(r ro)2 also called the harmonic potential. Force is then F ¼ k(r ro). Under such an assumption, no thermal expansion is found (Fig. A3.2). Now considering the fact that the potential is not symmetric, the average distance between atoms shifts towards the right-hand side of Fig. A3.1, or the materials are expected to expand when they are heated. Here, we do not consider any phase Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

272

Appendix 3: Thermal Expansion and Elasticity

Fig. A3.1 Potential energy as a function of distance for weak (dashed line) and strong (continuous line) bonds.

changes which either yield contraction or expansion. Materials showing a deeper potential (stiffer materials) show less potential asymmetry (for the same additional thermal energy kT ). Hence, these materials present a lower thermal expansion coefﬁcient than materials having a shallow potential (soft materials). Considering now silicate glasses, when modiﬁers are introduced in the silicate glass, NBOs are formed and yield Si–O potential asymmetry and hence lead to large thermal expansion. In contrast, in borosilicate glasses, B atoms participate in glass network formation and no NBOs are formed maintaining the potential symmetry and hence less thermal expansion is observed for these glasses.

A3.3 Expansion Modelling

In a ﬁrst approximation we may add one asymmetric term to the harmonic potential that we have deﬁned above: Ep ¼ ð1=2Þkðr ro Þ2 þ gðr ro Þ3 ¼ cx 2 þ gx 3

with c ¼ ½k, x ¼ r ro, g < 0 and we assume gx3 kT. When g ¼ 0, we get again a harmonic or parabolic potential.

Fig. A3.2 Potential energy as a function of distance curve showing the harmonic approximation.

A.3.4 Differential Expansion Measurement

Following Kittel 1983, we consider a Boltzmann distribution and the average distance shift at temperature T is R1 xexpðEp =kTÞ hxi ¼ R1 1 1 expðEp =kTÞ

With the following approximation: Ep cx 2 þ gx 3 cx 2 gx 3 ¼ exp ¼ exp 1 exp kT kT kT kT

a series of calculations yields hxi ¼

3g kT 4c2

This simple approach then yields a constant thermal expansion coefﬁcient proportional to g (asymmetric term): a¼

3g k 4c2 r0

We ﬁnd that stronger binding (larger value of c, stiffer materials) yields indeed lower thermal expansion while larger asymmetry (larger value of g) yields larger thermal expansion.

A3.4 Differential Expansion Measurement

A dilatometer is used to determine the thermal expansion coefﬁcient of a specimen submitted to a thermal ramp (constant heating rate). Not only does the specimen expand but also the dilatometer (Fig. A3.3). Hence, differential expansion is

Fig. A3.3 Schematic representation of thermal expansion of both sample and dilatometer.

273

274

Appendix 3: Thermal Expansion and Elasticity

measured and correction is necessary to include the dilatometer expansion in the experimental data. Consider for instance an alumina specimen in an alumina cylindrical support: the apparent expansion would be zero because all expand the same relative length. A diagram can be constructed showing the measured and actual (and superior) expansion (Fig. A3.3).

275

Appendix 4 Falling Sphere Viscometer and Fining of Glass A4.1 Falling Sphere A4.1.1 Asymptotic Regime

Let us consider a sphere of radius r, volume V and mass M ¼ rsV (rs being the sphere density) falling in a viscous ﬂuid of density r (Fig. A4.1). It is subjected to three different forces: (i) gravitational force, (ii) Archimedes reaction and (iii) viscous friction. Newton’s principle is written Mg þ A þ f ¼ Ma

where g is the gravitational acceleration and a is the acceleration of the ball. We have Mg ¼ rs Vg A ¼ rVg f ¼ kv

where v is the velocity and k is taken as the Stokes coefﬁcient: k ¼ 6phr

The ball reaches a constant velocity after a transient period (v ¼ vl, a ¼ 0) that is given by Mg þ A þ f ¼ 0 ðrs rÞVg ¼ kvl

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

276

Appendix 4: Falling Sphere Viscometer and Fining of Glass

Fig. A4.1 Falling sphere in a viscous liquid.

We ﬁnally ﬁnd vl ¼

ðrs rÞVg 2gr 2 ðrs rÞ ¼ k 9h

A4.1.2 Transient Regime

When a falling sphere viscometer is used, one supposes that the asymptotic regime is reached or the transient regime (from velocity v = 0 to vl) is achieved. This regime is obtained solving Mg þ A þ f ¼ Ma

This equation is rewritten as rs V

dv þ kv ¼ Vgðrs rÞ dt

with initially

vðt ¼ 0Þ ¼ 0

The solution is vðtÞ ¼ vl ½1 expðt=TÞ

with T ¼ rs V=k

The solution is qualitatively plotted (Fig. A4.2) for two different values of k (or h). Notably when viscosity increases T and vl decrease. Hence, the asymptotic regime is

A4.2 Fining of Glass

Fig. A4.2 Velocity evolution with time of a falling sphere in a viscous liquid (k1 < k2).

reached more rapidly and after a shorter falling distance. Therefore such conditions are more favourable for the method to be employed. A4.2 1. Fining of Glass Fining of Glass Let us consider the limit velocity solution and consider a bubble formed in a glass melt. The asymptotic solution becomes vl ¼

2gr 2 r 9h

It is of utmost importance to eliminate bubbles in the glass (Fig. A4.3). Considering a period of time t, the distance d that a bubble travels is d ¼ vl t ¼

2gr 2 r t 9h

Fig. A4.3 Handmade and old-fashioned container showing a large amount of bubbles with different sizes.

277

278

Appendix 4: Falling Sphere Viscometer and Fining of Glass

showing a dependence on the square of the bubble size and an inverse dependence on the viscosity: d/

r2 t h

At 1330 8C in a standard melt, it takes 1 minute for a 1 mm diameter bubble to move a distance of 1 mm, while this time becomes 5 h and 20 days for 100 mm and 10 mm diameter bubbles respectively. There are two main ways to accelerate the elimination of bubbles (Chapter 10): (i) decreasing the viscosity, which is done by imposing a higher temperature at the surface; and (ii) increasing the bubbles size, which is done using ﬁning agents.

279

Appendix 5 Theoretical Strength of a Solid Let us consider like Orowan (1949) the potential energy of bonded atoms as shown schematically in Fig. A5.1. Parameter ro corresponds to the equilibrium distance (rigorously, only at T ¼ 0 K; see Appendix 3). Let us apply a force to separate the atoms: F ¼ dEp =dr ðpositive sign since it is the applied forceÞ

Figure A5.1 transforms into Fig. A5.2 when the applied force is plotted as a function of the distance, equilibrium distance ro being obtained for F ¼ 0. The force curve maximizes at Fm. Let us consider a specimen loaded under applied force F with unit section surface made of n atoms (Fig. A5.3). The applied stress is s ¼ nF

Note that we only consider the interactions between atoms in front of each other. This is the ﬁrst assumption. Theoretical strength is written sth ¼ nFm

We have in the elastic domain (for r ro) s ¼ Ee ¼ E

r ro ro

While in this domain we have also s¼n

dF ðr ro Þ dr r¼ro

The work W necessary to cause the fracture of the specimen corresponds to the area shown in Fig. A5.2 and is Z1 W¼

nFðr 0 Þdr 0 ¼ 2z

ro

where z is the surface energy (two surfaces are created on fracture). Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

280

Appendix 5: Theoretical Strength of a Solid

Fig. A5.1 Potential energy as a function of distance.

Next, we shall approximate the F(r) curve by a sinusoidal function to facilitate the calculations as suggested by Gilman (1949). This second approximation leads to the underestimation of the work W; the calculation shows that the theoretical strength is much greater than the observed one (see Section 7.1). In fact the model suggested here leads to the multiple fracture of the specimen since the situation for a given plane is to be considered for all planes. Thereafter, the specimen would be sliced into monatomic planes after such a test. rr o FðrÞ ¼ Fm sin 2p l

Fig. A5.2 Applied force as a function of distance.

Fig. A5.3 Tensile test on a unit surface (n atoms).

Appendix 5: Theoretical Strength of a Solid

Then in the elastic domain (for r ro) we have rr o FðrÞ ¼ Fm 2p l

so that r r o o ¼ sth 2p E ¼ nFm 2p l l

while ro þl=2 Z

nFðr 0 Þdr 0 ¼ nFm

W ¼ 2z >

l l ¼ sth p p

ro

Then multiplying the latter two equations allows one to obtain s2th ro ¼ Ez

that is rewritten rﬃﬃﬃﬃﬃﬃ Ez sth ¼ ro

281

283

Appendix 6 Weibull Analysis The investigation of the strength of brittle solids requires numerous experiments since fracture is statistical. This results from the ﬂaw size distribution of the material. For a ﬁrst experimental approach, one can consider a population of N ¼ 50 ﬁbre specimens of the same length sectioned in ﬂexure (Fig. A6.1). Care is taken in order not to damage the tested length (contact damage, ﬁnger moisture). We suggest the ﬁbre segments be manipulated only by their extremities. Theprocedure consists in testingundertensile stressopticalﬁbresupto fracture.The loading curve F Dl is checked as to its linearity up to fracture. The N stress values at fracture are then ranked in ascending order. Deﬁning x as the number of unfractured specimens at stress s, the probability estimator is taken as Ps ðVÞ ¼ ðx 0:5Þ=N

ðA6:1Þ

where V is the volume of the considered ﬁbres. We use here this simplest expression for the estimator. The precise form of the estimator is still the subject of ongoing research. Several expression for Ps(V) have been proposed in the literature (Bergman, 1984; Wu et al., 2004, 2006): Ps(V) ¼ x/N (simplest one but not generally used because it is not quite statistically correct), Ps(V) ¼ x/(N þ 1), Ps(V) ¼ (x 0.3)/(N þ 0.4), Ps(V) ¼ (x 0.25)/(N þ 0.25), Ps(V) ¼ (x 0.375)/(N þ 0.25) and more generally Ps(V) ¼ (x a)/(N þ b). The step-by-step procedure is then shown in Table A6.1. Figure A6.2 shows Ps(V) as a function of stress for a studied population. The next step consists in obtaining a Weibull diagram plotting ln{ln[1/Ps(V)]} as a function of ln(s). We use here the simplest method, i.e. the linear regression (LR) method. For the weighted linear regression, maximum likelihood and moments methods see Wu et al. 2006. For a single defect population (bimodal populations are not uncommon and lead to strong deviations from a linear plot) the Weibull diagram shows a linear evolution which allows determination of the Weibull modulus, that is, the slope of the linear ﬁt and so from the y-axis intercept

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

284

Appendix 6: Weibull Analysis Tab. A6.1

Glass fibre strength and step procedure to determine Weibull parameters.

s

ln(s)

x

Ps(V ) ¼ (x 0.5)/N

ln{ln[1/Ps(V )]}

Ps(V ), Weibull

2.10 2.11 2.11 2.26 2.26 2.30 2.30 2.30 2.30 2.31 2.32 2.32 2.32 2.32 2.34 2.34 2.34 2.36 2.37 2.38 2.42 2.42 2.42 2.44 2.46 2.46 2.47 2.47 2.47 2.47 2.47 2.50 2.50 2.50 2.52 2.52 2.54 2.54 2.55 2.55 2.58 2.58 2.58 2.58 2.58 2.62 2.62 2.63 2.65

0.74 0.75 0.75 0.82 0.82 0.83 0.83 0.83 0.83 0.84 0.84 0.84 0.84 0.84 0.85 0.85 0.85 0.86 0.86 0.87 0.88 0.88 0.88 0.89 0.90 0.90 0.90 0.90 0.90 0.90 0.90 0.92 0.92 0.92 0.92 0.92 0.93 0.93 0.94 0.94 0.95 0.95 0.95 0.95 0.95 0.96 0.96 0.97 0.97

49 48 48 46 46 44 44 44 44 40 39 39 39 39 35 35 35 32 31 30 29 29 29 26 25 25 23 23 23 23 23 18 18 18 15 15 13 13 11 11 9 9 9 9 9 4 4 2 1

0.99 0.97 0.97 0.93 0.93 0.89 0.89 0.89 0.89 0.81 0.79 0.79 0.79 0.79 0.70 0.70 0.70 0.64 0.62 0.60 0.58 0.58 0.58 0.52 0.50 0.50 0.46 0.46 0.46 0.46 0.46 0.36 0.36 0.36 0.30 0.30 0.26 0.26 0.21 0.21 0.17 0.17 0.17 0.17 0.17 0.07 0.07 0.03 0.01

4.58 3.47 3.47 2.60 2.60 2.13 2.13 2.13 2.13 1.53 1.42 1.42 1.42 1.42 1.05 1.05 1.05 0.82 0.75 0.68 0.61 0.61 0.61 0.43 0.37 0.37 0.25 0.25 0.25 0.25 0.25 0.03 0.03 0.03 0.20 0.20 0.31 0.31 0.43 0.43 0.56 0.56 0.56 0.56 0.56 0.97 0.97 1.25 1.52

0.98 0.97 0.97 0.89 0.89 0.84 0.84 0.84 0.84 0.83 0.81 0.81 0.81 0.81 0.78 0.78 0.78 0.74 0.72 0.70 0.60 0.60 0.60 0.54 0.48 0.48 0.45 0.45 0.45 0.45 0.45 0.36 0.36 0.36 0.29 0.29 0.24 0.24 0.21 0.21 0.13 0.13 0.13 0.13 0.13 0.07 0.07 0.05 0.03

Appendix 6: Weibull Analysis

Fig. A6.1 Rolled glass ﬁbre.

Fig. A6.2 Ps(V) as a function of stress s and Weibull modelled curve with the parameters extracted from least squares ﬁt of ln{ln[1/Ps(V)]} versus ln(s) as illustrated in Fig. A6.3.

Fig. A6.3 Procedure to determine Weibull parameters from a least squares ﬁt of ln{ln[1/Ps(V)]} versus ln(s).

285

286

Appendix 6: Weibull Analysis

since

1 ¼ m lnðsÞ m lnðso Þ ln ln Ps ðVÞ

ðA6:2Þ

This is illustrated in Table A6.1 and Fig. A6.3. The Weibull adjustment is then shown on the Ps(s) plot (Fig. A6.3). Two defect populations may sometimes be observed, due to damage induced while making the experiments. In such a case, the analysis can be made separately for the two populations.

287

Appendix 7 Photoelastic Set-Up for Lectures A7.1 Set-Up for Photoelastic Projection

The proposed set-up comprises a projector used for the projection of slides (Fig. A7.1). This is available in most classrooms and allows the demonstration of transient (Fig. A7.2) and residual stresses (Fig. A7.3). A polarizer or analyser can be obtained as 1 1 m2 panel (HN32 from Sarelec, 91560 Crosne, France, the panels being sold with one edge parallel to the polarization axis). It has to be cut into two squares with area covering the projector plate. For protection these square polarizers can be placed and sealed between two square and annealed glass sheets. One of the panels serves as the polarizer and is set on the projector. The other one serves as the analyser and is rotated by 908 from the polarizer. The glass specimens are then set in between. The image can be projected for a classroom focusing on the glass specimen, and examples are discussed below. Before setting a specimen one checks that polarizer and analyser are shifted by 908 when darkness appears on the screen.

A7.2 Example of a Beam under Flexion (Transient Stresses)

A 3.5 20 400 mm3 glass beam is cut from an annealed glass sheet and the edges abraded. It is to be set under ﬂexion taking the beam by its extremities. The beam is then placed at 458 from the polarization axis. Again analyser and polarizer are rotated preliminarily by 908 to get darkness on the screen, the contrast being maximum under such conditions while vanishing is observed when aligning the beam along polarization axis (isoclinics along principal stress). The photoelastic contrast increases as applied stresses increases. One observes in Fig. A7.2 under white contrast both edges, one being under compressive stress, the other being under tensile stress (top and bottom respectively) while the beam centre shows minimum

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

288

Appendix 7: Photoelastic Set-Up for Lectures

Fig. A7.1 Set-up for photoelasticity experiments in a classroom (A, analyser; P, polarizer; G, glass specimen; S, screen).

intensity at the neutral line. Note that one does not distinguish here tensile and compressive stresses. This can be done adding a wavelength sheet to the set-up. When ﬂexure is released, photoelastic contrast vanishes, showing that these applied stresses are transient.

A7.3 Example of Tempered Specimens (Residual Stresses)

Two glass specimens 3.5 100 100 and 6 100 100 mm3 were thermally tempered under the same conditions. The two shown in Fig. A7.3 correspond to these two specimens and were obtained under the same conditions with the analyser axis perpendicular to the polarizer axis. Again darkness is to be observed before starting the observation of glass specimens. The degree of temper is expected to be more important for the thicker glass since a larger thermal gradient is generated (Chapter 6). One indeed observes more contrast in the photoelastic image for the thicker specimen. This is particularly obvious at the four corners of the specimens where coloured contrasts are even obtained for the thicker specimens. Notably, not only

Fig. A7.2 Photoelasticity image of a beam under ﬂexion (P, polarizer; A, analyser).

A7.3 Example of Tempered Specimens (Residual Stresses)

Fig. A7.3 Photoelasticity images of two specimens, 3.5 100 100 and 6 100 100 mm3, thermally tempered and observed under the same conditions. The thicker one shows more contrast (P, polarizer; A, analyser).

does the stress intensity play a role in the photoelastic contrast here, but also the glass thickness tH since phase shift b ¼ (2p/l)d is proportional to glass thickness and principal stresses difference s1 s2 (Chapter 11). One further observes the signature left by the nozzles as seen at dawn on car backlights (Chapters 3 and 6). These contrasts appear without applying any forces on the specimens showing that stresses are residual.

289

291

Appendix 8 Instrumented Nanoindentation Applied to Thin Films A8.1 Instrumented Nanoindentation

Instrumented indentation allows for monitoring the penetration of a tip into a specimen as a function of load. This technique has become very popular in thin-ﬁlm technology (Fischer-Cripps, 2004a). In fact, when low loads are used, the observation of indents becomes tedious, requiring dedicated instruments like atomic force and/ or transmission electron microscopes, and is time consuming (Le Bourhis and Patriarche, 2003). Therefore, it has become of importance to extract the mechanical properties from the loading–unloading curves (Fig. A8.1). The test consists of loading up to a maximum value Fm (a hold period may be programmed) and unloading to zero. A typical curve is shown in Fig. A8.1. The loading and unloading curves separate when irreversible deformation is generated in the specimen (only the elastic deformation recovers on unloading). Most indentation machines are load controlled. The tip is ﬁxed to a coil merged into a magnetic ﬁeld. Controlling the intensity of the current through the coil allows the force to be controlled. Because of the Joule effect one has to consider carefully the inherent thermal drift of the machine. Displacement is determined using a capacitive sensor (Fig. A8.2). The tips are categorized into sharp and blunt (see also Chapter 8). Sharp tips are generally three-faced Berkovich tips allowing for a better deﬁnition of the contact area Ac than four-sided Vickers tips. However, the aspect ratio is the same for both tips (Ac ¼ 24.5hc2, where hc is the contact depth). Spherical ‘blunt’ tips are used to determine the overall stress–strain s(e) curves (Le Bourhis and Patriarche, 2003; Section A8.2). The proﬁle of a deformed surface under load is shown in Fig. A8.3. The cone loaded by force Fm penetrates the specimen down to hm. The specimen and cone are in contact to depth hc, that is, up to point B. The specimen is observed to deform elastically around the contact area as discussed also in Chapter 8. Assuming unloading is purely elastic, the surrounding surface recovers to its original position shown as A in Fig. A8.3. The mean pressure under load can be extracted from the load–penetration curves (Fig. A8.1) employing the well-known Oliver and Pharr and Field and Swain Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

292

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.1 Typical loading–unloading curve. These curves separate because the specimen has deformed ‘plastically’ on loading while unloading is mainly elastic.

methods, named after their respective authors (Oliver and Pharr, 1992; Field and Swain, 1993). These methods have several limitations. Firstly, one major assumption of both methods is that only elastic recovery happens while unloading; this might not be strictly the case as revealed for very slight indents and when ﬁlms show viscoelastic response (Le Bourhis and Patriarche, 2003). Secondly, the methodology was derived from the solution to elastic contact problems, while prior to unloading the contact conditions involve plastic deformation. Thirdly, the material around the contact may exhibit substantial pile-up or sink-in, the projected contact area being then either underestimated or overestimated, yielding errors in the hardness values (Oliver and Pharr, 1992; Field and Swain, 1993). Considering a sharp contact, the unloading curve can be ﬁtted by (Oliver and Pharr, 1992) F ¼ kðh hr Þm ; 1 < m < 2

Fig. A8.2 Instrumented indentation principle. Loading is electromagnetic while the displacement sensor is capacitive.

ðA8:1Þ

A8.1 Instrumented Nanoindentation

Fig. A8.3 (a) Schematic indentation proﬁle; (b) Experimental indentation proﬁle (Reprinted from Lim and Chaudhri, 2004, with permission from Taylor & Francis Ltd http://www.informa world.com). Original surface is shown as A; contact between specimen and indenter is up to B. Elastic deformation of the surface is observed all around the indenter.

where F is the load applied to the indenter, h its penetration and hr the residual depth (after complete unloading). Contact stiffness (S ¼ dF/dh) at maximum load is then determined as S ¼ kmðhm hr Þm1

ðA8:2Þ

where hm is the maximum penetration of the indenter. The contact depth hc (Fig. A8.3) is then given by hc ¼ hm eFm =S

ðA8:3Þ

293

294

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

where hm, Fm and S are the penetration, force and stiffness at maximum load and e is obtained from the following equations (Woirgard and Dargenton, 1997; Fig. A8.4). We adopt the modiﬁed Sneddon (1965) solution in the following, although it is still debated in the literature (Lim and Chaudhri, 2004, 2006): e ¼ mð1 gÞ

ðA8:4Þ

1 G½ð1=2Þn þ 1=2 g ¼ pﬃﬃﬃﬃ p G½ð1=2Þn þ 1

ðA8:5Þ

where G is the gamma function, GðxÞ ¼

Ð1 0

et tx1 dt, and

n ¼ 1=ðm 1Þ

ðA8:6Þ

where m is the exponent of the unloading curve deﬁned above. Then, from the contact depth knowledge, contact area is determined by Ac ¼ 24:5hc2

ðA8:7Þ

and hardness is calculated as H ¼ Fm =Ac

ðA8:8Þ

It should be noted that hardness values obtained from instrumented nanoindentation and microindentation may differ signiﬁcantly and this phenomenon is invoked as the indentation size effect (ISE).

Fig. A8.4 e(m) curve.

A8.2 Indentation Strain Field

Another advantage of instrumented nanoindentation is that the elastic properties of materials can be determined. The composite modulus (specimen–tip) E is extracted from rﬃﬃﬃﬃﬃ @F Ac ¼ 2bE S¼ ðA8:9Þ @h p where S is the stiffness at maximum penetration, Ac the contact depth and b is a correcting factor depending on the tip geometry (b ¼ 1.034 for a Berkovich tip). The composite modulus (specimen–tip) E is 1 1 n2D 1 n2S ¼ þ E ED ES

ðA8:10Þ

where E and n are Young’s modulus and Poisson’s ratio, and subscripts D and S indicate diamond and specimen respectively (ED ¼ 1141 GPa, nD ¼ 0.07). The reduced modulus is often referred to as 1 1 n2S ¼ Er ES

ðA8:11Þ

Note that when viscoelastic materials are considered, it is important to control carefully the loading–unloading procedure (Fischer-Cripps, 2004a; Mammeri et al., 2004, 2005). In fact, for such kinds of materials indentation response is time dependent with a characteristic relaxation time TR ¼ h/G, where h and G are the viscosity and shear modulus of the material (Chapter 6; see also Section A8.5.1). Interestingly, some instrumented machines allow for adding a force modulation to the applied force at a given frequency and hence dynamic mechanical analysis can be performed (Chapter 6; Fischer-Cripps, 2004a).

A8.2 Indentation Strain Field

When indenting a sample a plastic zone is generated and surrounded by the undeformed solid. Hence, a plastic strain gradient remains in the specimens after unloading. The representative indentation strain eR is deﬁned as (Tabor, 1951; Johnson, 1985) eR ¼ 0:2d=D for a spherical indenter

ðA8:12aÞ

eR ¼ 0:2tanb for a conical indenter

ðA8:12bÞ

and

where d and D are the residual indent diameter (or contact area diameter) and the sphere diameter respectively, while b is the angle between the original surface and the conical indenter ﬂank. eR increases continuously as load is increased under a spherical tip (Eq. A8.12a). This point has motivated the use of a spherical tip to

295

296

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

determine the overall s(e) stress–strain curve (Field and Swain, 1993). Under a conical indenter the representative strain remains unchanged (assuming a perfect sharpness of the tip), a property that is often referred to as self-similarity or autosimilarity. The self-similarity of the strain ﬁeld under a conical indenter is attributed to the geometric similarity of the tip (Ac / hc2 , where hc is the contact depth). Selfsimilarity is also assumed for non-axisymmetric tips like Berkovich and Vickers tips. Parameter b is then the angle between the original surface and the ﬂank of a conical indenter with equivalent aspect ratio. For instance, for the Vickers and Berkovich tips which are most commonly used, the contact area is Ac ¼ 24:5 hc2 so that b is to be taken as 198. A question has risen as to the signiﬁcance of eR in view of strain gradient (Chaudhri, 1998). Furthermore, Eqs (A8.12) were established originally for metals and applied regardless of the type of material. Indentation residual strain can be determined experimentally in brittle materials (AlAs/GaAs superlattice) using a focussed ion beam (FIB) milled cross-section through the centre of a Vickers indentation. The sub-layers in the superlattice allow then mapping of the deformation, the interfaces between the AlAs (or GaAs) sub-layers being used as markers (Largeau et al., 2005). The distance e between two GaAs layers at different points of the sample was compared to the period eo of the superlattice (Fig. A8.5) and the ez strain component along the loading axis can be calculated using equation ez ¼ (e eo)/eo. Figure A8.5 shows the ez contours, and as reported for metals very high strains and strain gradients are generated just beneath the indent site. The highest ez value is determined to be about 28 % in good agreement with Chaudhri (1998) who estimated the strain e to be as large as 20 % under a Vickers indenter in heavily work-hardened mild steel. These strain values are considerably higher than the representative strain value eR that is commonly accepted for a Vickers geometry (about 7.2 % (Eq. (A8.12b) with b ¼ 198 for a Vickers tip). The representative strain eR is hence to be considered as an averaged strain. Nonetheless, it is still unclear which deformed volume should be considered when averaging the strain (Chaudhri, 1998; Largeau et al., 2002).

A8.3 Hardness, Yield Stress and Representative Flow Stress

Hardness measures the resistance of a surface to contact loading (Tabor, 1951, 1996; Fischer-Cripps, 2004a). Traditionally, a spherical or a Vickers diamond (four-sided) pyramid is loaded on the investigated surface. The hardness (or mean pressure) p is deﬁned by the ratio between the applied load and the projected surface of the permanent deformation left by the indenter: p ¼ Fm =Ap

ðA8:13Þ

We denote it p in this appendix (H in the main text) in order to compare microhardness p and nanohardness H as extracted from nanoindentation curves. As discussed in detail, p and H may differ. Macro-, micro- and nanoindentation

A8.3 Hardness, Yield Stress and Representative Flow Stress

Fig. A8.5 (a) FIB-TEM cross-sectional view of an indented brittle semiconductor (AlAs/GaAs superlattice); (b) ez strain contours as obtained from (a). Strain values are given in percent. The dark area drawn on the graph represents the material punched into the sample (residual indentation).

domains have been deﬁned and hardness values are to be compared in the respective domain since an ISE is reported for many types of materials (Gao et al., 1999; Sangwal et al., 2000; Elmustafa and Stone, 2003). In the macro- and microindentation domains the surface is generally determined after unloading by optical microscopy. We shall refer to this area as Ap (projected area deﬁned above). Going to the nanoindentation domain, observation of the indent becomes tedious

297

298

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

and requires scanning electron microscopy (SEM), atomic force microscopy (AFM) or eventually transmission electron microscopy (TEM) resolutions. Hence, hardness is determined under load and is deﬁned as the ratio of the force to the projected contact area Ac (Section A8.1): H ¼ Fm =Ac

ðA8:14Þ

It should be noted also that hardness values p and H may differ signiﬁcantly. Let us consider for instance the elastic domain (before plastic onset). The indent recovers entirely so that Ap ¼ 0 and p is not deﬁned. In contrast, H can be determined advantageously by mean of an instrumented indentation machine. Also, plastic relaxation of the indents may yield differences between Ap and Ac and this phenomenon has been invoked sometimes to interpret the ISE. It should be noted that for elastic–perfectly plastic materials, the mean pressure under a conical indenter p is generally assumed to be three times the yield stress Y (Tabor, 1951; Johnson, 1985): p ¼ 3Y

ðA8:15aÞ

For the particular case of a Vickers tip, Eq. (A8.15a) is rewritten Hv ¼ 2:8Y

ðA8:15bÞ

These relationships can be extended to strain-hardening materials with good approximation if Y is replaced by the representative ﬂow stress YR measured in simple compression at the representative strain eR (Johnson, 1985): p ¼ 3YR ¼ 3YðeR Þ

ðA8:15cÞ

Strain hardening is often taken as YR ¼ Ke1=n (Hollomon, 1945). In the R literature, it must be said that there has been some confusion between the different Eqs (A8.15) which have been used regardless of their domain of validity. However, the aperture of the tips commonly used is generally large so that the representative strain is below 8 %, which for low strain-hardening materials leads to Y YR. Nonetheless, sharp cube-corner tips are now being employed to lower the plastic onset and, hence, to deform the specimens under smaller loads. For such a tip, Eqs. (A8.15) should be used more carefully. In terms of resolved yield stress Eqs (A8.15) and (A8.15c) are rewritten p ¼ 6tc and p ¼ 6tR (where tR is the representative resolved yield stress and using the Tresca factor). In fact, according to the class of materials, the relationship between and H and Y (or H and t) is to be reconsidered with care since ratio H/Y varies (Gilman, 1973; Johnson, 1985). Hence we shall introduce a constraint factor C into Eqs (A8.15) which is expected to vary according to the type of material: p ¼ CYR

ðA8:15dÞ

A8.3 Hardness, Yield Stress and Representative Flow Stress

A general relationship is written (Marsh, 1964; Johnson, 1985) p 2 1 EeR ¼ 1 þ ln YR 3 0:6 YR

ðA8:15eÞ

Indentation with a conical tip allows determination of the representative ﬂow stress YR at the representative indentation strain eR. Following Johnson’s model, Harvey et al. (1993) and Kramer et al. (1999) suggested that the representative ﬂow stress YR of a material could be determined measuring the plastic zone radius c as a function of the maximum load F applied to the indenter using Eq. (A8.16a) (Le Bourhis and Patriarche, 2003): YR ¼

3 F 2p c 2

ðA8:16aÞ

This relation is established balancing the radial forces at the elastic–plastic boundary (Kramer et al., 1999; Fig. A8.6): F ¼ pc2 sr ðcÞ

ðA8:16bÞ

where the radial stress sr at the elastic–plastic boundary is given by (Johnson, 1985) 2 sr ðcÞ ¼ YR 3

ðA8:16cÞ

The proper use of Eq. (A8.16a) supposes that small indenting loads are applied to the specimens in order to avoid fracture and remain in the plastic regime. This is possible using the nanoindentation technique. Equation (A8.16a) indicates that the plastic zone size varies linearly with the square root of the applied load. Figure A8.7b plots the central plastic zone size c as well as the rosette arm length (LA and SA, Fig. pﬃﬃﬃﬃﬃﬃﬃﬃ A8.7a) as a function of the square root of the maximum load, Fmax , measured in an indented brittle material (single-crystal (1 1 1) GaAs). All the sizes can be measured precisely on TEM plan views (Fig. A8.7a). Very interestingly it can be observed that all sizes (central zone radius c as well as the SA and LA sizes) are observed to increase pﬃﬃﬃﬃﬃﬃﬃﬃ linearly with Fmax as expected from Eq. (A8.16a) (greater discrepancy is obtained for the LA sizes however).

Fig. A8.6 Indentation stress balance.

299

300

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.7 (a) TEM plan view image of an indent site made under 5 mN at room temperature in a brittle semiconductor ((1 1 1)A face of GaAs, g ¼ [220] diffraction condition). The central plastic zone (c), long arms (LA), short arms (SA) and microtwins (M) are shown. (b) Central plastic zone radius c and lengths of the rosette arms (LA and SA) as p a ﬃﬃﬃﬃﬃ function of the square root of ﬃ the maximum applied load ( Fm ) ((1 1 1)A and (111)B indented surfaces of GaAs crystal; Le Bourhis et al., 2004).

It should be noted that AFM can also be employed to determine the plastic zone size measuring the topography of the indent proximity (Harvey et al., 1993; Kramer et al., 1999). In that case, the plastic zone size is estimated from the upset region or pile-up. Except for very small indents where plastic recovery is observed, the upset zone radius determined by AFM shows also a square root dependence on load (Lilleodden et al., 1995). Interestingly, microindentation at elevated temperature also yields a square root dependence on load of the rosette arm length in a wide variety of materials as reviewed by Chaudhri (2004). pﬃﬃﬃﬃﬃﬃﬃﬃ Using the linear variation of the central plastic zone with Fmax plotted in Fig. A8.7, the ﬂow stress is estimated to be about 3.4 GPa yielding an H/YR ratio about 2.5 close to the value expected from the expanding cavity model (H/YR 3; Johnson, 1985).

A8.4 Coating–Substrate Composite Response

Using low load and increasing progressively the load, the instrumented nanoindentation technique allows for investigation of the elastic–plastic response of coatings as well as their adhesion to the substrate (Fig. A8.8). Indeed, the probe size can be adjusted to the ﬁlm thickness using appropriate loads. For dedicated study, in particular when surface roughness is important, cross-sectional nanoindentation can be carried out on smoothly prepared cross-sections and a mechanical proﬁle is extracted (Marot et al., 2002).

A8.4 Coating–Substrate Composite Response

Fig. A8.8 Two different ways to characterize the indentation response of thin ﬁlms either testing a prepared cross-section under constant load (CSN) or testing the ﬁlm surface under decreasing loads (PN).

Mencik et al. 1997 reviewed models to predict the indentation modulus of homogeneous thin ﬁlms on a homogeneous substrate as a function of the penetration. All of them consider the substrate and ﬁlm properties and suppose the ﬁlms are homogeneous: 1 1 hc 1 hc þ f 1f ¼ sf Er Er Er e e

ðA8:17Þ

where superscripts s and f indicate the substrate and ﬁlm respectively. Er is the measured substrate–ﬁlm composite property. Assuming a given function f (for hc ! 0, f ! 0 and for hc ! 1, f ! 1), allows determination of the unknowns (Erf ) once Ers is characterized and Er measured as a function of contact penetration hc (Mencik et al., 1997). A similar procedure can be applied to determine the hardness of the ﬁlms. In fact, the combined contributions of the coating and the substrate are measured. Notably, at equal indentation depth, the inﬂuence of the substrate on the measured hardness is less than on the indentation modulus. Indeed, the plastic strain ﬁeld is much less extended spatially than the elastic strain ﬁeld (Fig. A8.9). From Fig. A8.9, one further observes that the 10 % rule of thumb (in other words, ﬁlm response is determined with relative penetration depth less than 0.1) has to be used very carefully. Beegan and Laugier (2005) reviewed models to predict the indentation hardness of homogeneous thin ﬁlms on a homogeneous substrate as a function of penetration. As for moduli, all of them consider the substrate and ﬁlm properties and suppose the ﬁlms are homogeneous (Bhattacharya and Nix, 1988; Puchi-Cabrera, 2002): hc H ¼ Hs þ ðHf Hs Þf e

0

ðA8:18Þ

301

302

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.9 Hardness and modulus evolution with relative penetration for the same ﬁlm deposited on two different substrates. More rapid convergence at small depth is observed for hardness. The ﬁlm is a hybrid TEOS–PMMA ﬁlm deposited onto glass or PMMA substrates (Mammeri, 2003).

where subscripts s and f indicate the substrate and ﬁlm respectively. H is the measured substrate–ﬁlm composite property. Assuming a given function f0 (for 0 0 hc ! 0, f ! 1 and for hc ! 1, f ! 0), allows determination of the unknowns (Hf) once Hs is characterized and H measured as a function of contact penetration hc. Recently Veprek et al. (2005) emphasized that to measure correctly the hardness of hard coatings on softer substrates, the maximum indentation depth must not exceed 10 % of the thickness of the coating because, above this value, plastic deformation occurs in the softer substrate. Recent FEM simulations of indentation into superhard coatings with hardness 40 GPa revealed that because of the higher strength of these materials, the maximum indentation depth should not exceed about 5 % of the coating thickness in order to avoid plastic deformation in the substrate. Therefore, in order to avoid possible artefacts, Veprek et al. (2005) recommend to use relatively high loads of 30–150 mN, with indentation depths >0.3 mm not exceeding about 5 % of the thickness of the coatings. Their conclusion is that to meet these requirements, coatings 6 mm thick are needed. This requirement is not straightforwardly met (Tavares et al., 2005). Instead, as discussed above the survey of the mechanical response as a function of penetration allows extraction of the ﬁlm contribution.

A8.5 Time-Dependent Response

As mentioned in Section A8.1, when viscoelastic materials are considered, the loading–unloading procedure has to be considered carefully since the mechanical response is time dependent (see also Chapter 6). Time dependence of the indentation

A8.5 Time-Dependent Response

response has been the subject of earlier work (Radok, 1957; Lee and Radok, 1960; Ting, 1966; Johnson, 1985). Because of the growing interest in polymeric and hybrid sol–gel coatings new interest has focused on this subject (Shimizu et al., 1999; Oyen and Cook, 2003; Fischer-Cripps, 2004b; Mammeri et al., 2004; Atanacio et al., 2005; Sakai et al., 2005). Moreover instrumented indentation allows for the monitoring of the overall F(h) curves and allows creep to be studied when a load plateau is programmed. It is important to separate again sharp and blunt indenter geometries. In fact, under a blunt indenter, a general assumption is that plasticity can be neglected. In that case the viscoelastic solution can be obtained from the elastic– viscoelastic correspondence using the hereditary Boltzmann integral. For a sharp indenter, it has to be considered whether plasticity can or cannot be neglected. In the ﬁrst case, the approach is the same as for a blunt contact. If plasticity is to be considered then the solution is complex since elastic, plastic and viscous behaviours are to be considered together. Under indentation, of course, the deformation and stress ﬁelds are complex with a combination of multiaxial compression and shear. We review here phenomenological approaches allowing for F(h) loading curves to be predicted and for creep to be analysed. A8.5.1 Viscoelastic Indentation Curves

The solution for an elastic contact was given by Hertz (1981) and Sneddon (1965) (Chapter 8) for a blunt and sharp indenter respectively. The solutions can be written in the general form (Chapter 8; we suppose the indenter is much more rigid than the specimen) F¼A

E hn 1 n2

ðA8:19aÞ

where A is a geometrical factor and n an exponent equal to 1.5 and 2 for a spherical and a cone indenter respectively. Equation (A8.19a) is rewritten for an incompressible solid (n ¼ 0.5) as F¼A

2G n h ¼ 4AGhn 1n

ðA8:19bÞ

Using the elastic–viscoelastic correspondence with hereditary Boltzmann integral allows for the general solution to be found as (Shimizu et al., 1999; Sakai, 2002; Fisher-Cripps, 2004b; Cheng and Cheng, 2005; Oyen, 2005) ðt dhðt0 Þn 0 FðtÞ ¼ 4A Gðt t0 Þ dt dt0

ðA8:20Þ

0

ðt 1 dFðt0 Þ 0 h ðtÞ ¼ Jðt t0 Þ dt 4A dt0 n

0

ðA8:21Þ

303

304

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.10 Viscoelastic solids (Voigt, Voigt and spring in series, Burger) used to model the indentation creep of viscoelastic solids.

The solution of this integral is completely dependent on the choice of the material relaxation modulus G(t) and compliance J(t). Fischer-Cripps (2004b) proposed empirical solutions for creep analysis during a load plateau (at Fm) based on Maxwell and Voigt elements. The solutions for a conical indenter (Fig. A8.10) are Maxwell element : h2 ðtÞ ¼

p 1 1 Fm cot a þ t 2 Er h

Voigt and spring elements in series : h2 ðtÞ ¼

ðA8:22Þ

p 1 1 Fm cot a þ 1 etEr2 =h 2 Er1 Er2 ðA8:23Þ

1 p 1 1 tEr2 =h2 Burger viscoelastic solid : h ðtÞ ¼ Fm cot a þ t þ 1e 2 Er1 Er2 h1 ðA8:24Þ 2

where a is the semi-angle of the cone, Eri the respective reduced moduli and hi the respective viscosities. These solutions can also be obtained for a spherical contact (Fisher-Cripps, 2004b). The models are applied to a HEMA–TEOS sol–gel ﬁlm under indentation creep (Fig. A8.11). The Maxwell element shows the expected linear dependence of the square of the penetration. This does not ﬁt the experimental data well. In fact, it is necessary to consider a more complex scheme of the solid in order to obtain a representative behaviour. A satisfactory ﬁt is obtained using either a combination in series of Voigt and spring elements or a Burger solid.

A8.5 Time-Dependent Response

Fig. A8.11 Indentation creep curve of HEMA–TEOS thin ﬁlm (Chemin, 2007).

A8.5.2 Viscous Elastic–Plastic Indentation F(h) Curves

Sharp indentation curves of time-dependent materials can be modelled using the Oyen and Cook (2003) viscous elastic–plastic (VEP) model which extends the Sakai (1999) representation of elastic–plastic (EP) materials (Chapter 8). The total displacement of the indenter is taken as the sum of the elastic he, plastic hp and viscous hv displacements: h ¼ he þ hp þ hv

ðA8:25Þ

Because of the geometric similarity of a sharp conical (or Berkovich) indenter, all constitutive equations show the square of the penetration and are assumed to be F ¼ AEr he2

ðA8:26aÞ

F ¼ BHhp2

ðA8:26bÞ

F ¼ Chðdhv =dtÞ2

ðA8:26cÞ

where A (4.4), B (24.6 for a Berkovich indenter) and C are geometrical factors, and Er , H and h the reduced modulus, the true hardness and the quadratic viscosity respectively. Taking the derivation of the displacement equation and combining with constitutive equations yields

h¼

pﬃﬃﬃ dh 1 1 dF 1 1 dF F ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ þ dt 2 AEr F dt 2 BH F dt Ch

ðA8:27Þ

305

306

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Fig. A8.12 Loading–unloading curves of a PMMA–TEOS specimen obtained under periodic load–reload sequence. The model curve is obtained for Er ¼ 7.6 GPa, H ¼ 3.9 GPa, Ch ¼ 1.0 1015 Pa s2. (Reprinted from Mammeri et al., 2004, with permission from Elsevier.)

Once the loading (or unloading) rate is set constant or zero (hold period), Eq (A8.27) can be solved easily yielding h(t). This is illustrated for PMMA–TEOS sol–gel coatings in Figs. A8.12 and A8.13 that show the h(t) solutions under two different loading procedures (Mammeri et al. 2004). One of these shows a holding

Fig. A8.13 Loading–unloading curves of a PMMA–TEOS specimen obtained under loading–hold–rapid unloading sequence. The model curve is obtained for Er ¼ 7.2 GPa, H ¼ 3.9 GPa, Ch ¼ 0.9 1015 Pa s2. (Reprinted from Mammeri et al., 2004, with permission from Elsevier.)

A8.6 Elastic–Plastic Ratios

Fig. A8.14 Normalized loading–unloading curves obtained under two different loads but same loading and unloading times. Specimen is PMMA. Note the superposition of the curves.

period during which time-dependent penetration is observed. Without this holding period, the unloading curve shows unusual curvature: a ‘nose’ can be observed under low unloading rates and results from viscous ﬂow. The presence of such a nose may be detrimental to extract the mechanical properties from the related unloading curves. It is observed that the time-dependent part of the deformation (viscous deformation hv) allows prediction of creep under a holding period (Fig. A8.13). It should be noted that viscous ﬂow happens during the whole indentation procedure. When the unloading time is not negligible as compared to the relaxation time of the material, viscous ﬂow cannot be neglected during unloading. The relaxation time t of the VEP solid may be extracted from the ﬁtting parameter (Oyen and Cook, 2003; Mammeri et al., 2004): t¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ch AE r

ðA8:28Þ

An interesting prediction of the VEP model is that the response is controlled by the total rise time and not by the actual loading rate, which is illustrated for PMMA in Fig. A8.14. The curves were obtained under two different loads but keeping the same loading and unloading time (about 30 s). It is observed using normalized load F/Fmax and normalized depth h/hmax that the curves obtained under two different maximum loads (namely 0.25 and 5 mN) but with the same loading and unloading time superimpose quite well.

A8.6 Elastic–Plastic Ratios

We introduced in Chapter 9 the brittleness index as the hardness–toughness ratio to characterize the competition between the plastic and brittle deformations of glass.

307

308

Appendix 8: Instrumented Nanoindentation Applied to Thin Films

Here again, a similar approach can be used instructively in order to balance the elastic and plastic deformations. Hence, we introduce hardness–elastic modulus ratios in order to quantify the competition between elastic and plastic responses. An instrumented indentation machine allows for extraction of hardness H and elastic modulus E; different ratios have been considered, the simplest one being H/E. The higher the ratio the higher the resistance to plastic deformation and hence the higher the elastic compliance of the ﬁlm. Some authors also use ratio H/E that can be related theoretically to residual depth–maximum depth ratio (Chen and Bull, 2006) and experimentally veriﬁed (Fouquet et al., 2004; Chen and Bull, 2006). Taking again the unloading curve function (Section A8.1) we have F ¼ kðh hr Þm

ðA8:29Þ

Contact stiffness at maximum load is S ¼ kmðhm hr Þm1 ¼ mFm =ðhm hr Þ Hence hm hr ¼ mFm =S

ðA8:30Þ

1 hr =hm ¼ mFm =ðShm Þ

ðA8:31Þ

or

Moreover hm ¼ (p/2)hc (Sneddon, 1965), Fm ¼ HAc and S ¼ @[email protected] ¼ 2bE then

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ac =p,

pﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃ hr HAc H Ac H m 24:5 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ p ﬃﬃﬃ ﬃ p pﬃﬃﬃﬃ 1 ¼m ¼m ¼ hm bE phc E b p 2bE Ac =pðp=2Þhc

or 1

hr H hm E

ðA8:32Þ

As regards indentation, Joslin and Oliver (1990) introduced the ratio H/E 2 that can be extracted without requiring any tip area calibration of the nanoindenter

Tab. A8.1

Elastic–plastic ratios and units.

Elastic–plastic ratio

Unit

H/E H/E H/E 2 H3/E 2

– – Pa1 Pa

A8.6 Elastic–Plastic Ratios

since we have a simple relationship between this ratio and force-to-stiffness ratio F/S2: H F 2b ¼ E 2 S2 p

ðA8:33Þ

Another important ratio is H3/E2 that has units of pressure and is representative of the ﬁlm resistance to plastic deformation (Johnson, 1985). This ratio is widely employed in the development of hard coatings for tribological applications (Musil, 2000). Various elastic–plastic ratios and units are summarized in Table A8.1.

309

311

Appendix 9 Strain and Stress A9.1 Stress and Strain

There are two kinds of forces: surface forces or body forces. Surface forces are distributed over the surface of the specimen (for instance contact between objects), while body forces are distributed within the volume (for instance gravitational, electric, magnetic forces). The mean stress sm resulting from a force F acting over a surface or section S is sm ¼

F S

where F is expressed in N, S in m2 and sm in Pa. Positive values are used for tensile stresses and negative for compressive stresses. In general, the force is inclined to the surface and decomposes into its normal N and tangential T components (Fig. A9.1). The related normal and shear stress components are s¼

N S

t¼

T S

Strain refers to the relative displacement resulting from the applied stresses. Consider a solid under normal stress s. It deforms from size lo to l (Fig. A9.2). Strain is deﬁned as the relative deformation and is written e¼

l lo lo

The logarithmic form is also used: e ¼ ln

l lo

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

312

Appendix 9: Strain and Stress

Fig. A9.1 Surface force, normal and shear stresses.

and reduces for small strains to (see also Appendix 12) e ¼ ln

l lo þ l lo l lo l lo ¼ ln ¼ ln 1 þ lo lo lo lo

Side deformation also occurs and lateral strain is ne where n is Poisson’s ratio (n 0.5). n ¼ 0.5 corresponds to volume conservative deformation. As detailed in the main part of this book, Poisson’s ratio depends on glass type and increases as glass structure packing density increases. It is 0.2 for oxide glasses (Cg 0.5) and 0.4 for metallic glasses (Cg > 0.7). Consider now a solid under shear stress t (Fig. A9.2). Distortion appears and shear strain g is written g ¼ tanu u

A9.2 Stress and Strain Tensors

Considering a general loading of a specimen requires the stress and strain tensors to be considered (Fig. A9.3). Stress tensor [s] is 0

s11 ½s ¼ @ s21 s31

s12 s22 s32

1 s13 s23 A s33

Fig. A9.2 Solid under (a) stress and (b) shear stress; elastic deformation and distortion are exaggerated for clarity.

A9.2 Stress and Strain Tensors

Fig. A9.3 Identiﬁcation of components of stress tensor.

Or using stress s and shear stress t notations 0

s11 ½s ¼ @ t21 t31

t12 s22 t32

1 t13 t23 A s33

Let us deﬁne u, v, w as the displacement vector of any point x, y, z of the solid (Fig. A9.4). Normal strains are written e11 ¼

qu ; qx

e22 ¼

qv ; qy

e33 ¼

qw qz

while shear strains are written g12 ¼ 2e12 ¼

qv qu þ ; qx qy

g23 ¼ 2e23 ¼

qw qv þ ; qy qz

Strain tensor [e] is 0

e11 ½e ¼ @ e21 e31

e12 e22 e32

1 e13 e23 A e33

Or using strain e and shear strain g notations 0 1 e11 g12 =2 g13 =2 ½e ¼ @ g21 =2 e22 g23 =2 A e33 g31 =2 g32 =2

Fig. A9.4 Displacement vector.

g31 ¼ 2e31 ¼

qu qw þ qz qx

313

314

Appendix 9: Strain and Stress

Fig. A9.5 Specimen under uniaxial stress.

A9.3 Uniaxial Tensile Test

Under uniaxial tensile testing (Fig. A9.5), the stress tensor is 0

1 s 0 0 @ 0 0 0A 0 0 0

The strain tensor is in the elastic domain 0

s=E @ 0 0

0 ns=E 0

1 0 0 A ns=E

where E is Young’s modulus and n Poisson’s ratio.

A9.4 Simple Shear

Under simple shear stress (Fig. A9.6), the stress tensor is 0

1 0 t 0 @t 0 0A 0 0 0

Fig. A9.6 Specimen under simple shear.

A9.5 Plane Stress

The strain tensor becomes in the elastic domain 0

1 0 t=2G 0 @ t=2G 0 0A 0 0 0

where G is the shear modulus (E ¼ 2G(1 þ n)). For a viscous ﬂow the strain tensor derivative is 1 0 0 t=2h 0 g=2 0 @ g=2 0 0 0 A ¼ @ t=2h 0 0 0 0 0 0

1 0 0A 0

A9.5 Plane Stress

Under plane stress or two-dimensional state of stress, the stress tensor becomes 0

s11 @ t21 0

t12 s22 0

1 0 sx 0 0 A ¼ @ txy 0 0

txy sy 0

1 0 0A 0

Principal stresses are obtained after diagonalization of the stress tensor. Eigenvalues l are obtained solving [s] [x] ¼ l[x] or ([s] l[1])[x] ¼ [0]. l are the roots of the equation detð½s l½1Þ ¼ 0 ¼ ðsx lÞðsy lÞ t2xy ¼ l2 lðsx þ sy Þ þ sx sy t2xy

We get then

l ¼

¼

sx þ sy

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðsx þ sy Þ2 4ðsx sy t2xy Þ

2 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sx þ sy ðsx sy Þ2 þ 4t2xy 2

Principal stress tensor is written 0

s1 @ 0 0

0 s2 0

1 0 0A 0

sx þ sy ¼ 2

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s s 2 x y þt2xy 2

315

316

Appendix 9: Strain and Stress

with s1 ¼

sx þ sy þ 2

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r s x s y 2 2 þtxy 2

s2 ¼

sx þ sy 2

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r s x s y 2 2 þtxy 2

Under equibiaxial stresses, the stress tensor becomes 0

1 s 0 0 @ 0 s 0A 0 0 0

Opposite principal stresses is also referred as pure shear 0

1 s 0 0 @ 0 s 0 A 0 0 0

A9.6 Hydrostatic Pressure and Stress Deviator

The stress tensor can be separated into a deviator (trace is null) and a hydrostatic tensor: 0 1 s11 s12 s13 B C @ s21 s22 s23 A s31 s32 s33 0 1 1 s12 s11 Trð½sÞ s13 B C 3 B C 1 B C ¼B C s23 s21 s22 Trð½sÞ B C 3 @ A 1 s31 s32 s33 Trð½sÞ 3 01 1 Trð½sÞ 0 0 B3 C B C 1 B C þB C 0 Trð½sÞ 0 B C 3 @ A 1 0 0 Trð½sÞ 3 0 1 0 1 s11 s12 s13 s11 s12 s13 1 B C B C ¼ @ s21 s22 s23 A þ Trð½sÞ½I ¼ @ s21 s22 s23 A þ s½I 3 s31 s32 s33 s31 s32 s33

A9.7 Generalized Hooke’s Law

with Trð½sÞ ¼ s11 þ s22 þ s33

The hydrostatic pressure is s ¼ Trð½sÞ=3 ¼ ðs11 þ s22 þ s33 Þ=3

For simple shear stress, the stress tensor reduces to its deviator (hydrostatic tensor is zero).

A9.7 Generalized Hooke’s Law

Under complex loading and in the elastic domain the stress–strain relationship is referred to as the generalized Hooke’s law: si j ¼ Ci jkl ekl

where Cijkl are the stiffness tensor components. This equation can be inverted into ei j ¼ Ji jkl skl

where Jijkl are the compliance tensor components. For cubic materials, there are only three independent components in the Cijkl matrix. Hooke’s law is then written 0s 1 11

0C

11

B s22 C B C12 B C B Bs C BC B 33 C B 12 B C¼B B s12 C B 0 B C B @ s13 A @ 0 s23 0

C12 C11 C12 0 0 0

C12 C12 C11 0 0 0

0 0 0 C44 0 0

0 0 0 0 C44 0

0 10 e11 1 B C 0 C CB e22 C B C 0 CB e33 C C CB C 0 CB 2e12 C CB C 0 [email protected] 2e13 A 2e23 C44

For an isotropic material, the stiffness tensor can be further simpliﬁed and Hooke’s law is written 0

s11 @ s21 s31

s12 s22 s32

1 0 1 0 s13 s23 A ¼ lTrð½eÞ@ 0 1 0 0 s33

1 0 0 e11 0 A þ [email protected] e21 1 e31

e12 e22 e32

1 e13 e23 A e33

with Tr([e]) ¼ e11 þ e22 þ e33, C11 ¼ l þ2m, C12 ¼ l and C44 ¼ m. C44 ¼ ½(C11 C12), A ¼ C44/½(C11 C12) ¼ 1; see also Appendix 12.

Then

317

318

Appendix 9: Strain and Stress

Parameters l and m are Lame coefﬁcients related to Poisson’s ratio n and Young’s modulus E: n¼

l C12 ¼ 2ðl þ mÞ C11 þ C12

E¼

mð3l þ 2mÞ ðC11 C12 ÞðC11 þ 2C12 Þ ¼ lþm C11 þ C12

The strain tensor is written 0

e11 @ e21 e31

e12 e22 e32

1 0 s11 e13 1 þ n @ s21 e23 A ¼ E e33 s31

s12 s22 s32

1 0 1 1 0 0 s13 n s23 A Trð½sÞ @ 0 1 0 A E s33 0 0 1

A9.8 Kelvin and Maxwell Models

Viscoelasticity is obtained combining elastic and viscous components, the Kelvin and Maxwell models being the most simple (Chapter 6). The stress tensor for a Kelvin solid is 0

s11 B @ s21

s12 s22

1 0 1 s13 1 0 0 C B C s23 A ¼ lðTrð½eÞ þ ul Trð½eÞÞ@ 0 1 0 A

s31

s32

s33

20

e11 6B þ [email protected] e21 e31

e12 e22 e32

0 0 1 1 0

e11 e13 dB C e23 A þ um @ e21 dt e33 e31

The strain tensor for a Maxwell solid is 0 e11 dB @ e21 dt e31

e12

e13

1

C e22 e23 A e32 e33 2 0 s11 s12 1 þ n6d B ¼ 4 @ s21 s22 E dt s31 s32

1 0 s13 s11 1 C B s23 A þ @ s21 t1 s33 s31 0 1 1 0 0 Trð½sÞ n B C Trð½sÞ þ @0 1 0A t2 E 0 0 1

s12 s22 s32

13 s13 C7 s23 A5 s33

e12 e22 e32

13 e13 C7 e23 A5 e33

A9.9 Generalized Maxwell Model

where ul, um, t1 and t2 are coefﬁcients that depend on the viscosity of the material.

A9.9 Generalized Maxwell Model

The stress and strain tensors are separated into their deviators (sij, eij) and volume (s[I], e[I] hydrostatic) tensors (Section A9.5). The stress deviator is written ðt si j ðtÞ ¼ 0

dei j Gðt t0 Þdt0 dt00

while hydrostatic tensor is written ðt sðtÞ ¼ 0

de Kðt t0 Þdt0 dt0

with si j ðtÞ ¼ si j ðtÞ þ sdi j

ei j ðtÞ ¼ si j ðtÞ þ edi j

di j ¼ 1 when i ¼ j; di j ¼ 0 when i 6¼ j

GðtÞ ¼ 2Gc1 ðtÞ

KðtÞ ¼ 3Ke ð3Ke 3Kg Þc2 ðtÞ

where G and Kg are the shear and bulk instantaneous elastic constants and Ke the bulk equilibrium elastic modulus. Using a generalized Maxwell model, relaxation functions is written c1 ðtÞ ¼

n X R w1k expðt=T1k Þ k¼1

and c2 ðtÞ ¼

n X R w2k expðt=T2k Þ k¼1

319

320

Appendix 9: Strain and Stress

Average shear relaxation time is given by TR ¼

n hR X R ¼ w1k T1k G k¼1

Hydrostatic relaxation time is often assumed to be ten times the shear relaxation time (Guillemet and Gy, 1996): c2 ðtÞ ¼ c1 ðt=10Þ

When stress is not pure shear or pure hydrostatic pressure, one can always consider any stress state be the sum of both former components. Under uniaxial loading, relaxation times should be multiplied by (Gy et al., 1994; Guillemet and Gy, 1996) 3 1:2 2ð1 þ nÞ

while for equibiaxial stresses (existing in ﬂat glass) the factor is 3ð1 nÞ 1:9 2ð1 þ nÞ

321

Appendix 10 Flow and Plasticity in Glass A10.1 Introduction

Mechanical properties were presented in two separated parts in the main text: i. Chapter 6 presented elevated temperature behaviour characterized by viscous ﬂow. ii. Chapters 7 and 8 presented low-temperature behaviour characterized by brittleness and plasticity. This presentation tends to separate the phenomena. Plasticity and viscous ﬂow might have similarities and Spaepen (1977) proposed a uniﬁed perspective, strain rate and temperature controlling the mechanical response (Spaepen, 1977; Steif et al., 1982). Figure A10.1 shows the shear stress–temperature map for a glass as proposed originally by Frost and Ashby (1982) for crystalline materials. At elevated temperatures and low strain rates, homogeneous ﬂow controls the glass behaviour. Going to lower temperatures and larger strain rates changes homogeneous ﬂow into heterogeneous ﬂow. As regards homogeneous ﬂow a transition from Newtonian to nonNewtonian ﬂow appears once strain rate increases. This is further analysed below. Spaepen (1977) proposed a general strain–stress relationship as v tV Dg exp 2nE sinh g˙ ¼ D f exp a 2kT kT vf

The ﬁrst term on the right-hand side refers either to the homogeneity (Df ¼ 1, deformed volume fraction being 100%) or to the heterogeneity (Df ! 0) of the deformation. The second term follows free-volume theory and takes into account the glass fragility, that is, the viscosity–temperature deviation from the Arrhenius law (Chapter 6). This term is a constant at a given temperature (constant free volume) unless elevated stresses allow for increasing free volume within the material. This in fact may happen in a reduced volume of the deformed specimen, that is, within slip bands (or less viscous bands). This phenomenon can be taken into account by taking Df ! 0 and reduced viscosity in related bands Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

322

Appendix 10: Flow and Plasticity in Glass

Fig. A10.1 Deformation map. (Reprinted from Spaepen, 1977, with permission from Elsevier.)

(heterogeneous ﬂow). The third term reveals that ﬂow is biased along the stress direction. For low stresses it reduces to tV tV sinh 2kT 2kT yielding Newtonian ﬂow (strain rate being proportional to shear stress). The fourth term is the Eyring term (Macedo and Litovitz (1965) hybrid solution; see also Section 6.1.3.4).

A10.2 From Newtonian to Non-Newtonian Flow

Simmons et al. (1988) showed evidences of a transition from Newtonian to nonNewtonian ﬂow when strain rate was increased or temperature lowered. The data plotted in Fig. A10.2 correspond to silico-soda-lime glass. As strain rate increase, apparent viscosity decreases. The empirical relationship proposed for the apparent viscosity by those authors was ho h¼ 1 þ je˙

A10.2 From Newtonian to Non-Newtonian Flow

Fig. A10.2 Normalized viscosity versus normalized strain rate. (Reprinted from Simmons et al., 1988, with permission from Elsevier.)

where ho is the Newtonian shear viscosity and j an adjustable parameter. Hence SLS glass shows a reduced apparent viscosity under elevated strain rate. Similar behaviour was reported more recently for metallic glasses in the supercooled domain (Kawamura et al., 1998; Lu et al., 2003). Moreover, homogeneous non-Newtonian ﬂow was observed to yield superplasticity, which has important industrial applications. At room temperature (below glass transition) non-Newtonian ﬂow has attracted much attention in the past two decades thanks to instrumented indentation tools that allow for strain rate controlled experiments (Appendix 8). Hardness H is related to yield stress Y,1) the dependence of which on strain rate may be written in the form (Han and Tomozawa, 1990; Keulen, 1993) Y ¼ H=3 ¼ bem

where b is a constant. Indentation strain rate e is for a sharp indenter (Han and Tomozawa, 1990; Le Bourhis and Patriarche, 2003) e¼ 1)

h h

We may neglect strain hardening in glass (Appendix 8; YR ¼ Y). Notably deformation of glass is shown to be elastic–perfectly plastic (Bruck et al., 1994; Xing et al., 1998; Inoue, 2000). In crystalline solids, the motion

and mutual interaction of dislocations gives rise to work hardening, that is, increasing ﬂow stress with strain that yields stable plastic ﬂow. Instead, in glasses there are no dislocations and plastic deformation is unstable.

323

324

Appendix 10: Flow and Plasticity in Glass

Fig. A10.3 (a) Strain rate exponent. T means Han and Tomozawa (1990), K means Keulen, 1993). (Reprinted from Grau et al., 1998, with permission from Blackwell Publishing.) (b) Viscosity as a function of strain rate. (Reprinted from Han and Tomozawa, 1990, with permission from Blackwell Publishing.)

When m ¼ 1 ﬂow is Newtonian, while non-Newtonian ﬂow is obtained for m 6¼ 1. A great deviation from Newtonian ﬂow for soda-lime-silica glass has been observed with m in the range 0.05–0.3 reported in Fig. A10.3 (Han and Tomozawa, 1990; Grau et al., 1998), that is, m is determined to be much below 1. This yields reduced viscous

A10.3 From Homogeneous to Heterogeneous Flow

resistance as observed in Fig. A10.3 and suggested by Douglas (1958). Apparent viscosity can be extracted from indentation data dividing stress and strain rate (Chapter 6). Hence viscosity is written h ¼ cem1

where c is a constant. For m ¼ 1, viscosity is independent of strain rate. The reported experimental viscosity values are shown in Fig. A10.3 as a function of strain rate showing instead a dramatic drop of the apparent viscosity as the strain rate increases. The reported changes in apparent viscosity explain in part the large discrepancy reported for glass viscosity at room temperature in the literature as extensively discussed in Chapter 6. Also, Han and Tomozawa (1990) insist on the inﬂuence of glass surface hydration. In fact, water is known to enter a glass surface and change its superﬁcial property (Chapter 5, Appendix 13). Both molecular diffusion and chemical reaction with the glass network happen. Of much importance also is the intrinsic structure of the glass at such a temperature that is not at equilibrium and dependent on the thermal history (Chapter 6).

A10.3 From Homogeneous to Heterogeneous Flow

At temperatures below the glass transition, non-Newtonian ﬂow is generally also associated with heterogeneous ﬂow. Figures A10.4 and A10.5 show such slip bands in indented and uniaxially compressed glass specimens. The nature of these slip bands has been the subject of controversy and still attracts much scientiﬁc interest. Hagan (1979) showed that conﬁned plasticity at an indent tip in silico-soda-lime glass yielded slip lines that could be observed on sectioning the sample through the indent site. It has been suggested that such slip bands could correspond to Na-rich zones allowing for enhanced ﬂow in soda-lime-silica glass. As discussed in Chapter 9, Na ion diffusion is known to be enhanced under elevated stresses as revealed by Nghiem (1998) at crack tip vicinity. Interestingly, in metallic glasses, ﬂow can be induced in large volumes and the resulting slip lines obtained under uniaxial compression look similar to those observed at the sides of crystalline samples deformed under compression (Pampillo and Chen, 1974; Fig. A10.5). More recently, Schuh et al. (2004) using instrumented indentation showed that metallic glass loading response was dependent on strain rate with emphasized discontinuities in the curves observed under low strain rate. In fact, serrated ﬂow has been reported extensively for many metallic glasses.2) Such serrations are observed in

2)

Metallic glasses have attracted much attention since they can be deformed as bulk over a wide range of temperature including temperatures below Tg (Hufnagel, 1996) and have become available as bulk, the most well known being

Vitreloy developed by Johnson’s team at Caltech (Johnson, 2006). This allowed for great progress in the understanding of plasticity and ﬂow of glass.

325

Fig. A10.4 Heterogeneous ﬂow in indented metallic glass. (Reprinted from Ramamurty et al., 2005, with permission from Elsevier.) (b) The shear band morphology underneath the indenter shown in a higher magniﬁcation image obtained from within the deformed region of (a).

Fig. A10.5 Heterogeneous ﬂow in uniaxially compressed metallic glasses. (Reprinted from Pampillo and Chen, 1974, with permission from Elsevier.)

A10.3 From Homogeneous to Heterogeneous Flow

Fig. A10.6 Serration on loading curves of metallic glasses. (Reprinted from Schuh et al., 2004, with permission from Elsevier.)

Fig. A10.6 as small jumps on the curve. The correlation between serration and slip lines is however still debated. All these observations led several authors to consider the dislocation concept in amorphous solids (G’Sell, 2001). Notably, phenomenologically plasticity and heterogeneous non-Newtonian ﬂow are similar and both characterized by localized ﬂow. Spaepen (1977) suggested that increased free volume (lower viscosity) in localized slip bands (Df ! 0) was responsible for this behaviour in glass. Figure A10.7 shows how under elevated stress an atom forces its path even though initially the free volume at its surrounding is too small for a jump (see also Chapter 6). Supposing such a phenomenon can happen implies that the free volume increases under elevated stresses. This is suspected to happen within slip bands where free volume increase leads to viscosity decrease. Experiments could be conducted on metallic glass bulk under compression showing localized bands along the maximum shear stress direction (458, in fact the angle is slightly less than 458 in compression (428)

Fig. A10.7 Free volume creation.

327

328

Appendix 10: Flow and Plasticity in Glass

Fig. A10.8 Transition from homogeneous Newtonian to non-Newtonian heterogeneous and non-Newtonian homogeneous ﬂow. (Reprinted from Schuh et al., 2004, with permission from Elsevier.)

and slightly above in tension (50–578); Fig. A10.5). It is of interest to mention that Pampillo and Chen (1974) showed preferential etching of these slip bands. More recently, slip bands were revealed under lighter contrast in TEM micrographs (Kim et al., 2002; Chang et al., 2006). Based on serration events, Schuh et al. (2004) showed a new transition from heterogeneous non-Newtonian to homogeneous non-Newtonian ﬂow in metallic glasses using indentation tools under different temperatures (Fig. A10.8). Those authors showed such transitions at very elevated loading strain rates for which only light serrations were observed similar to those observed for very small strain rates. Hence, they suggested that the inhomogeneous deformation domain was surrounded by homogeneous deformation domains; one at small strain rates, the other at large strain rates with frontiers depending on temperature. The question whether at high strain rates ﬂow is homogeneous or inhomogeneous with ﬁner slip bands and serration is still under debate (Jiang and Atzmon, 2003).

329

Appendix 11 Finite Element Analysis Finite element analysis (FEA) or ﬁnite element modelling (FEM) decomposes a solid into a mesh made of discrete elements. For each element, the relevant parameters are supposed to be known (physical, chemical, mechanical properties) or locally determined (stress, temperature). Then after each increment of time the overall behaviour of the object can be determined. A step-by-step procedure is used to determine the behaviour of a glass object with time. Notably, when the shape varies the mesh has to be redeﬁned continuously. This technique has become widely used since it allows complex loading and geometries to be considered that make it very attractive for industry and R&D.

A11.1 FEM of the Pressing of a Parison

We consider ﬁrst the pressing of a parison (Chapter 10; press-blow and press-press techniques). The parison is under a stress gradient and a temperature gradient. Also at elevated temperatures the inﬂuence of gravity on glass ﬂow comes into play. Figure A11.1 shows the mesh that is to be deﬁned again after each penetration increment. Pressure ﬁeld shows a gradient with maxima of intensity at the penetrator proximity. Such a pressure ﬁeld in the glass can be calculated under realistic conditions considering the outside pressure from the mould. The numerical tool can be iterated to adjust viscosity regime, mould geometry and hence achieve optimized glass distribution over the articles. This issue is very important in order to reduce container weight.

A11.2 FEM of the Precision Moulding of a Glass Lens

The second process example considers high-precision lens moulding (Fig. A11.2). Here, great precision in the dimensional calculation is required. The glass blank is moulded between two parallel moulds (upper and lower ones) under pressure. Both Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

330

Appendix 11: Finite Element Analysis

Fig. A11.1 FEM modelling of the pressing of a glass parison; mesh and pressure ﬁeld (Laevsky, 2003).

moulds are curved to achieve the ﬁnal lenses shape. The blank ﬂows progressively while stress and stress gradients increase. Stress gradient is more intense at mould folding where strain gradient is expected as well. One should consider friction between the tools and the lens, which FEM manages. Also, FEM allows adjustment of mould geometric characteristics and tool loading carrying out numerical iterations. In order to improve the prediction precision, Jain et al. (2005) recommend determining the viscosity regime under similar compressive conditions and using these inputs so that the FEM will achieve even more precise predictions of the moulding operation.

A11.3 FEM of Fracture

Moving to the mechanical response at fracture, numerical simulations are of great interest since fracture mechanics requires statistics to be considered. Modelling

A11.3 FEM of Fracture

Fig. A11.2 FEM modelling of the compression moulding of a BK7 glass lens at a forming temperature of 671 8C and with a transition temperature of 557 8C. Predicted stresses are shown. (a) Initial glass blank and mould set-up; (b) compression of the glass blank; (c) ﬁnal lens shape. (Reprinted from Jain et al., 2005, with permission from Blackwell Publishing.)

saves expensive and time-consuming experiments. Also, glazing may involve complex assemblies of several sheets of glass having different strengthening treatments and related interfaces. FEM yields helpful and valuable information in this domain. The study of the resistance of a laminated glass presented in Fig. A11.3 is difﬁcult because of interfaces and sliding. Both glass sheets and polyvinylbutyral (PVB) bond have to be taken into account. Moreover, an impact is a dynamic loading and thanks to FEM great insight into glazing crack propagation is obtained (Du Bois et al., 2003). The dynamic impact of a ball (diameter 300 mm, mass 70 kg and initial velocity 10 m s1) on a laminated safety glass (length 1500 mm, thickness 5 mm) is shown in Fig. A11.3, the

331

332

Appendix 11: Finite Element Analysis

Fig. A11.3 Temporal evolution of an impact on a laminated safety glass. (Reprinted from Du Bois et al., 2003, with permission from Elsevier.)

resistance with time being observed. Du Bois et al. 2003 show very a realistic fracture pattern of the laminated glass, and indicate that the fracture pattern is sensitive to mesh reﬁnement and regularity. The authors assume a failure strain at 0.1 % for the glass and no failure for the PVB interlayer. At 10 ms, the ﬁrst elements fail and cracks start to propagate in different directions (bright areas are failed elements where only the PVB interlayer carries the load). Between 30 and 40 ms, some larger glass fragments are formed, which are still joined by the membrane. This can be observed until the end of the impact at 80 ms. These studies are also helpful in understanding

A11.4 FEM of Contact Loading

how fracture propagates. Experimentally, high-speed photography is required (Chapters 7 and 8). Instead, FEM can be carried out at the appropriate time scale.

A11.4 FEM of Contact Loading

As detailed extensively in Chapter 8, glass response to contact loading is complex, in particular once plasticity and fracture are operating. Stress and strain ﬁelds are

Fig. A11.4 FEM mesh used in the threedimensional analysis of the Vickers indentation experiment by Zeng et al. (1995). (a) General view. (b) Detail of the mesh at the contact region (8524 eight-noded elements, 9914 nodes). (c) Loading–unloading curves of

Vickers indentation on soda-lime glass obtained from the FEM as compared to experimental data reported by Cook and Pharr (1990). H ¼ 5.9 GPa, Y ¼ 2.8 GPa, E ¼ 74.3 GPa. (Reprinted from Zeng et al., 1995, with permission from Elsevier.)

333

334

Appendix 11: Finite Element Analysis

complex (see also Appendix 8). Again FEM is shown to be valuable and allows one to get great insight into glass response. As shown in Fig. A11.4, contact mechanics FEM is shown to account well for plasticity. Zeng et al. (1995) used a mesh with higher resolution at the indenter proximity, where plasticity is important and where stress and strain ﬁelds change rapidly. Using elastic and plastic behaviour inputs, they were able to predict quite well the experimental curves obtained for glass by Cook and Pharr (1990). The next step is to take into account fracture and have a predictable model for contact fracture.

335

Appendix 12 X-Ray Diffraction Analysis of Thin-Film Residual Stresses A12.1 Thin-Film Stress and Strain

Let us consider a ﬁlm under simple equibiaxial stresses. The stress tensor is (Appendix 9) 0

1 s 0 0 @ 0 s 0A 0 0 0

and the strain tensor is 0

ek @0 0

0 ek 0

1 0 0 A e?

ejj and e? being the in-plane and out-of-plane strains respectively. Most deposited FCC metallic thin ﬁlms show two particular orientations or textures: either (0 0 1) or (1 1 1). Crystallites show a or preferential direction along the growth direction (surface normal). In such cases, stress–strain relationships are written s ¼ Mhkl ejj

and hhkl ¼ e ? =ejj

Mhkl is deﬁned as the biaxial modulus and hhkl the ratio of out-of-plane to inplane strains depending on crystallographic direction [hkl]. Mhkl and hhkl are listed for the two respective ﬁlms texture in Table A12.1 We deﬁne now anisotropy ratio A of cubic crystals as A¼

2C44 C11 C12

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

336

Appendix 12: X-Ray Diffraction Analysis of Thin-Film Residual Stresses Tab. A12.1 Biaxial modulus Mhkl and the ratio of out-of-plane to in-plane strains hhkl for the two most common textures of thin FCC films

(0 0 1)

(1 1 1)

ðMC11 C12 ÞðC11 þ 2C12 Þ C11

Mhkl hhkl

2

6C44 ðC11 þ 2C12 Þ C11 þ 2C12 þ 4C44

C12 C11

2

C11 þ 2C12 2C44 C11 þ 2C12 þ 4C44

Most metals (Table A12.2) show elastic anisotropy. Note that a thin ﬁlm is polycrystalline, that is, formed of monocrystalline grains, the size and orientation of which depend on deposition conditions. They will exhibit elastic macroscopic anisotropy only when texture is present, that is, when crystallites show a preferential orientation (001 or 111 for instance). Tungsten is an archetype since the crystallites are elastically isotropic. Hence tungsten ﬁlms show microscopic and macroscopic elastic isotropy. For A ¼ 1 the elastic properties are completely deﬁned by two elastic constants E and n and we have M ¼ E=ð1 nÞ

h ¼ 2n=ð1 nÞ

Note that for n ¼ 0.33, we have h ¼ 1, that is, out-of-plane strain is exactly opposite of the in-plane strain.

Tab. A12.2 Biaxial modulus Mhkl and the ratio of out-of-plane to in-plane strains hhkl for various elements

Element

C11 (GPa)

C12 (GPa)

C44 (GPa)

A

M001 (GPa)

h001

M111 (GPa)

h111

Al V Nb Ta Cr Mo W Fe Ni Pd Pt Cu Ag Au

108 228 246 267 350 460 501 238 246 227 346 168 124 186

61 119 134 161 57 176 198 133 147 176 250 121 93 157

28 42 28 82 101 110 151 110 124 71 76 75 46 42

1.2 0.8 0.5 1.6 0.7 0.8 1 2.1 2.5 2.8 1.6 3.2 3 2.9

100 222 234 233 388 501 542 222 217 130 234 114 76 78

1.1 1 1.1 1.2 0.3 0.8 0.8 1.1 1.2 1.5 1.4 1.4 1.5 1.7

114 187 140 317 324 428 542 352 389 287 337 261 173 188

1 1.2 1.5 0.9 0.6 0.9 0.8 0.6 0.6 1 1.2 0.7 0.9 1.2

A12.2 X-Ray Diffraction Method

Fig. A12.1 X-ray diffraction principle and experimental set-up (four-circle goniometer) with, from right to left, the X-ray source, the sample holder and the detector.

A12.2 X-Ray Diffraction Method

X-ray diffraction (XRD) allows for the precise measurement of diffraction peak positions from which we obtain the inter-planar spacing d according to Bragg’s law: 2d sin u ¼ kl

where l is the wavelength of the radiation and u the incident angle. Calling do the strain-free spacing one can derive the corresponding strain using (Fig. A12.1) e ¼ ðd do Þ=do

or in its rational form (this form is much helpful in the XRD frame; see Appendix 9) e ¼ lnðd=do Þ

Once in-plane djj and out-of-plane d? lattice parameters can be measured, one can determine the stress- and strain-free parameter using the biaxial modulus M, and the

337

338

Appendix 12: X-Ray Diffraction Analysis of Thin-Film Residual Stresses

ratio of out-of-plane to in-plane strains h since we have s¼M

dk do do

and do ¼

d ? þ hdk 1þh

Stress-free parameter do informs on the structure of ﬁlms, in particular the presence of impurities or vacancies that yield a different value of the stress-free parameter as compared to that of the bulk reference. Residual stress amplitude s is of utmost importance for ﬁlm mechanical stability as detailed in Chapter 12. A12.3 1. The e–sin2c Method

The X-ray diffraction method can be generalized in the so-called e–sin2c method (Clemens and Bain, 1992; Hauk, 1997; Faurie et al., 2004; Thomas et al., 2004). It encompasses the strain e measurement as a function of angle c deﬁned as the angle between surface normal and diffracting plane normal. A series of lattice spacing measurements is carried out for different orientations with respect to the surface normal (Fig. A12.2). For an equibiaxial stress state we have ec ¼ ek sin2 c þ e ? cos2 c

Fig. A12.2 X-ray diffraction method.

A12.3 The e–sin2c Method 339

Fig. A12.3 Strain e versus sin2c for a polycrystalline tungsten ﬁlm. Circles: as-deposited; diamonds, squares and triangles: increasing loading states (the specimens being tensile stressed). As stress state changes, the slope of the line, that is, stress varies. (Reprinted from Faurie et al., 2004, with permission from Elsevier.)

that shows only c angle dependence (shown in Fig. A12.2, independent of angle f) and which can be rewritten ec ¼

1þh h ssin2 c s M M

This latter equation shows that plotting ec–sin2c one should obtain a straight line the slope of which yields the stresses in the ﬁlm (Faurie et al., 2004; Fig. A12.3). For a particular direction co strain is zero as observed in Fig. A12.3. The zero strain relationship is written sin2 co ¼ h=ð1 þ hÞ

that for an isotropic material like tungsten is sin2 co ¼ 2n=ð1 þ nÞ

allowing for Poisson ratio to be determined.

341

Appendix 13 Diffusion Diffusion plays an important role in glass science and technology since it governs electrical conductivity, corrosion resistance, container permeability, ion exchange used for inducing index gradient or residual stresses, and ﬁning of glass. The diffusion of gas out of a bubble can control its rate of contraction and is then of utmost importance in bubble removal from glass melt. The rate of shrinkage can be determined from diffusion equations. Diffusion controls the atomic movement and hence the melt homogenization.

A13.1 Diffusion Laws

Diffusion is a time-dependent process. Without external force (electrical ﬁeld, temperature gradient, stress) the diffusion ﬂux Jx along the x direction is proportional to concentration gradient along this direction (we suppose concentration is only a function of x and t): Jx ¼ D

qc qx

The constant of proportionality D is called the diffusion coefﬁcient which is expressed in m2 s1, c is the concentration in m3 and hence Jx is expressed in m2 s1. The negative sign in this expression indicates that the direction of diffusion is opposite to the concentration gradient. This means that diffusion happens from a high- to a lowconcentration region. This relationship between concentration gradient and ﬂux is called Fick’s ﬁrst law and is formally identical to the Fourier law that relates thermal ﬂux to temperature gradient. Consider now matter conservation in an inﬁnitesimal volume of size dx (Fig. A13.1). We derive qc qJx q qc dxdt ¼ ðJx ðxÞ Jx ðx þ dxÞÞdt ¼ D dxdt dxdt ¼ qt qx qx qx Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

342

Appendix 13: Diffusion

Fig. A13.1 Elemental volume subjected to diffusion along x-axis.

qc q qc ¼ D qt qx qx

When D is independent of concentration, Fick’s second law is derived: qc q2 c ¼D 2 qt q x

This equation is to be solved to extract concentration as a function of time and position. The solution to extract c(x, t) is complex and we shall review in Section A13.3 two important solutions, namely for constant surface concentration and for instantaneous plan source. Diffusion coefﬁcient D increases with temperature and follows generally an Arrhenius-type law: DH D ¼ Do exp RT

where DH is the energy barrier and Do the pre-exponential factor. Let us consider ﬁrst the case of neutral molecule diffusion (rare gas) where the molecules do not interact with the glass network (Fig. A13.2). The molecules diffuse through the network excess volume. Values of D and DH are given in Table A13.1 and show that higher diffusion of atomic species is obtained for smaller species. The pre-exponential factor is often taken as a constant in a given range of temperatures. Studies over a wide range of temperatures in particular in silica showed that this factor changes with temperature almost linearly as expected from Fig. A13.2 that plots D/T as a function of reciprocal temperature (Doremus, 1994). Diffusion of water, hydrogen and oxygen is complicated by reactions of these gases with the silica lattice. Indeed corrosion of glass is known to result from the reaction of water with silica (with formation of –OH groups; Chapters 5 and 9). Therefore, molecular diffusion of such species is to be measured and considered carefully. A term has to be added to the diffusion equation: qc q2 c qr ¼D 2 qt q x qt

A13.1 Diffusion Laws

Fig. A13.2 Diffusion of neon in fused silica (open points from Frank et al. (1961); dark points from Perkins and Begeal (1971)).

where r is the concentration of reacted or immobilized species. As shown again in Table A13.1, molecular diffusion of a species is observed to depend on its size. When the diffusing species appear also in the glass network, one expects network diffusion to happen in addition to molecular diffusion and viscosity should be closely linked to diffusion when network diffusion is predominant. For instance viscous activation energy for silica is about 580 kJ mol1 and compares favourably with that measured for Si diffusion in silica (about 700 kJ mol1; Table A13.2). Moreover,

Tab. A13.1

Molecular diffusion coefficients in silica.

Species

Diameter (nm)

He Ne

0.2 0.24

Ar

0.32

H2

0.25

O2 H2O

0.32 0.33

D (cm2 s1) at 25 8C 8

2.4 10 5 1012

2.2 1011

D (cm2 s1) at 1000 8C 5

DH (kJ mol1)

5.5 10 2.5 106

1.1 2.1

1.4 109

0.6

7.3 106

2.0

6.6 109 2 107

6.0 4.0

Authors Swets et al. (1961) Frank et al. (1961); Perkins and Begeal (1971) Perkins and Begeal (1971); Nakayama and Shackelford (1990) Lee (1963); Perkins and Begeal (1971) Norton (1961) Shelby (1961); Doremus (1969)

343

344

Appendix 13: Diffusion Tab. A13.2

Diffusion coefficients.

Naþ in silica O2 in silica Si4þ in silica

Do (m2 s1)

DH (kJ mol1)

Range of temperature (8C)

Authors

2.6 104 328 104

90–125 453 579

200–1000 1200–1400 1100–1400

Frischat (1968) Mickelsen (1984) Brebec et al. (1980)

applying Stokes’ law (k ¼ 6phr) and calling r the radius of the ion, one gets the Stokes–Einstein law: D¼

kT 6prh

This allows determination of a ln(D) versus 1/T plot shown as a continuous line in Fig. A13.3. It applies well for O and Si that form the glass network. Below the transition temperature diffusion mechanisms are still debated. The variation of D is shown for alkali metal ions (Naþ) in Fig. A13.4 and shows a good ﬁt with a constant pre-exponential Do. Interestingly when the concentration of ions increases the diffusion rate increases as well. This is attributed to more lattice network discontinuities that facilitate ion transport. Alkali diffusion is important to consider since electrical conduction of most commercial glasses results from sodium ions. While in many applications glass serves as an electrical insulator, ionic transport

Fig. A13.3 Diffusion coefﬁcient D for oxygen in SLS glass as a function of temperature (according to Yinnon and Cooper, (1980)). We observe two regimes with Q ¼ 57.8 and 208 kJ mol1 below and above Tg respectively. Curvature is observed above Tg as suggested by the Stokes–Einstein law. Note the change in behaviour at Tg.

A13.2 Steady-State Diffusion

Fig. A13.4 Diffusion coefﬁcient D for Naþ in silica as a function of temperature. The line is a guide for the eye. (After Frischat, 1968).

and hence conduction plays an important role in the manufacture of glass. Ionic conduction can be approximately estimated from Einstein’s law s¼

Z2 F 2 Dc RT

where Z is the ionic charge, F the Faraday ¼Ne, N: Avogadro number, D the diffusion coefﬁcient, c the concentration, R the gas constant and T the temperature. A still debated issue is the so-called mixed alkali effect that is one of the classical anomalies of glass science and has important technological consequences. Curiously when a glass contains two alkalis, for instance Naþ and Kþ, diffusion is faster for the one in larger concentration. When chemically tempering a glass, this effect can be used to increase diffusion.

A13.2 Steady-State Diffusion

If diffusion ﬂux does not change with time, a steady-state condition exists. One common example is the diffusion of atoms of a gas through a vessel or tube for which the concentrations (or pressures) of diffusing species on both surfaces (external and internal) are held constant. This is represented in Fig. A13.5. Then J¼D

ci ce tH

345

346

Appendix 13: Diffusion

Fig. A13.5 Steady-state diffusion.

This simple relationship is applied to determine the diffusion coefﬁcient (so-called membrane technique) or the lost volume of gas when a tube is used to transport gaseous reactive species. Consider a tube (Fig. A13.6) of length L, radius r and thickness tH (r). The lost volume of gas is V ¼ VmJ 2prL ¼ VmD(ci ce) 2prL/ tH, where Vm is the molar volume (22.4 l mol1 in standard conditions). Also, air diffusion is to be prevented in electrical lamp envelopes and television tubes. In practice the concentration gradient is unknown in the glass so one has to use Henry’s law that relates internal and external pressures and concentrations: c ¼ SP

where S is the solubility. Alternatively permeability K ¼ DS is employed. Combining the above equations yields J ¼ DS

Pi Pe Pi Pe ¼K tH tH

When a vacuum is maintained inside the bulb or tube we have K ¼

tH J Pe

Fig. A13.6 Steady-state diffusion in liners.

A13.3 Non-steady-State Diffusion

Fig. A13.7 Permeability K variation for different gases in silica (according to Shelby, 1996).

One observes that permeability increases when the atom or molecule size decreases (Fig. A13.7). Since permeability K is proportional to D one observe an Arrhenius evolution of K in the studied domains.

A13.3 Non-steady-State Diffusion

Most practical diffusion situations are non-steady-state ones. The diffusion ﬂux and concentration gradient at some point in a solid vary with time, with a net accumulation or depletion of the diffusing species. This is illustrated in Fig. A13.8. Solutions to Fick’s second law can be extracted using boundary conditions. One practically important solution is for a semi-inﬁnite solid in which surface concentration cs is held constant. These conditions are met for chemical tempering when the

Fig. A13.8 Non-steady-state diffusion under constant surface concentration.

347

348

Appendix 13: Diffusion

Fig. A13.9 Erf(z) function.

glass is immersed in a molten salt solution (Chapter 6) as well as for glass surface hydration (Chapter 5; diffusion depth being much less than the thickness, the two opposite surfaces can be considered separately). We shall assume that before diffusion, solute atoms are uniformly distributed with concentration co. The solution is written cðx; tÞ co x ¼ 1 erf pﬃﬃﬃﬃﬃ cs co 2 Dt

pﬃﬃﬃﬃ R z The erf(z) function is plotted in Fig. A13.9 (erfðzÞ ¼ ð2= pÞ 0 expðy2 Þdy). When initial concentration is zero or negligible (co c or cs) the equation reduces to x cðx; tÞ ¼ cs 1 erf pﬃﬃﬃﬃﬃ 2 Dt

Note that for the same Dt value the diffusion proﬁle is the same. Hence, the same diffusion proﬁle can be obtained more rapidly using a higher temperature and maintaining the same Dt product (decreasing time accordingly). Another important solution is for an instantaneous plan source of diffusing species. This is used to determine diffusion coefﬁcient, using radioactive tracers and plotting log c as a function of x2. This also corresponds to the application of thin coatings with the diffusion element at a plane surface of the studied material (in practice it can be sandwiched, concentration being then taken as half the total value).

A13.3 Non-steady-State Diffusion

Fig. A13.10 Non-steady-state diffusion for an instantaneous plan source.

Diffusion solution is written Q x2 cðx; tÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ exp 4Dt pDt

where Q is the amount of substance per unit area at time zero. It is half a Gaussian curve and is shown in Fig. A13.10 (at x = 0, qc=qxjx¼0 ¼ 0).

349

351

Glossary Annealing: Thermal treatment to remove stress from glassware Batch: Raw materials, properly proportioned and mixed for delivery to the furnace Batch charger: Metallic device for mechanically conducting batch to furnace Batch house: Place where batch materials are received, weighed and mixed before being delivered Blister: Bubble or inclusion in glass Bloom: Surface ﬁlm resulting from attack by moisture or other vapour Blow mould: Metal mould for blowing glass to its ﬁnal shape Blower: Person who forms the glass by blowing Blowpipe: Pipe that the glassmaker uses for gathering glass and blowing Borosilicate glass: Glass containing boron oxide Chain marks: Marks left on the bottom of glass articles by the chain belt Check: Surface crack at glass article surface Chemical durability: Chemical resistance of glass to moisture Chip: Abraded and removed glass piece Cold end: Operations on cold glass (polymer coating, cutting, scoring) Continuous tank: Glass furnace allowing continuous delivery Cord: Glass inhomogeneity Cullet: Waste and recycled broken glass used at furnace input Devitriﬁcation: Crystallization in glass Etch: Glass surface chemical attack for marking and decorating Fining: Operation consisting in homogenizing and eliminating bubbles from glass melt Float glass: Flat glass used in house, building and vehicle windows Forming: Shaping hot glass Gather: Hot glass collected at blowpipe extremity Glass blowing: Shaping glass by air pressure Gob: Hot glass delivered by the feeder Hackle marks: Marks on fracture path Hot end: Operations on hot glass (melting, forming, annealing)

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

352

Glossary

Lehr: Long tunnel oven for annealing glass Melting temperature: Temperature used by commercial furnace for melting raw materials. This is well above the melting temperature deﬁning liquid-crystal phase change often called liquidus temperature Mould: metallic mould used to shape glass Mould mark: mark at mould joint Oven glass: Borosilicate glass Pressed glass: Glassware formed by pressure between a mould and plunger Quartz: Most common form of silica Residual stresses: Permanent stresses reinforcing glass Recycling: Using glass (cullet) as raw material to produce new glass Sagging: Glass deformation under gravity Silica glass: Pure SiO2 glass Silico-soda-lime glass: Glass containing silica associated with soda and lime Soda: Sodium oxide Na2O Stria: Cord Tank: Melting unit Temper: Strengthen glass (build in stress) Tempered glass: Strengthened glass Thermal shock resistance: Resistance to temperature variation Weathering: Attack of glass surface by atmosphere

353

References Aben, H. and Guillemet, C. (1993) Photoelasticity of Glass, Springer-Verlag, Berlin. Abrams, M.B., Green, D.J., Glass, S.J. (2003) J. Non-Cryst. Solids, 321, 10. Acloque, P. (1951) Verres Refract, 5, 247. Adams, G. and Gibbs, J.H. (1965) J. Chem. Phys, 43, 139. Adams, L.H. and Williamson, E.D. (1920) J. Franklin Inst, 190, 597. Akeyoshi, K., Kanai, E., Yamamoto, K., Shima, S. (1967) Rep. Res. Lab. Asahi Glass., 17, 23. Alliche, A. and Le Bourhis, E. (2000) Mater. Sci. Eng. A, 278, 255. Angell, C.A. (1995) Science, 267, 1924. Anstis, G.R., Chantikul, P., Lawn, B.R., Marshall, D.B. (1981) J. Am. Ceram. Soc., 64, 533. Arbad, M., Shelestak, L.J., Harris, C.S. (2005) Am. Ceram. Soc. Bull, 84, 34. Argon, A.S. (1979) Acta Metall., 27, 47. Arora, A., Marshall, D.B., Lawn, B.R., Swain, M.V. (1979) J. Non-Cryst. Solids, 31, 415. Ashby, M.F. (2001) Materials Selection in Mechanical Design, ButterworthHeinemann, Oxford, UK. Ashby, M. and Johnson, K. (2003) Mater. Today., 12, 24. Ashby, M.F. and Jones, D.R.H. (1991) Mate´riaux 1 & 2, Dunod, France. Askeland, D.R. (1989) The Science and Engineering of Materials, PWS-Kent Publishing, Boston, MA. Atanacio, A.J., Latella, B.A., Barbe´, C.J., Swain, M.V. (2005) Surf. Coat. Technol., 192, 254. Auerbach, F. (1891) Ann. Phys. Chem., 43, 61.

Avramov, I. (2005) J. Non-Cryst. Solids, 351, 3165. Barry, F., Chaunac, M., Chiale, D., Cordier, A., Criaud, A., De La Rochefoucauld, C., Deschanet, P., De´sert, C., De Zorzi, M., Faivre Delord, C., Grell, P., Holle, R., Lafarge, M., Levet, J., Macocco, B., Marozeau, D., Thibault, P. (1998) Verre., 12, 12. Bartoe, R.D. and McDanel, V. (2003) Industrie Ce´ram. & Verrie`re, 986, pp. 58. Barton, J. and Guillemet, C. (2005) Le verre, science et technologie, EDP Sciences, Les Ulis, France. Bather, J.M. and Gray, R.A.A.C. (1976) J. Chromatog, 122, 159. Beegan, D. and Laugier, M.T. (2005) Surf. Coat. Technol., 199, 32. Bergman, B. (1984) J. Mater. Sci. Lett., 3, 689. Bergonnier, S., Hild, F., Rieunier, J.B., Roux, S. (2005) J. Mater. Sci., 40, 5949. Berkovich, E.S. (1951) Ind. Diamond Rev., 11, 129. Bertin, M., Faroux, J.P., Renault, J. (1984) Electromagne´tisme 4, Dunod, Paris. Bertoldi, M. and Sglavo, V.M. (2004) J. NonCryst. Solids, 344, 51. Bhattacharya, A.K. and Nix, W.D. (1988) Int. J. Solids Struct., 24, 1287. Boccaccini, A.R. (1997) J. Mater. Sci. Proc. Tech., 65, 302. Bouyne, E. and Gaume, O. (2001) Proc. Int. Cong. Glass, 2, 106. Brebec, G., Seguin, R., Sella, C., Bevenot, J., Martin, J.C. (1980) Acta Metall, 28, 327. Briard, R. (2004) Renforcement du verre par un revetement hybride en formulation aqueuse, Thesis, Rennes.

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

354

References Brinker, C.J. and Scherrer, G.W. (1990) Sol-Gel Science: The Physics and Chemistry of Sol-Gel Processing, Academic Press, San Diego, CA. Brown, J.T., Kobayashi, H., (1998) Am. Ceram. Soc. Bull., 77, 81. Bruck, H.A., Christman, T., Rosakis, A.J., Johnson, W.L. (1994) Scripta Mater, 30, 429. Buehl, W.M. and Ryszyticoskyj, W.P. (1991) SID91 Digest., 667. Buijs, M. (1994) J. Am. Ceram. Soc, 77, 1676. Cable, M. and Smedley, J.W. (1989) Glass Sci. Technol, 30, 39. Caillot, E., Barlier, P., Moffatt-Fairbanks, D.M., Tennent, D.L. (1997) Verre., 3, 3. Carre´, H. (1996) Etude du comportement a` la rupture d’un mate´riau fragile pre´contraint: le verre trempe´, Thesis, Paris. Ce´larie´, F., Prades, S., Bonamy, D., Ferrero, L., Bouchaud, E., Guillot, C., Marlie`re, C. (2003) Phys. Rev. Lett., 90, 0755504. Chandrasekar, S. and Chaudhri, M.M. (1993) Phil. Mag. A, 67, 1187. Chang, H.J., Kim, D.H., Kim, T.M., Kim, T.J., Chattopadhyay, K. (2006) Scripta Mater, 55, 509. Charles, R.J., Hillig, W.B. (1962) The Kinetics of Glass Failure by Stress Corrosion, Union Scientiﬁque Continentale du Verre, Belgium. Chartier, P. (1997) Verre, 3, 5. Chaudhri, M.M. (1998) Acta Mater, 46, 3047. Chaudhri, M.M. (2004) in FRN Nabarro Collection, chapter 70. Chaudhri, M.M. and Kurkjian, C.R. (1986) J. Am. Ceram. Soc., 69, 404. Chaudhri, M.M. and Liangyi, C. (1986) Nature, 320, 48. Chaudhri, M.M. and Phillips, M.A. (1990) Phil. Mag. A, 62, 1. Chemin, N. (2007) Relation entre la structure et les proprie´te´s me´caniques de ﬁlms minces hybrides sol-gel, Thesis, Paris VI. Chen, J. and Bull, S.J. (2006) J. Mater. Res., 21, 2617. Cheng, Y.T. and Cheng, C.M. (2005) J. Mater. Res., 20, 1046. Clemens, B.M. and Bain, J.A. (1992) Mater. Res. Soc. Bull, 17, 46. Coes, L. (1971) Abrasives, Springer Verlag, New York.

Cohen, M.H. and Turnbull, D. (1959) J. Chem. Phys, 31, 1164. Cook, R.F. (2006) J. Mater. Sci., 41, 841. Cook, R.F. and Pharr, G.M. (1990) J. Am. Ceram. Soc., 73, 787. Creuzet, F., Guilloteau, E., Arribart, H. (1993) Fundamentals of Glass Science and Technology, Proc. Second Conf. ESG, 163. Dally, J.W. and Riley, W.F. (1965) Experimental Stress Analysis, McGraw-Hill, New York. DeBast, J. and Gilard, P. (1963) Phys. Chem. Glasses, 4, 117. Dejean-Arrecgros, J. (1978) Petit guide panoramique des roches, Delachaux & Niestle´, Paris. De´riano, S. (2002) Conception chimique de verres silicate´s a` hautes performances me´caniques, Thesis, Rennes. De´riano, S., Jarry, A., Rouxel, T., Sangleboeuf, J.-C., Hampshire, S. (2004) J. Non-Cryst. Solids, 344, 44. Dietzel, A. (1942) Z. Electrochem, 48, 3. Doremus, R.H. (1969) Reactivity of Solids eds J.W.Mitchell, R.C. Devries, R.W. Roberts, P. Cannon, Wiley, New York. pp. 667. Doremus, R.H. (1994) Glass Science, 2nd edn, John Wiley, New York. Doremus, R.H. (2003) Am. Ceram. Soc. Bull, 82, 1. Douglas, R.W. (1958) J. Soc. Glass Technol, 42, 145T. Du Bois, P.A., Kolling, S., Fassnacht, W. (2003) Comput. Mater. Sci, 28, 675. Dubois Petroff, M.P. (2001) Recettes d’Architecture-la cuisine, Massin, Paris. Dugdale, D.S. (1960) J. Mech. Phys. Solids, 8, 100. Durville, D. (2005) J. Mater. Sci., 40, 5941. Elmustafa, A.A. and Stone, D.S. (2003) J. Mech. Phys. Solids., 51, 357. Entwistle, K.M., (1993) J. Mater. Sci., 28, 2007. Ernout, A. et al. (eds) (1947) Pline l’Ancien, Histoire naturelle. Faraday, M. (1830) Phil. Trans. R. Soc, 49. Faraday, M. (1857) Phil. Mag, 14, 401. Faurie, D., Renault, P.O., Le Bourhis, E., Villain, P., Goudeau, P., Badawi, F. (2004) Thin Solid Films, 469/470, 201.

References Ferry, J.D. (1970) Viscoelastic Properties of Polymers, John Wiley, New York. Feynmann, R.P., Leighton, R.B., Sands, M. (1979) Physique, Volume 1, Interedition. Field, J.S. and Swain, M.V. (1993) J. Mater. Res., 8, 297. Fischer-Cripps, A.C. (2004a) Nanoindentation, Springer. Fischer-Cripps, A.C. (2004b) Mater. Sci. Eng. A, 385, 74. Flessel, J.M. (2003) Bull. Soc. Fran. Phys., 140, 28. Fokin, V.M., Zanotto, E.D., Yuritzyn, N.S., Schmelzer, J.W.P. (2006) J. Non-Cryst. Solids, 352, 2681. Fouquet, V., Le Bourhis, E., Pichon, L., Drouet, M., Straboni, A. (2004) Scripta Mater, 51, 899. Franc¸ois-Baillet and Marchi, 2006 Franc¸oisBaillet, B. and Marchi, A. (2006) Est Magazine, 3, 6. Frank, F.C., Lawn, B.R. (1967) Proc. R. Soc. A, 229, 291. Frank, R.C., Swets, D.E., Lee, R.W. (1961) J. Chem. Phys, 35, 1451. Freiman, S.W. (1985) Strength of Inorganic Glass (ed C.R.Kurkjian), Plenum, New York, 197. Friedman, G.S., Cushman, K., Doremus, R.H. (1982) J. Mater. Sci., 17, 994. Frischat, G.H. (1968) J. Am. Ceram. Soc, 51, 528. Frischat, G.H. (1987) in Glas-Struktur und Eigenschaften, (ed. Lohmeyer et al.), Werkstoff Glas I. Ehningen: ex-pert, p. 47. Frischat, G.H. (2002) C.R. Chimie, 5, 759. Frischat, G.H., Heide, G., Muller, B., Weeks, R.A. (2001) Phys. Chem. Glasses, 42, 179. Frost, H.J. and Ashby, M.F. (1982) Deformation-Mechanism Maps, Pergamon, New York, (electronic version available at http://thayer.dartmouth.edu/defmech/). Gadaud, P. and Pautrot, S. (2003) J. NonCryst. Solids, 316, 146. Gao, H., Huang, Y., Nix, W.D., Hutchinson, J.W. (1999) J. Mech. Phys. Solids., 47, 1239. Garcia-Valle`s, M., Gimeno-Torrente, D., Martinez-Manent, S., Fernandez-Turiel, J.L. (2003) Am. Miner, 88, 1996. Gardon, R. (1978) J. Am. Ceram. Soc, 61, 143. Gay, D. (1997) Mate´riaux composites, Hermes, France.

Geandier, G., Denis, S., Mocellin, A. (2003) J. Non-Cryst. Solids, 318, 284. Gilman, J.J. (1949) Rep. Prog. Phys, 12, 48. Gilman, J.J., (1973) The Science of Hardness Testing and Its Research Applications, in ed. J.H.Westbrook, H.Conrad, American Society for Metals, Metal Park, OH, chapter 4. Goodier, J.N. (1936) Phil. Mag, 22, 678. Grau, P., Berg, G., Meinhard, H., Mosch, S. (1998) J. Am. Ceram. Soc, 81, 1557. Greaves, G.N. (1985) J. Non-Cryst. Solids, 71, 203. Green, D.J., Tandon, R., Sglavo, V.M. (1999) Science, 283, 1295. Grifﬁth, A. (1920) Phil. Trans. R. Soc., A221, 163. Grifﬁth, A. (1924) Int. Congr. Appl. Mech., 61, 55. G’Sell, C. (2001) Mater. Sci. Eng. A, 309/310, 539. Guillemet, C. (1990) J. Non-Cryst. Solids, 123, 415. Guillemet, C. and Gy, R. (1996) Rev. Metall, 701. Guin, J.P. and Wiederhorn, S.M. (2004) Phys. Rev. Lett., 92, 215502. Guin, J.P., Rouxel, T., Sangleboeuf, J.C., Melscoe¨y, I., Lucas, J. (2002) J. Am. Ceram. Soc, 85, 1545. Gy, R. (1997) Verre, 3, 21. Gy, R. (1999) Proceedings of Glass Processing Days, Tempere, Finland. Gy, R. (2003) J. Non-Cryst. Solids., 316, 1. Gy, R., Duffre`ne, L., Labrot, M. (1994) J. Non-Cryst. Solids, 175, 103. Hagan, J.T. (1979) J. Mater. Sci., 14, 462. Hainsworth, S.V., Chandler, H.W., Page, T.F. (1987) J. Mater. Res., 11, 2283. Han, W.T. and Tomozawa, M. (1990) J. Am. Ceram. Soc., 73, 3626. Hand, R., Ellis, B., Whittle, B., Wang, F. (2003) J. Non-Cryst. Solids., 315, 276. Harvey, S., Huang, H., Venkataraman, S., Gerberich, W.W. (1993) J. Mater. Res., 8, 1291. Hauk, V. (1997) Structural and Residual Stress Analysis by Non Destructive Methods: Evaluation, Application, Assessment, Elsevier, Amsterdam. Heide, K., Kletti, H., Vo¨lksch, G. (2003) Glass Sci. Technol, 76, 118. Heilmaier, M. and Eckert, J. (2005) Adv. Eng. Mater, 7, 833.

355

356

References Heller, A. (1995) Acc. Chem. Res., 28, 503. Hertz, H.H. (1881) J Reine Angew. Math, 92, 156. Translated and reprinted in English in Hertz’s Miscellaneous Papers, Macmillan, London, 1896. Hillig, W.B. (1962) Modern Aspects of the Vitreous State, vol. II (ed J.D.Mackenzie), Butterworths, London, pp. 152. Ho¨hne, G., Hemminger, W., Flammershein, H.J. (1996) DSC: An Introduction to Practitioners, Springer-Verlag, Berlin. Hollomon, J.H. (1945) AIME Trans., 162, 268. Hufnagel, T.C. (ed) (2006) Scripta Mater, 54, pp. 317. Inglis, C. (1913) Trans. Inst. Naval. Archit., 55. Inoue, A. (2000) Acta Mater, 48, 279. Inoue, A. and Takeuchi, A. (2002) Mater. Trans. JIM, 43, 1892. Inoue, A., Kawamura, Y., Shibata, T., Sasamori, K. (1996) Mater. Trans, 37, 1337. Irwin, G.R. (1958) Fracture, Handbuch der Physik, Springer-Verlag, Berlin. Ishikawa, H. and Shinkai, N. (1982) J. Am. Ceram. Soc., 65, C124. Ito, S. and Taniguchi, T. (2004) J. Non-Cryst. Solids, 349, 173. Jain, A., Firestone, G.C., Yi, A.Y. (2005) J. Am. Ceram. Soc, 88, 2409. James, F.A.J.L. (1991) Phys. Educ, 26, 296. Jiang, W.H. and Atzmon, M. (2003) J. Mater. Res, 18, 755. Johnson, K.L. (1985) Contact Mechanics, University Press, Cambridge. Johnson, W.L. (1996) Mater. Sci. Forum, 225/227, 35. Jones, G.O. (1956) Glass, Methuen’s Monographs on Physical Subjects, Methuen, London. Joslin, D.L. and Oliver, W.C. (1990) J. Mater. Res., 5, 123. Kawamura, Y., Nakamura, T., Inoue, A. (1998) Scripta Mater, 39, 301. Kennedy, C.R., Bradt, R.C., Rindone, G.E. (1980) Phys. Chem. Glasses, 21, 99. Keulen, N.M. (1993) J. Am. Ceram. Soc, 76, 904. Kieffer, J. (2002) Am. Ceram. Soc. Bull, 81, 1. Kim, J.J., Choi, Y., Suresh, S., Argon, A.S. (2002) Science, 25, 654. Kittel, C. (1983) Physique de l’e´tat solide, Dunod, France.

Kittl, P. and Diaz, G. (1988) Int. J. Struc. Mech. Mater. Sci., 24, 99. Klement, W., Willens, R.H., Duwez, P. (1960) Nature, 187, 869. Koike, A. and Tomozawa, M. (2006) J. Non-Cryst. Solids, 352, 3787. Kramer, D., Huang, H., Kriese, M., Robach, J., Nelson, J., Wright, A., Bahr, D., Gerberich, W.W. (1999) Acta Mater, 47, 333. Krause, J.T., Testardi, L.R., Thurston, R.N. (1979) Phys. Chem. Glasses., 20, 135. Kurkjian, C.R. (1963) Phys. Chem. Glasses, 4, 128. Kurkjian, C.R. and Prindle, W.R. (1998) J. Am. Ceram. Soc, 81, 795. Kurkjian, C.R., Kammlot, G.W., Chaudhri, M.M. (1995) J. Am. Ceram. Soc., 78, 737. Laevsky, K.Y. (2003) Pressing of glass in bottle and jar manufacturing: numerical analysis and computation, PhD thesis, Eindhoven University of Technology. Landau, L. and Levich, B. (1942) Acta Physiochim., 17, 42. Langmuir, I. (1933) J. Chem. Phys., 1, 756. Largeau, L., Patriarche, G., Le Bourhis, E. (2002) J. Mater. Sci. Lett, 21, 401. Lawn, B. (1993) Fracture of Brittle Solids, Cambridge Solid State Science Series, Cambridge. Lawn, B. (1998) J. Am. Ceram. Soc., 81, 1977. Lawn, B.R. and Evans, A.G. (1977) J. Mater. Sci., 12, 2195. Lawn, B.R. and Marschall, D.B. (1979) J. Am. Ceram. Soc., 62, 347. Le Bourhis, E. (1996) Vitriﬁed bonded abrasives: post-annealing inﬂuence on residual stresses and wheel strength, Saint-Gobain internal report. Le Bourhis, E. (1998a) Endommagement du verre par contact, Saint-Gobain internal report. Le Bourhis, E. (1998b) Verre, 4, 5. Le Bourhis, E. and Le Guiner, F. (1986) Report, Laboratoire de recherche des Muse´es de France, Paris. Le Bourhis, E. and Metayer, D. (2000) J. Non-Cryst. Solids, 272, 34. Le Bourhis, E. and Patriarche, G. (2003) Prog. Cryst. Growth Charac. Mater, 47, 1. Le Bourhis, E. and Rouxel, T. (2003) J. NonCryst. Solids, 316, 153.

References Le Bourhis, E., Gadaud, P., Guin, J.-P., Tournerie, N., Zhang, X.H., Lucas, J., Rouxel, T. (2001a) Scripta Mater, 45, 317. Le Bourhis, E., Largeau, L., Patriarche, G., Rivie`re, J.P. (2001b ) J. Mater. Sci. Lett, 20, 1361. Le Bourhis, E., Patriarche, G., Largeau, L., Rivie`re, J.P. (2004) J. Mater. Res, 9, 131. Le Houe´rou, V., Sangleboeuf, J.C., De´riano, S., Rouxel, T., Duisit, G. (2003) J. NonCryst. Solids, 316, 54. Lee, E.H. and Radok, J.R.M. (1960) Trans. ASME Ser. E, J. Appl. Mech., 27, 438. Lee, E.H., Rogers, T.G., Woo, T.C. (1965) J. Am. Ceram. Soc, 48, 480. Lee, R.W. (1963) J. Chem. Phys, 38, 448. Lehmann, J.C. (2005) Bull. Soc. Fran. Phys., 150, 4. English version: Europhysicsnews 2006, 37, 23. Levelut, C., Faivre, A., Le Parc, R., Champagnon, B., Hazemann, J.-L., David, L., Rochas, C., Simon, J.P. (2002) J. Non-Cryst. Solids, 307/310, 426. Lilleodden, E.T., Bonin W, W., Nelson, J., Wyrobek, J.T., Gerberich, W.W.(1995) J. Mater. Res.,10,2162. Lim, Y.Y. and Chaudhri, M.M. (2004) Phil. Mag., 84, 2877. Lim, Y.Y. and Chaudhri, M.M. (2006) Mech. Mater., 38, 1213. Livshits, V.Y., Tennison, D.G., Gukasyan, S.B. (1982) Sov. J. Glass Phys. Chem., 8, 463. Lornage, T. (2004) Optimisation des bouteilles par mode´lisation, Lecture, Re´union annuelle GDR Verre. Loubet, J.L., Georges, J.M., Meille, J. (1986) Microindentation Techniques in Materials Science and Engineering (eds P.J.Blau and B.R.Lawn), ASTM International, Philadelphia, PA, pp. 72. Lu, J., Ravichandran, G., Johnson, W.L. (2003) Acta Mater, 51, 3429. Lucas, J. (1999) Curr. Opin. Solid State Mater Sci. 4, 181. McCurty, C. (2000) Proceedings of Coating on Glass Workshop, Livermore, CA, p. 5. Macedo, P.B. and Litovitz, T.A. (1965) J. Chem. Phys, 42, 245. Mackenzie, J.D. (1963) J. Am. Ceram. Soc., 46, 461. McKown, C. (2000) Proceedings of Coating on Glass Workshop, Livermore, CA, p. 8.

McMillan, P.W. (1979) Phys. Educ, 14, 441. Macosco, C.W. (1994) Rheology: Principles, Measurements and Applications, VCH, New York. Malkin, S. (1989) Grinding Technology, Theory and Applications of Machining with Abrasive, Ellis Horwood, Chichester, UK. Malzbender, J., de With, G., den Toonder, J. (2000) J. Mater. Res., 15, 1209. Mammeri, F. (2003) Relation entre la structure et les proprie´te´s me´caniques de ﬁlms minces hybrides organiquesinorganiques pre´pare´s par voie sol-gel, Thesis, Paris VI. Mammeri, F., Le Bourhis, E., Rozes, L., Sanchez, C., Huignard, A., Lefevre, D. (2004) J. Non-Cryst. Solids, 345/346, 610. Mammeri, F., Le Bourhis, E., Rozes, L., Sanchez, C. (2005) J. Mater. Chem., 15, 3787. Mamor, M., Dufour-Gergam, E., Finkman, L., Tremblay, G., Meyer, F., Bouziane, K. (1995) Appl. Surf. Sci., 91, 342. Markovsky, A. and Soules, T.F. (1984) J. Am. Ceram. Soc, 67, C56. Marot, L., Le Bourhis, E., Straboni, A. (2002) Mater. Lett., 56, 76. Marschall, D.B., Lawn, B.R., Evans, A.G. (1982) J. Am. Ceram. Soc., 65, 561. Marsh, D.M. (1964) Proc. R. Soc, A279, 420. Mattoni, A., Colombo, L., Cleri, F. (2005) Phys. Rev. Lett., 95, 115501. Mencik, J., Munz, D., Quandt, E., Weppelmann, E.R., Swain, M.V. (1997) J. Mater. Res., 12, 2475. Meyerhofer, D. (1978) J. Appl. Phys., 49, 3993. Mickelsen, J.C. (1984) Appl. Phys. Lett, 45, 1187. Mills, J.J. (1974) J. Non-Cryst. Solids, 14, 255. Morris, D.J., Myers, S.B., Cook, R.F. (2004) J. Mater. Sci., 39, 2399. Moseler, D., Heide, G., Frischat, G.H. (2002) Glass Sci. Technol., 75, 174. Moynihan, C.T. (1996) Structural relaxation and the glass transition, Structure, Dynamics and Properties of Silicate Melts (eds J.F. Stebbins, P.F. McMillan, D.B. Dingwell), Mineral Society of America. Mozdierz, N., Le Bourhis, E., Peyrot, A., Rivie`re, J.P. (1993) Ce´ramiques, polyme`res et mate´riaux composites, Encyclope´die CLARTE, 1, 3390.

357

358

References Murphy, D.L. (2005) Am. Ceram. Soc. Bull, 84, 41. Musil, J. (2000) Surf. Coat. Technol., 125, 515. Nakayama, G.S. and Schackelford, J.F. (1990) J. Non-Cryst. Solids, 126, 249. Narayanaswamy, O.S. (1978) J. Am. Ceram. Soc, 61, 146. Neely, J.E. and Mackenzy, J.D. (1968) J. Mater. Sci., 3, 603. Nghieˆm, B. (1998) Thesis, Universite´ Paris-VI. Ngoˆ, H. and Ngoˆ, C. (1988) Physique statistique, Masson, Paris. Nieh, T.G., Schuh, C., Wadsworth, J., Li, Y. (2002) Intermetallics, 10, 1177. Norton, F.J. (1961) Nature, 191, 701. Novikov, V.N. and Sokolov, A.P. (2004) Nature, 431, 961. Oliver, W.C. and Pharr, G.M. (1992) J. Mater. Res., 7, 1564. Orowan, E. (1949) Rep. Prog. Phys., 12, 185. Oyen, M.L. (2005) J. Mater. Res., 20, 2094. Oyen, M.L. and Cook, R.F. (2003) J. Mater. Res., 18, 139. Palucka, T. (2006) Mater. Res. Soc. Bull, 31, 697. Pampillo, C.A. and Chen, H.S. (1974) Mater. Sci. Eng., 13, 181. Pantano, C.G., Bojan, V., Verita, M., GeottiBianchini, F., Hreglich, S. (1993) 2nd Conf. European Soc. Glass Sci. Techn., Venice. Paris, P.C. and Sih, G.C. (1965) ASTM Spec. Tech. Publ., 381, 30. Patriarche, G., Le Bourhis, E., Khayyat, M.M., Chaudhri, M.M. (2004) J. Appl. Phys., 96, 1464. Pavelchek, E.K. and Doremus, D.H. (1974) J. Mater. Sci., 9, 1803. Pe´rez, J.P., Carles, R., Fleckinger, R. (1997) Electromagne´tisme, Masson, Paris. Perkins, W.G. and Begeal, D.R. (1971) J. Chem. Phys, 54, 1683. Perriot, A. (2005) Nanoindentation de couches minces deposes sur substrat de verre de silice, Thesis, Paris VI. Peter, K.W. (1964) Glasstech. Ber., 37, 333. Piellard, M., 2005 Etude de la liaison Platine-Alumine, Thesis, Poitiers. Pilkington, A. (1969) Proc. R. Soc. Lond. A, 314, 1. Priven, A.I. (2004) Glass Technol, 45, 244.

Puchi-Cabrera, E.S. (2002) Surf. Coat. Technol, 160, 177. Pugno, N.M. and Ruoff, R.S. (2006) J. Appl. Phys., 99, 024301. Radok, J.R.M. (1957) Q. Appl. Math, 15, 198. Ramamurty, U., Jana, S., Kawamura, Y., Chattopadhyay, K. (2005) Acta Mater, 53, 705. Rawlings, R.D., Wu, J.P., Boccaccini, A.R. (2006) J. Mater. Sci, 41, 733. Redner, A.S. (1998) Measurement of Residual Strain in Glass Products, Short course lecture notes, Strainoptics Technologies. Rehren, T. (2006) GEO, 334, 118. Rekhson, S.M. (1986) (eds D.R.Uhlmann and N.J.Kreidl), Glass Science and Technology, Academic, Orlando, FL, vol. 3, chap. 1. Reuss, R.H., Hopper, D.G., Park, J.G. (2006) Mater. Res. Soc. Bull., 31, 447. Ridealgh, J.A. (2006) Mater. Res. Soc. Symp. Proc., 890, Y01-10.1. Rizkalla, A.S., Jones, D.W., Miller, R.P. (1996) Brit. Ceram. Trans., 95, 151. Rouxel, T. (2006) C. R. Mecanique, in press. Rouxel, T. and Sangleboeuf, J.C. (2000) J. Non-Cryst. Solids, 271, 224. Rouxel, T., Yoshida, S., Shang, H., Sangleboeuf, J.C. (2006) Mater. Res. Soc. Proc., 904, BB02-03.1. Ryu, S.R. and Tomozawa, M. (2006) J. Non-Cryst. Solids, 352, 3929. Sado, G. and Sado, M.C. (1991) Les plans d’expe´riences, AFNOR Technique, France. Sakaı¨, M. (1999) J. Mater. Res, 14, 3630. Sakaı¨, M. (2002) Phil. Mag. A, 82, 1841. Sakaı¨, M., Sasaki, M., Matsuda, A. (2005) Acta Mater, 53, 4455. Sangwal, K.J. (2000) Opto Adv. Mater., 2, 105. Scherer, G.W. (1982) J. Am. Ceram. Soc, 65, 352. Scherer, G.W. (1996) Relaxation in Glass and Composites, Wiley Interscience, New York. Scholze, H. (1991) Glass: Nature, Structure, and Properties, Springer-Verlag, New York. Schottner, G. (2001) Chem. Mater., 13, 3422. Schuh, C.A., Lund, A.C., Nieh, T.G. (2004) Acta Mater, 52, 5879. Schzalke, K. (1981) Test Technique in Fracture, Pergamon Press. Sehgal, J., Nakao, Y., Takahashi, H., Ito, S. (1995) J. Mater. Sci. Lett., 14, 167.

References Sehgal, J. Nakao, Y. Takahashi, H. Ito, S. Patent EP 07570020A1. Sglavo, V.M. and Green, D.J. (2001) J. Eur. Ceram. Soc., 21, 561. Shang, H. and Rouxel, T. (2005) J. Am. Ceram. Soc., 88, 2625. Shelby, J.E. (1961) J. Am. Ceram. Soc, 54, 125. Shelby, J.E. (1996) Handbook of Gas Diffusion in Solids and Melts, ASM International, Materials Park, OH. Shen, J. and Green, D.J. (2004) J. Non-Cryst. Solids, 344, 79. Sheng, H.W., Luo, W.K., Alamgir, F.M., Bai, J.M., Ma, E. (2006) Nature, 439, 419. Shimizu, S., Yanagimoto, T., Sakai, M. (1999) J. Mater. Res., 14, 4075. Shiue, Y.S., Matthewson, M.J., Kurkjian, C.R., Biswas, D.R. (1996) SPIE, 2611, 117. Sih, G. (1972) Mechanics of Fracture, Wolters Noordhoff. Simmons, J.H., Ochoa, R., Simmons, K.D., Mills, J.J. (1988) J. Non-Cryst. Solids, 105, 313. Smith, J.F. and Zheng, S. (2000) Surf. Eng., 16, 143. Sneddon, I.N. (1965) Int. J. Eng. Sci., 3, 47. Spaepen, F. (1977) Acta Metall., 25, 407. Steif, P.S., Spaepen, F., Hutchinson, J.W. (1982) Acta Metall, 30, 447. Stella, A. and Verita, M. (1993) 2nd Conf. European Soc. Glass Sci. Techn., Venice. Stoney, G.G. (1909) Proc. R. Soc. Lond., A82, 172. Sundar, V.C., Yablon, A.D., Grazul, J.L., Ilan, M., Aizenberg, J. (2003) Nature, 424, 899. Suscavage, M.J. and Pantano, C.G. (1983) Glastech. Ber., 56K, 498. Swain, M.V. (1981) J. Mater. Sci., 16, 151. Swets, D.E., Lee, R.W., Frank, R.C. (1961) J. Chem. Phys, 34, 17. Tabor, D. (1951) The Hardness of Metals, Oxford at Clarendon Press, London. Tabor, D. (1996) Phil. Mag A., 4, 1207. Tammann, G. (1925) The States of Aggregation, Van Nostrand, New York. Tanaka, H. (2005) J. Non-Cryst. Solids, 351, 3371, 3385, 3396. Tandon, R. and Cook, R.F. (1992) J. Am. Ceram. Soc., 75, 2877. Tandon, R. and Cook, R.F. (1993) J. Am. Ceram. Soc., 76, 885.

Tavares, C.J., Vidrago, C., Rebouta, L., Rivie`re, J.P., Le Bourhis, E., Denanot, M.F. (2005) Surf. Coat. Technol, 200, 288. Tawakoli, T. (1993) High Efﬁciency Deep Grinding, VDI-Verlag, Germany. Thomas, O., Labat, S., Bigault, T., Gergaud, P., Bocquet, F. (2004) J. Meta. Nanocryst. Mater, 19, 129. Thonggoom, R. and Funkenbusch, P.D. (2005) J. Mater. Sci., 40, 4279. Thornston, J.A. and Hoffman, D.W. (1989) Thin Solid Films., 171, 5. Tillett, J.P.A. (1956) Proc. Phys. Soc. B, 69, 47. Timoshenko, M. (1951) The´orie des plaques et des coques, Librairie Polytechnique, France. Ting, T.C.T. (1966) J. Appl. Mech, 33, 845. Tomozawa, M. (1998) Phys. Chem. Glasses., 39, 65. Tool, A.Q. (1946) J. Am. Ceram. Soc, 29, 240. Turnbull, D. and Cohen, M.H. (1961) J. Chem. Phys, 34, 120. Tyagi, V. and Varshneya, A.K. (1998) J. NonCryst. Solids, 238, 186. Van Mol, A.M.B., Alcott, G.R., Allendorf, M.D. (2005) Am. Ceram. Soc. Bull., 84, 37. Veprek, S., Veprek-Heijman, M.G.J., Karvankova, P., Prochazka, J. (2005) Thin Solid Films., 476, 1. Wang, T.J. (1997) Glass Technol, 38, 104. Wang, W.H., Dong, C., Shek, C.H. (2004) Mater. Sci. Eng. R, 44, 45. Warren, P.D. (1995) J. Eur. Ceram. Soc., 15, 201. Watanabe, T., Puratsubaki, K., Benino, Y., Saitoh, H., Komatsu, T. (2001) J. Mater. Sci., 36, 2427. Weibull, W.A. (1951) J. Appl. Phys., 18, 293. Weibull, W.A. (1952) Appl. Mech. Rev., 5, 11. Westbrook, J.H. (1960) Phys. Chem. Glasses, 1, 32. Wiederhorn, S.M. (1967) J. Am. Ceram. Soc., 50, 407. Wiederhorn, S.M. and Bolz, L.H. (1970) J. Am. Ceram. Soc., 53, 543. Wiederhorn, S.M. and Hockey, B.J. (1980) J. Non-Cryst. Solids, 38/39, 433. Williams, K.F.E., Johnson, C.E., Greegrass, J., Tilley, B.P., Gelder, D., Johnson, J.A. (1997) J. Non-Cryst. Solids, 211, 164. Williams, M.L., Landel, R.F., Ferry, J.D. (1955) J. Am. Chem. Soc, 77, 3701. Woirgard, J. and Dargenton, J.C. (1997) J. Mater. Res., 12, 2455.

359

360

References Wu, D., Lu, G., Jiang, H., Li, Y. (2004) J. Am. Ceram. Soc., 87, 1799. Wu, D., Zhou, J., Li, Y. (2006) J. Mater. Sci, 41, 5630. Xing, L.Q., Bertrand, C., Dallas, J.P., Cornet, M. (1998) Mater. Sci. Eng. A, 241, 216. Yinnon, H. and Cooper, A.R. (1980) Phys. Chem. Glasses, 21, 204. Yoshida, S., Isono, S., Matsuoka, J., Soga, N. (2001) J. Am. Ceram. Soc., 84, 2141. Yoshida, S., Sangleboeuf, J.C., Rouxel, T. (2005) J. Mater. Res., 20, 3404. Zachariasen, W.H. (1932) J. Am. Chem. Soc, 54, 3841. Zandonella, C. (2005) Courrier Int, 755, 60. Zarzycki, J. (1982) Les verres et l’e´tat vitreux, Masson, Paris. [Glasses and the Vitreous State, Cambridge University Press, Cambridge, 1991.] Zeng, K., Giannakopoulos, A.E., Rowcliffe, D.J. (1995) Acta Metall. Mater, 43, 1945. Zhou, J., Wang, Y., Xia, Y. (2006) J. Mater. Sci., 41, 5778. Zinck, P., Pays, M.F., Rezakhnlou, R., Gerard, J.F. (1999) Phil. Mag. A., 79, 2103. Zou, X. and Toratani, H. (2001) J. Non-Cryst. Solids, 290, 180.

Web Sites http://thayer.dartmouth.edu/~defmech/ http://www.musee.ensmp.fr/gm// lettres.html http://www.saint-gobain.com/fr/html/ groupe/verre_plat.asp http://www.saint-gobain-glass.com/fr/ b1107.htm http://www.saint-gobain-glass.com/saint-just/ http://www.saint-gobain.com/fr/html/ investisseurs/pdf/LeGuide2i.pdf http://www.sharplesstress.com/ http://www.strainoptic.com/ http://www.tamglass.com/ http://www.webelements.com/webelements/

Video ‘C’est pas sorcier se met au verre’, France Te´le´vision (FR3).

361

Index a abrasion –performance 186–188 –principles 186–188 Adams and Williamson 121 ageing 191ff Akeyoshi chart 151 alkali –diffusion 78–81, 130, 131, 195, 196, 341–345 –mixed 345 –modiﬁer 57–60 –rich regions 60 alumino-silicate glass 37, 85, 88, 131, 134 –applications 130, 131, 235ff –composition 27 annealing 83ff, 203ff annealing point 85 applications of glass –abrasive tools 49 –containers 44–46 –ﬁbres for –insulation 48f –reinforcement 48f –glazing 39–44 –optical glass 46 atmosphere 29, 36, 61, 78f, 208, 210, 212 atomic bond see bonds Auerbach’s law 165f

blowing 30, 35, 207, 216f blowpipe 30 blunt contact 162 Botzmann hereditary integral 116 bonds –covalent 6–8 –data 5–10 –energy 6–10, 267–270 –formation 267–270 –ionic 5–8 –metallic 7 –Van der Waals 6f borosilicate glass –applications 44–46 –composition 37 –structure 64 Brewster 229 bridging oxygen 53ff, 135ff, 161ff brittle fracture see fracture brittleness –deﬁnition 180f –index 180f –measurement 180f bubble –detection 225 –diffusion 341–345 –elimination 83–86, 207f, 277f –size 277f buckling 18 Burger solid 111–113, 303f

b

c

batch 204f beam –fracture 155f –ﬂexure 19–22 –photoelasticity 287f –shape 18–23

calorimetry 103f ceramics –advantages/drawbacks 7 –brittle fracture 135ff –contact resistance 161ff –group 7f, 15–17

Glass; Mechanics and Technology. Eric Le Bourhis Copyright ß 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim ISBN: 978-3-527-31549-9

362

Index chalcogenide glass –applications 47f –contact resistance 174–177 –structure 65 Charles and Hillig theory 195 chart –thermal expansion/Young modulus 15–18 –toughness 10–12 –transparency 15–18 –strain at rupture/thermal expansion 15–18 –yield strength 10–12 –Young modulus 10–12 –Young modulus/density 18–23 –Young modulus/transition temperature 136–139 chemical –inertness 13, 39, 44f –reactions 78f –tempering 44, 130f, 138, 148, 151f, 181, 345ff –vapour deposition (CVD) 39ff, 235ff, 257 –process 243f chip 167–169 class of materials 5–10 coating 240–245, 248–151, 300–303, 306, 309 compaction 171f, 174 composites –advantages/drawbacks 7 –group 6 compositions of glasses 25–29 computer simulation see ﬁnite element analysis conductivity 206, 341 cold end coating 218 cone crack 164–167 contact mechanics 161ff, 291ff container –applications 44–50 –coating 203ff –history 34f –process 203ff continuous random network (CRN) 54 corrosion 53ff, 191ff cost 5ff, 235ff covalent bond 6, 8, 59, 65 crack 135ff, 161ff, 191ff –branching 139 –healing 201 –propagation 147, 193, 196

crash 329ff creep 107f, 113f, 118, 303–307 crown 33f crystallisation 53, 66, 70–76 cullet 204, 225 cutting –machine 189 –principles 188–190 CVD see chemical vapour deposition

d delayed –elastic strain 113 –fracture 191ff density 7, 9, 10, 12, 17, 61–66, 77, 184, 185 deposition 212, 218, 220, 237, 239–241, 243f, 252, 254 devitriﬁcation 75f Dietzel’s ﬁeld 59 diffusion –coefﬁcient 341–345 –laws 341–345 –of alkali 80f, 195f, 341–345 –of gas 341–345 –non-steady state 347–349 –steady state 345–347 dilatometry 101–103, 271 dip coating 250 display panels –stability 238f –structure 236f distance of order 7f drawing 218f drilling 188–190 dynamic mechanical analysis 109–111

e early glasses 29–32 elasticity 83ff, 135ff, 311ff elastic modulus 115, 129, 137, 163, 174, 271, 308, 319 elastic–viscoelastic correspondence 116, 303 electromagnetic –absorption 259–261 –dispersion 261–263 –polarization 262, 263 –spectrum 259 –wave 227–230 engineered stress proﬁle 132 etching 139 Evan’s law 194f, 197–199 excess volume 63, 66, 78–80, 100

Index

f

glass

fatigue 191ff ﬁbre 5, 11–13, 21, 39f, 46–49, 51, 161, 184, 188, 190, 203–205, 208, 218–224 ﬁbre process 218ff Fick’s law 80, 131, 341f, 347 ﬁctive temperature 123–127 ﬁlms 240–243, 245, 247, 250–255 ﬁning 83, 90f, 203–205, 207ff, 275ff, 341 ﬁnite element analysis –of contact loading 333ff –of crash 330ff –of the pressing of a parison 329ff –of the pression moulding of a glass lens 329ff ﬁnite element modelling see ﬁnite element analysis ﬂat (ﬂoat) glass 1ff, 30, 33ff, 51, 83ff, 203ff, 226ff, 232ff, 250, 254 ﬂaw 135, 138ff, 175, 183 ﬂaw size distribution 157, 283 ﬂint 39ff ﬂoat 35, 39, 41, 203ff ﬂow 83, 89, 94, 98, 103–106, 108, 110, 113, 121f, 171–174, 183, 185 force-penetration curve 162ff, 183, 291, 293–295, 301–305, 307, 329 former 58f, 64, 68, 78 forming 83, 91–93, 105, 203–205, 207f, 214–220 fracture –of bulk 141 –under contact 161ff fragile glass 83ff fragmentation of glass 148, 151 –chart 152 –mechanisms 151f –norm 151f free volume 96, 321, 327 freezing 90, 100, 120 furnace 208, 211 fusion draw 37, 212, 213

–anomalous 172 –assembly 235f –blowing 30, 32, 35, 216f –former 58f, 64, 68 –industry 1–3, 210, 258 –leaching 80, 237f –manufacturers 50f –modiﬁer 53 –network 53 –normal 171f –properties/application 12–14 –process 203 ff –structure 53, 55, 60f –surface 78, 80f –transition 85, 90, 92f, 97, 99, 100ff, 106, 108, 111, 121, 125, 127 –data 99f –deﬁnition 90, 99 –measurement 86–88, 101, 103 –wool 13, 21, 39, 48f, 51, 81 glass-ceramics see vitroceramics glass ﬁber reinforced composites 10–12 glassy state 1, 8, 25, 55f, 90f, 125 glazing –applications –in building 39–44 –in vehicles 41, 43f –coating 240–245, 248–255 –control 225, 232ff –history 27, 35, 37 –mechanical design 18f, 21 –process 203, 205, 210ff –strength 138, 150, 152 –tempering 130f, 133, gob 29 gob feeder 214f Grifﬁth 141, 145 growth of crystals 71–74

g gas 78, 205–208, 219, 341f, 345f

h Hackle zone 139 hardness 170, 172ff –data 173f –deﬁnition 170 –measurement 170, 323 heat soak test 201 history of glass 25–33 hot end coating 218 hydrated glass 81

363

364

Index

i impact fracture 152, 334 indentation –cracks 164–167, 169, 174ff, 189 –curves 303, 305, 333f –plasticity 171 –representative strain 171–173, 296, 298f –stress 162, 167f, 296–300 –toughness 164, 166, 177–179 industrial tools 1, 203, 258 infrared rays 40, 235, 259 ion exchange 80, 130–134, 341 ionic bond 8, 267f

k Kelvin solid 107f, 318

l lateral crack 179 Lehr 210, 212 lenses moulding 203, 329f lifetime 196–199, 201 light see electromagnetic wave liquid state 8, 99–101 liquidus temperature 53, 57, 59, 67, 73, 75f, 99 loss modulus 109f

molecular diffusion 79, 341ff mould –ﬁnishing 216, 218 –mark 216f –parison 216–218

n nanoindentation 291ff natural glass 25–29 network –former 58f –modiﬁer 57–60 –polymerization 55 Newtonian ﬂow 84, 96f, 321–324 nickel sulphide inclusion 199, 205 non-bridging oxygen 57–59, 171 non-Newtonian ﬂow 84, 321–328 nucleation –agents 76f –of crack 174, 178, 189 –of crystals 67, 75 –heterogeneous 70f –homogeneous 68–70

o obsidian 25–27 optical glass 13, 32–34, 46–48, 51 organic glasses 65 Owens process 35

p m Market 235f, 257 materials –properties 10–12 –selection 12–14 matter state 8 Maxwell solid 107f, 304, 318 mechanical design 18–23 median crack 174–177 melting of glass 33f, 205–207 Mendeleev table 5, 6, 54, 64, 266f metallic –bond 6–10 –glasses 63, 65f, 323, 325–328 metals 46 –advantage/drawbacks 7 –group 6–8 mirror zone 138f mist zone 138 mixed-alkali effect 345 modes of fracture 141 modiﬁer 57f, 60 moisture 191, 193f, 199

packing density 62f, 66, 185 performance indices 15–18 permeability 341, 346f photoelasticity –images 288f –principles 227–230 physical vapour deposition (PVD) 43, 240, 241, 244–247, 250, 252, 254f, 258 –process 244–247 –diode sputtering 245 –magnetron sputtering 247f physisorption 78 plane stress 228, 315 plastic deformation 169f, 323 –compaction 171–174, 185 –shear ﬂow 171f, 174 plastics 48 polishing 33, 36, 210, 213 polymers –advantages/drawbacks 7 –group 5f polyvinylbutyral (PVB) 39, 241, 331 precursors 76, 246, 249–251

Index pressing 213, 215–217 process 1ff, 3ff, 203ff proof testing 199 propagation of crack 147, 167, 177, 185, 189, 193, 196, 331 Pyrex 27, 37 PVD see physical vapour deposition

q quality control 225

r radial –distribution 60–63 –median crack 174–177 radioactive wastes 29 recycling 1, 204f reduced time 116, 118 reference temperature 116, 118 refractive index 33f, 46f, 221, 228, 260f refractory 35, 212f regenerators 34, 206f relaxation 6ff, 291ff, 311ff research and development (R&D) 1–3 residual stresses 44, 6–12, 287ff, 335ff –build in 121f, 127 –measurement 231f, 234, 254, 337f –curvature method 253 –photoelastic method 226 –X-ray method 335–339 –proﬁle 119, 131 ring of atoms 54 rule of mixture 12

s sagging 211, 216, 218 scoring 188–190, 210 scratch 185f selection of materials 12–14 self-cleaning 240f, 249 serration 325, 327f shape factor 18–23 sharp contact 169, 175 shear stress 83, 84, 90, 94, 105, 107, 109, 125, 311–314, 317 silica 54–63 silica-soda-lime glass –applications 39ff –composition 25ff –history 25ff –structure 54–63

size effect 157–159 sizing 219f, 240, 254 softening 85f, 90, 102 sol-gel 240–243, 249–252, 254, 255 –process 249–251 spin coating 250 spontaneous fracture 200 static fatigue 191–193, 196f, 201 statistical –analysis 153–159 –fracture 135, 146, 153 strength –deﬁnition 135 –measurement 287–289 –theoretical 135f storage modulus 109–111 strain 5ff, 83ff, 135ff, 161ff, 191ff, 311ff –at fracture 15–17, 136–141 –point 85 –rate 321–325, 328 –tensor 312f strength 135ff, 161, 166, 168, 180 stress 5ff, 83ff, 135ff, 161ff, 191ff, 311ff –concentration 141f –corrosion 192–195 –deviator 316f –ﬁeld –at crack tip 144f –in a beam under ﬂexure 155f –intensity factor 139f, 147f, 167, 181, 192–194 –under non-uniform stress 145, 146 –under uniform stress 138f –meters 231–234 –edge 231–233 –surface 234 –principal 315f –relaxation 107f, 114, 116, 118, 122f, 125, 131–134 –strain curve 136 –tensor 312f structural relaxation 90, 99f, 123–127, 130, 132 sub-critical crack growth 193, 196 super-cooled liquid 90, 92f, 96, 99f, 123, 125f surface 53ff, 161ff, 191ff, 291ff –energy 39–42, 81, 135f, 140, 193, 250 –data 81, 136–141 –mechanics 161f, 165, 291ff –structure 78

365

366

Index

t

v

tektites 28 tempered glass 119, 121, 132, 152, 166, 182f tempering 83, 119, 120–123, 125, 130f, 148, 151f, 181, 203, 211f tensile –drawing 219–221 –stresses 136, 138f –test 136 theoretical strength 135, 158, 279ff thermal –endurance see thermal shock resistance –expansion 6, 10, 15–17, 89, 97, 101–103, 122f, 127, 129, 131, 271ff –shock resistance 15–18 –chart 17 –deﬁnition 15 –tempering 44, 83, 119–128, 130–134, 138, 148, 151f, 181, 200f, 203, 211f thermorheological simplicity 116 thin ﬁlms –function 240–251 –process 240–251 –residual stress 252–254 toughness 7, 10, 12, 136, 140f, 146–148, 153, 164, 166, 177–181, 183f, 192f –chart 10–12 –data 136–141 –deﬁnition 140 –measurement 146–148 –compact tension 146 –double torsion 147–148, 177–179 –indentation 164–167 –notch beam test 146 transient stresses 128–130, 225, 287f transition –homogeneous to heterogeneous ﬂow 328 –Newtonian to non-Newtonian ﬂow 322f –temperature see glass transition transparency 12ff, 39–41, 44–46, 48 TTT diagram 74

van der Waals bond 6, 65 viscoelasticity 107, 114, 122, 292, 295, 302–304 viscometry 86–89, 275ff –falling sphere viscometer 88 –ﬁber elongation viscometer 88f –rotation viscometer 87 viscosity 83ff, 171–173, 203, 207f, 211, 215, 221, 276, 278, 295, 305, 319, 321–325, 327, 329f –data 83–86 –deﬁnition 83 –measurement 86–89 –Newtonian 84, 92 –non-Newtonian 321–325, 327f viscous ﬂow 85, 89, 91, 105, 108, 111, 113, 121, 129, 173, 183, 307, 321 vitroceramics 76 Vogel-Fulcher-Tamman formula 94

w water –corrosion 81 –diffusion 61, 78–80, 95f, 342 –repellence 240–242 weathering 29 weibull –modulus –data 157f –deﬁnition 155 –determination 283–285 –statistics 153, 157, 198, 283ff wetting 49, 241 –angle 242 working point 85, 90

x X-ray diffraction 60f, 63, 335ff

y yield stress 7, 10, 145 Young modulus 10, 12, 15f, 19, 22, 106, 111f, 122, 129, 131, 135–138, 140, 314, 318 –chart 10, 13 –data 136–141 –deﬁnition 137

z Zachariasen model 54

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close